The 4th edition of this highly successful textbook features copious material for a complete upper-level undergraduate or

*1,294*
*208*
*71MB*

*English*
*Pages 926
[905]*
*Year 2021*

- Author / Uploaded
- Marius Grundmann

*Table of contents : PrefaceContentsAbbreviationsSymbolsPhysical Constants1 Introduction 1.1 Timetable and Key Achievements 1.2 Nobel Prize Winners 1.3 General InformationPart I Fundamentals2 Bonds 2.1 Introduction 2.2 Covalent Bonds 2.2.1 Electron-Pair Bond 2.2.2 sp3 Bonds 2.2.3 sp2 Bonds 2.3 Ionic Bonds 2.4 Mixed Bonds 2.5 Metallic Bonding 2.6 Van-der-Waals Bonds 2.7 Hamilton Operator of the Solid3 Crystals 3.1 Introduction 3.2 Crystal Structure 3.3 Lattice 3.3.1 2D Bravais Lattices 3.3.2 3D Bravais Lattices 3.3.3 Unit Cell 3.3.4 Point Group 3.3.5 Space Group 3.3.6 Polycrystalline Semiconductors 3.3.7 Amorphous Semiconductors 3.4 Important Crystal Structures 3.4.1 Rocksalt Structure 3.4.2 CsCl Structure 3.4.3 Diamond Structure 3.4.4 Zincblende Structure 3.4.5 Wurtzite Structure 3.4.6 Chalcopyrite Structure 3.4.7 Spinel Structure 3.4.8 Fluorite Structure 3.4.9 Delafossite Structure 3.4.10 Perovskite Structure 3.4.11 NiAs Structure 3.4.12 Further Structures 3.5 Polytypism and Polymorphism 3.6 Reciprocal Lattice 3.6.1 Reciprocal Lattice Vectors 3.6.2 Miller Indices 3.6.3 Brillouin Zone 3.7 Alloys 3.7.1 Random Alloys 3.7.2 Phase Diagram 3.7.3 Virtual Crystal Approximation 3.7.4 Lattice Parameter 3.7.5 Ordering4 Structural Defects 4.1 Introduction 4.2 Point Defects 4.2.1 Point Defect Types 4.2.2 Thermodynamics 4.2.3 Diffusion 4.2.4 Dopant Distribution 4.2.5 Large Concentration Effects 4.3 Dislocations 4.3.1 Dislocation Types 4.3.2 Visualization of Dislocations by Etching 4.3.3 Impurity Hardening 4.4 Extended Defects 4.4.1 Micro-cracks 4.4.2 Stacking Faults 4.4.3 Grain Boundaries 4.4.4 Antiphase and Inversion Domains 4.5 Disorder5 Mechanical Properties 5.1 Introduction 5.2 Lattice Vibrations 5.2.1 Monoatomic Linear Chain 5.2.2 Diatomic Linear Chain 5.2.3 Mode Patterns and Topological States 5.2.4 Lattice Vibrations of a Three-Dimensional Crystal 5.2.5 Density of States 5.2.6 Phonons 5.2.7 Localized Vibrational Modes 5.2.8 Phonons in Alloys 5.2.9 Disorder 5.2.10 Topological Edge States of a Linear Chain 5.3 Elasticity 5.3.1 Thermal Expansion 5.3.2 Stress–Strain Relation 5.3.3 Biaxial Stress 5.3.4 Three-Dimensional Stress 5.3.5 Substrate Bending 5.3.6 Scrolling 5.4 Plasticity 5.4.1 Critical Thickness 5.4.2 Cleaving 5.4.3 Wafer Breakage6 Band Structure 6.1 Introduction 6.2 Electrons in a Periodic Potential 6.2.1 Bloch's Theorem 6.2.2 Free-Electron Dispersion 6.2.3 Non-Vanishing Potential 6.2.4 Kramer's Degeneracy 6.2.5 Symmetry Considerations 6.2.6 Topological Considerations 6.3 Band Structures of Selected Semiconductors 6.3.1 Silicon 6.3.2 Germanium 6.3.3 GaAs 6.3.4 GaP 6.3.5 GaN 6.3.6 Lead Salts 6.3.7 MgO, ZnO, CdO 6.3.8 Chalcopyrites 6.3.9 Spinels 6.3.10 Delafossites 6.3.11 Perovskites 6.4 Systematics of Semiconductor Band Gaps 6.5 Alloy Semiconductors 6.6 Amorphous Semiconductors 6.7 Temperature Dependence of the Band Gap 6.8 Isotope Dependence of the Band Gap 6.9 Electron Dispersion 6.9.1 Equation of Electron Motion 6.9.2 Effective Mass of Electrons 6.9.3 Nonparabolicity of Electron Mass 6.10 Holes 6.10.1 Hole Concept 6.10.2 Hole Dispersion Relation 6.10.3 Valence-Band Fine Structure 6.11 Band Inversion 6.12 Strain Effects on the Band Structure 6.12.1 Strain Effect on Band Edges 6.12.2 Strain Effect on Effective Masses 6.12.3 Interaction With a Localized Level 6.13 Density of States 6.13.1 General Band Structure 6.13.2 Amorphous Semiconductors 6.13.3 Free-Electron Gas7 Electronic Defect States 7.1 Introduction 7.2 Carrier Concentration 7.3 Intrinsic Conduction 7.4 Doping 7.4.1 Concept 7.4.2 Doping Principles 7.5 Shallow Defects 7.5.1 Donors 7.5.2 Acceptors 7.5.3 Compensation 7.5.4 Multiple Impurities 7.5.5 Amphoteric Impurities 7.5.6 Autodoping 7.5.7 High Doping 7.6 Quasi-fermi Levels 7.7 Deep Levels 7.7.1 Charge States 7.7.2 Double Donors 7.7.3 Double Acceptors 7.7.4 Jahn–Teller Effect 7.7.5 Negative-U Center 7.7.6 DX Center 7.7.7 EL2 Defect 7.7.8 Semi-insulating Semiconductors 7.7.9 Isoelectronic Impurities 7.7.10 Surface States 7.8 The Charge Neutrality Level 7.9 Hydrogen in Semiconductors8 Transport 8.1 Introduction 8.2 Conductivity 8.3 Low-Field Transport 8.3.1 Mobility 8.3.2 Microscopic Scattering Processes 8.3.3 Ionized Impurity Scattering 8.3.4 Deformation Potential Scattering 8.3.5 Piezoelectric Potential Scattering 8.3.6 Polar Optical Scattering 8.3.7 Dislocation Scattering 8.3.8 Grain Boundary Scattering 8.3.9 Alloy Scattering 8.3.10 Dipole Scattering 8.3.11 Temperature Dependence 8.3.12 Doping Dependence 8.3.13 Superconductivity 8.3.14 Piezoresistivity 8.4 High-Field Transport 8.4.1 Drift-Saturation Velocity 8.4.2 Negative Differential Resistivity 8.4.3 Velocity Overshoot 8.4.4 Impact Ionization 8.5 High-Frequency Transport 8.6 Impurity Band Transport 8.7 Polarons 8.7.1 Large Polarons 8.7.2 Small Polarons 8.8 Hopping Transport 8.9 Transport in Amorphous Semiconductors 8.10 Ionic Transport 8.11 Diffusion 8.12 Continuity Equation 8.13 Heat Conduction 8.14 Coupled Heat and Charge Transport 8.14.1 Thermopower and Seebeck Effect 8.14.2 Peltier Effect9 Optical Properties 9.1 Spectral Regions and Overview 9.2 Complex Dielectric Function 9.3 Reflection and Diffraction 9.4 Absorption 9.5 Dielectric Function due to Optical Phonons 9.6 Electron–Photon Interaction 9.7 Band–Band Transitions 9.7.1 Joint Density of States 9.7.2 Direct Transitions 9.7.3 Indirect Transitions 9.7.4 Urbach Tail 9.7.5 Amorphous Semiconductors 9.7.6 Excitons 9.7.7 Phonon Broadening 9.7.8 Exciton Polariton 9.7.9 Bound-Exciton Absorption 9.7.10 Biexcitons 9.7.11 Trions 9.7.12 Band Gap Renormalization 9.7.13 Electron–Hole Droplets 9.7.14 Two-Photon Absorption 9.8 Impurity Absorption 9.8.1 Shallow Levels 9.8.2 Deep Levels 9.9 Absorption in the Presence of Free Charge Carriers 9.9.1 Absorption Coefficient, Plasma Frequency 9.9.2 Burstein–Moss Shift 9.9.3 Inter-Valenceband Transitions 9.9.4 Inter-Valley Transitions 9.9.5 Intra-Band Transitions 9.10 Lattice Absorption 9.10.1 Dielectric Constant 9.10.2 Reststrahlenbande 9.10.3 Polaritons 9.10.4 Phonon–Plasmon Coupling10 Recombination 10.1 Introduction 10.2 Band–Band Recombination 10.2.1 Spontaneous Emission 10.2.2 Absorption 10.2.3 Stimulated Emission 10.2.4 Net Recombination Rate 10.2.5 Recombination Dynamics 10.2.6 Lasing 10.3 Exciton Recombination 10.3.1 Free Excitons 10.3.2 Bound Excitons 10.3.3 Alloy Broadening 10.4 Phonon Replica 10.5 Self-Absorption 10.6 Donor–Acceptor Pair Transitions 10.7 Inner-Impurity Recombination 10.8 Auger Recombination 10.9 Band–Impurity Recombination 10.9.1 Shockley–Read–Hall Kinetics 10.9.2 Multilevel Traps 10.10 ABC Model 10.11 Field Effect 10.11.1 Thermally Activated Emission 10.11.2 Direct Tunneling 10.11.3 Assisted Tunneling 10.12 Recombination at Extended Defects 10.12.1 Surfaces 10.12.2 Grain Boundaries 10.12.3 Dislocations 10.13 Excess-Carrier Profiles 10.13.1 Generation at Surface 10.13.2 Generation in the BulkPart II Selected Topics11 Surfaces 11.1 Introduction 11.2 Surface Crystallography 11.3 Surface Energy 11.4 Surface Reconstruction 11.5 Surface Morphology 11.6 Surface Physical Properties 11.6.1 Surface Phonons 11.6.2 Surface Plasmons 11.6.3 Electronic Surface States12 Heterostructures 12.1 Introduction 12.2 Heteroepitaxy 12.2.1 Growth Methods 12.2.2 Substrates 12.2.3 Growth Modes 12.2.4 Heterosubstrates 12.2.5 Patterned Substrates 12.2.6 Pseudomorphic Structures 12.2.7 Plastic Relaxation 12.2.8 Surfactants 12.3 Energy Levels in Heterostructures 12.3.1 Band Lineup in Heterostructures 12.3.2 Quantum Wells 12.3.3 Superlattices 12.3.4 Heterointerface Between Doped Materials 12.3.5 Heterointerface Between Semiconductors with Band Structures of Different Topology 12.4 Recombination in Quantum Wells 12.4.1 Thickness Dependence 12.4.2 Broadening Effects 12.4.3 Quantum Confined Stark Effect 12.5 Isotope Superlattices 12.6 Wafer Bonding13 Two-Dimensional Semiconductors 13.1 Graphene and Related Materials 13.1.1 Structural Properties 13.1.2 Band Structures 13.1.3 Electrical Properties 13.1.4 Optical Properties 13.2 Two-Dimensional Compound Semiconductors 13.2.1 Structural Properties 13.2.2 Band Structures 13.2.3 Optical Properties and Valley Polarization 13.2.4 Excitons 13.3 Van-der-Waals Heterostructures14 Nanostructures 14.1 Introduction 14.2 Quantum Wires 14.2.1 V-Groove Quantum Wires 14.2.2 Cleaved-Edge Overgrowth Quantum Wires 14.2.3 Nanowhiskers 14.2.4 Nanobelts 14.2.5 Quantization in Two-Dimensional Potential Wells 14.3 Carbon Nanotubes 14.3.1 Structure 14.3.2 Band Structure 14.3.3 Optical Properties 14.3.4 Other Anorganic Nanotubes 14.4 Quantum Dots 14.4.1 Quantization in Three-Dimensional Potential Wells 14.4.2 Electrical and Transport Properties 14.4.3 Self-Assembled Preparation 14.4.4 Optical Properties15 External Fields 15.1 Electric Fields 15.1.1 Bulk Material 15.1.2 Quantum Wells 15.2 Magnetic Fields 15.2.1 Classical Hall Effect 15.2.2 Free-Carrier Absorption 15.2.3 Energy Levels in Bulk Crystals 15.2.4 Magnetic Field Effect on Impurities 15.2.5 Magnetic Field Effect on Excitons 15.2.6 Energy Levels in a 2DEG 15.2.7 Shubnikov-De Haas Oscillations 15.2.8 Quantum Hall Effect16 Polarized Semiconductors 16.1 Introduction 16.2 Spontaneous Polarization 16.3 Ferroelectricity 16.3.1 Materials 16.3.2 Soft Phonon Mode 16.3.3 Phase Transition 16.3.4 Domains 16.3.5 Optical Properties 16.4 Piezoelectricity 16.4.1 Piezoelectric Effect 16.4.2 Zincblende Crystals 16.4.3 Wurtzite Crystals 16.4.4 Piezoelectric Effects in Nanostructures17 Magnetic Semiconductors 17.1 Introduction 17.2 Magnetic Semiconductors 17.3 Diluted Magnetic Semiconductors 17.4 Spintronics 17.4.1 Spin Transistor 17.4.2 Spin LED18 Organic Semiconductors 18.1 Introduction 18.2 Materials 18.2.1 Small Organic Molecules, Polymers 18.2.2 Organic Semiconductor Crystals 18.3 Electronic Structure 18.4 Doping 18.5 Transport Properties 18.6 Optical Properties19 Dielectric Structures 19.1 Photonic Band Gap Materials 19.1.1 Introduction 19.1.2 General 1D Scattering Theory 19.1.3 Transmission of an N-Period Potential 19.1.4 The Quarter-Wave Stack 19.1.5 Formation of a 3D Band Structure 19.1.6 Disorder 19.1.7 Defect Modes 19.1.8 Topological Photonic Band Structures 19.1.9 Coupling to an Electronic Resonance 19.1.10 Hyperbolic Optical Metamaterials 19.2 Microscopic Resonators 19.2.1 Microdiscs 19.2.2 Purcell Effect 19.2.3 Deformed Resonators 19.2.4 Hexagonal Cavities20 Transparent Conductive Oxide Semiconductors 20.1 Introduction 20.2 Materials 20.3 PropertiesPart III Applications21 Diodes 21.1 Introduction 21.2 Metal-Semiconductor Contacts 21.2.1 Band Diagram in Equilibrium 21.2.2 Space-Charge Region 21.2.3 Schottky Effect 21.2.4 Capacitance 21.2.5 Current-Voltage Characteristic 21.2.6 Ohmic Contacts 21.2.7 Metal Contacts to Organic Semiconductors 21.3 Metal-Insulator-Semiconductor Diodes 21.3.1 Band Diagram for Ideal MIS Diode 21.3.2 Space-Charge Region 21.3.3 Capacitance 21.3.4 Nonideal MIS Diode 21.4 Bipolar Diodes 21.4.1 Band Diagram 21.4.2 Space-Charge Region 21.4.3 Capacitance 21.4.4 Current-Voltage Characteristics 21.4.5 Breakdown 21.4.6 Heterostructure Diodes 21.4.7 Organic Semiconductor Diodes 21.5 Applications and Special Diode Devices 21.5.1 Rectification 21.5.2 Frequency Mixing 21.5.3 Voltage Regulator 21.5.4 Zener Diodes 21.5.5 Varactors 21.5.6 Fast-Recovery Diodes 21.5.7 Step-Recovery Diodes 21.5.8 Pin-Diodes 21.5.9 Tunneling Diodes 21.5.10 Backward Diodes 21.5.11 Gunn Diodes22 Light-to-Electricity Conversion 22.1 Photocatalysis 22.2 Photoconductors 22.2.1 Introduction 22.2.2 Photoconductivity Detectors 22.2.3 Electrophotography 22.2.4 QWIPs 22.2.5 Blocked Impurity-Band Detectors 22.3 Photodiodes 22.3.1 Introduction 22.3.2 Pn Photodiodes 22.3.3 Pin Photodiodes 22.3.4 Position-Sensing Detector 22.3.5 MSM Photodiodes 22.3.6 Avalanche Photodiodes 22.3.7 Traveling-Wave Photodetectors 22.3.8 Charge Coupled Devices 22.3.9 Photodiode Arrays 22.4 Solar Cells 22.4.1 Solar Radiation 22.4.2 Ideal Solar Cells 22.4.3 Real Solar Cells 22.4.4 Design Refinements 22.4.5 Modules 22.4.6 Solar-Cell Types 22.4.7 Economic Issues23 Electricity-to-Light Conversion 23.1 Radiometric and Photometric Quantities 23.1.1 Radiometric Quantities 23.1.2 Photometric Quantities 23.2 Scintillators 23.2.1 CIE Chromaticity Diagram 23.2.2 Display Applications 23.2.3 Radiation Detection 23.2.4 Luminescence Mechanisms 23.3 Light-Emitting Diodes 23.3.1 Introduction 23.3.2 Spectral Ranges 23.3.3 Efficiencies 23.3.4 Device Design 23.3.5 White LEDs 23.3.6 Quantum Dot LEDs 23.3.7 Organic LEDs 23.4 Lasers 23.4.1 Introduction 23.4.2 Applications 23.4.3 Gain 23.4.4 Optical Mode 23.4.5 Loss Mechanisms 23.4.6 Threshold 23.4.7 Spontaneous Emission Factor 23.4.8 Output Power 23.4.9 Temperature Dependence 23.4.10 Mode Spectrum 23.4.11 Longitudinal Single-Mode Lasers 23.4.12 Tunability 23.4.13 Dynamics and Modulation 23.4.14 Surface-Emitting Lasers 23.4.15 Optically Pumped Semiconductor Lasers 23.4.16 Quantum Cascade Lasers 23.4.17 Hot-Hole Lasers 23.5 Semiconductor Optical Amplifiers24 Transistors 24.1 Introduction 24.2 Bipolar Transistors 24.2.1 Carrier Density and Currents 24.2.2 Current Amplification 24.2.3 Ebers-Moll Model 24.2.4 Current–Voltage Characteristics 24.2.5 Basic Circuits 24.2.6 High-Frequency Properties 24.2.7 Heterojunction Bipolar Transistors 24.2.8 Light-Emitting Transistors 24.3 Field-Effect Transistors 24.4 JFET and MESFET 24.4.1 General Principle 24.4.2 Static Characteristics 24.4.3 Normally On and Normally Off FETs 24.4.4 Field-Dependent Mobility 24.4.5 High-Frequency Properties 24.5 MOSFETs 24.5.1 Operation Principle 24.5.2 Current–Voltage Characteristics 24.5.3 MOSFET Types 24.5.4 Complementary MOS 24.5.5 Large-Scale Integration 24.5.6 Tunneling FETs 24.5.7 Nonvolatile Memories 24.5.8 Heterojunction FETs 24.6 Thin-Film Transistors 24.6.1 Annealing of Amorphous Silicon 24.6.2 TFT Devices 24.6.3 Transistors with 2D Materials 24.6.4 OFETsAppendix A TensorsA.1 IntroductionA.2 Rotation of Coordinate SystemA.3 Rank-n TensorsAppendix B Point and Space GroupsAppendix C Kramers–Kronig RelationsAppendix D Oscillator StrengthAppendix E Quantum StatisticsE.1 IntroductionE.2 Partition SumE.3 Photon StatisticsE.4 Fermi–Dirac StatisticsE.5 Bose–Einstein DistributionAppendix F Kronig-Penney ModelAppendix G Tight-Binding ModelG.1 ConceptG.2 One-Dimensional ModelG.3 Two-Dimensional LatticesG.3.1 Square LatticeG.3.2 Honeycomb LatticeG.4 Edge States and Topological AspectsG.4.1 One-Dimensional ModelG.4.2 Two-Dimensional ModelsAppendix H k cdotp Perturbation TheoryAppendix I Effective-Mass TheoryAppendix J Boltzmann Transport TheoryJ.1 Boltzmann Transport EquationJ.2 ConductivityJ.3 Hall EffectJ.4 ThermopowerAppendix K NoiseK.1 Fluctuating signalsK.2 CorrelationsK.3 Noise spectrumK.3.1 Thermal NoiseK.3.2 1/f NoiseK.3.3 Shot NoiseK.3.4 Generation-Recombination NoiseAppendix ReferencesIndex*

Graduate Texts in Physics

Marius Grundmann

The Physics of Semiconductors An Introduction Including Nanophysics and Applications Fourth Edition

Graduate Texts in Physics Series Editors Kurt H. Becker, NYU Polytechnic School of Engineering, Brooklyn, NY, USA Jean-Marc Di Meglio, Matière et Systèmes Complexes, Bâtiment Condorcet, Université Paris Diderot, Paris, France Morten Hjorth-Jensen, Department of Physics, Blindern, University of Oslo, Oslo, Norway Bill Munro, NTT Basic Research Laboratories, Atsugi, Japan William T. Rhodes, Department of Computer and Electrical Engineering and Computer Science, Florida Atlantic University, Boca Raton, FL, USA Susan Scott, Australian National University, Acton, Australia H. Eugene Stanley, Center for Polymer Studies, Physics Department, Boston University, Boston, MA, USA Martin Stutzmann, Walter Schottky Institute, Technical University of Munich, Garching, Germany Andreas Wipf, Institute of Theoretical Physics, Friedrich-Schiller-University Jena, Jena, Germany

Graduate Texts in Physics publishes core learning/teaching material for graduate- and advanced-level undergraduate courses on topics of current and emerging ﬁelds within physics, both pure and applied. These textbooks serve students at the MS- or PhD-level and their instructors as comprehensive sources of principles, deﬁnitions, derivations, experiments and applications (as relevant) for their mastery and teaching, respectively. International in scope and relevance, the textbooks correspond to course syllabi sufﬁciently to serve as required reading. Their didactic style, comprehensiveness and coverage of fundamental material also make them suitable as introductions or references for scientists entering, or requiring timely knowledge of, a research ﬁeld.

More information about this series at http://www.springer.com/series/8431

Marius Grundmann

The Physics of Semiconductors An Introduction Including Nanophysics and Applications Fourth Edition

123

Marius Grundmann Felix Bloch Institute for Solid State Physics Universität Leipzig Leipzig, Germany

ISSN 1868-4513 ISSN 1868-4521 (electronic) Graduate Texts in Physics ISBN 978-3-030-51568-3 ISBN 978-3-030-51569-0 (eBook) https://doi.org/10.1007/978-3-030-51569-0 1st–3rd editions: © Springer International Publishing Switzerland 2006, 2010, 2016 4th edition: © Springer Nature Switzerland AG 2021 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, expressed or implied, with respect to the material contained herein or for any errors or omissions that may have been made. The publisher remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations. Cover Credit line: “Whispering gallery mode in circular cavity. Image: Th. Nobis, M. Grundmann, Universität Leipzig” This Springer imprint is published by the registered company Springer Nature Switzerland AG The registered company address is: Gewerbestrasse 11, 6330 Cham, Switzerland

To Michelle, Sophia Charlotte and Isabella Rose

Preface

Semiconductor electronics is commonplace in every household. Semiconductor devices have enabled economically reasonable ﬁber-based optical communication, optical storage and high-frequency ampliﬁcation and have recently revolutionized photography, display technology and lighting. By now solar energy harvesting with photovoltaics contributes a signiﬁcant portion to the energy mix. Along with these tremendous technological developments, semiconductors have changed the way we work, communicate, entertain and think. The technological progress of semiconductor materials and devices is evolving continuously with a large worldwide effort in human and monetary capital. For students, semiconductors offer a rich and exciting ﬁeld with a great tradition, offering diverse fundamental and applied topics [1] and a bright future. This book introduces students to semiconductor physics and semiconductor devices. It brings them to the point where they can specialize and enter supervised laboratory research. It is based on the two semester semiconductor physics course taught at Universität Leipzig in its Master of Science physics curriculum. Since the book can be followed with little or no pre-existing knowledge in solid-state physics and quantum mechanics, it is also suitable for undergraduate students. For the interested reader many additional topics are included in the book that can be covered in subsequent, more specialized courses. The material is selected to provide a balance between aspects of solid-state and semiconductor physics, the concepts of various semiconductor devices and modern applications in electronics and photonics. The ﬁrst semester contains the fundamentals of semiconductor physics (Part I, Chaps. 1–10) and selected topics from Part II (Chaps. 11–20). Besides important aspects of solid-state physics such as crystal structure, lattice vibrations and band structure, semiconductor speciﬁcs such as technologically relevant materials and their properties, doping and electronic defects, recombination, surfaces, heteroand nanostructures are discussed. Semiconductors with electric polarization and magnetization are introduced. The emphasis is put on inorganic semiconductors, but a brief introduction to organic semiconductors is given in Chap. 18. Dielectric structures (Chap. 19) serve as mirrors, cavities and microcavities and are a vital part of many semiconductor devices. Other sections give introductions to 2D materials (Chap. 13) and transparent conductive oxides (TCOs) (Chap. 20). The third part (Part III—Chaps. 21–24) is dedicated to semiconductor applications and devices that are taught in the second semester of the course. After a general and detailed discussion of various diode types and their physical mechanisms, their applications in electrical circuits, photodetectors, solar cells, light-emitting diodes and lasers are treated. Finally, bipolar and ﬁeld-effect transistors including thin ﬁlm transistors are discussed. In the present text of the fourth edition many passages have been revised and updated, e.g. lead halide perovskites, dipole scattering, anisotropic dielectric function, valley polarization, Dember ﬁeld, new CMOS image sensors. A new chapter is devoted to 2D semiconductors and an appendix on tight-binding theory has been added. The concept of topological properties now permeates the book; it is introduced for mechanical vibrations in the diatomic linear chain model and appears in chapters on band structure and photonic dielectric structures. Last but not least a few errors and misprints have vii

viii

Preface

Fig. 1 Histogram of references in this book together with simpliﬁed ﬁts visualizing major developments

been corrected. More than 300 additional references, some old and many brand new, have been included (compared to the third edition) and doi's for most of them are provided for easy retrieval. The references have been selected to (i) cover important historical and milestone papers, (ii) direct to reviews and topical books for further reading and (iii) give access to original literature and up-to-date research. In Fig. 1, a histogram of the references by year is shown. Roughly four phases of semiconductor physics and technology can be seen. Before the realization of the ﬁrst transistor in 1947, only a few publications are noteworthy. Then an intense phase of understanding the physics of semiconductors and developing semiconductor technology and devices based on bulk semiconductors (mostly Ge, Si, GaAs) followed. At the end of the 1970s, a new era began with the advent of quantum wells and heterostructures, and later nanostructures (nanotubes, nanowires and quantum dots) and new materials (e.g. organic semiconductors, nitrides or graphene). Another peak develops with emerging topics such as 2D materials, topological insulators or novel amorphous semiconductors. I would like to thank numerous colleagues for their various contributions to this book, in alphabetical order (if no afﬁliation is given, at the time at Universität Leipzig): Gabriele Benndorf, Klaus Bente, Rolf Böttcher, Matthias Brandt, Christian Czekalla, Christof Peter Dietrich, Pablo Esquinazi, Heiko Frenzel, Volker Gottschalch, Helena Hilmer, Axel Hoffmann (TU Berlin), Alois Krosty (Otto-von-Guericke Universität Magdeburg), Evgeny Krüger, Michael Lorenz, Stefan Müller, Thomas Nobis, Rainer Pickenhain, Hans-Joachim Queisser (Max-Planck-Institut für Festkörperforschung, Stuttgart), Bernd Rauschenbach, Bernd Rheinländer, Heidemarie Schmidt, Mathias Schmidt, Rüdiger Schmidt-Grund, Matthias Schubert, Jan Sellmann, Oliver Stier (TU Berlin), Chris Sturm, Florian Tendille (CNRS-CRHEA), Gerald Wagner, Eicke Weber (UC Berkeley), Holger von Wenckstern, Michael Ziese and Gregor Zimmermann. This book has beneﬁtted from their comments, proof reading, experimental data and graphic material. Also, numerous helpful comments from my students on my lectures and the previous editions of this book are gratefully acknowledged. I am also indebted to many other colleagues, in particular to (in alphabetical order) Gerhard Abstreiter, Zhores Alferovy , Martin Allen, Levon Asryan, Günther Bauer, Manfred Bayer, Friedhelm Bechstedt, Dieter Bimberg, Otto Breitenstein, Len Brillson, Fernando Briones, Immanuel Brosery , Jean-Michel Chauveau, Jürgen Christen, Philippe De Mierry, Steve Durbin, Laurence Eaves, Klaus Ellmer, Guy Feuillet, Elvira Fortunato, Ulrich Göseley , Alfred Forchel, Manus Hayne, Frank Heinrichsdorff, Fritz Hennebergery , Detlev Heitmann, Robert Heitzy , Evamarie Hey-Hawkins, Detlef Hommel, Evgeni Kaidashev, Eli Kapon, Nils Kirstaedter, Claus Klingshirn, Fred Kochy , Jörg Kotthaus, Nikolai Ledentsov, Peter Littlewood, Dave Look, Axel Lorke, Anupam Madhukar, Jan

Preface

ix

Meijer, Ingrid Mertig, Bruno Meyery , David Mowbray, Hisao Nakashima, Jörg Neugebauer, Michael Oestreich, Louis Piper, Mats-Erik Pistol, Fred Pollaky , Emil V. Prodan, Volker Riedey , Bernd Rosenow, Hiroyuki Sakaki, Lars Samuelson, Darrell Schlom, Vitali Shchukin, Maurice Skolnick, Robert Suris, Volker Türck, Konrad Ungery , Victor Ustinov, Borge Vinter, Leonid Vorob’jev, Richard Warburton, Alexander Weber, Peter Werner, Wolf Widdra, Ulrike Woggon, Roland Zimmermann, Arthur Zrenner, Alex Zunger and Jesús Zúñiga-Pérez, with whom I have worked closely, had enjoyable discussions with and who have posed questions that stimulated me. It is my distinct privilege and joy that this list becomes longer as I pursue studies in semiconductor physics but sadly the number of y-symbols increases too rapidly from edition to edition. Leipzig, Germany May 2020

Marius Grundmann

Contents

1

Introduction . . . . . . . . . . . . . . . . . . . . . 1.1 Timetable and Key Achievements 1.2 Nobel Prize Winners . . . . . . . . . . 1.3 General Information . . . . . . . . . .

Part I

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

1 1 12 14

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

Fundamentals

2

Bonds . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Introduction . . . . . . . . . . . . . . 2.2 Covalent Bonds . . . . . . . . . . . 2.2.1 Electron-Pair Bond . . 2.2.2 sp3 Bonds . . . . . . . . 2.2.3 sp2 Bonds . . . . . . . . 2.3 Ionic Bonds . . . . . . . . . . . . . . 2.4 Mixed Bonds . . . . . . . . . . . . . 2.5 Metallic Bonding . . . . . . . . . . 2.6 Van-der-Waals Bonds . . . . . . . 2.7 Hamilton Operator of the Solid

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

21 21 21 21 22 25 27 28 31 31 32

3

Crystals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Introduction . . . . . . . . . . . . . . . . . . . . . 3.2 Crystal Structure . . . . . . . . . . . . . . . . . . 3.3 Lattice . . . . . . . . . . . . . . . . . . . . . . . . . 3.3.1 2D Bravais Lattices . . . . . . . . 3.3.2 3D Bravais Lattices . . . . . . . . 3.3.3 Unit Cell . . . . . . . . . . . . . . . . 3.3.4 Point Group . . . . . . . . . . . . . . 3.3.5 Space Group . . . . . . . . . . . . . 3.3.6 Polycrystalline Semiconductors 3.3.7 Amorphous Semiconductors . . 3.4 Important Crystal Structures . . . . . . . . . 3.4.1 Rocksalt Structure . . . . . . . . . 3.4.2 CsCl Structure . . . . . . . . . . . . 3.4.3 Diamond Structure . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

. . . . . . . . . . . . . . .

35 35 35 36 36 37 40 41 42 43 43 44 45 45 45

. . . . . . . . . . .

. . . . . . . . . . .

xi

xii

Contents

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

46 47 48 49 51 51 52 53 53 54 56 56 57 60 60 61 63 65 65 67

4

Structural Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Point Defects . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.1 Point Defect Types . . . . . . . . . . . . . . . . 4.2.2 Thermodynamics . . . . . . . . . . . . . . . . . 4.2.3 Diffusion . . . . . . . . . . . . . . . . . . . . . . . 4.2.4 Dopant Distribution . . . . . . . . . . . . . . . 4.2.5 Large Concentration Effects . . . . . . . . . 4.3 Dislocations . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.1 Dislocation Types . . . . . . . . . . . . . . . . . 4.3.2 Visualization of Dislocations by Etching 4.3.3 Impurity Hardening . . . . . . . . . . . . . . . 4.4 Extended Defects . . . . . . . . . . . . . . . . . . . . . . . . 4.4.1 Micro-cracks . . . . . . . . . . . . . . . . . . . . 4.4.2 Stacking Faults . . . . . . . . . . . . . . . . . . . 4.4.3 Grain Boundaries . . . . . . . . . . . . . . . . . 4.4.4 Antiphase and Inversion Domains . . . . . 4.5 Disorder . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

69 69 69 69 70 73 75 78 81 82 85 88 88 88 89 90 93 94

5

Mechanical Properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 Lattice Vibrations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.1 Monoatomic Linear Chain . . . . . . . . . . . . . . . . . 5.2.2 Diatomic Linear Chain . . . . . . . . . . . . . . . . . . . . 5.2.3 Mode Patterns and Topological States . . . . . . . . . 5.2.4 Lattice Vibrations of a Three-Dimensional Crystal 5.2.5 Density of States . . . . . . . . . . . . . . . . . . . . . . . . 5.2.6 Phonons . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2.7 Localized Vibrational Modes . . . . . . . . . . . . . . . . 5.2.8 Phonons in Alloys . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

95 95 95 96 99 101 104 107 109 110 112

3.5 3.6

3.7

3.4.4 Zincblende Structure . . . . . . . . 3.4.5 Wurtzite Structure . . . . . . . . . 3.4.6 Chalcopyrite Structure . . . . . . 3.4.7 Spinel Structure . . . . . . . . . . . 3.4.8 Fluorite Structure . . . . . . . . . . 3.4.9 Delafossite Structure . . . . . . . . 3.4.10 Perovskite Structure . . . . . . . . 3.4.11 NiAs Structure . . . . . . . . . . . . 3.4.12 Further Structures . . . . . . . . . . Polytypism and Polymorphism . . . . . . . Reciprocal Lattice . . . . . . . . . . . . . . . . . 3.6.1 Reciprocal Lattice Vectors . . . 3.6.2 Miller Indices . . . . . . . . . . . . . 3.6.3 Brillouin Zone . . . . . . . . . . . . Alloys . . . . . . . . . . . . . . . . . . . . . . . . . 3.7.1 Random Alloys . . . . . . . . . . . 3.7.2 Phase Diagram . . . . . . . . . . . . 3.7.3 Virtual Crystal Approximation 3.7.4 Lattice Parameter . . . . . . . . . . 3.7.5 Ordering . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . .

Contents

5.3

5.4

6

xiii

5.2.9 Disorder . . . . . . . . . . . . . . 5.2.10 Topological Edge States of Elasticity . . . . . . . . . . . . . . . . . . . . 5.3.1 Thermal Expansion . . . . . . 5.3.2 Stress–Strain Relation . . . . 5.3.3 Biaxial Stress . . . . . . . . . . 5.3.4 Three-Dimensional Stress . 5.3.5 Substrate Bending . . . . . . 5.3.6 Scrolling . . . . . . . . . . . . . Plasticity . . . . . . . . . . . . . . . . . . . . 5.4.1 Critical Thickness . . . . . . . 5.4.2 Cleaving . . . . . . . . . . . . . 5.4.3 Wafer Breakage . . . . . . . .

..................... the Diatomic Linear Chain . ..................... ..................... ..................... ..................... ..................... ..................... ..................... ..................... ..................... ..................... .....................

Band Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . 6.2 Electrons in a Periodic Potential . . . . . . . . . 6.2.1 Bloch’s Theorem . . . . . . . . . . . . . 6.2.2 Free-Electron Dispersion . . . . . . . . 6.2.3 Non-Vanishing Potential . . . . . . . . 6.2.4 Kramer’s Degeneracy . . . . . . . . . . 6.2.5 Symmetry Considerations . . . . . . . 6.2.6 Topological Considerations . . . . . . 6.3 Band Structures of Selected Semiconductors 6.3.1 Silicon . . . . . . . . . . . . . . . . . . . . . 6.3.2 Germanium . . . . . . . . . . . . . . . . . 6.3.3 GaAs . . . . . . . . . . . . . . . . . . . . . . 6.3.4 GaP . . . . . . . . . . . . . . . . . . . . . . . 6.3.5 GaN . . . . . . . . . . . . . . . . . . . . . . 6.3.6 Lead Salts . . . . . . . . . . . . . . . . . . 6.3.7 MgO, ZnO, CdO . . . . . . . . . . . . . 6.3.8 Chalcopyrites . . . . . . . . . . . . . . . 6.3.9 Spinels . . . . . . . . . . . . . . . . . . . . 6.3.10 Delafossites . . . . . . . . . . . . . . . . 6.3.11 Perovskites . . . . . . . . . . . . . . . . . . 6.4 Systematics of Semiconductor Band Gaps . . 6.5 Alloy Semiconductors . . . . . . . . . . . . . . . . . 6.6 Amorphous Semiconductors . . . . . . . . . . . . 6.7 Temperature Dependence of the Band Gap . . 6.8 Isotope Dependence of the Band Gap . . . . . 6.9 Electron Dispersion . . . . . . . . . . . . . . . . . . 6.9.1 Equation of Electron Motion . . . . 6.9.2 Effective Mass of Electrons . . . . . . 6.9.3 Nonparabolicity of Electron Mass 6.10 Holes . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.10.1 Hole Concept . . . . . . . . . . . . . . . . 6.10.2 Hole Dispersion Relation . . . . . . . 6.10.3 Valence-Band Fine Structure . . . . . 6.11 Band Inversion . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

114 115 118 118 118 122 123 126 127 129 129 133 133

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

135 135 135 135 136 137 140 141 142 144 144 145 145 146 146 146 147 147 149 149 149 150 152 153 154 158 158 158 159 162 163 163 164 168 169

xiv

Contents

6.12

6.13

Strain Effects on the Band Structure . . . . . . 6.12.1 Strain Effect on Band Edges . . . . . 6.12.2 Strain Effect on Effective Masses . 6.12.3 Interaction With a Localized Level Density of States . . . . . . . . . . . . . . . . . . . . 6.13.1 General Band Structure . . . . . . . . . 6.13.2 Amorphous Semiconductors . . . . . 6.13.3 Free-Electron Gas . . . . . . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

. . . . . . . .

170 170 172 173 173 173 174 175

7

Electronic Defect States . . . . . . . . . . . . . . . . . . 7.1 Introduction . . . . . . . . . . . . . . . . . . . . . . 7.2 Carrier Concentration . . . . . . . . . . . . . . . 7.3 Intrinsic Conduction . . . . . . . . . . . . . . . . 7.4 Doping . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4.1 Concept . . . . . . . . . . . . . . . . . . 7.4.2 Doping Principles . . . . . . . . . . . 7.5 Shallow Defects . . . . . . . . . . . . . . . . . . . 7.5.1 Donors . . . . . . . . . . . . . . . . . . 7.5.2 Acceptors . . . . . . . . . . . . . . . . . 7.5.3 Compensation . . . . . . . . . . . . . 7.5.4 Multiple Impurities . . . . . . . . . . 7.5.5 Amphoteric Impurities . . . . . . . 7.5.6 Autodoping . . . . . . . . . . . . . . . 7.5.7 High Doping . . . . . . . . . . . . . . 7.6 Quasi-fermi Levels . . . . . . . . . . . . . . . . . 7.7 Deep Levels . . . . . . . . . . . . . . . . . . . . . . 7.7.1 Charge States . . . . . . . . . . . . . 7.7.2 Double Donors . . . . . . . . . . . . . 7.7.3 Double Acceptors . . . . . . . . . . 7.7.4 Jahn–Teller Effect . . . . . . . . . . . 7.7.5 Negative-U Center . . . . . . . . . . 7.7.6 DX Center . . . . . . . . . . . . . . . . 7.7.7 EL2 Defect . . . . . . . . . . . . . . . 7.7.8 Semi-insulating Semiconductors 7.7.9 Isoelectronic Impurities . . . . . . . 7.7.10 Surface States . . . . . . . . . . . . . 7.8 The Charge Neutrality Level . . . . . . . . . . 7.9 Hydrogen in Semiconductors . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . .

179 179 179 182 184 184 185 186 187 192 195 199 199 200 201 204 205 206 208 209 210 211 213 214 215 216 217 219 219

8

Transport . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . 8.2 Conductivity . . . . . . . . . . . . . . . . . . . . . . . 8.3 Low-Field Transport . . . . . . . . . . . . . . . . . 8.3.1 Mobility . . . . . . . . . . . . . . . . . . . 8.3.2 Microscopic Scattering Processes 8.3.3 Ionized Impurity Scattering . . . . . 8.3.4 Deformation Potential Scattering . 8.3.5 Piezoelectric Potential Scattering . 8.3.6 Polar Optical Scattering . . . . . . . 8.3.7 Dislocation Scattering . . . . . . . . . 8.3.8 Grain Boundary Scattering . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

223 223 224 225 226 227 227 229 230 230 230 231

Contents

8.3.9 Alloy Scattering . . . . . . . . . . . . . 8.3.10 Dipole Scattering . . . . . . . . . . . . 8.3.11 Temperature Dependence . . . . . . 8.3.12 Doping Dependence . . . . . . . . . . 8.3.13 Superconductivity . . . . . . . . . . . . 8.3.14 Piezoresistivity . . . . . . . . . . . . . . High-Field Transport . . . . . . . . . . . . . . . . . 8.4.1 Drift-Saturation Velocity . . . . . . . 8.4.2 Negative Differential Resistivity . 8.4.3 Velocity Overshoot . . . . . . . . . . . 8.4.4 Impact Ionization . . . . . . . . . . . . High-Frequency Transport . . . . . . . . . . . . . Impurity Band Transport . . . . . . . . . . . . . . Polarons . . . . . . . . . . . . . . . . . . . . . . . . . . 8.7.1 Large Polarons . . . . . . . . . . . . . . 8.7.2 Small Polarons . . . . . . . . . . . . . . Hopping Transport . . . . . . . . . . . . . . . . . . Transport in Amorphous Semiconductors . . Ionic Transport . . . . . . . . . . . . . . . . . . . . . Diffusion . . . . . . . . . . . . . . . . . . . . . . . . . Continuity Equation . . . . . . . . . . . . . . . . . Heat Conduction . . . . . . . . . . . . . . . . . . . . Coupled Heat and Charge Transport . . . . . 8.14.1 Thermopower and Seebeck Effect 8.14.2 Peltier Effect . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

231 232 232 233 235 235 236 237 237 238 239 241 243 243 243 244 245 247 248 248 250 251 251 252 254

Optical Properties . . . . . . . . . . . . . . . . . . . . . . . . 9.1 Spectral Regions and Overview . . . . . . . . . 9.2 Complex Dielectric Function . . . . . . . . . . . 9.3 Reﬂection and Diffraction . . . . . . . . . . . . . 9.4 Absorption . . . . . . . . . . . . . . . . . . . . . . . . 9.5 Dielectric Function due to Optical Phonons 9.6 Electron–Photon Interaction . . . . . . . . . . . . 9.7 Band–Band Transitions . . . . . . . . . . . . . . . 9.7.1 Joint Density of States . . . . . . . . 9.7.2 Direct Transitions . . . . . . . . . . . . 9.7.3 Indirect Transitions . . . . . . . . . . . 9.7.4 Urbach Tail . . . . . . . . . . . . . . . . 9.7.5 Amorphous Semiconductors . . . . 9.7.6 Excitons . . . . . . . . . . . . . . . . . . . 9.7.7 Phonon Broadening . . . . . . . . . . 9.7.8 Exciton Polariton . . . . . . . . . . . . 9.7.9 Bound-Exciton Absorption . . . . . 9.7.10 Biexcitons . . . . . . . . . . . . . . . . . 9.7.11 Trions . . . . . . . . . . . . . . . . . . . . 9.7.12 Band Gap Renormalization . . . . . 9.7.13 Electron–Hole Droplets . . . . . . . . 9.7.14 Two-Photon Absorption . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

257 257 258 260 262 263 265 267 267 268 271 273 274 274 277 279 281 283 283 284 285 286

8.4

8.5 8.6 8.7

8.8 8.9 8.10 8.11 8.12 8.13 8.14

9

xv

xvi

Contents

9.8

9.9

9.10

Impurity Absorption . . . . . . . . . . . . . . . . . . . . . . . 9.8.1 Shallow Levels . . . . . . . . . . . . . . . . . . . . 9.8.2 Deep Levels . . . . . . . . . . . . . . . . . . . . . . Absorption in the Presence of Free Charge Carriers 9.9.1 Absorption Coefﬁcient, Plasma Frequency 9.9.2 Burstein–Moss Shift . . . . . . . . . . . . . . . . 9.9.3 Inter-Valenceband Transitions . . . . . . . . . 9.9.4 Inter-Valley Transitions . . . . . . . . . . . . . 9.9.5 Intra-Band Transitions . . . . . . . . . . . . . . Lattice Absorption . . . . . . . . . . . . . . . . . . . . . . . . 9.10.1 Dielectric Constant . . . . . . . . . . . . . . . . . 9.10.2 Reststrahlenbande . . . . . . . . . . . . . . . . . . 9.10.3 Polaritons . . . . . . . . . . . . . . . . . . . . . . . . 9.10.4 Phonon–Plasmon Coupling . . . . . . . . . . .

10 Recombination . . . . . . . . . . . . . . . . . . . . . . . . 10.1 Introduction . . . . . . . . . . . . . . . . . . . . . 10.2 Band–Band Recombination . . . . . . . . . . 10.2.1 Spontaneous Emission . . . . . . 10.2.2 Absorption . . . . . . . . . . . . . . . 10.2.3 Stimulated Emission . . . . . . . . 10.2.4 Net Recombination Rate . . . . . 10.2.5 Recombination Dynamics . . . . 10.2.6 Lasing . . . . . . . . . . . . . . . . . . 10.3 Exciton Recombination . . . . . . . . . . . . . 10.3.1 Free Excitons . . . . . . . . . . . . . 10.3.2 Bound Excitons . . . . . . . . . . . 10.3.3 Alloy Broadening . . . . . . . . . . 10.4 Phonon Replica . . . . . . . . . . . . . . . . . . 10.5 Self-Absorption . . . . . . . . . . . . . . . . . . 10.6 Donor–Acceptor Pair Transitions . . . . . . 10.7 Inner-Impurity Recombination . . . . . . . . 10.8 Auger Recombination . . . . . . . . . . . . . . 10.9 Band–Impurity Recombination . . . . . . . 10.9.1 Shockley–Read–Hall Kinetics . 10.9.2 Multilevel Traps . . . . . . . . . . . 10.10 ABC Model . . . . . . . . . . . . . . . . . . . . . 10.11 Field Effect . . . . . . . . . . . . . . . . . . . . . 10.11.1 Thermally Activated Emission . 10.11.2 Direct Tunneling . . . . . . . . . . 10.11.3 Assisted Tunneling . . . . . . . . . 10.12 Recombination at Extended Defects . . . . 10.12.1 Surfaces . . . . . . . . . . . . . . . . . 10.12.2 Grain Boundaries . . . . . . . . . . 10.12.3 Dislocations . . . . . . . . . . . . . . 10.13 Excess-Carrier Proﬁles . . . . . . . . . . . . . 10.13.1 Generation at Surface . . . . . . . 10.13.2 Generation in the Bulk . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

287 287 289 291 291 294 295 297 297 298 298 299 300 300

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

303 303 304 304 306 306 306 308 309 309 309 310 315 318 321 321 322 322 325 325 328 328 329 329 329 330 330 330 331 331 332 333 334

Contents

Part II

xvii

Selected Topics . . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

339 339 340 341 341 343 345 345 346 347

12 Heterostructures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2 Heteroepitaxy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.1 Growth Methods . . . . . . . . . . . . . . . . . . . . . 12.2.2 Substrates . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.3 Growth Modes . . . . . . . . . . . . . . . . . . . . . . . 12.2.4 Heterosubstrates . . . . . . . . . . . . . . . . . . . . . . 12.2.5 Patterned Substrates . . . . . . . . . . . . . . . . . . . 12.2.6 Pseudomorphic Structures . . . . . . . . . . . . . . . 12.2.7 Plastic Relaxation . . . . . . . . . . . . . . . . . . . . . 12.2.8 Surfactants . . . . . . . . . . . . . . . . . . . . . . . . . . 12.3 Energy Levels in Heterostructures . . . . . . . . . . . . . . . . 12.3.1 Band Lineup in Heterostructures . . . . . . . . . . 12.3.2 Quantum Wells . . . . . . . . . . . . . . . . . . . . . . 12.3.3 Superlattices . . . . . . . . . . . . . . . . . . . . . . . . . 12.3.4 Heterointerface Between Doped Materials . . . 12.3.5 Heterointerface Between Semiconductors with of Different Topology . . . . . . . . . . . . . . . . . . 12.4 Recombination in Quantum Wells . . . . . . . . . . . . . . . . 12.4.1 Thickness Dependence . . . . . . . . . . . . . . . . . 12.4.2 Broadening Effects . . . . . . . . . . . . . . . . . . . . 12.4.3 Quantum Conﬁned Stark Effect . . . . . . . . . . . 12.5 Isotope Superlattices . . . . . . . . . . . . . . . . . . . . . . . . . . 12.6 Wafer Bonding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

351 351 352 352 352 355 356 359 362 363 363 365 365 368 372 373

11 Surfaces . . . . . . . . . . . . . . . . . . . . . . . . . 11.1 Introduction . . . . . . . . . . . . . . . . . 11.2 Surface Crystallography . . . . . . . . 11.3 Surface Energy . . . . . . . . . . . . . . . 11.4 Surface Reconstruction . . . . . . . . . 11.5 Surface Morphology . . . . . . . . . . . 11.6 Surface Physical Properties . . . . . . 11.6.1 Surface Phonons . . . . . . . 11.6.2 Surface Plasmons . . . . . . 11.6.3 Electronic Surface States .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

13 Two-Dimensional Semiconductors . . . . . . . . . . . . . . . . . 13.1 Graphene and Related Materials . . . . . . . . . . . . . . 13.1.1 Structural Properties . . . . . . . . . . . . . . . . 13.1.2 Band Structures . . . . . . . . . . . . . . . . . . . 13.1.3 Electrical Properties . . . . . . . . . . . . . . . . 13.1.4 Optical Properties . . . . . . . . . . . . . . . . . . 13.2 Two-Dimensional Compound Semiconductors . . . . 13.2.1 Structural Properties . . . . . . . . . . . . . . . . 13.2.2 Band Structures . . . . . . . . . . . . . . . . . . . 13.2.3 Optical Properties and Valley Polarization 13.2.4 Excitons . . . . . . . . . . . . . . . . . . . . . . . . . 13.3 Van-der-Waals Heterostructures . . . . . . . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

Band Structures . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

374 375 375 375 379 380 381

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

. . . . . . . . . . . .

383 383 384 385 387 390 390 391 392 395 396 398

xviii

Contents

14 Nanostructures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.2 Quantum Wires . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.2.1 V-Groove Quantum Wires . . . . . . . . . . . . . . . . . . 14.2.2 Cleaved-Edge Overgrowth Quantum Wires . . . . . . 14.2.3 Nanowhiskers . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.2.4 Nanobelts . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.2.5 Quantization in Two-Dimensional Potential Wells . 14.3 Carbon Nanotubes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.1 Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.2 Band Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.3 Optical Properties . . . . . . . . . . . . . . . . . . . . . . . . . 14.3.4 Other Anorganic Nanotubes . . . . . . . . . . . . . . . . . 14.4 Quantum Dots . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14.4.1 Quantization in Three-Dimensional Potential Wells 14.4.2 Electrical and Transport Properties . . . . . . . . . . . . 14.4.3 Self-Assembled Preparation . . . . . . . . . . . . . . . . . . 14.4.4 Optical Properties . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . .

401 401 401 401 403 404 406 407 408 408 410 411 412 413 413 416 420 425

15 External Fields . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15.1 Electric Fields . . . . . . . . . . . . . . . . . . . . . . . 15.1.1 Bulk Material . . . . . . . . . . . . . . . . . 15.1.2 Quantum Wells . . . . . . . . . . . . . . . 15.2 Magnetic Fields . . . . . . . . . . . . . . . . . . . . . . 15.2.1 Classical Hall Effect . . . . . . . . . . . . 15.2.2 Free-Carrier Absorption . . . . . . . . . 15.2.3 Energy Levels in Bulk Crystals . . . . 15.2.4 Magnetic Field Effect on Impurities . 15.2.5 Magnetic Field Effect on Excitons . . 15.2.6 Energy Levels in a 2DEG . . . . . . . . 15.2.7 Shubnikov-De Haas Oscillations . . . 15.2.8 Quantum Hall Effect . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

. . . . . . . . . . . . .

429 429 429 431 432 432 438 439 440 441 441 442 444

16 Polarized Semiconductors . . . . . . . . . . . . . . . . . . . . . . 16.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . 16.2 Spontaneous Polarization . . . . . . . . . . . . . . . . . . 16.3 Ferroelectricity . . . . . . . . . . . . . . . . . . . . . . . . . 16.3.1 Materials . . . . . . . . . . . . . . . . . . . . . . 16.3.2 Soft Phonon Mode . . . . . . . . . . . . . . . 16.3.3 Phase Transition . . . . . . . . . . . . . . . . . 16.3.4 Domains . . . . . . . . . . . . . . . . . . . . . . 16.3.5 Optical Properties . . . . . . . . . . . . . . . . 16.4 Piezoelectricity . . . . . . . . . . . . . . . . . . . . . . . . . 16.4.1 Piezoelectric Effect . . . . . . . . . . . . . . . 16.4.2 Zincblende Crystals . . . . . . . . . . . . . . 16.4.3 Wurtzite Crystals . . . . . . . . . . . . . . . . 16.4.4 Piezoelectric Effects in Nanostructures .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

451 451 451 453 453 454 455 457 458 459 459 459 460 462

. . . . . . . . . . . . .

17 Magnetic Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 465 17.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 465 17.2 Magnetic Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 465

Contents

17.3 17.4

xix

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

466 470 470 471

18 Organic Semiconductors . . . . . . . . . . . . . . . . . . . . . 18.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . 18.2 Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.2.1 Small Organic Molecules, Polymers 18.2.2 Organic Semiconductor Crystals . . . 18.3 Electronic Structure . . . . . . . . . . . . . . . . . . . . 18.4 Doping . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 18.5 Transport Properties . . . . . . . . . . . . . . . . . . . 18.6 Optical Properties . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

473 473 473 473 474 476 476 478 479

19 Dielectric Structures . . . . . . . . . . . . . . . . . . . . . . . . . . 19.1 Photonic Band Gap Materials . . . . . . . . . . . . . . 19.1.1 Introduction . . . . . . . . . . . . . . . . . . . . 19.1.2 General 1D Scattering Theory . . . . . . . 19.1.3 Transmission of an N-Period Potential . 19.1.4 The Quarter-Wave Stack . . . . . . . . . . . 19.1.5 Formation of a 3D Band Structure . . . . 19.1.6 Disorder . . . . . . . . . . . . . . . . . . . . . . . 19.1.7 Defect Modes . . . . . . . . . . . . . . . . . . . 19.1.8 Topological Photonic Band Structures . 19.1.9 Coupling to an Electronic Resonance . . 19.1.10 Hyperbolic Optical Metamaterials . . . . 19.2 Microscopic Resonators . . . . . . . . . . . . . . . . . . 19.2.1 Microdiscs . . . . . . . . . . . . . . . . . . . . . 19.2.2 Purcell Effect . . . . . . . . . . . . . . . . . . . 19.2.3 Deformed Resonators . . . . . . . . . . . . . 19.2.4 Hexagonal Cavities . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . .

485 485 485 486 487 489 492 494 494 497 499 502 504 504 506 506 508

20 Transparent Conductive Oxide Semiconductors . 20.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . 20.2 Materials . . . . . . . . . . . . . . . . . . . . . . . . . 20.3 Properties . . . . . . . . . . . . . . . . . . . . . . . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

511 511 511 512

21 Diodes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 21.2 Metal-Semiconductor Contacts . . . . . . . . . . . . . . . . . 21.2.1 Band Diagram in Equilibrium . . . . . . . . . . 21.2.2 Space-Charge Region . . . . . . . . . . . . . . . . 21.2.3 Schottky Effect . . . . . . . . . . . . . . . . . . . . . 21.2.4 Capacitance . . . . . . . . . . . . . . . . . . . . . . . 21.2.5 Current-Voltage Characteristic . . . . . . . . . . 21.2.6 Ohmic Contacts . . . . . . . . . . . . . . . . . . . . 21.2.7 Metal Contacts to Organic Semiconductors

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

517 517 518 518 523 526 527 529 540 543

Part III

Diluted Magnetic Semiconductors Spintronics . . . . . . . . . . . . . . . . . 17.4.1 Spin Transistor . . . . . . . 17.4.2 Spin LED . . . . . . . . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

Applications

xx

Contents

21.3

21.4

21.5

Metal-Insulator-Semiconductor Diodes . . . . . . 21.3.1 Band Diagram for Ideal MIS Diode . 21.3.2 Space-Charge Region . . . . . . . . . . . 21.3.3 Capacitance . . . . . . . . . . . . . . . . . . 21.3.4 Nonideal MIS Diode . . . . . . . . . . . Bipolar Diodes . . . . . . . . . . . . . . . . . . . . . . . 21.4.1 Band Diagram . . . . . . . . . . . . . . . . 21.4.2 Space-Charge Region . . . . . . . . . . . 21.4.3 Capacitance . . . . . . . . . . . . . . . . . . 21.4.4 Current-Voltage Characteristics . . . . 21.4.5 Breakdown . . . . . . . . . . . . . . . . . . . 21.4.6 Heterostructure Diodes . . . . . . . . . . 21.4.7 Organic Semiconductor Diodes . . . . Applications and Special Diode Devices . . . . 21.5.1 Rectiﬁcation . . . . . . . . . . . . . . . . . . 21.5.2 Frequency Mixing . . . . . . . . . . . . . 21.5.3 Voltage Regulator . . . . . . . . . . . . . 21.5.4 Zener Diodes . . . . . . . . . . . . . . . . . 21.5.5 Varactors . . . . . . . . . . . . . . . . . . . . 21.5.6 Fast-Recovery Diodes . . . . . . . . . . . 21.5.7 Step-Recovery Diodes . . . . . . . . . . 21.5.8 Pin-Diodes . . . . . . . . . . . . . . . . . . . 21.5.9 Tunneling Diodes . . . . . . . . . . . . . . 21.5.10 Backward Diodes . . . . . . . . . . . . . . 21.5.11 Gunn Diodes . . . . . . . . . . . . . . . . .

22 Light-to-Electricity Conversion . . . . . . . . . . . . . . 22.1 Photocatalysis . . . . . . . . . . . . . . . . . . . . . 22.2 Photoconductors . . . . . . . . . . . . . . . . . . . 22.2.1 Introduction . . . . . . . . . . . . . . . . 22.2.2 Photoconductivity Detectors . . . . 22.2.3 Electrophotography . . . . . . . . . . 22.2.4 QWIPs . . . . . . . . . . . . . . . . . . . . 22.2.5 Blocked Impurity-Band Detectors 22.3 Photodiodes . . . . . . . . . . . . . . . . . . . . . . 22.3.1 Introduction . . . . . . . . . . . . . . . . 22.3.2 Pn Photodiodes . . . . . . . . . . . . . 22.3.3 Pin Photodiodes . . . . . . . . . . . . 22.3.4 Position-Sensing Detector . . . . . . 22.3.5 MSM Photodiodes . . . . . . . . . . . 22.3.6 Avalanche Photodiodes . . . . . . . 22.3.7 Traveling-Wave Photodetectors . . 22.3.8 Charge Coupled Devices . . . . . . 22.3.9 Photodiode Arrays . . . . . . . . . . . 22.4 Solar Cells . . . . . . . . . . . . . . . . . . . . . . . . 22.4.1 Solar Radiation . . . . . . . . . . . . . 22.4.2 Ideal Solar Cells . . . . . . . . . . . . . 22.4.3 Real Solar Cells . . . . . . . . . . . . . 22.4.4 Design Reﬁnements . . . . . . . . . . 22.4.5 Modules . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . .

544 545 548 551 553 553 554 555 559 560 569 573 573 576 576 578 578 580 581 582 583 583 584 587 588

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . .

589 589 591 591 591 593 593 597 599 599 600 602 603 604 609 613 614 618 623 623 624 629 630 630

Contents

xxi

22.4.6 22.4.7

Solar-Cell Types . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 632 Economic Issues . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 635

23 Electricity-to-Light Conversion . . . . . . . . . . . . . . . . . . . 23.1 Radiometric and Photometric Quantities . . . . . . . . 23.1.1 Radiometric Quantities . . . . . . . . . . . . . 23.1.2 Photometric Quantities . . . . . . . . . . . . . 23.2 Scintillators . . . . . . . . . . . . . . . . . . . . . . . . . . . . 23.2.1 CIE Chromaticity Diagram . . . . . . . . . . 23.2.2 Display Applications . . . . . . . . . . . . . . 23.2.3 Radiation Detection . . . . . . . . . . . . . . . 23.2.4 Luminescence Mechanisms . . . . . . . . . 23.3 Light-Emitting Diodes . . . . . . . . . . . . . . . . . . . . 23.3.1 Introduction . . . . . . . . . . . . . . . . . . . . . 23.3.2 Spectral Ranges . . . . . . . . . . . . . . . . . . 23.3.3 Efﬁciencies . . . . . . . . . . . . . . . . . . . . . 23.3.4 Device Design . . . . . . . . . . . . . . . . . . . 23.3.5 White LEDs . . . . . . . . . . . . . . . . . . . . . 23.3.6 Quantum Dot LEDs . . . . . . . . . . . . . . . 23.3.7 Organic LEDs . . . . . . . . . . . . . . . . . . . 23.4 Lasers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 23.4.1 Introduction . . . . . . . . . . . . . . . . . . . . . 23.4.2 Applications . . . . . . . . . . . . . . . . . . . . . 23.4.3 Gain . . . . . . . . . . . . . . . . . . . . . . . . . . 23.4.4 Optical Mode . . . . . . . . . . . . . . . . . . . . 23.4.5 Loss Mechanisms . . . . . . . . . . . . . . . . 23.4.6 Threshold . . . . . . . . . . . . . . . . . . . . . . 23.4.7 Spontaneous Emission Factor . . . . . . . . 23.4.8 Output Power . . . . . . . . . . . . . . . . . . . 23.4.9 Temperature Dependence . . . . . . . . . . . 23.4.10 Mode Spectrum . . . . . . . . . . . . . . . . . . 23.4.11 Longitudinal Single-Mode Lasers . . . . . 23.4.12 Tunability . . . . . . . . . . . . . . . . . . . . . . 23.4.13 Dynamics and Modulation . . . . . . . . . . 23.4.14 Surface-Emitting Lasers . . . . . . . . . . . . 23.4.15 Optically Pumped Semiconductor Lasers 23.4.16 Quantum Cascade Lasers . . . . . . . . . . . 23.4.17 Hot-Hole Lasers . . . . . . . . . . . . . . . . . 23.5 Semiconductor Optical Ampliﬁers . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. .. ..

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

639 639 639 639 641 641 644 644 645 646 646 646 647 648 653 656 657 659 659 660 661 664 669 670 671 672 675 676 677 678 679 684 686 688 688 689

24 Transistors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 24.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . 24.2 Bipolar Transistors . . . . . . . . . . . . . . . . . . . 24.2.1 Carrier Density and Currents . . . . . 24.2.2 Current Ampliﬁcation . . . . . . . . . . 24.2.3 Ebers-Moll Model . . . . . . . . . . . . 24.2.4 Current–Voltage Characteristics . . . 24.2.5 Basic Circuits . . . . . . . . . . . . . . . . 24.2.6 High-Frequency Properties . . . . . . 24.2.7 Heterojunction Bipolar Transistors . 24.2.8 Light-Emitting Transistors . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

691 691 691 693 695 697 699 701 702 702 703

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

xxii

Contents

24.3 24.4

24.5

24.6

Field-Effect Transistors . . . . . . . . . . . . . . . . . . JFET and MESFET . . . . . . . . . . . . . . . . . . . . 24.4.1 General Principle . . . . . . . . . . . . . . . 24.4.2 Static Characteristics . . . . . . . . . . . . . 24.4.3 Normally On and Normally Off FETs 24.4.4 Field-Dependent Mobility . . . . . . . . . 24.4.5 High-Frequency Properties . . . . . . . . MOSFETs . . . . . . . . . . . . . . . . . . . . . . . . . . . 24.5.1 Operation Principle . . . . . . . . . . . . . . 24.5.2 Current–Voltage Characteristics . . . . . 24.5.3 MOSFET Types . . . . . . . . . . . . . . . . 24.5.4 Complementary MOS . . . . . . . . . . . . 24.5.5 Large-Scale Integration . . . . . . . . . . . 24.5.6 Tunneling FETs . . . . . . . . . . . . . . . . 24.5.7 Nonvolatile Memories . . . . . . . . . . . 24.5.8 Heterojunction FETs . . . . . . . . . . . . . Thin-Film Transistors . . . . . . . . . . . . . . . . . . . 24.6.1 Annealing of Amorphous Silicon . . . 24.6.2 TFT Devices . . . . . . . . . . . . . . . . . . 24.6.3 Transistors with 2D Materials . . . . . . 24.6.4 OFETs . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . .

703 706 706 706 709 710 712 712 713 714 718 718 721 727 727 731 733 734 736 737 738

Appendix A: Tensors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 739 Appendix B: Point and Space Groups . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 743 Appendix C: Kramers–Kronig Relations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 747 Appendix D: Oscillator Strength . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 749 Appendix E: Quantum Statistics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 755 Appendix F: Kronig-Penney Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 761 Appendix G: Tight-Binding Model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 765 Appendix H: k p Perturbation Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 773 Appendix I: Effective-Mass Theory. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 777 Appendix J: Boltzmann Transport Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 779 Appendix K: Noise . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 785 References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 793 Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 869

Abbreviations

0D 1D 2D 2DEG 3D AAAS AB ac ACS ADF ADP AFM AHE AIP AM APD APS AR ARPES ASE AVS bc BC bcc BD BEC BGR BIA BJT BZ CAS CCD CD CEO CIE CIGS CIS

Zero-dimensional One-dimensional Two-dimensional Two-dimensional electron gas Three-dimensional American Association for the Advancement of Science Antibonding (position) Alternating current American Chemical Society Annular dark ﬁeld (STEM method) Acoustic deformation potential (scattering) Atomic force microscopy Anomalous Hall effect American Institute of Physics Air mass Antiphase domain, avalanche photodiode American Physical Society Antireflection Angle-resolved photoemission spectroscopy Ampliﬁed spontaneous emission American Vacuum Society (The Science & Technology Society) Body-centered Bond center (position) Body-centered cubic Blu-rayTM disc Bose–Einstein condensation Band gap renormalization Bulk inversion asymmetry Bipolar junction transistor Brillouin zone Calorimetric absorption spectroscopy Charge coupled device Compact disc Cleaved-edge overgrowth Commission Internationale de l’Éclairage Cu(In,Ga)Se2 material CuInSe2 material, CMOS image sensor

xxiii

xxiv

CL CMOS CMY CNL CNT COD CPU CRT CSL CVD cw CZ DAP DBR dc DF DFB DH(S) DLTS DMS DOS DPSS DRAM DVD EA EBL EEPROM EHL EIL EL ELA ELO EMA EML EPR EPROM ESF ESR ETL EXAFS F4 -TCNQ FA fc fcc FeRAM FET FIB FIR FKO FLG

Abbreviations

Cathodoluminescence Complementary metal–oxide–semiconductor Cyan-magenta-yellow (color system) Charge neutrality level Carbon nanotube Catastrophical optical damage Central processing unit Cathode ray tube Coincident site lattice Chemical vapor deposition Continuous wave Czochralski (growth) Donor–acceptor pair Distributed Bragg reflector Direct current Dielectric function Distributed feedback Double heterostructure Deep level transient spectroscopy Diluted magnetic semiconductor Density of states Diode-pumped solid-state (laser) Dynamic random access memory Digital versatile disc Electron afﬁnity Electron blocking layer Electrically erasable programmable read-only memory Electron–hole liquid Electron injection layer Electroluminescence Excimer laser annealing Epitaxial lateral overgrowth Effective mass approximation Emission layer Electron paramagnetic resonance Erasable programmable read-only memory Extrinsic stacking fault Electron spin resonance Electron transport layer Extended X-ray absorption ﬁne structure 2,3,5,6-tetrafluoro-7,7,8,8-tetracyano-quinodimethane Formamidinium, HC(NH2 )2 Face-centered Face-centered cubic Ferroelectric random access memory Field-effect transistor Focused ion beam Far infrared Franz–Keldysh oscillation Few layer graphene

Abbreviations

FPA FQHE FWHM FZ Gb GIZO GLAD GRINSCH GSMBE GST HBL HBT hcp HCSEL HEMT HIGFET hh HIL HJFET HMM HOMO HOPG HR HRTEM HTL HWHM IBM IC IDB IE IEEE IF IOP IPAP IQHE IR ISF ITO JDOS JFET KKR KOH KTP LA LCD LDA LEC LED 1

xxv

Focal plane array Fractional quantum Hall effect Full width at half-maximum Float-zone (growth) Gigabit GaInZnO Glancing-angle deposition Graded-index separate conﬁnement heterostructure Gas-source molecular beam epitaxy Ge2 Sb2 Te5 Hole blocking layer Heterobipolar transistor Hexagonally close packed Horizontal cavity surface-emitting laser High electron mobility transistor Heterojunction insulating gate FET Heavy hole Hole injection layer Heterojunction FET Hyperbolic metamaterial Highest occupied molecular orbital Highly ordered pyrolithic graphite High reflection High-resolution transmission electron microscopy Hole transport layer Half-width at half-maximum International Business Machines Corporation Integrated circuit Inversion domain boundary Ionization energy Institute of Electrical and Electronics Engineers1 Intermediate frequency Institute of Physics Institute of Pure and Applied Physics, Tokyo Integral quantum Hall effect Infrared Intrinsic stacking fault Indium tin oxide Joint density of states Junction ﬁeld-effect transistor Kramers–Kronig relation Potassium hydroxide KTiOPO4 material Longitudinal acoustic (phonon) Liquid crystal display Local density approximation Liquid encapsulated Czochralski (growth) Light-emitting diode

pronounced Eye-triple-E.

xxvi

lh LO LPCVD LPE LPP LST LT LUMO LVM MA MBE MEMS MHEMT MESFET MIGS MILC MIOS MIR MIS MIT ML MLC MMIC MO MOCVD MODFET MOMBE MOPA MOS MOSFET MOVPE MQW MRAM MRS MS MSA MSM MTJ MWNT NDR NEP NIR NMOS NTSC OLED OMC ONO OPSL PA PBG

Abbreviations

Light hole Longitudinal optical (phonon), local oscillator Low-pressure chemical vapor deposition Liquid phase epitaxy Longitudinal phonon plasmon (mode) Lyddane–Sachs–Teller (relation) Low temperature Lowest unoccupied molecular orbital Local vibrational mode Methylammonium, methylammonium Molecular beam epitaxy Micro-electro-mechanical system Metamorphic HEMT Metal–semiconductor ﬁeld-effect transistor Midgap (surface) states Metal-induced lateral crystallization Metal–insulator–oxide–semiconductor Mid-infrared Metal–insulator–semiconductor Massachusetts Institute of Technology Monolayer Multi-level cell Millimeter-wave integrated circuit Master oscillator Metalorganic chemical vapor deposition Modulation-doped ﬁeld-effect transistor Metalorganic molecular beam epitaxy Master oscillator power ampliﬁer Metal–oxide–semiconductor Metal–oxide–semiconductor ﬁeld-effect transistor Metalorganic chemical vapor deposition Multiple quantum well Magnetic random access memory Materials Research Society Metal–semiconductor (diode) Mobility spectral analysis Metal–semiconductor–metal (diode) Magneto-tunneling junction Multi-walled (carbon) nanotube Negative differential resistance Noise equivalent power Near infrared n-channel metal–oxide–semiconductor (transistor) National television standard colors Organic light emitting diode Organic molecular crystals Oxide/nitride/oxide Optically pumped semiconductor laser Power ampliﬁer Photonic band gap

Abbreviations

pc PCM PFM PHEMT PL PLD PLE PMC PMMA PMOS PPC PPLN PV PWM PZT QCL QCSE QD QHE QW QWIP QWR RAM RAS RF RFID RGB RHEED RIE RKKY rms ROM RRAM RSC SAGB SAM sc SCH SCLC SdH SEL SEM SET SGDBR SHG si SIA SIA SIMS SL

xxvii

Primitive cubic Phase change memory Piezoresponse force microscopy Pseudomorphic HEMT Photoluminescence Pulsed laser deposition Photoluminescence excitation (spectroscopy) Programmable metallization cell Poly-methyl methacrylate p-channel metal–oxide–semiconductor (transistor) Persistent photoconductivity Perodically poled lithium niobate Photovoltaic(s) Pulsewidth modulation PbTix Zr1x O3 material Quantum cascade laser Quantum conﬁned Stark effect Quantum dot Quantum Hall effect Quantum well Quantum-well intersubband photodetector Quantum wire Random access memory Reflection anisotropy spectroscopy Radio frequency Radio frequency identiﬁcation Red-green-blue (color system) Reflection high-energy electron diffraction Reactive ion etching Ruderman–Kittel–Kasuya–Yoshida (interaction) Root mean square Read-only memory Resistance random access memory The Royal Society of Chemistry Small-angle grain boundary Separate absorption and ampliﬁcation (structure) Simple cubic Separate conﬁnement heterostructure Space-charge limited current Shubnikov-de Haas (oscillation) Surface-emitting laser Scanning electron microscopy Single-electron transistor, single electron tunneling Sampled grating distributed Bragg reflector Second-harmonic generation Semi-insulating Semiconductor Industry Association Structural inversion asymmetry Secondary ion mass spectrometry Superlattice

xxviii

SLC SLG SNR s-o SOA SOFC SPD SPICE SPIE SPP SPS sRGB SRH SSH SSR STEM STEM-ADF STM SWNT TA TAS TCO TE TED TEGFET TEM TES TF TFET TFT TM TMAH TMDC TMR TO TOD TPA TSO UHV UV VCA VCO VCSEL VFF VGF VIS VLSI WGM WKB WS

Abbreviations

Single-level cell Single layer graphene Signal-to-noise ratio Spin-orbit (or split-off) Semiconductor optical ampliﬁer Solid-oxide fuel cells Spectral power distribution Simulation Program with Integrated Circuit Emphasis Society of Photographic Instrumentation Engineers Surface plasmon polariton Short-period superlattice Standard RGB Shockley–Read–Hall (kinetics) Su–Schrieffer–Heeger (model) Side-mode suppression ratio Scanning transmission electron microscopy Scanning transmission electron microscopy with annular dark ﬁeld imaging Scanning tunneling microscopy Single-walled (carbon) nanotube Transverse acoustic (phonon) Thermal admittance spectroscopy Transparent conductive oxide transverse electric (polarization) transferred electron device Two-dimensional electron gas ﬁeld-effect transistor Transmission electron microscopy Two-electron satellite Thermionic ﬁeld emission Transparent FET, tunneling FET Thin ﬁlm transistor Transverse magnetic (polarization) Tetramethyl-ammonium-hydroxide Transition metal dichalcogenide Tunnel-magnetoresistance Transverse optical (phonon) Turn-on delay (time) Two-photon absorption Transparent semiconducting oxide Ultrahigh vacuum Ultraviolet Virtual crystal approximation Voltage-controlled oscillator Vertical-cavity surface-emitting laser Valence force ﬁeld Vertical gradient freeze (growth) Visible Very large scale integration Whispering gallery mode Wentzel–Kramer–Brillouin (approximation or method) Wigner–Seitz (cell)

Abbreviations

X XPS XSTM XX YSZ ZnPc

xxix

Exciton X-ray photoelectron spectroscopy Cross-sectional STM Biexciton Yttria-stabilized zirconia (ZrO2 ) Zinc-phthalocyanine

Symbols

a aðxÞ am an ap aT b c C c1 , c2 , c3 dij D0 ðxÞ 0 i r s S ij g gd gext gint gw h HD HB j k kp l l0 lh lH ln

Madelung constant, disorder parameter, linewidth enhancement factor absorption coefﬁcient mirror loss electron ionization coefﬁcient hole ionization coefﬁcient base transport factor used as abbreviation for e=ðkB TÞ, spontaneous emission coefﬁcient, two-photon absorption coefﬁcient broadening parameter, Berry phase, Grüneisen parameter, emitter efﬁciency, tight-binding nearest-neighbor coupling parameter broadening parameter Luttinger parameters Kronecker symbol spin-orbit splitting dielectric function permittivity of vacuum dielectric constant of insulator relative dielectric function dielectric function of semiconductor (¼ r 0 ) gain compression coefﬁcient components of strain tensor quantum efﬁciency differential quantum efﬁciency external quantum efﬁciency internal quantum efﬁciency wall-plug efﬁciency angle Debye temperature typical phonon energy parameter imaginary part of index of refraction, heat conductivity wavelength plasma wavelength mobility magnetic susceptibility of vacuum hole mobility Hall mobility electron mobility xxxi

xxxii

m P pij q qij qP r Rn rij rn rp rP s sn snr sp sr HD / U0 v vex vsc vðrÞ w WðrÞ x xLO xp xTO X a a A A A, A A a0 b b B B, B c C Cn , Cp C ij , C ijkl d di D D, D

Symbols

frequency, ﬁlling factor (QHE), winding number Peltier coefﬁcient components of piezoresistivity tensor mass density, charge density, resistivity components of resistivity tensor polarization charge density (per volume) standard deviation, conductivity, stress, effective mass ratio grain boundary type components of stress tensor, conductivity tensor electron capture cross section hole capture cross section polarization charge density (per area) lifetime, time constant electron (minority carrier) lifetime non-radiative lifetime hole (minority carrier) lifetime radiative lifetime Debye temperature phase photon flux electron afﬁnity, electric susceptibility light extraction efﬁciency electron afﬁnity (of semiconductor) envelope wavefunction angle wavefunction angular frequency longitudinal optical phonon frequency plasma frequency transverse optical phonon frequency interaction parameter hydrostatic deformation potential, lattice constant accelaration atomic mass (A ¼ 12 for 12 C) area, band-impurity recombination coefﬁcient vector potential Richardson constant (cubic) lattice constant bowing parameter, deformation potential Burger's vector bimolecular recombination coefﬁcient, bandwidth magnetic induction ﬁeld velocity of light in vacuum, lattice constant (along c-axis) capacitance, spring constant, Auger recombination coefﬁcient Auger recombination coefﬁcient elastic constants distance, shear deformation potential insulator thickness density of states, diffusion coefﬁcient electric displacement ﬁeld

Symbols

D De ðEÞ Dh ðEÞ Dn Dp e ei E E, E EA E bA EC E xc ED E bD EF Eg Ei Em EP EV E vac EX E bX E XX f F F, F FðMÞ FB fe fi fh Fn Fp FP g G G, G gm Gth h H H, H h i I ID Is I sc

xxxiii

detectivity electron density of states hole density of states electron diffusion coefﬁcient hole diffusion coefﬁcient elementary charge strain components (Voigt notation) energy electric ﬁeld energy of acceptor level acceptor ionization energy energy of conduction-band edge exchange interaction energy energy of donor level, Dirac energy (in graphene) donor ionization energy Fermi energy band gap intrinsic Fermi level maximum electric ﬁeld energy parameter energy of valence-band edge energy of vacuum level exciton energy exciton binding energy biexciton energy oscillator strength free energy force excess noise factor Schottky barrier height Fermi–Dirac distribution function (for electrons) ionicity Fermi–Dirac distribution function for holes (¼ 1 f e ) electron quasi-Fermi energy hole quasi-Fermi energy Purcell factor degeneracy, g-factor, gain free enthalpy, generation rate reciprocal lattice vector transconductance thermal generation rate Planck constant enthalpy, Hamiltonian magnetic ﬁeld h/(2p) imaginary number current, light intensity drain current saturation current short circuit current

xxxiv

I thr j; j j js jthr k k kB kF l L L LD Lz m m0 m mij mc M M, M me mh mj ml mr mt n n NðEÞ n NA Nc NC ND ni nif nr ns Nt ntr nthr NV p p, p P P, P pcv pi q

Symbols

threshold current current density total orbital momentum saturation current density threshold current density wavenumber, Boltzmann constant wavevector Boltzmann constant Fermi wavevector angular orbital momentum length of line element line vector (of dislocation) diffusion length quantum-well thickness mass free electron mass effective mass effective mass tensor cyclotron mass mass, multiplication factor magnetization effective electron mass effective hole mass magnetic quantum number longitudinal mass reduced mass transverse mass electron concentration (in conduction band), ideality factor normal vector number of states complex index of refraction (¼ nr þ ij) acceptor concentration critical doping concentration conduction-band edge density of states donor concentration intrinsic electron concentration ideality factor due to image force effect index of refraction (real part) sheet electron density trap concentration transparency electron concentration threshold electron concentration valence-band edge density of states pressure, free hole density momentum power electric polarization momentum matrix element intrinsic hole concentration charge

Symbols

q, q Q r r R Rk R rH RH s S Sij , Sijkl t tox T u U unk v, v V VðkÞ Va VA V bi vg VG V oc VP vs V SD vth w wB Wm X Y Z

xxxv

heat flow charge, quality factor, impurity-bound exciton localization energy radius spatial coordinate resistance, radius, recombination rate responsivity vector of direct lattice Hall factor Hall coefﬁcient spin entropy, Seebeck coefﬁcient, total spin, surface index, surface recombination velocity stiffness coefﬁcients time (gate) oxide thickness temperature displacement, cell-internal parameter energy Bloch function velocity volume, voltage, potential (standardized) sensitivity of human eye unit-cell volume Early voltage built-in voltage group velocity gate voltage open circuit voltage pinch-off voltage velocity of sound, drift-saturation velocity source-drain voltage thermal velocity depletion-layer width, width base width (bipolar transistor) (metal) work function electronegativity Young's module, CIE brightness parameter partition sum, atomic order number

Physical Constants

Constant

Symbol

Numerical value (new SI units) Unit

Speed of light in vacuum Permeability of vacuum Permittivity of vacuum Elementary charge Electron mass Planck constant

c0 μ0

2.99792458 × 108 (exact) 4π × 10−7 8.854187817 × 10−12 1.602176634 × 10−19 (exact) 9.1093837 × 10−31 6.62607015 × 10−34 (exact) 1.05457182 × 10−34 6.58211957 × 10−16 1.380649 × 10−23 (exact) 8.6173333 × 10−5 25812.8075 13.605693123 5.29177211 × 10−11 6.02214076 × 1023 (exact)

0

(μ0 c02 )−1

e me h h/(2π )

Boltzmann constant

kB

von-Klitzing constant Rydberg constant Bohr radius Avogadro constant

RK aB NA

h/e2

m s−1 N A−2 F m−1 C kg Js Js eV s J K−1 meV K−1 eV m mol−1

xxxvii

Chapter 1

Introduction

The proper conduct of science lies in the pursuit of Nature’s puzzles, wherever they may lead. J.M. Bishop [2]

Abstract Important dates and events in the history of semiconductors are chronologically listed, from the early days (Volta, Seebeck and Faraday) to the latest achievements like the blue and white LED. Many known and not so well known scientists are mentioned. Also a list of semiconductor related Nobel prizes and their winners is given.

The historic development of semiconductor physics and technology began in the second half of the 19th century. Interesting discussions of the history of the physics and chemistry of semiconductors can be found in [3–5]. The development of crystal growth is covered in [6]. The history of semiconductor industry can be followed in [7, 8]. In [9] 141 pioneering papers on semiconductor devices are compiled. In 1947, the commercial realization of the transistor was the impetus to a fast-paced development that created the electronics and photonics industries. Products founded on the basis of semiconductor devices such as computers (CPUs, memories), optical-storage media (lasers for CD, DVD), communication infrastructure (lasers and photodetectors for optical-fiber technology, high frequency electronics for mobile communication), displays (thin film transistors, LEDs), projection (laser diodes) and general lighting (LEDs) are commonplace. Thus, fundamental research on semiconductors and semiconductor physics and its offspring in the form of devices has contributed largely to the development of modern civilization and culture.

1.1 Timetable and Key Achievements In this section important milestones in semiconductor physics and technology are listed. 1782 A. Volta—coins the phrase ‘semicoibente’ (semi-insulating) which was translated then into English as ‘semiconducting’ [10].

© Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_1

1

2

1 Introduction

Fig. 1.1 Current through a silver–CuFeS2 –silver structure as a function of the current through the metal only, 1874. Data points are for different applied voltages. Experimental data from [24]

1821 T.J. Seebeck—discovery of thermopower (electrical phenomena upon temperature difference) in metals and PbS, FeS2 , CuFeS2 [11, 12]. 1833 M. Faraday—discovery of the temperature dependence of the conductivity of Ag2 S (sulphuret of silver, negative dR/dT ) [13]. 1839 A.E. Becquerel1 —photoelectric effect (production of a photocurrent when electrodes covered by copper or silver halides salts (in an electrolyte) were illuminated by solar light) [14–17]. 1834 J. Peltier—discovery of the Peltier effect (cooling by current) [18]. 1873 W. Smith—discovery of photoconductivity in selenium [19, 20]. Early work on photoconductivity in Se is reviewed in [21, 22]. 1874 F. Braun2 —discovery of rectification in metal–sulfide semiconductor contacts [24], e.g. for CuFeS2 and PbS. The current through a metal–semiconductor contact is nonlinear (as compared to that through a metal, Fig. 1.1), i.e. a deviation from Ohm’s law. Braun’s structure is similar to a MSM diode. 1876 W.G. Adams and R.E. Day—discovery of the photovoltaic effect in selenium [25]. W. Siemens—large response from selenium photoconductor [26], made by winding two thin platinum wires to the surface of a sheet of mica, and then covering the surface with a thin film of molten selenium. Resistance ratio between dark and illuminated by sunlight was larger than ten [26] and measured to 14.8 in [27]. 1879 E.H. Hall—measurement of the transverse potential difference in a thin gold leaf on glass [28, 29]. Experiments were continued by his mentor H.A. Rowland [30]. A detailed account of the discovery of the Hall efect is given in [31, 32]. 1 This is Edmond Becquerel; his son Henri Becquerel received the Nobel Prize in Physics for the discovery of radioactivity. 2 F. Braun made his discoveries on metal–semiconductor contacts in Leipzig while a teacher at the Thomasschule zu Leipzig [23]. He conducted his famous work on vacuum tubes later as a professor in Strasbourg, France.

1.1 Timetable and Key Achievements

3

Fig. 1.2 Circuit diagram for a radio receiver with a point-contact diode (TJ). Adapted from [34]

1883 Ch. Fritts—first solar cell, based on an gold/selenium rectifier [27]. The efficiency was below 1%. 1901 J.C. Bose—point contact detector for electromagnetic waves based on galena (PbS) [33]. At the time, the term semiconductor was not introduced yet and Bose speaks about ‘substances of a certain class (...) presenting a decreasing resistance to the passage of the electric current with an increasing impressed electromotive force’. 1906 G.W. Pickard—rectifier based on point contact (cat’s whisker) diode on silicon [34–36]. Erroneously, the rectifying effect was attributed to a thermal effect, however, the drawing of the ‘thermo-junction’ (TJ in Fig. 1.2) developed into the circuit symbol for a diode (cmp. Fig. 21.63a). 1907 H.J. Round—discovery of electroluminescence investigating yellow and blue light emission from SiC [37]. K. Bädeker—preparation of metal (e.g. Cd, Cu) oxides and sulfides and also CuI from metal layers using a vapor phase transport method [38]3 . CuI is reported transparent (∼ 200 nm thick films) with a specific resistivity of ρ = 4.5 × 10−2 cm, the first transparent conductor.4 Also CdO (films of thickness 100–200 nm) is reported to be highly conductive, ρ = 1.2 × 10−3 cm, and orange-yellow in color, the first reported TCO (transparent conductive oxide). 1909 K. Bädeker—discovery of doping. Controlled variation of the conductivity of CuI by dipping into iodine solutions (e.g. in chloroform) of different concentrations [41]. 1910 W.H. Eccles—negative differential resistance of contacts with galena (PbS), construction of crystal oscillators5 [45].

3 This work was conducted as Habilitation in the Physics Institute of Universität Leipzig. Bädeker became subsequently professor in Jena and fell in WW I. His scientific contribution to semiconductor physics is discussed in [39, 40] 4 CuI is actually a p-type transparent conductor; at that time the positive sign of the Hall effect [41, 42] could not be interpreted as hole conduction yet. 5 Historical remarks on Eccles’ contributions to radio technology can be found in [43, 44]

4

1 Introduction

Fig. 1.3 Laue images of ’regular’ (cubic) ZnS along three major crystallographic directions, directly visualizing their 4-, 3- and 2-fold symmetry. Adapted from [48] Fig. 1.4 Sketch of a field-effect transistor, 1926. From [53]

1911 The term ‘Halbleiter’ (semiconductor) is introduced for the first time by J. Weiss [46] and J. Königsberger and J. Weiss [47]. Königsberger preferred the term ‘Variabler Leiter’ (variable conductor). 1912 M. von Laue—X-ray diffraction of bulk crystals including ZnS (Fig. 1.3) [48, 49]. 1925 J.E. Lilienfeld6 —proposal of the metal-semiconductor field-effect transistor (MESFET) [53], with suggested copper sulfide thin film channel and aluminum gate.7 (Fig. 1.4). Lilienfeld was also awarded patents for a depletion mode MOSFET [55] with proposed copper sulfide, copper oxide or lead oxide channel and current amplification with nppn- and pnnp-transistors [56]. Due to the lack of other publications of Lilienfeld on transistors, it is under discussion whether Lilienfeld just patented ideas or also build working devices with mounting evidence for the latter [51, 54, 57]. 1927 A. Schleede, H. Buggisch—synthesis of pure, stoichiometric PbS, influence of sulphur excess and impurities [58]. A. Schleede, E. Körner—activation of luminescence of ZnS [59, 60].

6 After obtaining his PhD in 1905 from the Friedrich-Wilhelms-Universität Berlin, Julius Edgar Lilienfeld joined the Physics Department of Universität Leipzig and worked on gas liquefaction and with Lord Zeppelin on hydrogen-filled blimps. In 1910 he became professor at the Universität Leipzig where he mainly researched on X-rays and vacuum tubes [50]. To the surprise of his colleagues he left in 1926 to join a US industrial laboratory [51, 52]. 7 In [51] it is suggested that the device works as a npn transistor, in [54] it is suggested to be a JFET.

1.1 Timetable and Key Achievements

(a)

5

(b)

Fig. 1.5 a I –V characteristic of SiC/steel wire light emitting diode. The dotted curve is the flipped curve for negative voltage (3rd quadrant). b Recording of current modulated (at 500 Hz) LED on moving photographic plate. Adapted from [65] Fig. 1.6 First band structure calculation from Peierls (ξ = k a). Adapted from [69]

1928 F. Bloch—quantum mechanics of electrons in a crystal lattice, ‘Bloch functions’ [61]. O.V. Losev—description of the light emitting diode8 (SiC) [65]; light emission was observed in forward direction and close to breakdown (Fig. 1.5a). Also current modulation of LED light output was reported (Fig. 1.5b) [65]. 1929 R. Peierls—explanation of positive (anomalous) Hall effect with unoccupied electron states [66, 67]. 1930 R. Peierls—first calculation of a band structure and band gap9 (Fig. 1.6) [69]. 1931 W. Heisenberg—theory of hole (‘Löcher’) states [70]. R. de L. Kronig and W.G. Penney—properties of periodic potentials in solids [71]. 8 The

historic role of Losev regarding the invention of the LED and oscillators is discussed in [62–64]. performed this work at suggestion of W. Pauli at ETH Zürich. The mathematical problem of Schrödinger’s equation with a sinusoidal potential had been already treated by M.J.O Strutt in 1928 [68] 9 Peierls

6

1 Introduction

(a)

(b)

Fig. 1.7 a Optical image of directionally solidified silicon. The lower part contains predominantly boron, the upper part contains predominantly phosphorous. First the growth is porous and subsequently columnar. Adapted from [90]. b Spectral response of silicon pn-junction photoelement, 1940. The inset depicts schematically a Si slab with built-in pn-junction formed during directed solidification as shown in panel (a). The arrow denotes the direction of solidification (cmp. Fig. 4.6). Adapted from [89]

A.H. Wilson10 —development of band-structure theory [74, 75]. 1933 C. Wagner—excess (‘Elektronenüberschuss-Leitung’, n-type) and defect (‘Elektronen-Defektleitung’, p-type) conduction [76–79]. Anion deficiency in ZnO causes conducting behavior [80]. 1934 C. Zener—Zener tunneling [81]. 1936 J. Frenkel—description of excitons [82]. 1938 B. Davydov—theoretical prediction of rectification at pn-junction [83] and in Cu2 O [84]. W. Schottky—theory of the boundary layer in metal–semiconductor contacts [85], being the basis for Schottky contacts and field-effect transistors. N.F. Mott—metal–semiconductor rectifier theory [86, 87]. R. Hilsch and R.W. Pohl—three-electrode crystal (KBr) [88]. 1940 R.S. Ohl—Silicon-based photoeffect (solar cell, Fig. 1.7) [89] from a pn-junction formed within a slab of polycrystalline Si fabricated with directed solidification due to different distribution coefficients of p- and n-dopants (boron and phosphorus, cmp. Fig. 4.6b) (J. Scaff and H. Theurer) [90, 91].

10 Wilson was theoretical physicist in Cambridge, who spent a sabbatical with Heisenberg in Leipzig and applied the brand new field of quantum mechanics to issues of electrical conduction, first in metals and then in semiconductors. When he returned to Cambridge, Wilson urged that attention be paid to germanium but, as he expressed it long afterward, ’the silence was deafening’ in response. He was told that devoting attention to semiconductors, those messy entities, was likely to blight his career among physicists. He ignored these warnings and in 1939 brought out his famous book ’Semiconductors and Metals’ [72] which explained semiconductor properties, including the much-doubted phenomenon of intrinsic semiconductivity, in terms of electronic energy bands. His academic career seems indeed to have been blighted, because despite his great intellectual distinction, he was not promoted in Cambridge (he remained an assistant professor year after year) [73]. Compare the remark of W. Pauli (p. 179)

1.1 Timetable and Key Achievements

7

Fig. 1.8 Characteristics of a silicon rectifier, 1941. Adapted from [92]

1941 R.S. Ohl—Silicon rectifier with point contact [92, 93] (Fig. 1.8), building on work from G.W. Pickard (1906) and using metallurgically refined and intentionally doped silicon (J. Scaff and H. Theurer) [90]. 1942 K. Clusius, E. Holz and H. Welker—rectification in germanium [94]. 1945 H. Welker—patents for JFET and MESFET [95]. 1947 W. Shockley, J. Bardeen and W. Brattain fabricate the first transistor in the AT&T Bell Laboratories, Holmdel, NJ in an effort to improve hearing aids [96].11 Strictly speaking the structure was a pointcontact transistor. A 50-µm wide slit was cut with a razor blade into gold foil over a plastic (insulating) triangle and pressed with a spring on n-type germanium (Fig. 1.9a) [97]. The surface region of the germanium is p-type due to surface states and represents an inversion layer. The two gold contacts form emitter and collector, the large-area back contact of the germanium the base contact [98]. For the first time, amplification was observed [99]. Later models use two close point contacts made from wires with their tips cut into wedge shape (Fig. 1.9b) [98].12 More details about the history and development of the semiconductor transistor can be found in [100], written on the occasion of the 50th anniversary of its invention. 1948 W. Shockley—invention of the bipolar (junction) transistor [101]. 1952 H. Welker—fabrication of III–V compound semiconductors13 [104–107]. 11 Subsequently, AT&T, under pressure from the US Justice Department’s antitrust division, licensed the transistor for $25,000. This action initiated the rise of companies like Texas Instruments, Sony and Fairchild. 12 The setup of Fig. 1.9b represents a common base circuit. In a modern bipolar transistor, current amplification in this case is close to unity (Sect. 24.2.2). In the 1948 germanium transistor, the reversely biased collector contact is influenced by the emitter current such that current amplification ∂ IC /∂ IE for constant UC was up to 2–3. Due to the collector voltage being much larger than the emitter voltage, a power gain of ∼ 125 was reported [98]. 13 An early concept for III–V semiconductors was developed in [102, 103].

8

1 Introduction

(a)

(b)

Fig. 1.9 a The first transistor, 1947 (length of side of wedge: 32 mm). b Cutaway model of a 1948 point contact transistor (‘Type A’) based on n-type bulk Ge (n = 5×1014 cm−3 ) and common base circuit diagram. The surface region (∼ 100 nm depth) of the Ge is p-type due to surface states and represents an inversion layer. The two wires are made from phosphor bronze. Adapted from [98]

W. Shockley—description of today’s version of the (J)FET [108]. 1953 G.C. Dacey and I.M. Ross—first realization of a JFET [109]. D.M. Chapin, C.S. Fuller and G.L. Pearson—invention of the silicon solar cell at Bell Laboratories [110]. A single 2 cm2 photovoltaic cell from Si, Si:As with an ultrathin layer of Si:B, with about 6% efficiency generated 5 mW of electrical power.14 Previously existing solar cells based on selenium had very low efficiency (< 0.5%). 1958 J.S. Kilby made the first integrated circuit at Texas Instruments. The simple 1.3 MHz RC-oscillator consisted of one transistor, three resistors and a capacitor on a 11 × 1.7 mm2 Ge platelet (Fig. 1.10a). J.S. Kilby filed in 1959 for a US patent for miniaturized electronic circuits [111]. At practically the same time R.N. Noyce from Fairchild Semiconductors, the predecessor of INTEL, invented the integrated circuit on silicon using planar technology [112]. A detailed and (very) critical view on the invention of the integrated circuit can be found in [113]. Figure 1.10b shows a flip-flop with four bipolar transistors and five resistors. Initially, the invention of the integrated circuit15 met scepticism because of concerns regarding yield and the achievable quality of the transistors and the other components (such as resistors and capacitors).

14 A solar cell with 1 W power cost $300 in 1956 ($3 in 2004). Initially, ‘solar batteries’ were only used for toys and were looking for an application. H. Ziegler proposed the use in satellites in the ‘space race’ of the late 1950s. 15 The two patents led to a decade-long legal battle between Fairchild Semiconductors and Texas Instruments. Eventually, the US Court of Customs and Patent Appeals upheld R.N. Noyce’s claims on interconnection techniques but gave J.S. Kilby and Texas Instruments credit for building the first working integrated circuit.

1.1 Timetable and Key Achievements

(a)

9

(b)

Fig. 1.10 a The first integrated circuit, 1958 (germanium, 11 × 1.7 mm2 ). b The first planar integrated circuit, 1959 (silicon, diameter: 1.5 mm)

Fig. 1.11 (a) Optical image of planar pnp silicon transistor (2N1613 [120]), 1959. The contacts are Al surfaces (not bonded). (b) Housing of such transistor cut open

1959 J. Hoerni16 and R. Noyce—first realization of a planar transistor (in silicon) (Fig. 1.11) [115–119]. 1960 D. Kahng and M.M. Atalla—first realization of a MOSFET [121, 122]. 1962 The first semiconductor laser on GaAs basis at 77 K at GE [123, 124] (Fig. 1.12) and at IBM [125] and MIT [126]. First visible laser diode [127].17 1963 Proposal of a double heterostructure laser (DH laser) by Zh.I. Alferov [130, 131] and H. Kroemer [132, 133]. J.B. Gunn—discovery of the Gunn effect, the spontaneous microwave oscillations in GaAs and InP at sufficiently large applied electric field (due to negative differential resistance) [134]. 16 The Swiss born Jean Hoerni also contributed $12 000 for the building of the first school in the Karakoram Mountain area in Pakistan and has continued to build schools in Pakistan and Afghanistan as described in [114]. 17 Remarks on the discovery and further development of the laser diode can be found in [128, 129].

10

1 Introduction

Fig. 1.12 Schematics of GaAs-based laser diode. The active layer is highlighted in red. Adapted from [124]

1966 C.A. Mead—proposal of the MESFET (‘Schottky Barrier Gate FET’) [135]. 1967 Zh.I. Alferov—report of the first DH laser on the basis of Ga(As,P) at 77 K [136, 137]. W.W. Hooper and W.I. Lehrer—first realization of a MESFET [138]. 1968 DH laser on the basis of GaAs/(Al,Ga)As at room temperature, independently developed by Zh.I. Alferov [139] and I. Hayashi [140]. GaP:N LEDs with yellow-green emission (550 nm) and 0.3% efficiency [141]. 1968 SiC blue LED with efficiency of 0.005% [142]. 1970 W.S. Boyle and G.E. Smith—invention of the charge coupled device (CCD) [143, 144]. 1971 R.F. Kazarinov and R.A. Suris—proposal of the quantum cascade laser [145]. 1975 R.S. Pengelly and J.A. Turner—first monolithic microwave integrated circuit (MMIC) (Fig. 1.13) [146] 1992 S. Nakamura—growth of high-quality group-III–nitride thin films [147], blue nitride heterostructure LED with efficiency exceeding 10% (1995) [148] (Fig. 1.14a). Later the white LED was built by combining a blue LED with yellow phosphors (Fig. 1.14b, c).

1.1 Timetable and Key Achievements

11

Fig. 1.13 Equivalent circuit and optical image of first monolithic microwave integrated circuit (exhibiting gain (4.5 ± 0.9 dB) in the frequency range 7.0–11.7 GHz). Adapted from [146]

Fig. 1.14 a Blue LED (standard housing). 50 W, 4000 lm, b warm white and c cold white LED (45 × 45 mm2 )

1994 J. Faist and F. Capasso—quantum cascade laser [149]. N. Kirstaedter, N.N. Ledentsov, Zh.I. Alferov and D. Bimberg—quantum dot laser [150]. 2004 H. Hosono and T. Kamiya—thin film transistor (TFT) from amorphous oxide semiconductor [151].

12

1 Introduction

1.2 Nobel Prize Winners Several Nobel Prizes18 have been awarded for discoveries and inventions in the field of semiconductor physics (Fig. 1.15). 1909 Karl Ferdinand Braun ‘in recognition of his contributions to the development of wireless telegraphy’ 1914 Max von Laue ‘for his discovery of the diffraction of X-rays by crystals’ 1915 Sir William Henry Bragg William Lawrence Bragg ‘for their services in the analysis of crystal structure by means of X-rays’ 1946 Percy Williams Bridgman ‘for the invention of an apparatus to produce extremely high pressures, and for the discoveries he made therewith in the field of high pressure physics’ 1953 William Bradford Shockley John Bardeen Walter Houser Brattain ‘for their researches on semiconductors and their discovery of the transistor effect’ 1973 Leo Esaki ‘for his experimental discoveries regarding tunneling phenomena in semiconductors’ 1985 Klaus von Klitzing ‘for the discovery of the quantized Hall effect’ 1998 Robert B. Laughlin Horst L. Störmer Daniel C. Tsui ‘for their discovery of a new form of quantum fluid with fractionally charged excitations’ 2000 Zhores I. Alferov Herbert Kroemer ‘for developing semiconductor heterostructures used in high-speed and optoelectronics’ Jack St. Clair Kilby ‘for his part in the invention of the integrated circuit’ 2009 Willard S. Boyle George E. Smith ‘for the invention of an imaging semiconductor circuit—the CCD sensor’

18 www.nobel.se

1.2 Nobel Prize Winners

Fig. 1.15 Winners of Nobel Prize in Physics and year of award with great importance for semiconductor physics

13

14

1 Introduction

Fig. 1.15 (continued)

2010 Andre Geim Konstantin Novoselov ‘for groundbreaking experiments regarding the two-dimensional material graphene’ 2014 Isamu Akasaki Hiroshi Amano Shuji Nakamura ‘for the invention of efficient blue light-emitting diodes which has enabled bright and energy-saving white light sources’

1.3 General Information In Fig. 1.16, the periodic table of elements is shown. In Table 1.1 the physical properties of various semiconductors are summarized. Data on semiconductors can be found in [152–166].

1.3 General Information Fig. 1.16 Periodic table of elements. From [167]

15

16

1 Introduction

Table 1.1 Physical properties of various (bulk) semiconductors at room temperature. ‘S’ denotes the crystal structure (d: diamond, w: wurtzite, zb: zincblende, ch: chalcopyrite, rs: rocksalt) S

a0 (nm)

C Si

d d

0.3567 0.5431

Ge

d

α-Sn 3C-SiC 4H-SiC

d zb w

6H-SiC

w

AlN

w

AlP AlAs

zb zb

AlSb GaN

zb w

GaP GaAs

zb zb

GaSb InN

zb w

InP InAs InSb ZnO

zb zb zb w

ZnS ZnSe ZnTe CdO

zb zb zb rs

Eg (eV)

m ∗e

5.45 () 1.124 (X) 0.98 (m l ) 0.19 (m t ) 0.5658 0.67 (L) 1.58 (m l ) 0.08 (m t ) 0.64892 0.08 () 0.02 0.436 2.4 0.3073 (a) 3.26 1.005 (c) 0.30806 3.101 (a) 1.5117 (c) 0.3111 (a) 6.2 0.4978 (c) 0.54625 2.43 (X) 0.13 0.56605 2.16 (X) 0.5

0.61335 0.3189 (a) 0.5185 (c) 0.54506 0.56533

1.52 X) 3.4 ()

0.11 0.2

2.26 () 1.42 ()

0.13 0.067

0.60954 0.3533 (a) 0.5693 (c) 0.58686 0.60584 0.64788 0.325 (a) 0.5206 (c) 0.54109 0.56686 0.61037 0.47

0.72 () 0.69 ()

m ∗h

0

5.5 0.16 (m lh ) 11.7 0.5 (m hh ) 0.04 (m lh ) 16.3 0.3 (m hh )

nr

μe (cm2 /Vs)

μh (cm2 /Vs)

2.42 3.44

2200 1350

1600 480

4.00

3900

1900

2000 1000

1000 50 120

1140

850

80 1000

80

9.7 9.6

2.7 2.7

10.2

2.7

8.5

3.32

9.8 0.49 (m lh ) 12 1.06 (m hh ) 0.39 11 0.8 12

3.0

3.4 2.4

200 1500

300

3.37 3.4

300 8500

150 400

0.045

0.67 10 0.12 (m lh ) 12.5 0.5 (m hh ) 0.39 15

3.9

5000

1000

1.35 () 0.36 () 0.18 () 3.4 ()

0.07 0.028 0.013 0.24

0.4 0.33 0.18 0.59

12.1 12.5 18 6.5

3.37 3.42 3.75 2.2

4000 22 600 100 000 220

600 200 1700

3.6 () 2.58 () 2.25 () 2.16

0.3 0.17 0.15

8.3 8.1 9.7

2.4 2.89 3.56

110 600

(continued)

1.3 General Information

17

Table 1.1 (continued) S

a0 (nm)

Eg (eV)

m ∗e

m ∗h

0

nr

μe (cm2 /Vs)

CdS

w

2.42 ()

0.2

0.7

8.9

2.5

250

CdSe CdTe

zb zb S

0.4 0.35 m ∗h

10.6 10.9 0

2.75 nr

650 1050 μe (cm2 /Vs)

100 μh (cm2 /Vs)

rs zb zb zb rs rs

1.73 () 1.50 () Eg (eV) 7.3 2.0 () −0.15 () −0.15 () 0.37 (L) 0.26 (L)

0.13 0.11 m ∗e

MgO HgS HgSe HgTe PbS PbSe

0.416 (a) 0.6756 (c) 0.650 0.64816 a0 (nm) 0.421 0.5852 0.6084 0.64616 0.5936 0.6147

100 600 930

rs

0.645

0.29 (L)

25 0.3 20 0.1 170 0.06 (m lh ) 250 0.03 (m hh ) 0.3 (m lh ) 412 0.02 (m hh )

50 18 500 22 000 500 1800

PbTe

1400

1100

ZnSiP2

ch

2.96 ()

ZnGeP2

ch

ZnSnP2

ch

CuInS2

ch

CuGaS2

ch

CuInSe2

ch

CuGaSe2

ch

0.54 (a) 1.0441 (c) 0.5465 (a) 1.0771 (c) 0.5651 (a) 1.1302 (c) 0.523 (a) 1.113 (c) 0.5347 (a) 1.0474 (c) 0.5784 (a) 1.162 (c) 0.5614 (a) 1.103 (c)

0.045 0.029 0.1 0.07 (m lh ) 0.039 (m hh ) 0.24 (m lh ) 0.02 (m hh ) 0.07

2.34 () 1.66 () 1.53 () 2.5 () 1.0 () 1.7 ()

0.5

3.7 3.7

μh (cm2 /Vs)

Part I

Fundamentals

Chapter 2

Bonds

Protons give an atom its identity, electrons its personality. B. Bryson [168]

Abstract A little bit of solid state physics... The schemes of covalent, ionic and mixed bonds are explained which are the basis for the atomic arrangement and crystal structures of semiconductors.

2.1 Introduction The positively charged atomic nuclei and the electrons in the atomic shells of the atoms making up the semiconductor (or any other solid) are in a binding state. Several mechanisms can lead to such cohesiveness. First, we will discuss the homopolar, electron-pair or covalent bond, then the ionic bond and subsequently the mixed bond. We will only briefly touch on the metallic bond and the van-der-Waals bond. A classical book on bonds in semiconductors is [169, 170].

2.2 Covalent Bonds Covalent bonds are formed due to quantum-mechanical forces. The prototype covalent bond is the bonding of the hydrogen molecule due to overlapping of the atomic shells. If several electron pairs are involved, directional bonds can be formed in various spatial directions, eventually making up a solid.

2.2.1 Electron-Pair Bond The covalent bond of two hydrogen atoms in a H2 molecule can lead to a reduction of the total energy of the system, compared to two single (distant) atoms (Fig. 2.1). For fermions (electrons have spin 1/2) the two-particle wavefunction of the two (indistinguishable) electrons A and B must be antisymmetric, i.e. (A, B) = −(B, A) (Pauli principle). The wavefunction of each electron has degrees of freedom in real space (r) and spin (σ ), (A) = r (A) σ (A). The two-particle wavefunction © Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_2

21

22

2 Bonds

(a)

(b) A

S

Fig. 2.1 Binding of the hydrogen molecule. a Dashed line: classical calculation (electrostatics), ‘S’, ‘A’: quantummechanical calculation taking into account Pauli’s principle (S: symmetric orbital, antiparallel spins, A: antisymmetric orbital, parallel spins). The distance of the nuclei (protons) is given in units of the Bohr radius aB = 0.053 nm, the energy is given in Rydberg units (13.6 eV). b Schematic contour plots of the probability distribution ( ∗ ) for the S and A states

of the molecule is nonseparable and has the form (A, B) = r (r A , r B ) σ (σ A , σ B ). The binding state has a wavefunction with a symmetric orbital and antiparallel spins, i.e. r (r A , r B ) = r (r B , r A ) and σ (σ A , σ B ) = −σ (σ B , σ A ). The antisymmetric orbital with parallel spins is antibinding for all distances of the nuclei (protons).

2.2.2 sp3 Bonds Elements from group IV of the periodic system (C, Si, Ge, . . .) have 4 electrons on the outer shell. Carbon has the electron configuration 1s2 2s2 2p2 . For an octet configuration bonding to four other electrons would be optimal (Fig. 2.2). This occurs through the mechanism of sp3 hybridization.1 First, one electron of the ns2 np2 configuration is brought into a p orbital, such that the outermost shell contains one s, px , p y , and pz orbital each (Fig. 2.3a–e). The energy necessary for this step is less than regained in the subsequent formation of the covalent bonds. The four orbitals can be reconfigured into four other wavefunctions, the sp3 hybrids (Figs. 2.3f–i), i.e. 1 = (s + px + p y + pz )/2 2 = (s + px − p y − pz )/2

(2.1a) (2.1b)

3 = (s − px + p y − pz )/2 4 = (s − px − p y + pz )/2 .

(2.1c) (2.1d)

These orbitals have a directed form along tetrahedral directions. The binding energy (per atom) of the covalent bond is large, for H–H 4.5 eV, for C–C 3.6 eV, for Si–Si 1.8 eV, and for Ge–Ge 1.6 eV. Such energy is, for neutral atoms, comparable to the ionic bond, discussed in the next section.

1 It is debated in femtosecond chemistry whether the bond really forms in this way. However, it is a picture of overwhelming

simplicity.

2.2 Covalent Bonds

23

Fig. 2.2 Octet, the favorite card game of the ‘Atomis’ (trying to reach octet configuration in a bond by swapping wavefunctions). The bubble says: ‘Do you have a 2p?’. Reprinted with permission from [171], ©2002 Wiley-VCH

(a) -1

0

(b)

1

-1

0

(c)

1

-2 1

0

0 -1

-2 0

1 -1

0

0

1

-1

1 0

0

-1 -1

(d)

2

-1

1

1

1

0

-1

-1 -1

0

1

-1

1

0

2

1

(e) 2py

2px

2pz

(f) -2

-1

0

1

2

2py

2px

2s

2pz

2s

(g) -2

-1

0

1

2

(h) -2

-1

0

1

2

(i) -2

2

2

2

2

1 0 -1 -2

1 0 -1 -2

1 0 -1 -2

1 0 -1 -2

-2

-1

-2 0

1

2

-1

-2 0

1

2

-1

-1

-2 0

1

2

0

-1

1

2

0

1

2

Fig. 2.3 a s orbital, b, c, d px , p y and pz orbital, e hybridization, f, g, h, i orbitals of the sp3 hybridization: f (s+px +p y +pz )/2, g) (s+px −p y −pz )/2, h (s−px +p y −pz )/2, (i) (s−px −p y +pz )/2

In Fig. 2.4a the energy of a crystal made up from silicon atoms is shown for various crystal structures2 or phases (cf. Chap. 3). We note that the crystal energy of further silicon structures are discussed in [175]. The lattice constant with the lowest total energy determines the lattice spacing for each crystal structure. The thermodynamically stable configuration is the phase with the lowest overall energy for given external conditions. The covalent bond of a group-IV atom to other group-IV atoms has a tetrahedral configuration with electron-pair bonds, similar to the hydrogen molecule bond. In Fig. 2.4b the energy states of the n = 2 shell for tetrahedrally bonded carbon (diamond, see Chap. 3.4.3) are shown as a function of 2 Hexagonal

diamond is wurtzite structure with identical atoms in the base.

24

2 Bonds

(a)

(b) conduction band 6 states per atom

4 states per atom

2p

Energy

2s 2 states per atom

valence band 4 states per atom

observed lattice constant

lattice constant

Fig. 2.4 a Energy per atom in silicon for various crystal structures. Adapted from [172]. b Electron energy levels in (diamond structure) carbon as a function of the distance of the atomic nuclei (schematic). Adapted from [173, 174]

Fig. 2.5 Schematic of the origin of valence and conduction band from the atomic s and p orbitals. The band gap E g and the position of the Fermi level E F are indicated

Fig. 2.6 Schematic representation of a bonding and b antibinding p orbitals. The signs denote the phase of the wavefunction

the distance from the nuclei. First, the energetically sharp states become a band due to the overlap and coupling of the atomic wavefunctions (cf. Sect. 6). The mixing of the states leads to the formation of the filled lower valence band (binding states) and the empty upper conduction band (antibinding states). This principle is valid for most semiconductors and is shown schematically also in Fig. 2.5. The configuration of bonding and antibinding p orbitals is depicted schematically in Fig. 2.6. The bonding and antibinding sp3 orbitals are depicted in Figs. 2.7a, b and 2.13. We note that the energy of the crystal does not only depend on the distance from the nuclei but also on their geometric arrangement (crystal structure). Per carbon atom there are (in the second shell) four electrons and four unoccupied states, altogether eight. These are redistributed into four states (filled) per atoms in the valence band and four states per atom (empty) in the conduction band. Between the top of the valence band and the bottom of the conduction band there is an energy gap, later called the band gap (cf. Chap. 6).

2.2 Covalent Bonds

-1

0

25 2

1

-1

2

1

-1

0

2

1

-1

3-2

3-2

3-2

3-2

2

2

2

2

1

1

1

0

0

0

-1

-1

-1

-1

-1

-2 -2 0

1

2

(b)

-1

-2 -2 0

1

2

(c)

0

2

1

1

0

-2 -2

(a)

0

-1

-2 -2 0

1

2

(d)

-1

0

1

2

Fig. 2.7 Schematic representation of a, c bonding and b, d antibinding symmetric a, b and nonsymmetric c, d sp3 orbitals

(a)

(b)

(c)

Fig. 2.8 Schematic representation of the a σ and b π bonds in benzene, c schematic symbol for benzene

2.2.3 sp2 Bonds Organic semiconductors (see Chap. 18) are made up from carbon compounds. While for inorganic semiconductors the covalent (or mixed, cf. Sect. 2.4) bond with sp3 hybridization is important, the organic compounds are based on the sp2 hybridization. This bonding mechanism, which is present in graphite, is stronger than the sp3 -bond present in diamond. The prototype organic molecule is the benzene ring3 (C6 H6 ), shown in Fig. 2.8. The benzene ring is the building block for small organic molecules and polymers. In the benzene molecule neighboring carbon atoms are bonded within the ring plane via the binding σ states of the sp2 orbitals (Fig. 2.8a). The wavefunctions (Fig. 2.9) are given by (2.2ac). √ √ 2 px )/ 3 √ 2 = (s − 1/2 px + 3/2 p y )/ 3 √ 3 = (s − 1/2 px − 3/2 p y )/ 3 . 1 = (s +

(2.2a) (2.2b) (2.2c)

The ‘remaining’ pz orbitals do not directly take part in the binding (Fig. 2.8b) and form bonding (π , filled) and antibinding (π *, empty) orbitals (see Fig. 2.10). The π and π * states are delocalized over the ring. A more in-depth view considers the alternating ’staggered’ spin configuration around the ring [177]. Between the highest populated molecular orbital (HOMO) and the lowest unoccupied molecular orbital (LUMO) is typically an energy gap (Fig. 2.11). The antibinding σ ∗ orbitals are energetically above the π * states.

3 Supposedly, the chemist Friedrich August Kekulé von Stadonitz had a dream about dancing carbon molecules and thus came up with the ring-like molecule structure [176].

26

2 Bonds 1 1

1

0

0

(e)

2px

2s 0

-1

0

2py

-1

1

(c)

2

2pz

2s

1

0

2px

0

(d)

1

2py

2pz

1

0 -2

-2

2

2

2

1

1

1

0

0

0

-1

-1

-1

-2

-2

-2 -2

-1

-2 0

1

(g)

1

-1

-1

-1 -2

(f)

-1

-1

(b)

1

1

0 -2

0

1

-1

-1

-1

0

1

0

-1

0 -1

-2

1

0

2

0

-1

1

(a)

1

0

-1

-1

-2 0

1

(h)

-1

0

1

√ √ Fig. 2.9 a s orbital, b,c,d px , p y and pz orbital, e hybridization, f,g,h orbitals of the sp2 hybridization: f (s+ 2 px )/ 3, √ √ √ √ √ √ g (s− 1/2 px + 3/2 p y )/ 3, h (s− 1/2 px − 3/2 p y )/ 3 Fig. 2.10 Orbitals due to binding and antibinding configurations of various π orbitals

2.3 Ionic Bonds

27

Fig. 2.11 Schematic energy terms of the benzene molecule

6

pz

18 sp2

} }

LUMO HOMO

2.3 Ionic Bonds Ionic crystals are made up from positively and negatively charged ions. The heteropolar or ionic bond is the consequence of the electrostatic attraction between the ions. However, the possibly repulsive character of next neighbors has to be considered. For I–VII compounds, e.g. LiF or NaCl, the shells of the singly charged ions are complete: Li: 1s2 2s1 → Li+ : 1s2 , F: 1s2 2s2 2p5 → F− : 1s2 2s2 2p6 . Compared to ions in a gas, a Na–Cl pair in the crystal has a binding energy of 7.9 eV that mostly stems from the electrostatic energy (Madelung energy). Van-der-Waals forces (cf. Sect. 2.6) only contribute 1–2%. The ionization energy of Na is 5.14 eV, the electron affinity of Cl is 3.61 eV. Thus the energy of the NaCl pair in the solid is 6.4 (=7.9−5.1+3.6) eV smaller than in a gas of neutral atoms. The interaction of two ions with distance vector ri j is due to the Coulomb interaction UiCj =

qi q j 1 e2 1 =± 4π 0 ri j 4π 0 ri j

(2.3)

and a repulsive contribution due to the overlap of (complete) shells. This contribution is typically approximated by a radially symmetric core potential = λ exp(−λ/ρ) Uicore j

(2.4)

that only acts on next neighbors. λ describes the strength of this interaction and ρ parameterizes its range. The distance of ions is denoted as ri j = pi j R, where R denotes the distance of next neighbors and the pi j are suitable coefficients. The electrostatic interaction of an ion with all its neighbors is then written as e2 1 , (2.5) UiCj = −α 4π 0 R where α is the Madelung constant. For an attractive interaction (as in a solid), α is positive. It is given (calculated for the i-th ion) as ±1 α= . (2.6) pi j ij For a one-dimensional chain α = 2 ln 2. For the rocksalt (NaCl) structure (cf. Sect. 3.4.1) it is α ≈ 1.7476, for the CsCl structure (see Sect. 3.4.2) it is α ≈ 1.7627, and for the zincblende structure (see Sect. 3.4.4) it is α ≈ 1.6381. This shows that ionic compounds prefer the NaCl or CsCl structure.

28

2 Bonds Na

Na

Cl

Cl

Cl

(a) Na

Na

Cl

Na

Na

Cl

Cl

Cl

(b) Na

Na

Cl

Fig. 2.12 a Experimental and b theoretical charge distribution in the (100) plane of NaCl.√The lowest contour in the interstitial region corresponds to a charge density of 7 e/nm3 and adjacent contours differ by 2. Differences are mainly due to the fact that the X-ray experiments have been made at room temperature. Adapted from [178]

The charge distribution for NaCl is shown in Fig. 2.12. For tetragonal and orthorhombic structures, the Madelung constant has been calculated in [179].

2.4 Mixed Bonds The group-IV crystals are of perfectly covalent nature, the I–VII are almost exclusively ionically bonded. For III–V (e.g. GaAs, InP) and II–VI compounds (e.g. CdS, ZnO) we have a mixed case. The (screened) Coulomb potentials of the A and B atoms (in the AB compound) shall be denoted V A and VB . The origin of the coordinate system is in the center of the A and B atom (i.e. for the zincblende structure (cf. Sect. 3.4.4) at (1/8, 1/8, 1/8)a. The valence electrons then see the potential Vcrystal =

V A (r − rα ) +

α

VB (r − rβ ) ,

(2.7)

β

where the sum α (β) runs over all A (B) atoms. This potential can be split into a symmetric (Vc , covalent) and an antisymmetric (Vi , ionic) part (2.8b), i.e. Vcrystal = Vc + Vi 1 Vc = 2

+ 1 Vi = 2

V A (r − rα ) +

α

VB (r − rβ ) +

β

+

VB (r − rα )

α

V A (r − rα ) −

α

VB (r − rβ ) −

β

(2.8a)

⎭

VB (r − rα )

α

β

V A (r − rβ )

β

⎫ ⎬

V A (r − rβ )

⎫ ⎬ ⎭

.

(2.8b)

2.4 Mixed Bonds

29

(a)

(b)

Fig. 2.13 Schematic representation of a bonding and b antibinding sp3 orbitals. From [169]

For homopolar bonds Vi = 0 and the splitting between bonding and antibinding states is E h , which mainly depends on the bond length l AB (and the related overlap of atomic wavefunctions). In a partially ionic bond the orbitals are not symmetric along A–B, but the center is shifted towards the more electronegative material (Figs. 2.7c, d and 2.13). The band splitting4 between the (highest) bonding and (lowest) antibinding state E ba is then written as (2.9) E ba = E h + iC , where C denotes the band splitting due to the ionic part of the potential and depends only on V A − VB . C is proportional to the difference of the electronegativities X of the A and B atoms, C(A, B) = 5.75(X A − X B ). A material thus takes a point in the (E h ,C) plane (Fig. 2.14). The absolute value for 2 = E h2 + C 2 . the band splitting is given as E ba The ionicity of the bond is described with the ionicity (after Phillips) f i , defined as [181, 182] fi =

C2 . E h2 + C 2

(2.10)

The covalent part is 1 − f i . In Table 2.1 the ionicity is given for a number of binary compounds. The ionicity can also be interpreted as the angle tan(φ) = C/E h in the (E h ,C) diagram. The critical value of f i = 0.785 for the ionicity separates quite exactly (for about 70 compounds) the 4-fold (diamond, zincblende and wurtzite) from the 6-fold (rocksalt) coordinated substances ( f i = 0.785 is indicated by a dashed line in Fig. 2.14). For ionic compounds, an effective ionic charge e∗ is defined connecting the displacement u of negative and positive ions and the resulting polarization P = (e∗ /2a 3 ) u [183]. Connected with the ionicity is the so-called s-parameter, describing the change of the charge upon change of bond length b from its equilibrium value b0 [184] ∗

∗

e (b) = e (b0 )

b b0

s

≈ e0∗ (1 + s ) ,

(2.11)

being the strain of the bond length, b/b0 = 1 + . It seems justified to assume that e∗ (b0 ) is always positive at the metal atom in III–V and II–VI compounds. The relation of s with the ionicity f i is shown in Fig. 2.15 for various compound semiconductors.

4 This energy should not be confused with the band gap E

cv , the energy separation of the highest valence-band state and the lowest conduction-band state. The energy splitting E ba is the energy separation between the centers of the valence and conduction bands. Mostly, the term E g is used for E cv .

30

2 Bonds

Fig. 2.14 Values of E h and C for various A N B 8−N compounds. The dashed line f i = 0.785 separates 4-fold from 6-fold coordinated structures. Most data taken from [180] Table 2.1 Ionicity f i (2.10) for various binary compounds C Si Ge Sn BAs BP BeTe SiC AlSb BN GaSb BeSe

0.0 0.0 0.0 0.0 0.002 0.006 0.17 0.18 0.25 0.26 0.26 0.26

Fig. 2.15 s-Parameter as defined in (2.11) as a function of the ionicity f i (2.10) for various compound semiconductors. Dashed lines are guides to the eye. Data from [185], value for CuCl from [184]

AlAs BeS AlP GaAs InSb GaP InAs InP AlN GaN MgTe InN

0.27 0.29 0.31 0.31 0.32 0.33 0.36 0.42 0.45 0.50 0.55 0.58

BeO ZnTe ZnO ZnS ZnSe HgTe HgSe CdS CuI CdSe CdTe CuBr

0.60 0.61 0.62 0.62 0.63 0.65 0.68 0.69 0.69 0.70 0.72 0.74

CuCl CuF AgI MgS MgSe CdO HgS MgO AgBr LiF NaCl RbF

0.75 0.77 0.77 0.79 0.79 0.79 0.79 0.84 0.85 0.92 0.94 0.96

2.5 Metallic Bonding

31

2.5 Metallic Bonding In a metal, the positively charged atomic cores are embedded in a more or less homogeneous sea of electrons. The valence electrons of the atoms become the conduction electrons of the metal. These are freely moveable and at T = 0 K there is no energy gap between filled and empty states. The bonding is mediated by the energy reduction for the conduction electrons in the periodic potential of the solid compared to free atoms. This will be clearer when the band structure is discussed (Chap. 6). In transition metals the overlap of inner shells (d or f) can also contribute to the bonding.

2.6 Van-der-Waals Bonds The van-der-Waals bond is a dipole bond that leads to bonding in the noble-gas crystals (at low temperature). Ne, Ar, Kr and Xe crystallize in the densely packed fcc lattice (cf. Sect. 3.3.2.1). He3 and He4 represent an exception. They do not solidify at zero pressure at T = 0 K due to the large zero-point energy. This quantum-mechanical effect is especially strong for oscillators with small mass. When two neutral atoms come near to each other (distance of the nuclei R), an attractive dipole– dipole interaction −A R −6 arises (London interaction) the van-der-Waals interaction. The quantummechanical overlap of the (filled) shells leads to a strong repulsion +B R −12 . Altogether, a binding energy minimum results for the Lennard–Jones potential VLJ (see Fig. 2.16) VLJ (R) = −

A B + 12 . R6 R

(2.12)

The energy minimum E min = −A2 /(2B) is at R = (2B/A)1/6 . The origin of the attractive dipole–dipole interaction can be understood from a one-dimensional (1D) model as follows: Two atoms are modeled by their fixed positively charged nuclei in a distance R and their negatively charged electron shells that are polarizable, i.e. can be displaced along one direction x. Additionally, we assume (two identical) 1D harmonic oscillators for the electron motion at the positions 0 and R. Then, the Hamilton operator H0 of the system without interaction (R is very large) 1 2 1 2 p1 + C x12 + p + C x22 . (2.13) H0 = 2m 2m 2

Fig. 2.16 Lennard–Jones potential (2.12) for A = 1 and two values of B

32

2 Bonds

The indices 1 and 2 denote the two electrons of atoms. x1 and x2 √ are the displacements of the electrons. Both harmonic oscillators have a resonance frequency ω0 = C/m, and the zero-point energy is ω0 /2. Taking into account the Coulomb interaction of the four charges, an additional term H1 arises H1 =

e2 e2 e2 e2 2e2 + − − ≈ − 3 x1 x2 . R R + x1 + x2 R + x1 R − x2 R

(2.14)

The approximation is valid for small amplitudes xi R. A separation of variables can be achieved by transformation to the normal modes xs =

x1 + x2 x1 − x2 . √ , xa = √ 2 2

(2.15)

Then we find H = H0 + H1

1 2 1 2e2 2e2 1 2 1 2 p + C − 3 xs + p + C − 3 xa2 . = 2m s 2 R 2m a 2 R

(2.16)

This equation is the Hamiltonian of two decoupled harmonic oscillators with the normal frequencies ω± =

2e2 C± 3 R

/m ≈ ω0

1 1± 2

2e2 C R3

1 − 8

2e2 C R3

2 + ...

.

(2.17)

The coupled system thus has a lower (zero-point) energy than the uncoupled. The energy difference per atom is (in lowest order) proportional to R −6 . 1 1 U = ω0 − (ω+ − ω− ) ≈ −ω0 2 8

2e2 C R3

2 =−

A . R6

(2.18)

The interaction is a true quantum-mechanical effect, i.e. the reduction of the zero-point energy of coupled oscillators.

2.7 Hamilton Operator of the Solid The total energy of the solid, including kinetic and potential terms, is H=

p2 P2j i + 2m i 2M j i j + −

Z j Z j e2 e2 1 1 + 2 j, j 4π 0 |R j − R j | 2 i,i 4π 0 |ri − ri | i, j

Z j e2 , 4π 0 |R j − ri |

(2.19)

2.7 Hamilton Operator of the Solid

33

where ri and Ri are the position operators and pi and Pi are the momentum operators of the electrons and nuclei, respectively. The first term is the kinetic energy of the electrons, the second term is the kinetic energy of the nuclei. The third term is the electrostatic interaction of the nuclei, the fourth term is the electrostatic interaction of the electrons. In the third and fourth terms the summation over the same indices is left out. The fifth term is the electrostatic interactions of electrons and nuclei. In the following, the usual approximations in order to treat (2.19) are discussed. First, the nuclei and the electrons tightly bound to the nuclei (inner shells) are united with ion cores. The remaining electrons are the valence electrons. The next approximation is the Born–Oppenheimer (or adiabatic) approximation. Since the ion cores are much heavier than the electrons (factor ≈ 103 ) they move much slower. The frequencies of the ion vibrations are typically in the region of several tens of meV (phonons, cf. Sect. 5.2), the energy to excite an electron is typically 1 eV. Thus, the electrons always ‘see’ the momentary position of the ions, the ions, however, ‘see’ the electron motions averaged over many periods. Thus, the Hamiltonian (2.19) is split into three parts: H = Hions (R j ) + He (ri , R j0 ) + He−ion (ri , δR j ) .

(2.20)

The first term contains the ion cores with their potential and the time-averaged contribution of the electrons. The second term is the electron motion around the ion cores at their averaged positions R j0 . The third term is the Hamiltonian of the electron–phonon interaction that depends on the electron positions and the deviation of the ions from their average position δR j = R j − R j0 . The electron– phonon interaction is responsible for such effects as electrical resistance and superconductivity.

Chapter 3

Crystals

La science cristallographique ne consiste donc point à décrire scrupuleusement tous les accidens des formes cristallines; mais à spécifier, en décrivant ces formes, les rapports plus ou moins immédiats qu’elles ont entre elles. Crystallographic science does not consist in the scrupulous description of all the accidental crystalline forms, but in specifying, by the description of these forms, the more or less close relationship they have with each other. J.-B. Romé de l’Isle, 1783 [186]

Abstract A little bit of crystallography. The concepts of the direct and reciprocal lattice, point and space groups, unit and elementary cells and the Wigner- Seitz cell are laid out. The important crystal structures for semiconductors (diamond, sphalerite, wurtzite, chalcopyrite, ...) are discussed in some detail. Also alloys and ordering are covered.

3.1 Introduction The economically most important semiconductors have a relatively simple atomic arrangement and are highly symmetric. The symmetry of the atomic arrangement is the basis for the classification of the various crystal structures. Using group theory [187], basic and important conclusions can be drawn about the physical properties of the crystal, such as its elastic and electronic properties. The presence of highly symmetric planes is obvious from the crystal shape of the minerals and their cleavage behavior. Polycrystalline semiconductors consist of grains of finite size that are structurally perfect but have various orientations. The grain boundaries are a lattice defect (see also Sect. 4.4.3). Amorphous semiconductors are disordered on the atomic scale, see Sect. 3.3.7.

3.2 Crystal Structure A crystal is built up by the (quasi-) infinite periodic repetition of identical building blocks. This translation lattice [188–190] is generated by the three fundamental translation vectors a1 , a2 and a3 . These three vectors may not lie in a common plane. The lattice (Fig. 3.1) is the set of all points R R = n 1 a1 + n 2 a2 + n 3 a3 .

(3.1)

© Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_3

35

36

3 Crystals

(a)

(b)

Fig. 3.1 a Two-dimensional lattice. It can be generated by various pairs of translation vectors. b Elementary cells of the lattice. Primitive elementary cells are shaded Fig. 3.2 Crystal structure, consisting of a lattice and a base

Base

The crystal structure is made up by the lattice and the building block that is attached to each lattice point. This building block is called the base (Fig. 3.2). In the simplest case, e.g. for crystals like Cu, Fe or Al, this is just a single atom (monoatomic base). In the case of C (diamond), Si or Ge, it is a diatomic base with two identical atoms (e.g. Si–Si or Ge–Ge), in the case of zincblende compound semiconductors, such as GaAs or InP, it is a diatomic base with nonidentical atoms such as Ga–As or In–P. For wurtzite crystals such as GaN or ZnO the base has four atoms like Ga–N–Ga–N. There exist far more involved structures, e.g. NaCd2 where the smallest cubic cell contains 1192 atoms. In protein crystals, the base of the lattice can contain 10,000 atoms. In summary: Crystal structure = Lattice × Base.

3.3 Lattice As described in Sect. 3.2 the lattice is spanned by three vectors ai . The lattice symmetry is decisive for the physical properties of the semiconductor. It is described by the appropriate groups of the symmetry operations.

3.3.1 2D Bravais Lattices There are five two-dimensional (2D) Bravais lattices (Fig. 3.3) which are distinct and fill all (2D) space. These are very important for the description of symmetries at surfaces. The 2D Bravais lattices are the square, hexagonal, rectangular and centered-rectangular lattice.

3.3 Lattice

37 a

Fig. 3.3 The two-dimensional Bravais lattices with the primitive unit cells: a square lattice (a = b, φ = 90◦ ), b hexagonal lattice (a = b, φ = 60◦ ), c rectangular lattice (a = b, φ = 90◦ ), d centered-rectangular lattice (a = b, φ = 90◦ , for the (nonprimitive) rectangular unit cell shown on the right)

a

b

b

(a)

(b) a

(c)

a

a

b

b

b

(d)

3.3.2 3D Bravais Lattices In three dimensions, the operations of the point group results in fourteen 3D Bravais lattices (Fig. 3.4), that are categorized into seven crystal classes (trigonal, monoclinic, rhombic, tetragonal, cubic, rhombohedral and hexagonal). These classes are discerned by the conditions for the lengths and the mutual angles of the vectors that span the lattice (Table 3.1). Some classes have several members. The cubic crystal can have a simple (sc), face-centered (fcc) or body-centered (bcc) lattice. In the following, some of the most important lattices, in particular those most relevant to semiconductors, will be treated in some more detail.

3.3.2.1

Cubic fcc and bcc Lattices

The primitive translation vectors for the cubic face-centered (fcc) and the cubic body-centered (bcc) lattice are shown in Fig. 3.5 and Fig. 3.6, respectively. Many metals crystallize in these lattices, e.g. copper (fcc) and tungsten (bcc).

Table 3.1 Conditions for lengths and angles for the 7 crystal classes. Note that only the positive conditions are listed. The rhombohedral system is a special case of the trigonal class. Conditions for the trigonal and hexagonal classes are the same, however, trigonal symmetry includes a single C3 or S6 axis, while hexagonal symmetry includes a single C6 or S65 axis System

#

Lattice symbol

Triclinic Monoclinic

1 2

s, c

Orthorhombic Tetragonal Cubic

4 2 3

s, c, bc, fc s, bc s, bc, fc

Trigonal

1

(Rhombohedral) Hexagonal

1 1

Conditions for the usual unit cell None α = γ = 90◦ or α = β = 90◦ α = β = γ = 90◦ a = b , α = β = γ = 90◦ a=b=c, α = β = γ = 90◦ a = b , α = β = 90◦ , γ = 120◦ a =b=c,α=β =γ a = b , α = β = 90◦ , γ = 120◦

38

3 Crystals

Fig. 3.4 The 14 three-dimensional Bravais lattices: cubic (sc: simple cubic, bcc: body-centered cubic, fcc: face-centered cubic), tetragonal (simple and body-centered), orthorhombic (simple, centered, body-centered and face-centered), monoclinic (simple and centered), triclinic, rhombohedral and hexagonal

bcc

fcc

tetragonal

orthorhombic

triclinic

monoclinic

rhombohedral

hexagonal

In the fcc lattice, one lattice point sits in the center of each of the six faces of the usual cubic unit cell. The vectors spanning the primitive unit cell are a1 =

a a a (1, 1, 0) , a2 = (0, 1, 1) , a3 = (1, 0, 1) . 2 2 2

(3.2)

In the bcc lattice, one extra lattice point sits at the intersection of the three body diagonals at (a1 + a2 + a3 )/2. The vectors spanning the primitive unit cell are a1 =

a a a (1, 1, −1) , a2 = (−1, 1, 1) , a3 = (1, −1, 1) . 2 2 2

(3.3)

3.3 Lattice

39

Fig. 3.5 Primitive translations of the fcc lattice. These vectors connect the origin with the face-center points. The primitive unit cell is the rhombohedron spanned by these vectors. The primitive translations a , b and c are given in (3.2). The angle between the vectors is 60◦

c'

a'

Fig. 3.6 Primitive translations of the bcc lattice. These vectors connect the origin with the lattice points in the cube centers. The primitive unit cell is the rhombohedron spanned by these vectors. The primitive translations a , b and c are given in (3.3). The angle between the vectors is ≈ 70.5◦

3.3.2.2

b'

a

a

b'

c'

a'

Hexagonally Close Packed Structure (hcp)

The 2D hexagonal Bravais lattice fills a plane with spheres (or circles) with maximum filling factor. There are two ways to fill space with spheres and highest filling factor. One is the fcc lattice, the other is the hexagonally close packed (hcp) structure.1 Both fcc and hcp have a filling factor of 74%. For the hcp, we start with a hexagonally arranged layer of spheres (A), see Fig. 3.7. Each sphere has six next-neighbor spheres. This could, e.g., be a plane in the fcc perpendicular to the body diagonal. the next plane B is put on top in such a way that each new sphere touches three spheres of the previous layer. The third plane can now be added in two different ways: If the spheres of the third layer are vertically on top of the spheres of layer A, a plane A’ identical to A has been created that is shifted from A along the stacking direction (normally called the c-axis) by chcp =

8/3 a ≈ 1.633 a .

(3.4)

The vectors spanning the primitive unit cell are a1 =

1 The

√ a a √ 1, − 3, 0 , a2 = 1, 3, 0 , a3 = c (0, 0, 1) . 2 2

hcp structure is not a Bravais lattice since the individual lattice sites are not completely equivalent.

(3.5)

40

3 Crystals

Fig. 3.7 Structure of the a hcp and b fcc lattice. For hcp the stacking (along the c-axis) is ABABAB. . ., for fcc (along the body diagonal) it is ABCABCABC. . .

(a)

(b)

The hcp stacking order is ABABAB. . . for hcp, the coordination number is 12. In the fcc structure, the third layer is put on the thus far unfilled positions and forms a new layer C. Only the forth layer is again identical to A and is shifted by cfcc =

√

6 a ≈ 2.45 a .

(3.6)

The fcc stacking order is ABCABCABC. . . In the hexagonal plane of the√fcc lattice (which will later be called a {111} plane) √ the distance between lattice points is a = a0 / 2, where a0 is the cubic lattice constant. Thus c = 3 a0 , just what is expected for the body diagonal. For real materials with hexagonal lattice the ratio c/a deviates from the ideal value given in (3.4). Helium comes very close to the ideal value, for Mg it is 1.623, for Zn 1.861. Many hcp metals exhibit a phase transition to fcc at higher temperatures.

3.3.3 Unit Cell The choice of the vectors ai making up the lattice is not unique (Fig. 3.1). The volume that is enclosed in the parallelepiped spanned by the vectors a1 , a2 and a3 is called the elementary cell. A primitive elementary cell is an elementary cell with the smallest possible volume (Fig. 3.1b). In each primitive elementary cell there is exactly one lattice point. The coordination number is the number of nextneighbor lattice points. A primitive cubic (pc) lattice, e.g. has a coordination number of 6. The typically chosen primitive elementary cell is the Wigner–Seitz (WS) cell that reflects the symmetry of the lattice best. The Wigner–Seitz cell around a lattice point R0 contains all points that are closer to this lattice point than to any other lattice point. Since all points fulfill such a condition for some lattice point Ri , the Wigner–Seitz cells fill the volume completely. The boundary of the Wigner– Seitz cell is made up by points that have the same distance to R0 and some other lattice point(s). The

3.3 Lattice

41

(b)

(a)

Fig. 3.8 a Construction of a two-dimensional Wigner–Seitz cell, b filling of space with WS cells

Wigner–Seitz cell around R0 is constructed by drawing lines from R0 to the next neighbors Rj , taking the point at half distance and erecting a perpendicular plane at (Rj + R0 )/2. The WS cell is the smallest polyhedron, circumscribed by these planes. A two-dimensional construction is shown in Fig. 3.8.

3.3.4 Point Group Besides the translations there are other operations under which the lattice is invariant, i.e. the lattice is imaged into itself. These are: Identity. The neutral element of any point group is the identity that does not change the crystal. It is denoted as 1 (E) in international (Schönfließ) notation. Rotation. The rotation around an axis may have a rotation angle of 2π , 2π /2, 2π /3, 2π /4 or 2π /6 or their integer multiples. The axis is then called n = 1-, 2-, 3-, 4- or 6-fold, respectively2 , and denoted as n (international notation) or Cn (Schönfließ). Objects with Cn symmetry are depicted in Fig. 3.9. Mirror operation with respect to a plane through a lattice point. Different mirror planes are discerned (Fig. 3.10) (after Schönfließ) σh : a mirror plane perpendicular to a rotational axis, σv : a mirror plane that contains a rotational axis, and σd : a mirror plane that contains a rotational axis and bisects the ¯ angle between two C2 axes. The international notation is 2. Inversion. All points around the inversion center r are replaced by −r. The inversion is denoted 1¯ (i) in international (Schönfließ) notation. Improper rotation. The improper rotation Sn is a rotation Cn followed immediately by the inversion ¯ 4¯ and 6¯ and their powers. Only the operation i denoted as n¯ in international notation. There are 3, combined operation n¯ is a symmetry operation, while the individual operations Cn and i alone are not symmetry operations. In the Schönfließ notation the improper rotation is defined as Sn = σh Cn , with σh being a mirror operation with a plane perpendicular to the axis of the Cn rotation, denoted as Sn .

C1

C2

C3

C4

C6

Fig. 3.9 Two-dimensional objects with perpendicular rotation axis Cn . Note that the circles do not exhibit σh symmetry with respect to the paper plane, i.e. they are different on the top and bottom side

2 5-fold

periodic symmetry is geometrically impossible. However, quasicrystals with aperiodic five-fold symmetry exist [191, 192], some of them possibly being semiconducting [193, 194].

42

3 Crystals C4

C2 C2

v v

O H

H

H

(a)

d

(b)

F C2

F

(c)

C2

H

Fig. 3.10 Mirror planes: a σv (at H2 O molecule), b σh (at F2 H2 molecule) and c σd

S1

S2

S6

S4

S3

Fig. 3.11 Two-dimensional objects with perpendicular improper rotation axis Sn . Note that the white and black circles do not exhibit σh symmetry with respect to the paper plane, i.e. they are white on the top and black on the bottom. The circles with a dot in the center exhibit σh symmetry, i.e. they look the same from top and bottom

There are S3 , S4 and S6 and 3¯ = S65 , 4¯ = S43 and 6¯ = S35 . For successive applications, the Sn yield previously known operations, e.g. S42 = C2 , S44 = E, S62 = C3 , S63 = i, S32 = C32 , S33 = σh , S34 = C3 , S36 = E. We note that formally S1 is the inversion i and S2 is the mirror symmetry σ . Objects with Sn symmetry are schematically shown in Fig. 3.11. These symmetry operations form 32 point groups. These groups are shown (with their different notations and elements) in Table B.2. The highest symmetry is the cubic symmetry Oh = O × i. The tetraeder group Td (methane molecule) is a subgroup of Oh , lacking the inversion operation. Important for surface symmetries, there are ten two-dimensional point groups (Sect. 11.2 and Table B.1).

3.3.5 Space Group The space group is formed by the combination of the elements of the point group with translations. The combination of a translation along a rotational axis with a rotation around this axis creates a screw axis n m . In Fig. 3.12a, a so-called 41 screw axis is shown. The first index n indicates the rotation angle, i.e. 2π/n, the second index indicates the translation, i.e. c m/n, c being the periodicity along the axis. There are eleven crystallographically allowed screw rotations.3 The combination of the mirror operation at a plane that contains a rotational axis with a translation along this axis creates a glide reflection (Fig. 3.12b). For an axial glide (or b-glide) the translation is parallel to the reflection plane. A diagonal glide (or d-glide) involves translation in two or three directions. A third type of glide is the diamond glide (or d-glide). There are 230 different space groups, listed in Appendix B. A detailed treatment can be found in [195].4 Important for surface symmetries, there are 17 two-dimensional space groups (Sect. 11.2).

32 , 3 , 3 , 4 , 4 , 4 , 6 , 6 , 6 , 6 , 6 . 1 1 2 1 2 3 1 2 3 4 5 4 One should in particular consider the pitfalls

pointed out in Appendix 10 of this reference.

3.3 Lattice

43

c

41

(a)

c/2

c/2

c/4

42

(b)

glide

21

Fig. 3.12 a Schematic drawing of a 41 and 42 screw axis. b Schematic drawing of an axial glide reflection. The mirror plane is shown with dashed outline. Opposite faces of the cube have opposite color. For comparison a 21 screw axis is shown

(a)

(b)

(c)

Fig. 3.13 Transmission electron micrographs of polycrystalline silicon (poly-Si). a As-deposited material from lowpressure chemical vapor deposition (LPCVD) at about 620 ◦ C, grain size is about 30 nm. b After conventional processing (annealing at 1150 ◦ C), average grain size is about 100 nm. c After annealing in HCl that provides enhanced point defect injection (and thus increased possibility to form larger grains), average grain size is about 250 nm. Adapted from [196]

3.3.6 Polycrystalline Semiconductors A polycrystalline material consists of crystal grains that are randomly oriented with respect to each other. Between two grains a (large-angle) grain boundary (see also Sect. 4.4.3) exists. An important parameter is the grain size and its distribution. It can be influenced via processing steps such as annealing. Polycrystalline semiconductors are used in cheap, large-area applications such as solar cells (e.g. polysilicon, CuInSe2 ) or thin-film transistors (poly-Si) or as n-conducting contact material in MOS diodes (poly-Si) as shown in Fig. 3.13 (see also Fig. 21.29). Polycrystalline material can be fabricated from amorphous material using annealing procedures as discussed in Sect. 24.6.1 for silicon.

3.3.7 Amorphous Semiconductors An amorphous material lacks the long-range order of the direct lattice. It is disordered on the atomic scale. Historically, amorphous Se (a-Se) has been investigated first; since the 1950’s amorphous chalco-

44

3 Crystals

(a)

(b)

Fig. 3.14 a Radial atomic distribution functions of crystalline (c-Ge, solid line) and amorphous (a-Ge, dashed line) germanium, determined from EXAFS (extended X-ray absorption fine structure [201]). Adapted from [202]. b A continuous random network model of amorphous silicon containing a dangling bond in the center of the figure. Reprinted with permission from [203]

genides and a-Ge [197] and since the late 1960s a-Si [198] are researched. The field of amorphous oxides started in the mid 1950s with vanadate glasses [199] and is currently very active with mixedmetal-based oxides [200] (cmp. Chap. 20). The local quantum mechanics provides almost rigorous requirements for the bond length to next neighbors. The constraints for the bond angle are less strict. Covalently bonded atoms arrange in an open network with the next-neighbor distance essentially preserved and correlations up to the third and fourth neighbors (Fig. 3.14a). The short-range order is responsible for the observation of semiconductor properties such as an optical absorption edge and also thermally activated conductivity. In Fig. 3.14b a model of a continuous random network (with a bond-angle distortion of less than about 20%) of a-Si is depicted. The diameter dSR of the short-range order region is related to a disorder parameter α via [204] a , (3.7) dSR = 2α where a is the next-neighbor interatomic distance. For a diamond structure it is related to the lattice √ constant by a = 3 a0 /4. Typically, a significant number of dangling bonds exists. Bonds try to pair but if an odd number of broken bonds exists locally, an unsaturated, dangling bond remains. This configuration can be passivated by a hydrogen atom. Thus, the hydrogenation of amorphous semiconductors is very important, in particular for a-Si. A hydrogen atom can also break an overlong (and therefore weak) bond, saturate one side and eventually leave a dangling bond. Amorphous material can be (re-)crystallized into crystalline, mostly polycrystalline material upon annealing. This is technologically very important for a-Si (see Sect. 24.6.1).

3.4 Important Crystal Structures Now the crystal structures that are important for semiconductor physics will be discussed. These are mainly the rocksalt (PbS, CdO, . . .), diamond (C, Si, Ge), zincblende (GaAs, InP, . . .) and wurtzite (GaN, ZnO, . . .) structures.

3.4 Important Crystal Structures

45

Fig. 3.15 a Rocksalt (NaCl) structure, b CsCl structure

(a)

(b)

(a)

(b)

Fig. 3.16 a Diamond structure and b zincblende structure (red spheres: A atoms, green spheres: B atoms). The tetragonal bonds are indicated

3.4.1 Rocksalt Structure ¯ The rocksalt (rs, NaCl, space group 225, Fm3m) structure (Fig. 3.15a) consists of a fcc lattice with the period a and a diatomic base in which the Cl atom is positioned at (0,0,0) and the Na atom √ at (1/2,1/2,1/2)a with a distance 3 a/2. Materials that crystallize (under normal conditions) in the rocksalt lattice are, e.g., KCl, KBr, PbS (galena), PbSe, PbTe, AgBr, MgO, CdO, MnO. AlN, GaN and InN undergo, under high pressure, a phase transition from the wurtzite into the rocksalt structure.

3.4.2 CsCl Structure ¯ (Fig. 3.15b) consists of a simple cubic lattice. Similar The CsCl structure (space group 221, Pm3m) as for the rocksalt structure, the base consists of different atoms at (0,0,0) and (1/2,1/2,1/2)a. Typical crystals with CsCl-structure are TlBr, TlI, CuZn (β-brass), AlNi.

3.4.3 Diamond Structure ¯ (Fig. 3.16a) has the fcc lattice. The base consists The diamond structure (C, space group 227, Fd3m) of two identical atoms at (0,0,0) and (1/4,1/4,1/4)a. Each atom has a tetrahedral configuration. The packing density is only about 0.34. The ABC-type stacking along the [111]-direction is visualized in Fig. 3.17a. The materials that crystallize in the diamond lattice are C, Ge, Si and α-Sn. Silicon as the most important semiconductor is particularly well researched [205]. The diamond structure (point group Oh ) has an inversion center, located between the two atoms of the base, i.e. at (1/8,1/8,1/8)a. The radii of the wavefunctions for various group-IV elements increases with the order number (Table 3.2), and accordingly the lattice constant increases. In Fig. 3.18a the unit cell with tetragonal symmetry of three places along the 111 direction is shown. In Fig. 3.18b the arrangement of atoms along 111 is depicted. The symmetry along this line is at least C3v . At the atoms sites it is Oh . The bond center (BC) and the hexagonal (H) position are a center of inversion and have D3d symmetry. The unoccupied ‘T’ positions have Td symmetry. High-pressure phases of silicon are already found in indentation experiments [206].

46

3 Crystals

diamond

wurtzite

[111]

[00.1]

C B A

A

(a)

B

(b)

Fig. 3.17 HRTEM images of a diamond structure (Si, {110} cross section) and b wurtzite structure (GaN, 10.0 azimuth). The ABC and AB stacking is indicated Table 3.2 Radii of the wavefunctions in the diamond structure, rs and r p are related to s1 p3 , rd to s1 p2 d1 and lattice constant a0 C Si Ge

rs (nm)

r p (nm)

rd (nm)

a0 (nm)

0.121 0.175 0.176

0.121 0.213 0.214

0.851 0.489 0.625

0.3567 0.5431 0.5646

(a)

(b)

Fig. 3.18 a Unit cell of the zincblende structure with the indication of tetragonal symmetries. The position of the small yellow (blue) sphere is the tetrahedrally configured unoccupied positions of the A (B) sublattice, denoted with ‘T’ in part (b). b Line along [111] in the zincblende structure. The positions of the A and B atoms are denoted by red and green circles as labeled. Other positions are called the bond center (‘BC’), antibonding (‘AB’) relative to A and B atoms (‘A–AB’, ‘B–AB’), hexagonal (‘H’) and tetrahedral position (‘T’, blue and yellow circles)

We note that α-Sn has little current importance. The diamond structure α–Sn phase is stable below 13.2 ◦ C. The addition of Ge inhibits the retransformation to metallic tin up to higher temperatures (e.g. 60 ◦ C for 0.75 weight percent Ge). The properties of gray tin are reviewed in [207].

3.4.4 Zincblende Structure ¯ The zincblende (sphalerite,5 ZnS, space group 216, F43m) structure (Fig. 3.16b) has a fcc lattice with a diatomic base. The metal (A) atom is at (0, 0, 0) and the nonmetal (B) atom is at (1/4, 1/4, 1/4)a. 5 Zincblende

technically means the material ZnS which occurs in sphalerite (cubic) and wurtzite (hexagonal) phase. However, in the literature the term ‘zincblende’ for the sphalerite structure is common and used throughout this book.

3.4 Important Crystal Structures

47

Fig. 3.19 a Top view (along the c-axis) and b side view of the wurtzite structure with the tetragonal bonds indicated. The top (bottom) surface of the depicted structure is termed the Zn-face, (00.1) ¯ (O-face, (00.1))

(a)

(b)

Fig. 3.20 Comparison of the tetragonal bonds in the a zincblende and b wurtzite structure (i: inversion center, m: symmetry plane)

Thus the cation and anion sublattices are shifted with respect to each other by a quarter of the body diagonal of the fcc lattice. The atoms are tetrahedrally coordinated, a Zn atom is bonded to four S atoms and vice versa. However, no inversion center is present any longer (point group Td ). In the zincblende structure the stacking order of diatomic planes along the body diagonal is aAbBcCaAbBcC. . . Many important compound semiconductors, such as GaAs, InAs, AlAs, InP, GaP and their alloys (cf. Sect. 3.7), but also the II–VI compounds ZnS, ZnSe, ZnTe, HgTe and CdTe and halides, including AgI, CuF, CuCl, CuBr, and CuI, crystallize in the zincblende structure. Four-fold coordinated materials (zincblende and wurtzite) typically undergo a phase transition into 6-fold coordinated structures upon hydrostatic pressure [208]. For GaAs under pressure see [209].

3.4.5 Wurtzite Structure The wurtzite structure (ZnS, space group 186, P63 mc) is also called the hexagonal ZnS structure (because ZnS has both modifications). It consists of a hexagonal lattice with a unit cell of four atoms (Fig. 3.19). Typically, it is thought √ of as a hcp structure with a diatomic base. The c/a ratio typically deviates from the ideal value ζ0 = 8/3 ≈ 1.633 (3.4) as listed in Table 3.3. The c-axis is a 63 screw axis. √ The Zn atom is located at (0, 0, 0), the S atom at (0, 0, 3/8)a. This corresponds to a shift of 3/8 c along the c-axis. This factor is called the cell-internal parameter u. For real wurtzite crystals u deviates from its ideal value u 0 = 3/8 = 0.375, e.g. for group-III nitrides u > u 0 . The diatomic planes have a stacking order of aAbBaAbB. . . along the [00.1]-direction as visualized in Fig. 3.17b. In Fig. 3.20 the different local structural environment of the atoms in the zincblende and wurtzite structure is shown.

48

3 Crystals

Table 3.3 c/a ratio of various wurtzite semiconductors. Listed is ξ = (c/a − ζ0 )/ζ0 . Data based on [210] Material

ξ (%)

Material

ξ(%)

Material

ξ (%)

Material

ξ (%)

AlN GaN InN ZnS ZnSe

−2.02 −0.49 −1.35 0.25 0.06

CdS CdSe CdTe MgS MgSe

−0.61 −0.18 0.25 −0.80 −0.67

CuBr CuCl CuI AgI ZnTe

0.43 0.55 0.74 0.12 0.74

BeO ZnO 6H-SiC BN MgTe

−0.61 −1.9 0.49 0.74 −0.67

Many important semiconductors with large band gap crystallize in the wurtzite structure, such as GaN, AlN, InN, [211] ZnO, [212] SiC, [213], CdS und CdSe.

3.4.6 Chalcopyrite Structure ¯ The chalcopyrite [214] (ABC2 , named after ‘fool’s gold’ CuFeS2 , space group 122, I42d) structure is relevant for I–III–VI2 (with chalcogenide anions) and II–IV–V2 (with pnictide anions) semiconductors such as, e.g., (Cu,Ag)(Al,Ga,In)(S,Se,Te)2 and (Mg,Zn,Cd)(Si,Ge,Sn)(As,P,Sb)2 . In Fig. 3.21, the derivation of zincblende and chalcopyrite compounds is shown schematically, including the kesterite materials of type I2 -II-IV-VI6 . In the chalcopyrite structure, a nonmetallic anion atom (‘C’) is tetrahedrally bonded to two different types of cation atoms (‘A’ and ‘B’) as shown in Fig. 3.22. The local surrounding of each anion is identical, two of both the A and B atoms. The structure is tetragonal. The aspect ratio η = c/(2a) deviates from its ideal value 1; typically η < 1 [215, 216]. If the C atom is in the tetrahedral center of the two A and two B atoms, the bond lengths RAC and RBC of the A–C and B–C bonds, respectively, are equal. Since the ideal A–C and B–C bond lengths dAC and dBC are typically unequal, this structure is strained. The common atom C is therefore displaced

Fig. 3.21 Scheme of II–VI zincblende and related chalcopyrite and kesterite compounds

Fig. 3.22 Chalcopyrite structure, red and yellow spheres denote the metal species. The bigger green spheres represent the nonmetal anion

3.4 Important Crystal Structures

49

Table 3.4 Lattice nonideality parameters η and u (from (3.10)) of various chalcopyrite compounds and their experimentally observed disorder stability (+/− indicates compound with/without order–disorder (D–O) transition, respectively). Data from [216] CuGaSe2 CuInSe2 AgGaSe2 AgInSe2 CuGaS2 CuInS2 AgGaS2 AgInS2

η

u

D–O

0.983 1.004 0.897 0.96 0.98 1.008 0.895 0.955

0.264 0.237 0.287 0.261 0.264 0.236 0.288 0.262

+ + − +

ZnSiAs2 ZnGeAs2 CdSiAs2 CdGeAs2 ZnSiP2 ZnGeP2 CdSiP2 CdGeP2

+ −

η

u

D–O

0.97 0.983 0.92 0.943 0.967 0.98 0.92 0.939

0.271 0.264 0.294 0.287 0.272 0.264 0.296 0.288

− + − − + − −

along [100] and [010] such that it is closer (if dAC < dBC ) to the pair of A atoms and further away from the B atoms. The displacement parameter is u=

R2 − R2 1 + AC 2 BC 4 a

(3.8)

and it deviates from the ideal value u 0 = 1/4 for the zincblende structure as listed in Table 3.4 for a number of chalcopyrite compounds. In the chalcopyrite structure

1 + η2 16 1 2 1 + η2 . =a + u− 2 16

RAC = a RBC

u2 +

(3.9a) (3.9b)

The minimization of the microscopic strain yields (in first order) [217] 2 2 1 3 dAC − dBC u∼ . = + 2 2 4 8 dAC + dBC

(3.10)

Compounds with u > u c , u c = 0.265 being a critical displacement parameter, (or u < 1/2 − u c = 0.235) are stable with regard to cation disorder [216]. In Fig. 3.23 the correlation of the calculated value for u according to (3.10) and the experimental values is shown.

3.4.7 Spinel Structure A large variety of ternary compounds of type AII BIII 2 CVI 4 crystallize inb the cubic spinel structure (spinel, MgAl2 O4 , space group 227, Fd3m). Typical elements are A: Mg, Cr, Mn, Fe, Co, Ni, Cu, Zn, Cd, Sn, B: Al, Ga, In, Ti, V, Cr, Mn, Fe, Co, Rh, Ni, and C: O, S, Se, Te. As an example ZnGa2 O4 (zinc gallate) has received attention as interfacial layer in ZnO/GaAs epitaxy [218], luminescent material [219], and as ferromagnetic semiconductor [220]. Also the (unwanted) appearance of zinc gallate inclusions is in competition with the formation of highly doped wurtzite ZnO:Ga; in the (normal) spinel cubic structure of ZnGa2 O4 the Zn2+ ions still occupy tetrahedral

50

3 Crystals

Fig. 3.23 Experimental values u exp of the displacement parameter for various chalcopyrites vs. the calculated value u calc according to (3.10). The dashed line indicates u exp = u calc . Adapted from [217]

Fig. 3.24 Spinel AB2 C4 crystal structure, the cations are depicted as yellow (A atoms) and silver (B atoms) spheres, the anions (C atoms) as blue spheres

sites, but the Ga3+ ions occupy octahedral sites instead of tetrahedral sites in doped wurtzite ZnO:Ga. (Sc,Al)MgO4 (SCAM) is available as substrate material. Also AVI BII 2 CVI 4 compounds exist, e.g. GeB2 O4 (with B=Mg, Fe, Co, Ni). The anion atoms (C2− ) sit on a fcc lattice. The A atoms fill 1/8 of all tetraeder spaces and the B atoms fill half of all octaeder places (Fig. 3.24). Often the cations are charged A2+ and B3+ , e.g. in ZnAl2 O4 , MgCr2 O4 or ZnCo2 O4 . Also A6+ and B1− exists, e.g. in WNa2 O4 . The cubic lattice constant is denoted as a. In real spinels, the anions deviate from the ideal fcc array which is accounted for by the parameter u, measuring the displacement of anions along the [111]direction [221]; if the A-site cation is at (0,0,0), an anion is at (u, u, u). The cation-anion distances are given by [222] 3 (u − 1/8) , = a 3 u 2 − 2 u − 3/8 .

RAC = a

(3.11a)

RBC

(3.11b)

The ideal value is u = 1/4; examples are u = 0.2624 for MgAl2 O4 , u = 0.2617 for ZnGa2 O4 and u = 0.2409 for SiFe2 O4 [222]. In the inverted spinel structure, for AII BIII 2 CVI 4 compounds, the cations are distributed like B(AB)C4 , i.e. the B cations occupy tetraeder and octaeder places, e.g. in Mg2+ (Mg2+ Ti4+ )O2− 4 or . Examples are magnetite (Fe O ), a material with high spin polarization, or Fe3+ (Ni2+ Fe3+ )O2− 3 4 4 MgFe2 O4 . Also AVI BII 2 CVI 4 compounds exist in this structure, e.g. SnB2 O4 (with B = Mg, Mn, Co, Zn), TiB2 O4 (with B = Mg, Mn, Fe, Co, Zn), and VB2 O4 (with B = Mg, Co, Zn).

3.4 Important Crystal Structures

51

Fig. 3.25 Fluorite crystal structure, the cations are depicted as red spheres, the anions as blue spheres

Fig. 3.26 Hexagonal unit cell of delafossite CuGaO2 . Oxygen atoms are bonded to the Cu in a dumbbell (‘DB’) configuration. In the edge-sharing (‘ES’) layer the Ga atoms are octahedrally configured as GaO6

Ga Cu O c

ES DB ES

2uc a

3.4.8 Fluorite Structure Named after the minerale fluorite (CaF2 , space group 225, Fm3m), this structure for binary ionic compounds occurs when the cation valence is twice the anion valence, e.g. for (cubic) ZrO2 (zirconia) or HfO2 . The lattice is fcc with a triatomic base. At (0,0,0) is the cation (e.g. Zr4+ ), the anions (e.g. O2− ) are at (1/4, 1/4, 1/4) a (as in the zincblende structure) and (3/4, 3/4, 3/4) a (Fig. 3.25). The anion atom positions are on a simple cubic lattice with lattice constant a/2. Zirconia can crystallize in various phases [223], the most prominent being the monoclinic, tetragonal and cubic phases. The cubic phase can be extrinsically stabilized using yttrium [224, 225] (YSZ, yttria-stabilized zirconia). Hafnium oxide has the remarkable property that the HfO2 /Si interface is stable and allows the fabrication of transistor gate oxides with high dielectric constant (see Sect. 24.5.5).

3.4.9 Delafossite Structure ¯ structure The I–III–O2 materials crystallize in the trigonal delafossite (CuFeO2 , space group 166, R3m) (Fig. 3.26). This structure is also called caswellsilverite (NaCrS2 ). In Table 3.5 the lattice parameters of some delafossite compounds are given. The (Cu,Ag) (Al,Ga,In)O2 materials are transparent conductive oxides (TCO). We note that Pt and Pd as group-I component create metal-like compounds because of the d9 configuration as opposed to the d10 configuration of Cu and Ag.

52

3 Crystals

3.4.10 Perovskite Structure The perovskite structure for ABO3 materials (calcium titanate, CaTiO3 , space group 62, Pnma) (Fig. 3.27) is relevant for ferroelectric semiconductors (cf. Sect. 16.3). It is cubic with the Ca (or Ba, Sr) ions (charge state 2+) on the corners of the cube, the O ions (2−) on the face centers and the Ti (4+) in the body center. The lattice is simple cubic, the base is Ca at (0,0,0), O at (1/2,1/2,0), (1/2,0,1/2) and (0,1/2,1/2) and Ti at (1/2,1/2,1/2). The ferroelectric polarization is typically evoked by a shift of the negatively and positively charged ions relative to each other. LaAlO3 (lanthanium alumi¯ [227]). Perovskites are also important nate) is available as substrate material (space group 226, Fm3c for materials for high temperature superconductivity. Another group of ABX3 perovskites is formed by halogen atoms (Cl, Br, I) instead of oxygen on the X-site (in −1 charge state). The B-site (former Ti-position) is taken up by lead (Pb) or other elements of same +2 valence. The A-site (former Ba-position) is populated with an organic molecule (+1) such as CH3 NH3 (methylammonium, or MA) [228] or HC(NH2 )2 (formamidinium, or FA). In a purely inorganic version of such halogen perovskite, the A-site site is populated with Cs [229]. In order to avoid Pb, CsSnX3 has been investigated. Various phases are observed next to the cubic phase (α-CsPbI3 ) such as orthorhombic (δ-CsPbBr3 ) or tetragonal [230]. Also, angular distortions of the PbX6 octahedrons are common and depend on material composition (Fig. 3.28). The phase stability depends on the octahedral factor μ = RB /RX and the tolerance factor t, t=√

RA + RX , 2(RB + RX )

(3.12)

with RA , RB and RX denoting the radius of the A-site and B-site cation, and X-site anion, respectively. The stability of 138 different halide perovskites has been calculated in terms of μ and t [231] (Fig. 3.29) and stability criteria have been given. A stable cubic phase requires 0.44 < μ < 0.9 and 0.8 ≤ t ≤ 1 [232].

Table 3.5 Lattice parameters a, c, and u of some delafossite compounds. Theoretical values are shown with asterisk. Data from [226] CuAlO2 CuGaO2 CuInO2

a (nm)

c (nm)

u (nm)

0.2858 0.2980 0.3292

1.6958 1.7100 1.7388

0.1099 0.1073∗ 0.1056∗

Fig. 3.27 Perovskite structure (BaTiO3 ), a A cell with 12-fold (cuboctahedrally) configured Ba, b B cell with octahedrally configured Ti

O

O

Ba

2-

Ti4+

Ti

(a)

(b)

Ba2+

3.4 Important Crystal Structures

53

Fig. 3.28 Schematic molecular models of orthorhombic- and cubic-phase CsPbBr3 perovskites with and without PbCl2 and Cl2 doping. Adapted from [232]

Fig. 3.29 Stability of ABX3 halide perovskites in terms of octahedral factor μ and tolerance factor t. Red (black) dots indicate stable (unstable) compounds. The region of unstable materials is shown in grey. Adapted from [231]

3.4.11 NiAs Structure The NiAs structure (space group 194, P63 /mmc) (Fig. 3.30) is relevant for magnetic semiconductors, such as MnAs, and also occurs in the formation of Ni/GaAs Schottky contacts [233]. The structure is hexagonal. The arsenic atoms form a hcp structure and are trigonal prismatically configured with six nearest metal atoms. The metal atoms form hcp planes and fill all octahedral holes of the As lattice. For a cubic close packed, i.e. fcc, structure this would correspond to the rocksalt crystal. The stacking is ABACABAC... (A: Ni, B,C: As).

3.4.12 Further Structures There are many other crystal structures that have relevance for semiconductor materials. Among them are the

54

3 Crystals

Fig. 3.30 NiAs structure, metal atoms: dark grey, chalcogenide atoms: light grey

(a)

(b)

¯ occurring, e.g., for sapphire substrates used in • corundum structure (Al2 O3 , space group 167, R3c) epitaxy or for gallium oxide α-Ga2 O3 (Ga2 O3 is a multiphase material [234, 235]) ¯ (see Fig. 20.3) • bixbyite structure (In2 O3 , δ-Ga2 O3 , space group 206, Ia3) • β-Ga2 O3 monoclinic structure (space group 12, C2/m) [235] • quartz (SiO2 ) structures, α-quartz (space group 154, P32 21) and β-quartz (space group 180, P62 22) Space does not permit to discuss these and other structures in more detail here. The reader should refer to textbooks on crystallography, e.g. [236–238], and space groups [195, 239]. A good source for information and images of crystal structures on the web is [240].

3.5 Polytypism and Polymorphism In polytype materials, several stacking orders are possible. One of them represents the thermodynamic ground state but others have very similar energy. An example is GaN which has been extensively investigated in its (equilibrium) wurtzite and also in its (zincblende) cubic form. But not only hcp or fcc but many different sequences, such as, e.g., ACBCABAC as the smallest unit cell along the stacking direction, are possible. A typical example is SiC, for which besides hcp and fcc many other (>40) stacking sequences are known. The largest primitive unit cell of SiC [213] contains 594 layers. Some of the smaller polytypes are sketched in Fig. 3.31. In Fig. 3.32 cubic diamond crystallites and metastable hexagonal and orthorhombic phases (in silicon) are shown. For the ternary alloy (cf. Sect. 3.7) Zn1−x Cdx S the numbers n h of diatomic layers with hexagonal stacking (AB) and n c of layers with cubic stacking (ABC) have been investigated. CdS has wurtzite structure and ZnS mostly zincblende structure. The hexagonality index α as defined in (3.13) is shown in Fig. 3.33 for Zn1−x Cdx S nh α= . (3.13) nh + nc Some semiconductor materials possess several crystal phases (polymorphs) that can be readily prepared under various (non-equilibrium) conditions. Due to their different physical properties, eventually they can be employed for different device applications. GaN with its hexagonal and cubic phases can be counted as such material. A prominent example of a multi-phase semiconductor is Ga2 O3 that exhibits, next to its monoclinic equilibrium structure, various other phases such as a rhombohedral (corundum, α-Ga2 O3 ) and an orthorhombic (κ-Ga2 O3 ) phase [244].

3.5 Polytypism and Polymorphism

55

C A B

C

C

B

B

A 2H wurtzite

A 3C zincblende

Zn S

C

B

B

B

A

C

C

A

C

A

A

B

A

B

C

C

B

A

B

A

C

A

B

A

A

B

4H 6H

C B A B C A C B C

A

8H

A B

10H

A 15R

(a)

(b) Fig. 3.31 a Polytypes of the zincblende and wurtzite lattice (found in SiC), the letters A, B and C denote the three possible positions of the diatomic layers (see Fig. 3.7). b High resolution TEM image of 6H-SiC. For the enlarged view on the left, the unit cell and the stacking sequence are indicated. Adapted from [241]

(a)

(b)

(c)

Fig. 3.32 Polytypes of diamond found in crystallites (metastable phases in silicon). a cubic type (3C) with stacking ABC, inset shows a diffractogram and the alignment of the C and Si lattice, b rhombohedral 9R crystallite with ABCBCACABA stacking, c 9R phase with interface to a hexagonal 2H (AB stacking) phase. Reprinted from [242] with permission, ©2001, Springer Nature

56

3 Crystals

(a)

(b)

Fig. 3.33 a Hexagonality index α (3.13) of Zn1−x Cdx S for various ternary compositions. Dashed line is a guide to the eye. b Regions of different polytypes in ZnSex S1−x . Adapted from [243]

3.6 Reciprocal Lattice The reciprocal lattice is of utmost importance for the description and investigation of periodic structures, in particular for X-ray diffraction [245], surface electron diffraction, phonon dispersion or scattering and the electronic band structure. It is the quasi-Fourier transformation of the crystal lattice. The crystal lattice is also called the direct lattice, in order to distinguish it from the reciprocal lattice.

3.6.1 Reciprocal Lattice Vectors When R denotes the set of vectors of the direct lattice, the set G of the reciprocal lattice vectors is given by the condition6 exp (i G · R) = 1 (3.14) for all R ∈ R and G ∈ G. Therefore, for all vectors r and a reciprocal lattice vector G exp (i G · (r + R)) = exp (i G · r) .

(3.15)

Each Bravais lattice has a certain reciprocal lattice. The reciprocal lattice is also a Bravais lattice, since when G1 and G2 are two reciprocal lattice vectors, then this is obviously true also for G1 + G2 . For the primitive translation vectors a1 , a2 and a3 of the direct lattice, the vectors b1 , b2 and b3 that span the reciprocal lattice are given directly for any lattice as 2π (a2 × a3 ) Va 2π b2 = (a3 × a1 ) Va 2π b3 = (a1 × a2 ) , Va b1 =

(3.16a) (3.16b) (3.16c)

where Va = a1 · (a2 × a3 ) is the volume of the unit cell spanned by the vectors ai . The volume of the unit cell in reciprocal space is Va∗ = (2π )3 /Va . 6 The

dot product a · b of two vectors shall also be denoted as ab.

3.6 Reciprocal Lattice

57

The vectors bi fulfill the conditions ai · b j = 2π δi j .

(3.17)

Thus, it is clear that (3.14) is fulfilled. For an arbitrary reciprocal lattice vector G = k1 b1 + k2 b2 + k3 b3 and a vector R = n 1 a1 + n 2 a2 + n 3 a3 in direct space we find G · R = 2π (n 1 k1 + n 2 k2 + n 3 k3 ) .

(3.18)

The number in brackets is an integer. Additionally, we note that the reciprocal lattice of the reciprocal lattice is again the direct lattice. The reciprocal lattice of the fcc is bcc and vice versa. The reciprocal lattice of hcp is hcp (rotated by 30◦ with respect to the direct lattice). For later, we note two important theorems. A (sufficiently well behaved) function f (r) that is periodic with the lattice, i.e. f (r) = f (r + R) can be expanded into a Fourier series with the reciprocal lattice vectors according to (3.19) f (r) = aG exp (i G · r) ,

where aG denotes the Fourier component of the reciprocal lattice vector G, aG = V f (r) exp(−i G · r) d3 r. If f (r) is lattice periodic, the integral given in (3.20) is zero unless G is a reciprocal lattice vector.

f (r) exp (−i G · r) d r = 3

V

aG . 0, G ∈ /G

(3.20)

3.6.2 Miller Indices The Miller indices [246] form a triplet of integer numbers to denote directions and lattice planes in the crystal. A vector R in direct space is denoted with its components h, k, and l relative to the lattice vectors ai , i.e. h = a1 · R and so forth. In order to arrive at the set of smallest possible integer numbers, the values possibly must be divided by a suitable fraction. Directions are denoted in square brackets [hkl], and go into the direction of ha1 + ka2 + la3 . A set of crystallographically equivalent directions ¯ is denoted with hkl. For negative indices, [−1 00] can also be written with a bar, [100]. A lattice plane is the set of all lattice points in a plane spanned by two independent lattice vectors R1 and R2 . Lattice planes are denoted as (hkl) with parentheses; a set of equivalent planes is denoted with curly brackets as {hkl}. The lattice points on that plane form a two-dimensional Bravais lattice. The entire lattice can be generated by shifting the lattice plane along its normal n = (R1 × R2 )/|R1 × R2 |. The plane belongs to the reciprocal lattice vector Gn = 2π n/d, d being the distance between planes. This correspondence between reciprocal lattice vectors and sets of planes allows the orientation of planes to be described in a simple manner. The shortest reciprocal lattice vector perpendicular to the plane is used. The coordinates with respect to the primitive translation vectors of the reciprocal space bi form a triplet of integer numbers and are called Miller indices of the plane, i.e. Gn = h b1 + k b2 +l b3 . The plane described by Gn ·r = A fulfills the condition for a suitable value of A. The plane intersects the axes ai at the points x1 a1 , x2 a2 and x3 a3 . Thus we find Gn xi ai = A for all i. From (3.18) follows Gn · a1 = 2π h, Gn · a2 = 2π k and Gn · a3 = 2π l, where h, k and l are integers. The Miller indices (hkl) are thus proportional to the reciprocal values 1/xi of the axis intersections of the plane with the lattice vectors of the direct lattice. An example is shown in Fig. 3.34.

58

3 Crystals

Fig. 3.34 The plane intersects the axes at 3, 2, and 2. The inverse of these numbers is 1/3, 1/2, and 1/2. The smallest integer numbers of this ratio form the Miller indices (233)

Fig. 3.35 a Miller indices of important planes for the simple cubic (and fcc, bcc) lattice. (b) Directions within three low index planes of cubic crystals

(a)

(001)

(110)

[110] [010]

[110]

[111]

[001] [112] [111]

[100]

[100]

[110]

[110]

[110] [001]

[110]

[111]

(b)

[001]

[111]

(111) [112] [121]

[211]

[110] [211]

[110] [112]

[121]

In a cubic lattice, the faces of the cubic unit cell are {001} and the planes perpendicular to the area (body) diagonals are {110} ({111}) (Fig. 3.35a). For example, in the simple cubic lattice (100), (010), (001), (−1 00), (0−1 0) are (00−1 ) equivalent and are denoted by {100}. In the zincblende lattice, the {111} planes consist of diatomic planes with Zn and S atoms. It depends on the direction whether the metal or the nonmetal is on top. These two cases are denoted by A and B. We follow the convention that the (111) plane is (111)A and the metal is on top (as in Fig. 3.16b). For ¯ each change of sign the type changes from A to B and vice versa, e.g. (111)A, (11¯ 1)B and (1¯ 1¯ 1)B. In Fig. 3.35b the in-plane directions for the (001), (110) and (111) planes are visualized. We note that for orthogonal lattices, the (outward) normal direction of a plane (hkl) is the same direction as [hkl]. Caveat: in non-rectangular lattices this is not the case! This can be easily seen for a monoclinic lattice, depicted as example in Fig. 3.36.

3.6 Reciprocal Lattice

59

Fig. 3.36 Sketch of lattice directions and planes in a monoclinic lattice. The [100] direction and the normal of the (100) plane are not parallel

Fig. 3.37 (a, b) Miller indices for the wurtzite (or hcp) structure. (c) Orientation of the a-, r-, m-, and c-plane in the wurtzite structure (00.1) [2110] [1100] [1210] [1010] [0110] [1120] [1120] [0110] [1010] [1210] [1100] [2110]

(b)

(a)

a

(c)

r

m

c

In the wurtzite lattice, the Miller indices are denoted as [hklm] (Fig. 3.37). Within the (0001) plane three indices hkl are used that are related to the three vectors a1 , a2 and a3 (see Fig. 3.37a) rotated with respect to each other by 120◦ . Of course, the four indices are not independent and l = −(h + k). The third (redundant) index can be denoted as a dot. The c-axis [0001] is then denoted as [00.1]. Wurtzite (and trigonal, e.g. sapphire) substrates are available typically with (polished) a (11.0), m (01.0) and r (01.2), c (00.1) surfaces (Fig. 3.37b). The distance of lattice planes d = 2π/|G| can be expressed via the Miller indices for cubic (3.21a), tetragonal (3.21b) and hexagonal (3.21c) crystals as c = √ dhkl t dhkl = h dhkl =

a h2

+ k2 + l2 a

h 2 + k 2 + l 2 (a/c)2 a 4 (h 2 + hk + k 2 )/3 + l 2 (a/c)2

(3.21a) (3.21b) (3.21c)

Useful formulas for the angle θ between a [hk.l]-plane and the [00.1]-direction in the cubic, tetragonal and wurtzite structures are: cos θ c = √

l h2 + k2 + l 2

(3.22a)

60

3 Crystals

Table 3.6 High symmetry points and directions from -point in the Brillouin zone of the fcc lattice Point

k ( 2aπ )

X K L W U

(0, 0, 0) (0, 1, 0) 3/4 (1, 1, 0) 1/2 (1, 1, 1) (1, 1/2, 0) (1, 1/4, 1/4)

Direction

Multiplicity 1 6 12 8 24 24

Table 3.7 High symmetry points and directions from -point in the Brillouin zone of the hcp lattice Point

k (2 π )

Direction

Multiplicity

A L

(0, 0, 0) (0, 0, 21c ) (0, √1 , 21c )

1 2 12

M

(0,

6

H K

3a √1 , 0) 3a (− 31a , √1 , 21c ) 3a (− 31a , √1 , 0) 3a

cos θ t = l2 + cos θ h = l2 +

12 T

6

l

(3.22b)

c2 (h 2 a2

+ k2) l

4 c2 3 a2

(h 2 + h k + k 2 )

.

(3.22c)

3.6.3 Brillouin Zone The Wigner–Seitz cell in reciprocal space is called the (first) Brillouin zone. In Fig. 3.38, the Brillouin zones for the most important lattices are shown. High symmetry points in the Brillouin zone are labeled with dedicated letters. The point always denotes k = 0 (zone center). High symmetry paths in the Brillouin zone are labeled with dedicated Greek symbols. In the Brillouin zone of the fcc lattice (Si, Ge, GaAs, ...) the X point denotes the point at the √ zone 2a boundary in 001-directions (at distance 2 π/a from ), K for 110-directions (at distance 3 π/ √ from ) and L for the 111-directions (at distance 3 π/a from ) (see Table 3.6). The straight paths from to X, K, and L are denoted as , , and , respectively. High symmetry points and directions of the Brillouin zone of the hcp lattice are given in Table 3.7.

3.7 Alloys When different semiconductors are mixed various cases can occur: • The semiconductors are not miscible and have a so-called miscibility gap. They will tend to form clusters that build up the crystal. The formation of defects is probable.

3.7 Alloys

61 kz

kz

X X

W R

L U

S T M

kx

Z

X

ky

K

kx

(a)

ky

(b) H

kz

P

kx

K

H L

P

ky

N

G

H

F

D

L R A

S

M

U

P

T M

H

(c)

S' H

T'

K

A

(d)

L

H

kz

X

Z

T

T

U Y

N

X

(e)

ky

S

(f)kx

Fig. 3.38 Brillouin zones and special k points for the a primitive cubic (pc), (b) fcc, c bcc, and d hcp lattice. e Brillouin zone for chalcopyrite structure with fcc Brillouin zone shown as dashed outline f Brillouin zone for orthorhombic lattice with one quadrant shown with dashed lines

• They form an ordered (periodic) structure that is called a superlattice. • They form a random alloy.

3.7.1 Random Alloys Alloys for which the probability to find an atom at a given lattice site is given by the fraction of these atoms (i.e. the stoichiometry), independent of the surrounding, are called random alloys. Deviations from the random population of sites is termed clustering.

62

3 Crystals

For a Gex Si1−x alloy this means that any given atom site has the probability x to have a Ge atom and 1 − x to have a Si atom. The probability pn that a Si atom has n next-neighbor Ge atoms is pn =

4 n x (1 − x)4−n , n

(3.23)

and is depicted in Fig. 3.39 as a function of the alloy composition. The symmetry of the Si atom is listed in Table 3.8. If it is surrounded by four of the same atoms (either Ge or Si), the symmetry is Td . If one atom is different from the other three next neighbors, the symmetry is reduced to C3v since one bond is singled out. For two atoms each the symmetry is lowest (C2v ). In an alloy from binary compound semiconductors such as Alx Ga1−x As the mixing of the Al and Ga metal atoms occurs only on the metal (fcc) sublattice. Each As atom is bonded to four metal atoms. The probability that it is surrounded by n Al atoms is given by (3.23). The local symmetry of the As atom is also given by Table 3.8. For AlAsx P1−x the mixing occurs on the nonmetal (anion) sublattice. ¯ surface (UHV If the alloy contains three atom species it is called a ternary alloy. In Fig. 3.40 the (110) cleave) of an In0.05 Ga0.95 As alloy is shown. Indium atoms in the first layer show up as brighter round dots [247]. Along the [001]-direction the positions are uncorrelated, along [110] an anti-correlation is

Fig. 3.39 Probability that a Si atom has n next-neighbor Ge atoms in a random Gex Si1−x alloy

¯ surface of an MBE-grown In0.05 Ga0.95 As alloy Fig. 3.40 a STM empty-state image (17.5 × 17.5 nm2 ) of the (110) on GaAs, b curvature-enhanced image. c Schematic atomic arrangement of the first and second atomic layer. Adapted from [248]

3.7 Alloys

63

Table 3.8 Probability pn (3.23) and symmetry of an A atom being surrounded by n B atoms in a tetrahedrally configured Bx A1−x random alloy n

pn

Symmetry

0 1 2 3 4

x4 4 x 3 (1 − x) 6 x 2 (1 − x)2 4 x (1 − x)3 (1 − x)4

Td C3v C2v C3v Td

found, corresponding to an effective repulsive pair interaction energy of 0.1 eV for the nearest neighbor In–In pairs along the [110]-direction due to strain effects [248]. If the binary end components have different crystal structure, the alloy shows a transition (or compositional transition range) from one structure to the other at a particular concentration. An example is the alloy between wurtzite ZnO and rocksalt MgO. Mgx Zn1−x O alloy thin films exhibits wurtzite structure up to about x = 0.5 and rocksalt structure for x > 0.6 [249] (cmp. Fig. 3.43). If the alloy contains four atom species it is called quaternary. A quaternary zincblende alloy can have the mixing of three atom species on one sublattice, such as Alx Ga y In1−x−y As or GaAsx P y Sb1−x−y or the mixing of two atom species on both of the two sublattices, such as Inx Ga1−x As y N1−y . The random placement of different atoms on the (sub)lattice in an alloy represents a perturbation of the ideal lattice and causes additional scattering (alloy scattering). In the context of cluster formation, the probability of an atom having a direct neighbor of the same kind on its sublattice is important. Given a Ax B1−x C alloy, the probability pS to find a single A atom surrounded by B atoms is given by (3.24a). The probability pD1 to find a cluster of two neighbored A atoms surrounded by B atoms is given by (3.24b). pS = (1 − x)12 pD1 = 12 x (1 − x)18 .

(3.24a) (3.24b)

These formulas are valid for fcc and hcp lattices. For larger clusters [250, 251], probabilities in fcc and hcp structures differ.

3.7.2 Phase Diagram The mixture Ax B1−x with average composition x between two materials A and B can result in a single phase (alloy), a two-phase system (phase separation) or a metastable system. The molar free enthalpy G of the mixed system is approximated by G = x (1 − x) + kT [x ln(x) + (1 − x) ln(1 − x)] .

(3.25)

The first term on the right-hand side of (3.25) is the (regular solution) enthalpy of mixing with the interaction parameter , which can depend on x. The second term is the ideal configurational entropy based on a random distribution of the atoms. The function is shown for various ratios of kT / in Fig. 3.41a. In an equilibrium phase diagram (see Fig. 3.41b) the system is above the binodal curve in one phase (miscible). On the binodal line Tb (x) in the (x, T ) diagram the A- and B-rich disordered phases have equal chemical potentials, i.e. ∂G/∂ x = 0. For independent of x the temperature Tb

64

3 Crystals

is given by (3.26a). A critical point is at the maximum temperature Tmg and concentration xmg of the miscibility gap. For independent of x it is given by Tmg = /2 and xmg = 1/2. In the region below the spinodal boundary, the system is immiscible and phases immediately segregate (by spinodal decomposition). On the spinodal line Tsp (x) the condition ∂ 2 G/∂ x 2 = 0 is fulfilled. For independent of x the temperature Tsp is given by (3.26b). The region between the binodal and spinodal curves is the metastable region, i.e. the system is stable to small fluctuations of concentration or temperature but not for larger ones. 2x − 1 ln(x) − ln(1 − x) kTsp (x) = 2 x (1 − x) . kTb (x) =

(3.26a) (3.26b)

In Fig. 3.42 calculated diagrams for GaAs-AlAs and GaAs-GaP [252] are shown. The arrows denote the critical point. These parameters and the interaction parameters for a number of ternary alloys are given in Table 3.9. For example, for Alx Ga1−x As complete miscibility is possible for typical growth temperatures (> 700 K), but for Inx Ga1−x N the In solubility at a typical growth temperature of 1100 K is only 6% [253]. The alloy system (Al,Ga,In)(As,P,Sb) always crystallizes in the zincblende structure and (Al,Ga,In)N always in the wurtzite structure. If the binary end components of a ternary alloy have a different crystal structure things become more complicated and the crystal phase has to be determined experimentally (and modelled) for each composition. As an example the energy of the wurtzite, hexagonal and rocksalt

(a)

(b)

Fig. 3.41 a Free enthalpy G of mixed binary system (3.25) in units of for =const. and various values of kT / as labeled. b Schematic phase diagram for binary mixture. The temperature is given in units of /k. The solid (dashed) line denotes the binodal (spinodal) line 100

350

(a)

AlxGa1-xAs

90 80

(b)

250

70

binodal

200

60

150

spinodal

50 40 GaAs

GaPxAs1-x

300

x=0.5

AlAs

100 GaAs

x=0.5

GaP

Fig. 3.42 Calculated phase diagrams for a Alx Ga1−x As and b GaPx As1−x . The binodal (spinodal) curve is shown as solid (dashed) line. Adapted from [252]

3.7 Alloys

65

Table 3.9 Calculated interaction parameter (x) (at T = 800 K, 1 kcal/mol= 43.39 meV), miscibility-gap temperature Tmg and concentration xmg for various ternary alloys. Data for (In,Ga)N from [253], other data from [252] Alloy

Tmg (K)

xmg

(0) (kcal/mol)

(0.5) (kcal/mol)

(1) (kcal/mol)

Alx Ga1−x As GaPx As1−x Gax In1−x P GaSbx As1−x Hgx Cd1−x Te Znx Hg1−x Te Znx Cd1−x As Inx Ga1−x N

64 277 961 1080 84 455 605 1505

0.51 0.603 0.676 0.405 0.40 0.56 0.623 0.50

0.30 0.53 2.92 4.51 0.45 2.13 2.24 6.32

0.30 0.86 3.07 3.96 0.80 1.88 2.29 5.98

0.30 1.07 4.60 3.78 0.31 2.15 2.87 5.63

1.0 0.6

0.9 0.8

0.5

0.7

Energy (eV)

Mg-concentration x

Fig. 3.43 Calculated energy vs. volume of the formula unit for Mgx Zn1−x O in the wurtzite (WZ), hexagonal (HX) and rocksalt phase (RS). The separations between the three phase are denoted by straight bold lines. Adapted from [254]

0.4

0.6 0.5

0.3

0.4

0.2

0.3 0.2

0.1

0.1 0

18

20 24 22 Volume (Å3)

26

0

structure of Mgx Zn1−x O has been calculated [254] as depicted in Fig. 3.43 (cmp. Fig. 2.4 for silicon). The transition between wurtzite and rocksalt structure is predicted for x = 0.33.

3.7.3 Virtual Crystal Approximation In the virtual crystal approximation (VCA) the disordered alloy ABx C1−x is replaced by an ordered binary compound AD with D being a ‘pseudoatom’ with properties that are configuration averaged over the properties of the B and C atoms, e.g. their masses or charges. Such an average is weighted with the ternary composition, e.g. the mass is MD = x MB + (1 − x)MC . For example, the A–D force constant would be taken as the weighted average over the A–B and A–C force constants.

3.7.4 Lattice Parameter In the VCA for an alloy a new sort of effective atom is assumed that has an averaged bond length that depends linearly on the composition. Typically, Vegard’s law (3.27), which predicts that the lattice constant of a ternary alloy Ax B1−x C depends linearly on the lattice constants of the binary alloys AC

66

3 Crystals

(a)

(b)

√ Fig. 3.44 a Near-neighbor distance ( 3 a0 /4) of Inx Ga1−x As as measured by standard X-ray diffraction (Bragg reflection, solid squares) and VCA approximation (dash-dotted line). Near-neighbor Ga–As and In–As distances as determined by EXAFS (extended X-ray absorption fine structure, solid squares). Dashed lines are guides to the eye. Data from [255]. b Second-neighbor distances for Inx Ga1−x As as determined from EXAFS, top: anion–anion distance√(for As–As), bottom: cation–cation distance (for In–In, Ga–Ga, and Ga–In). Solid lines in both plots are the VCA (a0 / 2). Data from [256] Fig. 3.45 Theoretical values (T = 0 K) for the cell-internal parameter u as a function of the composition for group-III nitride alloys. The solid lines are quadratic curves (bowing parameter b is shown) through the points for x = 0, 0.5, and 1.0. Data from [257]

and BC, is indeed fulfilled a0 (Ax B1−x C) = a0 (BC) + x [a0 (AC) − a0 (BC)] .

(3.27)

In reality, the bond length of the AC and BC bonds changes rather little (Fig. 3.44a) such that the atoms in the alloy suffer a displacement from their average position and the lattice is deformed on the nanoscopic scale. In a lattice of the type Inx Ga1−x As the anions suffer the largest displacement since their position adjusts to the local cation environment. For Inx Ga1−x As a bimodal distribution, according to the As–Ga–As and As–In–As configurations, is observed (Fig. 3.44b). The cation–cation second-neighbor distances are fairly close to the VCA. While the average lattice parameter in alloys changes linearly with composition, the cell-internal parameter u (for wurtzite structures, see Sect. 3.4.5) exhibits a nonlinear behavior as shown in Fig. 3.45.

3.7 Alloys

67

Fig. 3.46 CuPt-ordered ternary alloy In0.5 Ga0.5 P; the lattice symmetry is reduced from Td to C3v

Ga In P Td

(a)

C3v

(b)

Fig. 3.47 (a) Cross-sectional transmission electron microscope image along the [110] zone axis of a Cd0.68 Zn0.32 Te epilayer on GaAs showing ordered domains having a doublet periodicity on the {111} and {001} lattice planes. Two different {111} variants are labeled ‘a’ and ‘b’. The doublet periodicity in the [001] is seen in the ‘c’ region. (b) Selectedarea diffraction pattern along the [110] zone. Strong peaks are fundamental peaks of the zincblende crystal, weak peaks are due to CuPt ordering, labeled A and B, and CuAu-I ordering, labeled C and D. The latter are the weakest due to a small volume fraction of CuAu-ordered domains. Adapted from [259]

Therefore physical properties connected to u, such as the spontaneous polarization, will exhibit a bowing.

3.7.5 Ordering Some alloys have the tendency for the formation of a superstructure [258]. Growth kinetics at the surface can lead to specific adatom incorporation leading to ordering. For example, in In0.5 Ga0.5 P the In and Ga atoms can be ordered in subsequent (111) planes (CuPt structure) instead of being randomly mixed (Fig. 3.46). This impacts fundamental properties such as the phonon spectrum or the band gap. ¯ ¯ planes CuPtB ordering. In ¯ planes is called CuPtA , on (111) and (111) CuPt ordering on (111) and (1¯ 11)

68

3 Crystals [001] [110]

(a)

Cd Zn Se

(b)

(c)

Fig. 3.48 Schematic diagrams of zincblende Cdx Zn1−x Te along [110] with (a) CuAu-I type ordering and (b, c) two ¯ ¯ and (c) [111]. ¯ types of the CuPtB type ordering. Doublet periodicity is along (a) [001] and [110], (b) [111] Adapted from [259]

Fig. 3.47, a TEM image of a Cd0.68 Zn0.32 Te epilayer is shown with simultaneous ordering in the CuPt ¯ and [111]) ¯ structure (doublet periodicity along [111] and in the CuAu-I structure7 (doublet periodicity ¯ along [001] and [110]).

7 The

CuAu-I structure has tetragonal symmetry. There exists also the CuAu-II structure that is orthorhombic.

Chapter 4

Structural Defects

Crystals are like people: it is the defects in them which tend to make them interesting! C.J. Humphreys, 1979 [260]

Abstract No crystal is perfect. Various point defects and their thermodynamics, diffusion and distribution of defects are discussed. Also dislocations and extended defects such as cracks, stacking faults, grain boundaries and antiphase domains are covered.

4.1 Introduction In an ideal lattice each atom is at its designated position. Deviations from the ideal structure are called defects. In the following, we will briefly discuss the most common defects. The electrical activity of defects will be discussed in Sects. 7.5 and 7.7. For the creation (formation) of a defect a certain free enthalpy G fD is necessary. At thermodynamical equilibrium a (point) defect density ∝ exp(−G fD /kT ) will always be present (cf. Sect. 4.2.2). Point defects (Sect. 4.2) are deviations from the ideal structure involving essentially only one lattice point. The formation energy for line defects (Sect. 4.3) or area defects (Sect. 4.4) scales with N 1/3 and N 2/3 , respectively, N being the number of atoms in the crystal. Therefore, these defects are not expected in thermodynamic equilibrium. However, the path into thermodynamical equilibrium might be so slow that these defects are metastable and must be considered quasi-frozen. There may also exist metastable point defects. By annealing the crystal, the thermodynamic equilibrium concentration might be re-established. The unavoidable two-dimensional defect of the bulk structure is the surface, discussed in Chap. 11.

4.2 Point Defects 4.2.1 Point Defect Types The simplest point defect is a vacancy V, a missing atom at a given atomic position. If an atom is at a position that does not belong to the crystal structure an interstitial I (or Frenkel defect) is formed. © Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_4

69

70

4 Structural Defects

Fig. 4.1 Images of occupied (upper frames) and empty (lower frames) density of states of typical defects on Si-doped GaAs (110) surfaces. (a1, a2) show a Ga vacancy, (b1, b2) a SiGa donor, (c1, c2) a SiAs acceptor and (d1, d2) a SiGa –VGa complex. Adapted from [261]

Depending on the position of the interstitial different types are distinguished. An interstitial atom that has the same chemical species as the crystal is called ‘self-interstitial’. If an atom site is populated with an atom of different order number Z , an impurity is present. An impurity can also sit on interstitial position. If the number of valence electrons is the same as for the original (or correct) atom, then it is an isovalent impurity and quasi fits into the bonding scheme. If the valence is different, the impurity adds extra (negative or positive) charge to the crystal bonds, which is compensated by the extra, locally fixed charge in the nucleus. This mechanism will be discussed in detail in the context of doping (Chap. 7). If in an AB compound an A atom sits on the B site, the defect is called an antisite defect A B . A Ga vacancy, a silicon impurity atom on Ga- and As-site and a SiGa -vacancy complex at the (110) surface of Si doped GaAs are shown in Fig. 4.1 as observed with STM [261, 262]. Also antisite defects in GaAs can be observed with STM [263, 264]. A point defect is typically accompanied by a relaxation of the surrounding host atoms. As an example, we discuss the vacancy in Si (Fig. 4.2a). The missing atom leads to a lattice relaxation with the next neighbors moving some way into the void (Fig. 4.2b). The bond lengths of the next and secondnext neighbor Si atoms around the neutral vacancy are shown in Fig. 4.2c. The lattice relaxation depends on the charge state of the point defect (Jahn–Teller effect) which is discussed in more detail in Sect. 7.7. In Fig. 4.2d the situation for the positively charged vacancy with one electron missing is shown. One of the two bonds is weakened since it lacks an electron. The distortion is therefore different from that for V 0 . Also the (self-)interstitial is accompanied with a lattice relaxation as shown in Fig. 4.3 for a silicon interstitial at tetrahedral place. Self-interstitials in silicon and germanium are reviewed and compared in [265] for their various charge states.

4.2.2 Thermodynamics For a given temperature, the free enthalpy G of a crystal (a closed system with regard to particle exchange) G = H −TS (4.1) is minimum. H is the enthalpy and S the entropy. The enthalpy H = E + pV is the thermodynamic potential for a system whose only external parameter is the volume V . It is used when the independent variables of the system are the entropy S and pressure p. The free enthalpy is used when the independent parameters are T and p. G 0 (H0 ) is the free energy (enthalpy) of the perfect crystal. H f is the formation

4.2 Point Defects

71

(a)

(b)

(c)

(d)

Fig. 4.2 (a) Schematic diamond lattice with vacancy, i.e. a missing Si atom without relaxation. (b) Si with neutral vacancy (V 0 ), lattice relaxation and formation of two new bonds. (c) Schematic diagram showing the (inward) relaxation of the neighbors around the neutral Si vacancy defect site (empty circle) calculated by an ab initio method. The distances of the outer shell of atoms (red circles) from the vacant site is labeled (in nm). The bond lengths of the two new bonds and the second-neighbor (blue circles) distance are also indicated. The bond length in bulk Si is 0.2352 nm, the secondneighbor distance 0.3840 nm. Adapted from [266]. (d) Si unit cell with positively charged vacancy (V + ). Parts (a, b, d) reprinted with permission from [267] Fig. 4.3 Silicon tetrahedral interstitial SiTi and its next atoms in ideal (white spheres) and relaxed (black spheres) position. Adapted from [175]

enthalpy of an isolated defect. This could be, e.g., the enthalpy of a vacancy, created by bringing an atom from the (later) vacancy site to the surface, or an interstitial, created by bringing an atom from the surface to the interstitial site. In the limit that the n defects do not interact with each other, i.e. their concentration is sufficiently small, they can be considered independent and the enthalpy is given by H = H0 + n H f .

(4.2)

The increase of entropy due to increased disorder is split into the configurational disorder over the possible sites, denoted as S d , and the formation entropy Sf due to localized vibrational modes. The total change G of the free energy is

72

4 Structural Defects

Table 4.1 Formation enthalpy H f and entropy S f of the interstitial (I ) and vacancy (V ) in Si and the Ga vacancy in GaAs. Data for Si from [268, 269], for GaAs from [270] Material

Defect

H f (eV)

S f (kB )

Si Si GaAs

I V VGa

3.2 2.8 3.2

4.1 ∼1 9.6

G = G − G 0 = n (H f − T S f ) − T S d = n G f − T S d ,

(4.3)

where G f = H f − T S f denotes the free enthalpy of formation of a single isolated defect. In Table 4.1 experimental values for the formation entropy and enthalpy are given for several defects. Surprisingly, despite their fundamental importance in semiconductor defect physics, these numbers are not very well known and disputed in the literature. The defect concentration is obtained by minimizing G, i.e. ∂ Sd ∂G = Gf − T =0. ∂n ∂n

(4.4)

The entropy S d due to disorder is given as S d = kB ln W ,

(4.5)

where W is the complexion number, usually the number of distinguishable ways to distribute n defects on N lattice sites N! N . (4.6) W = = n n! (N − n)! With Stirling’s formula ln x! ≈ x(ln x − 1) for large x we obtain N N N −n ∂ Sd = kB ln + ln . ∂n n N −n n

(4.7)

If n N , ∂ N /∂n = 0 and the right side of (4.7) reduces to kB ln(N /n). The condition (4.4) reads G f + kB T ln(n/N ), or Gf n = exp − . (4.8) N kT In the case of several different defects i with a degeneracy Z i , e.g. a spin degree of freedom or several equivalent configurations, (4.8) can be generalized to G if ni . = exp − Zi N kT

(4.9)

eq

In [271] the equilibrium concentration of interstitials C I in silicon has been given as 3.8 eV eq C I = 1.0 × 1027 cm−3 exp − , kT

(4.10)

4.2 Point Defects

73

about 1014 cm−3 at 1200 ◦ C. The vacancy concentration has been investigated in [272]. Around a temperature of 1200 ◦ C it is in the 1014 –1015 cm−3 range. Due to the reaction 0 I +V ,

(4.11)

a mass action law holds for the concentrations of interstitials and vacancies eq

eq

C I CV = C I CV .

(4.12)

4.2.3 Diffusion The diffusion of point defects is technologically very important, in particular for silicon as host material. Typically a dopant profile should be stable under following technological processing steps and also during device performance. Also defect annihilation is crucial after implantation processes. Diffusion of an interstitial I and a vacancy V to the same site is prerequisite for recombination of defects (so called bulk process) according to the scheme I + V → 0. We note that the process 0 → I + V is called Frenkel pair process.1 Also the self-diffusion of silicon has been studied, e.g. using radioactively marked isotopes [271]. The diffusion of point defects including dopants in silicon has been reviewed in [273, 274]. Usually Fick’s law is applied, stating how the flux J depends on the concentration gradient, for an interstitial it reads: (4.13) JI = −D I ∇C I , D I being the interstitial diffusion coefficient. For interstitials in Si it was found [271] that 1.2 eV D I = 0.2 exp − cm2 /s . kT

(4.14)

The diffusion of neutral vacancies occurs with [275] 0.45 eV cm2 /s . DV = 0.0012 exp − kT

(4.15)

The temperature dependent diffusion coefficients of point defects and dopants in silicon are shown in Fig. 4.4. The self-diffusion coefficient of silicon has been determined from the annealing of isotope superlattices (Sect. 12.5) of sequence 28 Sin /30 Sin , n = 20 to be [276] 3.6 eV 4.95 eV SD + 0.0023 exp − cm2 /s , = 2175.4 exp − DSi kT kT

(4.16)

the first (second) term being due to interstitial (vacancy) mechanism, dominant for temperatures larger (smaller) than 900 ◦ C. The enthalpy in the exponent, e.g. HV = 3.6+0.3 −0.1 eV [276], consists of the formation and migration enthalpies, (4.17) HV = HVf + HVm .

1 At higher temperatures a silicon atom can occasionally acquire sufficient energy from lattice vibrations to leave its lattice site and thus an interstitial and a vacancy are generated.

74

4 Structural Defects

Fig. 4.4 The temperature dependent diffusion coefficient of Si interstitials I , vacancies V and various impurities in silicon. Also the self-diffusion coefficient, labeled with ‘Si’ is shown. Based on data from [273]

(d)

(e)

Fig. 4.5 Configurations of boron in Si: (a) Substitutional boron and Si self-interstitial at ‘T’ site (BS –SiTi ). Interstitial T boron at (b) ‘H’ (BH i ) and (c) ‘T’ site (Bi ), each with the Si atoms on the Si lattice sites. The large bright ball represents the boron atom, large and small dark balls represent Si atoms. (d) Lowest energy barrier diffusion paths for positively charged and neutral B–Si states, total energy vs. configuration. (e) Two diffusion pathways for positively charged B–Si, kick-out (dashed line) and pair diffusion (solid line); the activation energy is labeled. Adapted from [279]

Using the experimental value HVf = 2.8 ± 0.3 eV [269] from Table 4.1, for the migration enthalpy a value around HVm ≈ 0.8 eV is obtained. As an example for a dopant diffusion process that has been understood microscopically, we discuss here boron in silicon. In Fig. 4.5a the lowest-energy configuration of a boron-related defect in silicon is depicted, Bs –SiTi , i.e. boron on a substitutional site and a self-interstitial Si on the ‘T’ place with highest symmetry2 (see Fig. 3.18). Due to its importance as an acceptor in Si, the configuration and diffusion 2 The positive charge state is stable, the neutral charge state is metastable since the defect is a negative-U center (see Sect. 7.7.5).

4.2 Point Defects

75

of B in Si has found great interest [277–279]. The diffusion depends on the charge state of boron. The diffusion of positively charged boron has been suggested [279] to occur via the following route: The boron leaves its substitutional site and goes to the hexagonal site (‘H’) (Fig. 4.5b) with an activation energy of about 1 eV (Fig. 4.5d). It can then relax (∼ 0.1 eV) without barrier to the tetrahedral ‘T’ →BT+ has a higher activation energy of 1.12 eV position (Fig. 4.5c). The direct migration Bs –SiT+ i i and is thus unlikely. The boron atom can then diffuse through the crystal by going from ‘H’ to ‘T’ to ‘H’ and so on (Fig. 4.5e). However, long-range diffusion seems to be not possible in this way because the kick-in mechanism will bring back the boron to its stable configuration. The pair diffusion mechanism T for neutral boron Bs –SiTi →BH i →Bs –Sii via the hexagonal site has an activation energy of about T 0.5 eV (Fig. 4.5d) while the path via Bi has a larger 0.9 eV barrier. The concentration dependence of the diffusion mechanism has been discussed in [280]. Similarly, indium diffusion in silicon has been investigated suggesting a minimum energy Ins – SiTi →InTi →Ins –SiTi diffusion pathway via the tetrahedral site with 0.8 eV activation energy [281]. Microscopic modeling has been reported also for diffusion of phosphorus [282].

4.2.4 Dopant Distribution The introduction of impurities into a semiconductor (or other materials such as glasses) is termed doping. The unavoidable incorporation of impurities in the nominally pure (nominally undoped) material is called unintentional doping and leads to a residual or background impurity concentration. Several methods are used for doping and the creation of particular doping profiles (in depth or lateral). All doping profiles underly subsequent diffusion of dopants (Sect. 4.2.3). Various methods of doping are used. A straightforward method of doping is the incorporation during crystal growth or epitaxy. For semiconductor wafers a homogeneous doping concentration is targeted, both laterally and along the rod from which the wafer is cut (Sect. 12.2.2). When a crystal is grown from melt, containing a concentration c0 of the impurity, the concentration in the solid is given by (‘normal freezing’ case [283–285])3 c(x) = c0 k (1 − x)k−1 ,

(4.18)

where c(x) is the impurity concentration in the crystal at the freezing interface, x is the frozen melt fraction (ratio of solid mass to total mass, 0 ≤ x ≤ 1). k is the distribution coefficient (or segregation coefficient) which is the fraction of impurities that is built into the crystal at the liquid–solid interface. Since the melt volume reduces during the solidification, the impurity concentration rises over time. For small distribution coefficients (4.18) can be approximated to c(x) ≈ c0

k , 1−x

(4.19)

An experimental example for Ge:In is shown in Fig. 4.6a. In Table 4.2 the distribution coefficients for various impurities in Si, Ge and GaAs is given. The modification of distribution coefficients in SiGe alloys is discussed in [286]. Equilibrium values (keq ) are obtained for ‘slow’ crystal growth. For finite growth rates, k becomes a function of the growth rate x m (1−x)+ 0

c(x ) dx = c0 , where cm is the (remaining) concentration in the melt. At the beginning cm (0) = c0 . At the interface c(x) = k cm (x). Putting this into the mass preservation, building c (x) and solving the resulting differential equation c = c(1 − k)/(1 − x) with c(0) = k c0 leads to (4.18).

3 Mass preservation of the impurities can be written at any time c

76

4 Structural Defects

(b)

(a)

Fig. 4.6 (a) Relative concentration of indium along a CZ-grown germanium crystal. Absolute concentration is in the 1016 cm−3 range. Solid line follows (4.19) with k = 1.2 × 10−3 . Symbols are experimental data from [288]. (b) Impurity distribution (relative concentration c(x)/c0 ) for CZ (4.18) (solid lines) and FZ (4.20) (dashed lines, z = 0.01) silicon crystals for B (blue), P (red), and Al (green). Distribution coefficients have been taken from Table 4.2. Note crossing of B and P lines and possibly associated change from p-type to n-type (cmp. Fig. 1.7) Table 4.2 Equilibrium distribution coefficients (at melting point) of various impurities in silicon, germanium and GaAs. Data for Si from [285, 287], for Ge from [164, 288–290] and for GaAs from [164] Impurity

Si

Ge

GaAs

C Si Ge N O B Al Ga In P As Sb S Fe Ni Cu Ag Au Zn

0.07

> 1.85 5.5

0.8 0.1 0.03

0.33 7 × 10−4 ≈1 0.8 2.8 × 10−3 8 × 10−3 4 × 10−4 0.35 0.3 0.023 10−5 6.4 × 10−6 ≈ 3 × 10−5 8 × 10−4 ≈ 1 × 10−6 2.5 × 10−5 2.5 × 10−5

0.3 12.2 0.1 0.087 1.2 × 10−3 0.12 0.04 3.3 × 10−3 > 5 × 10−5 3 × 10−5 2.3 × 10−6 1.3 × 10−5 10−4 1.5 × 10−5 6 × 10−4

3 0.1 2 < 0.02 0.3 2 × 10−3 6 × 10−4 2 × 10−3 0.1 0.1

and is then called the effective distribution coefficient. For k < 1, keff > keq . keff approaches 1 for high growth rates, i.e. all impurities at the rapidly moving interface are incorporated. Equation (4.18) applies to Czrochalski growth where the crystal is pulled out of the melt [291]. In float-zone (FZ) growth [291] a polycrystalline rod is transformed into a crystalline one while a

4.2 Point Defects

(a)

77

(b)

Fig. 4.7 (a) Depth of peak concentration of boron implanted in silicon for various acceleration voltages U . Data from various sources, for U < 1 keV from [299]. Dashed line is linear dependence. (b) Simulated depth profiles of impurity concentration for B, P, As, and Sb implanted into crystalline silicon with U = 100 keV and a dose of 1015 cm−2 . Adapted from [300]

RF-heated and liquid ‘float’ zone is moved through the crystal. In this case the impurity distribution is given by4 kx , (4.20) c(x) = c0 1 − (1 − k) exp − z where x is the ratio of the crystal mass to the total mass, i.e. crystal, liquid and feed rod. z is the relative mass of the (liquid) float zone, i.e. the ratio of liquid mass to the total mass. The impurity distribution for CZ and FZ crystals is compared in Fig. 4.6b. Obviously the FZ process can create much more homogeneous profiles.5 Using epitaxy arbitrary doping profiles along the growth directions can be created by varying the impurity supply during growth. Impurities can be introduced through the surface of the material by diffusion from a solid or gas phase. In ion implantation [292] the impurity atoms are accelerated towards the semiconductor and deposited with a certain depth profile due to multiple scattering and energy loss events, depending on the acceleration voltage (increasing deposition depth with increasing voltage, Fig. 4.7a) and ion mass (decreasing deposition depth with increasing mass, Fig. 4.7b). The depth profile is often investigated using secondary ion mass spectrometry (SIMS) [293, 294]. The profile also depends on the matrix material whose stopping power depends on its density and atomic mass. While an implantation depth of about 50 nm is reached for boron in silicon (A ≈ 28) for 10 keV, 20 keV are necessary in germanium (A ≈ 72.6) [295]. The mean path length6 dm depends also on the crystallographic direction (channeling effects, Fig. 4.8) [296]. A simulation of the interaction of ions and solids can be performed using the SRIM software [297, 298].

the float zone moves through the crystal, the change of mass of impurities m m = cm z in the liquid is m m = c0 − kcm . The first term stems from the melting of the polycrystalline part, the second from the solidification of the

= (c − kc )/z with c (0) = c and using c(x) = kc (x) yields crystal. Solving the resulting differential equation cm 0 m m 0 m (4.20). 5 We note that during directed solidification of Si:(B,P) a pn-junction forms due to the different distribution coefficients of boron and phosphorus. This has been used in [89]. 6 The mean path length is the distance integrated along the ion trajectory until its direction deviates by more than 4 ◦ from the incident direction. 4 When

78

4 Structural Defects 40

Fig. 4.8 Simulated mean path length as a function of implantation direction (azimuthal angle φ and polar angle θ) near [001] for 5 keV boron in silicon. The [001] channeling peak appears as a ridge at the left side of the plot (θ = 0, any value of φ). Adapted from [296]

B in Si

dm (nm)

30

[112] [101]

20 [111]

10

[114]

0 50 40 30 (°) 20

10 0

0

10

20

30 (°)

40

50

60

4.2.5 Large Concentration Effects 4.2.5.1

Lattice Constant

At high doping concentration, a noticeable effect on the lattice constant a0 is found. For silicon the atom density7 is NSi = 5×1022 cm−3 . A doping level of N = 1019 cm−3 corresponds thus to a dopant fraction of 0.02%. Such crystal could also be considered a very dilute alloy. About each (NSi /N )1/3 ≈ 17-th atom in a given direction is a dopant. The effect of high doping on the lattice constant is due to different ionic radius of the dopant and the hydrostatic deformation potential of the band edge occupied by the free carriers [301]. In a linear approach, the effect is summarized in the coefficient β via β=

1 a0 . N a0

(4.21)

The effect due to charge carriers on β is negative (positive) for p-doping (n-doping). Experimental data for Si, Ge, GaAs and GaP are compiled in [302, 303] and theoretically discussed. The effect is in the order of β = ±(1–10)×10−24 cm3 . For example, in the case of Si:B, the shrinkage of the lattice constant is mostly due to the charge carrier effect, for Si:P both effects almost cancel. In [304] it is shown that boron incorporation in silicon changes the lattice constant in various directions quite differently, e.g. d333 is shrunk by 0.4% for a doping level of 1019 cm−3 while the {620} lattice constant remains constant.

4.2.5.2

Clustering

Point defects can cluster, i.e. several point defects aggregate at neighboring sites. An example the configuration of five nearby vacancies in silicon, the so-called V5 cluster is shown in Fig. 4.9a. In [305] the ring-like hexavacancy in silicon is predicted a very stable defect. A large number of clustered vacancies is equivalent to a void. An example is depicted in Fig. 4.9b for an In2 O3 crystal which has locally ’decomposed’ into an indium particle and a void as revealed by TEM [306]. Also impurities can exhibit clustering.

7 eight

atoms per cubic unit cell of length a0 = 0.543 nm.

4.2 Point Defects

79

In2O3

[001] [110]

void

[110]

indium

(a)

(b)

Fig. 4.9 (a) Predicted configuration of the V5 -cluster (five vacancies) in silicon. Yellow spheres indicate more distorted atoms than the rest of the lattice atoms (white spheres). Adapted from [307]. (b) Indium particle with adjacent void embedded in In2 O3 (STEM image revealing Z -contrast in [001]). Adapted from [306] Fig. 4.10 Minimum energy path for the breakup of a B3 I2 cluster into B2 I and BI. Silicon (boron) atoms are shown as yellow (blue) spheres. Adapted from [310]

Typically a random distribution of dopants in the host is assumed (cmp. Sect. 3.7.1 on random alloys). The introduction of several impurities can lead to pairing effects, e.g. described for Se and B, Ga, Al or In in silicon [308]. A high concentration of a single impurity makes the existence of clusters, i.e. two or more neighboring dopant atoms, more probable. This effect has been extensively studied for B in Si [309], showing that several boron atoms with interstitials I form thermodynamically stable clusters, e.g. B3 I2 . This cluster forms from B2 I and BI with only 0.2 eV activation barrier [310] as shown in Fig. 4.10. The formation is limited by diffusion of the smaller clusters to the same site. The number of free carriers (here holes) released from such cluster is smaller than the number of boron atoms since it forms a deep acceptor [309]. This autocompensation mechanism is thus limiting the maximum achievable free carrier concentration due to doping and is technologically unfavorable. Reactions between boron atoms and silicon self-interstitials often lead to boron clustering in the peak region of an implantation profile and require detailed optimization of the annealing process [311].

80

4 Structural Defects

1022

Si

As P

-3

10

21

B

1020

Sb Li

1019

Ga Al

~Ei

-4

Cu

1018

Au

1017 10

Fe

16

0.01

0.1 i

(eV)

1.0

Fig. 4.11 Solubility limit for various impurities in silicon vs. their ionization energy. Adapted from [314] Table 4.3 Maximum solubility Ns of some impurities in silicon. Data for B, P, As, Sb from [313], other data from [316] Impurity

Ns (1020 cm−3 )

B P As Sb Al Cu Au Fe

4 5 4 0.7 0.13 1.4 × 10−2 1.2 × 10−3 3 × 10−4

4.2.5.3

Solubility Limit

The steady-state impurity solubility can be defined as the maximum concentration of impurity atoms in a crystal allowing thermodynamic balance between the crystal and another phase, e.g. a liquid phase, an extended defect or a precipitate. Precipitates are small inclusions of a second phase in a crystal, exhibiting a high concentration of ‘gathered’ impurities that cannot be solved in the crystal. Solubility limits for impurities in silicon have been first determined in [312] with a bulk of subsequent research [313] due to its practical relevance in device fabrication. The solubility limits for a few impurities in silicon are listed in Table 4.3. It is related to the ionization energy of the defect (cmp. Sect. 7.4) as shown in Fig. 4.11. The temperature dependence of the solubility for a few dopants is depicted in Fig. 4.12a. The solubility depends also on the present strain [315]. The simple empirical relation xs = 0.1 k (Fig. 4.12b) between the maximum molar solubility xs and the distribution coefficient k in silicon and germanium has been pointed out in [316]. A typical example for the formation of precipitates is Fe in InP, used for compensation of shallow donors in order to produce semi-insulating material (Sect. 7.7.8). The solubility of Fe in InP is fairly low, about 1017 cm−3 at growth temperature [317]. In Fig. 4.13 a high-resolution TEM image of a precipitate in InP doped with 3 × 1018 cm−3 Fe is shown. The precipitate exhibits a lattice constant

4.3 Dislocations

(a)

81

(b)

Fig. 4.12 a Steady-state solubility of impurities (P, As, B and Sb as labeled) in silicon. Solid lines are theoretical model matching various experimental data. Arrow denotes the melting point of silicon (1410 ◦ ). Adapted from [313]. b Maximum molar solid solubility xs vs. the distribution coefficient for various impurities in crystalline silicon and germanium. Solid line follows xs = 0.1 k. Adapted from [316] Fig. 4.13 High resolution TEM image of a FeP precipitate in iron-doped InP. Adapted from [318]

InP of d111 = 0.240 nm in [111]-direction, much different from that of InP (d111 = 0.339 nm). The angle ◦ ◦ between the [101] and [111] direction is 50 instead of 35 for InP. This is consistent with orthorhombic FeP [318]. Typically FeP and FeP2 precipitates are found in highly Fe-doped InP [319].

4.3 Dislocations Dislocations are line defects along which the crystal lattice is shifted by a certain amount. The vector along the dislocation line is called line vector L. A closed path around the dislocation core differs from that in an ideal crystal. The difference vector is called the Burger’s vector b. Dislocations for which the Burger’s vector is a vector of the lattice are called full dislocations. In contrast, dislocations with Burger’s vectors that are not translation vectors of the lattice are called partial dislocations. The history of dislocation theory is described in [320].

82

4 Structural Defects

(a)

(c)

(b)

(d)

Fig. 4.14 a High-resolution transmission electron microscopy image (HRTEM) in the 110 projection of a network of misfit dislocations at a GaAs/CdTe/ZnTe interface. Substrate: GaAs (001), 2◦ off 110 , ZnTe buffer layer is 2 monolayers thick. b Fourier transform with round mask around the (111) Bragg reflection. (c) Phase and d amplitude images for the mask from (b). From [321]

Since the energy of a dislocation is proportional to b2 , only dislocations with the shortest Burger’s vector are stable. The plane spanned by L and b is called the glide plane. In Fig. 4.14 a high-resolution image of the atoms around a dislocation and the phase and amplitude of the (111) reflection are shown. The phase corresponds to the atomic columns, the amplitude to the displacement of the atoms at the dislocation core (see also Fig. 4.14).

4.3.1 Dislocation Types 4.3.1.1

Edge Dislocations

For an edge dislocation (Fig. 4.15a) b and L are perpendicular to each other. An extra half-plane spanned by L and b × L is inserted.

4.3 Dislocations

83

b b

L (a)

L

(b)

Fig. 4.15 Model of a an edge and b a screw dislocation. The line vector L and the Burger’s vector b are indicated

(a)

(b)

Fig. 4.16 a Atomic force microscopy image of growth spiral around a screw dislocation on a silicon surface; image width: 4 µm. (textbfb STM image (width: 75 nm) of a screw-type dislocation with a Burgers vector of [000-1] on the ¯ N-face of GaN. The reconstruction is c(6×12). The c(6×12) row directions correspond to 1100 . Reprinted with permission from [322], ©1998 AVS

4.3.1.2

Screw Dislocations

For a screw dislocation (Fig. 4.15b) b and L are collinear. The solid has been cut along a half-plane up to the dislocation line, shifted along L by the amount b and reattached. Around the intersection of a screw dislocation with a surface, the epitaxial growth occurs, typically in the form of a growth spiral that images the lattice planes around the defect.

4.3.1.3

60◦ Dislocations

The most important dislocations in the zincblende lattice (Fig. 4.17) have the line vector along 110 . With the Burger’s vector a/2 110 three different types of dislocations can be formed: edge, screw and 60◦ dislocations. The vicinity of the core of the latter is shown in more detail in Fig. 4.17d. We note that the atomistic structure of 60◦ dislocations is different for L along [110] and [−1 10]; depending on whether the cations or anions are in the core, they are labeled α or β dislocations.

84

4 Structural Defects

[110]

L

b L

(a)

(b)

=0°

(c)

=60°

=90°

(d)

Fig. 4.17 Dislocations in the zincblende structure. The line vector is along [100]. The Burger’s vector a/2 110 can create an a edge dislocation, a b screw dislocation, and c a 60◦ dislocation. d Atomistic structure of a 60◦ dislocation

(a)

(b)

Fig. 4.18 a Plan-view transmission electron microscopy image of a network of 110 dislocation lines in (In,Ga)As ¯ Adapted from [323]. b on InP (001) with a lattice mismatch of about 0.1%. The TEM diffraction vector is g = [220]. ¯ GaN heterostructure with inPanchromatic cathodoluminescence image of partially relaxed Al0.13 Ga0.87 N on (3031) plane directions indicated. Adapted from [324], reprinted under a Creative Commons Attribution (CC BY 3.0) unported licence

4.3.1.4

Misfit Dislocations

When materials with different lattice constants are grown on top of each other, the strain can plastically relax via the formation of misfit dislocations. A typical network of such dislocations is shown in Fig. 4.18a for (In,Ga)As on InP (001). Another example is given in Fig. 4.18b for the (Al,Ga)N/GaN ¯ lattice plane tilted to the c-axis. This leads to non-rectangular dislocation system on a semipolar (3031) directions which are universal for dislocations from glide on a- and m-planes in heterostructures of trigonal and hexagonal materials [325] (Fig. 4.19).

4.3.1.5

Partial Dislocations

Partial dislocations, i.e. the Burger’s vector is not a lattice vector, must necessarily border a twodimensional defect, usually a stacking fault (Sect. 4.4.2). A typical partial dislocation in diamond or zincblende material is the Shockley partial dislocation (or just Shockley partial) with Burger’s vector b = (a0 /6) 112 . Another important partial is the Frank partial with b = (a0 /3) 111 . A perfect

4.3 Dislocations

85

Fig. 4.19 Dislocation line orientation angle α (versus the projected c-axis direction) for the a-plane prismatic slip system for m-azimuth and vice versa (solid line) and the m-plane prismatic slip system for m-azimuth (and a/a) (dashed line) as a function of interface inclination angle θ. Experimental data from epitaxy on semipolar planes are shown for (Al,Ga)2 O3 /Al2 O3 (square), (Al,Ga)N/GaN (diamond, cmp. Fig. 4.18b), (In,Ga)N/GaN (circles), GaN/Si (hexagon) and (Mg,Zn)O/ZnO (star). Adapted from [325, 326]

dislocation can be dissociated into two partials. This is energetically favorable. As an example we consider the reaction (Fig. 4.20a) 1 ¯

1 ¯ ¯ 1 ¯

101 → 112 + 211 . (4.22) 2 6 6 √ √ The length of the full dislocation is a0 / 2. The length of the Shockley partial is a0 / 6. Thus the energy E = G b2 of the full dislocation is E 1 = Ga02 /2 and the sum of the energies of the partials is smaller, E 2 = 2Ga02 /6 = Ga02 /3. In Fig. 4.20b a TEM image of a Ge/Si interface with a Shockley partial is shown.

4.3.2 Visualization of Dislocations by Etching Defects can be made visible using etching techniques. This is particularly popular for finding dislocations. Many etches are anisotropic, i.e. the etch velocity varies for different crystal directions. As an example the result of etching a silicon sphere in molten KOH and a germanium sphere in a HNO3 /HF solution are shown in Fig. 4.21. The remaining bodies exhibit those planes with low etching velocity. The etch velocity of various etch solutions has been investigated in detail in particular for silicon (Fig. 4.22). In a planar geometry, etch pits indicate the presence of dislocations, as shown in Fig. 4.23 for Ge of different orientation. The anisotropic etch prepares {111} planes. The dislocation core is at the ¯ are developed by intersection of the planes. In Fig. 4.24 hexagonal etch pits stretched along [110] molten KOH [330, 331]. The sides of the base are along [110], 130 and 310 . The depth and width ¯ surface, the orientation of the pits is of the pits increases with increasing etching time. On the (001) rotated by 90◦ because of the polar [111]-axis of the zincblende structure [330]. Such etch pit develops

86

4 Structural Defects

(a)

(b)

Fig. 4.20 a Graphical representation of the dislocation reaction of (4.22). b TEM image of the interface of a Ge/Si

¯ /6 Shockley partial dislocation. The image is overlayed with empty rod positions (as heterostructure with a 211 schematically shown in the lower left part of the figure) colored according to the stacking position (A: blue, B: red, C: green). The arrows labeled ‘I’ denote the position of the interface. Based on [327]

at a dislocation with Burger’s vector a/2 [011] (inclined to the (001) surface) [332]. Other types of etch pits indicate dislocations with other Burger’s vectors [332, 333]. Recipies how to wet chemically etch various semiconductors can be found in [328, 334–337]. Other etching techniques include dry processes such as plasma etching or reactive ion etching (RIE) [338–341].

Fig. 4.21 a Resulting shape of Si sphere (‘Lösungskörper’) after 3 h at 100◦ C in molten KOH. b Resulting shape of Ge sphere after etching in HNO3 :HF:CH3 COOH, 35:30:35 weight percent. The octaedric form indicates {111} faces. Markers are 1 mm. Adapted from [328]

4.3 Dislocations

(a)

87

(b)

Fig. 4.22 a Etch rate of silicon for tetramethyl-ammonium-hydroxide (TMAH) water solution (25%) at 86◦ C and 40% KOH at 70 ◦ C as a function of crystallographic direction. b Detail of the anisotropy around the (111) direction for TMAH solutions with three different concentrations and 40% KOH, all at 86 ◦ C. Adapted from [329]

Fig. 4.23 Etch pits on germanium with (a) (001) and (b) (111) surface orientation. In both cases {111} facets are prepared by the etch. As etch in (b) a HNO3 /HF/CH3 COOH solution with AgNO3 additive has been used. Width of the triangular etch pits is about 100 µm. Adapted from [334]

Fig. 4.24 Etch pits on GaAs (001) after a 3 min and b 10 min etch time in molten KOH at 300◦ C. Adapted from [330]

88

4 Structural Defects

Fig. 4.25 Dislocation density (as revealed by etch pits) for GaAs and InP as a function of the carrier concentration for various concentrations of impurities (S, Te, and Zn). Adapted from [343]

4.3.3 Impurity Hardening It has been found that the addition of impurities can lead to a substantial reduction of the dislocation density. This effect is known as impurity hardening and is caused by a hardening of the lattice due to an increase of the so-called critical resolved shear stress [342]. In Fig. 4.25 the dependence of the dislocation density in GaAs and InP is shown as a function of the carrier density that is induced by the incorporation of (electrically active) group-II or group-VI atoms (acceptors or donors, cf. Sect. 7.5). The high carrier concentration is unwanted when semi-insulating substrates (cf. Sect. 7.7.8) or low optical absorption (cf. Sect. 9.9.1) are needed. Thus the incorporation of isovalent impurities, such as In, Ga or Sb in GaAs and Sb, Ga or As in InP, has been investigated and found to be remarkably effective. Material containing such impurities in high concentration (>1019 cm−3 ) must be considered a low-concentration alloy. The lattice constant is thus slightly changed, which can cause problems in the subsequent (lattice-mismatched) epitaxy of pure layers.

4.4 Extended Defects 4.4.1 Micro-cracks If the stress in a material becomes too big to be accommodated by dislocations, cracks may form to release strain energy.8 In Fig. 4.26 an example is shown. In this case, micro-cracks have formed in a bulk mercury indium telluride crystal upon incorporation of residual stress and thermal stress during cooling of the material from growth temperature (about 1000 K) to room temperature. See also Fig. 12.19 for micro-cracks in an epitaxial layer.

8 We

note that in elasticity theory a continuous deformation is assumed. Obviously the separation (fracture) into two unstrained blocks is the lowest strain energy state of a stressed piece of material.

4.4 Extended Defects

89

Fig. 4.26 Micro-cracks in a mercury indium telluride crystal. Adapted from [344]

4.4.2 Stacking Faults The ideal stacking of (111) planes in the zincblende structure, ABCABC. . ., can be disturbed in various ways and creates area defects. If one plane is missing, i.e. the stacking is ABCACABC, an intrinsic stacking fault is present. If an additional plane is present, the defect is called an extrinsic stacking fault, i.e. ABCABACABC. An extended stacking fault in which the order of stacking is reversed is called a twin lamella, e.g. ABCABCB AC BABCABC. If two regions have inverted stacking order they are called twins and their joint interface is called a twin boundary, e.g. . . .ABCABCABCBACBACBA. . . (Fig. 4.29). The various types of stacking faults are shown in Fig. 4.27. In Fig. 4.28 a cross-sectional image of stacking faults in GaAs on Si is shown. They block each other and thus partially annihilate with increasing thickness. A stacking fault is bounded by two partial dislocations (Sect. 4.3.1.5) formed by the dissociation of a perfect dislocation. A full (or perfect) dislocation with Burger’s vector a/2[110] in a III–V compound is dissociated into two Shockley partials according to (4.22) [348]. Since the dislocation energy is proportional to |b|2 , the dissociation is energetically favored (see Sect. 4.3.1.5). The stacking-fault energy in pure silicon is γ = 47 mJ m−2 [349]. A similar value is found for Ge, γ = 60 mJ m−2 [350] and undoped GaAs, γ = 45 mJ m−2 [351]. In diamond a much larger value is found, γ = 285 mJ m−2 [352]. Impurity incorporation typically reduces the stacking fault energy. The systematics of stacking fault energy for various III–V and II–VI compounds has been discussed [185, 353, 354]. It can be correlated with the s-parameter (2.11) as depicted in Fig. 4.30.

Fig. 4.27 HRTEM images of a thin-film silicon with intrinsic (labeled ‘ISF’) and extrinsic (‘ESF’) stacking faults and twin boundary (‘Twin’). b Six monolayer thick hexagonal (wurtzite) CdTe layer in cubic (zincblende) CdTe. Stacking order (from bottom to top) is: ABCABABABABC. . . Reprinted with permission from [345]

(a)

(b)

90

4 Structural Defects

Fig. 4.28 Cross-sectional TEM image showing stacking faults in heteroepitaxial GaAs on Si. Adapted from [346]

Fig. 4.29 High resolution TEM image of ZnS nanowire exhibiting periodical twin structures. Adapted from [347]

Fig. 4.30 Reduced stacking fault energy (stacking fault energy per bond) γ for various compound semiconductors plotted as a function of the s-parameter. Dashed line is guide to the eye. Data from [185]

4.4.3 Grain Boundaries The boundaries of crystal grains are called grain boundaries. They are defined by five parameters, three rotation angles (e.g. Euler angles) to describe how the orientation of grain II results from grain I and two parameters to define the boundary plane of the two grains in the coordinate system of reference grain I. Such defects can have a large impact on the electric properties. They can collect point defects and impurities, act as barriers for transport (Sect. 8.3.8) or as carrier sinks due to (nonradiative) recombination. Details of their structure and properties can be found in [355, 356]. The two crystal grains meet each other with a relative tilt and/or twist. The situation is shown schematically in Fig. 4.31a for a small angle between the two crystals. A periodic pattern of dislocations forms at the interface that is called a small-angle grain boundary (SAGB) (Fig. 4.31b). In Fig. 4.32, experimental results for pure

4.4 Extended Defects

91

Fig. 4.31 Schemes of a–c pure tilt and d–f pure twist boundary, dislocation formation in (c) pure tilt and f twist boundaries

(a)

(b)

(d)

(c)

(e)

(f)

6 5 4 3 2 1 0

(a)

(b)

(d)

(c)

0

1

3

-4

4 2

5

(e)

Fig. 4.32 a Scheme of a small-angle (pure tilt) grain boundary. b Model of edge dislocations in a {110} plane in Ge. c Relation of dislocation distance d and tilt angle θ for various small-angle grain boundaries in Ge. Solid line is relation d = 4.0 × 10−8 /θ. d Optical image of an etched (CP–4 etch) Ge sample with a small-angle grain boundary. Adapted from [359]. e HRTEM image of a small-angle grain boundary in Si with dislocations highlighted. From [360]

tilt SAGB are shown. The dislocation spacing is inversely proportional to the tilt angle θ . An image of a twist SAGB is shown in Fig. 4.33. Special large angle boundaries possess (for a certain angle) a coincident site lattice (CSL). Some of these grain boundaries have a low energy and are thus commonly observed. The ratio of lattice points of the CSL and the lattice unit cell is an odd integer number n; the corresponding grain boundary is then labeled n. SAGB are also termed 1. 3 grain boundaries are always twin boundaries. An

92

4 Structural Defects

Fig. 4.33 Bright-field TEM image of pure twist boundary with network of pure twist dislocations fabricated by wafer bonding of two Si (001) surfaces with a relative twist. Adapted from [361]

(a)

(b)

Fig. 4.34 a Schematic of 3 (111) twin boundary in a diamond or zincblende structure (cmp. Fig. 4.29). The grain boundary is marked by a dashed line shown in side-view. The hexagonal and rectangular grey boxes have the same area. The lattice points of the coincident site lattice (CSL) are shown with black circles in the lower part of the figure. The unit cell of the CSL has three times the volume of the unit cell of the fcc lattice. b Schematic of a 5 (001) grain boundary in a (simple) cubic crystal shown in plane-view. The blue and the red lattice are rotated by 36.86◦ , the lattice points of the CSL are shown in black. The unit cell of the CSL lattice (dark grey) has five times the volume of the cubic unit cell (light grey)

example with (111) grain boundary is schematically shown in an example in Fig. 4.34a. A 3 (twin) boundary in silicon with {112} grain boundary [357, 358] is depicted in Fig. 4.35 together with the atomic arrangement of the grain boundary itself. A 5 (001) grain boundary is schematically shown in Fig. 4.34b; the special angle is θ = arctan 3/4 ≈ 36.87◦ . Real grain boundaries may not be flat, contain impurities or precipitates and even consist of a thin amorphous layer.

4.4 Extended Defects

93

Fig. 4.35 TEM images in two magnifications of a 3 {112} boundary in silicon together with a schematic of the atomic arrangement. Adapted from [358]

Fig. 4.36 Monoatomic step on the Si (001) surface and subsequent formation of an antiphase boundary in InP (zincblende)

4.4.4 Antiphase and Inversion Domains Antiphase domains occur when one part of the crystal is shifted with respect to another by an antiphase vector p. This does not form a twin. If the polar direction changes between two domains they are called inversion domains. ¯ In the zincblende structure the [110] and [110] directions are not equivalent. In one case there is a Zn-S lattice and in the other a S-Zn lattice. Both lattices vary by a 90◦ rotation or an inversion operation (which is not a symmetry operation of the zincblende crystal). If, e.g., a zincblende crystal is grown on a Si surface with monoatomic steps (Fig. 4.36, cmp. Fig. 11.6), adjoint regions have a different phase; they are called antiphase domains (APD). The antiphase vector is (0, 0, 1) a0 /4. At the boundaries a two-dimensional defect, an antiphase domain boundary, develops. The APD boundary contains bonds between identical atom species. In Fig. 4.37, intertwining APD boundaries are shown on the surface of InP layers on Si. The antiphase domains can be visualized with an anisotropic etch. In Fig. 4.38a, inversion domains in iron-doped ZnO are shown. Between domains the direction of the c-axis is reversed. The iron is found preferentially in the inversion domain boundary (IDB) (Fig. 4.38b) and plays an important role in its formation [364, 365].

94

4 Structural Defects

Fig. 4.37 Antiphase domains in InP on Si. HCl etchs InP anisotropically and prepares (111)A planes. The etch patterns of layers with (without) APDs are cross-hatched (linear). Adapted from [362]

(21 15

)

(0001)

(a)

(b)

Fe

Fig. 4.38 Transmission electron microscopy of inversion domains in ZnO:Fe. a Inversion domains in iron-doped ZnO (ZnO:Fe2 O3 = 100:1). Arrows denote the orientation of the c-axis in the respective domains. b Top: bright field TEM, bottom Fe distribution from energy-filtered image. Adapted from [363]

4.5 Disorder Disorder is a general term for deviations from the ideal structure on a microscopic scale. Apart from the various structural defects discussed in the previous chapters, further examples of disorder are • The presence of various isotopes of an element. This introduces disorder with regard to the mass of the atoms and impacts mostly phonon properties (see Fig. 8.28). • The occupation of lattice sites in alloys (Sect. 3.7) ranging from a random alloy, clustering to (partially) ordered phases. • The (unavoidable) thermal and zero-point motion of atoms around their equilibrium position.

Chapter 5

Mechanical Properties

If you want to find the secrets of the universe, think in terms of energy, frequency and vibration. N. Tesla

Abstract Lattice vibrations and phonons are treated with one-dimensional models and examples for real phonon dispersions for several semiconductors including phonons in alloys and disordered materials are given. Then the theory of linear elasticity and its application to semiconductors with regard to epitaxial strain, substrate bending and sheet-scrolling is given. Finally plastic relaxation effects such as critical thickness and wafer breakage are discussed.

5.1 Introduction The atoms making up the solid have an average position from which they can deviate since they are elastically bonded. The typical atomic interaction potential looks like the one shown in Fig. 2.1. The atoms thus perform a vibrational motion (including zero point fluctuations) and the solid is elastic. The potential is essentially asymmetric, being steeper for small distances due to quantum-mechanical overlap of orbitals. However, for small amplitudes around the minimum a harmonic oscillator can be assumed (harmonic approximation). Beyond the elastic regime, plastic deformation occurs such as generation of defects, e.g. dislocations. Eventually also the crystal can break.

5.2 Lattice Vibrations In the following we will discuss the dispersion relations for lattice vibrations, i.e. the connection between the frequency ν (or energy hν = ω) of the wave and its wavelength λ (or k-vector k = 2π/λ). Acoustic and optical vibrations are introduced in one-dimensional models. A detailed treatment of the physics of lattice vibrations is given in [366].

© Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_5

95

96

5 Mechanical Properties

Fig. 5.1 Schematic linear chain models with a same masses and spring constants, b different masses and same spring constants, c same masses and different spring constants, d different masses and different spring constants. Mirror operation X (S) exchanges the A–B atoms in the dimer (the spring constants)

5.2.1 Monoatomic Linear Chain The essential physics of lattice vibrations can best be seen from a one-dimensional model that is called the linear chain model. The mechanical vibrations will also be called phonons, although technically this term is reserved for the quantized lattice vibrations resulting from the quantum-mechanical treatment. In the monoatomic linear chain the atoms of mass M are positioned along a line (x-axis) with a period (lattice constant) a at the positions xn 0 = na. This represents a one-dimensional Bravais lattice. The Brillouin zone of this system is [−π/a, π/a]. The atoms will interact with a harmonic potential, i.e. the energy is proportional to the displacement u n = xn − xn 0 to the second power. This can be thought of as if the atoms are coupled by massless springs (Fig. 5.1a). The total (mechanical) energy of the system is then: U=

1 (u n − u n+1 )2 . C 2 n

(5.1)

The model assumes that the mass points are connected via massless, ideal springs with a spring constant C. If φ(x) is the interaction energy between two atoms, C is given by C = φ (a). Again, the harmonic approximation is only valid for small displacements, i.e. u n a. The displacement of the atoms can be along the chain (longitudinal wave) or perpendicular to the chain (transverse wave), see Fig. 5.2. We note that for these two types of waves the elastic constant C must not be the same. When the sum in (5.1) has a finite number of terms (n = 0, . . . , N − 1), the boundary conditions have to be considered. There are typically two possibilities: The boundary atoms are fixed, i.e. u 0 = u N −1 = 0, the boundary conditions are periodic (Born–von Karman), i.e. u i = u N +i . If N 1, the boundary conditions play no significant role anyway, thus those with the greatest ease for subsequent math are chosen. In solid-state physics typically periodic boundary conditions are used. Boundary phenomena, such as at surfaces, are then treated separately (see Sect. 11.6.1). The equations of motion derived from (5.1) are M u¨ n = Fn = −

∂U = −C (2u n − u n−1 − u n+1 ) . ∂u n

(5.2)

We solve for solutions that are periodic in time (harmonic waves), i.e. u n (x, t) = u n exp(−i ωt). Then the time derivative can be executed immediately as u¨ n = −ω2 u n and we obtain:

5.2 Lattice Vibrations Fig. 5.2 Visualization of transverse (‘T’) and longitudinal (‘L’) waves in a linear monoatomic chain at different wavevectors

97

a

k=1/4 /a T L

k=1/2 /a T L

k= / a T L

Mω2 u n = C (2u n − u n−1 − u n+1 ) .

(5.3)

If, also, the solution is periodic in space, i.e. is a (one-dimensional) plane wave, i.e. u n (x, t) = v0 exp(i(kx −ωt)) with x = n a, we find from the periodic boundary condition exp(ik N a) = 1 and thus k=

2π n , n∈N. a N

(5.4)

It is important that, when k is altered by a reciprocal space vector, i.e. k = k+2π n/a, the displacements u n are unaffected. This property means that there are only N values for k that generate independent solutions. These can be chosen as k = −π/a, . . . , π/a, so that k lies in the Brillouin zone of the lattice (Fig. 5.3). Since the properties are periodic with the Brillouin zone, the k-values can be imagined being on a circle as visualized in Fig. 5.3; the angle φ = k a run from 0 to 2π or from −π to +π as you like. In the Brillouin zone there is a total number of N k-values, i.e. one for each lattice point. The distance between adjacent k-values is 2π 2π = , (5.5) Na L L being the lateral extension of the system. The displacements at the lattice points n and n + m are now related to each other via u n+m = v0 exp(ik (n + m) a) = v0 exp(ikna) exp(i k m a) = exp(i k m a) u n .

(5.6)

98

5 Mechanical Properties

Fig. 5.3 Brillouin zone of a one-dimensional lattice from −π/a to +π/a and mapping to a circle with angles from −π over 0 (at ) to +π

Fig. 5.4 Dispersion relation for a monoatomic linear chain

(k)

4C / M

0

-1

0

/a)

1

Thus, the equation of motion (5.3) reads Mω2 u n = C 2 − exp(−i k a) − exp(i k a) u n .

(5.7)

Using the identity exp(i ka) + exp(−i ka) = 2 cos(k a), we find the dispersion relation of the monoatomic linear chain (Fig. 5.4): 4C 4C 1 − cos(k a) = sin2 ω (k) = M 2 M 2

ka 2

.

(5.8)

The solutions describe plane waves that propagate in the crystal with a phase velocity c = ω/k and a group velocity vg = dω/dk, |k| a 4C a cos . (5.9) vg = ± M 2 2 In the vicinity of the point, i.e. k π/a the dispersion relation is linear in k ω(k) = a

C |k| . M

(5.10)

5.2 Lattice Vibrations

99

We are used to such linear relations for sound (and also light) waves. The phase and group velocity are the same and do not depend on k. Thus, such solutions are called acoustic. The sound velocity of the √ medium (vg (k = 0) in (5.9)) is given by vs = a C/M. It is characteristic of the non-continuous medium that for k approaching the boundary of the Brillouin zone, the behavior of the wave is altered. For k = π/a the wavelength is just λ = 2π/k = 2a, and thus samples the granularity of the medium. The maximum phonon frequency ωm is ωm =

4C . M

(5.11)

The group velocity is zero at the zone boundary, thus a standing wave is present. Since the force constants of the longitudinal and transverse waves can be different, the dispersion relations are different. The transverse branch of the dispersion relation is two-fold degenerate when the two directions perpendicular to k are equivalent.

5.2.2 Diatomic Linear Chain Now we consider the case that the system is made up from two different kinds of atoms (Fig. 5.5). This will be a model for semiconductors with a diatomic base, such as zincblende. We note that the diamond structure also needs to be modeled in this way, although both atoms in the base are the same. The lattice will be the same and the lattice constant will be a. Alternating atoms of sort 1 and 2 with a relative distance of a/2 are on the chain. The displacements of the two atoms are labeled u 1n and u 2n , both belonging to the lattice point n. The atoms have the masses M1 and M2 . The force constants are C1 (for the 1–2 bond within the base) and C2 (for the 2–1 bond between different bases) (Fig. 5.1d). The total energy of the system is then given as U= The equations of motion are

Fig. 5.5 Visualization of acoustic and optical waves in a diatomic linear chain

2 1 2 1 C1 u 1n − u 2n + C2 u 2n − u 1n+1 . 2 2 n n

(5.12)

100

5 Mechanical Properties

M1 u¨ 1n = −C1 u 1n − u 2n − C2 u 1n − u 2n−1 M2 u¨ 2n = −C1 u 2n − u 1n − C2 u 2n − u 1n+1 .

(5.13a) (5.13b)

With the plane-wave ansatz u 1n (x, t) = v1 exp(i(kna − ωt)) and u 2n (x, t) = v2 exp(i(kna − ωt)) and periodic boundary conditions we find 0 = −M1 ω2 v1 + C1 (v1 − v2 ) + C2 [v1 − v2 exp(−ika)] 0 = −M2 ω2 v2 + C1 (v2 − v1 ) + C2 [v2 − v1 exp(ika)] .

(5.14a) (5.14b)

These equations for v1 and v2 can only be solved nontrivially if the determinant vanishes, i.e.

M1 ω2 − (C1 + C2 ) C1 + e−ika C2

0=

C1 + eika C2 M2 ω2 − (C1 + C2 )

(5.15)

= M1 M2 ω4 − (M1 + M2 )(C1 + C2 ) ω2 + 2C1 C2 [1 − cos(k a)] . Using the substitutions C+ = (C1 + C2 )/2, C× = and accordingly for M+ and M× , the solution is 2 (k) ω±

ω2 = max 2

√ C1 C2 , the arithmetic and geometrical averages,

2 2 1 ± 1 − γ sin (k a/2) ,

with 0 C2 , the top of the acoustic branch has v−,2 (X ) = v−,1 (X ) and thus the same as at the -point, preserving the ‘acoustic’ nature of the band. For C2 > C1 , however, v−,2 (X ) = −v−,1 (X ) and thus out-of-phase, resembling an optical mode. For the upper branch the situation is vice versa. The situation can be visualized by plotting the relative phase of v2 and v1 , as expressed by

v±,2 (k) δφ± (k) = arg v±,1 (k)

,

(5.27)

for the two cases C2 /C1 ≷ 1 (note that |v2 | = 1 for all cases) for the lower branch in Fig. 5.7. The dispersions for the two cases C2 /C1 ≷ 1 with the phase δφ± depicted as color are compared in Fig. 5.8. For all cases of C2 /C1 > 1, v±,2 (π/a) − v±,2 (−π/a) = 0. For all cases of C2 /C1 < 1, v±,2 (π/a) − v±,2 (−π/a) = 2 π . Thus this number is a ‘topological invariant’ since it cannot be changed by smooth changes of the system, i.e. small and slow variations of C1 /C2 , unless one goes through the gapless state (C1 /C2 = 1). The case C1 = C2 , δφ− = k a/2 and δφ+ = π + k a/2 is shown as dotted lines in Fig. 5.7. It should be noted that the phase difference in (5.27) and the curves in Fig. 5.7 are independent of the mass ratio. Generally, the symmetry of a mode v with respect to the operation X that exchanges A- and B-sites, Xv= X

v v v1 = 2 = exp(ı δφ) 1 , v2 v1 v2

(5.28)

can be expressed by the phase δφ. X is a unitary transformation since X H X = 1. For a well defined parity-like symmetry, we demand X 2 = 1; it is present for a phase factor of 1 (δ = 0, positive

(a)

(b)

Fig. 5.7 Relative phase of the B-site to the A-site in the a lower (acoustic, δφ− ) branch and b upper (optical, δφ+ ) branch, expressed by arg(v2 /v1 ) from (5.27). The case C1 /C2 = 2 is shown as solid line; the inverted case of C1 /C/2 = 1/2 is shown as dashed line. The case C1 = C2 is shown as dotted lines

5.2 Lattice Vibrations

103

parity) and a phase factor of −1 (δ = ±π , negative parity). In Fig. 5.8b, for the non-trivial phase, the parity changes twice within the Brillouin zone, while for the trivial case it does not. In view of later discussions of electronic band structure we remind the reader that electronic s-states (p-states) have positive (negative) parity. The phase change summed up when going through the entire Brillouin zone must a multiple of 2 π since the physical properties are periodic with the Brillouin zone. The property to calculate for obtaining a proper topological invariant here is the Berry phase [369, 370] γn for a branch n with the more general recipe, ∂ (5.29) vn dk , γn = ı v∗n · ∂k C

where C is a closed loop in parameter space, here it is the integral over the entire Brillouin zone. The integrand is the one-dimensional equivalent to the ‘Berry connection’.1 For the diatomic linear chain, the integral yields ⎧ C2 < C1 ⎨0 γ± = −π C2 = C1 . (5.30) ⎩ −2 π C2 > C1 One should think also about the following: The situation for C2 > C1 means that the A–B inter-dimer spring constant is larger than the intra-dimer one. But our choice of unit cell is free and the situation can be thought of differently in terms of B–A dimers where then, for exactly the same physical situation, the inter-dimer spring constant (now C1 ) is smaller than the intra-dimer one (C2 ). Thus, the two bulk situations will not be much different per se and cannot be distinguished, in particular when the A- und B-sites are equivalent (here M1 = M2 ). However, when two media with different topology have an interface, edge states develop according to the bulk-boundary correspondence; this will be shown for the DLCM in Sect. 5.2.10. In the case C1 = C2 (Fig. 5.1b), C+ = C× = C and the dispersion relation can be simplified to

Fig. 5.8 Phonon dispersion with the phase of the wavefunction (relative phase between B- and A-sites) shown in false colors. Left: C1 /C2 = 2, right: C1 /C2 = 1/2. The parity symmetry of the mode with respect to exchange of A- and B-sites is indicated with ‘+’ (in-phase) and ‘−’ (out-of-phase)

1 For higher dimensions, the integral over a closed path (or surface) can be replaced via Stokes’ theorem with an area (or volume) integral of the Berry flux. Also it is invariant under a ‘gauge transformation’ where vn is replaced by exp(i θ) vn .

104

5 Mechanical Properties

2 C M M×2 + 2 2 ω± = 1 ± 1 − 2 sin (k a/2) . M×2 M+

(5.31)

At the zone √ boundary the frequencies for the acoustic and the optical branch are, √ assuming M2 < M1 , ω X,1 = 2C/M1 with v2 = 0 (oscillation of the larger mass) and ω X,2 = 2C/M2 with v1 = 0 (oscillation of the smaller mass), respectively. In the vibrations at the X-point thus only one atom species oscillates, the other does not move. Close to the point, the atoms are in phase in the√acoustic branch with v2 = v1 . For the optical branch, the frequency at the point is given by ω = 2C/Mr (with the reduced mass Mr−1 = M1−1 + M2−1 = 2M+ /M×2 ) and the amplitude ratio is given by the mass ratio: v2 /v1 = −M1 /M2 , i.e. the atoms are out of phase and the heavier atom has the smaller amplitude. It should be repeated that the relative phase of v2 and v1 , as defined in (5.27), is the same for all masses (dotted line in Fig. 5.7). The situation C1 = C2 is therefore for all masses topologically the same as the gapless state and the gap has different character when due to different spring constants or due to different masses. Finally, we consider the symmetry classification looking at Fig. 5.1 again. The monoatomic chain has two mirror-like symmetries, indicated by vertical dashed lines; it is symmetric with respect to exchange X of the A- and B-atoms and to the exchange S of the springs. The cases Fig. 5.1b, c preserve only one such symmetry while the general diatomic chain Fig. 5.1d preserves none of them individually but still possesses the so-called chiral symmetry which is the combination X S. In terms of the ‘periodic system’ of the CAZ classification of topological systems the diatomic linear chain is a BDI-type system [371] and the topological invariant is, derived from (5.30), an integer of the form, γ /2π ∈ Z.

5.2.4 Lattice Vibrations of a Three-Dimensional Crystal When calculations are executed for a three-dimensional crystal with a monoatomic base, there are 3N equations of motion. These are transformed to normal coordinates and represent 3 acoustic branches (1 LA phonon mode and 2 TA phonon modes) of the dispersion relation. In a crystal with a base with p

Fig. 5.9 Phonon dispersion in Si, experimental data and theory (solid lines: bond charge model, dashed lines: valence force field model). Adapted from [164]

5.2 Lattice Vibrations

105

Fig. 5.10 Phonon dispersion in a GaP and b GaAs. Experimental data (symbols) and theory (solid lines, 14-parameter shell model). ‘L’ and ‘T’ refer to longitudinal and transverse modes, respectively. ‘I’ and ‘II’ (along [ζ, ζ, 0]) are modes ¯ plane. The grey area in (a) denotes the gap between acoustical and optical states. a whose polarization is in the (110) Adapted from [375], b Adapted from [373]

atoms, there are also 3 acoustic branches and 3( p − 1) optical branches. For a diatomic base (as in the zincblende structure) there are 3 optical phonon branches (1 LO phonon mode and 2 TO phonon modes). The total number of modes is 3 p. The dispersion ω(k) now has to be calculated for all directions of k. In Figs. 5.9 and 5.10, the phonon dispersion in silicon, GaAs and GaP is shown along particular lines in the Brillouin zone (cf. Fig. 3.38). A detailed treatment can be found in [372]. The degeneracy of the LO and TO energies at the point for the covalent group-IV semiconductor is lifted for the III–V semiconductors due to the ionic character of the bond and the macroscopic electric field connected with the long-wavelength LO phonon (see Sect. 9.5). Comparing GaAs [373] and GaP [374], the quite different mass of Ga- and P-atoms (M× /M+ ≈ 0.92) leads to the formation of a clear gap between the acoustic and optical branches, while for GaAs M× /M+ ≈ 0.9994 is close to 1 and no gap forms. We note that the degeneracy of the TA phonon is lifted for propagation along the 110 directions ¯ are not equivalent. () because the two transverse directions 001 and 110 In boron nitride the masses of the two constituents are so similar that no gap exists between acoustical and optical branches (Fig. 5.11). Also the density of states (averaged over the entire Brillouin zone) is depicted (see the next chapter). The displacement of atoms is shown in Fig. 5.12 for the different phonon modes present in zincblende crystals. In Fig. 5.13 the optical phonon modes for wurtzite crystals are depicted. The E-modes with

106

5 Mechanical Properties

Fig. 5.11 Phonon dispersion in BN (left panel), experimental data (symbols) and theory (solid lines, first principles pseudopotential model). In the right panel the density of states is depicted. Adapted from [376]

A1

(1)

T2

(2)

T2

E

(1)

T2

(2)

T2

E

(1)

T2

(2)

T2

Fig. 5.12 Displacement of atoms for various phonon modes in zincblende crystals. Adapted from [377]

displacement perpendicular to the c-axis are double degenerate such that there are nine modes (the primitive unit cell has p = 4 atoms (Sect. 3.4.5)). The modes are labeled with their symmetry (in molecular notation) according to group theory (see remark in Sect. 6.2.5).

5.2 Lattice Vibrations

107

Fig. 5.13 Displacement of atoms for various phonon modes in wurtzite crystals. Adapted from [378]

(a)

(b)

Fig. 5.14 a Raman spectra of GaAs with different isotope content as labeled. b Energy of optical phonons in GaAs with c different isotope content [using the Raman spectra shown in (a)]. Reprinted with permission from [379], 1999 APS

√ The dependence of the phonon frequency on the mass of the atoms (∝ 1/ M) can be demonstrated with the isotope effect, visualized for GaAs in Fig. 5.14. The dependence of the phonon frequencies on the stiffness of the spring can be seen from Fig. 5.15; the smaller lattice constant provides the stiffer spring.

5.2.5 Density of States The density of states (DOS) tells how many of the total number of modes are in a given energy interval. The states are spaced equally in k-space but not on the energy scale (see also Sect. 6.13). For the monoatomic linear chain model, the number of states N (E ) from E = 0 up to E = ω = E (k ) for the dispersion of the acoustic phonons (5.8) is given as N (E ) = k

N L = k . π/a π

(5.32)

108

5 Mechanical Properties

Fig. 5.15 Optical phonon frequencies (TO: filled squares, LO: empty squares) for a number of III–V compounds with different lattice constant a0 . 1 meV corresponds to 8.065 wave numbers (or cm−1 ). Adapted from [380]

Using (5.8), we find for one polarization (E m = ωm ) 2N arcsin N (E) = π

E Em

.

(5.33)

The DOS D(E) is given by D(E) =

2N 1 dN (E) = . dE π E m 1 − (E/E m )2

(5.34)

Often the density of states is scaled by the (irrelevant) system size and given per atom (D/N ) or per volume (D/L 3 ), per area (D/L 2 ) or per length (D/L) for three-, two- or one-dimensional systems, respectively. In the diatomic linear chain model, additionally the optical phonons contribute to the density of states. In Fig. 5.16 the phonon density of states is shown for γ = 0.9 and for comparison for γ = 1 (gapless phonon dispersion). For small wavevector, the density of states is 4N /(π E m ).2 Within the gap the density of states vanishes. At the edges of the band gap the density of states is enhanced. The total number of states for both dispersions is the same. In a three-dimensional solid the total number of modes is 3 p N (N 1, p is the number of atoms in the base). Then (5.32) is modified to (for three degenerate polarizations) N (E ) =

3 4π k 3 , 3 (2π/L)3

(5.35)

taking into account all states within a sphere in k-space of radius k . Assuming a linear dispersion ω = vs k (for sufficiently small wave vector), we obtain

2 The

factor 2 compared to (5.34) stems from the folded Brillouin zone compared to the monoatomic chain model.

5.2 Lattice Vibrations

109

N (E) =

V E3 . 2π 2 3 vs3

(5.36)

Thus the density of states is approximately3 proportional to E 2 , D(E) =

3 V E2 . 2π 2 3 vs3

(5.37)

As realistic example for the phonon density of states, the DOS of bulk BN is depicted next to the dispersion in Fig. 5.11.

5.2.6 Phonons Phonons are the quantized quasi-particles of the lattice vibrations (normal modes). The energy of a phonon can take the discrete values of a harmonic oscillator 1 ω , (5.38) E ph = n + 2 where n denotes the quantum number of the state, which corresponds to the number of energy quanta ω in the vibration. The amplitude of the vibration can be connected to n via the following discussion. For the classical oscillation u = u 0 exp i(kx − ωt) the space and time average for the kinetic energy yields 2 ∂u 1 1 = ρ V ω2 u 20 , (5.39) E kin = ρ V 2 ∂t 8 where ρ is the density and V the volume of the (homogeneous) solid. The energy of the oscillation is split in half between kinetic and potential energy. From 2E kin = E ph we find

(a)

(b)

Fig. 5.16 a Phonon dispersion for the diatomic linear chain model for γ = 1 (black line) and γ = 0.9 (blue lines). b Corresponding density of states (in units of N /E m )

3 This dependence is the base for Debye law for the

T 3 temperature dependence of the heat capacity at low temperatures when only states with sufficiently small wave vector are thermally populated.

110

5 Mechanical Properties

u 20

4 1 . = n+ 2 ρVω

(5.40)

The number of phonons with which a vibrational mode is populated is thus directly related to the classical amplitude square. Phonons act with a momentum k, the so-called crystal momentum. When phonons are created, destroyed or scattered the crystal momentum is conserved, except for an arbitrary reciprocal-space vector G. Scattering with G = 0 is called a normal process, otherwise (for G = 0) it is called an umklapp process.

5.2.7 Localized Vibrational Modes A defect in the crystal can induce localized vibrational modes (LVM). The defect can be a mass defect, i.e. one of the masses M is replaced by Md , or the force constants in the neighborhood are modified to Cd . A detailed treatment can be found in [381]. LVM are discussed, e.g., in [382–384]. First we consider the LVM for the one-dimensional, monoatomic chain. If the mass at lattice point i = 0 is replaced by Md = M + M (M = M/M), the displacements are given by u i = AK |i| , A being an amplitude, with 1 + M , (5.41) K =− 1 − M and the defect phonon frequency ωd is ωd = ωm

1 . 2 1 − M

(5.42)

A real frequency √ is obtained for |M | < 1. ωd is then higher than the highest frequency of the bulk modes ωm = 4C/M (5.11). For M < 0, i.e. the mass of the defect is smaller than the mass of the host atoms, K is negative and |K | < 1. Thus, the displacement can be written as u i ∝ (−|K |)|i| = (−1)|i| exp (+ |i| log |K |) .

(5.43)

The numerical value of the exponent is negative, thus the amplitude decreases exponentially from the defect and indeed √ makes a localized vibrational mode. For small mass Md M (5.42) yields approximately ωd = 2C/Md . This approximation is the so-called one-oscillator model. Since typically the extension of the localized mode is only a few lattice constants, the picture of LVM remains correct for impurity concentrations up to ∼1018 –1020 cm−3 . For higher concentrations the concept of alloy modes has to be invoked (cf. Sect. 5.2.8). For the case of group-III or -V substitutional impurities in group-IV semiconductors the change in force constants (treated below) can be neglected to some extent. For silicon (M = 28) and germanium (M = 73) the effect of various substitutions is shown in Fig. 5.17. Now, additionally the force constants left and right of the defect are replaced by Cd = C + C (C = C/C). The displacements are still given by u i = AK |i| , now with K =−

(1 + M ) (1 + C ) . 1 − M − 2C

(5.44)

5.2 Lattice Vibrations

111

An exponential decrease of the LVM amplitude occurs for negative K that is ensured for M + 2C < 0 (and M > −1 and C > −1). The defect frequency is given by ωd = ωm

(1 + C ) (2 + C (3 + M )) . 2(1 + M ) (2C + 1 − M )

(5.45)

We note that for C = 0 (5.41) and (5.42) are recovered. For a given mass defect, the change of frequency with C is (in linear order, i.e. for C 1) 2 ∂ωd (M , C ) 1 − 4 M − M = C . ∂C 2 4 (1 − M ) 1 − M

(5.46)

The linear coefficient diverges for M → −1. For M between −0.968 and 0 the linear coefficient varies between 2 and 1/4. Therefore, a larger force constant (C > 0) increases the LVM frequency of the defect, as expected for a stiffer spring. In a binary compound the situation is more complicated. We assume here that the force constants remain the same and only the mass of the substitution atom Md is different from the host. The host has the atom masses M1 and M2 with M1 < M2 . Substitution of the heavy atom with a lighter one creates a LVM above the optical branch for Md < M2 . Additionally, a level in the gap between the optical and acoustic branch is induced. Such LVM is called a gap mode. Substitution of the lighter atom of the binary compound induces a LVM above the optical branch for Md < M1 . A gap mode is induced for Md > M1 . The situation for GaP is depicted in Fig. 5.18. LVM in GaAs have been reviewed in [382]. The energy position of a local vibrational mode is sensitive to the isotope mass of the surrounding atoms. In Fig. 5.19, a high-resolution (0.03 cm−1 ) spectrum of the 12 CAs LVM in GaAs is shown together with a theoretical simulation. The various theoretical peak positions are given as vertical bars, their height indicating the oscillator strength. Five experimental peaks are obvious that are due to a total of nine different transitions. The C atom can experience five different

Fig. 5.17 Energy of local vibrational modes in Si and Ge. Experimental values at T = 300 K (B in Ge: T = 80 K) taken from [381] and references therein and from [385] (C in Ge). The dashed lines are the mass dependence according to (5.42) scaled to the experimental frequency of the 10 B LVM

112

5 Mechanical Properties

surroundings (see Table 3.8) with the four neighbors being 69 Ga or 71 Ga. The natural isotope mix is an ‘alloy’ 69 Gax 71 Ga1−x As with x = 0.605. The configurations with Td symmetry contribute one peak each, the lowest (71 Ga surrounding) and highest (69 Ga surrounding) energy transitions. The configurations with C3v and C2v symmetry contribute each with 2 and 3 nondegenerate modes, respectively. The vibrations of impurity complexes have been discussed in [387].

5.2.8 Phonons in Alloys In an alloy of the type AB1−x Cx , the phonon frequencies will depend qualitatively and quantitatively on the ternary composition [388]. For the binary end materials AB and AC clearly TO and LO frequencies exist. The simplest behavior of the alloy is the one-mode behavior (Fig. 5.20d) where the mode frequencies vary continuously (and approximately linearly) with the composition. The oscillator strength (LO–TO splitting, (9.86)) remains approximately constant. In many cases, the two-mode behavior is observed where the LO–TO gap closes (accompanied by decreasing oscillator strength) and a localized vibrational mode and a gap mode occur for the binary end materials (Fig. 5.20a). Also, a mixed-mode behavior (Fig. 5.20b, c) can occur. The masses of the three constituent atoms will be MA , MB , and MC . Without limiting the generality of our treatment, we assume MB < MC . From the considerations in Sect. 5.2.7 on LVM and gap modes, the condition (5.47) MB < MA , MC for two-mode behavior can be deduced. This ensures a LVM of atom B in the compound AC and a gap mode of atom C in the compound AB. However, it turns out that this condition is not sufficient, e.g. Na1−x Kx Cl fulfills (5.47) but exhibits one-mode behavior. From a modified REI4 model (for k ∼ 0 modes) it has been deduced that

0

27

11

AlGa

20

BP

28

SiGa

12

40

CGa

10

BP

60 14

NP

80

(a)

100 400

(b)

GaP 450

500

550 -1

600

Fig. 5.18 a Numerical simulation of a linear chain model for GaP (M1 = 31, M2 = 70). Energy of local vibrational modes (dashed (solid) line): substitution on P (Ga) site) in units of the optical phonon frequency at (ωm = 45.4 meV, cf. Fig. 5.10a). The grey areas indicate the acoustic and optical phonon bands. Solid squares are experimental data (from [381]), scaled to the theoretical curve for the 27 AlGa LVM frequency. b Differential transmission spectrum of GaP structure (nitrogen-doped layer on zinc-doped compensated substrate) against pure crystal (T = 77 K). Data from [386]

4 Random

element isodisplacement.

5.2 Lattice Vibrations

113

GaAs 12

CAs

Exp. Th. -1

Fig. 5.19 Experimental (Exp., T = 4.2 K, resolution 0.03 cm−1 ) and theoretical (Th., artificial Lorentzian broadening) infrared spectra of LVM of 12 CAs in GaAs. The positions and oscillator strengths of the theoretical transitions involving different configurations with 69 Ga and 71 Ga isotopes are shown as vertical bars. Data from [382]

LO1

localized mode

LO1

localized mode

LO1

Frequency

LO TO1

TO1

LO2

TO1

LO2

LO2 TO

gap mode

TO2

TO2

(a) 0

0.5 1 Composition

gap mode

(b) 0

TO2

(c)

0.5 1 Composition

0

0.5 1 Composition

(d) 0

0.5 1 Composition

Fig. 5.20 Schematic behavior of phonon modes in an alloy. a Two-mode behavior with gap mode and localized mode, (b, c) mixed-mode behavior, b only localized mode allowed, c only gap mode allowed, d one-mode behavior with neither localized mode nor gap mode allowed

MB < μAC =

MA MC < MA , MC MA + MC

(5.48)

is a necessary and sufficient condition (unless the force constants between A–B and A–C are significantly different) for two-mode behavior [389]. A detailed discussion is given in [390]. Equation (5.48) is a stronger condition than the previous one (5.47). If (5.48) is not fulfilled the compound exhibits one-mode behavior. As an example, we show the mass relations for CdS1−x Sex and Cdx Zn1−x S in Table 5.1 and the experimental phonon energies in Fig. 5.21. Also in Table 5.1 the masses for GaP1−x Asx (GaAs1−x Sbx ) exhibiting two- (one-) mode behavior are shown.

114

5 Mechanical Properties

Table 5.1 Atomic masses (MB < MC ) of the constituents of various ternary compounds of type A(B,C), reduced mass μAC (5.48), fulfillment of the relation from (5.48) (‘+’: fulfilled, ‘−’: not fulfilled) and experimental mode behavior (‘2’: two-mode, ‘1’: one-mode) Alloy

A

B

C

MA

MB

MC

μAC

Rel.

Modes

GaP1−x Asx GaAs1−x Sbx CdS1−x Sex Cdx Zn1−x S Mgx Zn1−x O Alx Ga1−x N

Ga Ga Cd S O N

P As S Zn Mg Al

As Sb Se Cd Zn Ga

69.7 69.7 112.4 32.1 16.0 14.0

31.0 74.9 32.1 65.4 24.3 27.0

74.9 121.8 79.0 112.4 65.4 69.7

36.1 44.3 46.4 25.0 12.9 11.7

+ − + − − −

2 1 2 1 1 2(!)

360

320

CdxZn1-xS

-1

320

280 260

300

240

280

220

260

200

240

180

220

160

ZnS

CdS1-xSex

300

340 -1

Fig. 5.21 Phonon energies of Cdx Zn1−x S and CdS1−x Sex as a function of the ternary composition. Experimental data (solid circles) are from [389], dashed lines are guides to the eye

x

CdS

CdS

x

CdSe

If the binary end components of a ternary alloy have different crystal structure, a transition between the two occurs which is reflected in the phonon structure (energies and mode symmetries). As an example, the optical phonon energies of Mgx Zn1−x O are depicted in Fig. 5.22 (cmp. Fig. 3.43). An example for the variation of phonon oscillator strength (as defined in (9.86)) with alloy composition is depicted in Fig. 5.23 for (Al,Ga)N [392].5

5.2.9 Disorder An example of local disorder are the localized vibrational modes due to a single defect. Here we consider in our one-dimensional model random fluctuations of the model parameters. To that avail we set up a numerical implementation of an one-dimensional chain with masses M1 = M2 = 1 and spring constants C1 = C2 , here C2 = 2 C1 . Now each mass varies randomly by a factor with a

5 The

oscillator strengths f shown here have been calculated from the values S given in [392] divided by (∞).

5.2 Lattice Vibrations

700

MgxZn1-xO F1u

-1

Phonon energy (cm )

Fig. 5.22 LO (solid lines) and TO (dashed lines) phonon energies of Mgx Zn1−x O in the wurtzite structure (A1 symmetry: blue lines, E1 symmetry: red lines) and in the rocksalt phase (F1u symmetry: black lines). Experimental data are shown as symbols. Adapted from data of [391]

115

A1

600

E1 500 400 0.0

0.2

0.4 0.6 0.8 Mg-concentration x

1.0

Fig. 5.23 Oscillator strength f (cf. (9.86)) of alloy phonons in (Al,Ga)N thin films on c-Al2 O3 . Based on data from [392]

statistical distribution of mean M¯ = 1 and a standard deviation6 σM . The density of states is displayed for σM / M¯ = 0.1–0.5. The effects as shown in Fig. 5.24 are broadening of the peaks in the DOS, broadening of the band edges, the development of band tails into the gap and eventually a closing of the gap. This is a typical behavior that also exists for electronic states (cmp. Fig. 6.53).

5.2.10 Topological Edge States of the Diatomic Linear Chain Here we treat a finite diatomic linear chain with N unit cells, i.e. A–B dimers. In case of periodic boundary conditions, the rightmost B-atom is ‘connected’ to the leftmost A-atom, but now we chose N to be finite. The system of 2N equations of the type ω2 u n = (∂U/∂u n )/Mn (like (5.13a) or (5.13b)) is written in matrix form and the eigenproblem M − ω2 1 = 0 is solved numerically [393]. Also, we fix both B ends, i.e. the displacements u A 0 and u N are forced to be zero (Fig. 5.25). We set M1 = M2 and find two quite different situations for the cases (i) C1 > C2 and (ii) C1 < C2 . Case (i) is similar to the bulk case 6 In order to avoid negative values for the masses, not a normal or Gaussian distribution is used but the Gamma distribution with the parameters G(1/σ 2 , 1/σ 2 ).

116

5 Mechanical Properties

Fig. 5.24 Density of states versus energy (in units of maximum phonon energy E m = ωmax according to (5.18)) for the diatomic linear chain model (M1 = M2 , C2 = 2 C1 , 27 dimers, average over 212 configurations) for various levels of random relative variations of the masses (solid lines). The forbidden energy ranges for the ideal chain are shown in light grey. The DOS has been normalized such that its integral over all energies is 1 (the energy bins have a width of 0.01 E m )

Fig. 5.25 a Diatomic linear chain model (DLCM) with A–B dimers (one unit cell shown in grey) in an infinite chain; A-sites (B-sites) are shown in red (blue); the connecting springs have force constants C1 (green) and C2 (orange), respectively. b DLCM with finite number of dimers (shown for N = 6) with both end sites fixed (shown in black). The movable sites now consist of B–A dimers (one unit cell shown in grey)

(i.e. for periodic boundary conditions) where a ‘clean’ gap is present; for C1 √ = C2 of course no gap appears. In case (ii), two states appear within the gap with energy ωg = ωmax / 2. The eigenvalues of the problem are shown as a function of C2 /C1 in Fig. 5.26a. The mode pattern for the two gap states are depicted in Fig. 5.27a (for C2 /C1 = 1/2). All other states follow bulk like vibration patterns as expected from a vibrating string. For M1 = M2 the gap states are degenerate, otherwise split as shown in Fig. 5.26c. For the case of C2 > C1 , the patterns for the highest mode of the lower band and the lowest mode of the top band are depicted in Fig. 5.27b; the are obviously bulk-like as all others and no localized states exist. The appearance of end states in one of the cases is the expression of the fact that the two bulk band structures for C1 > C2 and C1 < C2 are topologically different7 (cmp. Sect. 5.2.3). The general effect is the so-called ‘bulk-boundary’ correspondence where edge states appear at the interface between different topological phases (one of these phases can be the topologically trivial vacuum outside the solid). Such edge states are termed more precisely end-states for (quasi-) one-dimensional systems.

7 Since the two outer atoms are fixed, the movable parts of the chain consists of B–A dimers (Fig. 5.25b), thus the topologically non-trivial case occurs here for C2 < C1 .

5.2 Lattice Vibrations

117

(a)

(b)

(c)

(d)

Fig. 5.26 a Eigenvalues of a diatomic chain with N = 32 unit cells (64 atoms) as a function of the ratio C2 /C1 (M1 = M2 ). The frequency is normalized (to ωmax from (5.18)). The abzissa is logarithmic. b Same calculation as for panel (a) but M1 /M2 = 1.5 (would look the same for M2 /M1 = 1.5). c Same calculation as for panel (a) but as a function of M2 /M1 (for C2 /C1 = 2). d Same calculation as for panel (c) but for C2 /C1 = 0.5

(a)

(b)

Fig. 5.27 Mode patterns for two states of the diatomic linear chain (N = 32 unit cells, M1 = M2 ) a within the gap for C2 /C1 = 1/2 and b closest to the gap for C2 /C1 = 2. The amplitudes of A-sites (B-sites) are shown in red (blue)

118

5 Mechanical Properties

Fig. 5.28 Linear thermal expansion coefficient of silicon (solid circles) and germanium (open circles). Adapted from [394] based on experimental data from various sources. Dashed lines are guide to the eye

5.3 Elasticity The elastic properties of the semiconductor are important if the semiconductor is subjected to external forces (pressure, temperature) or to lattice mismatch during heteroepitaxy.

5.3.1 Thermal Expansion The lattice constant depends on temperature. The (linear) thermal expansion coefficient is defined as

∂a0 (T )

α(T0 ) = ∂ T T =T0

(5.49)

and is temperature dependent. The temperature dependence of α for silicon and germanium is shown in Fig. 5.28. α is approximately proportional to the heat capacity (CV ) except at low temperatures. The negative values are due to negative Grüneisen parameters [394]. These anharmonicity effects are discussed in detail in [366].

5.3.2 Stress–Strain Relation In this section, we recall the classical theory of elasticity [395]. The solid is treated as a continuous medium (piecewise homogeneous) and the displacement vector is thus a continuous function u(r) of the spatial coordinates. When the spatial variation ∇u of u is small, the elastic energy can be written as

5.3 Elasticity

(a)

119

(b)

(c)

(d)

Fig. 5.29 Deformation of a square (a). (b) Pure hydrostatic deformation (x x = yy = 0.2, x y = 0), (c) pure shear deformation (x x = yy = 0, x y = 0.2), and (d) mixed deformation (x x = yy = 0.1, x y = 0.1)

1 U= 2

∂u n 3 ∂u l Cklmn d r, ∂ xk ∂ xm

(5.50)

where C is the (macroscopic) tensor of the elastic coefficients. 21 components of this tensor can be independent. For crystals with cubic symmetry the number of independent constants is reduced to 3. An exchange k ↔ l and m ↔ n does not matter, only six indices have to be considered (x x, yy, zz, yz, x z, and x y). The strain components i j are symmetrized according to i j =

1 2

∂u j ∂u i + ∂ xi ∂x j

.

The strains x x are along the main axes of the crystal as visualized in Fig. 5.29. The stresses8 σkl are then given by σkl = Cklmn mn .

(5.51)

(5.52)

The inverse relation is mediated by the stiffness tensor S. kl = Sklmn σmn .

(5.53)

Typically, the strain components ei j or ei are used with the convention x x → 1, yy → 2, zz → 3, yz → 4, x z → 5, and x y → 6 (Voigt notation): ei j = i j (2 − δi j ) .

(5.54)

Then, σm = Cmn en with the Ci j being the elastic constants. The x, y, and z directions are the main axes of the cubic solid, i.e. the 100 directions. For zincblende material, the stress–strain relation reads9 ⎛ ⎞ ⎛ ⎞⎛ ⎞ C11 C12 C12 0 e1 σ1 0 0 ⎜ σ2 ⎟ ⎜ C12 C11 C12 0 ⎟ ⎜ e2 ⎟ 0 0 ⎜ ⎟ ⎜ ⎟⎜ ⎟ ⎜ ⎟ ⎜ σ3 ⎟ ⎜ C12 C12 C11 0 0 0 ⎟ ⎜ ⎟=⎜ ⎟ ⎜ e3 ⎟ . (5.55) ⎜ ⎟ ⎜ σ4 ⎟ ⎜ 0 ⎟ 0 0 0 0 C 44 ⎜ ⎟ ⎜ ⎟ ⎜ e4 ⎟ ⎝ σ5 ⎠ ⎝ 0 0 0 0 C44 0 ⎠ ⎝ e5 ⎠ 0 0 0 0 0 C44 σ6 e6 Values of the compliances for several semiconductors are given in Table 5.2. The inverse relation is given by the matrix 8 The 9C

11

stress is a force per unit area and has the dimensions of a pressure. = C1111 , C12 = C1122 and C44 = C1212 = C1221 = C2121 = C2112 .

120

5 Mechanical Properties

Table 5.2 Elastic constants (in GPa) of some cubic semiconductors at room temperature. IK refers to the Keating criterion (5.59) Material

C11

C12

C44

IK

C Si Ge BN GaAs InAs AlAs ZnS MgO

1076.4 165.8 128.5 820 119 83.3 120.5 104.6 297

125.2 63.9 48.3 190 53.4 45.3 46.86 65.3 156

577.4 79.6 66.8 480 59.6 39.6 59.4 46.3 95.3

1.005 1.004 1.08 1.11 1.12 1.22 1.03 1.33 0.80

⎛

⎞ S11 S12 S12 0 0 0 ⎜ S12 S11 S12 0 0 0 ⎟ ⎜ ⎟ ⎜ S12 S12 S11 0 0 0 ⎟ ⎜ ⎟ , ⎜ 0 0 ⎟ 0 0 S44 0 ⎜ ⎟ ⎝ 0 0 0 0 S44 0 ⎠ 0 0 0 0 0 S44

(5.56)

with the stiffness coefficients in this notation given by C11 + C12 (C11 − C12 ) (C11 + 2C12 ) C12 = 2 2 −C11 − C11 C12 + 2C12 1 = . C44

S11 =

(5.57a)

S12

(5.57b)

S44

(5.57c)

We emphasize that in this convention (also called the engineering convention), e.g. e1 = x x and e4 = 2 yz . There is also another convention (the physical convention) without this factor of two; in this case the matrix in (5.55) contains the elements 2C44 . We introduce C0 = 2 C44 + C12 − C11 ,

(5.58)

and note that C0 = 0 for an isotropic material. The relation IK =

2 C44 (C11 + C12 ) =1 (C11 − C12 ) (C11 + 3C12 )

(5.59)

known as the Keating criterion [396, 397], stems from the consideration of bending and stretching of the tetrahedral bonds in the valence force field (VFF) model. It is closely fulfilled (Table 5.2) for many tetrahedrally bonded semiconductors, in particular for the covalent ones. For MgO, the Keating criterion is not fulfilled because it has (six-fold coordinated) rocksalt structure and is thus not tetrahedrally bonded. The Young’s modulus Y , σnn = Y (n) nn , (5.60)

5.3 Elasticity

121

Fig. 5.30 Elastic constants as a function of ionicity for various semiconductors with diamond or zincblende (circles) and wurtzite (squares) structure. Constants are normalized by the modulus C0 = e2 /d 4 , d being the average nearest-neighbor ∗ = C /C . distance. a Bulk modulus, B ∗ = (C11 + 2C12 )/(3C0 ), (b, c) shear moduli, b CS∗ = (C11 − C12 )/C0 , c C44 44 0 Solid lines are a simple model as discussed in [402]. Adapted from [403]

generally depends on the normal direction n of a strain. It is equivalent to 1/S11 of (5.57a). For isotropic material Y and the Poisson ratio ν are related to the elastic constants of cubic material by Y = C11 − ν=

2 2 C12 C11 + C12

C12 . C11 + C12

(5.61a) (5.61b)

For isotropic materials also Lamé’s constants λ and μ are used. They are given by10 C11 = λ + 2μ, C12 = λ and C44 = μ (note that C0 according to (5.58) is zero). The bulk modulus B (inverse of the compressibility), 1 ∂V 1 =− , B V ∂p for the zincblende crystal is given as B=

C11 + 2 C12 . 3

(5.62)

(5.63)

We note that Y , ν and Ci j of typical materials are both positive. Materials with negative Poisson ratio are called auxetic [398–400]. Also materials with negative compressibility are possible [401]. Beyond the dependence of the elastic constants on the bond length (as materialized in the phonon frequencies in Fig. 5.15), they depend on the ionicity. In Fig. 5.30, the elastic constants of various zincblende semiconductors are shown as a function of the ionicity f i . The values for the elastic constants are normalized by e2 /a 4 , a being the average nearest-neighbor distance. For wurtzite crystals, five elastic constant are necessary for the stress–strain relation that reads11

10 For 11 (C

an isotropic material, Ci jkl = λ δi j δkl + μ (δik δ jl + δil δ jk ). − C12 )/2 = C1212 , C44 = C1313 = C2323 .

11

122

5 Mechanical Properties

⎛

C11 C12 C13 0 0 ⎜ C12 C11 C13 0 0 ⎜ ⎜ C13 C13 C33 0 0 Ci j = ⎜ ⎜ 0 0 0 0 C 44 ⎜ ⎝ 0 0 0 0 C44 0 0 0 0 0

⎞ 0 ⎟ 0 ⎟ ⎟ 0 ⎟ . ⎟ 0 ⎟ ⎠ 0 1 (C − C ) 11 12 2

(5.64)

Experimental values for wurtzite materials are given in Table 5.3. The relation of the elastic tensor of wurtzite and zincblende materials, in particular viewed along the 111 -direction has been discussed in [403, 404]. The bulk modulus of the wurtzite crystal is given by B=

2 (C11 + C12 ) C33 − 2 C13 . C11 + C12 + 2 C33 − 4 C13

(5.65)

5.3.3 Biaxial Stress In heteroepitaxy (cf. Sect. 12.2.6), a biaxial stress situation arises, i.e. layered material is compressed (or expanded in the case of tensile strain) in the interface plane and is expanded (compressed) in the perpendicular direction.12 Here, we assume that the substrate is infinitely thick, i.e. that the interface remains planar. Substrate or wafer bending is discussed in Sect. 5.3.5. The simplest case is epitaxy on the (001) surface, i.e. e1 = e2 = . The component e3 is found from the condition σ3 = 0 (no forces in the z direction). All shear strains are zero. For zincblende material it follows C12 2 C12 (e1 + e2 ) = − . (5.66) ⊥100 = e3 = − C11 C11 In Fig. 5.31 the ratio ⊥ / is depicted for GaAs and various crystal orientations; the formulas for other orientations are more involved [409]: 2C12 − C0 /2 C11 + C0 /2 2C12 − 2C0 /3 . =− C11 + 2C0 /3

⊥110 = −

(5.67)

⊥111

(5.68)

Table 5.3 Elastic constants (in GPa) of some wurtzite semiconductors Material

C11

C12

C13

C33

C44

Refs.

GaN AlN ZnS ZnO

391 410 124 206

143 149 60.2 118

108 99 45.5 118

399 389 140 211

103 125 28.6 44

[405] [406] [407] [408]

12 In

a large amount of literature and in previous editions of this book, this situation has been labelled ‘biaxial strain’. However, there is in-plane and out-of-plane strain, thus the strain along all directions is non-zero. Since the out-of-plane stress is zero (for zero ambient pressure), it is actually a ‘biaxial stress’ situation.

5.3 Elasticity

123

(b)

(a)

Fig. 5.31 Ratio −⊥ / for GaAs under symmetric biaxial stress. The angle θ denotes the surface normal in the 110 azimuth (θ = 0: [001], θ = 90◦ : [110], the maximum of ⊥ / is for [111]). (b) is a three-dimensional visualization

For wurtzite crystals and pseudomorphic growth along [00.1] the strain along the epitaxial direction (c-axis) is given by ⊥ = −

C13 2C13 (e1 + e2 ) = − a , C33 C33

(5.69)

where ⊥ = c = (c − c0 )/c0 and a = (a − a0 )/a0 . For symmetric biaxial in-plane stress, the ratio ⊥ / is shown in Fig. 5.32 for GaN and varying angle θ of the c-axis against the epitaxy direction. For the growth of wurtzite on wurtzite for θ = 0, the epitaxial strain is actually asymmetric in the interface plane. For θ = 90◦ , e.g. the epitaxy on m-plane substrate (cmp. Fig. 3.37) (c-axis lies in-plane), the in-plane strains are e1 = a and e2 = c . For θ = 90◦ , we find ⊥ = −

C12 a + C13 c . C11

(5.70)

The situation for pseudomorphic growth in the (Al,Ga,In)N system has been discussed for various interface orientations in [410] (cmp. also Fig. 16.14). The strains ⊥ along the epitaxy direction and c along the c-direction are depicted for Al0.17 Ga0.83 N/GaN and Mg0.3 Ga0.7 O/ZnO in Fig. 5.33. The different behavior of the nitride and the oxide system, e.g. regarding the sign change of c , is due to the fact that a is negative (positive) for Alx Ga1−x N/GaN (Mgx Ga1−x O/ZnO) (c < 0 for both cases) [411]. We note that pseudomorphic growth and biaxial stress of rhombohedral/trigonal (e.g. Al2 O3 ) and monoclinic (e.g. β-Ga2 O3 ) thin films has been discussed as well [412–414]. A general treatment for all crystal symmetries and orientations has been provided in [415].

5.3.4 Three-Dimensional Stress The strain distribution in two-dimensional or three-dimensional objects such as quantum wires and dots (see also Sect. 14) is more complicated. A simple analytical solution for the problem of a strained inclusion is only possible for isotropic material parameters [416]. The solution for a sphere can be extended to yield the strain distribution of an inclusion of arbitrary shape. This scheme applies only for isotropic materials and identical elastic properties of the inclusion

124

5 Mechanical Properties

(a)

(b)

Fig. 5.32 Ratio −⊥ / for GaN under symmetric biaxial stress. In a θ denotes the angle of the c-axis with respect to the surface normal, b is a three-dimensional visualization, showing the in-plane isotropy

Fig. 5.33 Strains c (dashed lines) and ⊥ (solid lines) for Al0.17 Ga0.83 N/GaN (blue) and Mg0.3 Ga0.7 O/ZnO (red) as a function of the interface tilt angle θ with respect to [00.1]

and the surrounding matrix. The solution will be given in terms of a surface integral of the boundary of the inclusion, which is fairly easy to handle. Several disconnected inclusions can be treated by a sequence of surface integrals. The strain distribution for the inner and outer parts of a sphere with radius ρ0 is given (in spherical coordinates) by 2 0 3 2 = 0 3

in = ρρ out ρρ

1 − 2ν in in = θθ = φφ 1−ν 1 + ν ρ0 3 out out = −2θθ = −2φφ , 1−ν ρ

(5.71) (5.72)

where ρ denotes the radius, ν the Poisson ratio, and 0 the relative lattice mismatch of the inclusion and the matrix. The radial displacements are 2 0 3 2 = 0 3

u in ρ = u out ρ

1 − 2ν ρ 1−ν 1 − 2ν 3 1 ρ . 1 − ν 0 ρ2

(5.73) (5.74)

5.3 Elasticity

125

Fig. 5.34 Strain components in an InAs pyramid (quantum dot with {101} faces), embedded in GaAs. The cross section is through the center of the pyramid. The lattice mismatch between InAs and GaAs amounts to ≈ −7%. Reprinted with c permission from [417], 1995 APS

Dividing the displacement by the sphere’s volume, we obtain the displacement per unit volume of the inclusion. From the displacement we can derive the stress σi0j per unit volume. 1 Y 0 2xi2 − x j − xk 4π 1 − ν ρ5 3 1 Y 0 x i x j , σi0j = 2 4π 1 − ν ρ 5 σii0 =

(5.75) (5.76)

where i, j and k are pairwise unequal indices. Due to the linear superposition of stresses, the stress distribution σiVj for the arbitrary inclusion of volume V can be obtained by integrating over V σiVj =

σi0j (r − r0 ) d3 r .

(5.77)

V

The strains can be calculated from the stresses. When 0 is constant within V , the volume integral can be readily transformed into an integral over the surface ∂ V of V using Gauss’ theorem. With the ‘vector potentials’ Ai j we fulfill divAi j = σi j . 1 Y 0 xi ei 4π 1 − ν ρ 3 1 1 Y 0 xi e j + x j ei . Ai j = − 2 4π 1 − ν ρ3 Aii = −

(5.78) (5.79)

Equation (5.79) is valid for the case i = j. ei is the unit vector in the i-th direction. However, special care must be taken at the singularity r = r0 if r0 lies within V because the stress within the ‘δ-inclusion’ is not singular (in contrast to the electrostatic analog of a δ-charge). Thus, we find " σiVj (r0 ) =

Ai j dS + δi j ∂V

Y 0 1−ν

δ(r − r0 ) d3 r .

(5.80)

V

As an example, we show in Fig. 5.34 the numerically calculated strain components [417] (taking into account the different elastic properties of the dot and matrix materials) in the cross section of

126

5 Mechanical Properties

a pyramidal InAs quantum dot in a GaAs matrix on top of a two-dimensional InAs layer. The strain component zz is positive in the 2D layer, as expected from (5.66). However, in the pyramid zz exhibits a complicated dependence and even takes negative values at the apex.

5.3.5 Substrate Bending If a lattice-mismatched layer is pseudomorphically grown on top of a substrate it suffers biaxial strain. For finite substrate thickness part of the strain will relax via substrate bending. If the substrate is circular, a spherical cap is formed. If the lattice constant of the film is larger (smaller) than that of the substrate, the film is under compressive (tensile) strain and the curvature is convex (concave) with respect to the outward normal given by the growth direction (Fig. 5.35a). Substrate bending can also be induced by a f s and αth of the film and substrate, respectively. If a mismatch of the thermal expansion coefficients αth film/substrate system is flat at a given temperature, e.g. growth temperature, a decrease of temperature, f s is smaller (larger) than αth . e.g. during cooling, will lead to compressive (tensile) strain if αth t In a curved structure, the lattice constant in the tangential direction increases from ai at the inner surface (r = R = κ −1 ) to aut at the outer surface (r = R + d). Thus, the tangential lattice constant varies with the radial position a t (r ) = ait (1 + r κ) , (5.81) where d is the layer thickness (Fig. 5.35b). Therefore au = ai (1 + d/R). We note that (5.81) holds in all layers of a heterostructure, i.e. the film and the substrate. The lattice constant in the radial direction a r , however, depends on the lattice constant a0 of the local material and is calculated from the biaxial strain condition, such as (5.66). The in-plane strain is = (a t − a0 )/a0 (we assume a spherical cap with = θθ = φφ ). For an isotropic material we find a r = a0 (1 + ⊥ ) with ⊥ = −2ν /(1 − ν). The local strain energy density U is given by U=

Y 2 . 1−ν

(5.82)

The total strain energy per unit area U of a system of two layers with lattice constants a1 , a2 , Young’s moduli Y1 , Y2 and thickness d1 , d2 (we assume the same Poisson constant ν in both layers) is

d1

U =

d2 U1 dr +

0

U2 dr .

(5.83)

d1

The total strain energy needs to be minimized with respect to ai and R in order to find the equilibrium curvature κ. We find au

compressive

d

tensile

ai R

(a)

(b)

Fig. 5.35 a Schematic bending of a film/substrate system for compressive (left) and tensile (right) film strain. b Schematic deformation of curved film of thickness d. The lattice constants at the inner and outer surface are ai and au , respectively

5.3 Elasticity

127

epitaxy

1100

cooling

-0.05

1070

-0.1

1060 1050

0.0

-1

Temperature (°C)

6K

1080

Curvature (m )

0.05

1090

0

200 400 600 800 1000 1200 1400 Time (s)

-0.15

Fig. 5.36 Curvature of the middle of a Si wafer during GaN growth on an AlN interlayer grown at low temperatures on GaN and subsequent cooling. During growth the decrease in curvature indicates convex bowing due to compressive stress; during cooling the wafer flattens and becomes concave due to thermally induced tensile stress. Adapted from [422]

6a1 a2 (a2 − a1 ) d1 d2 (d1 + d2 ) Y1 Y2 a23 d14 Y12 + α Y1 Y2 + a13 d24 Y24 α = a1 a2 d1 d2 −a2 d1 (2d1 + 3d2 ) + a1 (6d12 + 9d1 d2 + 4d22 ) . κ=

(5.84)

For a2 = a1 (1 + ) we develop κ to first order of and find (χ = Y2 /Y1 ) [418, 419] κ=

d14

+ 4χ

d13

6χ d1 d2 (d1 + d2 ) . d2 + 6χ d12 d22 + 4χ d1 d23 + χ 2 d24

(5.85)

In the case of a substrate (ds ) with a thin epitaxial layer (df ds ), the radius of curvature is approximately (Stoney’s formula [420]) df Yf κ = 6 2 . (5.86) ds Ys Conversely, if the radius of curvature is measured [421], e.g. optically, the film curvature (and through models also the film strain) can be determined during epitaxy as depicted in Fig. 5.36.

5.3.6 Scrolling In some cases cylindrically scrolled structures are important, e.g. for thin-film flexible electronics, nanotubes, nanoscrolls or nanohelixes. The scrolling of thin layers must be avoided by suitable strain management for thin layers that are lifted off from their substrate for transfer to another flat substrate. If the film remains attached to its substrate, a scroll can be fabricated as schematically shown in Fig. 5.37. Such structures were first reported in [423], a review can be found in [424]. The shape of such scroll is investigated in [425] without a priori assumptions on its shape.

128

5 Mechanical Properties

(a)

(b)

(c)

Fig. 5.37 Schematic representation of nanoscroll formation. a Strained heterostructure (blue/green) that is planar due to large substrate thickness, b starting removal of sacrificial layer (black), c release of thin film into nanoscroll geometry

t

y

r

(a)

(b)

Fig. 5.38 a Schematic representation of a cylindrically rolled sheet with radial direction r , tangential direction t and direction along the cylinder axis y. b SEM images of multiwall (In,Ga)As/GaAs nanoscroll rolled up over about 50 µm. Part (b) from [426]

If bending strain occurs only in one of the tangential directions, the energy density is given by U=

Y ( 2 + y2 + 2ν t y ) , 2 (1 − ν 2 ) t

(5.87)

where y is the strain in the unbent direction (cylinder axis) as shown in Fig. 5.38a. For a strained heterostructure made up from two layers the curvature is given by (calculated analogous to (5.85), χ = Y2 /Y1 [419]) 6(1 + ν) χ d1 d2 (d1 + d2 ) κ= 4 , (5.88) d1 + 4χ d13 d2 + 6χ d12 d22 + 4χ d1 d23 + χ 2 d24 which differs from (5.85) only by the factor 1 + ν in the nominator. For cubic material and a (001) surface the energy is given as U100 =

C11 − C12 C11 (t2 + y2 + C12 (t + y )2 ) 2C11

(5.89)

for a scrolling direction along 100 . When the (001)-oriented film winds up along a direction hk0 having an angle φ with the [100] direction (φ = 45◦ for 110 ), the strain energy is given by (C0 is given by (5.58)) t − y 2 2 Uφ = U100 + C0 sin (2φ) . (5.90) 2

5.3 Elasticity

129

=14° [010] [100]

(a)

(b)

Fig. 5.39 a Strain energy (in units of the strain energy of the flat pseudomorphic layers) of a scroll of a 4-layer SiGe structure (Si0.3 Ge0.7 , Si0.6 Ge0.4 and Si0.8 Ge0.2 , each 3 nm thick and a 1 nm Si cap) as a function of radius for winding directions along 100 and 110 . Top (bottom) curves without (with complete) strain relaxation along the cylinder axis. Vertical lines indicate the positions of the respective energy minima [419]. b SEM image of curled (In, Ga)As/GaAs nanoscroll rolled φ = 14◦ off 100 . The stripe from which the film was rolled off is indicated by white dashed lines. Part (b) from [429]

The strain energy versus bending radius (= κ −1 ) is shown for a SiGe nanoscroll in Fig. 5.39. First, the relaxation along the cylinder axis plays a minor role. The smallest strain energy is reached for scrolling along 100 , also yielding the smaller bending radius (larger curvature). Therefore, the film preferentially scrolls along 100 . This explains the observed ‘curl’ behavior of scrolls winding up for φ = 0 [423, 427] (Fig. 5.39b). The effect of surface strain needs to be included to yield improved quantitative agreement with experimental values of κ(, d) [428].

5.4 Plasticity 5.4.1 Critical Thickness Strained epitaxial films are called pseudomorphic when they do not contain defects and the strain relaxes elastically, e.g. by tetragonal distortion. When the layer thickness increases, however, strain energy is accumulated that will lead at some point to plastic relaxation via the formation of defects. In many cases, a grid of misfit dislocations forms at the interface (Figs. 4.18 and 5.40). In Fig. 5.41 the strain around misfit dislocations at a GaAs/CdTe heterointerface, as calculated from a TEM image (Fig. 4.14), is shown. The average distance p of the dislocations is related to the misfit√f = (a1 − a2 )/a2 and the edge component b⊥ of the Burger’s vector (for a 60◦ dislocation b⊥ = a0 / 8) p=

b⊥ . f

(5.91)

Two mechanisms have been proposed for the formation of misfit dislocations (Fig. 5.42), the elongation of a grown-in threading dislocation [432, 433] and the nucleation and growth of dislocation half-loops [434]. For the modeling of such systems a mechanical approach based on the forces on dislocations [432] or an energy consideration based on the minimum strain energy necessary for defect formation

130

5 Mechanical Properties

[434–437] can be followed. Both approaches have been shown to be equivalent [438] (if a periodic array of dislocations is considered). In [439] it was pointed out that the finite speed of plastic flow also has to be considered to explain experimental data. Temperature affects the observed critical thickness and a kinetic model is needed. Another way of introducing dislocations is the plastic relaxation at the edge of coherent strained islands (cmp. Fig. 14.37). In the following, isotropic materials and identical elastic constants of substrate and thin film are assumed, following [438]. The interface plane is the (x,y)-plane, the growth direction is z. The energy E d of a periodic dislocation array with period p and Burgers vector b = (b1 , b2 , b3 ) is Ed =

Y β2 8π (1 − ν 2 )

(5.92)

β 2 = b12 + (1 − ν) b22 + b32 ln

p 1 − exp(−4π h/ p) 2π q

4π h exp(−4π h/ p) + b12 − b32 p 1 − exp(−4π h/ p) 1 exp(−4π h/ p) 4π h 2 − b12 + b32 2 2 p 1 − exp(−4π h/ p) 2π h exp(−2π h/ p) , +b32 p 1 − exp(−2π h/ p) where h is the film thickness and q denotes the cutoff length for the dislocation core, taken as q = b. The misfit strain including the relaxation due to dislocations with Burger’s vectors b and bˆ in the ˆ We chose the coordinate system such that n = two orthogonal interface 110 directions n and n. ˆ (1, 0, 0) and n = (0, 1, 0) (the z direction remains). With respect to these axes the Burger’s vectors are √ 1 1 √1 m ± 2 , 2 , 2 a0 / 2. The misfit strain i j is reduced due to the dislocation formation to the ‘relaxed’ misfit strain irj with bˆi nˆ j + bˆ j nˆ i bi n j + b j n i + , (5.93) irj = imj + 2p 2p

(a)

(b)

g 002

Fig. 5.40 a Series of cross-sectional TEM images of 100 nm thick Gex Si1−x layers on Si(001) with different ternary compositions x = 0.1, 0.2, 0.5, and 1.0. The growth temperature was 550 ◦ C. The transition from commensurate to incommensurate growth is obvious. Adapted from [430]. b Plan view 022 TEM bright field image of a 250 nm Ge0.15 Si0.85 layer on Si (001), annealed at about 700 ◦ C. The arrow denotes the position of a dislocation loop. Reprinted c with permission from [431], 1989 AVS

5.4 Plasticity

131

xz of the strain tensor (with respect to the GaAs lattice constant) of the dislocation array Fig. 5.41 Components xzxx zz shown in Fig. 4.14, red/blue: positive/negative value, white: zero. From [321]

c

h3 h2

a

h1

b

c

b

a

(a)

(b)

Fig. 5.42 Schematic formation of misfit dislocations by a elongation of a grown-in threading dislocation and b by the nucleation and growth of dislocation half-loops. a depicts a threading dislocation. Initially, for thickness h 1 the interface is coherent ‘a’, for larger thickness h 2 the interface is critical and the force of the interface on the dislocation is equal to the tension in the dislocation line, ‘b’. For larger thickness, e.g. h 3 , the dislocation line is elongated in the plane of the interface, ‘c’. In b ‘a’ denotes a subcritical dislocation half-loop, ‘b’ depicts a half-loop being stable under the misfit stress and for ‘c’ the loop has grown under the misfit stress into a misfit dislocation line along the interface

with an associated stress σi j . The strain energy E s of the layer due to the relaxed misfit is then 1 h σi j irj 2 Y (1 + ν) 2 lim E s = 2h f . p→∞ 1−ν Es =

(5.94) (5.95)

The total strain energy E is given by pE = 2E d + 2E c + p E s E ∞ = lim E , p→∞

(5.96) (5.97)

with the core energy E c of the dislocation that needs to be calculated with an atomistic model (not considered further here). This energy is shown in Fig. 5.43a for the material parameters of Ge0.1 Si0.9 /Si(001) (misfit −0.4%) for various layer thicknesses as a function of 1/ p. This plot looks similar to that for a first-order phase transition (with 1/ p as the order parameter). For a certain critical thickness h c1 the

132

5 Mechanical Properties

energy of the layer without any dislocation and the layer with a particular dislocation density p1 are identical (E − E ∞ = 0) and additionally ∂ E/∂ p| p= p1 = 0. However, between p → ∞ and p = p0 there is an energy barrier. The critical thickness h c2 is reached when ∂ E/∂ p | p→∞ = 0 ,

(5.98)

i.e. the energy decreases monotonically for increasing dislocation density up to the global energy minimum at a certain equilibrium dislocation spacing p2 . Equation (5.98) leads to the following implicit equation for the determination of h c2 : h c2 =

b −16 + 3b2 + 8 (−4 + ν) ln (2h c2 /q) , 128 f π (1 + ν)

(5.99)

√ with the length of the Burgers vector b = a0 / 2. The theoretical dependence of h c2 for Gex Si1−x /Si(001) with varying composition is shown in Fig. 5.43b together with experimental data. The critical thickness for a fairly high growth temperature is much closer to the energetic equilibrium than that deposited at lower temperature. This shows that there are kinetic limitations for the system to reach the mechanical equilibrium state. Also, the experimental determination of the critical thickness is affected by finite resolution for large dislocation spacing, leading generally to an overestimate of h c . In zincblende materials, two types of dislocations are possible, α and β, with Ga- and As-based ¯ cores, respectively. They have [110] and [110] line directions for a compressively strained interface. The α dislocation has the larger glide velocity. Therefore, strain relaxation can be anisotropic with regard to the 110 directions for zincblende material, e.g. (In,Ga)As/GaAs [441, 442]. A more complicated relaxation situation is visualized in Fig. 4.18 for an Al0.13 Ga0.87 N/GaN het¯ substrate. Below the critical thickness only threading dislocations stemming erostructure on (3031) from the substrate are visible. Above the critical thickness, misfit dislocations have developed along three directions which related to the intersections of the basal c-plane (00.1) and two prismatic m-plane ¯ interface plane [324, 443]. We like to mention that cathodolumi{10.1} glide systems with the (3031)

(a)

(b)

Fig. 5.43 a Theoretical calculation for the strain energy versus inverse dislocation density for various thicknesses of Ge0.1 Si0.9 layers on Si (001). The ordinate is b/2 p, b/2 being the edge component of the Burgers vector and p being the dislocation spacing. The abscissa is the strain energy E scaled with E ∞ (5.97). (b) Critical thickness for Gex Si1−x layers on Si (001). The solid line is theory (h c2 ) according to (5.99). Data points are from [440] (squares, growth temperature of 750 ◦ C) and from [430] (triangles for growth temperature of 550 ◦ C)

5.4 Plasticity

133

Fig. 5.44 Cleaving planes of the a diamond and b zincblende lattice

(a)

Fig. 5.45 Scanning tunneling microscopy images of a cleaved GaAs (110) surface with a good cleave and b bad cleave with defects dominating. Adapted from [446]

(a)

(b)

(b)

10 nm nescence (or X-ray imaging) offer a quite high sensitivity for plastic relaxation since a small number of dislocations can be detected in relatively large areas (while TEM finds defects but only within small areas and X-ray diffraction looks at large area but has only a low strain sensitivity).

5.4.2 Cleaving The cleavage planes of the diamond structure are {111} planes (Fig. 5.44a). It is easiest to break the bonds connecting the double layers in the 111 directions. The cleavage planes of the zincblende structure are {110} planes (Fig. 5.44b). Due to the ionic character, breaking the bonds connecting the double layers in the 111 directions would leave charged surfaces, which is energetically unfavorable. The {100} planes contain only one sort of atom and would also leave highly charged surfaces. The {110} planes contain equal amounts of A- and B-atoms and are neutral. Ideally, the cleaving plane is atomically flat (Fig. 5.45a) or exhibits large mono-atomically flat terraces. However, certain dopants in high concentrations, e.g. GaAs:Te, can induce a rough surface due to lattice distortion [444]. ¯ (m-type) planes [445]. The natural cleavage planes of wurtzite (GaN) are {11.0}

5.4.3 Wafer Breakage The thickness and thus strength of wafers for semiconductor production (cmp. Sect. 12.2.2) is an important issue. The wafer should be as thin as possible for saving expensive materials but thick enough to avoid loss due to stress during handling, in particular during the later steps in a process since the value of a wafer increases with number of process steps it has undergone.

134

5 Mechanical Properties

Reasons for wafer breakage is the mechanical handling (pick, place, transport) [447], stress loads due to processing (dielectrics, metals, asymmetric structures) and stress during processing for example due to thermal loads in annealing or deposition steps and cutting/dicing. The problem is less important in microelectronics but especially severe in photovoltaics (PV) industry, handling large total areas; on the other hand the profit loss per broken wafer is much higher in the microelectronics industry. An additional problem poses the grain structure of multicrystalline silicon wafers used for PV [448] and the effect of surface cracks and irregularities at wafer edges and corners. Just going from a wafer thickness of 270 µm to 250 µm can more than double the breakage rate at certain process steps [449]. The minimum strength of a wafer with surface cracks is about 100 MPa, while the strength of wafers with cracks at the edge can reach rather low values around 20 MPa. Also the careful shaping of the wafer edge is important to avoid breakage [450].

Chapter 6

Band Structure

Silicon is a metal. A.H. Wilson, 1931 [74]

Abstract A treatment of electron states in one-dimensional potentials introduces into the concepts of band gap and effective mass. The band structures of various semiconductors are reviewed. The systematics of band gaps, symmetry considerations, band gaps in alloys, amorphous semiconductors and the effect of strain and temperature are discussed. Electron and hole dispersions are treated and the density of states in various dimensions is derived.

6.1 Introduction Valence electrons that move in the crystals feel a periodic potential U (r) = U (r + R)

(6.1)

for all vectors R of the direct lattice. The potential1 is due to the effect of the ion cores and all other electrons. Thus a serious many-body problem is present. In principle, the band structure can be calculated from the periodic arrangements of the atoms and their atomic order number. We note that for some problems, e.g. the design of optimal solar cells, a certain band structure is known to be ideal and a periodic atomic arrangement, i.e. a material, needs to be found that generates the optimal band structure. This problem is called the inverse band structure problem.

6.2 Electrons in a Periodic Potential 6.2.1 Bloch’s Theorem First, we will deduce some general conclusions about the structure of the solution as a consequence of the periodicity of the potential. We first investigate the solution of a Schrödinger equation of the type 1 In

this book the form of the potential will never be explicitly given.

© Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_6

135

136

6 Band Structure

(a)

(b)

(c)

Fig. 6.1 Zone schemes for a band structure: a extended, b reduced and c repetitive zone scheme

2 2 ∇ + U (r) (r) = E (r) H (r) = − 2m

(6.2)

for an electron. U will be periodic with the lattice, i.e. it will obey (6.1). Bloch’s theorem says that the eigenstates of a one-particle Hamiltonian as in (6.2) can be written as the product of plane waves and a lattice-periodic function, i.e. nk (r) = A exp(i k r) u nk (r) .

(6.3)

√ The normalization constant A is often omitted. If u nk (r) is normalized, A = 1/ V , where V is the integration volume. The wavefunction is indexed with a quantum number n and the wavevector k. The key is that the function u nk (r), the so-called Bloch function, is periodic with the lattice, i.e. u nk (r) = u nk (r + R)

(6.4)

for all vectors R of the direct lattice. The proof is simple in one dimension and more involved in three dimensions with possibly degenerate wavefunctions, see [451]. If E nk is an energy eigenvalue, then E nk+G is also an eigenvalue for all vectors G of the reciprocal lattice, i.e. (6.5) E n (k) = E n (k + G) . Thus the energy values are periodic in reciprocal space. The proof is simple, since the wavefunction (for k + G) exp(i(k + G)r)u n(k+G) (r) is for u n(k+G) (r) = exp(−iGr)u nk (r) obviously an eigenfunction to k. A band structure along one k-direction can be displayed in various zone schemes as depicted in Fig. 6.1. The most frequently used scheme is the reduced zone scheme. In three dimensions, the band structure is typically shown along particular paths in the Brillouin zone, as depicted, e.g., in Fig. 6.2c.

6.2.2 Free-Electron Dispersion If the entire wavefunction (from (6.3)) obeys the Schrödinger equation (6.2), the Bloch function u nk fulfills the equation

6.2 Electrons in a Periodic Potential

137

X

4 3 2 1

(a)

(b)

(c)

0

X W

L

K X

Fig. 6.2 Dispersion of free electrons (empty lattice calculation, U = 0, shown in the first Brillouin zone) in a a onedimensional lattice (G = n 2π/a), b a simple cubic lattice (G = (h, k, l) 2π/a) and c in a fcc lattice. The energy is measured in units of the energy at the X-point, E X = (2 /2m)(π/a)2 . The shaded circle in (c) represents the region where the band gap develops for finite periodic potential U = 0

1 (p + k)2 + U (r) u nk (r) = E nk u nk (r) , 2m

(6.6)

which is easy to see from p = −i∇. First, we discuss the simplest case of a periodic potential, U ≡ 0. This calculation is also called the empty lattice calculation. The solution of (6.6) is then just constant, i.e. u k = c and k (r) = c exp(ikr). The dispersion of the free electron is then given by E(k) =

2 2 k , 2m

(6.7)

where k is an arbitrary vector in the reciprocal space. k is a vector from the Brillouin zone such that k = k + G with a suitable reciprocal lattice vector G. Because of (6.5) the dispersion relation can be written also as 2 (k + G)2 , (6.8) E(k) = 2m where k denotes a vector from the Brillouin zone. Thus, many branches of the dispersion relation arise from using various reciprocal lattice vectors in (6.8). The resulting dispersion relation for the free electron is shown in Fig. 6.2a for a one-dimensional system (k and G are parallel) and in Fig. 6.2b for the simple cubic lattice (in the so-called reduced zone scheme). In Fig. 6.2c, the (same) dispersion of the free electron is shown for the fcc lattice.

6.2.3 Non-Vanishing Potential Now the effect of a non-vanishing periodic potential on electron motion will be discussed. A simple, analytically solvable model that visualizes the effect of a periodic potential on the dispersion relation of the electrons and the formation of a (one-dimensional) band structure with gaps is the Kronig-Penney model [71] which is discussed in the Appendix F.

138

6.2.3.1

6 Band Structure

General Wave Equation

In this section, we will discuss the solution of a general wave equation for electrons in a periodic potential. The solution is investigated particularly at the zone boundary. The potential U is periodic with the lattice (6.1). It can be represented as a Fourier series with the reciprocal lattice vectors (lattice vector expansion, cf. (3.19)): UG exp (i G r) . (6.9) U (r) = G

Since U is a real function, U−G = UG∗ . The deeper reason for the success of such an approach is that for typical crystal potentials, the Fourier coefficients decrease rapidly with increasing G, e.g. for the unscreened Coulomb potential UG ∝ 1/G 2 . The wavefunction is expressed as a Fourier series (or integral) over all allowed (Bloch) wavevectors K, (r) =

CK exp (i K r) .

(6.10)

K

The kinetic and potential energy terms in the Schrödinger equation (6.6) are ∇2 = −

K2 CK exp (i K r)

(6.11a)

K

U =

G

UG CK exp (i (G + K) r) .

(6.11b)

K

With K = K + G, (6.11b) can be rewritten as U =

G

UG CK −G exp i K r .

(6.12)

K

Now, the Schrödinger equation can be written as an (infinite) system of algebraic equations: (λK − E) CK +

UG CK−G = 0 ,

(6.13)

G

with λK = 2 K2 /(2m).

6.2.3.2

Solution for One Fourier Coefficient

The simplest (non-trivial) potential energy has only one important Fourier coefficient −U (U > 0) for the shortest reciprocal lattice vector G. Also, we have U−G = UG . Thus, the (one-dimensional) potential has the form U (x) = −2 U cos(Gx). Then the equation system (6.13) has only two equations for CK and CK−G , leading to the condition λK − E −U −U λK−G − E = 0 . We find two solutions λK + λK−G E± = ± 2

λK − λK−G 2

(6.14)

2 + U2 .

(6.15)

6.2 Electrons in a Periodic Potential

139

Fig. 6.3 Periodic potential U (one-dimensional cosine, black) and the squares of the wavefunctions − (red) and + (blue) for the wavevector at the zone boundary, K = G/2 = π/a

6.2.3.3

Solution at the Zone Boundary

We consider the solution at the zone boundary, i.e. at K = G/2. The kinetic energy is then the same for K = ±G/2, i.e. λK = λK−G = (2 /2m) (G 2 /4) = λ. The determinant (6.14) reads then (λ − E)2 − U 2 = 0 .

(6.16)

Thus the energy values at the zone boundary are E± = λ ± U =

2 G 2 ±U . 2m 4

(6.17)

At the zone boundary, a splitting of the size E + − E − = 2U occurs. The center of the energy gap is given by the energy λK of the free-electron dispersion. The ratio of the coefficients is CG/2 /C−G/2 = ∓1. The ‘−’ solution of (6.17) (lower energy) is a standing cosine wave (− ), the ‘+’ solution (+ ) is a standing sine wave as visualized in Fig. 6.3. For the lower-energy (binding) state the electrons are localized at the potential minima, i.e. at the atoms, for the upper state (antibinding) the electrons are localized between the atoms. Both wavefunctions have the same periodicity since they belong to the same wavevector K = G/2. We note that the periodicity of is 2a, while the periodicity of 2 is equal to the lattice constant a.

6.2.3.4

Gap States

For energies within the gap, solutions with a complex wavevector K = G/2 + i q exist. Solving (6.16) results (in terms of q 2 = (2 /2m) q 2 ) to E± = λ − q ± 2

−4 λ q 2 + U 2 .

(6.18)

For energies E = λ + with −U ≤ ≤ U , the complex part of the wavevector is given by q 2 = −( + 2λ) +

4λ ( + λ) + U 2 .

(6.19)

The maximum value of q is in the center of the band gap ( = 0); for |U | 2 λ, it is q 2max ≈ U 2 /(4λ). At the band edges ( = ±U ), q = 0. q is the characteristic length of an exponentially decaying wave

140

6 Band Structure 0.25

Complex wavevector q'

Fig. 6.4 Complex band structure q () according to (6.19) for two different values of λ/U

=5U

0.2

0.15 =10U

0.1

0.05

0

1

0.5

0 /U

0.5

1

function. Such solutions occur at surfaces or interfaces. For larger band gaps, the localization length is smaller (larger q) (Fig. 6.4).

6.2.3.5

Solution in the Vicinity of the Zone Boundary

For K in the vicinity of the zone boundary the solutions (6.15) can be developed. Therefore, we use

= K − G/2. With λ = (2 /2m) (G 2 /4) we rewrite the (small) distance from the zone boundary K still exactly (6.15): 2

= E± K 2m

with For small K

2 GK 2m

1/2

2 2 K 1 2 2 G + K ± 4λ + U2 . 4 2m

(6.20)

|U |, the energy is then approximately given by

2 2 K

∼ E± K = λ±U + 2m

2λ 1± . U

(6.21)

Thus the energy dispersion in the vicinity of the zone boundary is parabolic. The lower state has a negative curvature, the upper state a positive curvature. The curvature is m∗ = m

U 1 ≈ ±m , 1 ± 2λ/U 2λ

(6.22)

and will be later related to the effective mass. The approximation in (6.22) is valid for |U | 2λ. We note that in our simple model m ∗ increases linearly with increasing band gap 2U (see Fig. 6.34 for experimental data).

6.2.4 Kramer’s Degeneracy E n (k) is the dispersion in a band. The time-reversal symmetry (Kramer’s degeneracy) implies E n↑ (k) = E n↓ (−k) ,

(6.23)

6.2 Electrons in a Periodic Potential

141

Spin splitting (meV)

Fig. 6.5 Theoretical calculation of the spin splitting of a the three lowest conduction bands (CB1, CB2, and CB3) and b the top three valence bands (VB1, VB2, and VB3) of GaAs. Adapted from [453]

120 100 80 60 40 20 0

(a)

(b) 120 100 80 60 40 20 0 X U,K

GaAs

W

where the arrow refers to the direction of the electron spin. If the crystal is symmetric under inversion, we have additionally (6.24) E n↑ (k) = E n↑ (−k) . With both time reversal and inversion symmetry the band structure fulfills E n↑ (k) = E n↓ (k) .

(6.25)

The inversion symmetry is particularly important for the spin-orbit interaction. In the absence of inversion symmetry, e.g. in (non-centrosymmetric) zincblende crystals (Fig. 3.16b) or in heterostructures (Fig. 12.35b), a spin splitting, e.g. E n↑ (k) = E n↓ (k), is present. It can be thought of as provoked by an effective magnetic field. Bulk inversion asymmetry (BIA) leads to the Dresselhaus spin splitting [452, 453] that is shown in Fig. 6.5 for GaAs (cmp. Fig. 6.10a). The spin splitting due to structural inversion asymmetry (SIA) is described by the Bychkov-Rashba Hamiltonian [454, 455]. A review on these topics can be found in [456].

6.2.5 Symmetry Considerations In general the symmetry of the lattice is a symmetry of the system’s Hamiltonian and thus transfers into the electronic (and other) properties of the semiconductor. The means to formulate this mathematically is group theory and representation theory. At a given reciprocal lattice point, the wave function must fulfill the given spatial symmetry. Additional symmetry due to spin and spin-orbit interaction enters via the double-group scheme. This problem has been treated for the 32 point groups (cmp. Table B.2) in [457] and in [458] particularly for the pc, fcc, bcc and hcp lattices. A detailed treatment for the zincblende [459] and wurtzite [460] structures have been given. The most popular Hamiltonians are treated in [461]. The symmetry at particular points in direct or reciprocal space is denoted by the irreducible representations of the symmetry (point) group, e.g. by the i -symbols used in Figs. 6.9, 6.10 or also Fig. 6.44. As an example, base functions with the symmetry of the irreducible representations of tetraeder group Td are listed in Table 6.1. With the knowledge of the wave functions at the points of high symmetry, it is possible to deduce the general nature of the energy bands in the vicinity of such symmetry points.

142

6 Band Structure

Table 6.1 Representations of the tetraeder group (zincblende structure) in molecular, BSW [462] and Koster [457] notation and (examples of) corresponding base functions (c.p.: cyclic permutations) molecular

BSW

Koster

base functions

A1 A2 E T2 T1

1 2 12 15 25

1 2 3 4 5

x y z, x 2 + y 2 + z 2 x 4 (y 2 − z 2 ) + c.p. 2 z 2 − (x 2 + y 2 ), (x 2 − y 2 ) x, y, z, x y, x z, yz z (x 2 − y 2 ) and c.p.

6.2.6 Topological Considerations Starting with research on the quantum Hall effect and based on previous mathematical theorems, it has become clear that the band structure of ‘insulators’ has topological properties which in turn lead to a elegant classification of materials (and many effects/phases) [370, 463, 464]. In this context, the term ‘insulator’ means a material with gap between filled and empty states, i.e. semiconductors are exactly like this if the temperature is not too high (related to the gap divided by kB ). We recall the discussion of the diatomic linear chain in Sect. 5.2.3 where the bands turned out to have different topological properties depending on the ratio of sporing constants. Topology is a branch of mathematics where objects that are related to each other by a smooth deformation are classified as the same. For example, a sphere and an ellipsoid are topologically the same. Also, a doughnut and a cup are the same since they have one hole. A quantity that is independent of such smooth transformations is termed ‘topological invariant’. Such a number is the genus g of a surface that counts the number of holes. According to the Gauss-Bonnet theorem, the integral of the Gaussian curvature K over a closed surface S is given by K d A = 2π (2 − 2 g) .

(6.26)

S

The Gaussian curvature K = κ1 κ2 of a (differentiable) surface in 3D is the product of the principal curvatures κ1 and κ2 (maximum and minimum curvature of the curves from all normal planes that contain the normal vector intersecting with the surface). For a sphere of radius r , the Gaussian curvature is 1/r 2 everywhere and the integral in (6.26) is 4 π , making g = 0. For a topologically different example we look at a torus (all points that have the fixed distance r from a circle of radius R, r < R). It is parametrized by ⎛ ⎛ ⎞ ⎞ cos φ cos φ cos θ r = R ⎝ sin φ ⎠ + r ⎝ sin φ cos θ ⎠ , (6.27) 0 sin θ with both the angles φ and θ running between 0 and 2 π . The principal curvature κ1 along the θ direction is 1/r (for all φ). The other principal curvature κ2 in azimuthal (φ) direction changes sign with θ (positive outside, negative inside) and is also independent of φ. Its integral over the outer and inner part cancel exactly, thus the integral of κ1 κ2 over the entire torus is zero and therefore g = 1. Next, we connect the periodicity of the Brillouin zone in two dimensions with variables on a torus in 3D as shown in Fig. 6.6 (cmp. Fig. 5.3 for the 1D case). This concept can be generalized for a 3D band structure and a torus in four dimensions. If a constant function f = n a b/(2 π ) is integrated over the Brillouin zone (X is at ±π/a, Y is at ±π/b), the integral is

6.2 Electrons in a Periodic Potential

143

Fig. 6.6 Brillouin zone of a two-dimensional rectangular lattice and mapping to a torus Fig. 6.7 Brillouin zone of a rectangular lattice with a a constant function and b a function that changes sign. On the right the topology of the situation is visualized

1 2π

f (k) d2 k = n .

(6.28)

BZ

If for example another function f that is independent of k x and changes sign in k y -direction with f dk y = 0, similar to the curvature of the torus, is integrated over the Brillouin zone, the results will be zero. This is schematically shown in Fig. 6.7 if the integrand is interpreted as curvature. The generalization of the Berry phase [369] to Bloch states has been made in [465, 466]. For a twodimensional system with Bloch bands and with Bloch functions u m (k) as in (6.3), the integrand leading to a topological invariant is given by the Berry connection (cmp. (5.29)) Am = u m (k)|ı ∇k |u m (k) and its Berry curvature or Berry flux in three-dimensional notation Fm = ∇k × Am . The Chern number Cm for a band (separated by gaps from other bands), defined as integral over the Brillouin zone, Cm =

1 2π

Fm d 2 k ,

(6.29)

BZ

takes only integer values and is a topological invariant. That means that small variations of the Hamilton operator behind the band structure do not change its value. In the case of degeneracies, still the sum of Chern numbers over all occupied bands, n = m n m , is a topological invariant as long as the empty

144

6 Band Structure

Fig. 6.8 Schematic band structures with (a) topologically trivial wave functions and c topologically non-trivial wave functions where within one band the character changes from s (blue, ‘+’ for positive parity) to p (red, ‘−’ for negative parity). In b the crossing point is visualized

states are separated by a gap. For a three-dimensional crystal and k-space several topological invariants exist but a Chern number can be assigned to the Fermi surface or surface states (cmp. Sect. 11.6.3). As an schematic example we show Fig. 6.8 for a topological trivial and non-trivial band structure. In the trivial bandstructure (as most semiconductors), the phase character of the wavefunction changes only little within the Brillouin zone, mostly p-type (negative parity) for the valence band and mostly stype (positive parity) for the conduction band (Fig. 6.8a). In the topologically non-trivial bandstructure, band inversion takes place and the character of the wave function changes within a band (Fig. 6.8c). This sketch should be compared to Fig. 5.8 where a similar situation had been discussed for the lattice vibrations. An example for a semiconductor with band inversion is HgTe while CdTe or MnTe have trivial topology. Alloying leads at the transition from trivial to non-trivial (Fig. 6.8b) to zero-gap semiconductors (cf. Sect. 6.11).

6.3 Band Structures of Selected Semiconductors In the following, the band structures of various important and prototype semiconductors are discussed. The band below the energy gap is called the valence band; the band above the gap is the conduction band. The band gap E cv , mostly denoted as E g , is the energy separation between the highest valenceband state and the lowest conduction-band state. The maximum of the valence band is for most semiconductors at the point.

6.3.1 Silicon For silicon, an elemental semiconductor, (Fig. 6.9a) the minimum of the conduction band is located close to the X-point at 0.85π/a in the 100 direction. Thus, it is not at the same point in k space as the top of the valence band. Such a band structure is called indirect. Since there are six equivalent 100 directions, there are six equivalent minima of the conduction band.

6.3 Band Structures of Selected Semiconductors 6

145

Si

4

2

2

0

0 Energy (eV)

Energy (eV)

Ge

4

-2 -4 -6

-2 -4 -6

-8

-8

-10

-10 -12

-12 L

X U,K

L

(a)

X U,K

(b)

Fig. 6.9 Band structure of a silicon (indirect) and b germanium (indirect). In Si, the minima of the conduction band are in the 100 direction, for germanium in the 111 direction. Adapted from [164], based on [467] 6

GaAs

4

4

2

2

0

0

Energy (eV)

Energy (eV)

6

-2 -4 -6

-2 -4 -6

-8

-8

-10

-10 -12

-12 L

(a)

GaP

L

X U,K

X U,K

(b)

Fig. 6.10 Band structure of a GaAs (direct) and b GaP (indirect). For GaAs the minimum of the conduction band is at , for GaP in the 100 direction. Adapted from [164], based on [467]

6.3.2 Germanium Germanium, another elemental semiconductor, (Fig. 6.9b) also has an indirect band structure. The conduction minima are at the L point in the 111 direction. Due to symmetry there are eight equivalent conduction-band minima.

6.3.3 GaAs GaAs (Fig. 6.10a) is a compound semiconductor with a direct band gap since the top of the valence band and the bottom of the conduction band are at the same position in k space (at the -point). The next highest (local) minimum in the conduction band is close to the L point.

146

6 Band Structure

6.3.4 GaP GaP (Fig. 6.10b) is an indirect compound semiconductor. The conduction-band minima are along the 100 directions.

6.3.5 GaN GaN (Fig. 6.11) is a direct semiconductor that has wurtzite structure but can also occur in the metastable cubic (zincblende) phase.

6.3.6 Lead Salts The band gap of PbS (Fig. 6.12), PbSe and PbTe is direct and located at the L point. The lead chalcogenide system shows the anomaly that with increasing atomic weight the band gap does not decrease monotonically. At 300 K, the band gaps are 0.41, 0.27 and 0.31 eV for PbS, PbSe and PbTe, respectively.

X 15

GaN

10

10

5

5

0

0

-5

-5

-10

W

15

zb

w

Fig. 6.11 Band structure of GaN (direct) in zincblende (zb) modification (left) and wurtzite (w) modification (right), both displayed in the wurtzite Brillouin zone to facilitate comparison Fig. 6.12 Calculated band structure of PbS (direct). The energy gap is at the L point. The forbidden band is shown in grey. Adapted from [468]

6.3 Band Structures of Selected Semiconductors

147

12 10

CdO

8 6 4 2 0 -2 -4 -6 X

K

L

Fig. 6.13 Calculated indirect band structure of CdO. The top of the valence band is at E = 0. Adapted from [470]

6.3.7 MgO, ZnO, CdO Cadmium oxide is a cubic semiconductor in the rocksalt structure. Due to symmetry considerations, coupling (repulsion) of oxygen 2p- and cadmium 3d-orbitals does not occur at the zone center in the rocksalt structure. Repulsion occurs though away from the -point and therefore the valence band maximum is not located at the zone center (Fig. 6.13). Thus CdO is an indirect semiconductor. A similar effect would occur in rs-ZnO due to zinc 3d orbitals; however, ZnO has wurtzite structure for which p–d coupling at the -point is allowed; thus ZnO is direct. In MgO, Mg of course only possesses populated s- and p-orbitals and no such repulsion is present; thus MgO even with its rocksalt structure is also direct [469].

6.3.8 Chalcopyrites The experimental band gaps of a number of chalcopyrite semiconductors are listed in Table 6.2. The band structures of CuAlS2 , CuAlSe2 , and CuGaSe2 are compared in Fig. 6.14. In Fig. 6.15, the theoretical band structure of GaN and its closest related chalcopyrite ZnGeN2 are compared, both shown in the chalcopyrite (orthorhombic) Brillouin zone. The band gap of ZnGeN2 is smaller than that of GaN and the difference of 0.4 eV is fairly well reproduced by the calculation2 (giving 0.5 eV).

2 Due

to the local density approximation (LDA) the absolute values of the band gaps are too small by about 1 eV.

148

6 Band Structure

Table 6.2 Band gaps of various chalcopyrite semiconductors Material

E g (eV)

CuAlS2 CuAlSe2 CuAlTe2 AgAlS2 AgAlSe2 AgAlTe2 ZnSiP2 ZnSiAs2 CdSiP2 CdSiAs2

3.5 2.71 2.06 3.13 2.55 2.2 2.96 2.12 2.45 1.55

E g (eV) CuGaS2 CuGaSe2 CuGaTe2 AgGaS2 AgGaSe2 AgGaTe2 ZnGeP2 ZnGeAs2 CdGeP2 CdGeAs2

CuAlS2

E g (eV)

2.5 1.7 1.23 2.55 1.83 1.1–1.3 2.34 1.15 1.72 0.57

CuInS2 CuInSe2 CuInTe2 AgInS2 AgInSe2 AgInTe2 ZnSnP2 ZnSnAs2 CdSnP2 CdSnAs2

CuGaSe2

CuAlSe2

T

N

1.53 1.0 1.0–1.15 1.87 1.24 1.0 1.66 0.73 1.17 0.26

T

N

T

N

Fig. 6.14 Calculated band structures of CuAlS2 , CuAlSe2 , and CuGaSe2 . The absolute values of the gap energies are incorrect due to LDA calculation. Adapted from [471] ZnGeN 2

GaN

15 10 5 0 -5 -10 -15 X

Z

U

R

S

Y

X

Z

U

R

S

Y

Fig. 6.15 Calculated (within LDA) band structures of ZnGeN2 and its related III–V compound GaN, both displayed in the chalcopyrite (orthorhombic) Brillouin zone to facilitate comparison. Adapted from [472]

6.3 Band Structures of Selected Semiconductors

149

ZnCo2O4

ZnIr2O4

8 6 4 2 0 -2 -4 -6 -8

X

W

L

X

W

L

Fig. 6.16 Calculated band structures of ZnCo2 O4 and ZnIr2 O4 . Adapted from [470]

6.3.9 Spinels The band structure of spinels (in particular CdIn2 S4 ) has been discussed in [473], the band structure of ZnM2 O4 has been calculated in [470] for (M = Co, Rh, Ir) (Fig. 6.16) and in [474] for (M = Al, Ga, In).

6.3.10 Delafossites In Fig. 6.17, the theoretical band structures of the delafossites CuAlO2 , CuGaO2 , and CuInO2 are shown. The maximum of the valence band is not at but near the F point. The direct band gap at decreases for the sequence Al → Ga → In, similar to the trend for AlAs, GaAs and InAs. The direct band gap at F and L, causing the optical absorption edge, increases, however (experimental values are 3.5, 3.6, and 3.9 eV).

6.3.11 Perovskites The calculated band structure of BaTiO3 in the tetragonal phase is shown in Fig. 6.18. The minimum of the conduction band is at the -point. The maximum of the valence band is not at the -point but at the M point. The band gap of the LDA3 calculation is too small (2.2 eV) compared to the experimental value ∼ 3.2 eV. The band structure of the halide perovskites has been calculated for hybrid organic-inorganic compounds like MAPbI3 and FAPbI3 [476] and fully inorganic compounds APbI3 (A = Li, Na, K, Rb, and Cs) [477]. Density of states and energy positions of (MA,FA,Cs)(Pb,Sn)(Cl,Br,I)3 compounds are 3 local

density approximation.

150

6 Band Structure CuAlO2

CuGaO2

CuInO2

6 4 2 0 -2

Fig. 6.17 Band structures of CuAlO2 , CuGaO2 , and CuInO2 , calculated with LDA (underestimating the absolute value of the band gaps). The arrows denote the maximum of the valence band that has been set to zero energy for each material. Adapted from [226]

Fig. 6.18 Calculated energy band structure of BaTiO3 along the major symmetry directions. The Fermi level (E F ) is set at zero energy. Adapted from [475]

discussed in [478]. The trends are summarized in Fig. 6.19. The band gap of halide perovskites can be varied across the visible range, e.g. within the CsPb(Cl,Br,I)3 the system (Fig. 6.20).

6.4 Systematics of Semiconductor Band Gaps The trends with regard to the size of the band gap for elemental, III–V and II–VI semiconductors can essentially be understood in terms of the bond strength and ionicity. In Fig. 6.21, the band gaps of many important semiconductors are shown as a function of the lattice constant. For elemental semiconductors, the band gap decreases with reduced bond strength, i.e. lattice constant (C→Si→Ge). A similar trend exists both for the III–V and the II–VI semiconductors.

6.3 Band Structures of Selected Semiconductors

151

Fig. 6.19 Schematic energy levels in ABX3 perovskites. Arrows indicate the shift of energy levels upon substitution of atoms or small organic molecules. Adapted from [478]

(a)

(b)

Fig. 6.20 a Photoluminescence of CsPbX3 nanocrystals of halide perovskites with various anions (colloidal solutions in toluene under UV lamp (λ = 365 nm)). Adapted from [479]. b Position of conduction and valence band edges of CsPbX3 halide perovskites (relative to vacuum level at zero). Adapted from [480]

Fig. 6.21 Band gaps as a function of the lattice constant for various elemental, III–V and√ II–VI semiconductors. The 3 lattice constant of wurtzite semiconductors has been recalculated for a cubic cell (acubic = 3 a 2 c)

For the same lattice constant, the band gap increases with increasing ionicity, i.e. IV–IV→ III–V→II–VI→I–VII. A typical example is the sequence Ge→ GaAs→ZnSe→ CuBr, for which all materials have almost the same lattice constant, and the band gaps increase 0.66 eV→1.42 eV→2.7 eV→ 2.91 eV.

152

6 Band Structure 60 50

2md E/h2

2

40 30 20 10 0 -10

(a)

Eg

-20 -30 -40 -50

(b)

(c)

0

0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0 4.5 P

Fig. 6.22 Kronig-Penney model (along 111, b/a = 3) for a a IV–IV semiconductor and b for a III–V (or II–VI) semiconductor, c resulting band structure (P0 = −3). d denotes the lattice constant (d = b + a). Adapted from [481] Fig. 6.23 Optical image of two inch wafers of GaAs (left), GaP (center) and ZnO (right). A GaN wafer would look like the ZnO wafer

This behavior can be understood within the framework of a modified Kronig-Penney model [481] (Appendix F). Double potential wells (b/a = 3) are chosen to mimic the diatomic planes along the 111 direction in the zincblende structure (Fig. 6.22a). The first investigation of such diatomic onedimensional bandstructure was reported in [482]. Symmetric wells (depth P0 ) are chosen to model covalent semiconductors and asymmetric wells with depths P0 ± P to model partially ionic semiconductors. Results are shown in Fig. 6.22a for P0 = −3. With increasing asymmetry, i.e. increasing ionicity, the band gap increases, mostly due to a downward shift of the valence band. The case of III–V (II–VI) semiconductors is reached for P ≈ 2 (4). The calculation of effective masses in [481] is incorrect and has been rectified in [483]; the effective mass increases monotonically with P. In Fig. 6.23, the visual impression of 2" wafers of GaAs, GaP and GaN on white paper is shown. GaAs (and GaSb) is opaque since the band gap is below the visible spectral range. GaP has a band gap in the green and appears red, GaN has a band gap in the ultra-violet and thus appears transparent. As can be seen from Table 6.3, the anion sequence Sb, As, P, and N leads to smaller lattice constant and higher ionicity. A notable deviation from this rule is InN whose band gap (0.7 eV) is much smaller than that of InP [484].

6.5 Alloy Semiconductors In alloy semiconductors [166], the size of the band gap and the character of the band gap will depend on the composition. The dependence of the band gap on the ternary composition is mostly nonlinear and can usually be expressed with a bowing parameter b that is mostly positive. For a compound Ax B1−x C

6.5 Alloy Semiconductors

153

Table 6.3 Comparison of band gap, lattice constant and ionicity of gallium–group V semiconductors for various anions. Lattice constant for GaN has been recalculated for a cubic cell Anion

E g (eV)

a0 (nm)

fi

N P As Sb

3.4 2.26 1.42 0.72

0.45 0.545 0.565 0.61

0.50 0.33 0.31 0.26

the band gap is written as E g (Ax B1−x C) = E g (BC) + x E g (AC) − E g (BC) − b x (1 − x) .

(6.30)

Even on the virtual crystal approximation (VCA) level (Sect. 3.7.3) a nonzero bowing parameter b is predicted. However, a more thorough analysis shows that the bowing cannot be treated adequately within VCA and is due to the combined effects of volume deformation of the band structure with the alloy lattice constant, charge exchange in the alloy with respect to the binary end components, a structural contribution due to the relaxation of the cation–anion bond lengths in the alloy and a small contribution due to disorder [485]. The discussion of Sect. 6.12.3 is related. The Six Ge1−x alloy has diamond structure for all concentrations and the position of the conductionband minimum in k-space switches from L to X at about x = 0.15 (Fig. 6.24a). However, for all concentrations the band structure is indirect. The Inx Ga1−x As alloy has zincblende structure for all compositions. The band gap is direct and decreases with a bowing parameter of b = 0.6 eV [486] (Fig. 6.24b). This means that for x = 0.5 the band gap is 0.15 eV smaller than expected from a linear interpolation between GaAs and InAs, as reported by various authors [487]. If one binary end component has a direct band structure and the other is indirect, a transition occurs from direct to indirect at a certain composition. An example is Alx Ga1−x As where GaAs is direct and AlAs is indirect. For all concentrations the crystal has zincblende structure. In Fig. 6.24c, the , L and X conduction-band minima for ternary Alx Ga1−x As are shown. Up to an aluminum concentration of x = 0.4 the band structure is direct. Above this value the band structure is indirect with the conductionband minimum being at the X-point. The particularity of Alx Ga1−x As is that its lattice constant is almost independent of x. For other alloys lattice match to GaAs or InP substrates is only obtained for specific compositions, as shown in Fig. 6.25. The band gap bowing in the group-III–nitride system has been discussed in [488]. If the two binary end components have different crystal structure, a phase transition occurs at a certain composition (range). An example is Mgx Zn1−x O, where ZnO has wurtzite structure and MgO has rocksalt structure. The band gap is shown in Fig. 6.24d. In this case, each phase has its own bowing parameter. All alloys of Fig. 6.24b–d have mixed cations. The band gap also varies upon anion substitution in a similar way as shown in Fig. 6.26 for ternary alloys with the cation Zn and the chalcogenides S, Se, Te and O.

6.6 Amorphous Semiconductors Since the crystal lattice in an amorphous semiconductor is not periodic, the concept of k-space and the related concepts such as band structure E(k) break down at least partially. The density of states, however, remains a meaningful and useful quantity (Sect. 6.13.2).

154

6 Band Structure

In a perfectly crystalline semiconductor the eigenenergies of the states in the bands are real. An amorphous semiconductor can be modeled using a spectrum of complex energies [495]. In Fig. 6.27 the band structure of crystalline silicon is shown next to that calculated for amorphous silicon with α = 0.05.

6.7 Temperature Dependence of the Band Gap The band gap of a semiconductor typically decreases with increasing temperature. A direct visual impression can be obtained from the same LED chain at room temperature and dipped into liquid nitrogen (Fig. 6.28). Experimental data of band gap versus temperature are shown in Fig. 6.29 for bulk Si and ZnO. The reasons for the temperature variation of the band gap are the change of electron–phonon interaction and the expansion of the lattice. The temperature coefficient may be written as

1.5

InxGa1-xAs 1.3

Eg (eV)

1.1 0.9 0.7 0.5 0.3 0.0

(a)

0.2

0.4

x

(b)

2.6 AlxGa1-xAs 1

2.4

L1

2.2 Eg (eV)

Fig. 6.24 a Band gap of Six Ge1−x alloy (T = 296 K) with a change from the conduction-band minimum at L (Ge-rich) to X. The inset depicts the transition energy of the indirect (–L) and direct (–) absorption edge for low Si content. Adapted from [489]. b Band gap (at room temperature) of Inx Ga1−x As. The solid line is an interpolation with bowing (b = 0.6 eV) and the dashed line is the linear interpolation. Data from [486]. c Band gap (at room temperature) in the ternary system Alx Ga1−x As. For x < 0.4 the alloy is a direct, for x > 0.4 an indirect, semiconductor. E dd denotes the energy position of a deep donor (cf. Sect. 7.7.6). Adapted from [490]. d Band gap (at room temperature) in the ternary system Mgx Zn1−x O. Data (from spectroscopic ellipsometry [491, 492]) are for hexagonal wurtzite phase (circles), and Mg-rich cubic rocksalt phase (squares). Dashed lines are fits to data with a different bowing parameter for each phase

2.0

X1 Edd

1.8 1.6 1.4 0.0

0.2

0.4

x

0.6

(c)

0.8

1.0

(d)

0.6

0 .8

1.0

6.7 Temperature Dependence of the Band Gap Fig. 6.25 Band gap versus lattice constant for Gax In1−x P and Alx In1−x P (lattice matched to GaAs) as well as for Inx Al1−x As and Inx Ga1−x As alloys (lattice matched to InP)

Fig. 6.26 Band gap of various Zn-based alloys with mixing in the anion sublattice. The lines are fits with (6.30), the bowing parameter b is labeled. Data for Zn(S,Se,Te) from [493], for Zn(O,Se/Te) from [494]

Fig. 6.27 a Calculated band structure of crystalline silicon. b Calculated band structure of amorphous silicon with α = 0.05 (cf. (3.7)). The solid lines denote the real part of the energy, the shaded areas denote the regions with a width of twice the imaginary part of the energies centered around the real part. Adapted from [496]

155

156

6 Band Structure

Fig. 6.28 LED chain with part at room temperature (left) and a part in a dewar filled with liquid nitrogen (right) 0

Si

Eg (meV)

-50

-100

-150

-200

(a)

0

100 200 300 400 500 600 700 800

(b)

Fig. 6.29 Temperature dependence of the band gap of a Si (data from [498]) and b ZnO (experimental data from photoluminescence (triangles) and ellipsometry (circles)). The solid lines are fits with (6.34) and the parameters given in Table 6.4

∂ Eg ∂T

= p

∂ Eg ∂T

− V

α β

∂ Eg ∂p

,

(6.31)

T

where α is the volume coefficient of thermal expansion and β is the volume compressibility. A recommendable discussion of the thermodynamic role of the band gap as chemical potential for the mass action law (7.12), entropy contributions and its temperature dependence can be found in [497]. An anomaly is present for the lead salts (PbS, PbSe, PbTe) for which the temperature coefficient is positive (Fig. 6.30a). Theoretical calculations [499] show that both terms in (6.31) are positive for the − lead salts. The L+ 6 and L6 levels (see Fig. 6.12) shift as a function of temperature in such a way that their separation increases (Fig. 6.30b). Also in copper and silver halides [500, 501] (Fig. 6.31a) and chalcopyrites [502] (Fig. 6.31b) the increase of band gap with increasing temperature has been found, sometimes only for a certain temperature range. This effect is attributed to the p-d electron hybridization in the valence band with Cu 3d electrons and to even stronger effect with Ag 4d electrons. For many semiconductors the temperature dependence can be described with the empirical, threeparameter Varshni formula [503],

6.7 Temperature Dependence of the Band Gap

157

0.35 0.34

8.0

PbS

PbTe 7.5

Eg (eV)

0.33 0.32

L6

7.0

0.31

L6

0.30

6.5

0.29

(a)

0.28 0

50

100

150

(b)

6.0 0

100

200

300

− Fig. 6.30 a Band gap versus temperature for PbS. b Theoretical position of L+ 6 and L6 as a function of temperature for PbTe. Adapted from [468]

1.82

CuI1-xBrx

AgGaSe2

3.05 x=0 1.81

x=1

3.00

x=0.1 x=0.8

2.95

1.80

x=0.2

2.90 0

(a)

x=0.64 x=0.42

100 T

200

1.79 0

300

(b)

100 T

200

300

Fig. 6.31 a Band gap versus temperature for zincblende CuI1−x Brx alloys with various compositions x (including binary CuI and CuBr) as labeled. Dashed lines are guide to the eye. Adapted from [500]. b Band gap vs. temperature for chalcopyrite AgGaSe2 . Solid line is fit with two-oscillator Bose-Einstein model. Adapted from [502]

E g (T ) = E g (0) −

α T2 , T +β

(6.32)

where E g (0) is the band gap at zero temperature. A more precise and physically motivated formula (based on a Bose-Einstein phonon model [504]) has been given in [505]

B αB B αB B coth − 1 = E g (0) − , E g (T ) = E g (0) − 2 2T exp(B /T ) − 1

(6.33)

where α B is a coupling constant and kB is a typical phonon energy; typical values are given in Table 6.4. This model reaches a better description of the fairly flat dependence at low temperatures. The more elaborate model of [506] takes into account a more variable phonon dispersion, including optical phonons, and proposes the four-parameter formula

3 2 1 − 3 2 6 + 1+β −1 E g (T ) = E g (0) − α exp (2/γ ) − 1 2

(6.34)

158

6 Band Structure

Table 6.4 Parameters for the temperature dependence of the band gap according to 6.33 (Si, GaAs: [505], GaN: [507], ZnO: [508]) and (6.34) for various semiconductors

Si Ge GaAs GaN InP InAs ZnSe ZnO

α (10−4 eV/K)

(K)

αB (10−4 eV/K)

B (K)

3.23 4.13 4.77 6.14 3.96 2.82 5.00 3.8

446 253 252 586 274 147 218 659

0.51 0.49 0.43 0.40 0.48 0.68 0.36 0.54

2.56

296

5.16 4.05

310 370

5.9

616

Fig. 6.32 Band gap of GaAs (at T = 10 K) as a function of the Ga isotope content. Dashed line is linear fit. Adapted from [509]

π2 3 2 − 1 3 8 4 γ2 + γ + γ + γ6 2 3 (1 + ) 4 3 γ = 2 T / , β=

where α is the high-temperature limiting magnitude of the slope (of the order of several 10−4 eV/K), is an effective average phonon temperature and is related to the phonon dispersion. takes typically values between zero (Bose-Einstein model) and 3/4 [506].

6.8 Isotope Dependence of the Band Gap The band edge slightly depends on the isotope composition of semiconductor, as shown for GaAs in Fig. 6.32. The effect is discussed in detail in [509].

6.9 Electron Dispersion 6.9.1 Equation of Electron Motion The equation of motion for the electron in the band structure is no longer given by Netwon’s law F = d(mv)/dt as in vacuum. Instead, the propagation of quantum-mechanical electron wave packets has to be considered. Their group velocity is given by (vg = ∂ω/∂k)

6.9 Electron Dispersion

159

v=

1 ∇k E(k) ,

(6.35)

where ∇k is the gradient with respect to k. Through the dispersion relation the influence of the crystal and its periodic potential on the motion enters the equation. An electric field E acts on an electron during the time δt the work δ E = −eEvg δt. This change in energy is related to a change in k via δ E = dE/dk δk = vg δk. Thus, we arrive at dk/dt = −eE. For an external force we thus have dk = −e E = F . (6.36) dt Thus, the crystal momentum p = k takes the role of the momentum. A more rigorous derivation can be found in [451]. In the presence of a magnetic field B the equation of motion is

e dk = −e v × B = − (∇k E) × B . dt

(6.37)

The motion in a magnetic field is thus perpendicular to the gradient of the energy, i.e. the energy of the electron does not change. It oscillates therefore on a surface of constant energy perpendicular to B.

6.9.2 Effective Mass of Electrons From the free-electron dispersion E = 2 k 2 /(2m) the mass of the particle is inversely proportional to the curvature of the dispersion relation, i.e. m = 2 /(d2 E/dk 2 ). This relation will now be generalized for arbitrary dispersion relations. The (inverse) tensor of the effective mass is defined as (m ∗−1 )i j =

1 ∂2 E . 2 ∂ki ∂k j

(6.38)

The equation F = m ∗ v˙ must be understood as a tensor equation, i.e. for the components of the force Fi = m i∗j a j . Force and acceleration must no longer be collinear. In order to find the acceleration from the force, the inverse of the effective-mass tensor must be used, a = (m∗ )−1 F. In Fig. 6.33 the energy dispersion of the (lowest) conduction band in a typical semiconductor, the related electron velocity and the effective mass are shown schematically. In (6.22) the ratio of the effective mass and the free-electron mass is of the order of m ∗ /m ≈ U/λ, the ratio of the free particle energy and the band gap. For typical semiconductors, the width of the (valence) band is of the order of 20 eV, and the gap is about 0.2–2 eV. Thus, the effective mass is expected to be 10–100 times smaller than the free-electron mass. Additionally, the relation m ∗ ∝ E g is roughly fulfilled (Fig. 6.34). From so-called k · p theory [510] (see Appendix H) the effective electron mass is predicted to be related to the momentum matrix element pcv pcv = c|p|v =

0

u ∗c,k (r) p u c, k (r) d3 r ,

(6.39)

with 0 being the unit cell volume and the Bloch functions |c and |v of the conduction and valence band, respectively, given as

160

6 Band Structure

Fig. 6.33 Schematic diagram of the electron dispersion E(k) in a typical semiconductor (blue) and corresponding carrier velocity (∝ ∂ E/∂k) (red) and effective mass (∝ 1/(∂ 2 E/∂k 2 )) (green)

Fig. 6.34 Effective electron mass (in units of the free-electron mass m 0 ) as a function of the (low-temperature) band gap for several (direct band gap) semiconductors. The dashed line fulfills m ∗/m 0 = E g /20 eV

|c = u c,kc (r) exp (i kc r) |v = u v,kv (r) exp (i kv r) .

(6.40a) (6.40b)

Typically, the k-dependence of the matrix element is small and neglected. The momentum matrix element will also be important for optical transitions between the valence and conduction bands (Sect. 9.6). Other related quantities that are often used are the energy parameter E P EP =

2 |pcv |2 , m0

(6.41)

and the bulk momentum matrix element Mb2 that is given by Mb2 =

1 m0 |pcv |2 = EP . 3 6

(6.42)

6.9 Electron Dispersion

161

Fig. 6.35 Energy isosurfaces in k-space in the vicinity of the conduction-band minima for a GaAs with isotropic (spehrical) minimum at -point, b ZnO with anisotropic (ellipsoidal) minimum at -point (anisotropy exaggerated), c silicon with six equivalent anisotropic minima (m l /m t = 5 not to scale) along 100 and d germanium with eight equivalent anisotropic minima along 111. The cube indicates the 100 directions for the cubic materials. For the wurtzite material (part b) the vertical direction is along [00.1]

(a)

(b)

(c)

(d)

The electron mass is given by4

2 1 + Eg E g + 0 E g + 2 0 /3 EP EP ≈1+ = 1 + EP ≈ . E g + 0 /3 Eg E g E g + 0

m0 EP = 1+ m ∗e 3

(6.43)

Comparison with the fit from Fig. 6.34 yields that E P is similar for all semiconductors [511] and of the order of 20 eV (InAs: 22.2 eV, GaAs: 25.7 eV, InP: 20.4 eV, ZnSe: 23 eV, CdS: 21 eV). In silicon there are six equivalent conduction-band minima. The surfaces of equal energy are schematically shown in Fig. 6.35c. The ellipsoids are extended along the 100 direction because the longitudinal mass (along the path) is larger than the transverse mass in the two perpendicular directions (Table 6.5). For example, the dispersion relation in the vicinity of one of the minima is given as (k x0 denotes the position of one of the conduction-band minima close to a X-point) E(k) =

2

k 2y + k z2 (k x − k x0 )2 + 2 ml 2 mt

.

(6.44)

For germanium surfaces of constant energy around the eight conduction-band minima in the 111 directions are depicted in Fig. 6.35d. The longitudinal and the transverse masses are again different. For GaAs, the conduction-band dispersion around the point is isotropic, thus the surface of constant energy is simply a sphere (Fig. 6.35a). In wurtzite semiconductors the conduction-band minimum is at the -point. The mass along the c-axis is typically smaller than the mass within the (00.1) plane [512] 4

0

is the spin-orbit splitting discussed in Sect. 6.10.2.

162

6 Band Structure

Table 6.5 Longitudinal direction of effective mass ellipsoid, longitudinal and transverse effective electron mass in several semiconductors. For the density of states mass m d,e see (6.72). Mass values in units of the free electron mass m 0 C Si Ge ZnO CdS

Long. dir.

ml

mt

m l /m t

m d,e

Ref.

100 100 111 [00.1] [00.1]

1.4 0.98 1.59 0.21 0.15

0.36 0.19 0.082 0.25 0.17

3.9 5.16 19.4 0.88 0.9

1.9 1.08 0.88

[514] [515] [515] [516] [517]

Fig. 6.36 Effective electron mass from cyclotron resonance experiments (at T = 4 K) on a Si and b Ge for the magnetic field in the (110) plane and various azimuthal directions θ. Experimental data (symbols) and fits (solid lines) using (6.45) with a m l = 0.98, m t = 0.19 and b m l = 1.58, m t = 0.082. Adapted from [515]

(b)

(a)

(m l /m t ≈ 0.8 for ZnO [513]), see Fig. 6.35b. In [512] also an anisotropy within the (00.1) plane is predicted. The directional dependence of the mass can be measured with cyclotron resonance experiments with varying direction of the magnetic field. In Fig. 6.36, the field B is in the (110) plane with different azimuthal directions. When the (static) magnetic field makes an angle ϑ with the longitudinal axis of the energy surface, the effective mass is given as [518] 1 = m∗

cos2 ϑ sin2 ϑ + . mt ml m 2t

(6.45)

6.9.3 Nonparabolicity of Electron Mass The dispersion around the conduction-band minimum is only parabolic for small k. The further away the wavevector is from the extremum, the more the actual dispersion deviates from the ideal parabola (see, e.g., Fig. 6.10). This effect is termed nonparabolicity. Typically, the energy increases less quickly with k than in the parabolic model. This can be described in a so-called two-level model with the dispersion relation

6.9 Electron Dispersion

163

2 k 2 E = E 1 + , 2m ∗0 E 0∗

(6.46)

where E 0∗ > 0 parameterizes the amount of nonparabolicity (a parabolic band corresponds to E 0∗ = ∞). The nonparabolic dispersion for GaAs is shown in Fig. 6.37a. The curvature is reduced for larger k and thus the effective mass is energy dependent and increases with the energy. Equation (6.46) leads to the energy-dependent effective mass ∗

m (E) =

m ∗0

2E 1+ ∗ , E0

(6.47)

where m ∗0 denotes here the effective mass at k = 0. Theory and experimental data for the effective electron mass of GaAs are shown in Fig. 6.37b.

6.10 Holes 6.10.1 Hole Concept Holes are missing electrons in an otherwise filled band. A Schrödinger-type wave-equation for holes (unoccupied electron states) was derived by Heisenberg [70] to interpret Hall effect data. The hole concept is useful to describe the properties of charge carriers at the top of the valence band. The hole is a new quasi-particle whose dispersion relation is schematically shown in Fig. 6.38 in relation to the dispersion of electrons in the valence band. The wavevector of the hole (filled circle in Fig. 6.38) is related to that of the ‘missing’ electron (empty circle in Fig. 6.38) by kh = −ke . The energy is E h (kh ) = −E e (ke ), assuming that E V = 0, otherwise E h (kh ) = −E e (ke ) + 2E V . The hole energy is larger for holes that are further away from the top of the valence band, i.e. the lower the energy state of the missing electron. The velocity of the hole, vh = −1 dE h /dkh , is the same, vh = ve , and the charge is positive, +e. The effective mass of the 18

[001] [111]

GaAs

GaAs 0.12

0.2

0.1

0.10 0.08 0.06 16 10

0

(a)

200

0.14

m*/m0

0.3

EF (meV)

-3

2

13

-2

k (10 cm )

(b)

10

17

10 )

-3

18

10

19

Fig. 6.37 a Dispersion relations for the conduction band of GaAs. The solid line is parabolic dispersion (constant effective mass). The dashed (dash-dotted) line denotes the dispersion for k along [001] ([111]) from a five-level k · p model (5LM). b Cyclotron resonance effective mass of electrons in GaAs as a function of the Fermi level (upper abscissa) and the corresponding electron concentration (lower abscissa). The dashed line is from a 2LM according to (6.47) with E 0∗ = 1.52 eV. The solid lines are for a 5LM for the three principal directions of the magnetic field. The symbols represent experimental data from different sources. Data from [519]

164

6 Band Structure E

Fig. 6.38 Hole dispersion dashed line in relation to the electron dispersion in the valence band (solid line)

ke

kh

k

hole is positive at the top of the valence band, m ∗h = −m ∗e . Therefore, the drift velocities of an electron and hole are opposite to each other. The resulting current, however, is the same.

6.10.2 Hole Dispersion Relation The valence band at the -point is 3-fold degenerate. The band developed from the atomic (bonding) p states; the coupling of the spin s = 1/2 electrons with the orbital angular momentum l = 1 leads to a total angular momentum j = 1/2 and j = 3/2. The latter states are degenerate at in zincblende bulk material and are called heavy holes (hh) for m j = ±3/2 and light holes (lh) for m j = ±1/2 due to their different dispersion (Fig. 6.39a). The two (m j = ±/ 2) states of the j = 1/2 state are split-off from these states by an energy 0 due to spin-orbit interaction and are called split-off (s-o) holes. The spin-orbit interaction increases with increasing atomic order number Z of the anion since the electrons are located preferentially there (Fig. 6.40). A detailed discussion of the spin-orbit splitting in zincblende semiconductors is given in [520]. All three holes have different mass. In the vicinity of the -point the dispersion for heavy and light holes can be described with (+:hh, −:lh)

Fig. 6.39 a Simplified band structure with conduction band and three valence bands and (b) three-dimensional visualization (E versus (kx , ky )) of the valence bands of Ge (including warping). Part b from [521]

(a)

(b)

6.10 Holes

165

Fig. 6.40 Spin-orbit splitting 0 for elemental (diamonds) and various III–V and II–VI (circles) semiconductors. The data are plotted as empty (filled) circles as a function of the cation (anion) order number. Obviously, 0 correlates with the anion Z . The dashed line is proportional to Z 2

Fig. 6.41 Dispersion at the valence band edge of GaAs for a, b heavy holes and c,d light holes. a,c Constant energy surfaces and b,d isolines in the (k x , k y )-plane (b and d have different energy scales)

2

0

-2

(a)

(b)

-4

-4

-2

0

2

4

-4

-2

0

2

4

2

0

-2

(c)

(d)

E(k) = A k ± 2

-4

B 2 k 4 + C 2 kx2 ky2 + ky2 kz2 + kx2 kz2 .

(6.48)

For heavy and light holes there is a dependence of the dispersion, i.e. the mass, in the (001) plane. This effect, sketched in Fig. 6.39b, is called warping. The warping at the GaAs valence-band edge is shown in Fig. 6.41. Equation (6.48) can also be expressed in terms of angular coordinates [522]. The s-o holes have the dispersion E(k) = − 0 + A k 2 .

(6.49)

166

6 Band Structure

Table 6.6 Valence-band parameters (for (6.48)) A and B in units of (2 /2m 0 ), C 2 in units of (2 /2m 0 )2 , and 0 in eV. From [164, 523, 524] Material

A

B

C2

0

C Si Ge GaAs InP InAs ZnSe

−4.24 −4.28 −13.38 −6.9 −5.15 −20.4 −2.75

−1.64 −0.68 −8.5 −4.4 −1.9 −16.6 −1.0

9.5 24 173 43 21 167 7.5

0.006 0.044 0.295 0.341 0.11 0.38 0.43

Values for A, B, C 2 and 0 for a number of semiconductors are given in Table 6.6. The valence-band structure is often described with the Luttinger parameters γ1 , γ2 , and γ3 that can be represented through A, B, and C via 2 γ1 = − A 2m 0 2 B γ2 = − 2m 0 2 2 B 2 + C 2 /3 . γ3 = 2m 0 2

(6.50a) (6.50b) (6.50c)

The mass of holes in various directions can be derived from (6.48). The mass along the [001] direction, i.e. 2 /(∂ 2 E(k)/∂k x2 ) for k y = 0 and k z = 0, is 1 2 = 2 (A + B) 100 m hh 1 2 = 2 (A − B) . 100 m lh

(6.51a) (6.51b)

The anisotropy of hole masses has been investigated with cyclotron resonance experiments (Fig. 6.42). For θ being the angle between the magnetic field and the [001] direction, the effective heavy hole (upper sign) and light hole (lower sign) mass in cubic semiconductors is given by [515] m∗ =

1 2 2 A ± B 2 + C 2 /4 ⎧ ⎫ ⎨ ⎬ C 2 (1 − 3 cos2 θ )2 × + ... . ⎩ 64 B 2 + C 2 /4 A ± B 2 + C 2 /4 ⎭

(6.52)

For C 2 = 0 the hole bands are isotropic, as is obvious from (6.48). In this case γ2 = γ3 , the so-called spherical approximation. The average of the hole masses over all directions is 2 1 av = 2 m hh

2 C2 A+ B 1+ 15 B 2

(6.53a)

6.10 Holes

167

(b)

(a)

Fig. 6.42 Effective hole masses from cyclotron resonance experiments (T = 4 K) for heavy and light holes in a Si and b Ge for the magnetic field in the (110) plane and various azimuthal directions θ. Experimental data (symbols) and fits (solid lines) using (6.52). Adapted from [515]

(a)

(b)

Fig. 6.43 Luttinger parameters for various III-V semiconductors versus their band gap. a Inverse values of γ1 (squares) and γ2 (diamonds). Dashed lines are guides to the eye. b γ3 − γ2 versus band gap

1 2 av = 2 m lh

2 C2 A− B 1+ . 15 B 2

(6.53b)

Similar to the correlation of the electron mass with the band gap (Fig. 6.34), the Luttinger parameters are correlated with the band gap as shown in Fig. 6.43. The parameters 1/γ1 and 1/γ2 increase about linearly with E g . The parameter γ3 − γ2 , which is responsible for the valence band warping, decreases with increasing band gap.

168

6 Band Structure

6.10.3 Valence-Band Fine Structure In Fig. 6.44, the schematic structure of the band edges for zincblende structure semiconductors is shown. The s-o holes in the zincblende structure are split-off due to the spin-orbit interaction so , the 8 band is degenerate (heavy and light holes). Degeneracies for the holes are removed in the wurtzite and chalcopyrite structures by the additional crystal field splitting cf due to the anisotropy between the a- and c-axes. Typically, e.g. for CdS, the topmost valence band in the wurtzite structure has 9 symmetry (allowed optical transitions only for E ⊥ c); an exception is ZnO for which the two upper bands are believed to be reversed. In the chalcopyrite structure optical transitions involving the 6 band are only allowed for E ⊥ c. The three hole bands are usually labeled A, B, and C from the top of the valence band. The energy positions of the three bands (with respect to the position of the 15 band) in the presence of spin-orbit interaction and crystal field splitting are given within the quasi-cubic approximation [525] by

so + cf 2

so + cf 2 2 =± − so cf . 2 3

E1 = E 2,3

(6.54a) (6.54b)

In chalcopyrites the crystal field splitting is typically negative (Fig. 6.45). It is approximately linearly related to 1 − η (for η = c/2a see Sect. 3.4.6).

Fig. 6.44 Schematic band structure of zincblende and the valence-band splitting due to spin-orbit interaction so and crystal field splitting cf for chalcopyrites (typically cf < 0, see Fig. 6.45) and wurtzites. For the wurtzites the situation is schematically shown for CdS ( so = 67 meV, cf = 27 meV) (or GaN) and ZnO ( so = −8.7 meV, cf = 41 meV)

6.11 Band Inversion

-0.3 AgGaS2 AgGaSe2

-0.2 AgInS2 CuAlS2

(eV) cf

Fig. 6.45 Crystal field splitting cf for various chalcopyrite compounds versus the tetragonal distortion 2 − c/a = 2 (1 − η). Dash-dotted line represents

cf = 1.5 b (2 − c/a) for b = 1 eV. Data from [526]

169

-0.1

CuGaS2 CuGaSe2

AgGaTe2 AgAlTe2

AgInSe2

AgInS2(w)

0

CuInS2 CuInSe2

0.0

0.1 2 c/a

0.2

Fig. 6.46 Schematic band structure of zincblende with vanishing energy gap for the ternary compounds Mnx Hg1−x Te. Note the linear dispersion for the zero-gap case at x ≈ 0.07

6.11 Band Inversion In certain compounds, typically mixing a semiconductor with a semimetal [527, 528], the band gap can shrink to zero (zero-gap semiconductor) and even become negative in the sense that the s-type 6 symmetry (conduction) band is inverted below the 8 (p-type) valence-band edge. HgTe is a classical example for such material as shown in Fig. 6.46, but similar effects are also present in other semiconductors, for example various chalcopyrites [529]. Remember that such band structures are topologically non-trivial (cf. Sect. 6.2.6). For the zero-gap case, the dispersion of the two crossing bands is linear (like for graphene, cf. Sect. 13.1.2). The dielectric function of zero-gap semiconductors is discussed in [530]. For the Cdx Hg1−x Te system, around the zero-gap concentration of x ≈ 0.16, the change from normal to inverted band structure will occur also as a function of temperature [531] as shown in Fig. 6.47. Such effect had been described already 50 years ago for (Pb,Sn)Te at the L-point (cf. Sect. 6.3.6) in [532].

170

6 Band Structure

Fig. 6.47 Band gap of Cdx Hg1−x Te for various alloy compositions and temperatures. On the right, the schematic band structure of (Hg,Cd)Te with positive, zero and negative band gap is shown. Adapted from [531], reprinted under a Creative Commons Attribution (CC BY 4.0) licence

6.12 Strain Effects on the Band Structure A mechanical strain (or equivalently stress) causes changes in the bond lengths. Accordingly, the band structure is affected. These effects have been exhaustively treated in [533, 534]. For small strain, typically 0.01 the shift of the band edges is linear with the strain, for large strain it becomes nonlinear [535]. Often homogeneous strain is assumed, the effect of inhomogeneous strain is discussed in [536].

6.12.1 Strain Effect on Band Edges In a direct-gap zincblende material the position of the conduction-band edge is only affected by the hydrostatic component of the strain E C = E C0 + ac xx + yy + zz = E C0 + ac Tr() ,

(6.55)

where ac < 0 is the conduction-band hydrostatic deformation potential and E C0 is the conduction-band edge of the unstrained material. Similarly, the valence-band edge is E V = E V0 + av Tr() ,

(6.56)

where av > 0 is the valence-band hydrostatic deformation potential. Therefore the band gap increases by (6.57)

E g = a Tr() = a xx + yy + zz , with a = aC − aV . Such linear behavior upon hydrostatic pressure has been found for many semiconductors and is shown in Fig. 6.48a for Ga0.92 In0.08 As. The anomaly for N-doping is discussed below in Sect. 6.12.3. In Fig. 6.49 the dependence of the direct and indirect gaps of GaAs is shown. The dependence of the direct gap on pressure is non-linear, that on the density is linear [537]. Biaxial and shear strains affect the valence bands and lead to shifts and splitting of the heavy and light holes at the -point: E v,hh/lh = E v0 ± E

(6.58a)

6.12 Strain Effects on the Band Structure

171

Fig. 6.48 a Dependence of the band gap of Ga0.92 In0.08 As alloy (squares) and nitrogen-doped (Ga,In)As on (compressive) hydrostatic pressure, determined by photomodulated transmission at T = 295 K. b Pressure dependence of band gap for two (Ga,In)(As,N) samples together with model calculation (6.62). The coupling parameter is V = 0.12 eV (0.4 eV) for a nitrogen content of 0.9% (2.3%). Adapted from [538]

V – C and indirect V –X C band gap of GaAs (T = 300 K) on pressure. Solid Fig. 6.49 Dependence of the direct 15 1 1 15 lines are interpolations of experimental data, dashed line is extrapolation to p = 0. The crossing of the direct and indirect band gap occurs at 4.2 GPa. The arrow denotes the pressure of the phase transition from zincblende to an orthorhomic structure around 17 GPa. Adapted from [537]

2 2 2 E = b2 /2 xx − yy + yy − zz + (xx − zz )2 2 2 2 + d 2 xy , + yz + xz where E v0 denotes the bulk valence-band edge. b and d are the optical deformation potentials. For compressive strain the heavy-hole band is above the light-hole band. For tensile strain there is strong mixing of the bands (Fig. 6.50). In Table 6.7 the deformation potentials for some III–V semiconductors are listed. Typical values are in the eV regime. In a wurtzite crystal, seven (or eight) deformation potentials are needed that are termed a (for the change of band gap with hydrostatic strain, again a = aC − aV ) and D1 –D6 (for the valence band structure) [539, 540]. In Si and Ge, three deformation potentials, termed a, b, d, are needed for the valence band and two for each conduction band minimum, u and d [541]. The energy position of the i-th conduction-band edge (with unit vector ai pointing to the valley) is

172

6 Band Structure E

E

Fig. 6.50 Schematic band structure of GaAs in unstrained state (center) and under compressive and tensile biaxial strain as labeled. Dashed lines indicate shift of band edges due to hydrostatic part of strain

E

electrons

k

k

k

mj=3/2 mj=1/2

mj=1/2 mj=3/2

mj=3/2 mj=1/2

unstrained

compressive

tensile

Table 6.7 Deformation potentials for some III–V semiconductors. All values in eV Material

a

b

d

GaAs InAs

−9.8 −6.0

−1.7 −1.8

−4.6 −3.6

Table 6.8 Deformation potentials for silicon and germanium. All values in eV from [542] ( )

( )

(L)

(L)

material

d

u

d

u

a

b

d

Si Ge

1.1 4.5

10.5 9.75

−7.0 −4.43

18.0 16.8

2.1 2.0

−2.33 −2.16

−4.75 −6.06

0 E C,i = E C,i + d Tr() + u ai ai ,

(6.59)

0 denotes the energy of the unstrained conduction-band edge. The deformation potentials for where E C,i Si and Ge are given in Table 6.8.

6.12.2 Strain Effect on Effective Masses In the presence of strain the band edges are shifted (cf. Sect. 6.12). Since the electron mass is related to the band gap, it is expected that the mass will also be effected. In the presence of hydrostatic strain H the electron mass is [543] (cf. to (6.43) for H → 0)

m0 3a EP 2 + 1 − , = 1 + H m ∗e E g + 0 /3 E g + 0 /3

(6.60)

with a being the hydrostatic deformation potential and H = Tr(). In [543], formulas are also given for biaxial and shear strain and also for hole masses. Since the effective mass enters the mobility, the electrical conductivity depends on the stress state of the semiconductor (piezoresistivity, see Sect. 8.3.14).

6.12 Strain Effects on the Band Structure

173 1.5

Fig. 6.51 Bandgap of GaAs1−x Nx , experimental data from various sources (symbols) and model (curve) according √ to (6.62) with V = V0 x for V0 = 2.7 eV. Adapted from [545]

GaAs1-xNx

Energy (eV)

1.4 1.3 1.2 1.1 1.0 0.9 0

1 2 3 4 Nitrogen concentration x (%)

5

6.12.3 Interaction With a Localized Level The normal dependence of the band gap on hydrostatic pressure is linear and given by (6.57). (Ga,In)As containing nitrogen exhibits a remarkable deviation from this behavior as shown in Fig. 6.48a. This is due to the interaction of the continuum states of the conduction band with the electron level of the isoelectronic nitrogen impurity (Sect. 7.7.9) E N , being within the conduction band. For GaAs it is 0.2 eV above the conduction band edge E C . This phenomenon has been investigated theoretically within microscopic detail [544]. Within a simple ‘band anticrossing’ two-level model, the coupling of the pressure-dependent conduction band edge E C and the nitrogen level can be obtained from the Eigenwert equation E − EC V =0, (6.61) V E − EN V being the coupling constant. The determinant vanishes for E± =

1 E C + E N ± (E C − E N )2 + 4V 2 . 2

(6.62)

Here the weak pressure dependence of E N is neglected for simplicity. This model can explain the pressure dependence of the band gap of (Ga,In)As:N fairly well [538] (Fig. 6.48b). The coupling parameter V is in the order of a few 0.1 eV for small nitrogen content. In photomodulated reflection also the E + levels can be observed [545]. The anti-crossing model can also model the dependence of the GaAs1−x Nx bandgap on the nitrogen concentration [545] (Fig. 6.51).

6.13 Density of States 6.13.1 General Band Structure The dispersion relation yields how the energy of a (quasi-) particle depends on the k vector. Now we want to know how many states are at a given energy. This quantity is called the density of states (DOS) and is written as D(E). It is defined in an infinitesimal sense such that the number of states between

174

6 Band Structure

E and E + δ E is D(E)δ E. In the vicinity of the extrema of the band structure many states are at the same energy such that the density of states is high. The dispersion relation of a band will be given as E = E(k). If several bands overlap, the densities of state of all bands need to be summed up. The density of states at the energy E˜ for the given band is ˜ dE = 2 D( E)

d3 k δ( E˜ − E(k)) , (2π/L)3

(6.63)

where, according to (5.5), (2π/L)3 is the k-space volume for one state. The factor 2 is for spin ˜ degeneracy. The integral runs over the entire k-space and selects only those states that are at E. ˜ The volume integral can be converted to a surface integral over the isoenergy surface S( E) with ˜ ˜ The volume element d3 k is written as d2 S dk⊥ . The vector dk⊥ is perpendicular to S( E) E(k) = E. and proportional to ∇k E(k), i.e. dE = |∇k E(k)| dk⊥ . ˜ =2 D( E)

˜ S( E)

d2 S 1 . (2π/L)3 |∇k E(k)|

(6.64)

In this equation, the dispersion relation is explicitly contained. At band extrema the gradient diverges, however, in three dimensions the singularities are integrable and the density of states takes a finite value. The corresponding peak is named a van-Hove singularity. The concept of the density of states is valid for all possible dispersion relations, e.g. for electrons, phonons or photons. The density of states for the silicon band structure (see Fig. 6.9a) is shown in Fig. 6.52.

6.13.2 Amorphous Semiconductors If disorder is introduced, the density of states is modified as shown in Fig. 6.53 for amorphous germanium using a calculation with complex eigenenergies. The defects, as compared to the perfect lattice, introduced states in the band gap and generally wash out the sharp features from the crystalline DOS. Several models exist for the defect level distributions within the band gap. The first model was the Mott model which has band tails at the valence and conduction band edges [547]. In the CohenFritzsche-Ovshinsky (CFO) model [548], the band tails are more severe and overlap; the Fermi energy lies at the minimum of the density of states. In the Davis–Mott model [549] deep states were added in the gap and eventually the Marshall-Owen model [550] assumes band tails and donor- and acceptorlike deep states. The four models are schematically shown in Fig. 6.54. These model densities of states allow also the interpretation of carrier transport in amorphous semiconductors, taking into account localized and delocalized states (see Sect. 8.9). The density of states for an amorphous semiconductor is best calculated from atomistic models, possibly averaging over many configurations. The typical features, compared to the clear band gap of a similar ordered material, are band tails due to disorder (cmp. Sect. 5.2.9) and deep levels within the gap due to specific atomic arrangements not present in ordered bulk. The most investigated system is amorphous silicon; in Fig. 6.55 a numerical calculation of the density of states is shown together with charge distribution of four states at selected energies [551]. The further the states are in the band tail, the stronger their localization is. The two most right states shown in Fig. 6.55 are not conducting. As another example, simulations of ZnSnO3 are shown in Fig. 6.56. The band tail between 0 and 0.5 eV is due to disorder of oxygen 2p orbitals [552]. At 0.9 eV a level due to under-coordinated oxygen appears. Deep levels are due to metal-metal bonds. Band tails due to chemically disordered oxygen have been experimentally observed for amorphous GIZO [553].

6.13 Density of States Fig. 6.52 Density of states in the silicon valence(blue) and conduction-band (red) as obtained from theoretical calculation using empirical pseudopotentials. Grey regions denotes the band gap. Critical points (cf. Fig. 6.9a) are labeled. In the lower three graphs, the DOS is decomposed into contributions from different angular momentum states (s (green), p (orange) and d (purple)). Top part adapted from [546], bottom part adapted from [175]

6.13.3 Free-Electron Gas In M dimensions, the energy states of a free-electron gas are given as

Fig. 6.53 Theoretical calculation for the density of states of amorphous Ge models as obtained for various degrees of disorder α (3.7). α = 0.09 corresponds to a mean short-range order distance of about 2.4 lattice constants (cmp. Fig. 3.14b). Adapted from [204]

175

176

6 Band Structure

Fig. 6.54 Model density of states in amorphous semiconductors (solid lines) according to Mott [547], Cohen-FritzscheOvshinsky [548], Davis–Mott [549] and Marshall–Owen [550]. Dashed lines represent the DOS of the same material without disorder

(a) DOS (arb. units)

(b)

EC

EV

EV

(c)

EC

DOS (arb. units)

(d)

EV

DOS (1022 eV-1cm-3)

-0.5 1.0

Energy

EC

EV

Energy (eV) 0.5

0.0

1.0

Energy

EC

1.5

a-Si

0.5

0

Fig. 6.55 Theoretical calculation of the density of electronic states of amorphous silicon. The charge distribution in four selected states at the indicated energies is shown, from right to left with decreasing localization. Adapted from [551]

E(k) =

M 2 2 k . 2 m ∗ i=1 i

(6.65)

The ki can take the values ±π n/L (in the first Brillouin zone) with n ≤ N , N being the number of unit cells in one dimension. These values are equidistant in k-space. Each M-dimensional k-point takes a 2 2 kF (later used as Fermi volume of (2π/L) M . The number of states N (E F ) up to the energy E F = 2m energy E F and Fermi vector kF ) is N (E F ) =

2 (2π/L) M

|k|=kF

k=0

dM k .

(6.66)

6.13 Density of States

177

Fig. 6.56 Theoretical calculation for the density of states of crystalline (dashed lines, conduction and valence bands indicated by greay areas) and amorphous ZnSnO3 with different configurations (solid lines). States due to under-coordinated oxygen (Ouc ) and metal-metal bonds are labelled. Adapted from [552]

ZnSnO3

Density of states (eV-1)

60

40

20

Ouc Sn-Sn

0

-1

0

Sn-Zn 2Sn 1Sn

1 2 3 Energy (eV)

4

5

The factor 2 is for spin degeneracy, the integration runs over M dimensions. The density of states is the derivative dN . (6.67) D(E) = dE In the following, the density of states for M = 3, 2, 1 and zero dimensions is derived. A visualization is given in Fig. 14.1.

6.13.3.1

M=3

This case relates to bulk material in which electrons are free to move in all three dimensions. Performing the integral (6.66) for M = 3 yields for an isotropic mass, N

3D

V 3 V = k = 3π 2 F 3π 2

2 m EF 2

3/2 .

(6.68)

Therefore, kF and E F are given by

1/3 3π 2 N kF = V

2/3 2 3π 2 N , EF = 2 m∗ V

(6.69) (6.70)

and the density of states in three dimensions is V D (E) = 2π 2 3D

2 m∗ 2

3/2

√

E.

(6.71)

Mostly the density of states is used as density of states per volume, then the factor V in (6.71) is omitted. If a conduction-band minimum is degenerate, a factor gv (valley degeneracy) must be included in the density of states, i.e. gv = 6 for Si and gv = 8 for Ge (gv = 1 for GaAs). This factor is typically included in the mass used in (6.71) that then becomes the density of states mass m d,e . If the conductionband minimum has cylindrical symmetry in k-space, such as for Si and Ge, the mass that has to be

178

6 Band Structure

used is

1/3 . m d,e = gv2/3 m 2t m l

(6.72)

In the case of a degeneracy of the valence band, the states of several bands need to be summed. In bulk material, typically the heavy and light hole bands are degenerate at the -point. If the split-off band is not populated because of insufficient temperature, the valence-band edge density of states is expressed by the density of states hole mass 2/3 3/2 3/2 . m d,h = m hh + m lh

(6.73)

The density of states (per volume) at the conduction and valence band edges are thus given by De3D (E) = Dh3D (E) 6.13.3.2

1 2π 2

1 = 2π 2

2 m d,e 2 2 m d,h 2

3/2

3/2

E − EC , E > EC

(6.74)

EV − E , E < EV .

(6.75)

M=2

This case is important for thin layers in which the electron motion is confined in one direction and free in a plane. Such structures are called quantum wells (see Sect. 12.3.2). We find for the 2D density of states (for each subband over which it is not summed here, including spin degeneracy) N 2D =

A 2 A m∗ kF = E, 2π π 2

(6.76)

where A is the area of the layer. The density of states is thus constant and given by D 2D (E) =

6.13.3.3

A m∗ . π 2

(6.77)

M=1

The case M = 1 describes a quantum wire in which the electron motion is confined in two dimensions and free in only one dimension. For this case, we find for a wire of length L N

1D

2L 2L kF = = π π

2m ∗ E 2

1/2 .

(6.78)

The density of states becomes singular at E = 0 and is given by (for one subband) D 1D (E) =

6.13.3.4

L π

2m ∗ 2

1/2

1 √ . E

(6.79)

M=0

In this case electrons have no degrees of freedom, as, e.g., in a quantum dot (Sect. 14.4), and each state has a δ-like density of states at each of the quantized levels.

Chapter 7

Electronic Defect States

Über Halbleiter sollte man nicht arbeiten, das ist eine Schweinerei, wer weiß ob es überhaupt Halbleiter gibt. One should not work on semiconductors. They are a mess. Who knows whether semiconductors even exist. W. Pauli, 1931[554]

Abstract After the carrier statistics for intrinsic conduction and general doping principles, donors and acceptors, compensation and high doping effects are treated in detail. The concept of quasi-Fermi levels is introduced. Finally for deep levels and their thermodynamics general remarks and several examples are given.

7.1 Introduction One cm3 of a semiconductor contains about 5 × 1022 atoms. It is practically impossible to achieve perfect purity. Typical low concentrations of impurity atoms are in the 1012 − 1013 cm−3 regime. Such a concentration corresponds to a purity of 10−10 , corresponding to about one alien in the world’s human population. In the beginning of semiconductor research the semiconductors were so impure that the actual semiconducting properties could only be used inefficiently. Nowadays, thanks to large improvements in high-purity chemistry, the most common semiconductors, in particular silicon, can be made so pure that the residual impurity concentration plays no role in the physical properties. However, the most important technological step for semiconductors is doping, the controlled incorporation of impurities, in order to manage the semiconductor’s conductivity. Typical impurity concentrations used in doping are 1015 − 1020 cm−3 . A milestone in the understanding of doping and the spreading of semiconductor technology was the 1950 textbook by Shockley [555].

7.2 Carrier Concentration Generally, the density of electrons in the conduction band is given by ∞ De (E) f e (E) dE ,

n=

(7.1)

EC

© Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_7

179

180

7 Electronic Defect States

and accordingly the density of holes in the valence band is EV Dh (E) f h (E) dE .

p=

(7.2)

−∞

The energy of the top of the valence band is denoted by E V , the bottom of the conduction band as E C . We assume here parabolic band edges, i.e. effective masses m h and m e for holes and electrons, respectively. The density of states (per volume) in the conduction band De and valence bands Dh is given by (6.74) and (6.75). The statistical distribution function for electrons is denoted by f e is given in thermodynamical equilibrium by the Fermi-Dirac distribution, (E.22), f e (E) =

exp

1 E−EF kT

+1

.

(7.3)

The distribution function for holes is f h = 1 − f e , f h (E) = 1 −

exp

1 E−EF kT

+1

=

1 . E−EF exp − kT + 1

(7.4)

If several hole bands (hh, lh, so) are considered, the same distribution is valid for all hole bands in thermal equilibrium. If the Boltzmann distribution (E.23) is a good approximation, the carrier distribution is called nondegenerate. If the Fermi-Dirac distribution needs to be invoked, the carrier ensemble is called degenerate. If the Fermi level is within the band, the ensemble is highly degenerate. If the Boltzmann approximation (E.23) cannot be applied, i.e. at high temperatures or for very small band gaps, the integral over D f cannot be analytically evaluated. In this case the Fermi integral is needed that is defined1 as ∞ yn 2 Fn (x) = √ dy . (7.5) 1 + exp(y − x) π 0

In the present case of bulk materials n = 1/2. For large negative argument, i.e. x < 0 and |x| 1, approximation. F1/2 (0) = 0.765 . . . ≈ 3/4. For large F1/2 (x) ≈ exp(x), which is the Boltzmann √ argument, i.e. x 1, F1/2 (x) ≈ (2/ π )(2/3)x 3/2 . Such fairly simple approximations are plotted in Fig. 7.1 in comparison with the Fermi integral. For computations, analytical [556–559] or numerical approximations [560, 561] are used. > 0. For n = 0, i.e. a The derivative of the Fermi integral is given by Fn (x) = n Fn−1 (x), n √ two-dimensional system, the integral can be executed explicitly, F0 (x) = (2/ π) ln[1 + exp(x)]. With the Fermi integral F1/2 (7.10) and (7.11) the free-carrier densities can be written as EF − EC kT EF − EV , p = NV F1/2 − kT

n = NC F1/2

(7.5) is restricted to n > −1. A form without restriction is Fn (x) = 2/ π is often omitted but must be then added explicitly in, e.g., (7.6). 1 Equation

√

(7.6) (7.7)

1 (n+1)

∞ 0

yn 1+exp(y−x) dy.

The factor

7.2 Carrier Concentration

181

(a)

(b)

√ ˆ Fig. √ 1/2 with approximations in three regions of the argument: A1 (x) = √ 7.1 Fermi integral F1/2 = ( π/2)F ( π/2) exp(x) for x < 2, A2 (x) = ( π/2)(1/4 + exp(−x))−1 for −2 < x < 2, A3 (x) = 2/3x 3/2 for x > 2. a linear, b semilogarithmic plot Table 7.1 Band gap, intrinsic carrier concentration, conduction band and valence-band edge density of states at T = 300 K for various semiconductors InSb InAs Ge Si GaAs GaP GaN

E g (eV)

n i (cm−3 )

0.18 0.36 0.67 1.124 1.43 2.26 3.3

1.6 × 1016 8.6 × 1014 2.4 × 1013 1.0 × 1010 1.8 × 106 2.7 × 100 1

NC (cm−3 )

NV (cm−3 )

1.04 × 1019 7.28 × 1019 4.35 × 1017

6.0 × 1018 1.05 × 1019 5.33 × 1018

with

m e kT 3/2 NC = 2 2π 2 m h kT 3/2 , NV = 2 2π 2

(7.8) (7.9)

where NC (NV ) is called the conduction-band (valence-band) edge density of states. The masses in (7.8) and (7.9) are the density of states masses given in (6.72) and (6.73). Values of NC,V for Si, Ge and GaAs are given in Table 7.1. Now, we assume that the Boltzmann approximation (E.23) can be used, i.e. the probability that a band state is populated is 1. Then, the integral (7.1) can be executed analytically and the concentration n of electrons in the conduction band is given as n=2

m e kT 2π 2

3/2 exp

EF − EC kT

= NC exp

EF − EC kT

.

(7.10)

For the Boltzmann approximation and a parabolic valence band, the density of holes is given by

m h kT p=2 2π 2

3/2

EF − EV exp − kT

EF − EV = NV exp − kT

.

(7.11)

182

7 Electronic Defect States

(a)

(b)

Fig. 7.2 a np for silicon at T = 300 K as a function of the position of the Fermi level. The valence-band edge E V is √ chosen as E = 0. np is constant for the range of Fermi energies given by (7.13) (4kT ≈ 0.1 eV). b n, p and np as a function of the Fermi level

Within the Boltzmann approximation, the product of the electron and hole density is Eg EC − EV = NV NC exp − n p = NV NC exp − kT kT 3 Eg kT (m d,e m d,h )3/2 exp − . =4 2π 2 kT

(7.12)

Thus, the product n p is independent of the position of the Fermi level, as long as the Boltzmann approximation is fulfilled. This is the case when the Fermi level lies within the band gap and it is sufficiently far away from the band edges, fulfilling about E V + 4 kT < E F < E C − 4 kT .

(7.13)

The relation (7.12) is called the mass-action law. In Fig. 7.2, the product np is shown for silicon over a wide range of Fermi energies. If E F is within the band gap, np is essentially constant. If the Fermi level is in the valence or conduction band, np decreases exponentially.

7.3 Intrinsic Conduction First, we consider the conductivity of the intrinsic, i.e. an ideally pure, semiconductor. At T = 0 all electrons are in the valence band, the conduction band is empty and thus the conductivity is zero (a completely filled band cannot conduct current). Only at finite temperatures the electrons have a finite probability to be in a conduction-band state and to contribute to the conductivity. Due to neutrality, the electron and hole concentrations in the intrinsic semiconductors are the same, i.e. each electron in the conduction band comes from the valence band, −n+ p =0, or n i = pi . Therefore

(7.14)

7.3 Intrinsic Conduction

183

(a)

(b)

Fig. 7.3 a Band gap of silicon versus temperature. b Intrinsic carrier concentration of silicon versus temperature. Solid line is (7.17) using E g = 1.204 eV − (2.73 × 10−4 eV/K) T [564], symbols are experimental data from [565]

Eg n i = pi = NV NC exp − 2kT 3/2 Eg kT 3/4 (m m ) exp − . =2 e h 2π 2 2kT

(7.15)

The mass-action law n p = n i pi = n 2i = pi2

(7.16)

will be essential also for light and moderately doped semiconductors. The intrinsic carrier concentration is exponentially dependent on the band gap. Thus, in thermodynamic equilibrium intrinsic wide-gap semiconductors have much smaller electron concentrations than intrinsic small-gap semiconductors (see Table 7.1). The intrinsic carrier concentration of Si (in cm−3 ) has been determined to be (within 1%, T in K) E g (T ) Si 15 1.706 exp − (7.17) n i = 1.640 × 10 T 2kT for temperatures between 77 and 400 K [562, 563] (Fig. 7.3). As we will see later in Part II, many semiconductor devices rely on regions of low conductivity (depletion layers) in which the carrier concentration is small. Since the carrier concentration cannot be smaller than the intrinsic concentration (n + p ≥ 2n i ), an increase of temperature leads to increasing ohmic conduction in the depletion layers and thus to a reduction or failure of device performance. The small band gap of Ge leads to degradation of bipolar device performance already shortly above room temperature. For silicon, intrinsic conduction limits operation typically to temperatures below about 300 ◦ C. For higher temperatures, as required for devices in harsh environments, such as close to motors or turbines, other semiconductors with wider band gaps need to be used, such as GaN, SiC or even diamond. From the neutrality condition for the intrinsic semiconductor (7.14) and (7.10) and (7.11), the Fermi level of the intrinsic semiconductor can be determined as EV + EC kT NV 3 mh EV + EC + ln + kT ln = . (7.18) EF = Ei = 2 2 NC 2 4 me Since the hole mass is perhaps a factor of ten larger than the electron mass, the second term has the order of kT . Thus, for typical semiconductors where E g kT , the intrinsic Fermi level, denoted by E i , is close to the middle of the band gap, i.e. E i ≈ (E C + E V )/2.

184

7 Electronic Defect States

Fig. 7.4 Density of states (left column), Fermi distribution (center column) and carrier concentration (right column) for a n-type, b intrinsic and c p-type semiconductors in thermal equilibrium

E

E

EC ED

EF

E

nn

EC

EV

EV

p

(a) E

D(E)

E

f(E)

EC

n,p

E

EC

n

EV

p

EF EV (b) E

D(E)

E

f(E)

EC

n,p

E

EC

n

EF

EA EV

EV

p

(c) D(E)

f(E)

n,p

The situation for an intrinsic semiconductor is schematically shown in Fig. 7.4b. In the following we will consider doping which can shift the Fermi level away from E i . Within the Boltzmann approximation (also n i = pi ),

EF − Ei kT EF − Ei . p = pi exp − kT

n = n i exp

(7.19) (7.20)

7.4 Doping 7.4.1 Concept The modification of the conductivity of a semiconductor using point defects is termed doping. In 1930 electrical conduction of semiconductors was attributed solely to impurities [566, 567]. However ‘chemically pure’ substances become conductive upon deviation from stoichiometry, e.g. historically

7.4 Doping

ZnO

NiO

MgO

E-EV

Fig. 7.5 Comparison of ZnO, NiO and MgO on a common energy scale, comparing conduction band and valence band edges and n-type (red) and p-type (blue) pinning energies (determined for metal-rich and oxygen-rich conditions, respectively). Adapted from [571]

185

found for changes in the anion concentration and conductivity in CuI [38] (p-type) and ZnO [80] (ntype). The modification of CuI by exposure to different partial pressure of iodine in organic solutions with different iodine concentration [41] and subsequently various concentrations of copper vacancies [568] can be considered the first doping of a semiconductor (1909). The electronic levels of a defect or an impurity can exist within the forbidden gap of the bulk host material. These levels can lie close to the band edges or in the vicinity of the middle of the band gap. In a simplified approach, the first stem from shallow defects (Sect. 7.5), the latter from deep defects (Sect. 7.7).

7.4.2 Doping Principles In [569] various doping principles are formulated. Essentially, the amount of impurities that lead to electrically active dopants is limited by the increasingly probable formation of compensating defects. In the case of donors, these are electron killers, e.g. n-type doping of Si:As is limited by the formation of VSi [570]. In the case of acceptors, the compensating defects are hole killers. The so-called n-type n,pin pinning energy E F is the Fermi level at which such killer defect (e.g. a cation vacancy) forms. When the Fermi level reaches the pinning energy, no further progress in n-type doping can be made, since the spontaneously generated electron killers will negate the introduced (impurity) donors. As a tendency, materials with low lying conduction band, i.e. large electron affinity (difference between vacuum level and conduction band) can be doped n-type. Similarly, p-type doping by acceptors, shifting the Fermi p,pin level towards the valence band, will meet at some point E F , called p-type pinning energy, when native hole killers, such as anion vacancies or cation interstitials form spontaneously. At this point, further p-type doping is no longer possible. p-type doping is facilitated by materials whose valance band maximum is close to the vacuum level [569]. A comparison of the wide gap materials ZnO, NiO and MgO is depicted in Fig. 7.5. The position of n,pin the pinning levels is marked on a common energy scale. From the position of E F it can be understood, p,pin that ZnO can be highly n-doped while NiO and MgO cannot [571]. From E F , NiO can be doped p-type, while MgO cannot be doped at all. For dopability, generally, it is also important that the ionized charges from impurities are free and thus contribute to the free charge carrier density and do not form localized states, e.g. due to polaronic effects (Sect. 8.7).

186

7 Electronic Defect States

(a)

(b)

(c) Fig. 7.6 Energetic position (ionization energy labeled in meV) of various impurities (A: acceptor, D: donor) in a Ge, b Si and c GaAs. Based on [574]

7.5 Shallow Defects In Fig. 7.6, the positions of the energy levels of a variety of impurities are shown for Ge, Si and GaAs. An impurity for which the long-range Coulomb part of the ion-core potential determines the energetic level is termed a shallow impurity. The extension of the wavefunction is given by the Bohr radius. This situation is in contrast to a deep level where the short-range part of the potential determines the energy level. The extension of the wavefunction is then of the order of the lattice constant. A view on the history of the science of shallow impurity states is given in [572, 573]. We will consider first a group-IV semiconductor, Si, and (impurities) dopants from the groups III and V of the periodic system. When these are incorporated on a lattice site (with tetrahedral bonds), there is one electron too few (group III, e.g. B) or one electron too many (group V, e.g. As). The first case is called an acceptor, the latter a donor. The doping of III–V semiconductors is detailed in [575].

7.5 Shallow Defects

187

Fig. 7.7 Arsenic impurity in silicon. Arsenic donates one electron, and a fixed positive charge remains

Si

Si As

Si Si

Si

Si

Si

7.5.1 Donors Silicon doped with arsenic is denoted as Si:As. The situation is schematically shown in Fig. 7.7. The arsenic atom has, after satisfying the tetrahedral bonds, an extra electron. This electron is bound to the arsenic atom via the Coulomb interaction since the ion core is positively charged compared to the silicon cores. If the electron is ionized, a fixed positive charge remains at the As site. Without being in the silicon matrix, an arsenic atom has an ionization energy of 9.81 eV. However, in the solid the Coulomb interaction is screened by the dielectric constant of the material, typically r is of the order of 10 for typical semiconductors. Additionally, the mass is renormalized (effective mass) by the periodic potential to a value that is smaller than the free electron mass. Within effective-mass theory (Appendix I) the hydrogen problem is scaled with the (isotropic) effective mass m ∗e and the dielectric constant r , the binding energy (ionization energy) E Db of the electron to the shallow donor is (relative to the continuum given by the conduction-band edge E C ) E Db =

m 0 e4 m ∗e 1 . 2 m 0 r 2 (4π 0 )2

(7.21)

The scaling with 1/ 2 has been pointed out first in [576]. The absolute energy position of the level is E D = E C − E Db . The first factor in the right side of (7.21) is the ratio of effective and free-electron mass, typically 1/10, the second factor is typically 1/100. The third factor is the ionization energy of the hydrogen atom, i.e. the Rydberg energy of 13.6 eV. Thus, the binding energy in the solid is drastically reduced by a factor of about 10−3 to the 10 meV regime. The excited states of the hydrogen-like spectrum can also be investigated experimentally (Sect. 9.8). The extension of the wavefunction of the electron bound to the fixed ion is given by the Bohr radius aD =

m0 r a B , m ∗e

(7.22)

where aB = 0.053 nm denotes the hydrogen Bohr radius. For GaAs aD = 10.3 nm. A similar value has been determined for InP [577]. For semiconductors with a nonisotropic band minimum, such as Si, Ge or GaP, an ‘elliptically deformed’ hydrogen problem with the masses m l and m t has to be treated [578]. An impurity that fulfills (7.21) is called an effective-mass impurity. For GaAs, the effective-mass donor has a binding energy of 5.715 meV, which is closely fulfilled for several chemical species (Table 7.3). In GaP, experimental values deviate considerably from the effective-mass donor (59 meV). For silicon, considering the anisotropic tensor of the effective masses, the result for the effectivemass donor binding energy is 29 meV [578]. Some experimentally observed values are summarized in Table 7.2. Deviations from the effective-mass theory are due to modification of the potential in the immediate vicinity of the impurity atom and breakdown of the effective-mass formalism. Different impurities can have quite similar binding energies. They can be distinguished, e.g., by electron spin resonance (ESR). At low temperatures the electron is localized on the impurity and the hyperfine interaction with the nucleus can be resolved in ESR. In Fig. 7.8 data are shown for As and P

188

7 Electronic Defect States

Fig. 7.8 Electron spin resonance signal from As and P in Ge with the magnetic field H parallel to [100], T ≈ 1.3 K. Adapted from [579]

Table 7.2 Binding energies E Db of Li and group-V donors in elemental semiconductors. Data for carbon from [580]. All values in meV Li C Si Ge

N

P

As

Sb

1700

≈500 45 12.0

49 12.7

39 9.6

33 9.3

Table 7.3 Binding energies E Db of donors in GaAs (data from [581]), GaP (data from [582]) and GaN (low concentration limits, data from [583, 584]). All values in meV V site GaAs

GaP

GaN

S Se Te O S Se Te O

III site 5.854 5.816 5.786 897 107 105 93 39

C Si Ge Si Ge Sn

5.913 5.801 5.937 85 204 72

Si Ge

22 19

in germanium. The multiplets distinguish the nuclear spins I = 3/2 for arsenic (75 As) and I = 1/2 for phosphorus (31 P) [579]. The donors are typically distributed statistically (randomly) in the solid. Otherwise their distribution is called clustered. The concentration of donors is labeled ND and usually given in cm−3 . The concentration of donors populated with an electron (neutral donors) is denoted by ND0 , the concentration of ionized donors (positively charged) is ND+ . Other conventions in the literature label the concentrations N1 and N0 , respectively: N1 = ND0 = ND f e (E D ) N0 = ND+ = ND (1 − f e (E D )) ,

(7.23a) (7.23b)

with f e (E D ) = [1 + exp(E D − E F )]−1 . For the sum of these quantities the condition ND = ND+ + ND0 holds.

(7.24)

7.5 Shallow Defects

189

The ratio of the two concentrations is first given as (caveat: this formula will be modified below) N1 f ND0 = = = exp N0 1− f ND+

EF − ED kT

.

(7.25)

Now, the degeneracy of the states has to be considered. The donor charged with one electron has a 2-fold degeneracy g1 = 2 since the electron can take the spin up and down states. The degeneracy of the ionized (empty) donor is g0 = 1. Additionally, we assume here that the donor cannot be charged with a second electron (cmp. Sect. 7.7.2). Due to Coulomb interaction, the energy level of the possible ND− state is in the conduction band. Otherwise, a multiply charged center would be present. We also do not consider excited states of ND0 that might be in the band gap as well. In the following, we will continue with gˆ D = g1 /g0 = 2 as suggested in [585].2 We note that the definition of the degeneracy factor for donors (and acceptors, see (7.38)) is not consistent in the literature as summarized in [586]. Considering now the degeneracy, (7.25) is modified to N1 ND0 = = gˆ D exp N0 ND+

EF − ED kT

.

(7.26)

This can be understood from thermodynamics (cf. Sect. 4.2.2), a rate analysis or simply the limit T → ∞. The probabilities f 1 and f 0 for a populated or empty donor, respectively, are N1 1 = −1 ED −EF ND +1 gˆ D exp kT N 1 0 = . f0 = −E F ND +1 gˆ D exp − EDkT f1 =

(7.27a) (7.27b)

First, we assume that no carriers in the conduction band stem from the valence band (no intrinsic conduction). This will be the case at sufficiently low temperatures when ND n i . Then the number of electrons in the conduction band is equal to the number of ionized donors, i.e. n = f 0 ND = N0 =

ND 1 + gˆ D exp

EF −ED = kT

1 ND , 1 + n/n 1

with n 1 = (NC /gˆ D ) exp(−E Db /kT ). The neutrality condition (its general from is given in equation (7.40)) is (7.28) − n + ND+ = −n + N0 = 0 , leading to the equation (n is given by (7.10)) NC exp

EF − EC kT

−

ND −ED = 0 . 1 + gˆ exp EFkT

(7.29)

Solving this equation will yield the Fermi level (as a function of temperature T , doping level E D and doping concentration ND ).3 The solution is 2 We do not agree with the treatment of the conduction band valley degeneracy in [585] for the donor degeneracy factor for Ge and Si. 3 As usual, the Fermi level is determined by the global charge neutrality, see also Sect. 4.2.2.

190

7 Electronic Defect States

⎛ 1 + 4gˆ D ⎜ E F = E C − E Db + kT ln ⎝

ND NC

exp

E Db kT

1/2

−1

2 gˆ D

⎞ ⎟ ⎠ .

(7.30)

For T → 0 the Fermi level is, as expected, in the center between the populated and unpopulated states, i.e. at E F = E C − E Db /2. In Fig. 7.9a the position of the Fermi is shown for a donor with 45 meV binding energy in Si. For low temperatures the solution can be approximated as (dashed curve in Fig. 7.9b) 1 1 ND . EF ∼ = E C − E Db + kT ln 2 2 gˆ D NC

(7.31)

The freeze-out of carriers in n-type silicon has been discussed in detail in [587], taking into account the effects of the fine structure of the donor states. We note that the fairly high donor binding energy in silicon leads to freeze-out of carriers at about 40 K and is thus limiting for the low-temperature performance of devices. Ge has smaller donor ionization energies and subsequently a lower freeze-out temperature of 20 K. For n-type GaAs, conductivity is preserved down to even lower temperatures. We note that the freeze-out of carriers involves the recombination of free electrons with the ionized donors. This aspect is considered in Sect. 10.9. Microscopically this process is equal to the emission of a (far infrared) photon [588, 589]. Similarly the release of an electron from the donor is due to the absorption of a photon. For higher temperatures, when the electron density saturates towards ND , the approximate solution is (dash-dotted curve in Fig. 7.9a) EF ∼ = E C + kT ln

ND NC

.

(7.32)

The electron density n is given (still in the Boltzmann approximation) by n = NC exp − =

1+ 1+

E Db

1 + 4 gˆ D

exp

E Db kT

1/2

2 gˆ D

kT 2 ND

4 gˆ D NNDC

ND NC

exp

E Db kT

−1 (7.33)

1/2 .

The theoretical electron density as a function of temperature is shown in Fig. 7.9b. It fits very well to experimental data for arsenic doped germanium [594] as shown in Fig. 7.10 (Arrhenius plot, ln n vs. 1/T ). For low temperatures, the solution (7.34) is close to n∼ =

ND NC E Db exp − = n 1 ND . gˆ D 2kT

(7.34)

For high temperatures, n ∼ = ND . This regime is called exhaustion or saturation since all possible electrons have been ionized from their donors. We note that even in this case np = n i pi holds, however, n p. While the characteristic energy for the ionization of electrons from donors is E Db , at high enough temperatures electrons are transferred also from the valence band into the conduction band. Thus, in order to make the above consideration valid for all temperatures, the intrinsic conduction also has to

7.5 Shallow Defects

191

(a)

(b)

Fig. 7.9 a Position of the Fermi level in Si:P (ND = 1015 cm−3 , E Db = 45 meV, no acceptors) as a function of temperature without consideration of intrinsic carriers. Zero energy refers to the (temperature-dependent, Table 6.4) conduction-band edge E C with approximative solutions for low (dashed line, (7.31)) and high (dash-dotted line, (7.32)) temperatures. b Corresponding density of conduction-band electrons as a function of temperature Fig. 7.10 Electron concentration as a function of temperature for a Ge:As sample with ND ≈ 1013 cm−3 . Solid line is fit to the data with a donor binding energy of 12.7 meV. Adapted from [594]

300 78

33.3

14

20.4

14.3

10

Ge:As

3

10

1013

1012 ni 1011 0

20

60 40 1000/T (1/K)

80

100

be considered. The neutrality condition (still in the absence of any acceptors) is − n + p + ND+ = 0 .

(7.35)

Using (7.10) and p = n 2i /n, the equation reads: NC exp

EF − EC kT

−

n 2i

−E C NC exp( EFkT )

−

ND −E D 1 + gˆ D exp( EFkT )

=0.

(7.36)

The solution can be given analytically but is more complicated4 . The temperature-dependent position of the Fermi level is shown in Fig. 7.11. The three important regimes are the intrinsic conduction at high temperatures when n i ND , the exhaustion at intermediate temperatures when n i ND and kT > E Db , and finally the freeze-out regime for kT E Db at low temperatures when the electrons condense back into the donors. The three 4 It

is given in the third edition of this book.

192

7 Electronic Defect States

Fig. 7.11 Position of the Fermi level in Si:P (ND = 1015 cm−3 , E Db = 45 meV, no acceptors) as a function of temperature. The temperature dependence of the band gap (as given in Table 6.4) has been taken into account. Zero energy refers to the conduction-band edge for all temperatures. The dotted curve shows E g /2. The dashed (dash-dotted) line shows the low- (high-) temperature limit according to (7.31) and (7.18), respectively. The corresponding electron concentration as a function of temperature is shown in Fig. 7.9b Fig. 7.12 Fermi level in silicon as a function of temperature for various doping levels (n-type (blue lines) and p-type (red lines)) of 1012 , 1013 , . . . , 1018 cm−3 . The intrinsic Fermi level is chosen as zero energy for all temperatures. The (temperature-dependent) conduction and valence band edges are shown as dashed lines

regimes can be seen in the experimental data on carrier density of electrons in n-Ge (Fig. 7.10) and of holes in p-Ge (Fig. 7.15). A similar plot as in Fig. 7.11 is shown in Fig. 7.12 but for different doping levels. With increasing temperature, the Fermi level shifts from close to the band edge towards the band center. At higher doping, this shift begins at higher temperatures. The electronic states of individual donors can be directly visualized by scanning tunneling microscopy (STM) as shown in Fig. 7.13 for Si:P. For small negative bias, tunneling occurs through the charged dopant that is located within the first three monolayers. At high negative bias the large contribution from the filled valence band masks the effect of the donor. This image, however, shows that the contrast attributed to the dopant atom is not due to surface defects or absorbates.

7.5.2 Acceptors A group-III atom in Si has one electron too few for the tetrahedral bond. Thus, it ‘borrows’ an electron from the electron gas (in the valence band) and thus leaves a missing electron (termed hole) in the

7.5 Shallow Defects Fig. 7.13 Filled-state image of a phosphorus atom underneath a Si (001) surface at a tunneling current of 110 pA. The doping level is 5 × 1017 cm−3 . a Sample bias −0.6 V, b sample bias −1.5 V between Si:P and tip. Image sizes are 22 × 22 nm2 . Reprinted with permission from [595], ©2004 APS. Lower row under parts b, c: Schematic band diagrams for the two bias situations

193

(a)

(b)

tip

Si EF

D EF

Fig. 7.14 Boron impurity in silicon. Boron accepts one electron and a fixed negative charge remains

Si

Si Si

Si

Si B

Si

Si

valence band (Fig. 7.14). The energy level of the impurity is in the gap close to the valence-band edge. The latter consideration is made in the electron picture. In the hole picture, the acceptor ion has a hole and the hole ionizes (at sufficient temperature) into the valence band. After ionization the acceptor is charged negatively. Also, for this system a hydrogen-like situation arises that is, however, more complicated than for donors because of the degeneracy of the valence bands and their warping. In Table 7.4 the acceptor binding energies E Ab for group-III atoms in C, Ge and Si are listed. The absolute acceptor energy is given as E A = E V + E Ab . In Table 7.5 acceptor binding energies are listed for GaAs, GaP and GaN. While in GaAs some acceptors are close to the effective mass value of 27 meV, in GaP the deviation from the effective-mass value ≈50 meV is large. When the conductivity is determined by holes or electrons, the material is called p-type or n-type, respectively. We note that some metals also show hole conduction (e.g. Al). However, for metals the

194

7 Electronic Defect States

Table 7.4 Binding energies E Ab of group-III acceptors in elemental semiconductors. Data for diamond from [596, 597]. All values in meV C Si Ge

B

Al

Ga

In

369 45 10.4

57 10.2

65 10.8

16 11.2

Table 7.5 Binding energies E Ab of acceptors in GaAs, GaP and GaN (low concentration values, data from [598, 599]). All values in meV V site GaAs

GaP

GaN

III site

C Si Ge Sn C Si Ge

27 34.8 40.4 167 54 210 265

C Si

230 224

Be Mg Zn Cd Be Mg Zn Cd Mg Zn Cd

28 28.8 30.7 34.7 57 60 70 102 220 340 550

conductivity type is fixed, while the same semiconductor can be made n- or p-type with the appropriate doping. The acceptor concentration is denoted by NA . The concentration of neutral acceptors is NA0 , the concentration of charged acceptors is NA− . Of course NA = NA0 + NA− .

(7.37)

The ratio of the degeneracy of the (singly) filled and empty acceptor level is gˆ A . In Ge gˆ A = 4 since the localized hole wave function may be formed in EMA with four Bloch wave functions (heavy and light holes) [600]. For Si with its small split-off energy (Table 6.6) gˆ A = 6 according to [601]. For doubly ionized acceptors, e.g. Zn in Si and Ge (see Sect. 7.7.3), the more shallow level (Zn− → Zn0 ) has gˆ A = 6/4 = 1.5 in Ge [601]. A more general discussion of the degeneracy factor for multiply charged acceptors can be found in [585, 602]. Similar to the considerations for electrons and donors we have EF − EA NA0 = g ˆ exp − . (7.38) A kT NA− The population of the acceptor levels is given by NA− =

NA . −E A 1 + gˆ A exp − EFkT

(7.39)

The formulas for the position of the Fermi level and the hole density are analogous to those obtained for electrons and donors and will not be explicitly given here. The analogue to Fig. 7.11b is shown for data on p-doped Ge [603, 604] in Fig. 7.15. The acceptor activation energy is 11 meV which could be

7.5 Shallow Defects

195

Fig. 7.15 Carrier concentration as a function of temperature for p-type Ge. The net shallow level concentration is 2 × 1010 cm−3 . Solid line is fit to the data, the dashed line indicates the intrinsic hole concentration pi . Adapted from [604]

due to various impurities (cf. Table 7.4). The different impurities (B, Al, Ga) can be distinguished by photothermal ionization spectroscopy [604] (cmp. Sect. 9.8). In Fig. 7.12, the temperature dependence of the Fermi level is included for p-type Si. With increasing temperature the Fermi level shifts from the valence-band edge (For T = 0, E F = E V + E Ab /2) towards the middle of the band gap (intrinsic Fermi level). Also, the wavefunction at acceptors can be imaged using scanning tunneling microscopy [605]. In [606] images of ionized and neutral Mn in GaAs have been reported (Fig. 7.16b). The tunneling I –V characteristics are shown in Fig. 7.16a. At negative bias, the acceptor is ionized and appears spherically symmetric due to the effect of the A− ion Coulomb potential on the valence-band states. At intermediate positive voltages, tunneling is through the neutral state. The wavefunction of A0 looks like a bow-tie due to the admixture of d-wavefunctions [607]. The Mn atom is presumably in the third subsurface atomic layer. At even higher positive bias the contrast due to the dopant is lost because the image is dominated by a large tunneling current from the tip to the empty conduction band.

7.5.3 Compensation When donors and acceptors are simultaneously present, some of the impurities will compensate each other. Electrons from donors will recombine with holes on the acceptors. Depending on the quantitative situation the semiconductor can be n- or p-type. This situation can be invoked by intentional doping with donors or acceptors or by the unintentional background of donors (acceptors) in p-doped (n-doped) material. Also the formation of pairs, exhibiting a new defect level different from the single donor or single acceptor, has been described, e.g. for Se and B in silicon [308]. The charge-neutrality condition (now finally in its most general form) reads − n + p − NA− + ND+ = 0 .

(7.40)

We will now discuss the case of the presence of donors and acceptors, but limit ourselves to sufficiently low temperatures (or wide band gaps) such that the intrinsic carrier density can be neglected. We assume Boltzmann statistics and assume here ND > NA . Then it is a very good approximation to use NA− = NA

196

7 Electronic Defect States (b)

(c)

GaAs:Mn 40 Mn A0 channel 20 GaAs

UFB

EF

MnGa

0

A

GaAs

-0.8

-0.4

0.0

0.4

0.8

1.2

tip

EF

A

1.6

(a)

negative bias

Fig. 7.16 a Tunneling I –V characteristic of GaAs:Mn sample. Solid (dashed) line is for pure GaAs (subsurface Mn on Ga site). UFB denotes the simulated flat-band voltage. Adapted from [606]. (b, c) STM images of a Mn atom underneath a GaAs (110) surface. The doping level is 3 × 1018 cm−3 . b Sample bias −0.7 V, c sample bias +0.6 V. Below the images are schematic band diagrams of GaAs:Mn and tip. Image sizes are b 8 × 8 nm2 and c 5.6 × 5 nm2 . Reprinted with permission from [606], ©2004 APS. Lower row under parts a, b: Schematic band diagrams for the two bias situations

since there are enough electrons from the donors to recombine with (and thus compensate) all acceptors. Under the given assumptions regarding the temperature p = 0 and the material is n-type. Thus, in order to determine the position of the Fermi level, the charge-neutrality condition n + NA − ND+ = 0

(7.41)

must be solved (compare to (7.29)) NC exp

EF − EC kT

+ NA −

ND −E D 1 + gˆ exp( EFkT )

We rewrite (7.41) and find ND − NA − n = ND0 = ND+ gˆ D exp and also (7.10), (7.42) can be written as

EF −ED kT

=0.

(7.42)

using (7.26). Using again (7.41)

Eb NC n (n + NA ) exp − D , = ND − NA − n gˆ D kT

(7.43)

a form given in [608]. Analogously for compensated p-type material Eb NV p ( p + ND ) exp − A = NA − ND − p gˆ A kT

(7.44)

holds. The solution of (7.42) is ⎛ ⎜ E F = E C − E Db + kT ln ⎝

α + 2

A 4gˆ D NDN−N C

exp

2 gˆ D

E Db kT

1/2

−α

⎞ ⎟ ⎠ ,

(7.45)

7.5 Shallow Defects

197

(a)

(b)

Fig. 7.17 a Position of Fermi level in partially compensated Si:P,B (ND = 1015 cm−3 , E Db = 45 meV, E Ab = 45 meV, solid line: NA = 1013 cm−3 , dashed line: NA = 0, dash-dotted line: NA = 1012 cm−3 , short-dashed line: NA = 1014 cm−3 , dash-double dotted line: NA = 5 × 1014 cm−3 ) as a function of temperature. b Corresponding electron concentration for NA = 1013 cm−3 as a function of temperature (neglecting intrinsic carriers), dashed line for NA = 0 according to (7.34), dash-dotted line approximation for n NA as in (7.49)

with b NA ED NA α = 1 + gˆ D exp =1+ NC kT β E Db NC exp − . β= gˆ D kT

(7.46a) (7.46b)

The carrier density is best obtained from (7.43), 2n =

(NA − β)2 + 4 ND β − (NA + β) .

(7.47)

For NA = 0 we have α = 1 and (7.30) is reproduced, as expected. For T = 0 (and NA = 0) the Fermi energy lies at E F = E D since the donor level is partially filled (ND0 = ND − NA ). For low temperatures the Fermi level is approximated by EF ∼ = E C − E Db + kT ln

ND /NA − 1 gˆ D

.

(7.48)

The corresponding carrier density at low temperatures is E Db ND NC exp − −1 . n= gˆ D kT NA

(7.49)

For higher temperatures (7.34) holds approximately for n > NA ; the slope is now given by E Db /2 as in the uncompensated case (Fig. 7.17b). For sufficiently high temperatures in the exhaustion regime (but still n i < n) the electron density is given by n∼ = ND − NA .

(7.50)

At even higher temperatures the electron density will be determined by the intrinsic carrier concentration. Only in this case p = 0!

198

7 Electronic Defect States

Fig. 7.18 Hole density in p-type silicon (NA = 7.4 × 1014 cm−3 , E Ab = 46 meV (probably boron) and partial compensation with ND = 1.0 × 1011 cm−3 ). Adapted from [609]

Fig. 7.19 Carrier concentration and conductivity type (red circles: p, blue squares: n) for MOVPE-grown Inx Ga1−x As1−y N y layers on GaAs (001) (layer thickness ≈ 1 µm, x ≈ 5%, y ≈ 1.6%) doped with different amounts of silicon. The ordinate is the ratio of the partial pressures of disilane and the group-III precursors (TMIn and TMGa) in the gas phase entering the MOVPE reactor. Lines are guides to the eye. Experimental data from [610]

An experimental example is shown in Fig. 7.18 for partially compensated p-Si (with ND NA ). The change of slope around p ≈ ND is obvious. If donors are added to a p-type semiconductor, first the semiconductor remains p-conducting as long as ND NA . If the donor concentration becomes larger than the acceptor concentration, the conductivity type switches from p- to n-conduction. If the impurities are exhausted at room temperature, the lowest carrier concentration is reached for ND = NA . Such a scenario is shown for p-type Inx Ga1−x As1−y N y doped with various concentrations of Si in Fig. 7.19. At high Si incorporation, the number of charge carriers saturates due to autocompensation (see Sect. 7.5.5) and the formation of Si precipitates. Since the ionization energies of donors and acceptors are typically different, the situation for ND ≈ NA needs, in general, to be investigated carefully and will depend on the temperature.

7.5 Shallow Defects

199

7.5.4 Multiple Impurities If more than one donor species is present, (7.42) can be generalized, e.g. for the case of two donors D1 and D2 in the presence of compensating acceptors, n + NA −

ND1 1+

D1 gˆ 1 exp( EF −E ) kT

−

ND2 D2 1 + gˆ 2 exp( EF −E ) kT

=0.

(7.51)

This case is treated in [611]. Simple high and low temperature approximations can be found where the trap with the larger and smaller activation energy, respectively, dominates. The case for multiple acceptors (and compensating donors) is treated analogously. As detailed in [612], the function dn/dE F has a maximum at the donor level position; this can be used to visualize the contribution of several donors (with sufficiently different binding energies) from n(T ) as measured by Hall effect (Fig. 7.20).

7.5.5 Amphoteric Impurities If an impurity atom can act as a donor and acceptor it is called amphoteric. This can occur if the impurity has several levels in the band gap (such as Au in Ge or Si). In this case, the nature of the impurity depends on the position of the Fermi level. Another possibility is the incorporation on different lattice sites. For example, carbon in GaAs is a donor if incorporated on the Ga-site. On the As-site carbon acts as an acceptor. Thus, e.g., crystal growth kinetics can determine the conductivity type. In Fig. 7.21 the conductivity due to carbon background is shown for GaAs grown using MOVPE under various growth conditions. At high (low) arsine partial pressure incorporation of carbon on As-sites is less (more) probable, thus the conductivity is n-type (p-type). Also, growth on different surfaces can evoke different impurity incorporation, e.g., n-type on (001) GaAs and p-type on (311)A GaAs, since the latter is Ga-stabilized. The charge density at an impurity nucleus can be investigated via the isomer shift as determined by Mössbauer spectroscopy [614, 615]. The incorporation of the isotope 119 Sn can be controlled in III-V compounds to be on cation or anion site as donor or acceptor, respectively. This is accomplished by introducing 119 In or 119 Sb on group-III and group-V site, respectively, both decaying into 119 Sn

(a)

(b)

Fig. 7.20 a Electron concentration versus temperature as determined from Hall effect for a CdTe sample doped with indium. b −kT dn/dE F , as determined from the experimental Hall data (symbols). The solid line is theory for three donor levels (E D1 = E C −0.37 eV, ND1 = 2.5×1012 cm−3 ; E D2 = E C −0.24 eV, ND2 = 7.0×1011 cm−3 ; E D3 = E C −0.18 eV, ND3 = 2.5 × 1011 cm−3 ) whose energy positions are indicated by dashed lines. Adapted from [612]

200

7 Electronic Defect States

without leaving their lattice site. The isomer shifts of 119 Sn in various III-V compounds are shown in Fig. 7.22. In [615] it is concluded from these data that the tin donor is formed by a positive tin ion and the electron charge transfer to its neighboring (group-V) atoms is rather small. For tin as an acceptor, for the present conditions an ionized, i.e. negatively charged acceptor, the isomer shift follows closely the trend from substitution in group-IV semiconductors. Therefore four electrons form the tetrahedral bond, while the extra electron is located rather at the (positively charged) group-III next neighbors and not in the impurity cell. The difference to the point charge Coulomb distribution is called central-cell correction. Deviation from the ideal stoichiometry introduces point defects that can be electrically active and change conductivity type and carrier concentration. In the case of CuInSe2 , excess Cu could go on interstitial positions or promote selenium vacancies, both leading to n-type behavior. This material is particularly sensitive to deviations from ideal stoichiometry for both Cu/In ratio (Fig. 7.23) and Se deficiency [616].

7.5.6 Autodoping If intrinsic defects such as vacancies or interstitials, possibly as a result of non-stoichiometry, or antisite defects cause electronic levels relevant for conductivity one speaks of autodoping. An example is the role of A-B antisites in AB2 O4 spinels (Sect. 3.4.7). In the perfect crystal the A (B) atoms occupy tetraeder (octaeder) places. Typical charges are A2+ and B3+ . Thus (without charge transfer) the A

Fig. 7.21 Background doping of GaAs due to carbon in MOVPE for different ratios of the partial pressures of AsH3 and TMG (trimethylgallium). The conductivity type (blue squares: n-type, red circles: p-type) depends on the incorporation of C from CH3 radicals on Ga- or As-site. Lines are guides to the eye. Experimental data from [613] Fig. 7.22 Isomer shift (relative to CaSnO3 ) of 119 Sn in various group-IV and III-V compound semiconductors as labeled. Dashed line is trend from isoelectronic substitution. Experimental data from [615]

7.5 Shallow Defects

201

Fig. 7.23 Carrier concentration and conductivity type (blue squares: n-type, red circles: p-type) as a function of stoichiometry for CuInSe2 thin films. Lines are guides to the eye. Experimental data from [616]

Fig. 7.24 Schematic position of electronic levels of AB (blue, 0/− transition level) and BA (red, +/0 transition level) defects in AB2 O4 spinels and resulting material properties (compensated, n- or p-type or semi-insulating). After [617]

comp. p-type n-type

s.i.

CB BTd EF Aoh VB

atom on octaeder site (AOh ) acts like a donor and the B atom on a tetraeder site (BTd ) as an acceptor. Such defects have been classified in [617] as being able to create compensated, semi-insulating, ntype or p-type material depending on the defect formation energies and the position of the electronic levels of the AB and BA defects in the band gap (Fig. 7.24). An example for a p-type spinel oxide is ZnCo2 O4 [618].

7.5.7 High Doping For low doping concentrations, the impurity atoms can be considered to be decoupled. At low temperature, only hopping from one impurity to the next is possible due to thermal emission or tunneling and the semiconductor becomes an insulator.

202

7 Electronic Defect States

With increasing concentration, the distance between impurities decreases and their wavefunctions can overlap. Then, an impurity band develops (Fig. 7.25). A periodic arrangement of impurity atoms would result in well-defined band edges as found in the Kronig-Penney model. Since the impurity atoms are randomly distributed, the band edges exhibit tails. For high doping, the impurity band overlaps with the conduction band. In the case of compensation, the impurity band is not completely filled and contains (a new type of) holes. In this case, conduction can take place within the impurity band even at low temperature, making the semiconductor a metal. This metal–insulator transition has been discussed by Mott [619]. Examples for highly doped semiconductors are transparent conductive oxides (Sect. 20), the contact layer for an ohmic contact (Sect. 21.2.6) or the active layers in a tunneling diode (Sect. 21.5.9). The physics, properties and preparation of highly doped semiconductors are treated in detail in [620]. The formation of the impurity band leads to a reduction of the impurity ionization energy as known from (7.21). Typical results are shown in Fig. 7.26a for n-type Ge [594] and Fig. 7.26b for p-type ZnTe [621]. At the critical doping concentration of Nc = 1.5 × 1017 , the activation energy for the carrier concentration disappears. Similar effects have been observed for Si [622] and GaAs [623]. The freeze-out of the carrier concentration (see Fig. 7.9) disappears as shown in Fig. 7.27. Critical doping concentrations are listed in Table 7.6. The decrease of the ionization energy E b (donor or acceptor) follows the dependence [594, 622] E b = E 0b − α

1/3 Ni

= E 0b

1−

Ni Nc

1/3 ,

(7.52)

where Ni is the concentration of ionized dopants. A refined theory, considering screening, shift and tails of the conduction band and most importantly broadening of the donor level has been presented in [624]. The critical density can be estimated from the Mott criterion when the distance of the impurities becomes comparable to their Bohr radius (7.22) 2aD =

3 1/3 N . 2π c

(7.53)

The pre-factor 3/(2π ) stems from the random distribution of impurities and disappears for a periodic arrangement. The Mott criterion is (rewriting (7.53)) E

E

EC ED

EC

EV

EV

(a)

D(E)

E

EV

(b)

D(E)

(c)

D(E)

Fig. 7.25 Principle of the formation of a (donor) impurity band. a Small doping concentration and sharply defined impurity state at E D , b increasing doping and development of an impurity band that c widens further and eventually overlaps with the conduction band for high impurity concentration. The shaded areas indicate populated states at T = 0 K

7.5 Shallow Defects

203 15 b

ED

Ge:As

10 5

(a)

0 1012 1013 1014 1015 1016 1017 1018 -3 ND-NA (cm ) (b)

Fig. 7.26 a Donor ionization energy in n-type Ge for various doping concentrations. Dashed line is a guide to the eye. The arrow labeled E Db denotes the low-concentration limit (cf. Table 7.2). Experimental data from [594]. b Acceptor ionization energy for ZnTe:Li and ZnTe:P as a function of the third root of the ionized acceptor concentration. Data from [621]

1020 (iii)

-3

Fig. 7.27 Electron concentration versus inverse temperature for Si:P for three different doping concentrations ((i): 1.2 × 1017 cm−3 , (ii): 1.25 × 1018 cm−3 , (iii): 1.8 × 1019 cm−3 ). Experimental data from [622]

1019 1018

(ii)

1017 1016 1015 0

aD Nc1/3 ≈ 0.24 .

(i)

Si:P 2

4

6 8 10 1/T (1000/K)

12

14

(7.54)

For GaAs with aD = 10.3 nm, the criterion yields Nc = 1.2×1016 cm−3 , in agreement with experiment. The achievable maximum concentration of electrically active dopants is limited by the concentration dependence of the diffusion coefficient, Coulomb repulsion, autocompensation and the solubility limit [575]. In Table 7.7 the maximum carrier concentrations for GaAs with various dopants are listed. As an example we show the Ga-doping of epitaxial ZnO layers on sapphire in Fig. 7.28. Under slightly Zn-rich (O-polar) conditions the growth mode is two-dimensional and the carrier concentration increases linearly with the Ga concentration, n ≈ cGa , up to high values in the 1020 cm−3 range [630]. For O-rich (Zn-polar) conditions the growth mode changes to three-dimensional growth and the activation ratio of Ga donors becomes low [631]. Above a gallium content of 2%, the octahedral coordination of gallium and thus the partial segregation into a parasitic ZnGa2 O4 spinel phase is observed for [Ga] = 4% [632]. The doping of semiconductors beyond the solubility limit is termed ‘hyperdoping’. It involves non-equilibrium preparation methods [637, 638].

204

7 Electronic Defect States

Table 7.6 Critical doping concentration for various semiconductors (at room temperature) Material C:B Ge:As Si:P Si:B GaAs GaP:Si GaP:Zn GaN:Si GaN:Mg Al0.23 Ga0.77 N:Si ZnTe:Li ZnTe:P ZnO:Al

Type

Nc (cm−3 )

References

p n n p n n p n p n p p n

2 × 1020

[597] [594] [622] [622] [623] [625] [626] [627] [598] [628] [621] [621] [629]

1.5 × 1017 1.3 × 1018 6.2 × 1018 1.0 × 1016 6 × 1019 2 × 1019 2 × 1018 4 × 1020 3.5 × 1018 4 × 1018 6 × 1018 8 × 1018

Table 7.7 Maximum electrically active doping concentration for GaAs Material

Type

Nc (cm−3 )

References

GaAs:Te GaAs:Si GaAs:C GaAs:Be

n n p p

2.6 × 1019 1.8 × 1019 1.5 × 1021 2 × 1020

[633] [634] [635] [636]

Fig. 7.28 Electron concentration as a function of gallium concentration in MBE grown ZnO:Ga on sapphire for the two different polarities. Adapted from [630, 631]

7.6 Quasi-fermi Levels The carrier concentrations were given by (7.6) and (7.7). So far, we have only considered semiconductors in thermodynamic equilibrium for which np = n 2i . In a nonequilibrium situation, e.g. for external excitation or carrier injection in a diode, the electron and hole densities can each take arbitrary values, in principle. In particular, np will no longer be equal to n 2i and there is no Fermi level constant throughout the structure. In this case, however, quasi-Fermi levels Fn and Fp for electrons and holes, respectively, are defined via

7.6 Quasi-fermi Levels

205

Fn (r) − E C n(r) =NC F1/2 kT Fp (r) − E V . p(r) =NV F1/2 − kT

(7.55a) (7.55b)

A quasi-Fermi level is sometimes called imref5 and can also be denoted as E Fn or E Fp . We emphasize that the quasi-Fermi levels are only a means to describe the local carrier density in a logarithmical way. The quasi-Fermi levels can be obtained from the density via

n Fn =E C + kT ln NC p . Fp =E V − kT ln NV

(7.56a) (7.56b)

The quasi-Fermi levels do not imply that the carrier distribution is actually a Fermi distribution. This is generally no longer the case in thermodynamical nonequilibrium. However, in ‘well-behaved’ cases the carrier distribution in nonequilibrium can be approximated locally as a Fermi distribution using a local quasi-Fermi level and a local temperature, i.e. f e (r, E) ∼ =

exp

1 E−Fn (r) kT (r)

+1

.

(7.57)

Using the quasi-Fermi levels, np is given by n(r) p(r) =

n 2i

exp

Fn (r) − Fp (r) kT

.

(7.58)

We note that for an inhomogeneous semiconductor or a heterostructure (cf. Chap. 12), n i may also depend on the spatial position. In the case of thermodynamic equilibrium the difference of the quasiFermi levels is zero, i.e. Fn − Fp = 0 and Fn = Fp = E F .

7.7 Deep Levels For deep levels the short-range part of the potential determines the energy level. The long-range Coulomb part will only lead to a correction. The term ‘deep level’ implies that the level is within the band gap and far from the band edges. However, some deep levels (in the sense of the potential being determined by the ion core) have energy levels close to the band edges or even within a band. Details can be found in [267, 639–642]. The wavefunction is strongly localized. Thus, it cannot be composed of Bloch functions, as has been done for the shallow levels for the effective-mass impurity. The localization in r space leads to a delocalization in k space. Examples are Si:S, Si:Cu or InP:Fe, GaP:N, ZnTe:O. Deep levels can also be due to intrinsic defects such as vacancies or antisite defects. Due to the larger distance to the band edges, deep levels are not efficient at providing free electrons or holes. Quite the opposite, they rather capture free carriers and thus lead to a reduction of conductivity. 5 W. Shockley had asked E. Fermi for permission to use his name reversed. Fermi was not too enthusiastic but granted permission.

206

7 Electronic Defect States

Centers that can capture electrons and holes lead to nonradiative recombination of electrons through the deep level into the valence band (see also Chap. 10). This can be useful for the fabrication of semi-insulating layers with low carrier concentration and fast time response of, e.g., switches and photodetectors. While the electronic properties of deep levels can be readily characterized, the microscopic origin is not immediately apparent. Next to theoretical modeling of defects and correlation with experimental results, paramagnetic hyperfine interactions have proven useful to identify the microscopic nature of various defects [643].

7.7.1 Charge States The deep level can have different charge states depending on the occupancy with electrons. The energy position within the gap varies with the charge state due to the Coulomb interaction. Also, the lattice relaxation around the defect depends on the charge state and modifies the energy level. The localized charge qd at the defect is the integral over the change ρ of the charge density compared to the perfect crystal over a sufficiently large volume V∞ around the defect qd =

ρ(r) d3 r = V∞

ne . r

(7.59)

In semiconductors, the charge qd r is an integer multiple of the elementary charge. The defect is said to be in the nth charge state. Each charge state has a certain stable atomic configuration Rn . Each charge state has a ground state and excited states that can each have different stable atomic configurations. Now, we discuss how the concentration of the various charge states depends on the position of the Fermi level. The overall constraint of global charge neutrality determines the chemical potential of the electron, i.e. the Fermi level in Fermi–Dirac statistics. We use the approximation that the concentration of defects is so small that the mutual interaction of defects becomes negligible. As an example, we treat the possible reaction V 0 V + + e− , where V 0 denotes a neutral vacancy and V + is a positively charged vacancy, created by the ionization of an electron from the vacancy into the conduction band. The free energy G depends on the numbers n 0 of neutral and n + of positively charged vacancies. The minimum condition is met by dG =

∂G ∂G dn 0 + dn + = 0 . ∂n 0 ∂n +

(7.60)

The neutrality constraint is dn 0 + dn + = 0 and therefore the minimum condition reads ∂G ∂G = . ∂n 0 ∂n +

(7.61)

For noninteracting defects and using (4.9) we write n0 ∂G f 0 =G (V ) + kT ln ∂n 0 N0 ∂G ∂G(V + ) ∂G(e− ) n+ f = + = G V + + kT ln + μe− , ∂n + ∂n + ∂n + N+

(7.62a) (7.62b)

7.7 Deep Levels

(a)

207

(b)

Fig. 7.29 a Silicon cubic unit cell with an interstitial iron atom (red) at tetrahedral site. b EPR intensity (at T = 95 K from interstitial iron in neutral state, Fe0 with S = 1) versus Fermi level position for iron-doped silicon with varying Fermi level due to different amounts of shallow impurity levels from to Al, B and P as labeled. The shaded areas indicate the valence and conduction band. The dashed line at E t = E V + 0.375 eV indicates the trap level. The inset shows a typical EPR spectrum of Fe0 . Adapted from [649], inset adapted from [650]

where N0 = N Z 0 and N+ = N Z + are the number of available sites, given by the number N of atomic sites and including possible internal degeneracies Z 0 and Z + , respectively. Degeneracy factors of deep levels are not a simple subject [601] and , e.g., the degeneracy factors of Au donor and acceptor levels in Si are under discussion [644–646]. G f denotes the free enthalpy of formation of the respective defect, as in (4.3). We have written the free enthalpy of the separated pair V + and e− as the sum G(V + ) + G(e− ). μe− = ∂G(e− )/∂n + is (by definition) the chemical potential of the electron, i.e. the Fermi energy E F of Fermi–Dirac statistics.6 From (7.62a,b) we find for the ratio of the concentrations of defects c0 = n 0 /N and c+ = n + /N G fV + − G fV 0 + E F Z+ E t (V 0 ) − E F Z+ c0 = exp − exp = , c+ Z0 kT Z0 kT

(7.63)

where the trap level energy (for the particular charge transition), E t (V 0 ) = G fV 0 − G fV + , is the free enthalpy of ionization of V 0 . We note that c0 can be obtained from (4.9) and E F is determined by the charge-neutrality condition. As example experimental data on the charge transition Fe0 Fe+ + e− of interstitial iron (in tetrahedral position, Fig. 7.29a, cmp. Fig. 3.18) in silicon is shown. The concentration of Fe0 is tracked via the EPR signal from the neutral S = 1 state7 with g-factor g = 2.07 [647]. For n-type samples the iron is in neutral state and the maximum EPR signal is found. For strongly p-type samples, the Fermi energy is below the trap level and all iron is in Fe+ state, yielding no EPR signal at the given gfactor. From the investigation of various silicon samples with different doping levels and consequently

6 The chemical potential in a one-component system is μ = ∂G/∂n = G/n. In a multicomponent system it is, for the ith component, μi = ∂G/∂n i = G/n i . 7 The electron configuration is 3d8 with two paramagnetic electrons. Under uniaxial stress along [100] the EPR line splits into a doublet [647]. Further details can be found in [648].

208

7 Electronic Defect States

Table 7.8 Binding energies (to conduction band) of double donor chalcogenide impurities in Si and Ge. All energies in meV, data from [651, 652] Host

State

S

Se

Te

Si

D0 D+ D0 D+

318 612 280 590

307 589 268 512

199 411 93 330

Ge

different position of the Fermi level, the trap (deep donor) energy is found to be E V + 0.375 eV as indicated in Fig. 7.29b.

7.7.2 Double Donors An impurity that has two extra electrons available after bonding in the matrix may give rise to a double donor. Typical examples are substitutional chalcogenide atoms (S, Se or Te) in silicon [651] and germanium [652], interstitial impurities such as Mgi in Si [653], or group-V atoms on a group-III site in a III–V compound (antisite defect), such as PGa in GaP [654] or AsGa in GaAs [655]. The double donor is electronically similar to a helium atom. Due to the repulsive Coulomb interaction of the two electrons on the neutral double donor, the (single) ionization energy E 1 (also often labeled E(0, 1) or E(0, +)) of D0 is smaller than that of D+ (E 2 , also labeled E(1, 2) or E(+, ++)). For He and He+ the ratio of ionization energies is 0.45; for chalcogenides in Si and Ge similar ratios have mostly been found (Table 7.8). The carrier statistics and the degeneracy factors for a double donor have been discussed in [585, 656]. Typically, the degeneracy factor for the ionization of the double donor D0 → D+ is gˆ D = g2 /g1 = 1/2 and for the ionization D+ → D++ is gˆ D = g1 /g0 = 2/1 = 2. For the probabilities to find a neutral, single and double ionized donor we find following the treatment in [656] d0 =

ND0 = ND exp

d+ =

ND+ = ND exp

d ++ =

ND++ = ND exp

E 1 +E 2 kT

exp 2kTEF + exp 2kTEF + 2 exp

E 1 +E 2 kT 2 EF + exp kT + +E F 2 exp E1kT E 1 +E 2 + exp 2kTEF + 2 kT

E 1 +E F kT

exp

E 1 +E 2 kT

2 exp exp

E 1 +E F kT

E 1 +E F kT

(7.64a) (7.64b) (7.64c)

The probabilities are depicted in Fig. 7.30a. The maximum of d + is at the energy (E 1 + E 2 )/2. Its value is 1 E1 + E2 (7.65) 1 −E2 = d+ 2 1 + exp − E2kT and reaches a value close to one for (E 1 − E 2 )/kT 1. In Fig. 7.30b the number of electrons per donor n˜ = (ND+ + 2 ND++ )/ND is shown as a function of the Fermi level; at (E 1 + E 2 )/2, exactly n˜ = 1. In Fig.7.31 the temperature dependent electron concentration in Si:Te is depicted. Up to 570 K the single ionization is visible (other shallow impurities present in the sample in lower concentrations < 1014 cm−3

7.7 Deep Levels

209

(a)

(b)

Fig. 7.30 a Population of states of a double donor (neutral: black, single ionized: red, double ionized: blue) according to (7.64a–c) as a function of the Fermi level. The ionization energies have been chosen as E 1 = −0.2 eV and E 2 = −0.4 eV and are indicated by dashed lines (kT = 25 meV); these energies are similar to Si:Te (cmp. Table 7.8). The conduction band edge is taken as zero energy. b depicts the according number of electrons n˜ ionized from the donor

10

18

1000 500

300

200

17

2 10

Si:Te

900

700 600

500

400

(b)

Si:Te

-3

(a)

1017

10

17

8 1016 16

6 10

1016

4 1016 10

15

0

1

2 3 4 1000/T (1000/K)

5

6

1.0

1.5 2.0 2.5 1000/T (1000/K)

3.0

Fig. 7.31 Temperature dependent electron concentration (from Hall data) for Si:Te. a Experimental data and fit with double donor model using NTe = 5 × 1016 cm−3 , E 1 = 200 meV and E 2 = 440 meV (solid line). Single donor models would fail (NTe = 5 × 1016 cm−3 and NTe = 2 × 1017 cm−3 , dashed lines). b Second ionization step in more detail with fits using different values for E 2 ; the solid line is for E 2 = 440 meV, the other dashed lines for E 2 = 420 and 460 meV. Adapted from [657]

play no role). From the fit E 1 = 200 ± 2.7 meV is determined [657]. Single donor models would fail. The second ionization step is somewhat masked by the onset of intrinsic conduction. According to (7.15), the slope of n i is E g /2 ≈ 500 meV which is similar to E 2 ≈ 440 meV.

7.7.3 Double Acceptors In analogy to double donor defects, double acceptors can introduce up to two holes into the valence band. A typical example is Zn in silicon [658], exhibiting its ‘normal’ acceptor level (Zn0 /Zn− ) at E V + 0.31 eV. In moderately n-doped silicon another level (Zn− /Zn2− ) is observed at E C − 0.55 eV,

210

7 Electronic Defect States

Fig. 7.32 Inverse (absolute) Hall coefficient −1 , (cmp. Sect. 15.2.1) RH i.e. charge concentration, for three Ge:Zn samples with different degree of compensation with Sb donors as labeled. The dash-dotted lines indicate typical slopes. The dashed lines sketch the Zn0 → Zn− and the Zn− → Zn−− processes. Adapted from [659]

when the n-doping is sufficient to partially compensate the Zn and supply one electron for each Zn atom but not two (2NZn > ND > NZn ). A similar situation has been observed for Zn in germanium, exhibiting the levels E V + 0.03 eV and E V + 0.09 eV [659]. In Fig. 7.32 three different Ge:Zn samples are compared. If the additional Sb donor concentration (ND ≈ 3.4 × 1016 cm−3 ) is larger than 2NZn (NZn ≈ 1.2 × 1016 cm−3 ), the sample is n-type (upper curve). The slope is similar to the Ge:Sb donor binding energy (Table 7.2). If compensation with donors is weak (NZn > ND , middle curve) first the shallow donor level with 0.03 eV activation energy is activated and subsequently the deeper one with 0.09 eV activation energy, creating p-conduction with a saturated hole density of p ≈ 2NA − ND > NZn (negative Hall coefficient). The two individual activation processes are sketched as dashed lines in Fig. 7.32. If the Sb concentration is larger than NZn but smaller than 2NZn , the shallow acceptor level is filled with electrons, leaving still the only partially filled deeper acceptor level available for ionization (lower curve). In this case the sample is still p-type, but the saturation hole density is p ≈ 2NA − ND < NZn . The degeneracy factors for Zn in Si and Ge have been discussed in [601].

7.7.4 Jahn–Teller Effect The lattice relaxation can reduce the symmetry of the defect. Many defects, such as a vacancy, a tetrahedral interstitial or an impurity, occupy initially tetrahedral sites in the zincblende structure. The lattice relaxation reduces the symmetry, e.g. to tetragonal or trigonal, and therefore causes initially degenerate levels to split. Such splitting is called the static Jahn–Teller effect [639, 660]. The energy change in terms of the atomic displacement Q can be denoted (using perturbation theory for the simplest, nondegenerate case) as −I Q (I > 0). Including the elastic contribution with a force constant C, the energy of a configuration Q is 1 (7.66) E = −I Q + C Q 2 . 2 The stable configuration Q min , for which the energy is minimal (E min ), is therefore given by

7.7 Deep Levels

211

Fig. 7.33 Charge states of the vacancy in silicon. Left: level scheme without lattice relaxation, right: level scheme including the Jahn–Teller effect. For a Fermi level below (above) E(0, 2) the charge state V ++ (V 0 ) is dominant

E0(0,1) E0(1,2)

V0 V V

Q min =

I C

E min = −

E(1,2) V0 E(0,2) E(0,1) V

(7.67a) I2 . 2C

(7.67b)

Several equivalent lattice relaxations may exist, e.g. a 3-fold minimum for remaining C3v symmetry. The energy barrier between them has a finite height. Therefore, e.g. at sufficient temperature, the defect can switch between different configurations and eventually again becomes isotropic (dynamic Jahn– Teller effect). The experimental observation depends on the relation between the characteristic time of the experiment and the reorientation time constant of the defect.

7.7.5 Negative-U Center We explain the principle of a so-called negative-U center [661] for the Si vacancy [662] (cf. Fig. 4.2). It was first proposed by Anderson to explain the properties of amorphous chalcogenide glasses [663]. Many defects in semiconductors exhibit negative-U behavior, e.g. also the boron interstitial in Si [662, 664]. Coulomb energy and the Jahn–Teller effect compete for the position of the occupancy level for different charge states. U refers to the additional energy upon charging of the defect with an additional electron. The Coulomb repulsion of electrons leads to an increase of the energy, i.e. positive U , which has been calculated to be 0.25 eV for the Si vacancy [665] for all charge states. The occupation level (cf. Sect. 4.2.2) E 0 (1, 2) (the index 0 indicates effects only due to many-electron Coulomb interaction), separating the domination of V ++ and V + (Fig. 7.33) is 0.32 eV above the valance-band edge. Therefore, the occupation level E 0 (0, 1) is expected to lie at about 0.57 eV about E V . The Jahn–Teller effect may lead to a splitting of the otherwise 4-fold degenerate states of the vacancy. A detailed experimental study using hyperfine interactions can be found in [666]. The schematic level diagram for the Jahn–Teller splitting is shown in Fig. 7.34. The V ++ state ( A1 is always populated

T2

A1 V

V

0

V

V

Fig. 7.34 Jahn–Teller splitting for different charge states of the vacancy. A1 and T2 refer to irreducible representations of the Td point symmetry group. A1 is nondegenerate and therefore does not exhibit a Jahn–Teller effect. T2 is triply degenerate. The arrows represent electrons and their spin orientation

212

7 Electronic Defect States

with two electrons) is resonant with the valence band. The T2 state lies in the band gap. When the Jahn–Teller effect (now on the T2 state) is included, the energies of the different charge states depend on the configuration coordinate (a mostly tetragonal distortion in the case of the Si vacancy). 1 E V 0 = E(0, Q) =E(0, Q = 0) − 2I Q + C Q 2 2 1 E V + = E(1, Q) =E(1, Q = 0) − I Q + C Q 2 2 1 2 E V ++ = E(2, Q) =E(2, Q = 0) + C Q . 2

(7.68a) (7.68b) (7.68c)

For the n = 2 state the T2 gap state is empty and thus no degeneracy and Jahn–Teller term arises. For n = 1 there is a linear Jahn–Teller term. The occupation with two electrons (V 0 ) causes an approximately twice as large Jahn–Teller splitting for the n = 0 state. The force constant is assumed to be independent of the charge state. The energies for the minimum configurations Q nmin are therefore

E(0, Q 0min ) =E(0, Q = 0) − 4 E(1, Q 1min ) =E(1, Q = 0) −

I2 2C

I2 2C

E(2, Q 2min ) =E(2, Q = 0) .

(7.69a) (7.69b) (7.69c)

The Jahn–Teller energy E JT = I 2 /2C lowers the position of the occupancy levels E 0 calculated with Coulomb terms only. The occupancy levels including the Jahn–Teller contribution are therefore given as E(1, 2) = E 0 (1, 2) − E JT E(0, 1) = E 0 (0, 1) − 3 E JT .

(7.70a) (7.70b)

For the vacancy in silicon the Jahn–Teller energy E JT is about 0.19 eV. Thus the E(1, 2) level is lowered from 0.32 eV to 0.13 eV. The E(0,1) occupancy level, however, is reduced from 0.57 eV to 0.05 eV [662, 667] (see Fig. 7.33). The occupancy level E(0, 2) is in the middle between E(0, 1) and E(1, 2) (E(0, 2) = (E(0, 1)+ E(1, 2))/2) and indicated in Fig. 7.35a. At this energy, c(V 0 ) = c(V ++ ) 1 −E 2 ) since E(0, 1) < E(1, 2) (cmp. (7.65)). and the value of c(V + ) is small (≈ exp E2kT The relative concentrations of the three charge states are determined by (7.63) (degeneracy and entropy terms have been neglected) E(1, 2) − E F c(V ++ ) = exp c(V + ) kT + c(V ) E(0, 1) − E F = exp . c(V 0 ) kT

(7.71a) (7.71b)

They are depicted in Fig. 7.35a in a plot related to Fig. 7.30a. Therefore, V ++ dominates if E F < E(0, 1) and V 0 dominates for E F > E(1, 2). In the intermediate range E(0, 1) < E F < E(1, 2) we know from (7.71a, b) that V + is dominated by V 0 and V ++ . However, at this point it is not clear whether V ++ or V 0 dominates overall. The ratio of the concentrations of V ++ and V 0 is given by

7.7 Deep Levels

213

(b)

(a)

Fig. 7.35 a Population of states of a negative-U defect (neutral: black, single ionized: red, double ionized: blue) according to (7.64a–c) as a function of the Fermi level. The ionization energies have been chosen as E 1 = −0.4 eV and E 2 = −0.2 eV (cmp. Fig. 7.30) and are indicated by dashed lines (kT = 25 meV). The occupancy level E(0, 2) is indicated with a dash-dotted line. The conduction band edge is taken as zero energy. b depicts the according number of electrons ionized from the defect

c(V ++ ) = exp c(V 0 )

E(1, 2) + E(0, 1) − 2E F kT

= e2 exp

E(0, 2) − E F kT

.

(7.72)

The occupancy level E(0, 2) is thus again given as E(0, 2) =

E(0, 1) + E(1, 2) , 2

(7.73)

and is shown in Fig. 7.33. V ++ dominates if E F < E(0, 2) and V 0 dominates for E F > E(0, 2). V + is, for no position of the Fermi level, the dominating charge state of the Si vacancy. We note that for n-doped Si the V − and V −− can also be populated. The population of the V 0 state with an extra electron introduces another Jahn–Teller splitting (Fig. 7.34) that has trigonal symmetry. Generally, the Jahn–Teller effect can make the addition of an electron cause an effectively negative charging energy; in this case the center is termed a negative-U center. We note that the single vacancy in germanium is not a negative-U center due to smaller Jahn–Teller distortion and smaller electron-lattice coupling [668].

7.7.6 DX Center The DX center is a deep level that was first investigated for n-doped (e.g. Si-doped) Alx Ga1−x As. It dominates the transport properties of the alloy for x > 0.22. For smaller Al concentrations and GaAs the DX level lies in the conduction band. DX-type deep levels have also been found for other alloys and dopants, e.g. GaAsP:S. It is experimentally found that the capture process of electrons into the DX center is thermally activated. The capture energy E c depends on the AlAs mole fraction (Fig. 7.36). The (average) barrier for electron capture has a minimum of 0.21 eV for x ≈ 0.35, near the crossover point between direct and indirect band gap (cf. Fig. 6.24). For lower Al concentrations, the capture barrier increases to 0.4 eV for x = 0.27; for x > 0.35 the capture barrier increases to about 0.3 eV for x around 0.7 [669]. The barrier for thermally releasing carriers from the DX center has been determined to be about 0.43 eV, independent of the Al mole fraction [669].

214

7 Electronic Defect States

Carriers can be removed from the DX center by optical absorption of photons with energy larger than about 1.2 eV. If carriers are removed by optical excitation at low temperatures the (re-)capture is so slow (σ < 10−30 cm2 ) that the carriers remain in the conduction band and cause persistent photoconductivity (PPC). The PPC is only reduced upon increasing the sample temperature. The concentration of the DX center is about the same as the net doping concentration. The properties of the DX center are reviewed in [670, 671]. So far, no definite microscopic model of the DX center has been agreed on. Lang [672] proposed that the DX center involves a donor and an unknown defect (probably a vacancy). It probably involves large lattice relaxation as in the configuration coordinates model of Fig. 7.37 where the donor binding energy E Db with respect to the conduction-band minimum, the barrier for electron capture E c , the barrier for electron emission E e and the optical ionization energy E o are labeled. The donor binding energy is measured with Hall effect (cf. Sect. 15.2.1) at temperatures sufficient to overcome the capture and emission barriers, the emission barrier is measured with deep level transient spectroscopy (DLTS). The capture barrier manifests itself in PPC experiments. We note that the DX center is related to the L-conduction band. For small Al mole fraction, the DX level is degenerate with the -related conduction band (see Fig. 7.37b). Theoretical models and experimental evidence hint at a vacancy-interstitial model for the Si-DX center [673]. The donor (Si) is displaced along the 111 direction from the Ga substitution site. The displacement is predicted to be 0.117 nm and the distorted geometry can be viewed as a Ga vacancy and a Si interstitial. The charge state of the (filled) DX center is proposed to be a two-electron negative-U state.

7.7.7 EL2 Defect The EL2 defect is a deep donor in GaAs. It is not related to impurities but occurs for intrinsic material, in particular grown under As-rich conditions. It has physical properties similar to the DX center. The bleaching of absorption due to EL2, i.e. the optical removal of electrons from the defect at low temperatures, is shown in Fig. 7.38. The microscopic model [674] describes the EL2 defect as an arsenic antisite defect, i.e. an arsenic atom on a Ga site, AsGa . In the charged state the arsenic atom is displaced from the lattice position and a complex of a Ga vacancy (symmetry T3d ) and an interstitial As (symmetry C3v ) with 0.14 nm displacement along 111 forms (VGa -Asi ). The charged state is filled with two electrons.

Fig. 7.36 Energy barrier for electron capture E c at the Si-DX center in Alx Ga1−x As for various compositions. Experimental data from [669]

0.5

AlxGa1-xAs:Si

0.4 0.3 0.2 0.1

0.3

0.4

0.5

0.6

0.7

7.7 Deep Levels

215

E

E

Eopt EC EDX

Ec EbD

q0

(a)

EL EDX EC

Ee

qt

q

L

DX

Ec

Ee

q0

(b)

qt

q

Fig. 7.37 a Schematic configuration coordinate diagram for the DX level with large lattice relaxation. q0 is the configuration of the empty defect, qt is the configuration of the filled defect. The donor binding energy E Db , the barrier for electron capture E c , the barrier for electron emission E e and the optical ionization energy E o are labeled. E C denotes the conduction-band edge. We note that in (Al,Ga)As the DX level is associated with the L conduction band (see Fig. 6.24). b Schematic configuration coordinate diagram for the DX level in Al0.14 Ga0.86 As with the DX level being degenerate with the (-related) conduction band

4 -1

GaAs 3 2 1 0

0.8

1.0

1.2

1.4

Fig. 7.38 Absorption spectrum of GaAs at low temperatures (T = 10 K) when cooled in the dark (solid line). The dashed (dash-dotted) line is the absorption after illuminating the sample for 1 min (10 min) with white light, leading to quenching of the EL2-related absorption. Adapted from [675]

7.7.8 Semi-insulating Semiconductors Semiconductors with high resistivity (107 –109 cm) are called semi-insulating (‘s.i.’ or ‘si’). Semiinsulating substrates are needed for high-speed devices. The high resistivity should stem from a small free-carrier density at finite temperature and not from a small mobility due to poor crystal quality. For sufficiently wide band gap, the intrinsic carrier concentration is small and such pure material is semi-insulating, e.g. GaAs with n i = 1.47 × 106 cm−3 and 5.05 × 108 cm [676]. Since shallow impurities are hard to avoid, another route is used technologically. Impurities that form deep levels are incorporated in the semiconductor in order to compensate free carriers. For example, a deep acceptor compensates all electrons if NA > ND . Since the acceptor is deep (E Ab kT ), it does not release holes for reasonable temperatures. Examples of suitable impurities for compensation of electrons are Si:Au [677], GaAs:Cr [678] and InP:Fe [679]. A deep donor, e.g. InP:Cr [680], is necessary to compensate p-type conductivity. Figure 7.39a shows the terms of Fe in InP [681, 682]. An overview of transition metals in III–V semiconductors can be found in [683]. The electron configuration of neutral Fe atoms is 3d6 4s2 (cf.

216

7 Electronic Defect States 1.34 T2

InP:Fe

InP:Sn

-3

EC 1.14

5

InP:Sn,Fe

1017

0.78

5

E

InP:Sn

n

0.25

(a)

0

3+

Fe

Fe

2+

1016 0

EV

0.2

0.4

0.6

0.8

1. 0

(b)

Fig. 7.39 a Schematic band diagram of InP with levels of Fe impurities in the 3+ and 2+ charge states at low temperature. All energies are given in eV. The arrow denotes capture of an electron (from the conduction band or a shallow donor) on the deep acceptor. Compare this figure also with Figs. 9.36 and 10.25. b Depth profile of electron concentration in an InP:Sn/InP:Sn,Fe/InP:Sn structure. The change n ≈ 4.5 × 1016 cm−3 of electron concentration is due to the compensation by Fe and corresponds to the chemical iron concentration determined by SIMS, [Fe] = 4.9 × 1019 cm−3 . Part b adapted from [688]

Table 17.2). The Fe is incorporated on the In site and thus has a Fe3+ state as a neutral acceptor (A0 ). The Fe3+ state has the electron configuration 3d5 . The arrow in Fig. 7.39a represents the capture of an electron from the conduction band or from a shallow donor. The charge state of the Fe becomes Fe2+ (charged acceptor, A− ) with the electron configuration 3d6 . The cubic crystal field (Td symmetry) splits this 5 D Fe state8 into two terms [684] that exhibit further fine structure [682]. The large thermal activation energy of 0.64 eV found in the Hall effect on semi-insulating InP:Fe [679] corresponds to the energy separation of the 5 E level and the conduction band. The maximum electron concentration that can be compensated in this way is limited by the solubility of Fe in InP [685], about 1 × 1017 cm3 . Higher Fe incorporation leads to the formation of Fe (or FeP) precipitates and degrades the crystal quality. Only a fraction of the incorporated Fe may then be electrically active and contribute to the compensation. The maximum electrically active Fe concentration is found to be 5–6×1016 cm−3 [686]. The compensation can be directly visualized via the depth profile of the electron concentration in a n-si-n structure (Fig. 7.39b). The poor thermal stability of Fe, i.e. high diffusion coefficient, has evoked proposals for more stable dopants such as InP:Ru [687].

7.7.9 Isoelectronic Impurities Isoelectronic impurities, generally represent a deep level with a short range potential. The isoelectronic trap introduces a bound state for an electron or a hole. Once a carrier has been captured, the defect becomes charged. The other carrier type is then easily trapped, forming a bound exciton (Sect. 10.3.2). The theory of isoelectronic impurities is outlined in [689]. A detailed theoretical treatment of N in GaAs and GaP is given in [544]. In GaP:N, an electron is spatially localized on the N impurity. Most of the wave function is at the X-point. The nitrogen-bound electron level in GaP (A1 symmetry) is close to the conduction band edge and within the band gap. Important for the energy position is the lattice relaxation, leading to an inward relaxation of the surrounding Ga atoms (Fig. 7.41). Due to the spatial localization of the wave function it is delocalized in k-space (Fig. 7.40a) and obtains a sizeable component at the -point, facilitating zero-phonon absorption from the valence band. This effect is present only when the lattice relaxation around the impurity is considered; without relaxation the -component is zero, with relaxation about 1% [544]. The -component of the wave-function is larger for localization at an isoelectronic impurity 8 The

notation is 2S+1 J (multiplicity), with S being the total spin and J being the total angular momentum.

7.7 Deep Levels Fig. 7.40 a Model calculation of the wave-vector dependence of the probability density of an electron bound to a 10 meV deep isoelectronic trap (N) and to a 100 meV deep shallow donor (S) in GaP. Adapted from [690]. b Wavefunction (isosurface at 20% of maximum) of isolated nitrogen (N) and neighboring N–N pair (NN1 ) in GaP. Adapted from [544]

217

(a)

(b)

Fig. 7.41 Energy levels of nitrogen impurity states in GaP (left) and GaAs (right). The energy scale is relative to the bulk GaP valence band maximum, the conduction band minima (CBM) are thus shown relative to the vacuum level. The conduction band is shown in grey. For both materials, (a) denotes the isolated N impurity level calculated without lattice relaxation (dashed line), and (b) with lattice relaxation. (c) denotes the position of N–N pair levels, m denoting the neighbor. (d) shows selected experimental data. NN1 denotes the direct neighbor NN-pair. The other NNn follow the usual nomenclature as in [694]. Data taken from [544]

than at a shallow donor such as sulfur [690]. This way a large oscillator strength for optical transitions occurs (Sects. 9.7.9, 10.3.2). The wavefunction of an isolated single N impurity and a neighboring N–N pair (NN1 ) in GaP are shown in Fig. 7.40b. Isolated nitrogen impurities in (unstrained) GaAs introduce states only within the conduction band (Fig. 7.41). The reason is that the GaAs conduction band edge is further from the vacuum level than that of GaP (see Fig. 12.21). Only the NN1 and NN4 pair levels are theoretically expected to be within the GaAs band gap. The index denotes the nth neighbor position. The NN1 level has been experimentally observed [691, 692]. The isolated nitrogen impurity level is forced into the GaAs band gap upon hydrostatic pressure [692, 693] (Fig. 7.42). Further levels deeper within the band gap are due to clusters containing more than two nitrogen atoms.

7.7.10 Surface States The investigation of (semiconductor) surfaces is a large field with sophisticated methods that allow real-space imaging with atomic resolution by scanning probe microscopy and highly depth resolved electronic studies. The surface represents first of all a break in the periodic crystal potential and thus a defect of the bulk crystal. The unsatisfied bonds partly rearrange, e.g. by building dimers, forming a surface reconstruction or remain as dangling bonds. The surface exhibits a surface density of states.

218

7 Electronic Defect States

Fig. 7.42 Pressure dependence of the energy of excitons bound to isolated nitrogen impurities in GaAs (circles), measured from the top of the GaAs valence band. The dashed lines are the pressure dependent GaAs bulk band gaps (cmp. Fig. 6.49). The solid (dash-dotted) line is a theoretical model for the nitrogen-bound exciton (electron) level. Adapted from [693] (b)

4.26 (d)

4.24

4.22

(a) 2 (c) 1 0 0

z=1.56nm 100

200

300

400

Fig. 7.43 Image of a topography (z = 2.8 nm) and b work function (φ = 4.21–4.26 eV) of a surface step along [111] on a n-GaP(110) surface cleaved in UHV. Adapted from [696]. c and d show the corresponding linescans. Adapted from [696]

Such states can lie in the band gap and capture electrons, leading to recombination and a depletion layer. For a brief introduction on semiconductor surface physics see Chap. 11; for more details we refer to [695]. As an example of the formation of electronic states at surface defects we show in Fig. 7.43 the comparison of topography and work function (measured by Kelvin probe force microscopy [696]) at a surface step on a GaP(110) surface that has been prepared by cleaving in-situ in ultrahigh vacuum (UHV). The depletion-type band bending of the surface is about 0.4 eV. The further increase of the position of the vacuum level at the step edge shows the presence of trap states in the band gap causing the conduction band to bend upwards (cf. Sect. 21.2.1). Modeling of the effect shows that the charge density at the surface is 6 × 1011 cm−2 and at the step edge 1.2 × 106 cm−1 .

7.8 The Charge Neutrality Level

219

7.8 The Charge Neutrality Level The charge neutrality level (CNL) of a semiconductor is defined as the maximum occupied surface state energy at a neutral surface. In this case it is identical with the Fermi level (which renders the surface without a net charge). The CNL is also termed Fermi level stabilization energy [700] or ‘branch point energy’ [697] and marks the energy at which the character of intrinsic defects changes from predominantly donor-like (below CNL) to predominantly acceptor-like (above CNL). If Fermi level in the bulk and CNL deviate, surface charges appear; when the Fermi level is above (below) the charge neutrality level, the surface is negatively (positively) charged. Whether this means a depletion or accumulation layer depends on the conductivity type of the semiconductor. Band bending and space charge regions are discussed in more detail further below (Sect. 12.3.4, Sect. 21.2.1). The position of the CNL can be calculated from the Brillouin zone average of the conduction-to-valence band difference [698, 699]. Experimentally, the Fermi level will be established at the CNL when a lot of deep defects are introduced, e.g. by irradiation. For many semiconductors, the CNL is close to the middle of the band gap (Si, GaAs). Notable exceptions are e.g. InAs or In2 O3 with a CNL within the conduction band leading to n-type surface conduction.

7.9 Hydrogen in Semiconductors The role of hydrogen in semiconductors was first recognized in studies of ZnO [701]. It is now clear that hydrogen plays an important role in the passivation of defects. As a ‘small’ atom, it can attach easily to dangling bonds and form an electron-pair bond. Thus, surfaces, grain boundaries, dislocations and shallow (donor and acceptor) and deep impurity levels become passivated. A good overview and many details of the physics and technological use of hydrogen in semiconductors can be found in [702, 703]. The hydrogen must be typically introduced as atomic species into semiconductors, e.g. from a plasma in the vicinity of the surface or by ion irradiation. With regard to silicon it is important to note that the Si–H bond is stronger than the Si–Si bond. Thus a silicon surface under atomic hydrogen exhibits Si–H termination rather than Si–Si dimers [704]. Due to the stronger bond, the hydrogenation leads to an increase of the silicon band gap, which can be used for surface passivation [705], leading to reduced reverse diode current. The hydrogen concentration in amorphous Si (a-Si) can be as high as 50% [706]. Electronic grade a-Si contains typically 10–30 atomic% hydrogen and is thus rather a silicon–hydrogen alloy. Hydrogen in crystalline silicon occupies the bond-center interstitial position (see Fig. 3.18b) as shown in Fig. 7.44a. The complexes formed by hydrogen with shallow acceptors and donors have been studied in detail. It is now generally accepted that for acceptors (e.g. boron) in silicon the hydrogen is located close to the bond-center position of the Si–B pair (BM, bond minimum) as sketched in Fig. 7.45a. The boron atom forms an electron-pair bond with three silicon atoms of the tetrahedra, the fourth silicon bonds to the hydrogen atom. The complex therefore no longer acts as an acceptor. The silicon atoms and the acceptor relax their positions. The adiabatic potential energy surface of hydrogen in Si:B is shown in Fig. 7.44b. The hydrogen can sit on four equivalent sites (BM) along the 111 directions of the initial B–Si4 tetrahedron. This reduces the symmetry, e.g. of H–B vibrations [708]. The energetic barrier for the hydrogen orientation has been determined to be 0.2 eV theoretically [707] for a hydrogen motion along the path BM–C–BM in Fig. 7.44b. Stress (along [100] and [112]) reduces the symmetry and leads to splitting of the local vibrational modes, now showing axial symmetry [709]. However, this preferential orientation disappears with an activation energy of 0.19 eV, close to the theoretical value.

220

7 Electronic Defect States Si/B

Si 0.5

Td

Td 0.0 -0.5 -1.0 AB

-1.5 -2.0 -0.5

+

H

0

BM -0.25

0.0

0.25

(b)

(a)

+ Fig. 7.44 a Energy for positions u of the hydrogen atom along the 111 direction for √ H in pure Si (Si atom at u = −0.25) and neutral hydrogen (B atom at u = −0.25). u is measured in units of 3a0 . For all positions of the hydrogen atom the positions of the other atoms have been relaxed in the calculation. Data from [707]. b Adiabatic potential energy in the (110) plane for hydrogen in Si:B. ‘BM’ denotes the bond minimum site (high valence electron density), C and C’ are equivalent for pure Si. Reprinted with permission from [707], ©1989 APS

Fig. 7.45 Schematic model for hydrogen in silicon forming a complex with a a shallow acceptor (boron, empty orbital) and b a shallow donor (phosphorus, double-filled orbital)

Hydrogen has experimentally been found to also passivate shallow donors. The microscopic configuration is sketched in Fig. 7.45b. The hydrogen atom sits on the Si–AB (antibonding) position and forms an electron-pair bond with the silicon atom. The donor, e.g. phosphorus, is left with a double-filled p-orbital (lone pair) whose level is in the valence band and thus no longer contributes to conductivity.

[001]

(a)

[110]

[110]

(b)

Fig. 7.46 a Structure of the V–O complex (A center) in silicon. The black sphere represents the oxygen atom. Reprinted with permission from [710], ©2004 APS. b Calculated ground-state structure for the V–O–H2 center in silicon. Oxygen is over the C2 axis, and the two white spheres represent hydrogen. Reprinted with permission from [711], ©2000 APS

7.9 Hydrogen in Semiconductors

221

Molecular hydrogen can passivate the so-called A center in Si, an oxygen–vacancy complex [711]. The atomistic configuration of the V–O–H2 complex is shown in Fig. 7.46. The deep double donor S in Si with a level at 0.3 eV below the conduction-band edge can also be passivated by two hydrogen atoms [712].

Chapter 8

Transport

Um über den Temperaturverlauf des Widerstandes Rechenschaft geben zu können, müssen andere Abweichungen von der strengen Periodizität entscheidend sein, nämlich diejenigen, welche von den thermischen Eigenschwingungen des Kristalls herrühren. In order to be able to account for the temperature dependence of the resistivity, other deviations from the strict periodicity must be decisive, namely those which result from the thermal vibrations of the crystal. F. Bloch, 1928 [61]

Abstract The physics of transport in semiconductors is treated foremost for charge transport. Band transport and scattering, mobility, low field and high field effects as well as polarons and hopping transport are covered. A short section mentions ionic transport before heat conduction and coupled heat and charge transport including thermopower and Peltier effect are discussed.

8.1 Introduction Charge and heat energy can be transported through the semiconductor in the presence of appropriate (generalized) forces. Such a force can be an electric field or a temperature gradient. Both transport phenomena are coupled since electrons transport energy and charge simultaneously through the crystal. First, we will treat the charge transport as a consequence of a gradient in the Fermi level, then the heat transport upon a temperature gradient and finally the coupled system, i.e. the Peltier and Seebeck effects. Detailed treatments of carrier transport can be found in [713, 714]. Practically all important semiconductor devices are based on the transport of charge, such as diode, transistor, photodetector, solar cell and laser. Carriers move in the semiconductor driven by a gradient in the Fermi energy. We distinguish • drift, as a consequence of an electric field E, • diffusion, as a consequence of a concentration gradient ∇n or ∇ p. In inhomogeneous semiconductors for which the position of the band edges is a function of position, another force occurs. This will not be treated here, since later (cf. Chap. 12) it will be included as an additional, internal electric field. © Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_8

223

224

8 Transport

In Sects. 8.2–8.5 we treat band conductivity, i.e. the transport of charge carriers in extended states, the conduction and valence bands characterized by an effective mass. Conductivity is then determined by the carrier concentration (free electrons and holes) and scattering mechanisms (mobility). In disordered semiconductors such as amorphous material, the charge transport due to hopping between localized states close to the Fermi level dominates the conductivity which is discussed in Sect. 8.8. Many semiconductor properties, such as the carrier concentration and the band gap, depend on the temperature. Thus, device properties will also depend on temperature. During operation of a device typically heat is generated, e.g. by Joule heating due to finite resistivity. This heat leads to an increase of the device temperature that subsequently alters the device performance, mostly for the worse. Ultimately, the device can be destroyed. Thus cooling of the device, in particular of the active area of the device, is essential. Mostly the thermal management of device heating limits the achievable performance (and lifetime) of the device. In high-power devices quite high energy densities can occur, e.g. the facet of a high-power semiconductor laser has to withstand an energy density beyond 10 MW cm−2 .

8.2 Conductivity Under the influence of an electric field the electrons accelerate according to (cf. (6.36)) F = m∗

dk dv = = q E = −e E . dt dt

(8.1)

In the following, q denotes a general charge, while e is the (positive) elementary charge. We also consider an isotropic effective mass m ∗ at first. After the time δt the k vector of all conduction electrons (and the center of the Fermi sphere) has been shifted by δk δk = −

eE δt .

(8.2)

In the absence of scattering processes this goes on further (similar to an electron in vacuum). This regime is called ballistic transport. In a (periodic) band structure, the electron will perform a closed cycle as indicated in Fig. 8.1. Such motion is called a Bloch oscillation. However, in a bulk crystal the period T of such an oscillation eE T / = 2π/a0 is of the order of 10−10 s for E = 104 V/cm. This time is much longer than a typical scattering time of 10−14 s. Thus, in bulk material the Bloch electron cannot reach the zone boundary. However, in artificial superlattices (cf. Chap. 12) with larger periodicity (≈10 nm), high electric fields (≈106 V/cm) and high quality (reduced collision time) such motion is possible. We note that in the absence of scattering, electrons also perform a periodic oscillation in a magnetic field (cyclotron motion).

Fig. 8.1 Schematic representation of a Bloch oscillation

/a

/a

8.2 Conductivity

225

In a real semiconductor, at finite temperatures, impurities, phonons and defects (finally also the surface) will contribute to scattering. In the relaxation-time approximation it is assumed that the probability for a scattering event, similar to friction, is proportional to the (average) carrier velocity. The average relaxation time τ is introduced via an additional term v˙ = −v/τ that sums up all scattering events.1 Thus, the maximum velocity that can be reached in a static electric field is given by (steady-state velocity) eEτ v=− ∗ . (8.3) m The current density per unit area is then linear in the field, i.e. fulfills Ohm’s law j = nqv =

n e2 E τ = σE . m∗

(8.4)

The conductivity σ in the relaxation-time approximation is given by σ=

1 n e2 τ . = ρ m∗

(8.5)

In the case of a cylindrically symmetric mass such as for electrons in silicon or germanium, for the effective mass in (8.5) the effective conductivity mass must be used, 1 1 = ∗ mσ 3

2 1 + mt ml

.

(8.6)

The specific resistivity is the inverse of the conductivity. Metals have a high conductivity (see Table 8.1), e.g. for Cu at room temperature σ = 5.8 × 105 −1 cm−1 . At low temperatures (4 K) the conductivity is even a factor of 105 higher. The mean free path d = τ vF is d=

σ m ∗ vF , n e2

(8.7)

vF being the Fermi velocity (E F = m ∗ vF2 /2). For copper, d = 3 mm at low temperature (and thus susceptible to the sample geometry) while at room temperature the mean free path is only about 40 nm. However, this becomes an issue when the metal line width and height of interconnects in integrated circuits approaches this length scale [715] (see Sect. 24.5.5). In semiconductors, the carrier concentration depends strongly on the temperature. At zero temperature the conductivity is zero. Also, the scattering processes and thus the relaxation time constant exhibit a temperature dependence. The conductivity spans a large range from insulating to almost metallic conduction (see Table 8.1).

8.3 Low-Field Transport First we consider only small electric fields. The real meaning of this will only become clear in Sect. 8.4 on high-field transport. In the low-field regime the velocity is proportional to the electric field.

1 Going

beyond the relaxation time approximation is discussed in Appendix J.

226

8 Transport

Table 8.1 Conductivity at room temperature for various metals, semiconductors, insulators and liquids Material

σ (−1 cm−1 )

Ag Al Au Cu Fe Pt Ge pure (ND ∼ 1013 cm−3 ) Ge (ND ∼ 1015 cm−3 ) Ge (ND ∼ 1017 cm−3 ) Ge (ND ∼ 1018 cm−3 ) Si pure Si:As (ND ∼ 3 × 1019 cm−3 ) Si:B (NA ∼ 1.5 × 1019 cm−3 ) GaAs pure ZnO:Al (highly doped) Pentacene SiO2 Al2 O3 H2 O pure Hexane

6.25 × 105 3.6 × 105 4.35 × 105 5.62 × 105 1.1 × 105 1.02 × 105 10−2 1 2 × 101 2 × 102 4.5 × 10−6 4 × 102 1.2 × 102 1.4 × 10−7 ≈1 × 104 10−8 – 10−4 ≈10−15 ≈10−16 4 × 10−8 ≈10−18

8.3.1 Mobility The mobility is defined (scalar terms) as μ=

v . E

(8.8)

By definition, it is a negative number for electrons and positive for holes. However, the numerical value is usually given as a positive number for both carrier types. In an intrinsic semiconductor the mobility is determined by scattering with phonons. Further scattering is introduced by impurities, defects or alloy disorder. The conductivity is (8.4) σ =qnμ (8.9) for each carrier type. Using (8.5) the mobility in the relaxation time approximation is μ=

qτ . m∗

(8.10)

In the presence of both electrons and holes, σ = σe + σh = −e n μn + e p μp ,

(8.11)

where μn and μp are the mobilities for electrons and holes, respectively. These are given by μn = −e τn /m ∗e and μp = e τp /m ∗h . As the unit for mobility, usually cm2 /Vs is used. While Cu at room temperature has a mobility of 35 cm2 /Vs, semiconductors can have much higher values. In two-dimensional electron gases (cf.

8.3 Low-Field Transport

227

Table 8.2 Mobilities of electrons and holes at room temperature for various semiconductors Material

−μn (cm2 /Vs)

μp (cm2 /Vs)

Si Ge GaAs GaN InSb InAs InP ZnO

1300 4500 8800 300 77 000 33 000 4600 230

500 3500 400 180 750 460 150 8

Chap. 12), the mobility can reach several 107 cm2 /Vs at low temperature (Fig. 12.37). In bulk semiconductors with small band gap, a high electron mobility is caused by its small effective mass. Some typical values are given in Table 8.2.

8.3.2 Microscopic Scattering Processes The relaxation time constant summarizes all scattering mechanisms. If the relaxation times τi of various processes are independent, the Matthiesen rule can be used to obtain the mobility (μi = q τi /m ∗ ) 1 1 = . μ μi i

(8.12)

A more detailed book keeping is provided within the framework of the Boltzmann transport theory (Appendix J). The various scattering mechanisms have quite different temperature dependences such that the mobility is a rather complicated function of temperature. In [716] the mechanisms determining the low and high-field transport properties of (cubic) semiconductors are reviewed. A schematic overview of the various carrier scattering processes discussed in the following is shown in Fig. 8.2.

8.3.3 Ionized Impurity Scattering Theoretically, this problem is treated similar to Rutherford scattering. A screened Coulomb potential is assumed, as the scattering potential r Ze 1 , exp − V (r ) = − 4π0 r r lD

(8.13)

where lD is the screening length. The problem has been treated classically by Conwell and Weisskopf [717] and quantum mechanically by Brooks [718] and Herring. An expression for the mobility that encompasses the Conwell–Weisskopf and Brooks–Herring results is derived in [719]. Further details are given in [720, 721]. For the mobility it is found that

228

8 Transport

Fig. 8.2 Scheme of microscopic carrier scattering mechanisms

μion.imp. =

1 27/2 (4π0 r )2 (kT )3/2 , √ 3/2 2 3 ∗ N ln(1 + b) − 1/(1 + 1/b) π Z e m ion

(8.14)

with b = 4(k/lD )2 = 8 m ∗ E (lD /)2 . In the Thomas-Fermi screening model lD2 = 4π

1/3 4 m ∗ e2 1/3 3 n . π 0 r 2

e2 N (E F ) = 0 r

(8.15)

The formula (8.14) is valid only for b 1, i.e. small carrier densities. A similar formula from [720] is μion.imp.

√ −1 24 m ∗ 0 r (kT )2 128 2π (0 r )2 (kT )3/2 ln = . m ∗1/2 Z 2 Nion e3 n e 2 2

(8.16)

For large ionized impurity (and carrier) density (b 1), the mobility is given by [555] μion.imp. =

4e n −2/3 , π 2/3 h

31/3

(8.17)

the value of the pre-factor being about 3 × 1014 (Vs)−1 . The scattering time depends like τ ∝ (E/kT )s on the kinetic energy; for moderate or weak scattering s = 3/2, for very strong scattering, s = −1/2 [714]. For typical substitutional impurities, the charge of the scattering center is |Z | = 1; in oxides, oxygen vacancies may have Z = 2. At high impurity densities, impurity clusters may form with |Z | > 1; this will have a strong influence on the scattering rate since it proportional to Z 2 . The decrease of mobility for ND > 1020 cm−3 (Fig. 8.3a) is attributed to such effect which can be described with an effective impurity clustering charge Z D (Fig. 8.3b) [722, 723].

8.3 Low-Field Transport

229

Si 200

100

n-Si

4 3 2

1

0 18 10

(a)

6 5 Impurity custering Z

Electron mobilty (cm2/Vs)

300

19

20

21

10 10 10 Donor concentration (cm-3)

10

22

(b)

1020 1021 -3 Donor concentration (cm )

Fig. 8.3 a Electron mobility in highly doped silicon. Experimental data (symbols) from various sources and modeling with ionized impurity scattering with (solid line) and without (dashed line) considering impurity clustering. b Effective impurity cluster charge Z D . Adapted from [722]

8.3.4 Deformation Potential Scattering Acoustic phonons with small wavevector, i.e. a wavelength large compared to the unit cell, can have TA or LA character. The TA phonons represent a shear wave (with zero divergence), the LA phonons are a compression wave (with zero rotation). The LA is a plane wave of displacement δR parallel to the k-vector q, δR = A sin (q · R − ωt) . (8.18) The strain tensor is given by i j =

1 qi A j + q j Ai cos (q R − ωt) . 2

(8.19)

It has a diagonal form i j = qi A j for q and ω → 0. Therefore, the LA phonon creates an oscillatory volume dilatation (and compression) with amplitude q · A. This volume modulation affects the position of the band edges. For the conduction-band edge the energy change is related to the volume change by the hydrostatic deformation potential E ac.def. = V ∂ E C /∂V . Since the modulation is small compared to the energy of the charge carriers, it is mostly an elastic scattering process. The Hamilton operator for the LA scattering is (8.20) Hˆ = E ac.def. (q · A) . The size of the LA amplitude is given by the number of phonons in the mode that is given by the Bose– )]−1 . The mobility due to acoustic deformation potential Einstein distribution, Nph (ω) = [exp( ω kT scattering is found to be √ 2 2π e 4 cl (kT )−3/2 , (8.21) μac.def. = 2 3 m ∗ 5/2 E ac.def. where cl = ρcsLA , ρ being the density and cs being the sound velocity. The scattering time increases like τ ∝ E −1/2 with the kinetic energy [714]. The acoustical deformation potential scattering is important at high temperatures. It is dominating in nonpolar semiconductors (Ge, Si) at high temperatures (typically at and above room temperature).

230

8 Transport

8.3.5 Piezoelectric Potential Scattering In piezoelectric crystals (see Sect. 16.4), i.e. crystals that show an electric polarization upon strain, certain acoustic phonons lead to piezoelectric fields. In GaAs, with 111 being the piezoelectric directions, this is the case for shear waves. In strongly ionic crystals, e.g. II–VI semiconductors, the piezoelectric scattering can be stronger than the deformation potential scattering. The mobility due to piezoelectric potential scattering is μpz.el. = with K =

ep2 /cl , ep 0 r +ep2 /cl

16

√ 3

2π

0 r (kT )−1/2 , m ∗ 3/2 e K 2

(8.22)

being the piezoelectric coefficient.

8.3.6 Polar Optical Scattering LO phonons are connected with an electric field antiparallel to the displacement (9.29). In the scattering mechanism the absorbed or emitted phonon energy ω0 is comparable to the thermal energy of the carriers. Therefore, the scattering is inelastic and the relaxation-time approximation does not work. The general transport theory is complicated. If the temperature is low compared to the Debye temperature, T D e D , (8.23) μpol.opt. = exp 2 m ∗ α ω0 T where α =

1 137

m ∗ c2 2kD

1 (∞)

−

1 (0)

is the dimensionless polar constant.

8.3.7 Dislocation Scattering Dislocations can contain charge centers and thus act as scattering centers citeyou. This has been first demonstrated for n-Ge crystals that have been deformed [725, 726]. The deformation has introduced acceptor-type defects reducing the mobility in particular at low temperatures (similar to ionized impurity scattering). The mobility due to dislocation scattering in an n-type semiconductor is given by [727, 728] √ √ n 30 2π 2 d 2 (kT )3/2 ∝ T , (8.24) μdisl. = √ 3 2 ∗ Ndisl Ndisl e f L D m d being the average distance of acceptor centers along the dislocation line, f their occupation rate, Ndisl 2 1/2 the area √ density of dislocations and L D = (kT /(e n)) the Debye screening length. The relation μ ∝ n/Ndisl has been confirmed for various n-type GaN samples [729].

8.3 Low-Field Transport

231

(b)

(a)

Fig. 8.4 a Electronic barrier (E b ) for (hole) transport at a grain boundary (GB). b Average hole mobility in polysilicon, experimental data (symbols) and theoretical model (solid line). The dependence for monocrystalline silicon is shown for comparison as dashed line. Adapted from [730]

8.3.8 Grain Boundary Scattering The lowering of mobility due to transport across grain boundaries is an important effect in polycrystalline materials, such as poly-silicon for solar cells or thin film transistors [730–733]. Grain boundaries contain electronic traps whose filling depends on the doping of the bulk of the grains. Charges will be trapped in the grain boundaries and a depletion layer will be created.2 At low doping the grains are fully depleted and all free carriers are trapped in the grain boundaries. This means low conductivity, however, no electronic barrier to transport exists. At intermediate doping, traps are partially filled and the partial depletion of the grain leads to the creation of an electronic barrier E b (Fig. 8.4a) hindering transport since it must be overcome via thermionic emission. At high doping the traps are completely filled and the barrier vanishes again. Accordingly the mobility goes through a minimum as a function of the doping concentration (Fig. 8.4b) [730]. In [734] these data have been modeled with a 20 nm grain size, the value found in [730] from TEM analysis. The expression for the limitation of the mobility due to scattering at grain boundaries is given by [733, 735] e LG E b , (8.25) T −1/2 exp − μGB = √ kT 8m ∗ πk where L G is the grain size.

8.3.9 Alloy Scattering The random population of lattice sites represents disorder from a perfectly periodic lattice. The charge carrier mobility in an alloy Ax B1−x due to scattering in this potential is proportional to the alloy scattering potential U [590], μalloy =

3π m ∗

kT 2e 1 + exp(E F /kT ) , 2 x (1 − x) (U ) n

(8.26)

2 The following arguments may only be followed once the concept of depletion layers and band bending is understood, see Sect. 21.2.1.

232

8 Transport

(a)

(b)

Fig. 8.5 a Temperature dependence of the electron mobility in n-doped Ge (for various doping levels from ND ≈ 1018 for sample A to 1013 cm−3 for sample F in steps of a factor of ten). Dashed line indicates T −3/2 dependence of deformation potential scattering, solid lines are guides to the eye. Adapted from [594]. b μn (T ) for n-type GaAs (ND ≈ 5×1013 cm−3 , NA ≈ 2 × 1013 cm−3 ). Solid lines are theoretical mobilities for various scattering mechanisms and combined mobility according to (8.12). Adapted from [736]

(x) being the volume of the unit cell over which the alloy-scattering potential is effective. Such effect is present in any alloy such as Inx Ga1−x As [591] of Alx Ga1−x N [592]. For the latter material, see also the following section.

8.3.10 Dipole Scattering In alloys of polar semiconductors (Chap. 16), i.e. lower-symmetric (non-cubic) semiconductors with an electric polarization, the additional potential due to the random variation of the polarization introduces an additional scattering mechanism, the so-called dipole scattering [592]. Dipole scattering originally has been studied in the context of scattering in highly compensated semiconductors due to ionized donor-acceptor pairs [593].

8.3.11 Temperature Dependence The sum of all scattering processes leads to a fairly complicated temperature dependence of the mobility μ(T ). In covalent semiconductors (Si, Ge) the most important processes are the ionized impurity scattering (μ ∝ T 3/2 ) at low temperatures and the deformation potential scattering (μ ∝ T −3/2 ) at high temperatures (Fig. 8.5a). In polar crystals (e.g. GaAs) at high temperatures the polar optical scattering is dominant (Fig. 8.5b). In Fig. 8.6 the electron mobility of bulk and thin-film ZnO is compared. Since ZnO is polar the mobility at room temperature is limited by polar optical phonon scattering. In the thin film, grainboundary scattering (Sect. 8.3.8) additionally occurs and limits the mobility. In Fig. 8.7 the temperature dependence of the mobility is depicted for an alloy of polar semiconductors, namely Al0.25 Ga0.75 N. The contributions of alloy scattering and dipole scattering determine the mobility [592].

8.3 Low-Field Transport

(a)

233

(b)

Fig. 8.6 Temperature dependence of the electron mobility in n-type a bulk ZnO and b a PLD-grown ZnO thin film on sapphire. In the latter, grain-boundary scattering is limiting the mobility. Squares are experimental data, solid lines are theoretical mobilities for various scattering mechanisms and combined mobility according to (8.12). Experimental data from [737] Fig. 8.7 Calculated temperature dependence of the electron mobility in n-type Al0.25 Ga0.75 N, (ND = 5 × 1017 cm−3 ). PO: polar optic scattering, PE: piezoelectric scattering, ADP: acoustic deformation potential scattering. Adapted from [592]

Since the carrier concentration increases with increasing temperature and the mobility decreases, the conductivity has a maximum, typically around 70 K (see Fig. 8.8). At very high temperature, when intrinsic conduction starts, σ shows a strong increase due to the increase in n. At low temperature, the disorder due to doping (random positions of the impurity atoms) leads to a temperature driven metal–insulator transition as depicted in Fig. 8.21.

8.3.12 Doping Dependence The mobility decreases with increasing dopant concentration as already shown in Figs. 8.3 and 8.5a. In Fig. 8.9a the low doping limit is due to deformation potential scattering; the decrease with doping is due

234

8 Transport

(a)

(b)

Fig. 8.8 a Carrier concentration and b conductivity of n-type Ge as a function of temperature. The doping level varies from ND ≈ 1013 to 1018 (samples A–F as in Fig. 8.5a where the mobility of the same samples is shown). The dashed lines are for intrinsic Ge. The solid lines are guides to the eye. Adapted from [594]

Fig. 8.9 a Electron mobility in Si:P at room temperature over a wide range of carrier concentrations. b Electron mobility in Si:P and hole mobility in Si:B for various high carrier concentrations. Adapted from [739]

to ionized impurity scattering. At high doping level, it becomes more important at room temperature than (acoustical or optical) phonon scattering [738]. The mobility of carriers in n- and p-type silicon with very high carrier concentrations is depicted in Fig. 8.9b. Thus, for bulk material high carrier density and high mobility are contrary targets and cannot be achieved simultaneously. A solution will be provided with the concept of modulation doping where the dopants and the (two-dimensional) carrier gas will be spatially separated in a heterostructure (cf. Sect. 12.3.4). At high doping, the substitutional character of the impurities may be lost and secondary phases can arise, e.g. as observed for highly doped ZnO:Ga, exhibiting octahedral coordination of gallium

8.3 Low-Field Transport

235

Fig. 8.10 Conductivity of B-doped diamond as a function of temperature. Adapted from [746]

in a parasitic ZnGa2 O4 spinel phase for [Ga]=4% [632]. The onset of such segregation phenomena is accompanied with the decrease of mobility and conductivity.

8.3.13 Superconductivity It has been found that highly doped semiconductors do not only behave like metals in the sense that the carrier concentration is largely independent of temperature but that they can also exhibit superconductivity. Theoretical and early experimental investigations suggested the possibility of such behavior [740–743] even when the electron concentration is much smaller than one per atom. Experimentally, robust superconductivity in semiconductors has been found more recently for a number of semiconductors [744, 745], namely boron-doped diamond (C:B) [746] (Fig. 8.10), Si:B [747] and Ge:Ga [748]. The preparation of superconducting semiconductors with critical temperature above 1 K typically involves hyperdoping with impurity concentrations of several atomic percent. The detailed physics of these materials, such as the superconductor type (type-II behavior was found for C:B) or the electron coupling mechanism (generally, phonon-assisted pairing is assumed), are still under debate. Another type of superconducting semiconductor structure are twisted monolayers in Van-der-Waals heterostructures for particular values of twist angle and carrier concentration (cf. Sect. 13.3).

8.3.14 Piezoresistivity The dependence of resistivity on stress or strain is known as piezoresistive effect, first described in [749]. It is a consequence of the modification of the band structure upon stress and the change of effective masses (Sect. 6.12.2). In a cubic material, the resistivity ρi for transport in cartesian direction i changes compared to the unstrained state in a phenomenological description according to ρi = πi j σ j , ρi

(8.27)

where π is the piezoresistivity tensor (8.28) and the σ j form the six-component stress tensor (5.55),

236

8 Transport

Fig. 8.11 Piezoresistive coefficient for current parallel (perpendicular) to the stress πl as blue lines (πt , red lines) for uniaxially stressed Si (001) at room temperature, a for p-type Si, b for n-type Si. The upper (lower) halves of the graphs show positive (negative) values of the piezoresistive coefficient, i.e. resistivity increases (decreases) with tensile stress. The solid circle indicates the value of |π| = 10−9 Pa−1 , the dashed circle half that value. Adapted from [752] Table 8.3 Piezoresistivity coefficients (in 10−11 Pa−1 ) for Si, Ge and GaAs at room temperature Material

ρ (Ω cm)

π11

π12

p-Si n-Si p-Ge (Ge:Ga) n-Ge (Ge:As) p-GaAs n-GaAs

7.8 11.7 15.0 9.9 ∼10−3 ∼10−3

6.6 −102.2 −10.6 −4.7 −12.0 −3.2

⎛

π11 ⎜ π12 ⎜ ⎜ π12 π=⎜ ⎜ 0 ⎜ ⎝ 0 0

−1.1 53.4 5.0 −5.0 −0.6 −5.4

π12 π11 π12 0 0 0

π12 π12 π11 0 0 0

0 0 0 π44 0 0

0 0 0 0 π44 0

π44

References

138.1 −13.6 98.6 −137.9 46 −2.5

[749] [749] [749] [749] [753] [753, 754]

⎞ 0 0 ⎟ ⎟ 0 ⎟ ⎟ . 0 ⎟ ⎟ 0 ⎠ π44

(8.28)

Values for the piezoelectric coefficients are given in Table 8.3 for Si, Ge and GaAs. The piezoelectric effect has been discussed in detail [750] and modeled for p-type Si [751]. We shall only give a simple example which is particularly relevant for advanced CMOS design (Sect. 24.5.5); the directional dependence of the piezoresistive coefficient of silicon is shown for uniaxial stress within in the (001) plane in Fig. 8.11. Uniaxial tensile stress increases hole resistivity along 110 stress directions, compressive stress thus increases hole conductivity.

8.4 High-Field Transport In the case of small electric fields the scattering events are elastic. The drift velocity is linearly proportional to the electric field. The average thermal energy is close to its thermal value 3kT /2 and the carriers are close to their band edges (Fig. 8.12a). The scattering efficiency, however, is reduced

8.4 High-Field Transport

(a)

237

(b)

(c)

Fig. 8.12 Distribution of electrons in silicon in momentum space (cmp. Fig. 6.35c) for electric fields of a 10 kV/cm, b 102 kV/cm and c 103 kV/cm. Adapted from [756]

already at moderate fields. Then, the electron temperature [755] becomes larger than the lattice temperature. With increasing electrical field the carriers can gain more and more energy and will on average populate higher states, assuming a non-Boltzmann (and non-Fermi) statistical distribution [756]. The electron distribution in k-space is depicted for silicon for three different electric fields in Fig. 8.12b,c. Hot carriers suffer additional scattering processes that are discussed in the following, namely optical phonon emission, intervalley scattering and impact ionization.

8.4.1 Drift-Saturation Velocity If the carrier energy is large enough it can transfer energy to the lattice by the emission of an optical phonon. This mechanism is very efficient and limits the maximum drift velocity. Such behavior is non-ohmic. The limiting value for the drift velocity is termed the drift-saturation velocity. It is given by [757] 8 ωLO . (8.29) vs = 3π m∗ This relation can be obtained from an energy-balance consideration. The energy gain per unit time in the electric field is equal to the energy loss by the emission of an optical phonon. qv·E=

ωLO , τ

(8.30)

where τ is the typical relaxation time constant for LO phonon emission. Together with (8.3) we find (8.30) except for the pre-factor, which is close to 1. The exact pre-factor results from a quantummechanical treatment. For Ge the drift-saturation velocity at room temperature is 6 × 106 cm/s, for Si it is 1 × 107 cm/s (Fig. 8.13a). The carrier velocity also depends on the crystallographic direction [758].

8.4.2 Negative Differential Resistivity In GaAs, the initially linear regime (constant mobility) saturates at a maximum drift velocity of about 2 × 107 cm/s for about 3 kV/cm; for higher fields, a reduction in drift velocity (with increasing field!) is present (1.2 × 107 cm/s at 10 kV/cm, 0.6 × 107 cm/s at 200 kV/cm), as shown in Fig. 8.13a. This

238

8 Transport 10

8

ZnO 3.0 7

GaAs 10

7

GaN InP

2.0

Ge 10

InGaAs

6

GaAs

1.0

electrons holes

Si

Si

5

10 2 10

10

3

10

4

10

5

10

(a)

0 0

6

100

200

300

(b)

Fig. 8.13 Drift velocity at room temperature as a function of applied electric field for a high-purity Si, Ge, and GaAs on a double-logarithmic plot and b on linear plots for Si [759], Ge [760], GaAs [676], InP [761], (In, Ga)As [762], GaN and ZnO [763] Table 8.4 Material parameters for multi-valley bandstructure of GaAs and InP. E denotes the energetic separation of the two lowest valleys of the conduction band, E thr the threshold field for NDR and vP the peak velocity (at E thr ). Most values from [766] Material

GaAs InP

Eg (eV)

E (eV)

E thr (kV/cm)

vP (107 cm/s)

Lower valley () m∗ μn (m 0 ) (cm2 /Vs)

1.42 1.35

0.36 0.53

3.2 10.5

2.2 2.5

0.068 0.08

≈8000 ≈5000

Upper valley (L) m∗ μn (m 0 ) (cm2 /Vs) 1.2 0.9

≈180 ≈100

regime, above the threshold field of E thr = 3.2 kV/cm in GaAs, is called negative differential resistivity (NDR) and was predicted in [764]. This phenomenon can be used in microwave oscillators, e.g. the Gunn element (Sect. 21.5.11). The effect occurs in a multi-valley band structure (see Fig. 8.14, for values cf. Table 8.4), e.g. in GaAs or InP, when the carrier energy is high enough to scatter (Fig. 8.14c,d) from the minimum (small mass and high mobility) into the L valley (large mass and low mobility) [765]. The temperature dependence of the saturation velocity is shown in Fig. 8.15. With increasing temperature the saturation velocity decreases since the coupling with the lattice becomes stronger.

8.4.3 Velocity Overshoot When the electric field is switched on, the carriers are at first in the minimum (Fig. 8.14a). Only after a few scattering processes are they scattered into the L minimum. This means that in the first moments transport occurs with the higher mobility of the lowest minimum (Fig. 8.14e). The velocity is then larger than the (steady-state) saturation velocity in a dc field. This phenomenon is called velocity overshoot and is a purely dynamic effect (Fig. 8.16). Velocity overshoot in GaN is discussed in [769]. It is an important effect in small transistors.

8.4 High-Field Transport

239

Fig. 8.14 Charge-carrier distribution in a multi-valley band structure (e.g. GaAs, InP) for a zero, b small (E < E a ), c intermediate and d large (E > E b ) field strength. The situation shown in e is reached temporarily during velocity overshoot (see also Fig. 8.16) Fig. 8.15 Temperature dependence of the saturation velocity for Si (following vs = vs0 (1 + 0.8 exp(T /600 K ))−1 with vs0 = 2.4 × 107 cm/s from [759]) and GaAs [676, 767, 768]

8.4.4 Impact Ionization If the energy gain in the field is large enough to generate an electron–hole pair, the phenomenon of impact ionization occurs. The kinetic energy is ∝ v2 . Momentum and energy conservation apply. Thus, at small energies (close to the threshold for impact ionization) the vectors are short and collinear to fulfill momentum conservation. At higher energy, larger angles between the velocity vectors of the impact partners can also occur. If the process is started by an electron (Fig. 8.17a) the threshold energy is given by [770] me Eg . (8.31) E ethr = 1 + m e + m hh If the process starts with a heavy hole, the threshold [770],

240

8 Transport

Fig. 8.16 Time dependence of the electron velocity at room temperature upon a step-like electric field (40 kV/cm) for GaAs (dash-dotted line), InP (dashed line) and In0.53 Ga0.47 As (solid line)

In0.53Ga0.47As

8

7

6

4

InP

2 GaAs 0

Fig. 8.17 Electron and hole transitions for impact ionization close to the threshold energy. Ionization is triggered by a an electron and b a split-off hole of velocity vi

0.2

0

0.4

0.6

E

E

e

0.8

vi e

Eg Eg

lh

hh

lh

hh

vi so

so

k (b)

(a)

thr E hh

m hh = 1+ m e + m hh

k

Eg ,

(8.32)

is larger because of the larger hole mass. The threshold for impact ionization triggered by a split-off hole (shown schematically in Fig. 8.17b) is [771] m so (1 − 0 /E g ) (8.33) Eg . E hthr = 1 + 2 m hh + m e − m so

8.4 High-Field Transport

241

Ionization rate (s-1)

Fig. 8.18 Impact ionization rate as a function of primary carrier energy for electrons (solid line) and holes (dashed line) in silicon at room temperature. The curves are fit to results from a Monte-Carlo simulation. Adapted from [772, 773]

10

15

10

14

10

13

10

12

Si

h e

1011 10

10

10

9

108 107 0

1 3 4 2 Primary energy (eV)

5

Thus so-holes have typically the smaller threshold.3 At energies where impact ionization occurs, nonparabolicities are typically important, thus (8.31)–(8.33) are only indicative. The threshold behavior and the dependence of the scattering rate as a function of the primary carrier energy in Si, calculated considering the detailed band structure, is shown in Fig. 8.18. The generation rate G of electron–hole pairs during impact ionization is given by G = αn n vn + αp p vp ,

(8.34)

where αn is the electron ionization coefficient. It describes the generation of electron–hole pairs per incoming electron per unit length. αp denotes the hole ionization coefficient. The coefficients depend strongly on the applied electric field. They are shown in Fig. 8.19. They also depend on the crystallographic direction. The impact ionization initiated by electrons and holes in silicon has been calculated considering the full band structure using a Monte Carlo technique in [772] and [773], respectively. In both cases the impact ionization rate is anisotropic for excess energies smaller than 3 eV and become isotropic above. The average energies at the moment of generation of secondary generated carriers depends linearly on the primary electron or hole energy. The energy dependence of the electron initiated impact ionization rate has been calculated for GaAs, GaN and ZnS considering details and anisotropy of the band structure in [774]. The rates averaged over the Brillouin zone are compared in Fig. 8.20. Because of the large band gap of GaN, impact ionization can only be generated by electrons in higher conduction bands. The sharp increase of ionization rate for GaN around 5.75 eV correlates with a large valence band DOS from hole states at the zone boundary.

8.5 High-Frequency Transport The above consideration pertained to dc (or slowly varying) fields. Now, we consider an ac field. It accelerates the carriers but at the same time the dissipative force in the relaxation-time approximation is present, i.e. (for electrons) v (8.35) m ∗ v˙ = −e E − m ∗ . τ 3 Assuming

thr /E thr ≈ 1 − (m /m )(1 + /E )/2 < 1. m so = m e , m e m hh and 0 E g , E so e hh g e

242

8 Transport

Fig. 8.19 Impact ionization rates for electrons and holes as a function of the inverse electric field for Si, Ge and other compound semiconductors at 300 K. Adapted from [574]

Fig. 8.20 Averaged rates for electron initiated impact ionization in GaAs (circles) and GaN (squares). Adapted from [774]

For a harmonic field E ∝ exp(−iωt) the complex conductivity (j = σE = nqv) is σ=

n e2 1 i n e2 τ = , ∗ ∗ m 1 − i ωτ m ω + iγ

(8.36)

with γ = 1/τ being the damping constant. Splitting into real and imaginary parts yields n e2 τ σ= m∗

1 ωτ +i 2 2 1+ω τ 1 + ω2 τ 2

.

(8.37)

For small frequencies (ω → 0) the dc conductivity from (8.5) is recovered, i.e. σ = ne2 τ /m ∗ . For high frequencies (ωτ 1) 1 1 n e2 τ . (8.38) +i σ= m∗ ω2 τ 2 ωτ

8.6 Impurity Band Transport

10

3

10

2

10

1

Si:P

(T=0) (S/cm)

Fig. 8.21 Zero temperature conductivity of Si:P for various (donor) doping concentrations. Experimental data (symbols) and guide to the eye (dashed line). Adapted from [781]

243

100 10-1 10-2 0

insulator 2

metal 4 ND (1018 cm-3)

6

8

8.6 Impurity Band Transport In Sect. 7.5.7, the formation of an impurity band in the presence of high doping and overlap of impurity wave functions was discussed. The hopping (tunneling) transport of carriers from impurity to impurity leads to an additional transport channel termed ’impurity band conduction’[775–777]. The phenomenon has been found for many doped semiconductors, among them more recently GaAs:Mn [778] or Ga2 O3 :Sn [779] where at low temperatures a constant carrier concentration is attributed to the impurity band conduction effect. The random distribution of dopants essentially makes a doped semiconductor a disordered system. The physics of electronic states in disordered systems has been reviewed in [780]. A metal–insulator transition is observed at a certain value of doping (NP = 3.8 × 1018 cm−3 ), as shown in Fig. 8.21 for Si:P [781]. For a certain value of disorder all states become localized (Anderson localization [782, 783], cmp. Sect. 8.9).

8.7 Polarons In an ionic lattice, the electron polarizes the ions and causes a change of their equilibrium position. Depending on the severity of this effect, the lattice polarization leads to a modification of carrier (electron or hole) mass during band transport (Sect. 8.7.1) (large polarons) or the lattice deformation is so strong that it leads to carrier localization on the length scale of the lattice constant. Such self-trapped carriers are termed small polarons and discusssed in Sect. 8.7.1. Reviews are given in [784, 785].

8.7.1 Large Polarons When the electron moves through the ionic crystal and must drag an ion displacement with it, the effective electron mass changes to the ‘polaron mass’ m p ,4 4 For the calculation, many-particle theory and techniques are needed; the best solution is still given by Feynman’s path integral calculation [786–788].

244

8 Transport

Table 8.5 Fröhlich coupling constant α for various semiconductors. Data from [165] GaSb 0.025 3C-SiC 0.26

GaAs 0.068 ZnO 1.19

GaP 0.201 ZnS 0.63

GaN 0.48 ZnSe 0.43

InSb 0.022 ZnTe 0.33

InAs 0.045 CdS 0.51

α m p = m ∗ 1 + + 0.025 α2 + · · · , 6

InP 0.15 CdSe 0.46

InN 0.24 CdTe 0.35

(8.39)

for α ≤ 1, with m ∗ being the band mass as defined in Sect. 6.9.2 and α the Fröhlich coupling constant5 1 e2 α= 2

2 m∗ ωLO

1 1 − ∞ 0

.

(8.40)

This process it called the polaronic effect and requires additional energy [786, 789]. Often, the polaron mass is given as m p = m ∗ /(1 − α/6) which is the result of perturbation theory [789] and an approximation to (8.39) for small α. For large coupling parameter, α 1, the polaron mass is given by [787] mp = m∗

16 α4 . 81 π 4

(8.41)

The energy of the electron is lowered due to the interaction with the lattice. The energy E 0 for k = 0 is given, relative to the uncoupled case, by E 0 = − α + 0.0098 α2 + · · · ω0 , α ≤ 1 E 0 = − 2.83 + 0.106 α2 ω0 , α 1

(8.42a) (8.42b)

Numerical results are reported in [790]. Polarons in semiconductors are typically ‘large’ or Fröhlich-type polarons, i.e. the coupling constant is small (Table 8.5). The dressing with phonons (as the ion displacement is called in a quantummechanical picture) is then only a perturbative effect and the number of phonons per electron (≈α/2) is small. If α becomes large (α > 1, α ∼ 6), as is the case for strongly ionic crystals such as alkali halides, the polaron becomes localized by the electron–phonon interaction6 and hopping occurs infrequently from site to site.

8.7.2 Small Polarons In a polaron, the charge carrier (electron or hole) sits in a potential well resulting from the ionic displacements it created. In some materials, the shape and strength of this potential well is such that the charge is confined to a volume of approximately one unit cell or less. In this case, the polaron is 5 This constant is part of the matrix element in the Hamiltonian of the electron–phonon interaction and is related to the electric field created by LO phonons, as given in (9.29). 6 One can think about it in the way that the electron strongly polarizes the lattice and digs itself a potential hole out of which it can no longer move.

8.7 Polarons

245

Fig. 8.22 Hole from Nb acceptor localized on Ti site (small polaron) in rutile TiO2 . Adapted from [793]

Fig. 8.23 Simulated and experimental TEM images of β-Ga2 O3 in (101) projection. The arrow denotes the position of a polaron. Adapted from [792]

simulation

experiment

(101)

called a small polaron. An example of a hole polaron in rutile TiO2 :Nb is depicted in Fig. 8.22. In oxides often the hole from an acceptor is bound to oxygen, e.g. in BaTiO3 :Na, as reviewed in [791]. In Fig. 8.23 the lattice relaxation due to a hole bound to oxygen in the monoclinc unit cell of β-Ga2 O3 is depicted directly using aberration corrected TEM. The bonding of the hole to the oxygen atom breaks the bond to a Ga atom which moves by 0.1 nm from its equilibrium position [792]. A proper theoretical analysis of a small polaron requires ab initio techniques that account for the motion of each atom in the few unit cells nearest the electron.7 The transport of small polarons occurs generally via thermally-activated hopping (cmp. Sect. 8.8). Under certain conditions the following mobilities for drift and Hall effect have been given [784]: μd ∝ T −1 exp(−W/(2kT )) , μH ∝ T −1/2 exp(−W/(6kT )) ,

(8.43) (8.44)

W being the polaron binding energy. Generally, materials with small polaron transport exhibit high carrier density, often due to structural defects, and low mobility.

8.8 Hopping Transport Disordered solids such as amorphous semiconductors, films containing quantum dots or material with many defects are characterized by a large density of localized states which can form band tails or a large density of states within the band gap. Hopping conduction is the tunneling between localized states and has been treated with various models [795–797]. 7 This

paragraph has been taken from the concise tutorial by S.J.F. Byrnes [794].

246

8 Transport

Fig. 8.24 Temperature dependence of the planar resistance for Si films deposited at room temperature. Solid line is linear fit with T0 = 8 × 107 K according to (8.45) (s = 1/4). Adapted from [798]

T 300

200

100

a-Si 1012 1011 1010 109 108 107 106

0.25

0.27

0.29 0.31 T-1/4 (K-1/4)

0.33

0.35

A commonly observed phenomenon is the variable range hopping with a conductivity given by σ = σ0 exp −(T0 /T )s

(8.45)

with s = 1/4. Such law is fulfilled for amorphous silicon (Fig. 8.24). Mott has derived [799] the exponent s = 1/4 using the following argument: The probability p to hop from one localized site to another is proportional to p ∝ exp(−2αR − W/kT ) . (8.46) The first term stems from the probability to find the electron within radius R from its initial site, α being the decay constant of its wave function, (r ) ∝ exp(−α r ). The second term is the Boltzmann factor for bridging the energy mismatch W between localized states with a phonon-assisted process, assuming a low temperature limit (kT W ). There is a trade-off between hopping to levels closer in energy but spatially further away (on average), preferred at low temperature and the hopping to energy levels with larger W but spatially closer at higher temperatures. Thus the hopping range changes with temperature, giving the mechanism its name. D(E F ) shall be the (constant) density of localized states around the Fermi level. Within a radius R, there is on average one state of energy between 0 and W (R) when (for three-dimensional bulk material) 1 W (R) = . (8.47) D(E F ) (4π/3) R 3 Substituting (8.47) in (8.45) and searching for the maximum yields the most probable hopping distance R ≈ (α kT D(E F ))−1/4 ,

(8.48)

showing again, the varying range of hopping with temperature. Thus we find for T0 in (8.45), T0 ≈

α3 . k D(E F )

(8.49)

Other types of hopping mechanisms are the Efros–Shklovskii variable range hopping (s = 1/2), emerging for an energy dependent density of states D(E) ∝ (E − E F )2 due to Coulomb interaction between hopping sites [800], or the next neighbor hopping (s = 1).

8.8 Hopping Transport T 100 0.0 -0.2

150

200

250

300

a-Si:H s=0.54±0.05

-0.4 -0.6 ln

Fig. 8.25 Temperature dependence of conductivity of a hydrogenated amorphous Si thin film, plotted as ln ξ vs. ln T (8.50). Solid lines are linear fits for constant s according to (8.50) as labelled. Adapted from [801]

247

-0.8 -1.0 s=1.08±0.14

-1.2 -1.4

5.0

delocalized

5.2 ln(T

5.4

localized

5.6

5.8

delocalized

DOS (arb. units)

Fig. 8.26 Schematic density of states of amorphous semiconductor with band tails and deep levels. The localized (delocalized) states are shown in dark (light) grey. The mobility edges for electrons and holes are indicated by dashed lines

4.8

EV

EF Energy

EC

From (8.45) one can rewrite for ξ = d(ln σ(T ))/d ln T , ln ξ = ln s + s ln T0 − s ln T .

(8.50)

Thus in a plot of ln ξ vs. ln T , the exponent s can be determined from the slope. As can be seen in Fig. 8.25, for the conductivity of a hydrogenated amorphous silicon thin film the transition of hopping mechanism from Efros–Shklovskii variable range hopping (s ≈ 1/2) to next neighbor hopping (s ≈ 1) takes place around T = 220 K, as discussed in detail in [801].

8.9 Transport in Amorphous Semiconductors Many models have been presented for the carrier transport in amorphous semiconductors [203]. The most important concept is that of a mobility edge, an energy separating localized from delocalized states [547, 548, 802]. This is schematically depicted in Fig. 8.26. The carrier transport between localized states is mediated via tunneling (hopping) which has been described in the previous section (Sect. 8.8). The localization of carriers in random lattices has been treated by Anderson [782] and reviewed in [780]. If the degree of disorder surpasses a certain value, diffusion is suppressed (at T = 0) and conductivity vanishes altogether (Anderson metal–insulator transition).

248

8 Transport

The transport in delocalized states is similar to band transport. The conductivity (for electrons) is given as σ = −e

∞

De (E) μe (E) f e (E) dE .

(8.51)

EC

If the Fermi energy is close to the middle of the gap, pinned to deep states, the Fermi-Dirac distribution can be replaced by the Boltzmann factor. Assuming a constant density of states and mobility for the delocalized states, EC − EF . (8.52) σ = −e De (E C ) μe (E C ) kT exp kT Charge carriers from localized states in the tails can be thermally excited into delocalized states and contribute to conductivity (thermally activated hopping). The mobility then contains an exponential thermal activation term [203].

8.10 Ionic Transport Ionic transport is the movement of ions upon application of a voltage. Here, we discuss only solid electrolytes. The transport can include the motion of one or several of the constituents of the lattice and the transport of other ions (e.g. hydrogen ions (protons), oxygen ions) through the crystal. Related to this is the diffusive ionic movement of impurities or defects through the crystal (cmp. Sect. 4.2.3). Ionic conduction of the lattice constituents under dc voltage will eventually destroy the crystal. In typical semiconductors like silicon or gallium arsenide, the conductivity is entirely due to electronic conduction. A typical solid electrolyte is zirconia (ZrO2 ) doped with yttria, so-called yttriastabilized zirconia (YSZ) that takes on a cubic fluorite lattice (see Sect. 3.4.8). It can conduct oxygen ions via the mobility of oxygen vacancies for use in solid-oxide fuel cells (SOFC) [803]. The conductivity is about 0.01 S/cm at a temperature around 1000 K, almost entirely due to ionic transport. Doping with calcium oxide results in an oxygen conductor that is used in oxygen sensors in automobiles (lambda sensor). The ionic conductivity can be significantly increased, compared to bulk material, along interfaces [804, 805]. Other typical solid electrolytes are copper iodide (CuI) [568] and also AgI. In the high temperature cubic phase (α-polymorph), the iodide ions form a fairly rigid cubic framework and the metal ions are mobile; the copper diffusion pathways have been discussed [806, 807]. The temperature dependence of conductivity of CuI is shown in Fig. 8.27.

8.11 Diffusion A gradient of a particle concentration n leads to a particle current proportional to −∇n. This diffusion law (Fick’s law) corresponds microscopically to a random walk. The gradients of the semiconductor carrier densities ∇n or ∇ p thus lead to electron and hole currents, respectively: jn = eDn ∇n

(8.53a)

jp = −eDp ∇ p .

(8.53b)

The coefficients Dn and Dp are called the electron and hole diffusion coefficient, respectively. Thus the total electron and hole currents in the presence of an electric field E and diffusion are

8.11 Diffusion Fig. 8.27 Total (circles) and electronic (squares) conductivity of CuI coexisting with copper. Filled (empty) symbols refer to polycrystalline (single crystal) samples. The different structural phases (α (cubic), β (wurtzite), γ (zincblende)) are indicated by shaded areas as labeled. Dashed lines are guides to the eye. Adapted from [808]

249

405

369350

300

275

CuI 101

10

0

10-1

10-2 1.3

1.4

1.5 1.6 1.7 1000/T (1000/K)

1.8

1.9

jn = −eμn n E + eDn ∇n

(8.54a)

jp = eμp p E − eDp ∇ p .

(8.54b)

This relation can also be deduced more generally from the gradient of the Fermi level as jn = −eμn n E − nμn ∇ E F

(8.55a)

jp = eμp p E − pμp ∇ E F .

(8.55b)

Using (7.6) and (7.7) for the concentrations (valid also in the case of degeneracy) and using dF j (x)/dx = F j−1 (x) we obtain F1/2 (η) ∇n F−1/2 (η) F1/2 (ζ) ∇p , jp = eμp p E − kT μp F−1/2 (ζ)

jn = −eμn n E − kT μn

(8.56a) (8.56b)

with η = (E F − E C )/kT and ζ = −(E F − E V )/kT . If the pre-factor of the density gradient is identified as the diffusion coefficient we find the (generalized) so-called ‘Einstein relations’ (β = e/(kT )) [608, 809]: F1/2 (η) F−1/2 (η) F1/2 (ζ) Dp = β −1 μp . F−1/2 (ζ)

Dn = −β −1 μn

(8.57a) (8.57b)

The effect of non-parabolicity has been included in [810]. Useful analytical approximations have been discussed in [811]. We note that, e.g., (8.57a) can also be written as [812, 813] ∂η . (8.58) Dn = −β −1 μn n ∂n

250

8 Transport

In the case of nondegeneracy, i.e. when the Fermi level is within the band gap and not closer than about 4kT to the band edges, η = ln(n/NC ). Then ∂η/∂n = 1/n, and the equation simplifies to D = (kT /q)μ, i.e. the ‘regular’ Einstein-relations, Dn = −β −1 μn

(8.59a)

Dp = β −1 μp .

(8.59b)

jn = −eμn n E − kT μn ∇n jp = eμp p E − kT μ p ∇ p .

(8.60a) (8.60b)

In this case, (8.54a,b) read

We recall that both diffusion coefficients are positive numbers, since μn is negative. Generally, the diffusion coefficient depends on the density. A Taylor series of the Fermi integral yields

−1

Dn = −β μn 1 + 0.35355

n NC

− 9.9 × 10

−3

n NC

2 + ···

.

(8.61)

8.12 Continuity Equation The balance equation for the charge is called the continuity equation. The temporal change of the charge in a volume element is given by the divergence of the current and any source (generation rate G), e.g. an external excitation, or drain (recombination rate U ). Details about recombination mechanisms are discussed in Chap. 10. Thus, we have ∂n = G n − Un − ∂t ∂p = G p − Up − ∂t

1 1 ∇ · jn = G n − U n + ∇ · jn q e 1 ∇ · jp . e

(8.62a) (8.62b)

In the case of nondegeneracy we find, using (8.54ab) ∂n = G n − Un − μn n ∇ · E − μn E ∇n + Dn n ∂t ∂p = G p − Up − μp p ∇ · E − μp E ∇ p + Dp p . ∂t

(8.63a) (8.63b)

In the case of zero electric field these read ∂n = G n − Un + Dn n ∂t ∂p = G p − Up + Dp p , ∂t and if the stationary case also applies:

(8.64a) (8.64b)

8.12 Continuity Equation

251

Dn n = −G n + Un Dp p = −G p + Up .

(8.65a) (8.65b)

8.13 Heat Conduction We consider here the heat transport [814] due to a temperature gradient. The heat flow q, i.e. energy ˆ is proportional to the local gradient of temperature. The per unit area per time in the direction q, proportionality constant κ is called, heat conductivity, q = −κ ∇T .

(8.66)

In crystals, the heat conductivity can depend on the direction and thus κ is generally a tensor of rank 2. In the following, κ will be considered as a scalar quantity. The quite generally valid Wiedemann–Franz law connects the thermal and electrical conductivities π2 κ= 3

2 k Tσ . e

(8.67)

The balance (continuity) equation for the heat energy Q is ∇· q = −

∂T ∂Q = −ρC +A, ∂t ∂t

(8.68)

where ρ denotes the density of the solid and C the heat capacity. A denotes a source or drain of heat, e.g. an external excitation. Combining (8.66) and (8.68), we obtain the equation for heat conductivity T =

A ρ C ∂T − , κ ∂t κ

(8.69)

which simply reads T = 0 for a stationary situation without sources. The random mixture of various atoms in natural elements represents a perturbation of the perfectly periodic lattice. Since the mass of the nuclei varies, in particular lattice vibrations will be perturbed. Thus we expect an effect on the heat conductivity. In Fig. 8.28, the thermal conductivity of crystals from natural Ge and enriched 74 Ge are compared [815], the latter having, as expected, the higher heat conductivity, i.e. less scattering. The T 3 -dependence of the heat conductivity at low temperature has been attributed to scattering of phonons at the sample boundary [816]. The thermal conductivity of isotopically pure 28 Si thin films has been measured to be 60% greater than natural silicon at room temperature and at least 40% greater at 100◦ C, a typical chip operating temperature [817, 818].

8.14 Coupled Heat and Charge Transport The standard effect of coupled charge and heat transport is that a current heats its conductor via Joule heating. However, more intricate use of thermoelectric effects can also be employed to cool certain areas of a device. For further details see [819, 820]. For the analysis of coupled charge and heat transport we first sum the electric field and the concentration gradient to a new field Eˆ = E + ∇ E F /e. Then, the heat flow and charge current are

252

8 Transport

Fig. 8.28 Thermal conductivity of Ge vs. temperature. The enriched Ge consists of 96% 74 Ge while the natural isotope mix is 20% 70 Ge, 27% 72 Ge, 8% 73 Ge, 27% 74 Ge and 8% 76 Ge. The dashed line shows a κ ∝ T 3 dependence at low temperatures. Adapted from [815]

100 3

T

50

enriched 74Ge

10

-1

-1

20

5 2 1 0.5 0.2 1

j = σ Eˆ + L ∇T q = M Eˆ + N ∇T ,

2

5

10

20

50 100 200

500

(8.70) (8.71)

where Eˆ and ∇T are the stimulators for the currents. From the experimental point of view there is interest to express the equations in j and ∇T since these quantities are measurable. With new coefficients they read Eˆ = ρ j + S ∇T

(8.72)

q = j − κ ∇T ,

(8.73)

where ρ, S and are the specific resistance, thermoelectric power and Peltier coefficient (transported energy per unit charge), respectively. The relations with the coefficients σ, L, M, and N are given by ρ=

1 σ

L σ M = σ ML −N . κ= σ S=−

(8.74a) (8.74b) (8.74c) (8.74d)

8.14.1 Thermopower and Seebeck Effect A semiconductor shall have two ends at different temperatures T2 and T1 and a temperature gradient in between in an open circuit, i.e. j = 0. Then a field Eˆ = S ∇T and a voltage U = S/(T2 − T1 ) will arise. This effect is called the thermoelectric or Seebeck effect. S is termed the Seebeck coefficient or the thermoelectric power, often also denoted as Q in the literature. The voltage can be measured and used to determine the temperature at one end if the temperature at the other end is known, forming

8.14 Coupled Heat and Charge Transport

253 0.6

0.9

(a)

0.6

Thermoelectric force S T (V)

Thermoelectric force S (mV/K)

Ge

0.3 0 -0.3 -0.6

Si

0.4 0.2 p-type 0 n-type -0.2 intrinsic

-0.4 -0.6

-0.9 100 200 300 400 500 600 700 800 900 1000 Temperature (K)

-0.8 200

300

(b)

400

500 600 700 Temperature (K)

800

900 1000

Fig. 8.29 a Seebeck coefficient S for n- and p-doped germanium. Experimental data (symbols) and theory (lines). NA − ND is 5.7 × 1015 cm−3 (white circles), 1.7 × 1017 cm−3 (grey) and 7.2 × 1018 cm−3 (black); ND − NA is 3.3 × 1015 cm−3 (white squares), 1.1 × 1017 cm−3 (grey) and 6.2 × 1017 cm−3 (black). Adapted from [821]. b Thermoelectric force of lowly doped n- and p-silicon as a function of temperature. Solid line is from simple model calculation and symbols represent data from silicon samples with the approximate doping of circles: 1 × 1015 cm−3 B, 2 × 1014 cm−3 donors, squares: 4 × 1014 cm−3 P, 9 × 1013 cm−3 acceptors. Adapted from [822]

a thermometer. The Seebeck coefficient is positive if the electric field is in the same direction as the temperature gradient. A famous relation from irreversible thermodynamics connects it to the Peltier coefficient via S=

. T

(8.75)

The Seebeck coefficient is related to the energy transport by charge carriers. The heat (energy) flow is obviously from the hot to the cold end (assuming here T2 > T1 ), so is the flow of charge carriers. In a simple picture, if the energy is carried by (hot) holes, the current (by definition the direction of positive charge carriers) is from the hot to the cold end (2 → 1); if the energy flow is carried by electrons, the current flows from the cold to the hot end (1 → 2). Accordingly, energy transport by electrons and holes gives rise to different signs of the thermoelectric coefficient (Fig. 8.29). If the cold (unheated) substrate is grounded, the sign of the voltage at a hot solder tip pressed (carefully) on the surface of the semiconductor yields the conductivity type, n-type (p-type) for a negative (positive) voltage. However, the semiconductor should not be heated so strongly that intrinsic conduction arises. In this case the conductivity and the thermoelectric power is determined by the carrier type with the higher mobility; typically, and for the case of silicon shown in Fig. 8.29, these are the electrons thus yielding a negative Seebeck coefficient in the intrinsic regime. For band conduction the thermopower (J.29) is given for electrons (Sn ) and holes (Sp ) by [823] (for a derivation see Appendix J.4) k EC − EF + AC Sn = − e kT k EF − EV + AV , Sp = e kT

(8.76a) (8.76b)

where Ai are constants (J.31a) depending on the energy dependence of the density of states and the mobility. The sign of the thermopower tells whether conduction takes place above (negative sign) or below (positive sign) the Fermi level.

8 Transport 0

500

Si

Thermoelectric power S ( V/K)

Thermoelectric power S (mV/K)

254

0 -500 -1000 -1500 -2000 0

10

(a)

20 30 40 Temperature (K)

50

Si

-500

-1000

60

10

(b)

14

10

15

16

17

10 10 ND-NA (cm-3)

10

18

10

19

Fig. 8.30 a Thermoelectric power S of highly doped n-type silicon as a function of temperature. Circles are experimental data and dashed lines guides to the eye. The approximate doping of the samples is white: 2.7 × 1019 cm−3 As, grey: 2.2 × 1018 cm−3 As, black: 1.1 × 1018 cm−3 As and 1.0 × 1018 cm−3 B with ND − ND = 1.25 × 1017 cm−3 at room temperature. Adapted from [822]. b Thermopower of doped n-type silicon at room temperature as a function of doping concentration. Experimental data (symbols) from [822] and theory (solid line) from [824]

If the Fermi level is fixed and both electrons and holes contribute (two-band conduction), the thermopower is (evaluating (J.32), b = σn /σ p and the gap center energy E M = (E C − E V )/2) S=

k e

1 − b Eg EF − EM AV − b AC + + 1 + b 2 kT kT 1+b

.

(8.77)

In the case of intrinsic conduction from (7.18) E F − E M = (kT /2) ln(NV /NC ). The thermoelectric power from some highly doped n-type silicon samples is depicted in Fig. 8.30a. At low temperature the (low) conductivity is due to conduction in a donor impurity band (cmp. Sect. 7.5.7). At high compensation of about 90% (grey data points in Fig. 8.30a), the band is only 10% filled and acts like a valence band with positive thermopower at sufficiently low temperature when the free carrier density is small. Without compensation, the thermopower remains negative since the almost completely filled impurity band acts conduction band like. The dependence of thermopower on doping has been simulated in [824] (Fig. 8.30); the decrease with increasing doping is mostly attributed to the reduced mobility due to ionized impurity scattering. The increase of thermopower at low temperatures is due to the phonon-drag effect which is discussed for the samples from [822] in [825]. As a figure of merit for the production of thermoelectric power the Z T -value is used, Z T = σ S 2 T /κ.

8.14.2 Peltier Effect In a semiconductor with a temperature difference at its ends a current flow will be allowed now (short circuit). The current leads via the charge transport also to a heat (or energy) transport. This effect is called the Peltier effect. The Peltier coefficient is negative (positive) for electrons (holes). The total amount of energy P that is transported consists of the generation term and the loss due to transport: P = j · Eˆ − ∇ · q . With (8.72) and (8.73) we find

(8.78)

8.14 Coupled Heat and Charge Transport Fig. 8.31 Schematic Peltier cooler. The heat sinks (grey) and the cold junction (black) on the left are metals that make ohmic contacts with the semiconductors. The current flow is such that electrons move through the n-type semiconductor from right to left

255 j heat sink

n-type

T

heat sink

p-type j

P=

j·j + S j ·∇T − ∇ · q + κ T . σ

(8.79)

The first term is Joule heating, the second term is Thomson heating. The third exists only when carriers are generated or when they recombine. The fourth term is the heat conduction. In the Thomson term S j ·∇T heat is generated in an n-type semiconductor if j and ∇T are in the same direction. This means that electrons that move from the hotter to the colder part transfer energy to the lattice. The effect can be used to construct a thermoelectric cooler, as shown in Fig. 8.31, that generates a temperature difference due to a current flow. For optimal performance σ should be large to prevent excess Joule heating and κ should be small such that the generated temperature difference is not rapidly equalized.

Chapter 9

Optical Properties

Do not Bodies and Light act mutually upon one another. Sir I. Newton, 1704 [826]

Abstract After introduction of the complex dielectric function, reflection, diffraction are briefly discussed. The focus lies on absorption mechanisms; several transition types (direct and indirect band-band transitions, impurity-related transitions, lattice absorption) are discussed including the effects of excitons, polaritons and high carrier density. Also the various effects of the presence of free carriers are given.

9.1 Spectral Regions and Overview The interaction of semiconductors with light is of decisive importance for photonic and optoelectronic devices as well as for the characterization of semiconductor properties. When light hits a semiconductor, reflection, transmission and absorption are considered, as for any dielectric material. The response of the semiconductor largely depends on the photon energy (or wavelength) of the light and various processes contribute to the dielectric function. An overview of the electromagnetic spectrum in the optical range is given in Table 9.1. The energy and wavelength of a photon are related by1 E = hν = hc/λ, i.e. E [eV] =

1240 . λ [nm]

(9.1)

In the infrared regime, energy is often measured in wave numbers (cm−1 ) for which the conversion 1 meV= 8.056 cm−1 holds.

1 The

more exact numerical value in (9.1) is 1239.84.

© Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_9

257

258

9 Optical Properties

Table 9.1 Spectral ranges with relevance to semiconductor optical properties Range Deep ultraviolet Ultraviolet Visible Near infrared Mid-infrared Far infrared THz region

DUV UV VIS NIR MIR FIR THz

Wavelengths

Energies

80 µm

>5 eV 3–5 eV 1.6–3 eV 0.6–1.6 eV 60 meV–0.6 eV 1.6–60 meV n 1 . The polarization plane is defined by the surface normal and the k-vector of the light (plane of incidence). The parallel (‘p’) polarized wave (TM-wave, electric field vector oscillates in the plane) is shown as ‘↔’; perpendicular (‘s’) polarization (TE-wave, electric field vector is perpendicular to plane) is depicted as ‘·’

262

9 Optical Properties

Fig. 9.4 Reflectance of the GaAs/vacuum interface (close to the band gap, n r = 3.347) for radiation from vacuum/air (left panel) and from the GaAs (right panel), respectively, as a function of incidence angle and polarization

R=

nr − 1 nr + 1

2 .

(9.15)

For GaAs, the reflectance for vertical incidence is 29.2%.

9.4 Absorption In the absorption process, energy is transferred from the electromagnetic field to the semiconductor. In the case of a linear absorption process, when the probability of light absorption is proportional to the incoming intensity, the decrease of intensity in the absorbing medium is exponential (Lambert–Beer’s law [835, 836]),2 I (x) = I (0) exp(−α x) . (9.16) The quantity α is the absorption coefficient, its reverse the absorption depth. The spectral dependence α(E), the absorption spectrum, contains the information of the possible absorption processes, their energy, momentum and angular momentum selection rules, and their oscillator strength. In Fig. 9.5 a schematic absorption spectrum of a semiconductor is depicted. The transition of electrons from the valence to the conduction band begins at the band gap energy. The band gaps of Si, Ge, GaAs, InP, InAs, InSb are in the IR, those of AlAs, GaP, AlP, InN in the VIS, those of GaN and ZnO in the UV, MgO and AlN are in the deep UV. The Coulomb correlation of electrons and holes leads to the formation of excitons that leads to absorption below the band gap. The typical exction binding energy is in the range of 1–100 meV (see Fig. 9.19). Optical transitions from valence-band electrons into donors and from electrons on acceptors into the conduction band lead to band–impurity absorption. In the region from 10–100 meV the interaction with lattice vibrations (phonons) leads to absorption if the phonons are infrared active. Further in the FIR lie transitions from impurities to the 2 In

[836], the absorption coefficient μ was defined via I (d)/I (0) = μd , i.e. μ = exp −α.

9.4 Absorption

263

Fig. 9.5 Schematic absorption spectrum of a typical semiconductor. From [837]

closest band edge (donor to conduction and acceptor to valence band). A continuous background is due to free-carrier absorption. If absorption is considered, the reflectance (9.15) needs to be modified. Using the complex index of refraction n ∗ = n r + iκ, it is given as

∗ 2 2

n − 1 2

= (n r − 1) + κ .

R= ∗ n + 1

(n r + 1)2 + κ2

(9.17)

9.5 Dielectric Function due to Optical Phonons In this section, the dielectric function around the resonance energy of optical phonons is developed. Adjacent atoms oscillate with opposite phase in an optical phonon. If the bond has (partial) ionic character, this leads to a time-dependent polarization and subsequently to a macroscopic electric field. This additional field will influence the phonon frequencies obtained from a purely mechanical approach. We consider in the following the case k ≈ 0. The phonon frequency for TO and LO vibrations is given by ω0 =

2C , Mr

(9.18)

where Mr is the reduced mass of the two different atoms (cf. Sect. 5.2.2). u is the relative displacement u1 − u2 of the two atoms in a diatomic base. When the interaction with the electric field E (which will be calculated self-consistently in the following) is considered, the Hamiltonian for the long-wavelength limit is given by [838]: 1 Hˆ (p, u) = 2

1 2 p + b11 u2 + 2b12 u · E + b22 E2 Mr

.

(9.19)

264

9 Optical Properties

The first term is the kinetic energy (p stands for the momentum of the relative motion of the atoms 1 ˙ the second the potential energy, the third the dipole interaction and the and 2 in the base, p = Mr u), fourth the electric-field energy. The equation of motion for a plane wave u = u0 exp[−i(ωt − k · r)] (u¨ = −ω 2 u) yields Mr ω 2 u = b11 u + b12 E . (9.20) Thus, the electric field is 2 E = (ω 2 − ωTO )

Mr u. b12

(9.21)

2 = b11 /Mr was introduced that is consistent with (9.18) and b11 = 2C. Here, the substitution ωTO ωTO represents the mechanical oscillation frequency of the atoms undisturbed by any electromagnetic effects. Already now the important point is visible. If ω approaches ωTO , the system plus electric field oscillates with the frequency it has without an electric field. Therefore the electric field must be zero. Since the polarization P = ( − 1)0 E is finite, the dielectric constant thus diverges. The polarization is (9.22) P = −∇E Hˆ = − (b12 u + b22 E) .

The displacement field is 2 /Mr b12 E = 0 (ω) E . D = 0 E + P = 0 E − b22 − 2 ωTO − ω 2

(9.23)

Therefore, the dielectric function is (ω) = (∞) +

(0) − (∞) . 1 − (ω/ωTO )2

(9.24)

2 /(b11 0 ) the Here, (∞) = 1 − b22 /0 is the high-frequency dielectric constant and (0) = (∞) + b12 static dielectric constant. The relation (9.24) is shown in Fig. 9.6. From the Maxwell equation ∇ · D = 0 for zero free charge we obtain the relation

0 (ω) ∇ · E = 0 .

(9.25)

Thus, either (ω) = 0 or ∇ · E = 0, i.e. u is perpendicular to k. In the latter case we have a TO phonon and, neglecting retardation effects, using ∇ × E = 0 we find E = 0 and therefore ω = ωTO , justifying our notation. In the case of (ω) = 0, we call the related frequency ωLO and find the so-called Lyddane–Sachs–Teller (LST) relation [839] 2 (0) ωLO . = 2 (∞) ωTO

(9.26)

This relation holds reasonably well for optically isotropic, heteropolar materials with two atoms in the basis, such as NaI and also GaAs. Since at high frequencies, i.e. ω ωTO , only the individual atoms can be polarized, while for low frequencies the atoms can also be polarized against each other, (0) > (∞) and therefore also ωLO > ωTO . For GaAs, the quotient of the two phonon energies is 1.07. Using the LST relation (9.26), we can write for the dielectric function (ω) = (∞)

2 ωLO − ω2 2 ωTO − ω 2

.

(9.27)

9.5 Dielectric Function due to Optical Phonons

265

Fig. 9.6 Dielectric function according to (9.24) with (0) = 3 and (∞) = 2 (without damping). Grey area denotes the region of negative

4 3

(0) ( )

2 1 0 1 2 3 0

1 Frequency ( /

)

2

T

The (long-wavelength) TO-phonon does not create a long-range electric field. Using ∇ · D = 0 and (9.23) and looking at the longitudinal fields, we have 0 E = b12 u + b22 E .

This can be rewritten as E = − ωLO

(9.28)

Mr 0

1 1 − u ∝ −u . (∞) (0)

(9.29)

The (long-wavelength) LO-phonon thus creates a long-range electric field acting against the ion displacement and represents an additional restoring force; this is consistent with the fact that ωLO > ωTO .

9.6 Electron–Photon Interaction The absorption process within the band structure is quantum mechanically described by the coupling of electrons and photons. The process is described with time-dependent perturbation theory. If Hem is the perturbation operator (electromagnetic field), the transition probability per time wfi for electrons from (unperturbed) state ‘i’ (initial) to state ‘f’ (final) is given (with certain approximations) by Fermi’s golden rule 2π

2 Hfi δ(E f − E i − ω) , (9.30) wfi (ω) = where ω is the photon energy, E i (E f ) is the energy of the initial (final) state. Hfi is the matrix element Hfi = f H i , where i (f ) are the wavefunctions of the unperturbed initial (final) state.

(9.31)

266

9 Optical Properties

˙ μH = ∇ × A, ∇ · A = 0 A is the vector potential for the electromagnetic field, i.e. E = −A, (Coulomb gauge). The Hamiltonian of an electron in the electromagnetic field is H=

1 (k − qA)2 . 2m

(9.32)

When terms in A2 are neglected (i.e. two-photon processes), the perturbation Hamiltonian is thus Hem = −

q i q Ap = A·∇ ≈qr·E. m m

(9.33)

The latter approximation is valid for small wavevectors of the electromagnetic wave and is termed the electric dipole approximation. In order to calculate the dielectric function of the semiconductor from its band structure we assume that A is weak and we can apply (9.30). The transition probability R for the photon absorption rate at photon energy ω is then given by3 R(ω) =

2π

|c|Hem |v|2 δ (E c (kc ) − E v (kv ) − ω) d3 kc d3 kv ,

(9.34)

kc kv

with the Bloch functions |c and |v of the conduction and valence band, respectively, as given in (6.40b). The vector potential is written as A = Aˆe with a unit vector eˆ parallel to A. The amplitude is connected to the electric-field amplitude E via A=−

E exp (i(qr − ωt)) + exp (−i(qr − ωt)) . 2ω

(9.35)

In the electric-dipole approximation the momentum conservation q + kv = kc , q being the momentum of the light wave is approximated by kv = kc . The matrix element is then given by |c|Hem |v|2 = with

2 e2 |A|2

c|ˆe · p|v , m2

2

1 c eˆ · p|v = |pcv |2 = Mb2 , 3

(9.36)

(9.37)

and the momentum matrix element pcv given in (6.39). A k-independent matrix element |pcv |2 is often used as an approximation. In Fig. 9.7 the matrix elements for valence to conduction band transitions in GaN are shown as a function of k. In terms of the electric-field amplitude E(ω) the transition probability is

2π e 2

E(ω)

2 2 |p | δ (E c (k) − E v (k) − ω) d3 k . R(ω) = cv mω 2

(9.38)

k

If the integration over k is restricted to those values allowed in unit volume, the power that is lost from the field in unit volume is given by R ω, leaving a 1/E factor. The dielectric function = + i is 3 Here we assume that the valence-band states are filled and the conduction-band states are empty. If the conduction-band states are filled and the valence-band states are empty, the rate is that of stimulated emission.

9.6 Electron–Photon Interaction

GaN

E c

60

20

40

10

20

E||c

C B A

2

|pcv| (eV)

30

267

0 A

L M

A

H K

0 A

L M

A

H K

Fig. 9.7 Theoretical momentum matrix elements | pcv |2 along high-symmetry directions in the Brillouin zone (see Fig. 3.38d) for transitions between valence and conduction bands in GaN and light polarized perpendicular (left panel) and parallel (right panel) to the c-axis. The transitions are A: 9 (A)→ 7c , B: 7 (B)→ 7c , C: 7 (C)→ 7c (see Fig. 6.44). Adapted from [840]

given by 2π e 2 1 = |pcv |2 δ (E c (k) − E v (k) − ω) d3 k 4π0 m ω k 2 e 2 |p |2 1 cv d3 k , = 1 + 2 2 0 m ωcv m ωcv 1 − ω 2 /ωcv

(9.39a)

(9.39b)

k

with ωcv = E c (k) − E v (k). Equation (9.39b) has been obtained via the Kramers–Kronig relations4 (see Appendix C). Comparison with (D.7) yields that the oscillator strength of the band–band absorption is given by f =

2 |pcv |2 e2 e2 = Ncv , 2 m ω 2 0 m ωcv 0 m ωcv cv

(9.40)

with the classical ’number’ of oscillators with the frequency ωcv , Ncv =

2 |pcv |2 . m ωcv

(9.41)

9.7 Band–Band Transitions 9.7.1 Joint Density of States The strength of an allowed optical transitions between valence and conduction bands is proportional to the joint density of states (JDOS) Dj (E cv ) (cf. (6.63), (6.64) and (9.39a))

4 The real and imaginary parts of the dielectric function are generally related to each other via the Kramers–Kronig relations.

268

9 Optical Properties

Table 9.3 Functional dependence of the joint density of states for critical points in 3, 2 and 1 dimensions. E 0 denotes the energy (band separation) at the critical point, C stands for a constant value. The type of critical point is given (min.: minimum, saddle: saddle point, max.: maximum) Dim.

3D

2D

1D

Label

Type

Dj for E < E 0

M0 M1 M2 M3 M0 M1 M2 M0 M1

min. saddle saddle max. min. saddle max. min. max.

0 √ C − E0 − E C √ E0 − E 0 − ln(E 0 − E) C 0 √ E0 − E

Dj (E cv ) = 2 ˜ S( E)

d2 S 1 , 3 (2π/L) |∇k E cv |

Dj for E > E 0 √ E − E0 C √ C − E − E0 0 C − ln(E − E 0 ) 0 √ E − E0 0

(9.42)

where E cv is an abbreviation for E c (k) − E v (k) and d2 S is a surface element of the constant energy surface with E˜ = E cv . The spin is assumed to generate doubly degenerate bands and accounts for the pre-factor 2. Singularities of the JDOS (van-Hove singularities or critical points) appear where ∇k E cv vanishes. This occurs when the gradient for both bands is zero or when both bands are parallel. The latter generates particularly large JDOS because the condition is valid at many points in k-space. Generally, the (three-dimensional) energy dispersion E(k) around a three-dimensional critical point (here developed at k = 0) can be written as E(k) = E(0) +

2 ky2 2 kz2 2 kx2 + + . 2m x 2m y 2m z

(9.43)

The singularities are classified as M0 , M1 , M2 and M3 with the index being the number of masses m i in (9.43) that are negative. M0 (M3 ) describes a minimum (maximum) of the band separation. M1 and M2 are saddle points. For a two-dimensional k-space there exist M0 , M1 and M2 points (minimum, saddle point and maximum, respectively). For a one-dimensional k-space, there exist M0 and M1 points (minimum and maximum, respectively). The functional dependence of the JDOS at the critical points is summarized in Table 9.3. The resulting shape of the dielectric function is visualized in Fig. 9.8.

9.7.2 Direct Transitions Transitions between states at the band edges at the point are possible (Fig. 9.9). The k conservation requires (almost) vertical transitions in the E(k) diagram because the length of the light k vector, k = 2π/λ, is much smaller than the size of the Brillouin zone |k| ≤ π/a0 . The ratio of the lengths of the k vectors is of the order a0 /λ and typically about 10−3 for NIR wavelengths. For isotropic parabolic bands the band-band transition energy versus wavevector relation is 2 E cv (k) = E g + 2

1 1 + ∗ m ∗e mh

k2 .

(9.44)

9.7 Band–Band Transitions

269 r

M0

M1

i

M2

M3

M0

M1

M2

M3

3D

M0

M1

M2

M0

M1

M2

2D

M0

M0

M1

M1

1D

Fig. 9.8 Shape of the real (left panel) and imaginary (right panel) parts of the dielectric function in the vicinity of critical points in 3, 2 and 1 dimensions (for labels see Table 9.3). The dashed line in each graph indicates the energy position of the critical point E 0 . Adapted from [841] Fig. 9.9 a Direct optical transition and b indirect optical transitions between valence and conduction bands. The indirect transition involves a phonon with energy ωph (index a: phonon absorption, e: phonon emission) and wavevector kph

E

E

h h

EC=EV+Eg

EC=EV+Eg h

EV

ph,e ph,a

kph k

EV

k

(b)

(a)

When the energy dependence of the matrix element is neglected, the absorption coefficient is determined by the corresponding square-root joint density of states (M0 critical point): α(E) ∝

E − Eg ≈ ∝ E − Eg . E

(9.45)

The approximation is valid if the considered energy interval, e.g. around a band edge, is small. Absorption spectra of (Inx Ga1−x )2 O3 alloy thin films at room temperature are shown in Fig. 9.10a. The α2 versus photon energy so-called Tauc plot shows a linear dependence with broadening and additional states at the band edge due to disorder effects. The extrapolation of the linear part yields the absorption edge (Fig. 9.10b). Absorption spectra of GaAs are shown in Fig. 9.11a for photon energies close to the band gap at various temperatures. The rapid increase, typical for direct semiconductors, is obvious. In particular at low temperatures, however, the absorption lineshape close to the band gap is dominated by an excitonic feature, discussed in Sect. 9.7.6. Due to the increasing density of states, the absorption increases with the photon energy (Fig. 9.11c). At 1.85 eV there is a step in the absorption spectrum of GaAs due to the beginning of the contribution of transitions between the s-o hole band and the conduction band (see E 0 + 0 transition in Fig. 9.1b).

270

9 Optical Properties

(b)

(a)

Fig. 9.10 a Absorption spectra of (Inx Ga1−x )2 O3 alloy thin films on Al2 O3 , plotted as α2 versus photon energy. b Band edge determined from extrapolation of linear parts

-1

1.2

GaAs

4

1.1 1.0 0.9 0.8 0.7 0.6 1.42

1.44

1.46

1.48

1.50

1.52

1.54

1.56

(a)

4

-1

GaAs

10

E+

0

0

5 E0

0

(b)

1.5

2.0

2.5

(c)

Fig. 9.11 a Absorption of GaAs close to the band gap at different temperatures. Adapted from [842]. b High-resolution absorption spectrum of highly pure GaAs at T = 1.2 K in the exciton region. Dashed line is theory without excitonic correlation. Adapted from [843]. c Absorption spectrum of GaAs at T = 21 K in the vicinity of the band gap. Adapted from [842]

9.7 Band–Band Transitions Fig. 9.12 Optical selection rules for band–band transitions in bulk material for a single photon transitions and b two-photon transitions (with photon energy equal to half the transition energy)

271

mj

mj

3/2 hh

1/2

1/2

1/2 lh

1/2 lh

(a)

electrons

3/2 hh

holes

3/2 hh

1/2

1/2

1/2 lh

1/2 lh

3/2 hh

(b )

When bands run in parallel, i.e. with the same separation, in the E(k) diagram, the absorption processes accumulate at the same transition energy. In this way peaks at higher energy in the complex part of the dielectric function and in the absorption spectrum due to the E 1 or E 0 transitions originate as shown in Fig. 9.1. The selection rules for transitions from valence to conduction band must take into account the angular momentum and spin states of the wavefunctions. The optical transitions for circularly polarized light are shown in Fig. 9.12a, fulfilling the selection rule m j = ±1. A lifting of the energetic degeneracies of these states occurs, e.g. by magnetic fields (cmp. Fig.15.12) or spatial confinement (cmp. Fig. 12.30). For two-photon absorption (Chap.9.7.14), the selection rule is m j = ±2 as shown in Fig. 9.12b [844]. We note that in some materials the direct transition between certain bands is forbidden. An example is SnO2 where the direct transition from the topmost valence band into the lowest conduction band (at ) is forbidden (cmp. Fig. 9.48). If the matrix element increases linearly with E − E g , the absorption coefficient varies like (9.46) α(E) ∝ (E − E g )3/2 .

9.7.3 Indirect Transitions In an indirect band structure the missing k difference (across the Brillouin zone) between valence- and conduction-band state needs to be provided by a second quantum. A phonon can provide the necessary momentum and additionally contributes a small amount of energy ωph . There are several steps in the absorption spectrum due to various involved phonons (or combinations of them). At low temperature (T = 1.6 K, Fig. 9.13) phonons can only be generated and the absorption starts at energies above the band gap. At higher temperatures (typically above 40 K [845], Fig. 9.13), acoustical phonons assisting the optical absorption transition can also be absorbed from the crystal; in this case due to energy conservation the absorption starts already at an energy E g − ωph below the band gap. At even higher temperatures (> 200 K, Fig. 9.13), also optical phonons can be absorbed. The perturbation calculation yields an absorption coefficient with a quadratic dependence on energy (9.47a) [846]. Essentially, for the absorption into a specific (empty) conduction band state (with squareroot density of states) various initial (filled) valence band states (also with square-root density of states) are possible, making the probability depend on the product of the DOS and thus on the energy to the first power. Integrating over all energy states with energy separation E ± ωph , yields an E 2 -dependence.5 5A

flat optical phonon dispersion is assumed.

272 8 (cm-1/2)

GaP

Absorption coefficient

Fig. 9.13√ Absorption edge of GaP ( α versus E) at various temperatures. The index ‘e’ (‘a’) indicates phonon emission (absorption) during the optical absorption process. The theoretical excitonic gap (E gX ) at T = 77 K is indicated. Adapted from [845]

9 Optical Properties

296K 77K

LAe

6 TAe

TOe

1.6K

4 216K TAa 2 (LO+TA)a 0 2.15

2.18

E77K gX

LAa TOa

TAe LAa

2.21

LAe

2.24

TAa

2.27 2.30 Energy (eV)

2.33

2.36

2.39

2.42

Considering the temperature dependent population of the phonon density of states (Bose statistics, (E.3)) the absorption coefficients for transitions with phonon emission (αe ) and phonon absorption (αa ) are: αe (E) ∝

(E − (E g + ωph ))2 1 − exp(−ωph /kT )

(9.47a)

αa (E) ∝

(E − (E g − ωph ))2 . exp(ωph /kT ) − 1

(9.47b)

The two-particle process is less probable than the direct absorption that only involves one photon. The strength of indirect absorption close to the band gap is about 10−3 smaller than for the direct transition. An 11-parameter formula based on terms like (9.47a) can describe the room temperature absorption spectrum of silicon in the visible with a precision of a few percent [847]. The absorption spectra close to√ the absorption edge are shown for GaP (Fig. 9.13) and Si (Fig. 9.14a). According to (9.47a), the plot of α versus energy (Macfarlane–Roberts plot [848]) yields a straight line beyond the spectral region of phonon effects. The complicated form close to the (indirect) gap energy is due to the contribution of different phonons. The phonon energies found to contribute to the silicon absorption edge [849] agree with the TA and TO energy at the X minimum [850] (Fig. 9.14b). Also multiple phonons can contribute (Fig. 9.13). The momentum conservation can also be achieved by impurity scattering or electron-electron scattering [851]. We note also that the indirect semiconductors have an optical transition between valence- and conduction-band states. However, this transition is at higher energies than the fundamental band gap, e.g. for Si (E g = 1.12 eV) at 3.4 eV (see Fig. 6.9a). In Fig. 9.15, the absorption scheme for indirect and direct absorption processes starting with an electron at the top of the valence band is shown together with an experimental absorption spectrum for Ge with the direct transition (8 → 7 ) at 0.89 eV, 0.136 eV above the fundamental band gap. In Fig. 9.16, the absorption edge of BaTiO3 is shown. An indirect transition with an increase of (weak) absorption ∝ E 2 and an indirect gap of E i = 2.66 eV and a direct transition with an increase of (strong) absorption ∝ E 1/2 and a direct gap of E d = 3.05 eV are observed. These transitions could be due to holes at the M (indirect gap) and (direct gap) points (cf. Sect. 6.3.11), respectively.

9.7 Band–Band Transitions

273

(a)

(b)

Fig. 9.14 a Absorption edge of Si at two different temperatures. Adapted from [849]. b Phonon energies in silicon along [001] obtained from neutron scattering (black: unidentified, green: TA, purple: LA, blue: LO, red: TO). The vertical grey bar indicates the position of the conduction band minimum, the horizontal grey bars the energies of the phonons observed at the indirect optical absorption edge. The dark grey overlap areas indicate that TO and TA phonons contribute. Adapted from [850]

-1

E

10

4

10

3

10

2

10

1

10

0

10

-1

10

-2

7

L6

k 8

(a)

L

Ge

0.76 0.78 0.80 0.82 0.84 0.86 0.88 0.90

(b)

Fig. 9.15 a Scheme of indirect and direct optical transitions starting at the top of the valence band in Ge. Vertical solid lines represent the involved photon, the horizontal dashed line the involved phonon. b Experimental absorption spectrum of Ge (T = 20 K). Adapted from [849]

9.7.4 Urbach Tail Instead of the ideal (E − E g )1/2 dependence of the direct band-edge absorption, often an exponential tail is observed (see Fig. 9.17). This tail is called the Urbach tail [853] and follows the functional dependence (for E < E g ) E − Eg , (9.48) α(E) ∝ exp E0 where E 0 is the characteristic width of the absorption edge, the so-called Urbach parameter. The Urbach tail is attributed to transitions between band tails below the band edges. Such tails can originate from disorder of the perfect crystal, e.g. from defects or doping, and the fluctuation of electronic energy bands due to lattice vibrations. The temperature dependence of the Urbach parameter E 0 is thus related to that of the band gap as discussed in [854, 855].

274

9 Optical Properties 1/2

k2

k

-4

10

15

15

10

10

5

5

0 2.5

2.75

3.0

3.25

0 3.0

3.05

3.1

3.15

Fig. 9.16 Absorption of BaTiO3 at room temperature. Experimental data (circles) from [852] with fits (dashed lines) ∝ E 2 and ∝ E 1/2 , respectively 104 -1

GaAs

10

3

10

2

10

1

15

10

GaAs 0

10 1.3

1.4

1.5

1.6

(a)

5 0

1.7

(b)

T

500

1000

Fig. 9.17 a Experimental absorption spectrum (circles) of GaAs at room temperature on a semilogarithmic plot. The exponential tail below the band gap is called the Urbach tail (the dash-dotted line corresponds to E 0 = 10.3 meV in (9.48)). The dashed line is the theoretical dependence from (9.45). Adapted from [856]. b Temperature dependence of Urbach parameter E 0 for two GaAs samples. Experimental data for undoped (solid circles) and Si-doped (n = 2 × 1018 cm−3 , empty circles) GaAs and theoretical fits (solid lines) with one-phonon model. Adapted from [854]

9.7.5 Amorphous Semiconductors The sharp features in the dielectric function due to critical points in the band structure of crystalline semiconductors are washed out in amorphous material. As an example the spectra of the imaginary part of the dielectric function for crystalline (trigonal) and amorphous selenium are shown in Fig. 9.18.

9.7.6 Excitons An electron in the conduction band and a hole in the valence band form a hydrogen-like state due to the mutual Coulomb interaction. Such a state is called an exciton. The center-of-mass motion is separated 2 K2 , where M = m e + m h is the total mass and K is the center-of-mass and has a dispersion E = 2M

9.7 Band–Band Transitions

275

Fig. 9.18 Imaginary part of the dielectric function of amorphous (solid line) and crystalline (trigonal) selenium (dash-dotted lines for two different polarization directions). From [857]

Se

20 trigonal 2nk

15 E||c

10

5

0

amorphous 2

4

6

8

10

b , see Sect. 9.7.10) binding energies in various bulk semiconductors. Values Table 9.4 Exciton (E Xb ) and biexciton (E XX for 10 nm GaAs/15 nm Al0.3 Ga0.7 As quantum well (QW) are taken from [861]

Material

E Xb (meV)

b (meV) E XX

b /E b E XX X

GaAs GaAs QW ZnSe GaN CdS ZnS ZnO

4.2 9.2 17 25 27 37 59

2.0 3.5 5.6 5.4 8.0 15

0.22 0.21 0.22 0.20 0.22 0.25

momentum K = ke + kh .

(9.49)

The relative motion yields hydrogen-like quantized states E n ∝ n −2 (n ≥ 1): E Xn = −

m 0 e4 1 m ∗r 1 , 2 2 m 0 r 2(4π0 ) n 2

(9.50)

where m ∗r denotes the reduced effective mass m ∗−1 = m ∗−1 + m ∗−1 r e h . The third factor is the atomic b −3 Rydberg energy (13.6 eV). The exciton binding energy E X = −E X1 is scaled by (m ∗ /m 0 ) −2 r ≈ 10 . A more detailed theory of excitons beyond the simple hydrogen model presented here, taking into account the valence-band structure, can be found in [858] for direct and [859] for indirect cubic and in [860] for wurtzite semiconductors. The exciton binding energies for various semiconductors are listed in Table 9.4 and shown in Fig. 9.19a versus the band gap. The radius of the exciton is m0 (9.51) rXn = n 2 ∗ r aB , mr where aB = 0.053 nm denotes the hydrogen Bohr radius.6 The Bohr radius of the exciton is aX = rX1 (14.6 nm for GaAs, ∼ 2 nm for ZnO). The exciton moves with the center-of-mass K-vector through 6 Cf.

(7.22); an electron bound to a donor can be considered as an exciton with an infinite hole mass.

276

9 Optical Properties

Fig. 9.19 a Exciton binding energy versus band gap for various semiconductors. b Schematic dispersion of excitonic levels. The K -vector refers to the center-of-mass motion

(b)

1PA (a.u.)

(a)

Cu2O (a)

4 green

(b) 2.030

2.035

2.14

2.15

2.16

2.17

Fig. 9.20 One-photon (top) and two-photon (bottom) absorption spectra of Cu2 O at T = 4.2 K. Arrows denote theoretical peak positions. Adapted from [864]

the crystal. The complete dispersion is (see Fig. 9.19b) E = E g + E Xn +

2 2 K . 2M

(9.52)

The oscillator strength of the exciton states decays ∝ n −3 . The absorption due to excitons is visible in Fig. 9.11a for GaAs at low temperatures. If inhomogeneities are present, typically only the n = 1 transition is seen. However, under special conditions also higher transitions of the exciton Rydberg series are seen (e.g. n = 2 and 3 in Fig. 9.11b). The exciton concept was introduced first for absorption in Cu2 O [862]. The J = 1/2 absorption spectrum (‘yellow series’) is shown in Fig. 9.20. In this particular material both the valence and conduction bands have s character, thus the 1s transition of the exciton is forbidden and the np transitions are observed in normal (one-photon) absorption. With two-photon absorption also the s (and d) transitions can be excited. On a piece of natural Cu2 O, the Rydberg series has been measured up to n = 25 [863] (Fig. 9.21a). The peak energy and the oscillator strength follow the n −2 (E Xb = 92 meV, E g = 2.17208 eV) and n −3 laws, respectively, expected from a hydrogen model (Fig. 9.21b). The deviation from the n −3 -dependence for the oscillator strength at large n is due to interaction effects of excitons with large radius at finite exciton density.

9.7 Band–Band Transitions

277

Oscillator strength (arb. units)

Optical density

En-Eg (meV)

10

Energy (eV)

(a)

(b)

1

10

-4

10

-5

10

-6

10-7 10

-8

2

5

n 10

20

Fig. 9.21 (One photon) Absorption spectrum of Cu2 O (thickness 34 µm) at T = 1.2 K with transitions labelled n = 2 . . . 25. Adapted from [863]

The scattering (unbound) states of the exciton [865] for E > E g contribute to absorption above the band gap. The factor by which the absorption spectrum is changed is called the Sommerfeld factor. For bulk material it is exp(η) , (9.53) S(η) = η sinh(η) with η = π[E bX /(E − E g )]1/2 . The change of the absorption spectrum due to the Coulomb correlation is shown in Fig. 9.22. There is a continuous absorption between the bound and unbound states. At the band gap there is a finite absorption (S(E → E g ) → ∞). The detail to which exciton peaks can be resolved depends on the spectral broadening. In Fig. 9.23 the energy separations of the A-, B-, and C-excitons in GaN are shown [540]. Thus, the ordering of the valence bands depends on the strain state of the semiconductor.

9.7.7 Phonon Broadening The scattering with phonons and the related dephasing leads to homogeneous broadening hom of absorption (and recombination) lines. Acoustic and optical phonons contribute to the broadening according to the dependence [867] hom (T ) = 0 + γAC T + γLO

1 , exp(ωLO /kT ) − 1

(9.54)

where ωLO is the optical phonon energy and the last factor is the Bose function (E.24). 0 is a temperature-independent contribution, 0 = (T = 0). The increasing broadening with increasing temperature is obvious, e.g., in absorption spectra (Fig. 9.24a). In Fig. 9.24b experimental data for GaAs, ZnSe and GaN are assembled. The data have been fitted with (9.54); the resulting phonon

278

9 Optical Properties

(a)

(b)

(c)

(d)

Fig. 9.22 Modification of the absorption edge of a direct transition by excitonic effects for different spectral (Lorentzian) broadening (∝ (E 2 + 2 /4)−1 ), a = 0.01E Xb , b = 0.1E Xb , c = E Xb . d is c in linear scale. Dashed lines are electron–hole plasma absorption according to (9.45) Fig. 9.23 Theoretical dependency (lines) for the the differences of the C-line and A-line as well as B-line and A-line exciton transition energies in GaN as a function of the c-axis strain. Symbols are experimental data from [866]. Adapted from [540]

broadening parameters are listed in Table 9.5.7 The optical transitions in polar semiconductors exhibit stronger coupling to optical phonons. The phonon coupling parameters from different measurements on GaN are discussed and compared in [870].

7 Such parameter can be directly determined from spectroscopic broadening (as in [868]) or a time-resolved measurement of the decay of the coherent polarization (four-wave mixing) as in [869]. In the latter, the decay constant of the dephasing T2 is related to the decay constant τ of the FWM-signal by T2 = 2τ for homogeneous broadening. The Fourier transform of exp −t/(2τ ) is a Lorentzian of the type ∝ ((E − E 0 )2 + 2 /4)−1 with = 1/τ being the FWHM.

9.7 Band–Band Transitions

279

(b)

(a)

Fig. 9.24 a Absorption spectra of GaN bulk (0.38 µm thick epilayer on sapphire) for various temperatures T = 100, 200, 300, 350, 400, 450, and 475 K. Adapted from [868] b Homogeneous broadening as a function of temperature, symbols are experimental data, solid lines are fits, rf. Table 9.5 Table 9.5 Phonon broadening parameters (FWHM) of various bulk semiconductors. Values from fits with (9.54) to experimental data for GaAs [871], ZnSe [869], GaN [868], ZnO [872] (phonon energy fitted) as shown in Fig. 9.25b Material

ωLO (meV)

0 (meV)

γAC (µeV/K)

γLO (meV)

GaAs ZnSe GaN ZnO

36.8 30.5 92 33

0 1.9 10 1.2

4±2 0±7 15 ± 4 32 ± 26

16.8 ± 2 84 ± 8 408 ± 30 96 ± 24

9.7.8 Exciton Polariton Electrons and holes are particles with spin 1/2. Thus, the exciton can form states with total spin S = 0 (para-exciton, singlet) and S = 1 (ortho-exciton, triplet). The exchange interaction leads to a splitting of these states, the singlet being the energetically higher. The singlet state splits into the longitudinal and transverse exciton with respect to the orientation of the polarization carried by the Bloch functions and the center-of-mass motion K of the exciton. Dipole transitions are only possible for singlet excitons (bright excitons). The triplet excitons couple only weakly to the electromagnetic field and are thus also called dark excitons. The coupling of these states to the electromagnetic field creates new quasi-particles, the exciton polaritons [873, 874]. The dielectric function of the exciton (with background dielectric constant b ) is (ω) = b 1 +

β β ∼ 1 + , = b 1 − (ω 2 /ωX )2 1 − (ω 2 /ωT )2 + K 2 /(M ωT )

(9.55)

where β is the oscillator strength and the energy is ωX = ωT + 2 K 2 /2M. ωT is the energy of the transverse exciton at K = 0. With this dispersion the wave dispersion must be fulfilled, i.e. c2 k 2 = ω 2 (ω) ,

(9.56)

where k is the k-vector of the light that needs to be k = K due to momentum conservation. The dependence of the dielectric function on k is called spatial dispersion [875]. Generally, up to terms in k 2 it is written as

280

9 Optical Properties

Table 9.6 Exciton energy (low temperature), LT splitting and exciton polariton oscillator strength for various semiconductors. Values for ZnO from [878], values for GaAs from [879], all other values from [880] ωT LT β

(eV) (meV) (10−3 )

CdS A

CdS B

ZnO A

ZnO B

ZnSe

GaN A

GaN B

GaAs

2.5528 2.2 1.7

2.5681 1.4 1.1

3.3776 1.45 0.9

3.3856 5 3.0

2.8019 1.45 1.0

3.4771 1.06 0.6

3.4816 0.94 0.5

1.5153 0.08 0.11

(ω) = b 1 +

β 2 1 − (ω /ω0 )2 + D k 2

.

(9.57)

The term k 2 with curvature D (for the exciton polariton D = /(M ωT )) plays a role in particular when ωT2 − ω 2 = 0. For k = 0 even a cubic material is anisotropic. The dimensionless curvature Dˆ = Dk 2 should fulfill Dˆ = /(Mc) 1 in order to make k 4 terms unimportant. For exciton polaritons8 typically Dˆ = ωT /(m c2 ) ≈ 2 × 10−5 for ωT = 1 eV and m ∗ = 0.1. From (9.56) together with (9.57) two solutions result: 2ω 2 = c2 k 2 + (1 + β + Dk 2 ) ω02 1/2 ± −4c2 k 2 (1 + Dk 2 ) ω02 + (c2 k 2 + (1 + β + Dk 2 ) ω02 )2 .

(9.58)

The two branches are shown schematically in Fig. 9.25a. Depending on the k value they have a photonic (linear dispersion) or excitonic (quadratic dispersion) character. The anticrossing behavior at k ≈ ωT /c (for ωT = 1 eV, k ≈ 0.5 × 10−5 cm−1 ) creates a bottleneck region in the lower polariton branch. This name stems from the small emission rate of acoustic phonons (i.e. cooling) in that region, as predicted in [876] and experimentally found, e.g. in CdS [877]. The polaritons decay into a photon when they hit the surface. The effect of the oscillator strength of the dispersion is shown in Fig. 9.26 for two-exciton resonance. In the case of several excitons (9.57) reads (ω) = b

1+

n i=1

βi 2 1 − (ω /ω0,i )2 + Di k 2

.

(9.59)

For k = 0 either ω = 0 (lower polariton branch) or (ωL ) = 0. For the latter we find from (9.57) ωL =

1 + β ωT .

(9.60)

Therefore, the energy splitting E LT , mostly denoted as LT , between the L- and T-exciton energy given by 1 + β − 1 ωT ≈ β ωT /2 (9.61) E LT = (ωL − ωT ) = is proportional to the exciton oscillator strength (for experimental values see Table 9.6). We note that if (D.9) is used for the dielectric function, β in (9.61) needs to be replaced by β/b . The effect of spatial dispersion on the reflection at the fundamental exciton resonance is depicted in Fig. 9.25b. For non-normal incidence an additional feature due to the longitudinal wave is observed for p-polarization [875]. For a detailed discussion additional effects due to anisotropy in wurtzite crystals, 8 The dependence of the optical-phonon energies on k is typically too small to make spatial dispersion effects important. According to (5.19) Dˆ = −(a0 ωTO /4c)2 ≈ 4 × 10−11 for typical material parameters (lattice constant a0 = 0.5 nm, TO phonon frequency ωTO = 15 THz).

Energy

9.7 Band–Band Transitions

281

UPB

ELX ETX

LPB

k

(a)

(b)

Fig. 9.25 a Schematic dispersion of exciton polaritons. The lower polariton branch (‘LPB’) is at small k photon-like, at large k exciton-like. The upper branch (‘UPB’) is exciton-like at small k and photon-like at larger k. The limit of the UPB for k → 0 is the energy of the longitudinal exciton. The dashed lines represent the pure exciton dispersions. b Theoretical effect of spatial dispersion on the reflectance at the fundamental exciton resonance at normal incidence for ZnSe material parameters (ωT =2.8 eV, β = 1.0 × 10−3 and a background dielectric constant of b = 8.1, damping was set to = 10−5 ωT ). The arrow denotes the position of ωL . The solid (dashed) line is with (without) spatial dispersion for Dˆ = 0.6 × 10−5 ( Dˆ = 0). Data from [875] 3

3

2

2

2

1

1

1

Energy

3

(a) 0

0

1

2

k

3

4

(b) 5

0

0

1

2

k

3

4

(c) 5

0

0

1

2

k

3

4

5

Fig. 9.26 Schematic polariton dispersion for a two-exciton resonance (curvature of exciton dispersion greatly exaggerated, Dˆ = 10−2 ) at ωT,1 = 1 and ωT,2 = 1.5 for three different oscillator strengths a f = 10−3 , b f = 10−2 , c f = 10−1 . The dashed lines in c represent the pure exciton dispersions

an exciton free layer at the semiconductor surface, additional boundary conditions and damping need to be considered [881, 882]. The polariton dispersions of ZnO and GaN are shown in Fig. 9.27.

9.7.9 Bound-Exciton Absorption Excitons can localize at impurities or inhomogeneities. Such excitons are called bound excitons. Here, the absorption due to such complexes is discussed. The recombination is discussed in Sect. 10.3.2.

282

9 Optical Properties

3.395

ZnO

E||c BL

GaN

5

3.390 BT B 3.380

5

6

AL

5

AT 3.375 A 5

1,2

10

0

5

(a)

20 -1

0

5

10 5

(b)

15

-1

Fig. 9.27 a Exciton polariton dispersion (k ⊥ c) of ZnO with experimental data (T = 1.8 K). Solid (dotted) lines are for polaritons with E c (E ⊥ c). The dashed lines refer to excitons. Adapted from [883]. b Exciton polariton dispersion (T = 2 K) in GaN (on sapphire) for E ⊥ c. Adapted from [884] Table 9.7 Index of nitrogen pairs NNn and energy separation E of bound-exciton transitions from the free-exciton line for n = 1 . . . 10 and the ‘A’ line n

1

2

3

4

5

6

7

8

9

10

∞ (A)

E (meV)

143

138

64

39

31

25

22

20

18

17

11

In GaP:N excitons are bound to isoelectronic N impurities (substituting P), resulting in the ‘A’ line at 2.3171 eV (at T = 4.2 K).9 The absorption due to A excitons is well resolved in the spectrum of Fig. 9.28b. At sufficiently high nitrogen doping, there exist nitrogen pairs, i.e. a complex where a nitrogen impurity has a second nitrogen impurity in the vicinity. The pairs are labeled NNn . It was believed that the second nitrogen atom is in the nth shell around the first one. However, the proper level asignment is probably different in the view of modern theory [544]. Also clusters with more than two nitrogen atoms may exist. NN1 is a prominent level and relates to a N–Ga–N complex having 12 equivalent sites for the second N atom on the next neighbor anion site. The transitions due to excitons bound to NNn , as shown in Fig. 9.28a, give a series of lines (see Table 9.7) that fulfill limn→∞ NNn = A. Although GaP has an indirect band structure, the absorption coefficient of Nrelated transitions is large, about 105 cm−1 for a nitrogen doping level of 1019 cm−3 .10 This is due to the fact that the electron spatially localized at the nitrogen isoelectronic trap (Sect. 7.7.9) has a sizeable k = 0-component of its wave-function (Fig. 7.40), leading to a large transition probability for -point holes with an oscillator strength of 0.09 [885].

9 The A line is due to excitons with J = 1, resulting of coupling of the electron spin 1/2 with the hole angular momentum of 3/2. The B-line is a dipole forbidden line due to ‘dark’ excitons with J = 2. 10 Also the recombination (Sect. 10.3.2) is efficient and allows green GaP:N and yellow GaAsP:N light emitting diodes.

9.7 Band–Band Transitions n=

Transmission

Fig. 9.28 a Transmission spectrum of GaP:N with a nitrogen concentration of about 1019 cm−3 at 1.6 K (thickness: 1.1 mm). n is indicated for the first eight transitions due to excitons bound to nitrogen pairs. NNn ’ indicate phonon replica. The ‘A’ line denotes the position of the transition due to excitons bound to a single nitrogen atom (observable for samples with low N doping). The ‘B’ line is forbidden and due to the J = 2 exciton. Adapted from [694]. b Absorption spectra of N-doped (NN = 7 × 1018 cm−3 ) and intrinsic GaP (T = 2 K). Adapted from [690]

283 12

3

4

5 67 8

NN1' NN1

NN2

GaP:N

NN3 BA

(a)

(b)

9.7.10 Biexcitons Similar to two hydrogen atoms forming a hydrogen molecule, two excitons can also form a bound complex, the biexciton involving two electrons and two holes. The biexciton binding energy is defined as b = 2 E X − E XX . E XX

(9.62)

Biexcitons are binding in bulk material. Accordingly, the biexciton recombination or absorption occurs at lower energy than that of the exciton. Values of the biexciton binding energy are listed in Table 9.4 for various semiconductors. The ratio of biexciton and exciton binding energies is fairly constant about 0.2. In semiconductors with small exciton binding energy, such as GaAs, biexcitons are hard to observe in bulk material but show up in heterostructures that provide additional carrier confinement (see also Sect. 14.4.4). While the exciton density increases linearly with external excitation, the density of biexcitons increases quadratically.

9.7.11 Trions The complexes ‘eeh’ and ‘ehh’ are called trions. Also, the notation X− and X+ is common. X− is typically stable in bulk material but hard to observe. In quantum wells or dots, trions are easier to observe. In quantum dots excitons with higher charge, e.g. X2− , have also been observed (see Fig. 14.45).

284

9 Optical Properties 0

0

Exc (Ry)

-1 Ge Si

-2

-5

-3 CdS CdSe CdTe ZnO

-4

(a)

-10 0

-5 1

rs

2

3

0

1

(b)

2

rs

3

4

5

Fig. 9.29 a Theoretical exchange and correlation energies in units of the exciton Rydberg energy as a function of the dimensionless variable rs for Ge, Si and a model system (with one isotropic conduction and valence band each). The solid line is a fit according to (9.64). Adapted from [886]. b Band gap renormalization in terms of the excitonic Rydberg for various II–VI semiconductors. Solid line is the relation according to (9.64), dashed line is the dependence predicted in [887] for T = 30 K. Data are compiled in [888]

9.7.12 Band Gap Renormalization The band structure theory has been developed so far for small carrier densities. If the carrier density is large the interaction of free carriers has to be considered. The first step was exciton formation. However, at high temperatures (ionization) and at large carrier density (screening) the exciton is not stable. Exchange and correlation energy leads to a decrease of the optical absorption edge that is called band gap renormalization (BGR). An effect due to significant carrier density is to be expected when the density is of the order of the exciton volume, i.e. n ∼ aB−3 . For aB ∼ 15 nm (GaAs) this means n ∼ 3×1017 cm−3 . The dimensionless radius rs is defined via 4π 3 1 r = . (9.63) 3 s n aB3 The sum of exchange and correlation energies E xc is found to be mostly independent of material parameters [886] (Fig. 9.29a) and follows the form E xc =

a + b rs , c + d rs + rs2

(9.64)

with a = −4.8316, b = −5.0879, c = 0.0152 and d = 3.0426. Thus the density dependence of the band gap at small carrier density is ∝ n 1/3 . Experimental data for a number of II–VI semiconductors roughly follow such a dependence (Fig. 9.29b). In Fig. 9.30, a theoretical calculation of the absorption spectrum of bulk GaAs for various carrier densities (n=p) [889] is shown. With increasing density, the excitonic resonance broadens and vanishes. The shape approaches the electron–hole plasma shape. The absorption edge shifts to smaller energies. At high carrier density, the absorption becomes negative in a spectral range before absorption sets in. In this spectral region, the material exhibits gain and an incoming light wave is amplified (cmp. Sect. 10.2.6).

9.7 Band–Band Transitions

285

5

-1

Fig. 9.30 Absorption of GaAs (low temperature, T = 10 K) as a function of the electron–hole density n (theory). Adapted from [889]

1.2

GaAs

1.0 0.8 0.6

n=0 n=5 1015 cm-3 n=3 1016 cm-3 n=8 1016 cm-3

0.4 0.2 0.0 -0.2

c

Tcexp EHG 6

1.500

sp

EHL

5 T (K)

1.495

screw

Ge

exp

7

1.490

4 3 EHL

2

EHL

1 0

(a)

0

0.5

1.0 1.5 2.0 17 -3 (10 cm )

2.5

(b)

Fig. 9.31 a Temperature–density phase diagram of electrons and holes in Ge. The regions of electron–hole gas (EHG) and liquid (EHL) and the droplet phase are labeled. Solid line is theoretical calculation, symbols are experimental data from [892]. The dash-dotted line denoted ρsp is the experimentally obtained temperature dependence of the liquid density exp exp due to single-particle excitations. ρc and Tc denote the experimental critical density and temperature, respectively. Adapted from [893]. b Photographic image of radiative recombination (at 1.75 µm wavelength) from a 300-µm diameter droplet of electron–hole liquid (EHL) in a stressed (001) Ge disk (diameter 4 mm, thickness 1.8 mm) at T = 2 K. The stress is applied from the top by a nylon screw along a 110 direction. Adapted from [894], reprinted with permission, ©1977 APS

9.7.13 Electron–Hole Droplets At low temperature and high density, electron–hole pairs in Ge and Si can undergo a phase transition into a liquid state. This electron–hole liquid (EHL) was suggested in [890] and is a Fermi liquid exhibiting the high conductivity of a metal and the surface and density of a liquid. The condensation is due to exchange interaction and correlation. The formation is fostered by the band structure of Ge [891] and the long lifetime of carriers in the indirect band structure. In unstressed Ge typically a cloud of electron–hole droplets with diameter in the µm range exists. The phase diagram is shown in Fig. 9.31a. In suitably stressed Ge electron–hole droplets with several hundred µm diameter form around the point of maximum shear strain in inhomogeneously strained crystals, as shown in Fig. 9.31b. The pair density in such a liquid is of the order of 1017 cm−3 . We note that the metallic EHL state hinders observation of the Bose–Einstein condensation (BEC) of (bosonic) excitons. The light-exciton mass offers a high condensation temperature in the 1 K range

286

9 Optical Properties

Fig. 9.32 Experimental two-photon absorption spectrum of GaAs (T = 4 K) (dots) plotted as a function of the difference of the double-photon energy 2ω from the GaAs band edge E g . The solid line is a theoretical calculation, the dashed lines represent slopes with exponent 1/2 and 3/2, respectively. Adapted from [901]

10

22

GaAs

1/2

1021

g

3/2

T

g

1020

10

19

10-3

10-2

10-1

1

g

(compared to the mK range for atoms). Recent experiments with spatially indirect excitons in coupled quantum wells lead towards BEC [895, 896]. A sufficiently long lifetime ensures cooling of the excitons close to the lattice temperature. Another potential candidate for BEC are long-living excitons (ms-range) in Cu2 O [897]. The condensation of polaritons (cf. Sect. 9.7.8) in microcavities to welldefined regions of k-space has been discussed in [898] and compared to bosonic condensation in bulk.

9.7.14 Two-Photon Absorption So far, only absorption processes that involve one photon have been considered. The attenuation of the intensity I of a light beam (of frequency ω0 ) along the z direction can be written as dI = −α I − β I 2 , dz

(9.65)

where α is due to the (linear) absorption coefficient (and possibly scattering) and β is the two-photon absorption coefficient. A two-photon process can occur in two steps, e.g. via a midgap level, which is not considered any further here. Here, we consider two-photon absorption (TPA) via the population of a state at 2ω0 higher energy than the initial state with a nonlinear optical process. The TPA coefficient is related to the nonlinear third-order electric dipole susceptibility tensor [899] χi jkl . Within the two-band approximation theory predicts [900] 3/2 . β ∝ 2 ω0 − E g

(9.66)

The exponent 3/2 is indeed found experimentally, as shown in Fig. 9.32 for GaAs. The strength of absorption depends on the relative orientation of the light polarization with respect to the main crystallographic directions, e.g. TPA for polarization along 110 is about 20% larger than for the 100 orientation.

9.8 Impurity Absorption

287

9.8 Impurity Absorption 9.8.1 Shallow Levels For charge carriers bound to shallow impurities long range Coulomb forces are most important and they exhibit a hydrogen-like term scheme En =

m∗ 1 1 × 13.6 eV , m 0 2r n 2

(9.67)

with the ionization limit E ∞ being the conduction (valence) band edge for donors (acceptors), respectively. They can be excited by light to the nearest band edge. Such absorption is typically in the FIR region and can be used for photodetectors in this wavelength regime. The optical absorption cross section of impurity absorption can be related to the carrier capture cross section [588, 589]. The actual transition energies can deviate from (9.67) due to deviation of the potential close to the impurity from the pure Coulomb potential. Such an effect is known as the chemical shift or central cell correction (cf. Sect. 7.5.5) and is characteristic of the particular impurity. In GaAs such shifts are small (∼100 µeV) [902]. The term scheme for P in Si is shown in Fig. 9.33a. The ground state (1s) is split because of a reduction of the tetrahedral symmetry due to intervalley coupling. The anisotropic mass at the X-valley in Si 5p0 4p±

0

±

3p± 4p0

h

...

3p0 2p±

2p0

ph

4p 3p

-45.31

(a)

44.09 43.25 42.41 42.25 40.07 39.14 34.08

11.62

1s(E) 1s(T1)

1.33

2p

1s(A1)

(b)

h

1s

Fig. 9.33 a Term scheme of phosphorus donor in silicon, all energies in meV. After [903]. b Schematic sequence for photothermal ionization, here absorption of a photon with ω = E 3p − E 1s and subsequent absorption of a phonon with energy ωph ≥ E ∞ − E 3p

288

9 Optical Properties

5

4

6

7

Si 2p

GaAs

GaAs

1s-3p0

2p0 Sn Pb 2p

illuminated

ED 3p 4p

0T

2s

1.9T 30

1s-3p

2p

40

dark

3p 3p0 50 -1

(a)

48

60

50

52

54

-1

)

(b)

Fig. 9.34 a Far-infrared photoconductivity response (Lyman-type s→p series) of not intentionally doped GaAs with residual donors Pb, Sn, and Si, NA = 2.6 × 1013 cm−3 , ND − NA = 8 × 1012 cm−3 . The upper (lower) curve is for a magnetic field of 0 (1.9) T. Measurement temperature is 4.2 K. b Photoconductive response of a (different) GaAs sample with the same impurities (ND = 1 × 1013 cm−3 ) with (upper curve) and without (lower curve) illumination with above-bandgap light (B = 1.9 T, T = 4.2 K). Adapted from [905]

causes the p states (and states with higher orbital angular momentum) to split into p0 and p± states. Such an effect is absent in a direct semiconductor with an isotropic conduction-band minimum such as GaAs (Fig. 9.34). Optical transitions between the 1s and various p states can be directly observed in absorption, e.g. for Si:P in [904]. These transitions are also observed in photoconductivity because the missing energy to the ionization into the continuum is supplied by a phonon at finite temperature (photothermal ionization) (Fig. 9.33b) [903]. The splitting of the 2p transition in Fig. 9.34a is the chemical shift due to different donors incorporated in the GaAs (Si, Sn, and Pb). Peak broadening is mostly due to Stark broadening due to neighboring charged impurities. The application of a magnetic field induces Zeeman-like splittings and increases the sharpness of the peaks. The peak width can be b

ED

-1

GaAs:Te

500 ND (cm-3) 2.1 1.0 6.7 1.0

0 0

50

-1

1016 1014 1015 1015

100

Fig. 9.35 Low-temperature (T = 1.35 K) absorption spectra of highly doped n-type GaAs:Te with doping concentrations as labeled (circles: ND = 2.1 × 1016 cm−3 , stars: 6.7 × 1014 , triangles: 1.0 × 1015 ). A sharp photoconductivity spectrum (in arbitrary units) from low-doped GaAs:Te (crosses, ND = 1.0 × 1014 cm−3 ) is shown for comparison (cf. Fig. 9.34a). The energy of the 1s→2p transition and the donor binding energy (onset of continuum absorption) are indicated. Adapted from [906]

9.8 Impurity Absorption

289

further increased by illuminating the sample with light having a higher energy than the band gap. The additional charge carriers neutralize charged impurities and allow higher resolution (Fig. 9.34b). In Fig. 9.35 absorption spectra of highly doped n-type GaAs are shown. For doping concentrations larger than the critical concentration of ∼1×1016 cm−3 (cf. Table 7.6) significant broadening is observed due to the formation of an impurity band.

9.8.2 Deep Levels The absorption of deep levels is typically in the infrared. In Fig. 9.36a the possible optical absorption processes involving the Fe levels in InP (cf. Sect. 7.7.8) during the charge transfer Fe3+ → Fe2+ are shown. These transitions and their fine structure (Fig. 9.36b) have been observed in calorimetric absorption spectroscopy (CAS) experiments [682]. In Fig. 9.37 photoproductivity of Si:Mg is shown. The sharp peaks are due to transitions of interstitial, singly ionized Mg, Mg+ i [907]. Mg in Si is a double donor [653] (see Sect. 7.7.2). Above the ionization limit of about 256 meV, the peaks are replicated, shifted by the LO phonon energy of 59.1 meV. However, now they rather appear as dips. This behavior is typical for a discrete state interacting with a continuum, also called Fano resonance[908, 909] with its characteristic lineshape, going below the continuum level. The absorption spectra due to various deep acceptors in√GaAs are compared in Fig. 9.38. The density of states in the band increases with k (proportional to E − E c ). The carrier on the impurity is strongly localized and described with a wave packet centered around , its k-components decreasing with increasing k. Thus the maximum absorption will be at an intermediate k-value and an associated energy larger than the ionization energy E i (lowest transition to continuum at for k = 0). The lineshapes in Fig. 9.38 fit to a model with a δ-potential (zero range model, neglecting long range Coulomb terms) [910] with maximum absorption close to 2 E i , 1/2

α(E) ∝

Ei

(E − E i )3/2 . E3

1.34

EC 5

InP:Fe

5

InP:Fe

1.14

T2

0.78

E

TA

0.25 (a)

0

(9.68)

Fe

VB

3+

Fe

2+

EV

0.77

5

E

VB

0.78

1.14

5

T2 1.15

(b)

Fig. 9.36 a Schematic band diagram of InP with levels of Fe impurities in the 3+ and 2+ charge states at low temperature. All energies are given in eV. The arrows denote the optical transition of a valence-band electron to the Fe center, Fe3+ + ω → Fe2+ + h. b Calorimetric absorption spectra (at T = 1.3 K) of InP:Fe, [Fe]=5 × 1016 cm−3 . Part b Adapted from [682]

290

9 Optical Properties

Fig. 9.37 Photocurrent spectrum of Si:Mg. Transitions are due to Mg+ i from its 1s state to excited states as labeled and indicated by vertical lines. CB denotes the conduction band edge (ionization limit). Above the CB edge (shaded area) phonon-assisted absorption occurs (Fano resonances). For comparison the absorption spectrum below CB is shown shifted by the phonon energy (dashed line). Above the plot, the transition mechanisms (photothermal ionization and Fano resonance) are schematically shown. Adapted from [907]

GaAs 2 2

Mn Ag

i

-17

1 Cu

Au

0.8 0.6

0.4 1

2

3

4 i

Fig. 9.38 Absorption spectra (σ = α/ p) due to various deep impurities in GaAs as labeled. The dashed line is a theoretical lineshape assuming a hole bound to a δ-potential. The energy axis is scaled by the ionization energy. The kink for Mn at 3.5 E i ≈ 450 meV is due to the onset of absorption into the split-off valence band. Adapted from [314]

9.9 Absorption in the Presence of Free Charge Carriers

291

9.9 Absorption in the Presence of Free Charge Carriers In the presence of charge carriers, various absorption processes can occur. First, the dissipative motion of carriers leads to infrared absorption, termed the free carrier absorption (Sect. 9.9.1). Filling of a band with carriers leads to a shift of the band-band absorption edge, the Burstein-Moss shift (Sect. 9.9.2). Besides the free-carrier absorption, free carriers present in the semiconductor can lead to further absorption processes with transition energies below the band gap. These processes are due to transitions within the band structure and can be • inter-valence band transitions of holes (Sect. 9.9.3), • phonon-assisted inter-valley transitions of electrons (Sect. 9.9.4), • phonon-assisted intra-band transitions of electrons (Sect. 9.9.5).

9.9.1 Absorption Coefficient, Plasma Frequency The absorption due to free carriers in the infrared spectral range (away from phonon resonances) can be described with the Drude model [911]. A time-dependent electric field accelerates the charge carriers within a band. The excess energy is subsequently transferred to the lattice via scattering with phonons. A review of the effect of free carriers on optical properties can be found in [912]. In the relaxation-time approximation energy is relaxed with a time constant τ . Thus energy is absorbed from the electromagnetic wave and dissipated. Effectively, this process represents an intra-band excitation. The complex conductivity (8.37) is given by σ ∗ = σr + iσi =

n e2 τ m∗

1 ωτ +i 2 2 1+ω τ 1 + ω2 τ 2

.

(9.69)

We note that a static magnetic field introduces birefringence as discussed in more detail in Sect. 15.2.2. The wave equation for the electric field is ¨ + σ ∗ μ0 E˙ . ∇ 2 E = r 0 μ0 E

(9.70)

For a plane wave ∝ exp[i(kr − ωt)] the wavevector obeys ω k= c

r + i

σ∗ , 0 ω

(9.71)

where c = (0 μ0 )−1/2 is the velocity of light in vacuum, r is the background dielectric constant (for large ω). The part FC of the dielectric function due to free carriers is FC =

i σ∗ . 0 ω

(9.72)

The complex index of refraction is n∗ = nr + i κ =

r + i

σ∗ . 0 ω

(9.73)

292

9 Optical Properties

Taking the square of this equation yields τ2 σi n e2 = r − ∗ 0 ω 0 m 1 + ω 2 τ 2 n e2 τ σr = 2 nr κ = . 0 ω 0 ω m ∗ 1 + ω 2 τ 2

n 2r − κ2 = r + i

(9.74a) (9.74b)

The absorption coefficient is related to κ by (9.9). For the case of higher frequencies, i.e. ωτ 1, the absorption is 1 n e2 α= ∝ λ2 . (9.75) ∗ 0 c n r m τ ω 2 The absorption decreases with increasing frequency like ω −r . The classical Drude treatment as followed here results in an exponent of r = 2. This is the case for neutral impurity scattering and also for small frequencies ω E F . A more detailed discussion of the energy dependence of free-carrier absorption can be found in [913]. Other exponents have been derived for scattering by acoustical phonons (r = 3/2), LO phonons (r = 5/2) and ionized impurities (r = 7/2). More detailed quantum mechanical treatments of free-carrier absorption in the presence of impurities and phonons can be found in [914–916]. For semiconductors free-carrier absorption is particularly important in the mid- and far-infrared regions when carriers are present due to doping or thermal excitation. In Fig. 9.39a absorption spectra of n-type Ge for various doping concentrations are shown. The absorption coefficient in the transparency regime varies proportionally to λ2 as predicted in (9.75). In Fig. 9.39a, the absorption can be seen to rise for photon energy above 0.7 eV due to absorption in the band structure. Electrons are excited from the valence band across the fundamental band gap into the conduction band (cmp. Sect. 9.7.3), which is an indirect transition in Ge. In Fig. 9.39b the absorption coefficient due to free carrier absorption at fixed wavelength is shown as a function of dopant concentration.11 The slope is slightly overlinear, indicating a weak dependence τ (n). A sub-linear relation has been found for heavily p-doped GaAs [917]. The index of refraction is given by (also for ωτ 1) n 2r

ω 2 2r ωp 4 1 ne2 p 2 1 − + = r − + κ = r 0 m ∗ ω 2 ω 4n 2r ω ω2 τ 2 ω 2 p , ≈ r 1 − ω

(9.76)

where ωp =

n e2 r 0 m ∗

(9.77)

is the plasma frequency. The approximation is valid for small absorption and when (ωτ )−2 can be neglected. A graphical representation is given in Fig. 9.40a. For coupling to electromagnetic waves (still ωτ 1) ω 2 c2 k 2 p = 2 (ω) = r 1 − (9.78) ω ω must be fulfilled. It follows that the dispersion relation in the presence of free carriers (Fig. 9.40b) is 11 Even

at low temperature, n ≈ ND since ND Nc (cf. [594] and Sect. 7.5.7).

9.9 Absorption in the Presence of Free Charge Carriers

(a)

293

(b)

Fig. 9.39 a Optical absorption spectra (at T = 4.2 K) of n-type Ge for various As dopant concentrations as labeled. The arrow denotes the band edge of undoped Ge, the vertical dashed line the energy for which the free-carrier absorption is measured in part b. The inclined dashed line visualizes the slope ∝ λ2 . Curved dashed lines are guides to the eye. Adapted from [851]. b Free-carrier absorption at λ = 2.4 µm as determined from part a of the figure (blue squares) as a function of As dopant concentration. Additionally data at 300 K (red circles) from the same samples are included [851]. The dashed lines visualizes the slope ∝ ND1.25 Fig. 9.40 a Dielectric constant for plasmon oscillations. Shaded area represents region of attenuation (negative ). b Dispersion relation (k in units of ωp /c, ω in units of ωp ) in the presence of free carriers (9.79, for r = 1). Shaded area represents forbidden frequency range for propagating solutions. Dashed line is photon dispersion ω = ck

2

1

0

1 -1

-2

(a)

0

1

ω 2 = ωp2 +

/

p

c2 k 2 . r

2

(b)

0 0

1

k

2

(9.79)

For ω > ωp , > 0, thus waves can propagate. For ω < ωp , however, the dielectric constant is negative, i.e. < 0. For such frequencies waves are exponentially damped and cannot propagate or penetrate a layer. This effect can be used in a plasmon waveguide or in metamaterials (cf. Sect. 19.1.10). The expected dependence of the plasmon wavelength on the carrier density λp = 2πc/ωp ∝ n −1/2 is depicted in Fig. 9.41 for GaAs. For semiconductors the plasmon frequency is in the mid-or far-infrared spectral region.12

12 The much higher free-electron density in metals shifts the plasma frequency to the UV, explaining the reflectivity of metals in the visible and their UV transparency.

294

9 Optical Properties

Fig. 9.41 Plasma wavelength λp for n-type GaAs with various electron concentrations due to different doping levels. Filled circles: experimental values, dashed line: n −1/2 dependence; the deviation is due to nonparabolicity of the electron mass (cf. Fig. 9.53b). Data from [918]

Fig. 9.42 Burstein–Moss effect at InSb (E g = 0.18 eV) at room temperature. Theoretical dependence and data points for intrinsic InSb and 5 × 1018 cm−3 n-type. Data from [919]

1

InSb 1.0 0.8

1.5

0.6

2

0.4

3 4 7

0.2

Eg

gap

1017

1018

1019 -3

9.9.2 Burstein–Moss Shift In the discussion so far it has been assumed that all target states in the conduction band are empty. In the presence of free carriers the absorption is modified by the • change of the distribution function • many-body effects (band gap renormalization). The latter is discussed in the next section. For a degenerate electron distribution all states close to the conduction-band edge are populated. Thus a transition from the valence band cannot take place into such states. This shift of the absorption edge to higher energies is called the Burstein–Moss shift [919, 920]. Originally, the Burstein–Moss shift was evoked to explain the absorption shift in InSb with varying carrier concentration (Fig. 9.42). k-conserving optical transitions between parabolic hole and electron bands have the dependence E = Eg +

2 k 2 2 k 2 2 k 2 + = Eg + , 2 me 2 mh 2 mr

(9.80)

where m r is the reduced mass of electron and hole. About 4kT below the Fermi level all levels in the conduction band are populated (Fig. 9.43). Thus the k value at which the absorption starts is given as kˆ =

2 me (E F − E C − 4kT ) . 2

(9.81)

9.9 Absorption in the Presence of Free Charge Carriers

295 E

Fig. 9.43 Principle of Burstein–Moss shift. Left panel: Schematic band structure with completely filled electron states shown in grey. The k-vector for the lowest photon energy optical absorption process ˆ Right is indicated as k. panel: Electron distribution function for a degenerate electron gas with Fermi level in the conduction band

E

EF EF-4kT EC

EV

k

fe

k

Besides the energy shift in the conduction band, the corresponding energy shift in the valence band kˆ 2 /(2m h ) must be considered. Thus, the Burstein–Moss shift of the absorption edge is me E = ω − E g = (E F − 4kT − E C ) 1 + . mh

(9.82)

The relation between n and the Fermi level is given by (7.6). If E F − E C kT the Fermi integral can −EC 3/2 be approximated by √2π 23 EFkT . Using (7.8) for NC , the Burstein–Moss shift can be written for this case as 2 2/3 3 me h 2 2/3 2/3 h 1+ ≈ 0.97 E = n n . (9.83) 8 me π mh 8 mr The n 2/3 dependence of the energy shift is found, e.g., for CdO13 with different carrier concentrations (due to different deposition temperature, no intentional doping) [921] and depicted in Fig. 9.44a. Similar behavior is found for ITO (indium-tin-oxide) thin films, deposited at different sputtering conditions, leading to different carrier concentrations (9.44b).

9.9.3 Inter-Valenceband Transitions Transitions within the valence band can occur between three bands, i.e. lh→hh, so→hh, and so→lh, as schematically depicted in Fig. 9.45. Theoretical treatments have been given in [923, 924]. For GaAs, such intravalence-band absorption occurs at photon energies close to 0 as shown in Fig. 9.46a for p-type GaAs:Zn [925]. For p-type GaSb, the absorption coefficient below the fundamental band gap is found almost entirely due to inter-valence band transitions, as shown in Fig. 9.46b for a hole concentration of p = 3.2 × 1016 cm−3 [926].

13 CdO is an indirect semiconductor, the optical band gap is the energy of the direct transition at the -point, typically obtained from extrapolation in the α2 versus energy plot. The indirect transitions involve holes from other points in the Brillouin zone (cmp. Fig. 6.13).

296

9 Optical Properties

(a)

(b)

Fig. 9.44 a Burstein–Moss effect in CdO. The linear fit is for E g = 2.22(8) eV and m r = 0.113(11) m e . The dashed lines indicate the confidence interval of ±0.08 eV. Adapted from [921]. b Burstein–Moss effect in ITO (indium-tin-oxide) versus the ’optical’ carrier density determined from the position of the plasma edge. The dashed line is guide to the eye. Data from [922]

E EV

EV

k

lh

hh

0

so

Fig. 9.45 Schematic optical transitions within the valence band

400 -1

-1

GaAs:Zn

p-GaSb

200 100 60 40 0

20 10

(a)

0.1

0.2

0.3

0.4

0.5

0.6

(b)

Fig. 9.46 a Optical absorption spectrum of GaAs:Zn with p = 2.7 × 1017 cm−3 at T = 84 K. The absorption above the split-off energy 0 is due to the hh/lh → s-o process. Adapted from [925]. a Optical absorption coefficient of GaSb with p = 3.2 × 1016 cm−3 . Experimental data (solid line) and calculation of inter-valence band contribution (squares). The free carrier contribution is less than 5 cm−1 in the considered spectral range. Adapted from [926]

9.9 Absorption in the Presence of Free Charge Carriers

297 10

2

n-InP -1

E

10

1

10

0

E 10-1

10

k

(a)

X

-2

0.2 0.4 0.6 0.8 1.0 1.2 1.4

(b)

Fig. 9.47 a Schematic of inter-valley conduction band transitions involving a photon (solid line arrow) and a phonon (dashed line arrow). b Optical absorption coefficient of InP with n = 1.65 × 1018 cm−3 . Experimental data (solid line) and calculation of inter-valley band contribution (dashed line). The extrapolated free carrier contribution is shown as dash-dotted line and the difference of experimental absorption and extrapolated free carrier contribution as circles. Adapted from [927]

9.9.4 Inter-Valley Transitions Electrons at the conduction band minimum can undergo optical transitions to the same band at a different point of the Brillouin zone. Such intervalley transition, as sketched in Fig. 9.47a, is phononassisted to fulfill momentum conservation and occurs around the energy difference E between the two valleys (cmp. Table 8.4). For InP with an electron concentration of n = 1.65 × 1018 cm−3 , below the fundamental band edge at 1.4 eV, an additional contribution starting around 0.8–0.9 eV is found besides the free carrier absorption (Fig. 9.47b) [927]. Taking into account the filling of the bottom of the conduction band, an energy separation for the two valleys of E = 0.90 ± 0.02 eV was found for various values of the electron concentrations. This energy corresponds to the energy difference of conduction band minima at and X in InP. The lineshape of this absorption processes can be modeled and fits well the difference of measured absorption and extrapolated free-carrier absorption spectra. Transitions to the lower minimum at L (E = 0.6 eV) are not observed, possibly masked by the free-carrier absorption.

9.9.5 Intra-Band Transitions Phonon-assisted transitions within the lowest conduction band (not to a different valley), as indicated schematically in Fig. 9.48a for the SnO2 band structure [928], can cause absorption at photon energies below the fundamental absorption edge. Actually in SnO2 , the optical transition across the fundamental band gap is only weakly dipole-allowed and leads to small absorption coefficient below 100 cm−1 directly above the fundamental band gap of about 3.6 eV. The strong dipole-allowed transition with absorption coefficient around 105 cm−1 begins at about 4.3 eV and stems from electrons in a lower valence band [929]. The free-carrier absorption due to transitions within the lowest conduction band are calculated to dominate below 2.8 eV (Fig. 9.48b) and thus can also impact transparency in the visible spectral range. The calculated slope is close to α ∝ λ3 (cmp. (9.75)), expected from the linear dispersion of the conduction band away from the -point [928]. A similar effect with the contribution

298

9 Optical Properties

9 SnO 2 2

(10 cm )

SnO2

-18

6 3 0

(a)

-3

X

Z

(b)

W

Fig. 9.48 a Band structure of SnO2 and indirect intra-band absorption process; the transition from the topmost valence band (dashed arrow) is forbidden. b Calculated free-carrier absorption(σ = α/n) for SnO2 . The solid and dashed lines are results including phonon-assisted transitions for two light polarizations. The dotted lines are fits of the Drude model to the infrared regime. Adapted from [928] Fig. 9.49 Calculated room temperature absorption coefficient Ga2 O3 as a function of energy (for light polarized along the z direction) for undoped/intrinsic material and three different electron concentrations as labelled. Adapted from [930]

of inter-band and intra-band transitions leading to absorption within the band gap transparency regime has been calculated for Ga2 O3 as shown in Fig. 9.49 for various doping levels [930].

9.10 Lattice Absorption Due to the lack of a dipole moment of the optical phonons, no first order interaction of optical phonons and (infrared) light exists in the diamond structure for Si and Ge due to crystal structure symmetry [931]. However, higher order processes contribute to lattice absorption in these materials [932, 933]. E.g., two-photon bands are due to a dipole moment that is of second order in the nuclear displacement. Strong absorption effects are present for compound semiconductors. A review can be found in [934].

9.10.1 Dielectric Constant The (relative) dielectric constant (with damping parameter ) in the vicinity of the optical phonon energies is given by (cf. (9.27))

9.10 Lattice Absorption

299

Fig. 9.50 Lattice absorption oscillator strength f from (9.86) for various elemental, III–V and II–VI semiconductors as a function of their ionicity f i (cf. Table 2.1). Dashed line is linear dependence on ionicity for similar (reduced) mass, dash-dotted lines are guides to the eye for similar ionicity and varying mass

(ω) = (∞)

2 − ω 2 − iω ωTO 2 ωTO − ω 2 − iω

.

(9.84)

The dispersion relation (without damping) can be rewritten as (0) − (∞) f (ω) = (∞) + . = (∞) 1 + 1 − (ω/ωTO )2 1 − (ω/ωTO )2

(9.85)

Thus the dimensionless oscillator strength (compare with (D.10)) is f = ((0)/(∞) − 1. With the LST relation (9.26) the oscillator strength is f =

ω2 − ω2 (0) − (∞) ωLO − ωTO = LO 2 TO ≈ 2 , (∞) ωTO ωTO

(9.86)

and thus proportional to the splitting LT = ωLO − ωTO between the longitudinal and transverse optical phonon frequency. The approximation in (9.86) is valid for LT ωTO . The oscillator strength increases with the ionicity, i.e. the electronegativity difference of the atoms in the base (Fig. 9.50). Additionally, the oscillator strength depends on the reduced mass and the highfrequency polarizability; this can be seen, e.g., for the series of the Zn compounds that all have similar ionicity. For the series of the nitrides, the mass effect is small since the reduced mass is dominated by the light N mass. We refer to Fig. 5.23 for the change of phonon oscillator strength in an (Al,Ga)N alloy.

9.10.2 Reststrahlenbande The absorption of electromagnetic radiation by optical phonons is governed by the dielectric function that has been derived in (9.84). For small damping, i.e. LT , the dielectric constant is negative between ωTO and ωLO . From r = n 2r − κ2 it follows that κ2 is much larger than n 2r . Therefore,

300

9 Optical Properties

GaAs

0

25

50

75

Fig. 9.51 Far-infrared absorption (linear scale) of GaAs. In the region around 35 meV is the reststrahlenbande with high absorption due to optical phonons. The sharp little peak at 45 meV is a LVM, probably from AlGa . Adapted from [935]

the reflectance (9.17) will be close to 1. This energy range is the so-called reststrahlenbande. This term stems from multiple reflections in this wavelength regime that suppresses neighboring spectral regions and thus achieves a certain monochromatization in the far-infrared spectral region. Within the semiconductor the absorption is large in the reststrahlenbande (Fig. 9.51).

9.10.3 Polaritons The coupled propagation of phonons and electromagnetic radiation is (without phonon damping) related to the dielectric function given in (9.27), (ω) = (∞)

2 − ω2 ωLO 2 ωTO − ω2

c2 k 2 . ω2

(9.87)

2 2 2 2 1 c2 k 2 2 c k ωTO 2 ωLO + − . 4 (∞) (∞)

(9.88)

=

There are two branches of propagating waves (real k): 1 c2 k 2 2 ωLO ± + ω = 2 (∞)

2

√ For k = 0 we √ find the solutions ω = ωLO and ω = k c/ (0). For large k we find ω = ωTO and ω = k c/ (∞). These solutions are shown in Fig. 9.52. Both branches have a phonon- and a photon-like part. The coupled state between the phonon and the photon field is called the (phonon-) polariton. ˜ For this case In the interval [ωTO , ωLO ] the wavevector is purely imaginary, i.e. k = ik˜ with real k. there is only one solution that is also depicted in Fig. 9.52, ! 2 2 2 ˜2 !1 2 k˜ 2 2 k˜ 2 ω 2 c k 1 c c TO 2 2 ω2 = + + + . ωLO +" ωLO 2 (∞) 4 (∞) (∞)

(9.89)

9.10.4 Phonon–Plasmon Coupling The coupling of phonons and plasmons in the spectral region of the reststrahlenbande leads to the development of two new branches, the longitudinal phonon plasmon modes (LPP+ and LPP−), in the

9.10 Lattice Absorption

301

Fig. 9.52 Dispersion of the polariton. The dotted line displays the dispersion for a purely imaginary wavevector with the absolute value k

(a)

(b)

Fig. 9.53 a Frequency of the coupled longitudinal-phonon plasmon (LPP) modes (lower (upper) polariton branch in blue (red)) as a function of the plasma frequency. Dashed line shows uncoupled plasmon frequency (ω = ωp ), grey area indicates spectral region between TO√ and LO modes. b Experimental data on the polariton energies in n-type GaAs with different carrier concentration ωp ∝ n m ∗ (9.77). Dashed (dash-dotted) line is plasmon frequency ωp without (with) consideration of conduction band non-parabolicity (cf. Fig. 6.37b). Data from [918, 936]

common dispersion. The dielectric function is

ωp2 ω2 − ω2 (ω) = (∞) 1 + LO − 2 ω2 ωTO − ω2

.

(9.90)

For (ω) = 0 for k = 0 (coupling to photons) the two solutions ωLPP+ and ωLPP− do not cross as a function of ωp (Fig. 9.53), ωLPP± =

# 1 2 2 2 ωLO + ωp2 ± (ωLO + ωp2 )2 − 4 ωTO ωp2 . 2

(9.91)

For small plasma frequencies ωLPP+ = ωLO , i.e. the optical phonons couple to the electromagnetic field without change. Also ωLPP− = ωp . For large carrier density, i.e. ωp ωLO , we find ωLPP− = ωTO and ωLPP+ = ωp . Thus, the carriers have effectively screened the electric field of the phonon that had led to the increase of the TO to the LO frequency.

Chapter 10

Recombination

Les hommes discutent, la nature agit. Men argue, nature acts. Voltaire

Abstract The various mechanisms and statistics of carrier recombination in semiconductors including band-band, excitonic, band-impurity (Shockley-Read-Hall kinetics) and Auger recombination are explained. Also recombination at extended defects and surfaces is treated. Using the diffusionrecombination theory, the one-dimensional carrier profiles for typical situations in experiments and devices are derived.

10.1 Introduction In thermodynamic nonequilibrium excess charges can be present in the semiconductor. They can be created by carrier injection through contacts, an electron beam or the absorption of light with wavelength smaller than the band gap. After the external excitation is turned off, the semiconductor will return to the equilibrium state. The relaxation of carriers into energetically lower states (and energy release) is called recombination. The term stems from the electron recombining with the hole created after absorption of a photon. However, there are other recombination mechanisms. A dedicated textbook is [937]. In the simplest picture an excitation generates carriers with a rate G (carriers per unit volume and unit time). In the steady state (after all turn-on effects) a constant excess charge n carrier density is present. Then the generation exactly compensates the recombination processes. The principle of detailed balance even says that each microscopic process is balanced by its reverse process. If the time constant of the latter is τ , n is given by n = G τ . This follows from the steady-state solution n˙ = 0 of n dn =G− . dt τ

(10.1)

In the literature two limiting cases have been discussed, the relaxation and the lifetime semiconductor, depending on the relation of two time constants. The one time constant τ0 is the relaxation time constant due to recombination as discussed in the following. The smaller τ0 is, the faster excited electrons and holes recombine and ‘disappear’. Fast lifetimes are typically present in direct semiconductors (compared to indirect ones), semiconductors with high defect density and amorphous semiconductors. © Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_10

303

304

10 Recombination

Fig. 10.1 Processes of band–band recombination: a spontaneous emission, b absorption and c stimulated emission. A full (empty) circle represents an occupied (unoccupied) electron state

Ec Eg

E=h

E=h

E=h

E=h E=h

Ev

(a)

(b)

(c)

The other time constant is τD = /σ, the dielectric relaxation time; it describes the transport of carriers due to mobility (and diffusion). Large dielectric relaxation times are present in semiconductors with high mobility (low defect density, small carrier mass), small τD typically for hopping conduction. The relaxation case is given for τ0 τD ; carriers will recombine quickly and it is hard to build up non-equilibrium carriers and separate them with an applied electric field. In the recombination case τD τ0 , non-equilibrium carriers can assume non-uniform distributions and an applied electrical field generates separate quasi-Fermi levels for electrons and holes.1 (cmp. Sect. 7.6).

10.2 Band–Band Recombination The band–band recombination is the relaxation from an electron in the conduction band into the valence (the empty state there is the hole). In a direct semiconductor, electrons can make an optical transition between the bottom of the conduction band to the top of the valence band. In an indirect semiconductor, this process is only possible with the assistance of a phonon and is thus much less probable.

10.2.1 Spontaneous Emission We consider the spontaneous recombination of an electron of energy E e and a hole of energy E h (Fig. 10.1a). C(E e , E h ) is a constant proportional to the matrix element of the optical transition (cf. Sect. 9.6). The spontaneous recombination rate rsp at photon energy E ≥ E C − E V = E g is (assuming energy conservation, i.e. E = E e − E h , but without k-conservation in a dense plasma [938]), ∞ rsp (E) =

EV dE e

EC

dE h C(E e , E h ) ×

−∞

De (E e ) f e (E e ) Dh (E h ) f h (E h ) δ(E − E e + E h ) E+E V = dE e C(E e , E e − E) × EC

De (E e ) f e (E e ) Dh (E e − E) f h (E e − E) , where f h denotes the hole occupation f h = 1 − f e . 1 In

the relaxation case, the separation of quasi-Fermi levels is kT .

(10.2)

10.2 Band–Band Recombination

305

5

GaAs

4 3

E= 46meV

2 Eg= 1.423eV

1

(a)

0 1.35

1.40

1.45

1.50

1.55

(b)

Fig. 10.2 a Photoluminescence spectrum of an undoped LPE-grown epitaxial GaAs layer at room temperature and low cw (λ = 647 nm) excitation density (10 W/cm2 ). The solid line is a lineshape fit with (10.3) and E g =1.423 eV and T = 293 K. (b) Room temperature, direct (e –h ) recombination from heavily n-doped (1019 cm−3 ) germanium (1 µm thick Ge layer on silicon (001)) with biaxial (thermal) tensile strain. The strain-split valence band edge (Fig. 6.50) causes the e–hh and e–lh transitions (individual contributions with lineshape according to (10.3) shown as dashed lines) to occur at different energies. Adapted from [939] 0.08

Fig. 10.3 Carrier temperature TC in GaAs as a function of excitation density at a lattice temperature of 1.6 K. The dashed line is guide to the eye, the solid line corresponds to an activation energy of 33 meV, similar to the GaAs optical phonon energy. Adapted from [940]

GaAs

0.07

15

20

0.05 0.04

TC (K)

1/TC (K-1)

0.06

0.03 0.02 0.01 -4 10

40

n-type p-type -3

-2

-1

10 10 10 Excitation density (arb. units)

1

100

The lineshape of the band–band recombination with k-conservation2 is proportional to the joint density of states (9.42) and the Fermi distribution function. At small excitation and at low doping it can be approximated by the Boltzmann distribution function and the lineshape is given as I (E) ∝

E . E − E g exp − kT

(10.3)

An experimental spectrum is shown in Fig. 10.2 together with a fit according to (10.3). The expected FWHM of the peak is 1.7954 kT , which is about 46 meV at T = 300 K. At low sample temperature, the temperature of the carrier gas is typically higher than the lattice temperature, depending on the cooling mechanisms (carrier–carrier scattering, optical phonon emission, acoustic phonon emission, recombination, . . .) and the excitation rate. The carrier temperature in GaAs, determined from the Boltzmann tail of spontaneous emission (photoluminescence) is depicted in Fig. 10.3 as a function of excitation density; clearly it increases with increasing excitation. The recombination rate in indirect semiconductors is small since the transition is phonon-assisted. For silicon, an internal quantum efficiency in the 10−6 -range has been reported [941]. For germanium, 2 Excitonic

effects are neglected here, e.g. for temperatures kT E Xb . Such effects are discussed in Sect. 10.3.

306

10 Recombination

the direct transition is energetically fairly close to the fundamental, indirect L– band edge transition (Fig. 9.15). The energy difference can be reduced from its bulk value of 136 meV by tensile strain. Additionally, the direct transition can be favored by heavily n-doping and filling the L conduction band minimum states (see Sect. 9.9.2). In this case, direct recombination from the conduction band -minimum can be observed [939] and the effective energy difference has been lowered to about 100 meV.

10.2.2 Absorption A similar consideration is made for the absorption process (Fig. 10.1b). An electron is transferred upon light absorption from a valence-band state (occupied) to a conduction-band state that must be empty. The coefficient is B1 . Also, the process is proportional to the light intensity, represented by the density of occupied photon states Nph (E), E+E V

rabs (E) =

dE e B1 (E e , E e − E) ×

(10.4)

EC

De (E e ) (1 − f e (E e )) Dh (E e − E) (1 − f h (E e − E)) Nph (E) .

10.2.3 Stimulated Emission In this case, an incoming photon ‘triggers’ the transition of an electron in the conduction band into an empty state in the valence band. The emitted photon is in phase with the initial photon (Fig. 10.1c). The rate is (with coefficient B2 ): E+E V

rst (E) =

dE e B2 (E e , E e − E) ×

(10.5)

EC

De (E e ) f n (E e ) Dh (E e − E) f h (E e − E) Nph (E) . The photon density Nph at a given energy is given by Planck’s law and the Bose–Einstein distribution (Appendix E) 1 . (10.6) Nph (E) = N0 exp (E/kT ) − 1 The pre-factor is the density of states of the electromagnetic field3 N0 (E) = 8 π E 2 (n r / hc)3 .

10.2.4 Net Recombination Rate In thermodynamical equilibrium the rates fulfill 3 The total number of photon states in vacuum between the frequencies zero and ν

is N (ν) = 8πν 3 /(3c3 ). With ν = E/ h and N0 = dN (E)/dE and considering c → c/n r we obtain the given value for N0 .

10.2 Band–Band Recombination

307

rsp (E) + rst (E) = rabs (E) .

(10.7)

Since for absorption and stimulated emission the same quantum-mechanical matrix element is responsible, B1 = B2 . If the population functions are Fermi-Dirac distributions with quasi-Fermi levels Fn and Fp (Sect. 7.6), the detailed balance (10.7) yields E − (Fn − Fp ) −1 . C(E 1 , E 2 ) = B1 (E 1 , E 2 ) Nph exp kT

(10.8)

In thermodynamic equilibrium, i.e. Fn = Fp , C(E 1 , E 2 ) = N0 B1 (E 1 , E 2 ) = B .

(10.9)

If the constant B, the bimolecular recombination coefficient, is independent of the energy E, the integration for the net bimolecular recombination rate rB can be executed analytically and we find ∞ rB =

rsp (E) + rst (E) − rabs (E) dE

(10.10)

Eg

Fn − Fp . = B n p 1 − exp − kT In thermodynamic equilibrium, of course, rB = 0. The recombination rate Bnp is then equal to the thermal generation rate G th G th = B n 0 p0 . (10.11) The bimolecular recombination rate typically used in Shockley–Read–Hall (SRH) [942, 943] kinetics is rB = B (n p − n 0 p0 ) .

(10.12)

Values for the coefficient B are given in Table 10.1. In the case of carrier injection, np is larger than in thermodynamical equilibrium, i.e. n p > n 0 p0 , and the recombination rate is positive, i.e. light is emitted. If the carrier density is smaller than in thermodynamical equilibrium, e.g.. in a depletion region, absorption is larger than emission. This effect is also known as ‘negative luminescence’ [944] and plays a role particularly at elevated temperatures and in the infrared spectral region. Table 10.1 Bimolecular recombination coefficient at room temperature for a number of semiconductors. Data for GaN from [945], Si from [946], SiC from [947], other values from [948] Material

B (cm3 /s)

GaN GaAs AlAs InP InAs 4H-SiC Si GaP

1.1 ×10−8 1.0 ×10−10 7.5 ×10−11 6.0 ×10−11 2.1 ×10−11 1.5 ×10−12 1.1 ×10−14 3.0 ×10−15

308

10 Recombination

10.2.5 Recombination Dynamics The carrier densities n and p, are decomposed into the densities n 0 and p0 in thermodynamic equilibrium and the excess-carrier densities δn and δ p, respectively n = n 0 + δn

(10.13a)

p = p0 + δ p .

(10.13b)

Here, only neutral excitations are considered, i.e. δn = δ p. Obviously the time derivative fulfills ∂n = ∂∂tδn , and correspondingly for the hole density. The equation for the dynamics ∂t n˙ = p˙ = −Bnp + G th = −B (n p − n 0 p0 ) = −B (n p − n 2i )

(10.14)

∂ δp = −B (n 0 δ p + p0 δn + δn δ p) . ∂t

(10.15)

can be written as

The general solution of (10.15) is given by δ p(t) =

(n 0 + p0 ) δ p(0) . [n 0 + p0 + δ p(0)] exp [B t (n 0 + p0 )] − δ p(0)

(10.16)

In the following, we discuss some approximate solutions of (10.15). First, we treat the case of a small (neutral) excitation, i.e. δn = δ p n 0 , p0 . The dynamic equation is in this case ∂ δp = −B (n 0 + p0 ) δ p . ∂t

(10.17)

Then the decay of the excess-carrier density is exponential with a time constant (lifetime) τ given by τ=

1 . B (n 0 + p0 )

(10.18)

In an n-type semiconductor additionally n 0 p0 , and thus the minority carrier lifetime τ p is τp =

1 . B n0

(10.19)

If the nonequilibrium carrier densities are large, i.e. n ≈ p n 0 , p0 , e.g. for strong injection, the kinetics obeys ∂ δp = −B (δ p)2 , (10.20) ∂t and the transient has the form δ p(t) =

δ p(0) , 1 + B t δ p(0)

(10.21)

where δ p(0) is the excess hole density at time t = 0. Such a decay is called hyperbolic and the recombination is bimolecular. The exponential decay time is formally τ −1 = Bδ p(t) and is thus time and density dependent. A detailed discussion of minority carrier lifetime is given in [949].

10.2 Band–Band Recombination

309

10.2.6 Lasing The net rate for stimulated emission and absorption is E − (Fn − Fp ) rst (E) − rabs (E) = 1 − exp kT

(10.22)

E+E V

×

dE e B De (E e ) f e (E e ) Dh (E e − E) f h (E e − E) Nph (E) . EC

The net rate at photon energy E = ω is only larger than zero (i.e. dominating stimulated emission) when (10.23) Fn − Fp > E ≥ E g . When the difference of the quasi-Fermi levels is larger than the band gap, the carrier population is inverted, i.e. close to the band edges the conduction-band states are more strongly populated with electrons than the valence-band states, as shown in Fig. 10.4. An incoming optical wave of energy E will then be net amplified by stimulated emission. Equation (10.23) is also called the thermodynamic laser condition. We note that lasing requires further conditions as discussed in Sect. 23.4.

10.3 Exciton Recombination 10.3.1 Free Excitons The observation of free-excitons is limited for semiconductors with a small exciton binding energies (such as in GaAs) to low temperatures. However, for large exciton binding energy, recombination from free-excitons is observed even at room temperature, as shown in Fig. 10.5 for ZnO.

Fig. 10.4 Charge-carrier distribution during inversion, necessary for lasing. Shaded areas are populated with electrons. A stimulated transition between an electron and a hole is indicated

E

Fn EC

EV Fp

D(E)

310

10 Recombination

PL Intensity (arb. units)

ZnO

1

D0,X

3.20

3.25 3.30 Energy (eV)

3.35

XA

3.40

Fig. 10.5 Temperature-dependent luminescence spectra of a ZnO thin film (on sapphire). At low temperatures, the spectra are dominated by donor-bound exciton transitions (Al0 ,X)). The vertical dashed line indicates the low-temperature position of the donor-bound exciton transition (D0 ,X). The curved dashed line visualizes the energy position of the free-exciton transition (XA ) that becomes dominant at room temperature

Fig. 10.6 Low temperature recombination spectra from silicon with low (solid lines) and sizeable (dashed line) phosphorus dopant concentration. Spectrum for NP = 2 × 1014 cm−3 (NP = 8 × 1016 cm−3 ) taken at 26 K (15 K). Transitions in pure Si are label with ‘I’, transitions involving P donors are labeled with ‘P’. Q indicates the dissociation energy of the bound exciton. Adapted from [950]

A low temperature recombination spectrum of silicon is shown in Fig. 10.6. In pure silicon, phononassisted exciton recombination (cmp. Sect. 10.4) is observed involving acoustic (ITA ) and optical (ITO ) phonons. The weakly observed no-phonon line (I0 ) is forbidden in perfect Si.

10.3.2 Bound Excitons Excitons can localize at impurities, defects or other potential fluctuations and subsequently recombine [951, 952]. Excitons can be bound to neutral or ionized donors and acceptors impurities [953]. Also

10.3 Exciton Recombination

311

20

Si In

15

10

Bi As Ga P Sb Al B

5

0

(a)

0

50 ED

150 100 b (meV)

200

(b)

Fig. 10.7 Energy Q required to remove an exciton from a neutral impurity (10.24) as a function of the ionization energy E Db (open circles) or E Ab (solid circles) of the involved impurity in (a) silicon (experimental data from [965]) and (b) ZnO (experimental data from [966])

they can be bound to isoelectronic impurities, the most prominent example being N in GaP [954] (cmp. Sect. 9.7.9) or isoelectronic clusters [955]. The recombination of excitons localized in quantum wells (Sect. 12.4) and quantum dots (Sect. 14.4.4) is discussed later. The transition energy ω of an exciton bound to a neutral impurity is ω = E g − E X b − Q ,

(10.24)

where Q is the binding (or localization) energy of the exciton to the impurity. The binding energy of an exciton to an ionized impurity is denoted with Q ∗ . A transition involving an exciton bound to a neutral donor is denoted (D0 ,X); correspondingly (D+ ,X), also denoted as (h,D0 ), and (A0 ,X). Values for donor-bound excitons in various semiconductors are listed in Table 10.2. The (D0 ,X) complex is stable for 0 < σ = m ∗e /m ∗h < 0.43 according to [956]. The (D+ ,X) peak can occur on the low- or high-energy side of the (D0 ,X) recombination. Whether Q ∗ < Q or Q ∗ > Q depends on σ being smaller or larger than 0.2, respectively [956], and is fulfilled for many semiconductors, e.g. GaAs, GaN, CdS, and ZnSe. Recombination in silicon due to excitons involving phosphorus donors is depicted in Fig. 10.6. The (D0 ,X) transition in Si:P is labeled ‘P0 ’ (Q = 6 meV). Other P-related transitions are discussed in [950]. In Si, the binding energy to the impurity is about one tenth of the binding energy of the impurity (Haynes’s rule [951, 965]), i.e. Q/E Db and Q/E Ab ≈ 0.1 (Fig. 10.7a). In GaP the approximate relations Q = 0.26E Db − 7 meV and Q = 0.056E Ab + 3 meV have been found [954]. For donors in ZnO, the relation Q = 0.365E Db − 3.8 meV holds (Fig. 10.7b) [966]. In Fig. 10.8, the recombination spectrum of GaAs:C is shown that exhibits recombination from excitons bound to the acceptor (carbon) and shallow donors. The exciton is more strongly bound to an ionized donor (D+ ) than to a neutral donor. Varying the concentration of a specific impurity and observing the corresponding change in the intensity of the (D0 ,X) transition allows to identify the chemical species to which the exciton is bound. This can be achieved via the comparison of different samples or more elegantly by introducing radioactive isotopes. This is shown in Fig. 10.9 for In in ZnO; the (111 In0 ,X) transition disappears with the characteristic time constant close to that (97 h) of the nuclear decay of 111 In into stable 111 Cd. However, in such experiments it should be considered that the decay product and accompanying highenergy radiation can create new electronic and structural defects, respectively. The peak labeled (D0 ,X)2s in Fig. 10.8 is called a two-electron satellite (TES) [968]. High-resolution spectra of the TES in GaAs [581, 969] are shown in Fig. 10.10a. The TES recombination is a (D0 ,X)

312

10 Recombination

Table 10.2 Localization energy Q (Q ∗ ) of excitons on selected impurities (ionized impurities, D+ or A− , respectively) in various semiconductors. σ is the ratio of effective electron and hole (polaron) masses. EMD: effective mass donor host GaAs GaN AlN CdS ZnSe

ZnO

donor

Q (meV)

Q ∗ (meV)

Q ∗ /Q

EMD Zn EMD Mg

0.88 8.1 6.8 20

1.8 31.1 11.2

2.0 3.8 1.6

Si Mg EMD Al Ga In Al Ga In

16 40 6.6 4.9 5.1 5.4 15.5 16.1 19.2

σ

Ref.

0.28

[957]

0.36

[959] [960]

3.8 5.4 6.6 7.5 3.4 4.1 8.5

0.6 1.1 1.3 1.4 0.21 0.25 0.44

0.17

[961]

0.27

[962, 963]

0.3

[964]

0

(A ,X)

GaAs:CAs

(h,D0) (D0,X) (e,A0)

0

(D ,A0)

0

(D0,X)2s

(h,D2s) 20

1.49

1.50

1.51

1.52

Fig. 10.8 Photoluminescence spectrum (T = 2 K, D = 10 mW cm−2 ) of GaAs:CAs (NA = 1014 cm−3 ) with donorand acceptor-related bound-exciton recombination around 1.512 eV, (e,A0 ), (h,D0 ) and (D0 ,A0 ) pair and free-exciton recombination. Adapted from [957]

recombination that leaves the donor in an excited state as schematically shown in Fig. 10.10b. Therefore a hydrogen-like series with n = 2, 3, . . . is observed with energies n E TES

=E

(D0 ,X)

−

E Db

1 1− 2 . n

(10.25)

The effect of isotope disorder on the sharpness and splitting of impurity states has been investigated in [970, 971]. The recombination of excitons bound to Al, Ga and In in natural silicon (92.23% 28 Si, 4.67% 29 Si, 3.10% 30 Si) is split into three lines due to the valley-orbit splitting [972] of electron states at the band minimum (Fig. 10.11). Each of these (A0 ,X) lines is split by 0.01 cm−1 for Si:Al due to a symmetry reduction of the 4-fold degenerate A0 ground state, as observed in the presence of applied axial strain or an electric field. The comparison to spectra from enriched 28 Si shows that the observed splitting without external perturbation is due to isotope disorder that causes random strains and splits the A0 ground state into two doublets [971] (Fig. 10.11). Similarly, the (unsplit) phosphorus-induced

10.3 Exciton Recombination

313

Fig. 10.9 a Low-temperature photoluminescence spectrum of ZnO implanted with 111 In featuring the so-called I9 -line. Spectra are recorded at various times after implantation as labeled. b Intensity of I9 -line as a function of time. Adapted from [967] (D0,X)

TES

D

exc.

EC

20 4

ED

40

0

X

D* n=3 n=2 n=1

1

1.510

(a)

0

1.515

(b) EV

Fig. 10.10 a Photoluminescence spectrum (T = 1.5 K, D = 50 mW cm−2 ) of high-purity GaAs with two donors (Ge and Se/Sn). The lower spectrum has been excited 6 meV above the band gap, the upper spectrum has been resonantly excited with the laser set to the (D0 ,X) transition and exhibits n = 2, 3, 4, and 5 TES transitions. α,β,γ denote excited (hole rotational) states of the (D0 ,X) complex. Adapted from [969]. b Schematic representation of the n = 2 TES process, left: initial, right: final state

(D0 ,X) transition in enriched Si is found to be much sharper (< 40 µeV) than in natural Si (330 µeV) [970]. At higher resolution, a hyperfine splitting of 485 neV due to the 31 P nuclear spin I = 1/2 (2 × 1012 cm−3 ) in isotopically pure (99.991%) 28 Si (I = 0) is observed for the (P0 ,X) recombination [973]. In a magnetic field, the Zeeman-split lines have a FWHM of about 150 neV. In Fig. 10.12 the recombination of excitons bound to the N isoelectronic impurity in lowly doped GaP is shown. The efficient recombination of nitrogen-bound electrons with holes at the point is due to the wave-function component of the localized electron at k = 0 [690] (Fig. 7.40). The decay time of the A exciton is about 40 ns [974] and thus larger than the typical lifetime of excitons in direct semiconductors (ns-range). The forbidden B exciton has a much longer lifetime of 4 µs [974]. In the case of In in GaAs it has been found that down to the regime of NIn < 1019 cm−3 the indium does not act as a substitutional isoelectronic impurity but still fully participates in the composition

314

10 Recombination

Si:Al 0

AX

A

0

natural Si 28

Si

1.1508

1.1509

1.1510

Fig. 10.11 High-resolution photoluminescence (PL) spectra of (A0 ,X) recombination in natural and 28 Si-enriched silicon doped with aluminum (T = 1.8 K). The 28 Si PL spectrum is shifted up in energy by 0.114 meV, as indicated by the arrow, to compensate for the shift in band gap. The inset shows a level scheme for the recombination in natural silicon. Adapted from [971], reprinted with permission, ©(2002) APS Fig. 10.12 Photoluminescence spectrum (T = 4.2 K) of GaP:N (NN ≈ 5 × 1016 cm−3 ). The A exciton is bound to an isolated nitrogen impurity, cmp. to Fig. 9.28. Adapted from [690]

Fig. 10.13 Spectral position of neutral donorand acceptor-bound exciton photoluminescence transition (T = 2 K) in GaAs doped with different amounts of indium relative to the donor-bound exciton luminescence in pure GaAs (1.5146 eV). Adapted from [975]

of a pseudo-binary system (Sect. 6.5). Recombination from excitons bound to single indium atoms or In–In pairs could not be found. The energy shift of donor- and acceptor-bound excitons in the dilute limit (Fig. 10.13) follows the band-gap dependence established for larger indium concentrations. The non-occurrence of localization effects is attributed to the small effective electron mass in InAs [544].

10.3 Exciton Recombination

315

Fig. 10.14 (Temperature dependent PL intensity of (D0 ,X) in GaN and (A0,X) in AlN:Mg recombination. Solid lines are fits with (10.26). Data from [960, 978]

The luminescence intensity I (T ) of bound exciton lines is quenched with increasing temperature due to ionization of the excitons from the impurities. The temperature dependence can be modeled using the relation [976] 1 I (T ) = , (10.26) I (T = 0) 1 + C exp(−E A /kT ) E A being the thermal activation energy and C a pre-factor. Often the activation energy is found equal to the localization energy, E A = Q (Fig. 10.14, cmp. Table 10.2). If several processes contribute, additional exponential terms can be added with further activation energies. For acceptor-bound excitons in GaAs two processes are found to contribute, the ionization from the impurity into a free exciton (E A1 ≈ Q) and into an electron-hole pair (E A2 ≈ Q + E Xb ) [976]. In [977] the model is refined by considering the temperature dependence of the parameter C due to the ionization of the impurity itself. So far single excitons bound to a center have been discussed. Also bound exciton complexes [979] containing up to six excitons have been observed at sufficient excitation density, e.g. for substitutional boron [980] or phosphorus [981] and interstitial Li [982] in silicon. In a multi-valley semiconductor several electrons are available to form bound excitons which follow approximately a shell model and exhibit further fine structure.

10.3.3 Alloy Broadening The bound-exciton recombination peak in a binary compound is spectrally fairly sharp (Sect. 10.3.2), even in the presence of isotope disorder (Fig. 10.11). In an alloy (see Sect. 3.7), the random distribution of atoms (with different atomic order number Z ) causes a significant broadening effect of the luminescence (and absorption) line, the so-called alloy broadening [983, 984]. As an example, we treat Alx Ga1−x As. The exciton samples, at different positions of the lattice, different coordinations of Ga and Al atoms. If the experiment averages over these configurations, an inhomogeneously broadened line is observed. The cation cc for the zincblende lattice is given as cc = 4/a03 , for the wurtzite lattice √ concentration 2 as cc = 4/( 3 a c). For example, cc = 2.2 × 1022 cm−3 for Alx Ga1−x As in the entire composition range 0 ≤ x ≤ 1 since the lattice constant does not vary significantly, and cc = 4.2 × 1022 cm−3 for wurtzite Mgx Zn1−x O [985]. In a random alloy, the probability p(N ) to find exactly N Ga atoms in a given volume V (with a total of cc V cations) is given by the binomial distribution

316

10 Recombination

(b)

(a)

Fig. 10.15 a Spectral width of the photoluminescence from CdSx Se1−x alloys. Solid line is theory according to (10.30). Adapted from [983]. (b) Spectral width of the bound exciton recombination in Alx Ga1−x As with various Al content within the direct-bandgap regime. Solid line is (10.30) with (10.28), dashed line with pre-factor 4π/3 instead of 10 π. Adapted from [987]

p(N ) =

cc V x N (1 − x)cc V −N . N

(10.27)

The sampling volume for a luminescence event is the exciton volume (cf. (9.51)) that is given for the free-exciton (in 1s hydrogen state) as [983, 986] Vex = 10 π aX3 = 10 π

m0 s aB m ∗r

3 .

(10.28)

One should note that due to the variation of the involved material parameters Vex depends itself on x. In GaAs there are about 1.2 × 106 cations in the exciton volume. In Alx Ga1−x As, there are on average xcc Vex Al atoms in the exciton volume. The fluctuation is given by the standard deviation of the binomial distribution [986] x (1 − x) σx2 = . (10.29) cc Vex The corresponding energetic broadening (full width at half-maximum) of the spectral line is given by E = 2.36 σ with

∂ E g x (1 − x) ∂ Eg σx = . (10.30) σ= ∂x ∂x cc Vex We note that instead of the quantum mechanically correct factor 10 π [983, 986], often the factor 4π/3 [984] is used, resulting in larger theoretical broadening. Experimental data for Cdx Se1−x in Fig. 10.15a are consistent with (10.30). The theoretical dependence (10.30) is shown in Fig. 10.15b also for Alx Ga1−x As together with experimental data and found to disagree [987]. Since the exciton volume is much smaller (cf. Sect. 9.7.6) than in Alx Ga1−x As, alloy broadening in Mgx Zn1−x O is much larger for a given for given x. The spectral broadening due to alloy disorder masks the fine structure of recombination lines near the band edge present for binary semiconductors. Often for all temperatures only a single recombination line appears for alloys. Spectra for three different Mgx Zn1−x O alloys are shown in Fig. 10.16a. The increasing inhomogeneous broadening is obvious, causing a single peak for x > 0.03. The temperature dependence of the peak positions is shown in Fig. 10.17 for the same samples. For x = 0.005 the bound exciton (Al-donor) (D0 ,X) and free exciton (XA ) recombination lines can still be resolved despite

10.3 Exciton Recombination

(a)

317

(b)

Fig. 10.16 a Photoluminescence spectra (T = 80 K, scaled) of three Mgx Zn1−x O alloy layers on sapphire with three different Mg-contents, x = 0.005, x = 0.03, and x = 0.06 as labeled. The energy positions of (D0 ,X) and XA peaks are marked. Adapted from [977]. b Peak energy of the photoluminescence spectrum (T = 2 K) of ZnO (I6 -line, star) and various Mgx Zn1−x O alloys (circles). For x ≤ 0.03 (filled circles) the (D0 ,X) recombination peak (Al donor) can be spectrally separated from the free exciton (XA ) recombination. For the samples with higher Mg content (empty circles) a single recombination peak is present at all temperatures. The dashed line is a linear least square fit for the alloys with 0 ≤ x ≤ 0.03, showing that also for x > 0.03 the low temperature recombination peak is due to donor-bound excitons. Adapted from [988]

Fig. 10.17 Temperature dependence of the shift of energy position of (D0 ,X) and XA photoluminescence peak in Mgx Zn1−x O alloys with three different Mg-contents, (a) x = 0.005, (b) x = 0.03, (c) x = 0.06. The energy positions are given relative to the low temperature position of the respective (D0 ,X) peaks. Adapted from [977]

the inhomogeneous broadening of σ = 2.6 meV. At low temperature the luminescence intensity is dominated by (D0 ,X) recombination, at room temperature by free exciton (XA ) recombination. Both peaks are present at low temperatures and exhibit a red-shift with increasing temperatures due to the shrinking of the band gap (Fig. 10.17a). The (D0 ,X) peak vanishes at about 180 K due to ionization of the excitons from the donors (Q ≈ 15 meV, similar as in pure ZnO). For larger Mg-content of x = 0.03 the two peaks can still mostly be separated (σ = 6.0 meV). The (D0 ,X) energy position shows a small dip (about 2 meV) due to exciton localization in the alloy

318 Fig. 10.18 Schematic representation of 1 LO exciton scattering of an exciton at K = 0 to an intermediate state with K ≈ 0 and subsequent radiative decay. ω represents the phonon energy and E 1 the energy of the emitted photon

10 Recombination

E

n=3 n=2 n=1

continuum

h

ph

E1

K

disorder potential (arrow in Fig. 10.17b). At low temperatures excitons are frozen in local potential minima and have a non-thermal (non-Boltzmann) population. With increasing temperature they can overcome energy barriers and thermalize, leading to a shift of the recombination peak to lower energies. Further increase of temperature populates higher levels and leads to a shift of the recombination peak to higher energies. Superimposed is the red-shift due to the band gap shrinkage. This so-called “S”-shape effect of E(T ) is discussed in Sect. 12.4 in detail with regard to exciton localization in a quantum well disorder potential. For x = 0.06 only a single photoluminescence peak is observed for the alloy (σ = 8.5 meV). The (D0 ,X) peak is the dominant for the Mgx Zn1−x O alloys at low temperatures even in the presence of large alloy broadening (Fig. 10.16(b)). The peak changes its nature from (D0 ,X) at low temperatures to XA at room temperature. In between, first exciton thermalization (red-shift) in the disorder potential and subsequently exciton ionization from the donors (blue-shift, arrow in Fig. 10.17c) are observed [977]. Such exciton ionization from impurities has also been observed for (Al,Ga)N:Si [628, 989].

10.4 Phonon Replica The momentum selection rule for free-exciton recombination allows only excitons with K ≈ 0 (for K, cf. (9.49)) to recombine. The fine structure of this recombination is connected to polariton effects (cf. Sect. 9.7.8). Excitons with large K can recombine if a phonon or several phonons are involved [990] that provide the necessary momentum q = K1 − K2 , with K1 (K2 ) being the wavevector of the initial (intermediate) exciton state (Fig. 10.18). A so-called zero-phonon line at energy E 0 is then accompanied by phonon replica below E 0 at integer multiples (at low temperature) of the (LO) phonon energy ωph E n = E 0 − n ωph . (10.31) Phonon replicas have been observed in many polar semiconductors such as CdS [991] and ZnSe [992]. A sequence of such phonon replica, as observed in GaN [993], is depicted in Fig. 10.19a. The lineshape of the n-th phonon-assisted line is proportional to the exciton population at a given excess energy, which is proportional to the density of states and the Boltzmann distribution function [994] E ex wn (E ex ) . (10.32) In (E ex ) ∝ E ex exp − kT

10.4 Phonon Replica

10

0

319

GaN 1LO

10

-1

10

-2

10

-3

2LO

5LO

4LO

92meV

3.1

(a)

3LO

3.2

3.3

3.4

3.5

(b)

Fig. 10.19 a Photoluminescence spectrum of GaN (grown on SiC substrate) at T = 50 K. In addition to emission from free (FE) and bound (BE) excitons several phonon replica (labeled as 1LO–5LO) are observed. Vertical dashed lines indicate energy positions of multiple LO-phonon energies (ωLO = 92 meV) below the FE peak. Adapted from [993]. b Photoluminescence spectrum of 1 LO phonon-assisted recombination peak at T = 103 K (from the data of Fig. 10.5). Data points (dots) and lineshape fit (solid line) according to (10.32) with the parameters L 1 = 0.9 and E 1 = 3.2955 eV (and background)

Here, E ex represents the exciton kinetic energy. The factor wn (E ex ) accounts for the q-dependence of the matrix element. It is typically expressed as Ln . wn (E ex ) ∝ E ex

(10.33)

Accordingly, as temperature dependent refinement of (10.31), the energy separation E n of the energy of the peak maximum of phonon replica from E 0 is given by

1 E n = E n − E 0 = −n ωph + L n + kT . 2

(10.34)

It is found theoretically that L 1 = 1 and L 2 =0 [994]. These relations are approximately fulfilled for GaN [995]. A lineshape fit for the 1 LO phonon-assisted transition in ZnO is shown in Fig. 10.19b. In Fig. 10.20a the ‘green band’ emission of ZnO is shown as presented in [996]. This band is mostly attributed to a Cu impurity; recently, evidence has grown from isotope decay and annealing studies that it is related to the zinc vacancy [997] (Fig. 10.20b). The zero phonon line is followed by many replica with a maximum at about 6 LO phonons. The intensity I N of the N -th replica is given by [998, 999] I N ∝ exp(−S)

SN , N!

(10.35)

where S is the so-called Huang–Rhys parameter. In [997], a coupling parameter of S = 6.9 has been determined. Equation (10.35) is obtained from the consideration of transitions in the configuration diagram [998, 1000] (Fig. 10.21), using the Born–Oppenheimer approximation. Here the electronic wavefunctions are separated from the vibrational wavefunctions, leading to the Franck–Condon principle, that optical transitions occur with the positions of the nuclei fixed and thus vertical in the configuration diagram Fig. 10.21. Assuming low temperatures, only the lowest state is (partially) occupied. The Huang–Rhys parameter, the average number of phonons involved in the transition, is related to the displacement δq = q1 − q0 of the two configurations

320

10 Recombination

650

600

550

ZnO

-7

500 -6 -5

-8

450 -4 -3

-9

-2 -1 2.0

2.2

2.4

2.6

2.8

(b)

(a)

Fig. 10.20 a Luminescence spectrum of ZnO in the visible. The arrow denotes the zero-phonon line at 2.8590 eV. The numbers of the phonon replica are labeled. Adapted from [996]. b Luminescence spectra (solid lines) of a ZnO bulk crystal before (‘untreated’) and after annealing in O2 atmosphere at T = 1073 K. After annealing in Zn atmosphere at the same temperature, the green band disappears again (dashed line). From [997]

S=

C δq 2 , 2 ωph

(10.36)

where C is the ‘spring constant’ of the parabola, C = d2 E/dq 2 . For small S 1, we are in the weak coupling regime and the zero-phonon line is the strongest. In the strong coupling regime, S > 1, the maximum is (red-) shifted from the zero-phonon line. We note that in absorption, phonon replica occur on the high-energy side of the zero-phonon absorption. For large S the peak intensities are close to a Gaussian. The correspondence of emission and absorption is nicely seen for excitons on isoelectronic oxygen traps in ZnTe [1001]. The oxygen is on substitutional Te site. Up to seven phonon replica are visible in Fig. 10.22 around the zero-phonon or A-line with a

E S= 0

Sh E1

1

E

h

2 4 8

E0 (a)

absorption

emission

q0 q1

q

ZPL

(b)

E

Fig. 10.21 a Configuration diagram of two states that differ in their configuration coordinate by δq = q1 − q0 . Both are coupled to phonons of energy ω. The absorption maximum (solid vertical line) and emission maximum (dashed vertical line) are shifted with respect to the zero-phonon line (dotted vertical line) with energy E 1 − E 0 . The Huang–Rhys parameter is S ∼ 4. (b) Intensity of zero-phonon line (‘ZPL’) and phonon replica (10.35) for emission and absorption processes with different values of the Huang–Rhys parameter S as labeled

10.5 Self-Absorption

321

Fig. 10.22 Photoluminescence (solid line) and absorption (dashed line) spectra of excitons bound to substitutional oxygen in ZnTe at T = 20 K. The energy position is relative to the A-line at 1.9860 eV. The vertical dashed lines have a separation of 25.9 meV. Adapted from [1001]

separation of about 26 meV, the optical phonon energy in ZnTe. The Huang-Rhys parameter is about 3–4. Other peaks are due to acoustic phonons.

10.5 Self-Absorption Luminescence that is emitted within the semiconductor can be (re-)absorbed before it may reach the surface and can leave the crystal. This effect is called self-absorption. It is particularly strong for radiation with an energy where the absorption α(ω) is high, i.e. above the band gap of a direct semiconductor. Similarly to the penetration depth 1/α for radiation entering the crystal, emission approximately occurs only from a layer of such thickness. For typical values of α in the range of 105 cm−1 , the ‘skin’ of the semiconductor that emits light with energy above the band gap is 100 nm. For light at the low energy side of the band gap or with energy within the band gap (deep levels), the emission depth can be much larger. After re-absorption, the energy has another chance to relax non-radiatively, thus reducing the quantum efficiency. Alternatively it can be reemitted, either at the same energy or at a lower energy. Possibly several re-absorption processes occur before a photon eventually leaves the semiconductor (‘photon recycling’). Such processes are important in LED structures where photon extraction has to be optimized (Sect. 23.3.4). Emission on phonon replica (Sect. 10.4) is red-shifted from the energy range of strong absorption and thus suffers no (or only little) self-absorption. This can be seen from the spectrum of a thick ZnO crystal excited homogeneously (via two-photon absorption with a red Ruby laser), Fig. 10.23. The zero phonon line (at E X ), originating from the ≈100 nm skin of the samples and being by far the strongest in thin films (Fig. 10.5), is practically absent and emission on the phonon replica collected from the entire volume dominates the spectrum.

10.6 Donor–Acceptor Pair Transitions Optical transitions can occur between neutral donors and acceptors. The (spatially indirect) donor– acceptor pair (DAP) recombination is present in (partially) compensated semiconductors and follows

322

10 Recombination

Fig. 10.23 Photoluminescence spectrum (at T = 55 K) from bulk ZnO excited homogeneously via two-photon excitation by a Q-switched ruby laser (pulse width 40 ns). Adapted from [1002]

the scheme D 0 A0 → D + A− eh → D + A− + γ, where γ is a photon with the energy ω. The energy of the emitted photon is given by ω = E g − E Db − E Ab +

1 e2 , 4π0 r R

(10.37)

where R is the distance between the donor and the acceptor for a specific pair. Since R is discrete, the DAP recombination spectrum consists of several discrete lines. If the donor and acceptor occupy the same sublattice, e.g.. O √and C both substituting P sites in GaP, the spatial distance of the donor and acceptor is R(n) = a0 n/2, where a0 is the lattice constant and n is an integer. However, for certain ‘magic’ numbers n = 14, 30, 46, . . . no lattice points exist and therefore the corresponding lines are missing (labeled ‘G’ in Fig. 10.24). No such gaps exist in DA spectra where donors and acceptors occupy different sublattices, e.g. GaP:O,Zn (see also Fig. 10.24). In this case, the spatial separation is √ given by R(n) = a0 n/2 − 5/16. If significant broadening is present, the lines are washed out and a donor–acceptor pair band forms.

10.7 Inner-Impurity Recombination The transitions of electrons between different states of an impurity level can be nonradiative or radiative. As an example, the radiative transition of electrons in the Fe2+ state in InP 5 T2 → 5 E (Fig. 10.25) and its fine structure were observed first in [1005] at around 0.35 eV. Certain defects, also termed ‘color centers’, have been investigated towards their ability to act as efficient single photon source. If a single defect is optically excited, it can emit a photon. However, it cannot be excited further. Also, it cannot emit another photon before it has been excited again. This can be measured through the correlation function for the time difference of emitted photons going to zero for zero time difference. A popular example of such center is the NV center in diamond, the complex of a vacancy and a nitrogen impurity [1006, 1007]. The emission rate saturates at about 2 × 105 photons/s (pick up with microscope objective). The sensitivity of the spectrum to magnetic fields makes the NV center a nanoscopic magnetic field sensor [1008]. Also the spins on the center are fairly isolated and can be manipulated coherently.

10.8 Auger Recombination In competition with the radiative, bimolecular recombination is the Auger recombination (Fig. 10.26). In the Auger process, the energy that is released during the recombination of an electron and hole is

10.8 Auger Recombination

323

1.57 1.56 1.55 1.54 1.53 1.52 1.51 1.50 1.49 1.48 1.47 1.46 1.45 1.44 1.43 1.42 1.41 1.40

C O

Zn O

GaP

Cd O

15.5 meV

0

0.5

1.0

1.5

2.0

2.5

3.0

Fig. 10.24 Transition energies in GaP (T = 1.6 K) of the donor–acceptor recombination involving the deep oxygen donor and C, Zn, and Cd acceptors, respectively. The lines follow (10.37) for E gGaP = 2.339 eV, r = 11.1 and (E Db )O = 893 meV, (E Ab )C = 48.5 meV, (E Ab )Zn = 64 meV, and (E Ab )Cd = 96.5 meV. Predicted missing modes for GaP:C,O are labeled with ‘G’. Adapted from [1003]

1.34

EC 5

T2

InP:Fe

5

E

InP:Fe

1.14

5

0.78

T2

5

E

0.25 (a)

0

Fe3+

Fe2+

EV (b)

0.340

0.345

0.350

Fig. 10.25 a Schematic band diagram of InP with levels of Fe impurities in the 3+ and 2+ charge states at low temperature. All energies are given in eV. The arrow denotes the optical transition from an excited Fe2+ state to the Fe2+ ground state. (b) Photoluminescence spectrum (at T = 4.2 K) of InP:Fe sample with [Fe]=5 × 1016 cm−3 . Part (b) adapted from [1004]

not emitted with a photon but, instead, transferred to a third particle. This can be an electron (eeh, Fig. 10.26a) or a hole (hhe, Fig. 10.26b). The energy is eventually transferred nonradiatively from the hot third carrier via phonon emission to the lattice. The probability for such process is ∝ n 2 p if two electrons are involved and ∝ np 2 if two holes are involved. The Auger process is a three-particle process and becomes likely for high carrier density, either through doping, in the presence of many excess carriers, or in semiconductors with small band gap. Auger recombination is the inverse of the impact ionization (cf. Sect. 8.4.4). Phonon-assisted Auger recombination relaxes the momentum conservation rule for the involved charge carriers at the cost of an additional particle being involved in the scattering process. It has been pointed out that this process is dominating in bulk material [1010, 1011] and quantum wells [1012]. In thermodynamic equilibrium the rates for Auger recombination and thermal Auger generation must be equal, thus

324

10 Recombination

Fig. 10.26 Schematic representation of Auger recombination. An electron recombines with a hole and transfers the energy to a another electron in the conduction band, b another electron in the valence band

e

E

e

E

Eg

Eg

lh

hh

lh

k

k (b)

(a)

hh

Table 10.3 Auger recombination coefficients for some semiconductors. Data for InSb from [1013], SiC from [947], others from [948] material 4H-SiC Si, Ge GaAs, InP InSb

Cn (cm6 /s)

Cp (cm6 /s)

×10−31

2 ×10−31 9.9 ×10−32 3.0 ×10−30

5 2.8 ×10−31 5.0 ×10−30 1.2 × 10−26

G th = Cn n 20 p0 + Cp n 0 p02 ,

(10.38)

where Cn and Cp denote the Auger recombination coefficients. The equation for the dynamics in the presence of excess carriers (if solely Auger recombination is present) is given as ∂ δn = G th − R = −Cn (n 2 p − n 20 p0 ) − Cp (n p 2 − n 0 p02 ) . ∂t

(10.39)

The Auger recombination rate typically used in SRH kinetics is rAuger = (Cn n + Cp p) (np − n 0 p0 ) .

(10.40)

Typical values for the Auger recombination coefficients are given in Table 10.3. In Fig. 10.27a the electron lifetime in heavily p-doped (In,Ga)As (lattice matched to InP) is shown [1014]. It follows τn−1 = Cp NA2 as expected from (10.39) for p-type material. The Auger process in silicon has been discussed in detail [1015]. In Fig. 10.27b experimental data for n-type and p-type Si are summarized. Auger theory can predict the lifetimes in n-type material. The predicted rate in p-type material is too small, thus a phonon-assisted process is evoked [1015].

10.9 Band–Impurity Recombination

325

(b)

(a)

Fig. 10.27 a Experimental values of the electron lifetime in heavily p-doped (In,Ga)As on InP at room temperature. The dashed lines show dependencies of Auger (∝ NA−2 , Cp = 8.1 × 10−29 cm−6 s−1 ) and band-band recombination (∝ NA−1 , B = 1.43 × 10−10 cm−3 s−1 ). Adapted from [1014]. (b) Experimental Auger lifetimes in p-type (squares) and n-type (circles) silicon at 300 K. The dashed (solid) line is theory for p-type (n-type) material. Adapted from [1015]

10.9 Band–Impurity Recombination A very important recombination process is the capture of carriers by impurities. This process is in competition with all other recombination processes, e.g. the radiative recombination and the Auger mechanism. The band–impurity recombination is the inverse process to the carrier release from impurities and intimately related to carriers statistics (Chap. 7). It is particularly important at low carrier densities, for high dopant concentration and in indirect semiconductors since for these the bimolecular recombination is slow. This process is generally considered to be non-radiative since no photons close to the band edge are emitted.4

10.9.1 Shockley–Read–Hall Kinetics The theory of capture on and recombination involving impurities is called Shockley–Read–Hall (SRH) kinetics [942]. An example of radiative band–impurity recombination (of the type shown in Fig. 10.28a) is shown in Fig. 10.8 for the (e,A0 ) recombination at the carbon acceptor in GaAs. We consider electron traps [1016] (see Fig. 10.28) with a concentration Nt with an energy level E t . In thermodynamic equilibrium they have an electron population f t0 =

exp

1 Et −EF kT

+1

,

(10.41)

where f t is the nonequilibrium population of the trap. Then the capture rate rc is proportional to the ∝ n Nt (1 − f t ). The proportionality factor has the unoccupied traps and the electron concentration, rc √ form vth σn , where vth is the thermal velocity vth = 3kT /m ∗ ≈ 107 cm/s and σn is the capture cross section that is of atomic scale, typically ∼ 10−15 cm2 . The capture cross section can be related to the optical absorption cross section [588, 589]. √ In order to make the following calculation more transparent, we put the effective-mass ratio m 0 /m ∗ √ into σ in the following and thus have the same thermal velocity vth = 3kT /m 0 for electrons and 4 Depending

on the energetic depth of the trap, mid or far infrared photons can be emitted.

326

10 Recombination

holes. The capture rate of electrons is rc = vth σn n Nt (1 − f t ) .

(10.42)

gc = en Nt f t ,

(10.43)

The emission rate from filled traps is

where en denotes the emission probability. In a similar way, the emission and capture rates for holes can be written: rv = vth σp p Nt f t

(10.44)

gv = ep Nt (1 − f t ) .

(10.45)

In thermodynamical equilibrium, capture and generation rates are equal, i.e. rc = gc and rv = gv . Thus, the emission probability is 1 − f t0 . (10.46) en = vth σn n 0 f t0 Using

1− f t0 f t0

= exp

Et −EF , (7.10) and (7.11) the emission probabilities can be written as kT en = vth σn n t ep = vth σp pt ,

(10.47) (10.48)

with Et − EC kT Et − EV . pt = NV exp − kT

n t = NC exp

(10.49) (10.50)

We note that n t pt = n 0 p0 (cf. (7.15)). The temperature dependence of the thermal velocity is ∝ T 1/2 , the temperature dependence of the band-edge density of states is ∝ T 3/2 (7.8) and (7.9). Thus, the temperature dependence of the emission

EC Et EV (a)

(b)

(c)

(d)

Fig. 10.28 Band-to-impurity processes at an impurity with one level (left: initial, right: final state in each part): a electron capture (from conduction band), b electron emission (into conduction band), c hole capture (from valence band), d hole emission (into valence band). The arrows indicate the transition of the electron

10.9 Band–Impurity Recombination

327

rate en is (apart from the exponential term) ∝ T 2 if σ is temperature independent. Charge conservation requires in nonequilibrium (and of course in equilibrium) rc − rv = gc − gv . From this we obtain the population of the trap in nonequilibrium: ft =

σn n + σp p t . σn (n + n t ) + σp ( p + pt )

(10.51)

The recombination rate rb−i of the band–impurity recombination is then rb−i = −

∂δn = rc − gc ∂t =

(10.52)

σn σp vth Nt (n p − n 0 p0 ) . σn (n + n t ) + σp ( p + pt )

Using the ‘lifetimes’ τn 0 = (σn vth Nt )−1 τ p0 = (σp vth Nt )−1 ,

(10.53) (10.54)

this is typically written as rb−i =

1 (n p − n 0 p0 ) . τ p0 (n + n t ) + τn 0 ( p + pt )

(10.55)

For an n-type semiconductor the Fermi level is above E t and the traps are mostly full. Thus hole capture is the dominating process. The equation for the dynamics simplifies to p − p0 ∂δ p =− . ∂t τ p0

(10.56)

Thus, an exponential decay with minority-carrier lifetime τ p0 (or τn 0 for p-type material) occurs. A recombination center is most effective when it is close to the middle of the band gap (midgap level). The condition ∂rb−i /∂ E t = 0 leads to the trap energy E tmax with the maximum recombination rate being located at σn N C EC + EV . (10.57) − kT ln E tmax = 2 σp N V The curvature ∂ 2 rb−i /∂ E t2 at E tmax is proportional to −(np − n 0 p0 ) and thus indeed is negative in the presence of excess carriers. However, the maximum can be fairly broad. The SRH kinetic presented here is valid for low densities of recombination centers. A more detailed discussion and a more general model can be found in [1018]. A typical example for a recombination center is gold in silicon. The minority carrier lifetime decreases from 2 × 10−7 s to 2 × 10−10 s upon increase of the Au concentration from 1014 to 1017 cm−3 . The incorporation of recombination centers is an important measure for the design of high-frequency devices [1019]. Due to importance in silicon technology the recombination properties of many metals in silicon have been investigated, in particular Fe-contamination and the role of FeB-complexes [1020– 1022]. A reduction in minority-carrier lifetime can also be achieved by irradiation with high-energy particles and the subsequent generation of point defects with energy levels at midgap.

328

10 Recombination

Fig. 10.29 Minority carrier lifetime at room temperature as a function of majority carrier concentration in n-type and p-type silicon. The dashed lines have the slopes N −1 and N −2 . Data from [1024]

In Fig. 10.29 various data on minority carrier lifetime in silicon are compiled. Over some doping range, a dependence of the lifetime ∝ N −1 as in (10.54) prevails. For doping beyond the 1019 cm−3 range, Auger recombination (Sect. 10.8) with τ ∝ N −2 is dominant. A more detailed discussion can be found in [1023, 1024]. Generally the lifetimes are temperature dependent [1025] as expected from (10.52).

10.9.2 Multilevel Traps Traps with multiple levels in the band gap have generally similar but more complicated dynamics as compared to single-level traps. Lifetimes are an average over negatively and positively charged states of the trap.

10.10 ABC Model Summarizing the results on band-impurity recombination (Sect. 10.9), bimolecular recombination (Sect. 10.2) and Auger recombination (Sect. 10.8), the total recombination rate R can be written simplified as (10.58) R = A n + B n2 + C n3 , where A is the coefficient for the band-impurity recombination, B the bimolecular recombination coefficient and C the Auger recombination coefficient; n denotes the carrier density. This model is known as the ‘ABC’ model. It can be refined separating effects of electrons and holes and including higher terms. Often such model is used to investigate recombination in devices as a function of injection, e.g. [1026, 1027]. The internal radiative quantum efficiency ηint is given by ratio of the radiative recombination rate and the total recombination rate,

10.10 ABC Model

329

ηint =

B n2 Bn = . 2 3 An + Bn +C n A + B n + C n2

(10.59)

10.11 Field Effect The emission of electrons from a trap is thermally activated with an ionization energy E i = E C − E t . If the trap is in a strong electric field E, the emission probability can change. An acceptor-like trap after removal of the electron is neutral and its potential is short range. A donor has a long-range Coulomb potential after ionization. In an electric field, these potentials are modified as visualized in Fig. 10.30. Various additional processes can now occur.

10.11.1 Thermally Activated Emission For the δ-like potential the ionization energy remains unchanged. For the Coulomb potential the barrier in the field direction is lowered by

e √ E. (10.60) E i = e π 0 r The emission rate en is increased in the field by exp(E i /kT ). This effect is called the Poole–Frenkel effect [1028] and can be quite important. For silicon and E = 2 × 105 V/cm and E i = 100 meV a 50-fold increase of the emission rate at room temperature is expected. As an example the Poole–Frenkel + 0 − effect for the electron emission from (neutral) interstitial √ boron in silicon (Bi → Bi + e ) is shown in Fig. 10.31, following the enhancement of en ∝ exp( E). The extrapolation to E = 0 agrees with the EPR result [275, 1029].5

10.11.2 Direct Tunneling Carriers can tunnel from the trap level through the barrier in the field direction into the conduction band. This process is temperature independent. √ The transmission factor of a barrier is (in WKB approxima2m [V (x) − E] dE]. The emission probability for a triangular tion) proportional to exp[−(2/) Fig. 10.30 Field effect at a a δ-like potential and b a Coulomb potential

Ei

Ei

(a) 5 The

slope of the line in Fig. 10.31 is slightly smaller than expected from (10.60).

(b)

330

10 Recombination

Fig. 10.31 Field effect for electron emission from interstitial boron in silicon (T = 65 K). The filled circles represent experimental data from DLTS, the data point marked with an empty circle is from EPR (zero field). The line is a linear fit and extrapolation. Adapted from [1029]

Electron emission rate en (s-1)

10

3

0

2 10

E (V/cm) 4 4 10 2 10

3

4

Si:B 102

101

100 0

50 1/2

E

barrier is then

4 10

√ 3/2 eE 4 2m ∗ E i en = √ ∗ exp − . 3e E 4 2m E i

100 150 1/2 ( (V/cm) )

200

(10.61)

In the case of a Coulomb-like potential the argument of the exponent in (10.61) needs to be multiplied by a factor 1 − (E i /E i )5/3 with E i from (10.60).

10.11.3 Assisted Tunneling In a thermally assisted tunneling process the electron on the trap level is first excited to a virtual level E t + E ph by phonon absorption and then tunnels out of the trap (photon-assisted tunneling). From the energetically higher level the tunneling rate is higher. The probability is proportional to exp(E ph /kT ). The additional energy can also be supplied by a photon (photon-assisted tunneling).

10.12 Recombination at Extended Defects 10.12.1 Surfaces A surface (cmp. Chap. 11) is typically a source of recombination, e.g. through midgap levels induced by the break of crystal symmetry. The recombination at surfaces is modeled as a recombination current js = −e S (n s − n 0 ) ,

(10.62)

where n s is the carrier density at the surface and S is the so-called surface recombination velocity. The surface recombination velocity for GaAs is shown in Fig. 10.32. For InP, if the surface Fermi level is pinned close to midgap, the surface recombination velocity increases from ∼ 5 × 103 cm/s for a doping level of n ∼ 3 × 1015 cm−3 to ∼ 106 cm/s for a doping level of n ∼ 3 × 1018 cm−3 [1030]. For Si, the surface recombination rate depends on the treatment of the surface and lies in the range

10.11 Field Effect

331

between 1–104 cm/s [1031, 1032]. The Si-SiO2 interface can exhibit S ≤ 0.5 cm/s. Time-resolved measurements and detailed modeling for Si have been reported in [1033]. The recombination velocity at surfaces can be reduced using suitable passivation schemes. Typically inert layers or chemical treatments are used. Surface passivation can be accomplished in two fundamentally different ways: Either the surface defect states themselves are removed or an internal electrical field is established that screens excess charge carriers from the surface defects. Sulfur chemistry is a popular treatment of GaAs surfaces. A review of the passivation schemes for III–V semiconductors can be found in [1035].

10.12.2 Grain Boundaries Grain boundaries can be a source of non-radiative recombination. This is technologically important for solar cells made from polycrystalline silicon (cf. Sect. 22.4.6). The grain boundary can be understood as an inner surface in the crystal. Modeling of recombination at a grain boundary can be done using an interface recombination velocity [1036, 1037] or considering deep traps [1038]. The minority carrier lifetime decreases with decreasing grain boundary area A (Fig. 10.33a). The carrier loss at a grain boundary can be imaged directly via the efficiency of the collection of an electron beam induced current (EBIC) as shown in Fig. 10.33b. The minority carrier lifetime is only unaffected when the average distance to a grain boundary is much larger than the minority carrier diffusion length, √ A L D , otherwise the entire grain volume is subject to non-radiative recombination. The recombination velocity at grain boundaries can be reduced, similar to that at surfaces, using suitable passivation schemes. A famous one is the chlorine treatment of polycrystalline CdTe used in thin film solar cells [1041].

10.12.3 Dislocations Also dislocations typically act as recombination centers, sometimes called carrier sinks. In Fig. 10.34 it can be seen that the minority carrier lifetime depends on the dislocation density n d and follows a τ −1 ∝ n d law, as if each dislocation is a recombination center [1042]. The non-radiative recombination 107

GaAs 106

10

5

104 15 10

1016

1017

1018 -3

1019

Fig. 10.32 Surface recombination velocity for GaAs as a function of n-type doping concentration. Different experimental points correspond to different surface treatment methods. Dashed line is a guide to the eye. Experimental data from [1034]

332

10 Recombination

makes dislocations appear as ‘dark line defects’ in luminescence imaging [1043]. In [1044] also the decrease of carrier lifetime around (misfit) dislocations has been imaged. The effect of dislocations on the radiative recombination efficiency depends on the diffusion length [1044].

10.13 Excess-Carrier Profiles In this section, some typical excess-carrier profiles (in one-dimensional geometry) are discussed that arise from certain excitation conditions. The excess-carrier density p (here holes in an n-type semiconductor, i.e. p = pn − pn0 ) is determined by the diffusion equation (cf. (8.65a)) Dp

(a)

∂ 2 p p = −G(x) + . ∂x 2 τp

(10.63)

(b)

Fig. 10.33 a Minority carrier lifetime in (p-type) silicon as a function of grain boundary size. The dashed line has the slope ∝ A. Data from [1039]. b Linescan of the electron beam induced current (EBIC) perpendicular to a single grain boundary in silicon. The arrow denotes the position of the grain boundary. Compiled from [1040] Fig. 10.34 Inverse minority carrier lifetime in n-type silicon (40 cm), low resistivity Ge (3–5 cm) and high resistivity Ge (30–40 cm). Data from [1042]

10.13 Excess-Carrier Profiles

333

10.13.1 Generation at Surface First, the generation of excess carriers in a semi-infinite piece of semiconductor shall occur only at the surface at x = 0 (strong absorption limit). The generation is zero everywhere else and the excitation is incorporated via the boundary condition p(x = 0) = p0 . The general solution for the homogeneous equation (10.63), i.e. G = 0, is x x + C2 exp , p(x) = C1 exp − Lp Lp with the diffusion length L p = is (C2 = 0)

(10.64)

Dp τp . Taking the boundary condition p(x → ∞) = 0 the solution x . p(x) = p0 exp − Lp

(10.65)

In order to connect p0 with the total generation rate per unit area G tot , we calculate ∞ G tot = 0

Lp p(x) dx = p0 = p0 τp τp

Dp . τp

(10.66)

If a slab of finite thickness d is considered, the boundary condition on the back surface comes into play. Assuming a contact that extracts all excess charge carriers, p(d) = 0. In conjunction with (10.64), we find x d p0 exp − 1 + coth p(x) = 2 Lp Lp d x + 1 − coth exp , (10.67) Lp Lp with

d G tot = 0

Lp p(x) d . dx = p0 tanh τp τp 2 Lp

(10.68)

Generally, the excited electrons and holes diffuse into the bulk at different speed due to their different diffusion length (or mobility). As consequence, a spatial separation of electrons and hole densities occurs which leads to an electric field, the Dember field [1045–1047]. The illuminated surface becomes positive compared to the dark case since Dn > Dp . A treatment of the non-neutral diffusion situation is given in [1048]. As shown in Fig. 10.35, the non-equal electron and hole densities create locally a non-zero charge density δρ and an associated potential δφ; for a silicon material parameters (n i = 1010 cm−3 ), the Dember voltage is calculated as VDem = δφ(0) = 1.84 meV for a generation rate of G = 2 × 1010 /(cm2 s). Extensions of the theory have been given considering traps [1049] and the effect of finite sample thickness and surface recombination [1050] (under certain conditions, the sign of the field can be reverse).

334

10 Recombination

Fig. 10.35 Charge carrier density profiles (in a semi-infinite slab) for electrons and holes as well as their difference p − n = δρ/e, as well as the associated Dember potential δφ. The ratio of electron and hole mobility in this model calculation (using silicon material parameters) was 5. Adapted from [1048]

10.13.2 Generation in the Bulk Now, a generation rate following (9.16), realistic for photodiodes and solar cells, is considered, G(x) = G 0 exp (−α x) ,

(10.69)

i.e. due to light absorption with the (wavelength-dependent) absorption coefficient α. The total generation rate is ∞ G0 . (10.70) G tot = G(x) dx = α 0

The total generation rate is equal to the number of photons per second 0 that enter the semiconductor. The solution of (10.63) is the sum of the homogeneous solution (10.64) and a particular solution that is given by p(x) = C exp (−α x) . (10.71) The constant C is determined to be C=

G 0 τp . 1 − α2 L 2p

(10.72)

Therefore, the solution is G 0 τp x x + C2 exp + exp (−α x) . p(x) = C1 exp − Lp Lp 1 − α2 L 2p

(10.73)

Using again p(x → ∞) = 0 (leading to C2 = 0) and a recombination velocity S at the front surface, i.e.

10.13 Excess-Carrier Profiles

335

(b)

(a)

Fig. 10.36 Excess carrier density profile (10.75) in a linear and b semi-logarithmic plot for S = 0 and S = ∞. Other parameters are given in panel (a)

− e S p0 = −e Dp

∂p . ∂x x=0

(10.74)

The solution is given as G 0 τp S + α Dp x p(x) = exp (−α x) − . exp − 1 − α2 L 2p S + Dp /L p Lp

(10.75)

For vanishing surface recombination, S = 0, the solution is (Fig. 10.36) p(x) =

G 0 τp x exp x) − α L . exp − (−α p 1 − α2 L 2p Lp

(10.76)

For αL p 1, (10.65) is recovered. This dependence is the excess-carrier profile if the absorption is strong, which is a tendency for short wavelengths. The current at the surface, j (x = 0) ∝ ∇p, is zero. In the case of very strong surface recombination, S → ∞, (10.75) becomes p(x) =

G 0 τp x exp x) − exp − , (−α 1 − α2 L 2p Lp

(10.77)

with p(0) = 0 (Fig. 10.36). The current at the surface is (Dp τp = L 2p ) j (x = 0) = −e D

G0 Lp α Lp ∂p = −e = −e 0 . ∂x x=0 1 + α Lp 1 + α Lp

(10.78)

Part II

Selected Topics

Chapter 11

Surfaces

Gott schuf das Volumen, der Teufel die Oberfläche. God created the bulk; surfaces were made by the devil. attributed to W. Pauli

Abstract The specifics of semiconductors surfaces, their symmetry, equilibrium crystal shape, reconstructions, steps and faceting are summarized, being important for epitaxy. Physical surface properties such as vibrational and electronic states are discussed.

11.1 Introduction Obviously every crystal has a surface all around it, connecting it to the surrounding world. This represents a brutal perturbation of the bulk periodicity with the consequence of a whole new world of physics at the surface. With regard to semiconductor technology, the surface properties are of large importance in a number of instances: • The crystal growth of semiconductors always occurs at a surface. This subject will be discussed in Chap. 12. • The surface is subject to interaction with the chemistry of the surrounding atmosphere. This is of essential importance for catalysis, e.g., oxidation of CO at noble metals or photocatalytic water splitting, e.g., using TiO2 , into oxygen and hydrogen [1051, 1052]. Photocatalysis is briefly discussed in Sect. 22.1. The interaction and reaction with the surrounding atmosphere can lead modifications of the semiconductor such as change of conductivity, e.g.., in SnO2 , which can be used in the construction of gas detectors [1053–1055]. • Surface passivation and barriers, e.g., using photoresist, silicon oxides or nitrides, are often necessary in practical devices in order to avoid surface recombination (Sect. 10.12.1) or the interaction with atmospheric oxygen or water. But surface physics is interesting in its own right, investigating the properties of a complex mostly two-dimensional system. ‘Pure’ surfaces are studied using crystals cleaved in ultra-high vacuum or carefully prepared atomically clean surfaces. A special case are two-dimensional materials, also termed atomic sheets, such as graphene; these will be discussed in Sect. 13.1. At the surface the atoms rearrange, compared to their bulk positions, vertically and laterally, also forming new bonds (surface reconstructions). The mechanical properties (surface phonons) and elec© Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_11

339

340

11 Surfaces

tronic properties (surface states) are different from the bulk modes. Detailed treatments of surface physics and its experimental methods can be found in [695, 1056–1058].

11.2 Surface Crystallography The surface symmetry, i.e. the two-dimensional spatial periodicity of the constituent atoms, is described with the ten two-dimensional point groups (Table B.1). The point symmetries are 1-, 2-, 3-, 4-, and 6-fold rotational symmetry (Fig. 3.9) with or without mirror plane(s). The two-dimensional point symmetries of popular substrate orientations are compiled in Table 11.1; the different symmetry of the first layer and the half-space are notable. The combination of five 2D Bravais lattices (cmp. Sect. 3.3.1) with the 10 2D point groups leads to the 17 two-dimensional space groups (wallpaper groups) [1059]. For the treatment of surface in reciprocal space, the three-dimensional k-vector is split into the two-dimensional component k|| parallel and the one-dimensional component k⊥ perpendicular to the surface, (11.1) k = k|| + k⊥ . The three most important Brillouin zones in two-dimensional k-space are depicted in Fig. 11.1. Often the special points of the 2D Brillouin zones are denoted with a bar over the letter.

Table 11.1 Two-dimensional point symmetries of common substrates with ideal low-index surfaces Crystal

Surface

1st layer

1st & 2nd layers

Half space

Rocksalt

(001) (110) (111) (001) (110) (111) (001) (110) (111) (00.1) (10.1) (11.0)

4 mm 2 mm 6 mm 4 mm 2 mm 6 mm 4 mm 1m 6 mm 6 mm 2 mm 2 mm

4 mm 2 mm 3m 2 mm 2 mm 3m 2 mm 1m 3m 3m 2 mm 2 mm

4 mm 2 mm 3m 2 mm 2 mm 3m 2 mm 1m 3m 3m 1m 1m

Diamond

Zincblende

Wurtzite

X'

(a)

M

J' M

X

J (b)

K

M

(c)

Fig. 11.1 Two-dimensional Brillouin zones for a square, b rectangular and c hexagonal surface symmetry. Special points are labelled and the grey areas indicate the smallest irreducible area

11.3 Surface Energy

341

11.3 Surface Energy The surface energy, more precisely the surface energy per area γ, is related to the work that is necessary to split a crystal in two parts. Such process will leave broken (‘dangling’) bonds. This energy will depend on the crystal orientation as is already clear from the fact that there are easy cleaving planes (Sect. 5.4.2). The surface energy will also depend on the surface reconstruction (see Sect. 11.4), i.e. the rearrangement of surface bonds and atoms. Generally, the reduction of the number of dangling bonds on a surface lowers its energy, while the distortion of bonds increases its energy. The anisotropy of the surface energy for a given orientation hkl, γ(hkl), determines the equilibrium crystal shape (ECS) at a given temperature (below melting temperature). The crystallite is assumed to be of at least mesoscopic size such that energy effects due to edges and apexes can be neglected compared to the surface energy terms. As an example theoretically calculated surface energy values for covalent semiconductors are listed in Table 11.2. The equilibrium shape of silicon has been observed for µm-sized bulbs as shown in Fig. 11.2a for T = 1323 K ; the experimental anisotropy of surface energy of silicon is shown in Fig. 11.2b.

11.4 Surface Reconstruction When in a Gedankenexperiment the bulk crystal is split such that a surface with defined orientation develops, many bonds are cut. These dangling bonds can be saturated with other atoms such as hydrogen. In particular under vacuum conditions, the dangling bonds will rearrange and form new

Table 11.2 Surface energy (in J/m2 ) for various C, Si and Ge surfaces. Data from [1060] Material

{111}

{110}

{100}

{311}

C Si Ge

8.12 1.82 1.32

7.48 2.04 1.51

9.72 2.39 1.71

8.34 2.12 1.61

(111)

0)

(111) (113) (001) (113)

1.01

01 / (111)

(113)

(111 )

)

(110)

1.00 0.99 0.98

(111)

(a)

(110)

1.02

3)

(0

(11

(111) (11

0.97 0.96 -90

(b)

Si -60

-30 0 30 Angle (degree)

60

90

Fig. 11.2 a Equilibrium crystal shape (cross section in 110 azimuth) of 1.06 µm diameter Si bulb at T = 1323 K with facet orientations as labelled. a Anisotropy of surface energy (relative to γ(111)) for Si, the dashed line is guide to the eye. Adapted from [1061]

342

11 Surfaces

bonds such as dimers along the surface, lowering the total energy. This surface reconstruction displays two-dimensional periodicity of a surface unit cell. Since the forces from the split-away half-space are missing, the atomic planes will rearrange vertically1 and the surface-near layers will exhibit slightly different lattice spacing than in bulk. In [1062] the surface reconstructions of many semiconductors are reviewed. In Fig. 11.3a the rearrangement of surface atoms on GaAs(110) is depicted as an example. The anion is moved up, the cation moved down, preserving the bond length, rotating the bond by about γ = 30◦ for various III–V semiconductors [1063] (Fig. 11.3b). The height difference of the top anion and cation 1 scales with the bulk lattice constant (Fig. 11.3c). The details are specific to materials and orientations. Different reconstructions occur for different thermodynamical conditions, some of them being metastable, as depicted for GaAs(100) in Fig. 11.4. Several different surface reconstructions can also be present simultaneously at a surface within different domains. The stable reconstruction of the Si(111) surface is the somewhat complicated 7 × 7 reconstruction which is schematically depicted in Fig. 11.5a as proposed in [1066] (‘DAS’ dimer-adatom-stacking fault model’). A STM image of this surface has been reported first in [1067] and is depicted in Fig. 11.5b. Details of this surface are also recently a subject of interest [1068].

Ga As

ideal

reconstructed

(a)

[110]

(b)

[100]

(c)

Fig. 11.3 a Schematic drawing of the GaAs(110) surface after cutting bonds (‘ideal’) and actual atomic rearrangement with asymmetric dimer in the reconstructed state. Adapted from [1064]. b Schematic of the III–V (110) surface relaxation (red circles: anions, blue circles: cations) with bond rotation ω and atom shift . c Experimental values for he relaxation 1 as shown in panel (b) for various semiconductors vs. their bulk lattice constant a0 ; dashed line is straight line as guide to the eye. Data from [1063]

1 Typically the distance between the first and second layer is reduced, and the distance between the second and third layer a little bit increased.

11.5 Surface Morphology

343 (4 2)

0.2 0.1 c(4 4)

Energy (eV)

[110] [110]

0 -0.1 -0.2 -0.3 -0.4

(a)

2(2 4)

mixed dimer

2(2 4)

(2 6)

(b)

GaAs(100) -0.5 Ga chemical potential

0 (eV)

Fig. 11.4 a Various reconstructions of the GaAs(100) surface. Filled (empty) circles represent As (Ga) atoms. Atom positions in the top two atomic layers are indicated by larger symbols. b The relative formation energy per (1 × 1) unit cell of various reconstructions as a function of the Ga chemical potential. Vertical dashed lines mark the approximate anion- and cation-rich limits of the thermodynamically allowed range of μ. Adapted from [1065]

[110]

1nm

[112] [111]

(b)

(a)

Fig. 11.5 a Schematic drawing of the 7 × 7 reconstruction of Si(111) surface. The large grey circles represent adatoms, the small balck circles rest atoms. Adapted from [1066] b STM image (empty states) of such surface. Adapted from [1067]

11.5 Surface Morphology The surface reconstruction is related to the local atomic arrangement of the surface atoms. On larger length scales, surfaces can exhibit roughness in general and various specific morphologies, among them steps, step bunches, facets, hillocks or pits. When atomically flat terraces are separated by steps of equal heights, the surface is termed vicinal. The step height can be an atomic monolayer or more. The step edges can be straight, smoothly curved or rugged, depending on the formation energy of kinks. If the substrate surface is inclined by a small ‘off-cut’ angle θ with respect to a low index plane, for a step height h the average terrace width L is given by L=

h h ≈ . tan θ θ

(11.2)

The Si(001) surface (under certain conditions) exhibits monoatomic steps between the A-type 1×2 and B-type 2 × 1 terraces [1069]; clearly also the step edges between A–B and B–A are quite different, one being much rougher than the other (Fig. 11.6). The surface is thus a two domain surface, the symmetry of both A- and B-type terraces being 2 mm, rotated by 90◦ against each other.

344

11 Surfaces

Fig. 11.6 STM image of Si(001) surface with an off-cut θ = 0.5◦ . Adapted from [1069]

(a)

10nm

(b)

Fig. 11.7 a STM images a ZnO(00.1) O-terminated surface, left (right) panel with zero (about 1.3◦ ) off-cut, exhibiting monolayer step heights of 0.27 nm. a LEED pattern of such surface (recorded at 70 eV). Adapted from [1070]

A similar example is the Zn(00.1) surface. The found step height of the monoatomic steps is 0.27 nm and corresponds c/2 [1070]. The terrace width is about 12 nm (Fig. 11.7a), yielding an off-cut (11.2) of about 1.3◦ . The surface pattern shows triangular features in two orientations, rotated by 60◦ . The 3m symmetry of the surface, although the first monolayer has 6 m point symmetry (Table 11.1), occurs in two domains rotated against each other by 60◦ . The LEED pattern from each individual terrace is expected to have three-fold symmetry; the mixed character of the surface yields a six-fold pattern (Fig. 11.7b). Steps can gather and form step bunches with a height much larger than a monolayer (Fig. 11.8). Faceting of higher index planes occurs when it is energetically favorable to form alternating facets of low energy low index planes, for example Si(223) exhibits periodic ridges with (111) and (113) facets [1071]. The faceting of a surface close to (113), exhibiting smooth (113) and rough (114) planes, is depicted in Fig. 11.9.

11.6 Surface Physical Properties

345

5µm Fig. 11.8 SEM image of the surface of a 4H–SiC layer on [00.1]-oriented substrate with 8◦ misorientation towards [11.0]. Adapted from [1072]

(114)

(113) (114)

100nm

(113)

10nm

Fig. 11.9 STM images of a silicon surface close to (113), 21.5◦ from (001) towards (111), i.e. (113)-3.7◦ . Adapted from [1073]

11.6 Surface Physical Properties 11.6.1 Surface Phonons As a model for surface vibrational states, the diatomic one-dimensional chain model discussed in Sect. 5.2.2 can be modified to allow for a different surface spring constant Cs instead of C1 or C2 . Such model can be solved numerically for finite chain length. The bulk dispersion is found with an extra mode in the gap or above the maximum frequency for a range of values of Cs as depicted in Fig. 11.10. When the spring constant of the surface atom is smaller than the larger of the two spring constants C1 and C2 (in our model calculation C2 > C1 ), a state in the gap forms; for a surface spring constant larger than C2 , first the surface vibration lies within the optical bulk band and then forms a state above the maximum optical frequency ωm , given by (5.18).2 In order to display the dispersion of surface states together with the bulk band structure, the latter is projected to the surface k|| -vector: E n (k) is considered as E n,k⊥ (k|| ) = E ν (k|| ), where ν = n, k⊥ is a new, continuous index. In the plot of E nsurf vs. k|| , for each value of k|| a range of energies reflects the appearance of states within the gap and above ωm resembles that of localized vibrational modes of substitutional masses (Sect. 5.2.7).

2 The

346

11 Surfaces C2 M2=M1 , C2=2C1

Frequency (ωmax)

1.0

0.5

0.0 0

1

2 Csurface (C1)

3

4

Fig. 11.10 One-dimensional model calculation of surface vibrational state frequency (in units of the maximum bulk optical phonon frequency ωm ) as a function of the spring constant Csurface of the surface atom replacing C1 (blue curve) or C2 (black curves). As model parameters we use equal masses and C2 = 2 C1 (γ = 0.943 from (5.17)). The grey areas represent the energy range of the acoustic and optical phonon bulk bands

40

GaAs (110)

Energy (eV)

30

20

10

0 J‘

J

Fig. 11.11 Surface phonon dispersion for GaAs(110) (solid lines) with the surface projected bulk band structure (light grey area). The symboles are experimental data from two different methods. The dark grey areas at about 10 meV indicate regions where the A1 -peak is present in the calculated scattering cross-section. Adapted from [1063]

bulk band structure (Fig. 11.11). This concept pertains to phonon dispersion as well as to electronic states.

11.6.2 Surface Plasmons Free-carrier oscillations in the bulk had been discussed in Sect. 9.9.1. A surface plasmon is the quantum of a surface-bound plasma oscillation. Such effect has been discussed in [1074] and reviewed in [1075, 1076]. A metal (or conductive semiconductor) with dielectric constant according to (9.77) 1 = m = r (ωp /ω)2 and a dielectric (or vacuum) with 2 = d are assumed (Fig. 11.12).

11.6 Surface Physical Properties

347

Fig. 11.12 Sketc.h of surface plasmon field distribution. Adapted from [1077]

Fig. 11.13 Surface plasmon polariton dispersion for ZnO:Ga/air for three different carrier concentrations as labelled, experimental data (symbols) and theory (lines). Adapted from [1078]

0.9 0.8

ZnO:Ga

20

n=7.2 10 cm

-3

1.5

0.6

n=3.2 1020 cm-3

2

0.5 0.4

3

n=1.2 1020 cm-3

4 5

0.3

Wavelength (µm)

Energy (eV)

0.7

0.2

10

0.1 0

0

2 4 6 6 -1 Wave vector (10 m )

8

The surface plasmon (polariton) (SPP) is a wave localized at the surface with evanescent parts into the metal and the dielectric. The dispersion of the surface plasmon (polariton) is given by kSPP =

ω c

1 2 . 1 + 2

(11.3)

For large k, the limiting frequency is the SPP frequency (from 1 = 2 ) ωp ωSPP = √ < ωp , 1 + d /r

(11.4)

√ which is smaller than the plasma frequency. For a metal against vacuum, ωSPP = ωp / 2. The SPP dispersion for a ZnO:Ga/air interface is depicted in Fig. 11.13 for three different doping concentrations.

11.6.3 Electronic Surface States The bulk band structure is given by the energy eigenvalues E n (k). The surface adds its own states E nsurf (k|| ), many of them in the gap. The calculation of gap states has been already briefly discussed in Sect. 6.2.3. The nature of bulk states is oscillatory in the bulk and exponentially decaying in the outside (Fig. 11.14a), the nature of surface states is localized at the surface and decaying both towards

348 Fig. 11.14 Schematic wavefunction versus coordinate for a bulk state in the vicinity of the surface (its position indicated by the vertical dashed line), b surface state and c surface resonance state

11 Surfaces

(a)

(b)

(c)

Si(100)-(2 1)

2.0

Energy (eV)

Fig. 11.15 Surface band structure of Si(100)-(2 × 1), lines denote a theoretical quasi-particle calculation, symbols represent experimental data. The grey areas indicate the projected bulk band structure. Adapted from [1079]

1.0

0

-1.0 J M Surface wave vector

J‘

the bulk and the outside (Fig. 11.14b). A third type of states is a surface resonance which is oscillatory in the bulk and has enhanced probability at the surface, of course also decaying towards the outside (Fig. 11.14c); such states are surface related but energetically degenerate with states of the bulk band structure. Surface states for Si(100) in 2 × 1 reconstruction are shown in Fig. 11.15. The surface bands arise from (filled and unfilled) π- and π ∗ -orbitals from the dangling bonds on the threefold-coordinated surface atoms [1079]. A calculation for the ideal (unreconstructed) (100), (110) and (111) surfaces of Si, Ge and GaAs can be found in [1080]. Further work on silicon surface states (clean and with adsorbates) is compiled in [1081]. For a conventional insulating material (with gap) the states of conduction and valence band have defined s- and p-type symmetry (cmp. Fig. 2.5) and the surface states can be populated with spin up and down electrons as is schematically drawn in Fig. 11.16a. Such ‘normal’ surface states are thus not spin-polarized. This has been shown, e.g., for the well-known surface states of Si(111)-(7 × 7) [1082] in [1083]. In a so-called topological insulator [464], a band inversion is present (cf. Sect. 6.2.6). In HgTe-like materials, s- and p-type bands are inverted at the point (cmp. Sect. 6.11). In layered (orthorhombic) Bi2 Se3 -like tri-chalcogenide materials two pz -orbitals with opposite parity are inverted at the point. Reasons for the band inversion are spin-orbit interaction but also scalar relativistic effects and lattice distortions [1084]. The spin-orbit interaction is responsible for opening a gap; the associated surface

11.6 Surface Physical Properties E

349

(a)

(b)

E

k

k

Fig. 11.16 a ‘Normal’ band structure with surface states, the valence band states are antisymmetric (‘–’) from p-states, the conduction band states are symmetric (‘+’) from s-states. The arrows denote the electron spin orientation of the states. b ‘Topological’ band structure with surface states crossing the gap and electrons in the two surface states having unique spin orientations

0.4 0.3 Energy (eV)

Fig. 11.17 Density of states for Bi2 Se3 (111) surface. Adapted from [1086]

Bi2Se3

0.2 0.1 0 -0.1 -0.2 -0.3 K

M

states cross the band gap (Fig. 11.16b) and are spin-polarized (Fig. 11.16c) [1085, 1086]. A review of various systems is given in [463]. Charge transport in such spin-polarized surface states suffers no scattering (thus these states are called ‘topologically protected’) unless by a center that breaks time reversal symmetry (magnetic impurity). The more or less linear dispersion of these states forms a ‘Dirac cone’ (cmp. Sect. 13.1.2 for the band structure of graphene with six Dirac cones) (Fig. 11.17). Topological surface states have been observed in various systems [463]. As an example we show data on bulk Bi2 Se3 [1087] for which the surface states are found to cross the band gap (Fig. 11.18a) and spin-polarized measurements (Fig. 11.18b) show a strong spin polarization (about 50%) of the two branches. Another situation where topological edge states appear is the interface between two semiconductors with bands of different topology, such as HgTe and CdTe (cf. Sect. 6.11).

350

11 Surfaces K

Bi2Se3 surface states

-0.2

-0.4

Dirac point

-0.01 0 -1 0.01 ky (nm )

M ARPES intensity (arb. units)

Energy (eV)

K

-0.1

-0.3

(a)

M

-0.01 0 -1 0.01 kx (nm )

Intensity (arb. units)

M EF=0

-0.01

(b)

M

Bi2Se3

0 -1 ky (nm )

0.01

Fig. 11.18 a Angle-resolved photoemission spectra from Bi2 Se3 (111) surface along two different k-space directions. The Fermi level is at energy zero. The blue dashed line indicates the angular scan displayed in panel (b). b Spin-polarized momentum distribution curve at a binding energy of −140 meV, measured along the k y -direction. Adapted from [1088]

Chapter 12

Heterostructures

The interface is the device. H. Kroemer [133]

Abstract Heterostructures are the most important basis for modern devices and are covered regarding various aspects including heteroepitaxy on planar and patterned substrates, surfactants, heterostructure band lineup as well as energy levels and recombination in planar confined systems (quantum wells and two-dimensional electron gases).

12.1 Introduction Heterostructures consist of (at least two) different materials. The geometry of the interfaces between the two materials can be complicated. The simplest case is a planar interface, i.e., a layered system. A metal–semiconductor junction is generally a heterostructure. However, we will use the term mostly for structures of various semiconductors. Most of the heterostructures discussed here are epitaxial, i.e., fabricated by the successive epitaxy of the various layers on a substrate. Another method to fabricate heterostructures of different (and dissimilar) materials is wafer bonding that is briefly discussed in Sect. 12.6. Many modern semiconductor devices rely on heterostructures, such as the heterobipolar transistor (HBT), the high electron mobility transistor (HEMT), lasers and nowadays also light-emitting diodes. Shockley had already considered heterostructures in his 1951 patent for pn-junctions. For the development and the realization of heterostructures H. Kroemer and Zh.I. Alferov were awarded the 2000 Physics Nobel Prize. The properties of charge carriers in layers that are part of heterostructures can be quite different from those in bulk material, e.g., extremely high mobility, high radiative recombination efficiency or novel states of matter, as revealed in the quantum Hall effects.

© Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_12

351

352

12 Heterostructures

12.2 Heteroepitaxy 12.2.1 Growth Methods Since the thickness of layers in the active part of heterostructures has to be controlled to monolayer precision and the thickness of layers can go down to the single monolayer range, special growth methods have been developed [1089–1091]. Among these molecular beam epitaxy (MBE [1092]), chemical vapor deposition (CVD [1093, 1094]) and metalorganic vapor phase epitaxy (MOVPE [1095]) are the most common for Si, Ge, III–V and II–VI semiconductors. Thin films for many materials can also be fabricated by atomic layer deposition (ALD [1096, 1097]). In particular oxide semiconductors (and superconductors) are also fabricated with pulsed laser deposition (PLD [1098]). Liquid phase epitaxy (LPE [1099]) used to be very important for the fabrication of LEDs but has lost its role largely to MOVPE. MBE is performed in an ultrahigh vacuum (UHV) chamber, pumped by getter pumps and cryoshrouds. The source materials are evaporated from effusion cells and directed towards the heated substrate. If the source materials are supplied as a gas stream, the method is called gas-source MBE (GSMBE). If metalorganic compounds are used as precursors, the method is denoted as MOMBE. The atoms impinge on the substrate with thermal energy and are first physisorbed. After diffusion on the surface they either desorb or they are chemisorbed, i.e., incorporated into the crystal. In order to obtain high spatial homogeneity of material properties such as composition, thickness and doping, the substrate is rotated during deposition. During CVD and MOVPE the heated substrate is in a gaseous environment. The transport gas is typically H2 , N2 or O2 . Precursor materials are hydrides such as silane, germane, arsine or phosphine (SiH4 , GeH4 , AsH3 , PH3 ) and (for MOVPE) metalorganic compounds, such as, e.g., trimethylgallium (TMG). Due to the toxicity of the hydrides, alternative, i.e., less-toxic and less-volatile compounds are used, such as TBAs ((CH3 )3 CAsH2 ). The crystal growth occurs after pyrolysis and catalysis of the compounds close to or on the substrate surface. All remaining C and H atoms (and whatever else that is not incorporated into the crystal) leave the reactor and are neutralized and stopped in a scrubber. In ALD alternating injections of molecular precursors and purge cycles build up the thin film atomic layer by atomic layer; this method is particularly advantageous for achieving conformal coatings. In-situ monitoring is of importance to obtain information about the growth process while it is underway. Using the information in a feedback loop it is possible to achieve in-situ control of the process, e.g., for precise determination of growth rates or layer thickness. Techniques are RHEED (reflection high-energy electron diffraction) [1100] (only for UHV systems) and RAS (reflection anisotropy spectroscopy) [1101, 1102].

12.2.2 Substrates Thin-film epitaxy is mostly performed on wafers, i.e., thin circular slices of substrate material. The most common substrate materials are Si (currently up to 400 mm diameter [1103, 1104]), Ge (also up to 300 mm [1105]), GaAs (up to 6 inch), InP (up to 4 inch) and sapphire (up to 6 inch). Typical wafer thickness is 300–500 µm. Also, very thin, flexible Si wafers (8–10 µm) have been developed [1106]. A wafer is cut from a large single cylindrical crystal that is fabricated with suitable growth techniques such as Czochralski (CZ) growth [1107, 1108] modified by Teal and Little [1109–1111]. In CZ growth the crystal, starting with a small seed crystal, is pulled out of a melt of previously polycrystalline, pure or doped material. All dislocations stop in the narrow neck between the seed and the main body of the cylinder. The diameter of the crystal is controlled by the pulling rate (matching the crystallization

12.2 Heteroepitaxy

353

(b)

(c)

(a)

Fig. 12.1 a Silicon single crystal for 300-mm diameter wafers after opening of the crucible. From [1114] with permission. b Historic development (first year of larger production) of silicon wafer diameter and ingot mass. Data from [1104]. c GaAs single crystal (boule) for 4-inch wafers and some cut and polished wafers Fig. 12.2 Schematic semiconductor wafer geometry for various orientations and doping with the primary (P) and secondary (S) flats indicated

S S P

P

S (1

P

P (1

speed of the material) and the heating power. For the growth of III–V compound semiconductors, liquid encapsulated CZ (LEC) growth has been developed to counteract the high volatility of the group-V component. During LEC growth the melt is completely covered with molten boric oxide (B2 O3 ). The keys to optimization of the crystal growth process are numerical modeling and computer control. In Fig. 12.1a,c a large CZ silicon crystal and a smaller LEC GaAs crystal (boule) are shown. Over time wafer size and ingot mass have increased remarkably (Fig. 12.1b). For details on other important fabrication methods for bulk crystals, including float-zone (FZ [291, 1112]) or vertical gradient freeze (VGF), we refer to the literature [1113]. Significant expertise is necessary for cutting, grinding and polishing (lapping) wafers for epitaxy. For semiconductors, the wafer is marked with flats to indicate orientation and doping. In Fig. 12.2 the standard flats are shown for (100)- and (111)-oriented material. The primary (major) flat (OF, orientation flat) defines the crystallographic orientation1 is longer than the secondary (minor) flat which defines the conductivity type (IF, identification flat). For a 4-inch (100 mm) diameter wafer the OF is 32 and the IF 12 mm long. The front surface, on which the epitaxy is performed, typically undergoes 1 In

¯ surface, in the ‘EJ’ definition, the primary flat is (01¯ 1). ¯ the ‘US’ flat definition, the primary flat is the (011)

354

12 Heterostructures

Fig. 12.3 a AFM images of an as-received ZnO wafer, exhibiting small terraces and nm deep scratches from polishing. ¯ wafers with vicinal surfaces after thermal treatment (1000 ◦ C for 2 h in O2 ), exhibiting atomically (b, c) Two ZnO (0001) flat terraces with c/2 monoatomic step heights. Two different substrates with different off-cut (misorientation direction and angle) are shown. Adapted from [1122]

(a)

(b)

Fig. 12.4 Cross-sectional TEM of MBE-grown Alx Ga1−x As/GaAs heterostructures for (a) x = 0.41 and (b) x = 1.0. Using an AlAs/GaAs superlattice an excellent flattening of substrate roughness is achieved. From [1123]

an elaborate cleaning and polishing process. Silicon processes [1115, 1116] are based on the RCA cleaning procedure [1117] and the related Shiraki etch [1118] and can achieve clean, atomically flat surfaces [1119]. III-V semiconductors are typically prepared using a polishing etch [1120, 1121], often solutions containing bromine. It is possible to create compound semiconductor surfaces that exhibit large, essentially monoatomically flat terraces between individual surface steps. Polishing or other surface damage can also be removed prior to epitaxy with thermal (Fig. 12.3) or ion beam treatments. One prerequisite for making high-quality heterostructures with thin layers is a flat surface. Even if the polished substrate is not perfect, flat interfaces can be achieved with the growth of appropriate superlattice buffer layers (Fig. 12.4). Roughness can exist on all length scales and is typically investigated using atomic force microscopy scans. High throughput demands and the advent of multi-wafer reactors make prior cleaning and etching procedures tedious. For this purpose, substrates for well-developed material systems are offered ‘epiready’. Epiready wafers are often covered with a very thin protective film that can be released using a thermal treatment at or below typical growth temperature in the growth reactor immediately prior to epitaxy. The protective film separates the polished semiconductor wafer from the ambient. Examples are a few monolayers of arsenic on GaAs or two monolayers GaN on SiC. However, the suitability of a purchased substrate may depend on the duration and conditions of its storage.

12.2 Heteroepitaxy

(110)

(111)B (113)A (001) (113)B (111)A

(110)

140

GaAs

120 Growth rate (µm/h)

Fig. 12.5 Growth rate of GaAs in vapor phase transport at 725◦ as a function of crystal orientation. The dashed line is guide to the eye. Adapted from [1128]

355

100 80 60 40 20 0 90

60

30 0 30 Angle (degree)

60

90

A special case is the use of curved substrates which allow the study of growth on different crystal orientations in a continuous fashion. Such experiments have been performed using cylindrical substrates [1124] and hemispherical crystals. For the latter homoepitaxy has been reported for Si [1125, 1126], SiC [1127] or GaAs [1128]. Also heteroepitaxy has been investigated, for example for GaP and GaAs on Ge [1129] (cmp. Fig. 12.12). Using such curved substrates, the growth rate can be determined as a function of crystal orientation as shown for GaAs (on GaAs) in Fig. 12.5; large differences are found for (111)A and (111)B surfaces. For growth of silicon the variations with angle are much smaller in the range of 10% [1124].

12.2.3 Growth Modes The growth of a material A on a material B can occur via three fundamental growth modes (Fig. 12.6), the layer-by-layer or Frank-van der Merwe (FvdM) growth mode [435], the island or Volmer-Weber (VW) growth mode [1130] and the Stranski-Krastanow (SK) growth mode [1131, 1132]. In [1132] the possibility of island formation on an initially flat heteroepitaxial surface was proposed for the growth of lattice-matched ionic crystals that have different charges. The term SK growth is now typically used in lattice-mismatched heteroepitaxy for the island formation (and related relaxation of strain energy, cmp. Fig. 14.37) on an initially two-dimensional layer (wetting layer).2 Also growth of islands relaxed by misfit dislocations in strained heteroepitaxy has been termed SK growth [1133]. The growth mode is determined by the relation of the free energies (per area) of the surface σs , interface σi and film σf . Wetting of the substrate and growth of a coherent film (FvdM-growth) occurs for (12.1) σs > σi + σf . If the inequality has the opposite sign, Volmer-Weber or Stranski-Krastanow growth occurs. Additionally the strain energy of the film must be considered. The SK growth generally occurs when there is wetting of the substrate but layer strain is unfavorable and leads to islanding. Layer-by-layer growth typically involves nucleation of two-dimensional islands and ‘filling’ of the remaining monolayer before the next one is started. Another growth mode resulting in smooth

2 This

is the growth mode of self-assembled epitaxial quantum dots as discussed in Sect. 14.4.3.

356

12 Heterostructures

Fig. 12.6 Schematic of the three different fundamental epitaxial growth modes

epitaxial layers is step-flow growth where adatoms are incorporated mainly at step edges. A more detailed discusion can be found in [1134]. Further details on crystal growth can be found in [1135]. The nucleation and the initial film growth are important and determine the film quality. Several techniques have been developed to overcome common problems. A typical strategy is the growth of a low-temperature nucleation layer.

12.2.4 Heterosubstrates If homosubstrates are not available or very expensive, semiconductors are grown on dissimilar substrates, e.g., (Al,Ga)N and ZnO on sapphire (Al2 O3 ) or SiC.3 In Fig. 12.7 the interface region of hexagonal AlN on 6H-SiC (cmp. Fig. 3.31b) is shown. The change of crystallographic phase is obvious; the perfect atomic arrangement justifies the term ‘epitaxy’, literally meaning ‘order on top’. In many cases, the integration of III–V- or II–VI-based semiconductors for optoelectronic applications on silicon for electronic devices is desirable, such as GaAs/Si, InP/Si, GaN/Si or the growth on economic substrates is attractive such as GaN/Al2 O3 and ZnO/Al2 O3 . For all such combinations the epitaxial relationship, i.e., the alignment of the crystallographic directions of both materials, which can have different space groups, has to be considered. Some examples for epitaxial relationships are given in Table 12.1. The epitaxial relation is determined by the energetically favorite formation of the interface and the early stages of growth. In Fig. 12.8, X-ray diffraction data are shown from a ZnO layer on c-oriented sapphire. The hexagonal ZnO lattice is rotated by 30◦ with respect to the trigonal sapphire lattice. In the case of growth of ZnO on Si(111) an amorphous SiO2 layer can form at the interface such that the crystallographic information of the substrate is lost. The ZnO grains exhibit random in-plane orientation (Fig. 12.9).

Fig. 12.7 HRTEM cross section of the interface region of MOVPE grown hexagonal AlN on 6H-SiC substrate. Adapted from [1137]

2H-AlN

6H-SiC 1nm

3 For

ZnO, homosubstrates have recently been produced with 3-inch diameter [1136].

12.2 Heteroepitaxy

357

Table 12.1 Epitaxial relationship for various film/substrate combinations, ZnO (or GaN) on c-, a- and r -sapphire and Si(111) ZnO

Al2 O3 [00.1]

ZnO

Al2 O3 [11.0]

ZnO

[00.1] [11.0]

[00.1] [01.0]

[00.1] [11.0]

[11.0] [00.1]

[11.0] [00.1]

Fig. 12.8 X-ray diffraction intensity from the asymmetric ZnO (10.4) (upper panel) and the sapphire (10.10) (lower panel) reflections as a function of the azimuthal sample orientation (rotation angle φ around the [00.1] axis). The peaks appear at different tilt angles ω due to an overall tilt of the mounted sample (dashed sinusoidal lines). The ZnO [00.1] axis is not tilted with respect to the sapphire [00.1] direction

Al2 O3 ¯ [10.2] ¯ [10.2] ¯ [01.1]

ZnO / GaN

Si [111]

[00.1] ¯ — / [21.0]

[111] ¯ [110]

Tilt

(deg)

0.4

=30°

0.2 0 -0.2 -0.4

ZnO (1 0.4)

Tilt

(deg)

0.4 0.2 0 -0.2 -0.4 -180

Al2O3 (1 0.10) -90

0

90 (deg)

180

If substrate and epilayer have different space groups, the formation of domains can occur [1139]. The two-dimensional symmetries of various substrates are listed in Table 11.1. The group theoretical minimum number of domains NRD in dependence of the two-dimensional symmetries of substrate and epilayer with rotational symmetries Cn and Cm , respectively, is given by [1140] NRD =

lcm(n, m) , m

(12.2)

where lcm denotes the least common multiple. The values are listed in Table 12.2 and visualized in Fig. 12.10. If the main symmetry axes of substrate and epilayer are not aligned, mirror domains appear. An example is the growth of GaN(00.1) on Ge(111), for which it has been reported that the major symmetry directions do not align exactly. There is a 4◦ in-plane rotation of the lattices with respect to the usual ¯ in-plane relationship [1141] (cmp. the exact alignment for GaN/Si(111) in Table 12.1). [11.0] [110] Due to 3 m mirror symmetry of the substrate, the misaligment is equivalent for clockwise and counterclockwise rotation. Therefore two domains with an angle of 8◦ occur (Fig. 12.11). Another well-known domain effect in heteroepitaxy is the occurence of antiphase domains of zincblende semiconductors (e.g., GaAs, GaP, InP, . . .) grown on Si(001) with monoatomic steps;

358

12 Heterostructures

Fig. 12.9 a Plan-view TEM image (inset: electron diffraction diagram averaged over several grains) of ZnO on Si(111). b Cross-sectional TEM of the same sample. c High-resolution cross-sectional image of the ZnO/SiO2 /Si interface region. Adapted from [1138] (a)

ZnO

Si

(b) Si

SiOx

ZnO

Fig. 12.10 Visualization of the minimum number of rotational domains for different substrate and epilayer symmetries according to Table 12.2

epi

(c)

sub 2

3

4

6

2

3

4

6

12.2 Heteroepitaxy

359

Table 12.2 Number of rotational (or mirror) domains NRD for all 2D point groups of substrate (G S ) (rows) and epilayer (G E ) (columns). When two numbers are given (x|y), the first (second) number represents the number of domains if mirror symmetry planes of substrate and epilayer align (misalign) 1

m

2

2mm

3

3m

4

4 mm

6

6 mm

1 m 2 2 mm 3 3m 4 4 mm 6 6 mm

1 2 2 4 3 6 4 8 6 12

1 1|2 2 2|4 3 3|6 4 4|8 6 6|12

1 2 1 2 3 6 2 4 3 6

1 1|2 1 1|2 3 3|6 2 2|4 3 3|6

1 2 2 4 1 2 4 8 2 4

1 1|2 2 2|4 1 1|2 4 4|8 2 2|4

1 2 1 2 3 6 1 2 3 6

1 1|2 1 1|2 3 3|6 1 1|2 3 3|6

1 2 1 2 1 2 2 4 1 2

1 1|2 1 1|2 1 1|2 2 2|4 1 1|2

Fig. 12.11 X-ray diffraction φ-scans of GaN(00.1)/Ge(111). Adapted from [1141]

X-ray Intensity (arb. units)

G S \G E

GaN(10.1) Ge(220)

0

=8°

90

(degree)

180

270

such surface actually exhibits two kind of terraces (1 × 2 and 2 × 1 reconstructions) and is thus itself not homogeneous. The formation of antiphase domains can be avoided by using an off-cut of the surface against the (001)-planes promoting double-atomic steps [1142]. In Fig. 12.12a the growth of GaP on a Ge hemisphere with [111]-pole is depicted; spherical triangles meeting at the 100 poles can be seen. In a similar experiment GaAs was grown in a spherical depression in Ge(001) (Fig. 12.12b), allowing a more detailed look at the [001]-pole. Close to the it, within an approximately square area, antiphase domains (cmp. Sect. 4.4.4) form. Along the connection lines between different 001-poles, an antiphase domain boundary forms, microscopially broken up into domains [1129]. Details of the initial deposition steps can determine the orientation in polar materials. GaN directly grown on c-Al2 O3 grows with N-face orientation (see Fig. 3.19). The high surface mobility of Ga allows nitrogen to take its preferred position in the first atomic layer. Even under Ga-rich conditions the N atoms can kick-off the Ga from its favorite site on the surface. If an AlN buffer is used the strong bond between Al and oxygen leads to an Al atomic layer at the interface and subsequent GaN grows with a Ga-face [1143]. Also for the epitaxy of ZnO on on c-Al2 O3 the polarity of the epilayer can be controlled, e.g., via the details of an MgO buffer layer [1144].

12.2.5 Patterned Substrates Using patterning of the substrate certain growth modes and crystallographic directions of the growth front can be evoked.

360

12 Heterostructures

Fig. 12.12 The morphology of a GaP grown on a Ge hemisphere with [111]-pole and b GaAs grown in a Ge(001) spherical depression. Adapted from [1129]

(a)

Fig. 12.13 Side view of the heterointerfaces between AlN and c-oriented sapphire with nitrogen (a) and Al (b) being the first layer. Adapted from [1143]. c Phase image of piezoresponse force microscopy (PFM) of lateral polarity GaN heterostructure and d linescan of phase signal along white line in part (c). Adapted from [1146], part (c) reprinted with permission, ©2002 AIP

(b)

10µm

(c)

(a)

(b)

(d)

¯ growth of wurtzites, on a sapphire substrate with Returning to the discussion of [00.1] or [00.1] lateral AlN patterns, laterally orientation-modulated GaN can be grown (Fig. 12.13). At the juncture of the phases an inversion domain boundary forms [1145]. The defect density can be reduced in parts of the structure using pendeo-epitaxy [1147] or epitaxial lateral overgrowth (ELO) [1148]. The defects thread only from the limited contact area of the layer with the substrate and the part of the layer away from the mask (‘wing’) is free of defects (Fig. 12.14). While the patterning of a mask may be cumbersome and require interruption of growth, the insitu deposition of a random SiN mask with small holes has been found beneficial in the epitaxy of GaN [1149]. GaN islands nucleate selectively in the mask openings (Fig. 12.15a). The nucleation and subsequent coalescence of islands (Fig. 12.15b) leads to defect annihilation and eventually again to a flat film (Fig. 12.15c). The reduction of defect density is evident (Fig. 12.15d) and leads to improved optical properties [1150].

12.2 Heteroepitaxy

361

Fig. 12.14 SEM cross-sectional image of GaN grown on a structured Si(111) substrate. The laterally grown wings extend about 2.5 µm over the grooves. The thickness of the GaN layer is 0.5 µm on the bottom of the grooves, while it is 1.4 µm on top of the ridges. Reprinted with permission from [1148], ©2001 AIP

(a)

(b)

(c)

GaN

SiN mask GaN

(d)

sapphire

Fig. 12.15 SEM images of GaN a growing through the openings of a random SiN mask, b laterally overgrowing the mask and coalescing and c eventually forming a flat film. Bar widths are 2 µm, 1 µm and 10 µm. d Cross-section TEM image. Adapted from [1149]

Using patterned substrates with stripe-like mesas and promoting the growth on a sidewall of the mesa, the direction of GaN growth front can be steered into a semipolar direction (cmp. Sect. 16.4.3). The r-plane sapphire substrate with etched mesa stripes oriented along the [11.0] direction exposes [00.1]-oriented sidewall facets on which the GaN grows along its c-axis; The angle of 57.6◦ between the r- and the c-planes of sapphire is very close to the angle (3.22c) of 58.4◦ between the GaN semipolar (11.2) and the (00.1) plane. The flat growth front represents a (11.2) facet [1151] (Fig. 12.16). After coalescence of grains from various mesas, a flat (11.2) surface arises, allowing the reduction of various defects including basal stacking faults [1152, 1153].

362

12 Heterostructures

Fig. 12.16 SEM cross-sectional image of MOVPE GaN grown on patterned r-sapphire exposing a (11.2) growth front. Based on SEM image courtesy of F. Tendille

GaN

[11.2] C [00.1] [11.3] M [11.0]

R [11.2] C [00.1]

A [11.0]

r-Al2O3

1 µm

Fig. 12.17 Optical image of the surface of a supercritical, plastically relaxed Inx Ga1−x As film on GaAs. Image width is about 1 mm. The cross-hatch pattern is due to misfit dislocations along ¯ A [110] and [110]. pseudomorphic layer would exhibit no contrast under the given conditions

12.2.6 Pseudomorphic Structures Heterostructures can generally be made from any sequence of materials. However a mismatch in lattice constant (or a different crystal structure) leads to strains and stresses that are of the order of 103 atmos for strains of 1% (σ ∼ C, C ≈ 5 × 1010 Pa) as discussed in Sect. 5.3.3. The total strain energy is ∝ C2 . Above a critical thickness h c ∝ −1 (cf. Sect. 5.4.1) defects, e.g., misfit dislocations (relaxing strain with their edge components), are generated (Sect. 12.2.7). There are a number of semiconductor combinations that are lattice matched and thus can be grown with arbitrary thickness. Alx Ga1−x As is closely lattice matched to GaAs for all Al concentrations. See Fig. 6.25 for lattice-matched pairs, e.g., In0.53 Ga0.47 As/InP. Often, thin layers of lattice-mismatched materials with thickness smaller than the critical thickness are used. For many device applications the ability to grow pseudomorphic layers thicker than the critical layer thickness would be beneficial. The use of compliant substrates was proposed in [1154] to meet this demand. A recent review on compliant substrate technologies can be found in [445]. Schemes

12.2 Heteroepitaxy

363

Fig. 12.18 Average film strain (measured in-situ via substrate curvature) of In0.15 Ga0.85 As/GaAs grown at 450 ◦ C as a function of film thickness (determined from growth time × deposition rate). Relaxation for three different growth modes are shown (as labeled): continuous growth, employment of several growth interruptions (GRI) and GRI with annealing step (to 550◦ ). Adapted from [1155]

to accommodate part of the mismatch strain in the substrate include the use of cantilevered membranes, silicon-on-insulator, twist bonding, glass bonding or trenched substrates. In this sense also nanowhiskers (Sect. 14.2.3) represent a compliant substrate, enabling the growth of coherent (laterally confined) layers thicker than the critical thickness of a 2D layer (cmp. Fig. 14.8).

12.2.7 Plastic Relaxation Above the critical thickness, a film will relax plastically by forming defects, often misfit dislocations. A cross-hatch pattern at the surface due to misfit dislocations is shown in Fig. 12.17 (cf. also Sect. 4.3.1.4). The strain relaxation in mismatched heteroepitaxy can be determined experimentally via the wafer curvature of the heterostructure (Sect. 5.3.5). Data for the thickness dependent relaxation (d) of In0.15 Ga0.85 As on GaAs (mismatch ≈ 1%) are shown in Fig. 12.18. Growth interruptions lead to larger relaxation at smaller thickness. Therefore relaxation at early times or small thickness (above h c ) is kinetically hindered, i.e., the available dislocation density and glide velocity are not sufficient to relieve the strain. At large thickness the strain does not go to zero (saturation regime) and the film remains in a metastable, incompletely relaxed state as discussed in more detail in [1155]. An extreme case of plastic relaxation is cracking (Sect. 4.4.1) which can occur for example in thick films during cooling due to the mismatch of the thermal expansion coefficients of substrate and epilayer (Fig. 12.19). Such cracking can be avoided by the introduction of suitable stress-relaxing layers and growth on predefined mesas [1156, 1157].

12.2.8 Surfactants The condition (12.1) allows layer-by-layer growth (cf. Sect. 12.2.3), i.e., the substrate surface free energy is higher than the than the total of interface and film surface free energy. This makes wetting energetically favorable. For two elements A and B, one of them must have the lower surface free energy. If A can be grown on B in Frank-van der Merwe (or Stranski-Krastanow) growth mode, then (12.1) does not hold for B on A and the growth will occur in Volmer-Weber mode, i.e., with islands.

364

12 Heterostructures

Fig. 12.19 1 × 1 mm2 top view with a differential interference contrast microscope of a 1.3 µm thick GaN layer grown on Si(111). Reproduced with permission from [1156], ©2000 IPAP

Fig. 12.20 a, b 10 nm thick Ge layer on Si (100) deposited at room temperature with MBE and annealed up to 770 ◦ C without (a) and with (b) Sb surfactant. Adapted from [1165]. c Cross-section TEM image of a heterostructure of 70 monolayers germanium on Si (111), grown by MBE with Sb surfactant. The horizontal arrow labeled ‘I’ denotes the position of the interface. The arrows labeled ‘D1’ and ‘D2’ denote the positions of partial dislocations (cmp. Fig. 4.20). Adapted from [327]

This is a serious problem for the growth of embedded layers of the type A–B–A. If the embedded film grows well, the capping does not and vice versa. In the case of Ge on Si, Ge has the lower surface free energy than Si. Ge grows on Si in StranskiKrastanow mode [1158] (Fig. 12.20a). Si grows both on Ge(001) and Ge/Si(001) in a Volmer-Weber mode [1159] causing severe problems for the fabrication of Si/Ge/Si quantum wells or superlattices. A substantial modification of growth mode can be achieved by using a third element C as a capping layer, saturating surface bonds. It lowers the surface free energy of both materials A and B, thus favoring wetting of the substrate. Such element C is called surfactant (surface-active species) [1160, 1161]. Typical examples are As [1160] or Sb [327] on Si and Ge (Fig. 12.20b). Also the surfactant modifies defect nucleation and can lead to defect-free epitaxial Ge/Si layers (Fig. 12.20c). Surfactants have also been described for the growth of compound semiconductors, e.g., In [1162] or Sb [1163, 1164] for GaAs.

12.3 Energy Levels in Heterostructures

365

12.3 Energy Levels in Heterostructures 12.3.1 Band Lineup in Heterostructures In heterostructures, semiconductors with different band gaps are combined. The relative position of conduction and valence band (band alignment) is determined by the electron affinities χ as shown in Fig. 12.21. For a semiconductor, the electron affinity is the (positive) energy difference between vacuum level and conduction band edge. It can lead to different types of heterostructures. Early perspectives of semiconductor heterostructures are discussed in [1166]. The band alignment can be estimated from the position of the branch point energies (Sect. 7.8) of the two constituents [699] but additional interface dipoles may have to be considered. In Fig. 12.22, the band alignment for type-I, type-II and type-III heterostructures are shown. In the type-I structure (straddled band lineup) the lower conduction-band edge and the higher valence-band edge are both in the material with smaller band gap. Thus, electrons and holes will localize there. In the type-II structure a staggered lineup is present and electrons and holes will localize in different materials. In the type-III structure, also termed ‘broken gap’ structure, the conduction band of one material is below the valence band of the other material. The technologically most relevant are type-I structures. The design of heterostructures to fulfill a certain device functionality or to have certain physical properties is called ‘band gap engineering’.

Fig. 12.21 Position of conduction and valence-band edges for a variety of semiconductors (relative to a common vacuum level at E = 0 eV). Based on values from [1167], and from Al2 O3 (on InP) [1168], InN on diamond [1169], InN on MgO [1170], Ga2 O3 on GaN from [1171], and In2 O3 on Si from [1172, 1173]. On the right hand side, the work functions of several metals are shown for comparison

(a) type-I

(b) type-II

(c) type-III

Evac 2

2

2 1

1

1

Electron energy

Fig. 12.22 Position of band edges (band alignment) in a type-I, b type-II and c type-III heterostructure

EC

Eg2

Eg2 Eg1

Eg2

Eg1

EC,V Eg1

EV

Spatial coordinate

366

12 Heterostructures

(a)

(b)

Fig. 12.23 a XPS measurements of InN and GaN and a InN/GaN heterostructure. The vertical dashed lines indicate the core level positions in the bulk (black) and the heterostructure (red). The valence band offset is given by E V = E core,HS − E core,bulk (when E V is set to zero for both the bulk materials). b Schematic band lineup of the type-I InN/GaN heterojunction (all energies in eV). Adapted from [1174]

In a type-I heterostructure, the conduction- and valence-band discontinuities are given, respectively, by E C = χ1 − χ2

(12.3a)

E V = (χ1 + E g1 ) − (χ2 + E g2 ) .

(12.3b)

Experimentally, the valence band offset can be determined using X-ray photoelectron spectroscopy (XPS) probing the filled states; together with the band gap then also the conduction band offsets are obtained. As example, in Fig. 12.23a the binding energies of an indium and a gallium core level are shown with the valence band edges of InN and GaN, respectively, set to zero energy. Both core levels are then also investigated in a 5 nm InN on GaN heterostructure (the InN layer is sufficiently thin to allow photoelectrons to escape from the GaN underneath). The sum of the shifts represents the valence band offset (E V = 0.58(8) eV from the analysis of several core levels [1174]). Together with the band gaps, the conduction band offset results in E V = 2.22 eV as schematically depicted in Fig. 12.23b. Depending on the layer sequence of high- and low-bandgap materials various configurations, as shown in Fig. 12.24 have obtained special names, such as single heterointerface, quantum well (QW), multiple quantum well (MQW), superlattice (SL). In the extreme case the layer is only one monolayer thick (Fig. 12.25) and the concept of layer and interface blurs. Such atomically precise layer sequences are mastered nowadays for a variety of material systems such as (Al,Ga)As/GaAs/InAs, InP/(In,Ga)As, Si/SiGe, ZnO/(Mg,Zn)O and also BaTiO3 /SrTiO3 . The abruptness of interfaces is determined by the epitaxial machine through the switching precision of the incoming material flux and fundamentally limited by segregation phenomena which can be modeled with a segregation coefficient [1175] (cmp. Sect. 4.2.4). As shown in Fig. 12.25c, In has the tendency to be carried into the following GaAs layer. A quantitative evaluation is possible using aberration-corrected scanning transmission electron microscopy [1176].

12.3 Energy Levels in Heterostructures

(a)

367

(b)

(c)

(e)

(d)

Fig. 12.24 Heterostructures with different layer sequences (band gap engineering). a quantum well (QW), b multiple quantum well (MQW), c superlattice (SL), d single-barrier tunneling structure, e double-barrier tunneling structure Fig. 12.25 Ultrathin heterostructures: a Cross-sectional TEM of a MOVPE-grown short-period superlattice (SPS) of InAs layers in GaAs1−x Nx ). In high resolution (right image), the individual rows of atoms can be seen. From [1177]. b, c Cross-section STM image of 2 ML InAs on GaAs; the segregation of In into the top layer is visible atom by atom. Adapted from [1178]

InAs

(a)

368

12 Heterostructures

Fig. 12.26 Schematic energy levels and wavefunctions in a potential well with a infinite barriers, and b finite barrier height

n=3

n=2

n=2

n=1

(a)

Lz

n=1

(b)

Lz

12.3.2 Quantum Wells The energy in a single quantum well of thickness L z (along the growth direction z) can be calculated with the quantum-mechanical particle-in-a-box model. In the envelope function approximation (Appendix I) the wavefunction is written as a product of the Bloch function and the envelope function χ(z). A,B (r) = exp (i k⊥ r) u nk (r) χn (z) ,

(12.4)

where ‘A’ and ‘B’ denote the two different materials. The envelope function χ fulfills, approximately, the one-dimensional Schrödinger-type equation, 2 ∂ 2 − ∗ 2 + Vc (z) χn (z) = E n χn (z) , 2m ∂z

(12.5)

where m ∗ denotes the effective mass. Vc is the confinement potential determined by the band discontinuities. Typically, Vc = 0 in the well and V0 > 0 outside in the barrier. E n are the resulting energy values of the quantized levels. In the case of infinite barriers (V0 → ∞, Fig. 12.26a) the boundary conditions χ(0) = χ(L z ) = 0 yield nπ 2 Lz nπ z , χn (z) = An sin Lz En =

2 2m ∗

(12.6) (12.7)

where E n is called the confinement energy. For finite barrier height V0 (Fig. 12.26b) the calculation leads to a transcendental equation. The wavefunction tunnels into the barrier. While for infinite barrier height the lowest level diverges for L z → 0, for finite barrier height E 1 → V0 . A complication arises from the different effective mass in the well and barrier material. This is taken into account by forcing the continuity of χ and χ /m ∗ across the interfaces4 (‘BenDaniel-Duke’ boundary conditions [1180]). The Schrödinger equation and 4 The

kinetic energy term in (12.5) is written as

1 ∂χ 2 ∂ 2 ∂z m ∗ (z) ∂z

for varying mass across the structure [1179].

12.3 Energy Levels in Heterostructures

369

Fig. 12.27 Schematic representation of the development of hole levels in a quantum well: a degenerate bulk levels at , b splitting at the subband edge (due to different quantized values of k z ), c in-plane dispersion (mass reversal), d anticrossing behavior. Based on [1123]

(semi-)analytical solutions for special and numerical methods for arbitrary potential distributions are discussed in [1181]. The application of k · p theory (Appendix H) to heterostructures is discussed in [1182]. The motion of carriers in the plane is still free and has a two-dimensional dispersion. Thus, each quantized level contributes m ∗ /(π2 ) to the density of states at each subband edge E n . For holes, the situation is a little more complicated than for electrons (Fig. 12.27). First, the degeneracy of heavy and light holes is lifted since their mass enters the confinement energy. The effective hole masses along the z direction, i.e., those that enter (12.5), are 1 z = γ1 − 2 γ2 m hh 1 z = γ1 + 2 γ2 . m lh

(12.8a) (12.8b)

The light holes have the higher quantization energy. The angular momentum is quantized along the z direction. The transverse masses for the dispersion in the interface plane are 1 x y = γ1 + γ2 m hh 1 x y = γ1 − γ2 . m lh

(12.9a) (12.9b)

Now the heavy hole, i.e., the Jz = ± 23 state, has the smaller mass and the light hole (Jz = ± 21 ) the larger (Fig. 12.27c). However, this consideration is only an approximation since the lifting of degeneracy and the dispersion have to be treated on the same level. Higher terms of the perturbation calculation lead to band mixing and remove the band crossing that seems to originate from the situation at the point. In reality, the bands show anticrossing behavior and are strongly deformed. The hole dispersion in a superlattice and the anticrossing behavior is shown in Fig. 12.28. Experimentally observed transition energies in quantum wells of varying thickness are shown in Fig. 12.29 and are in good agreement with the theoretical calculation. We note that for infinite barriers optical transitions are only allowed between confined electron and hole states with the same quantum number n. For finite barriers this selection rule becomes relaxed, and other transitions become partially allowed, e.g., e1 –hh3 . The optical matrix element from the Bloch part of the wavefunction, which was isotropic for (cubic) bulk material (9.37), is anisotropic for quantum wells. TE (TM) polarization is defined with the electromagnetic field in (perpendicular to) the plane of the quantum well (Fig. 12.30a). At the subband edge, i.e., for in-plane wavevector k|| = 0 the matrix elements for the various polariza-

370 Fig. 12.28 Hole dispersion in a 68-ML GaAs/71 ML Al0.25 Ga0.75 As superlattice (numerical calculation). The double curves originate from a lifting of time-reversal symmetry at k = 0. Reprinted with permission from [1183], ©1985 APS

12 Heterostructures 0

hh1 hh2

-10

GaAs/ AlGaAs

lh1

hh3

-20 hh4 lh2

-30 0.04 0.03 0.02 0.01 [110]

0

0.01 0.02 0.03 0.04 [100]

Fig. 12.29 Observed electron–hole transitions (energy difference to the first e–h transition from excitation spectroscopy) in GaAs/(Al,Ga)As quantum wells of varying thickness. Symbols are experimental data, solid lines are theoretical model. Data from [1184]

tions and propagation directions are given in Table 12.3. The matrix elements averaged over all in-plane directions for TE-polarization are 3/2Mb2 (1/2Mb2 ) for the electron to heavy (light) hole transition. For TM polarization the values are 0 and 2Mb2 , respectively [1185]. The optical selection rules are shown in Fig. 12.30 (see Fig. 9.12 for bulk material). For propagation along the quantum-well plane, the ratio between the strength of the TE polarized e–hh and e–lh transitions is 3:1. The confinement potential squeezes charge carriers bound to impurities closer to the ion. Therefore, the binding energy increases as shown in Fig. 12.31. This behavior can be modeled theoretically with good precision. It makes a difference whether the impurity is located at the center or the interface of the quantum well. The confinement potential also squeezes electrons and holes in the exciton closer together and thus increases their Coulomb interaction. The binding energy of the quantum-well exciton is thus larger than in bulk material and depends on the well width (Fig. 12.32). In the simple hydrogen-like model with infinite barriers the exciton binding energy is 4 times the bulk binding energy in the limit L z → 0.

12.3 Energy Levels in Heterostructures

371 mj

1/2

1/2

1/2

1/2

lh

lh

electrons

TM TE

mj

TE

(a)

(b)

3/2 hh

3/2

holes

hh

Fig. 12.30 a Directions of electric-field vector relative to the quantum-well plane for TE and TM polarization. b Optical selection rules for band–band transitions in a quantum well. If the (in-plane averaged) relative strength of the e–hh transitions (solid lines) is 1, the relative strength of the TE-polarized e–lh transitions (dashed lines) is 1/3 and that of the TM-polarized e–lh transitions (dash-dotted lines) is 4/3 Table 12.3 Squared momentum matrix elements |c|ˆe · p|v|2 in a quantum well for various propagation directions in units of Mb2 . The quantum-well normal is along z e–hh

e–lh

e–so

Propagation

eˆ x (TE)

eˆ y (TE)

eˆ z (TM)

x y z x y z x y z

– 1/2 1/2 – 1/6 1/6 – 1/3 1/3

1/2 – 1/2 1/6 – 1/6 1/3 – 1/3

0 0 – 2/3 2/3 – 1/3 1/3 –

GaAs/Al Ga As

40

35

30

25 5

10 0

15

20

25

30

35

Fig. 12.31 Experimental values for the acceptor binding energy in GaAs/Al0.3 Ga0.7 As quantum wells (solid circles) from [1186] as a function of well width. Solid line is theory (variational calculation) for the well-center acceptor including top four valence bands and finite barriers, dashed line is hydrogen-like model with infinite barrier height. Adapted from [1187]

372

12 Heterostructures

15

Al0.4Ga0.6As/GaAs

InGaAs/ GaAs

10 9

10

5 0

8 mb m w , b mb mw , b= mb=mw , b mb=mw , b=

7

w w w

6

w

10

5

0

15

(a)

W

(b)

z

5

10

Fig. 12.32 a Theoretical (variational) calculation (solid line) of the heavy-hole exciton binding energy versus QW thickness in a GaAs/Al0.4 Ga0.6 As quantum well (using also different approximations, other lines). Adapted from [1188]. b Experimental exciton binding energy in Inx Ga1−x As/GaAs quantum wells of different thickness. Circles: data and error bars from [1189], x unspecified, squares: data from [1190], x = 0.18 0.45 0.40

E4

0.35 0.30 0.25

E3

0.20 0.15 E2

0.10 0.05 0 0

E1 1

2

3

4

5

6

7

8

9

10

Fig. 12.33 Band structure of a superlattice with a potential depth of 0.4 eV and well and barrier width w (L QW = L barr ). Adapted from [1191]

In a realistic calculation the effect of different dielectric constants in the well and barrier (image charge effect) need to be considered.

12.3.3 Superlattices In a superlattice, the barrier thickness is so small that carriers can tunnel in neighboring wells or, in other terms, that there exists a significant wavefunction overlap between adjacent wells. This leads to a band structure (Fig. 12.33), similar to the Kronig-Penney model (Appendix F). For the superlattice the bands are called minibands, the gaps are called minigaps. The density of states does not make a step at the subband edge but follows an arccos function. The modification of the density of states, as seen in the absorption spectrum, are shown in Fig. 12.34 for 1, 2, 3 and 10 coupled wells.

12.3 Energy Levels in Heterostructures

373

Fig. 12.34 Absorption spectra of a single, double, triple and ten coupled quantum wells. Theoretically predicted transitions with heavy (light) holes are labeled with filled (empty) bars at their respective transition energies. Adapted from [1192] Fig. 12.35 Schematic formation of a triangular potential well in a n-(Al,Ga)As/n-GaAs heterostructure, a before and b after equilibration of Fermi levels

AlGaAs

Ec

GaAs

Ec

Ev

Ev (a)

(b)

12.3.4 Heterointerface Between Doped Materials We consider a single heterointerface between n-doped materials. As an example we take n-(Al,Ga)As/nGaAs (Fig. 12.35). First, we consider the materials without contact, forming a type-I structure. In thermodynamic equilibrium the system must have a constant Fermi level. Thus, charge is transferred from the region close to the interface from (Al,Ga)As to GaAs. This results in the formation of a triangular potential well in the GaAs close to the interface. A two-dimensional electron gas (2DEG) forms in this potential well (Fig. 12.36). The charge transfer in thermodynamic equilibrium adjusts the band bending and the charge density (quantized levels in the well) in such a way that they are self-consistent. The Poisson equation and the Schrödinger equation are simultaneously fulfilled. Numerically, both equations are iteratively solved and the solution is altered until it is self-consistent, i.e., it fulfills both equations.

374

12 Heterostructures

If the region of the 2DEG is not doped, the electron gas exists without any dopant atoms and ionized impurity scattering no longer exists. This concept is called modulation doping. Mobilities up to 3.1 × 107 cm2 /Vs have been realized (Fig. 12.37). The theoretical limits of mobility in a 2DEG at modulation-doped (Al,Ga)As/GaAs heterointerfaces are discussed in detail in [1194].

12.3.5 Heterointerface Between Semiconductors with Band Structures of Different Topology Let us remember the situation of the topological linear chain developing end states when sandwiched between trivial material (cf. Sect. 5.2.10). Also surface states develop between a material with nontrivial topological band structure and vacuum (which is trivial) (cf. Sect. 11.6.3). These effects are expression of the bulk-boundary correspondence, which says that at the interface of topologically different materials, edge states develop. If now a semiconductor heterointerface is made up from two topologically differnt materials, a conductive interface channel is expected. This effect has been found for the HgTe/CdTe system where HgTe represents the non-trivial material with inverted band structure. (cf. Sect. 6.11). A quantum well structure was proposed where HgTe is sandwiched between layers of Hgx Cd1−x Te [1196]. Taking the electron and hole quantization effects into account, normal band order is present for thickness of the HgTe layer up to a critical thickness of dc = 6.35 nm (for x = 0.32) and the sample should be insulating. For thicker QWs, the two-dimensional bands invert and edge states arise. The quantized electrical conductance due to the edge states was indeed found and measured [1197, 1198].

Fig. 12.36 a Conduction-band edge at a GaAs/Al0.3 Ga0.7 As heterointerface (T = 0 K) with two confined states at E 0 and E 1 marked with solid horizontal lines. In the GaAs channel there are 5 × 1011 cm−2 electrons. The barrier height is 300 meV, NDGaAs = 3 × 1014 cm−3 . The position of the Fermi level E F is at E = 0 and indicated with a dash-dotted line. b Envelope wavefunctions φ0 and φ1 of the two confined states, dash-dotted line: calculation without exchange and correlation for state at E 0 . Adapted from [1193]

12.4 Recombination in Quantum Wells

375

Fig. 12.37 Progress in the achievement of high electron mobility in GaAs, annotated with the technical innovation responsible for the improvement. Adapted from [1195], reprinted with permission, ©2003 Elsevier B.V

12.4 Recombination in Quantum Wells 12.4.1 Thickness Dependence The energy of exciton recombination in quantum wells is blue-shifted with respect to that in bulk material due to the quantum-confinement energies of electrons and holes (Fig. 12.38). The electron– hole recombination lineshape in quantum wells is given by the product of the joint density of states and the Boltzmann function (when Boltzmann statistics apply). The JDOS is given by a step function (Heavyside function H (E)). E , I (E) ∝ H (E − E 11 ) exp − kT

(12.10)

where E 11 = E g + E e1 + E h1 represents the energy of the E1–H1 subband edge as shown in Fig. 12.38. An experimental spectrum (Fig. 12.40a) shows that excitonic effects influence the recombination lineshape in a GaAs quantum well even at room temperature [1199]. The recombination decay constant of excitons decreases with decreasing well width, partly due to the increase of exciton binding energy as discussed in [1200].

12.4.2 Broadening Effects Many-Body Effects At high carrier densities when the electron (quasi-) Fermi level is above the electron subband edge, the spectrum broadens and reflects the Fermi–Dirac distribution (Fig. 12.40b). At low temperatures

376

12 Heterostructures

AlGaAs

QW1

AlGaAs

Ee2

GaAs AlGaAs

Ee1

EC Eg E11 E22

Eh1 Eh2

Eg EV

(b)

barr

(c) PL-intensity (arbitrary units)

E

QW2

QW2

QW1

AlGaAs *1000

1.5

(a)

GaAs/AlGaAs

1.6

1.7 Energy (eV)

1.8

1.9

Fig. 12.38 a Schematic energy diagram of a quantum well with confined electron (e1, e2) and hole (h1, h2) states and recombination between them at energies E 11 and E 22 . b Schematic sample structure with two GaAs/Alx Ga1−x As quantum wells with thicknesses 3 nm and 6 nm. c Photoluminescence spectrum (T = 300 K) of the structure from part (b). A small amount of barrier luminescence appears at 1.88 eV, according to x = 0.37 (cf. Fig. 6.24c)

a many-body effect, multiple electron–hole scattering with electrons at the Fermi edge, leads to an additional peak, termed Fermi-edge singularity that is discussed in [1201]. Homogeneous Broadening The temperature dependence of the homogeneous broadening of quantum well luminescence has been investigated in [1202]. It follows the dependence of the broadening known from bulk material (Sect. 9.7.7) with similar values for the LO broadening parameter. In Fig. 12.39a the reflectance spectra for different temperatures of a 17 nm GaAs/Al0.3 Ga0.7 As QW are shown. The optical phonon broadening parameter for various well widths is shown in Fig. 12.39b and coincides with the bulk value. The homogeneous broadening leads to excitons with in-plane center-of-mass wave-vector K = 0 being allowed to recombine radiatively. This leads to a linear increase of exciton lifetime as demonstrated for GaAs quantum wells up to 50 K in [1200]. In [1203] all exciton wave-vectors within the light cone are considered, explaining the linear increase of exciton lifetime in (non-polar) ZnO quantum wells up to room temperature.

12.4 Recombination in Quantum Wells Fig. 12.39 a Reflectance spectra at various temperatures from a 17 nm thick GaAs/Al0.3 Ga0.7 As quantum well. The inset shows the temperature dependence of the homogeneous linewidth. b LO phonon broadening parameter (FWHM) for various quantum well widths. Adapted from [1202]

377

(b)

(a)

InGaAs/InP

T=80K

104 GaAs/AlGaAs 103

102

T=25K

E11

101 T=4.7K

100

1.50

1.55

1.60

(a)

1.65

1.70

(b)

0.82

0.84

0.86

0.88

0.90

0.92

Fig. 12.40 a Photoluminescence spectrum of a 5-nm GaAs/(Al,Ga)As quantum well at T = 300 K. The solid (dashed) line is fit with (without) excitonic effects. The two peaks are due to transitions involving heavy and light holes. Adapted from [1199]. b Photoluminescence spectra at three different temperatures as labeled of a 10-nm modulation-doped (In, Ga)As/InP quantum well with an electron sheet density n s = 9.1 × 1011 cm−2 . The electron quasi-Fermi level is Fn − (E C + E e1 ) = 44.1 meV from the subband edge. The dashed line in the T = 80 K spectrum is the lineshape from JDOS and a Fermi–Dirac distribution without enhancement at the Fermi edge. Adapted from [1201]

Inhomogeneous Broadening Inhomogeneous broadening affects the recombination lineshape. Since the interfaces of the QW are not ideally flat, the exciton averages over different quantum-well thicknesses within its volume. Also, e.g., for the GaAs/(Al,Ga)As system, the wavefunction in the (binary) quantum well tunnels into the barrier, the amount depending on the QW width, and there ‘sees’ the alloy broadening (see Sect. 10.3.3). The problem of exciton dynamics in a potential with random fluctuations has been treated in detail [1204, 1205]. A simplified picture is as follows: At low temperatures the excitons populate preferentially the potential minima. A simple lineshape5 of the QW absorption or joint density of states is given by a step function (cf. Table 9.3) at the QW band edge E 0 . The inhomogeneous broadening has a Gaussian 5 neglecting

excitonic enhancement.

378

12 Heterostructures

Fig. 12.41 a Recombination spectra (solid lines, scaled to same height) of a model quantum well for different temperatures as labeled and complete thermalization, dashed (dash-dotted) line is unperturbed (inhomogeneously broadened by σ = 20 meV) shape of the QW absorption edge. The energy scale is relative to the energy position of the unperturbed QW absorption edge at E 0 . b Theoretical energy position and c linewidth of exciton recombination from a model disordered quantum well. The high-temperature limits are marked by arrows. Parts (b, c) adapted from [1204]

(a)

(b)

(c)

probability distribution p(δ E) ∝ exp[−(δ E)2 /2σ 2 )] with δ E being the deviation from the QW band edge δ E = E − E 0 . The resulting lineshape is given by the convolution of the Gaussian with the unperturbed absorption spectrum yielding an error-function-like spectrum6 as shown in Fig. 12.41a. For complete thermalization the level population is given by the Boltzmann function. The recombination spectrum is given by the product of the absorption spectrum (or JDOS) and the Boltzmann function. It is (red-) shifted with respect to E 0 by about7 E(T ) = −

σ2 = γ(T ) kT . kT

(12.11)

This shift between emission and absorption is also called the Stokes shift. Within their lifetime, limited at least by radiative recombination, the excitons are typically unable to reach the energy position required by the Boltzmann function, but only a local minimum. Thus, their thermalization may be incomplete due to insufficient lateral diffusion. This effect is particularly important at low temperatures when thermal emission into adjacent deeper potential minima is suppressed. In this case, the red-shift is smaller than expected from (12.11). A numerical simulation [1204] yields such behavior of the energy position of the recombination line as shown in Fig. 12.41b. Simultaneously, the width of the recombination spectrum also exhibits a minimum (Fig. 12.41c). These findings are in agreement with experiments [1206, 1207]. An analytical model for temperature dependent exciton localization in the presence of disorder has been given in [1208], yielding a value 0 ≤ γ ≤ γ0 = (σ/kT )2 in (12.11).

√ z error function is defined as erf(x) = (2/ π) 0 exp −t 2 dt. 7 Formula (12.11) is exact for the product of a Gaussian and the Boltzmann function. 6 The

12.4 Recombination in Quantum Wells

379

Fig. 12.42 Photoluminescence spectrum (T = 2 K) (dots) of GaAs/ (Al,Ga)As quantum well grown by MBE with 120 s growth interruptions. Recombination is due to excitons in islands of 19, 18, and 17 monolayers (a0 /2) height. The solid line is a lineshape fit including lifetime broadening ( = 1.34 meV) and residual inhomogeneous broadening (σ = 0.04 meV) due to (Al,Ga)As barrier alloy fluctuations. Note that the energy separation of the peaks is much larger than kT . The peak doublet structure is discussed in [1199]. Adapted from [1199]

A potential fluctuation can localize an exciton laterally at low temperatures [1199] and behave like a quantum dot (cf. Sect. 14.4). Localized and delocalized excitons are separated by a boundary called the mobility edge [1209]. The transition between the two regimes is a Mott transition [1210]. Monolayer Growth Islands Under certain growth conditions, quantum wells with piecewise very flat interfaces can be fabricated. The thickness difference between such regions (with lateral extension in the µm range) is an integer monolayer. Accordingly, the recombination spectrum yields several, typically two or three, discrete lines (Fig. 12.42).

12.4.3 Quantum Confined Stark Effect The quantum confined Stark effect (QCSE, Sect. 15.1.2) in quantum wells shifts energy levels when electric fields are present along the width of the quantum well. A strong effect exists for pyroand piezoelectric material combinations such as c-axis oriented (In,Ga)N/(Al,Ga)N [1211, 1212] or (Cd,Zn)O/(Mg,Zn)O [1213, 1214] quantum wells due to the built-in electric field (cf. Sect. 16.2). The QCSE induced red-shift is larger in thicker quantum wells and goes beyond the bulk band gap of the quantum well material (Fig. 12.43b). Also the wavefunction overlap is reduced with increasing well width, leading to an increase of the radiative recombination lifetime as shown in Fig. 12.43. The pyroelectric field and the related modification of lifetime are absent in quantum wells grown on non-polar directions such as [11.0] (Fig. 12.43a).

380

12 Heterostructures

(b)

(a)

Fig. 12.43 a Radiative lifetime of electron-hole pairs in polar [00.1]-oriented In0.2 Ga0.8 N/GaN (circles) and non-polar [11.0]-oriented GaN/Al0.2 Ga0.8 N (squares) quantum wells of varying thickness. Experimental data are shown in symbols. The solid line is the (scaled) theoretical dependence of the electron-hole overlap for (In,Ga)N/GaN QWs. The dashed line is guide to the eye. The arrow denotes the recombination time constant in bulk GaN. Adapted from [1215, 1216]. b Low temperature PL peak recombination energy (solid squares) for ZnO/Mg0.3 Zn0.7 O quantum wells for various well widths L z (barrier width L B = 5 nm). Dashed line indicates dependence for internal field of 0.9 MV/cm, horizontal dashed line indicates recombination energy in ZnO bulk. Carrier lifetime determined from PL (circles), dashed line is guide to the eye. Adapted from [1214]

320 74 Gen/ Gen SL

70 -1

Fig. 12.44 Measured (full circles) and theoretical (solid lines) confined LO phonon energies in 70 Ge /74 Ge superlattices n n versus the layer thickness (number of monolayers) n. The dashed lines represent a calculation that considers intermixing at the interfaces. On the right, the energies of bulk modes for isotopically pure 70 Ge and 74 Ge are shown together with that of an 70 Ge 70 Ge 0.5 0.5 alloy. Adapted from [1217]

70

LO1 LO3 LO5 70 LO7 74 LO1 74 LO3 74 LO5

310

70 70

300

70 Ge alloy 74

Ge

290 280 270 0

10

20

30

40

bulk

12.5 Isotope Superlattices A special type of heterostructure is the modulation of the isotope content. The first kind of heterostructures made like this were 70 Gen /74 Gen symmetric superlattices [1217]. Figure 12.44 shows phonon energies determined from Raman spectroscopy for various layer numbers n. The modes are classified by 70 LOm and 74 LOm denoting the material in which the amplitude is maximal and m being the number of maxima in that medium.8 Such modes are visualized in Fig. 12.45a for a 69 GaP16 /71 GaP16 superlattice. Theoretical mode energies as a function of the superlattice period are shown in Fig. 12.45b.

8 Only

modes with odd m are Raman-active.

12.6 Wafer Bonding

381

Fig. 12.45 a Atomic displacements [Ga (filled dots) and P (open circles)] of odd-index LO modes in a 69 Ga16 P/71 Ga16 P superlattice unit cell. These modes have even parity with respect to midlayer planes, which are at atom numbers 16 and 48 in this example. The labels on the left identify the predominant character of the mode, those on the right give the relative Raman intensities with respect to that of the 69 LO1 mode. The tick marks on the vertical axis indicate zero displacement of the respective mode. b Upper panel: Energies and characters of odd-index LO phonon modes in GaP isotope SLs as calculated within the planar bond charge model for the case of ideal interfaces. 69 LOm modes are shown as open symbols; 71 LOm modes as full symbols. The shaded area marks n = 16 for which the atomic displacements of the modes are shown in part (a). Lower panel: Calculated intensities of the modes relative to that of the 69 LO1 phonon mode. Adapted from [379], reprinted with permission, ©1999 APS

12.6 Wafer Bonding Wafer bonding is a fairly recently developed method to join different and dissimilar materials. Two wafers of the respective materials are put together face to face and are adequately fused. The idea is to not only ‘glue’ the wafers together with a sticky (and compliant) organic material, but to form strong atomic bonds between the two materials with possibly a perfect interface. In some cases, the interface needs to allow charge-carrier transport through it. Less stringent conditions need to be met for photon transport. Mechanical deficiencies such as surface roughness, dust particles and the like must be avoided in the wafer-bonding process since they result in voids. Several methods have been developed for bonding various materials [1220–1222]. Such processes are successful for large substrate sizes. With proper processing, ideal interfaces can be created, as shown in Fig. 12.46. Such structures, if made between a p-doped and a n-doped semiconductor, show diode characteristics.

382 Fig. 12.46 Highresolution TEM images of wafer-bonded a Si–Si and b GaAs–Si interfaces. White circles indicate the position of misfit dislocations. Part (a) reprinted from [1218], ©2003, with permission from Elsevier. Part (b) reprinted with permission from [1219], ©1998 AIP

12 Heterostructures

Si

(a)

Si

Si

(b)

GaAs

Chapter 13

Two-Dimensional Semiconductors

Introducing a new experimental system is generally more rewarding than trying to find new phenomena within crowded areas. [...] Of course, the fantastic results one originally hopes for are unlikely to materialise, but, in the process of studying any new system, something original inevitably shows up. A.K. Geim, 2010 [1223]

Abstract 2D materials or atomic sheets are materials without a bulk. They offer unique physics and properties, but also challenges in preparation and stability. Stacking of such 2D materials in van-derWaals heterostructures extends the possibilities.

2D materials are the ultimate thickness limit for semiconductors. While the thickness of quantum wells can be controlled to the sub-atomic average thickness, they are still impacted by the roughness or undulation of the underlying substrate. 2D materials are more like free two-dimensional molecules with giant lateral extension and a vertical structure well defined by atomic bonding. Paper collections and textbooks are available for this topic, e.g. [1224–1226].

13.1 Graphene and Related Materials Graphene, its name proposed in [1227], is the ultimately thin material, a single sheet of carbon atoms in honeycomb arrangement; this is not a hexagonal (cf. Fig. 3.3b) but a trigonal lattice with a two-atom basis (Fig. 13.1). Graphene possesses unique physical properties such as a linear dispersion around the Fermi energy, making it a solid-state analogue to ultra-relativistic physics [1228]. Graphene does not possess a band gap in its ideal form. An account of the history of graphene research, starting in 1840, is given in [1229]. Many applications for graphene and graphene-based composites have been envisioned in electronics such as superior conductor or transistor material [1230, 1231] as well as applications in energy, biomedical, membranes and sensors [1232, 1233], but the current industrial use is still rather limited. Here, we introduce ’flat’ graphene while quasi one-dimensional nanotubes based on graphene are treated in Sect. 14.3.

© Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_13

383

384

13 Two-Dimensional Semiconductors

Fig. 13.1 Unit cell of A–B compound honeycomb lattice in a real space and b reciprocal space. The irreducible part of the Brillouin zone is shown in dark grey

(a)

(b)

Fig. 13.2 a Schematic layer structure of graphite with bond length and layer distance labelled. b AFM image of graphene on oxidized silicon. The height of two areas relative to the background is labelled. Adapted from [1240]

13.1.1 Structural Properties The carbon bond length in graphene is dC−C = 0.142 nm (cmp. Table 13.1). Due to instabilities [1234, 1235], freely suspended graphene layers are not perfectly flat but exhibit corrugations [1236]. Graphene can be prepared from graphite via micromechanical cleavage, i.e. mechanical exfoliation (repeated peeling) of small mesas of highly oriented pyrolytic graphite [1237, 1238]. Epitaxial growth on SiC [1239] and the growth on copper in large sheets [1232] have been reported. Graphite is a stacked arrangement of such graphene sheets (Fig. 13.2a) held together by van-derWaals forces (cmp. Sect. 13.3) as shown in Fig. 13.2b. The carbon atoms bond via sp2 hybridization. Organic molecules such as, e.g., anthracene or coronene (Fig. 18.1) can be understood as molecular-size pieces of such two-dimensional graphene sheet with hydrogen saturating the outside, broken bonds. Single layer graphene sheets (SLG) and few-layer graphene (FLG) sheets must distinguished since for the latter the exact stacking arrangement and vertical coupling effects play a role. Ideally, such twodimensional crystal is infinitely extended, e.g. for band structure calculations. Of course real crystals always have a (quasi-) one-dimensional boundary which is topologically a line or very thin sidewall. Various defects have been studied in graphene. The vacancy is discussed in [1241] and exhibits a magnetic moment of 2μB . The unit are a1,2 = √ √ cells in real and reciprocal space are shown in Fig. 13.1. The lattice vectors a/2(3, ± 3) (Fig. 13.1a). The reciprocal lattice vectors are b1,2 = 2π/(3a)(1, ± 3), where a = dC−C . The Brillouin zone (Fig. 13.1b) has two triples of K-points that are labeled K and K’ (or K+

13.1 Graphene and Related Materials

(a)

385

(b)

Fig. 13.3 a Phonon dispersion in graphene (cmp. Fig. 13.1b). Symbols are experimental data from various methods. Dashed lines is DFT-LDA theory, solid lines GGA. Adapted from [1244], reprinted with permission, ©2004 Elsevier Ltd. b Comparison of graphite and graphene Raman spectra (excited at 514 nm). In the right panel the number of monolayers in FLG is labeled (1: graphene, ∞: graphite). Adapted from [1245], reprinted with permission, ©2006 APS

√ and K−) at K , K = 2π/(3a) (1, ±1/ 3). When the A- and B-sites are identical, as for graphene, the difference between K- and K’-points is often subtle and a –M–K Brillouin zone is sufficient. Mechanical properties of graphene are discussed in [1242, 1243]; it has exceptional strength (Young’s modulus in the range of 1 TPa). The breaking stress 200 times greater than steel, with a 2D tensile stress of 42 N/m, corresponding to a strain of 25%. The phonon dispersion of graphene is shown in Fig. 13.3a. For the ZA and ZO modes, the displacement is perpendicular to the graphene plane (out-of plane modes). In Fig. 13.3b the Raman spectra of graphite and graphene are compared. The peak (termed ‘G’) at about 1580 cm−1 ist due to the zone center mode. The peak at about 2680 cm−1 (termed ‘2D’) is due to two phonons (double resonance) with opposite momentum in the highest optical branch near the K-point. It splits into four peaks for bilayer graphene due to changes in the electronic band structure [1245].

13.1.2 Band Structures The band structure of graphene from first principles [1246] is depicted in Fig. 13.4a. Graphene is a zero-gap semiconductor (cf. Fig. 6.46) which shows a linear photon-like spectrum, E = k vF ,

(13.1)

around the Fermi energy at the K-point (Fig. 13.4b). Such point is also called ’Dirac’ point. The important bands close to the Fermi level stem from the (out-of-plane) π-orbitals while the (inplane) chemical bonds are sp2 -type (Sect. 2.2.3). The linear dispersion around the K-point is similar to that of relativistic particles without rest mass. The electrons in graphene are of course not really massless, their velocity (6.35) being vF ≈ 106 m/s, about 300 times smaller than the speed of light [1248, 1249]. In the simplest tight-binding approximation (cf. Appendix G), considering the coupling of the carbon (out-of-plane) pz -orbitals with three nearest neighbors, the band structure is given as [1250, 1251] (cf. (G.23) √ √ 3 a k 3 a k a k y y x E(k) = ±t 1 + 4 cos 3 cos + 4 cos2 , (13.2) 2 2 2

386

13 Two-Dimensional Semiconductors

(a)

(b)

Fig. 13.4 a Band structure of graphene from first principles (zero energy refers to the intrinsic Fermi level). The circle focusses on the linear band crossing at the Fermi level. Adapted from [1247], reprinted with permission, ©2004 WILEYVCH. b Three-dimensional representation E(k x , k y ) of the π-bands of graphene (left) and of graphene-like material with gap (right)

Fig. 13.5 Band structure of graphene, silicene and germanene as labeled. Adapted from [1255], reprinted with permission, ©2014 RSC

where t ≈ 2.8 eV is the next-neighbor hopping energy (cf. Fig. G.1). More elaborate tight-binding schemes have been reported [1252, 1365]. The second next-neighbor energy t is about a factor of 10–100 smaller; a tight-binding fit to cyclotron resonance experiments finds t = 0.1 eV [1253]. The two-dimensional band structure is visualized in Fig. 13.4b. Such band structure has been directly confirmed experimentally [1254] as shown in Fig. 13.6a–e. The distortion of the band structure with increasing electron concentration (Fig. 13.6e–h) from the conical bands is due to strong electronelectron, electron-phonon, and electron-plasmon coupling effects [1254]. The band structures of atomic sheets of C, Si and Ge are compared in Fig. 13.5. The bands cross for all three materials at the K-point while the band gap at the zone center decreases with increases order number. Any kind of asymmetry between the A- and B-sites, as might occur for example on certain corrugated substrates, will introduce a band gap at the Dirac points (Fig. 13.4b). The band structure of FLG has been theoretically analyzed in [1256, 1257]. For bilayers experimental data on the band structure can be found in [1258]. Subtle differences exist for different stacking orders of the graphene sheets (see below, Sect. 13.3). Bulk graphite shows a semi-metallic behavior with a band overlap of about 41 meV. For more than ten graphene layers the difference with the band overlap in bulk graphite is less than 10%.

13.1 Graphene and Related Materials

387

Fig. 13.6 Experimental bandstructure of graphene (on (0001) 6H-SiC) as determined from ARPES. a Energy distribution of states as a function of momentum along principal directions in the Brillouin zone. The single-orbital tight-binding model (13.2) with T = 2.82 eV is shown as solid lines. The Fermi level is shifted by 0.435 eV due to doping. b Constant energy map of the states at binding energy corresponding to the Dirac energy E D ; the boundary of the Brillouin Zone boundary is superimposed as dashed line. The arrow at the K-point indicates the directions over which the data in (e–h) were acquired. c, d Constant energy maps at the Fermi energy E F = E D + 0.45 eV and E D − 1.5 eV, respectively. e–h Experimental energy bands along the line through the K-point parallel to Γ –M direction as indicated in (b). The dashed lines are an extrapolation of the lower bands below the Dirac crossing energy, which are observed not to pass through the upper bands (above E D ), suggesting the kinked shape of the bands around E D . The sheet electron density is n S = 1.1, 1.5, 3.7, and 5.6 × 1013 cm−2 for (e)–(h), respectively, due to increased doping upon potassium adsorption. Adapted from [1254], reprinted with permission, ©2006, Springer Nature

13.1.3 Electrical Properties The Shubnikov-de Haas (SdH) oscillations from a graphene sheet exhibit a behavior [1249] 1 4e 1 , = B h nS

(13.3)

which corresponds to (15.39) for a two-dimensional electron system and a spin- and valley-degeneracy1 of both two. The cyclotron mass √ has been determined from the temperature dependence of the SdH oscillations to be proportional2 to n (Fig. 13.7). The cyclotron mass is generally related [1259] to the area S(E) = πk 2 in k-space of the orbits at the Fermi energy via mc =

2 ∂ S(E) 2π ∂ E

(13.4)

With the linear dispersion (13.1) we can write (13.4) as mc =

2 2π E E = 2 . 2π 2 vF2 vF

(13.5)

For the linear energy dispersion (13.1) the number of states up to energy E F is (with a degeneracy of 4) 1 Each of the six valleys at the K-points is shared by three Brillouin zones; keep in mind that the K- and K’-points are not equivalent. 2 In a parabolic dispersion as in (15.38), the cyclotron mass is independent of n.

388

13 Two-Dimensional Semiconductors

Fig. 13.7 Cyclotron mass in graphene as a function of the sheet electron concentration n S (negative values relate to hole concentration, E F < E D ). Adapted from [1249]

N (E F ) = 4

π kF2 4π E 2 = A 2 2F , 2 (2π/L) h vF

(13.6)

where A is the system area. Therefore we have (at low temperature) with (13.5) nS =

4π E F2 ∝ m 2c , h 2 vF2

(13.7)

as determined experimentally. Therefore the behavior of the SdH oscillations confirms the linear dispersion relation. The experimental value for the velocity is vF ≈ 106 m/s. From (13.7) the density of states (per area and energy) around the Dirac point increases linearly with energy, D(E) =

8π E. h 2 vF2

(13.8)

The carrier density in a graphene sheet can be controlled via the field effect. The graphene is positioned on an insulator/semiconductor structure, typically SiO2 /Si (cf. Sect. 21.3). The carrier density is then related to the applied (gate) voltage Vg via (21.93) and (21.95), i.e. nS =

i Vg , ed

(13.9)

where d is the thickness of the insulator and i its dielectric constant. By applying positive (negative) bias electron (holes) can be induced in the sheet. The electron and hole densities depend on the Fermi energies3 nS = pS =

8π h 2 vF2 8π h 2 vF2

∞

ED ED −∞

E − ED dE 1 + exp [(E − E F )/kT ]

(13.10a)

−(E − E D ) dE 1 + exp [−(E − E F )/kT ]

(13.10b)

as visualized in Fig. 13.8. These relations cannot be inverted to obtain E F (n, p) analytically. The total charge carrier density is ρS = e( pS − n S ). The Hall effect (Fig. 13.9) shows the expected ambipolar dependence according to (15.16) which takes the form 3 Here

we assume the linear dispersion for all thermally populated states.

13.1 Graphene and Related Materials

389

Fig. 13.8 Band structure of graphene with various positions of the Fermi energy E F in relation to the Dirac energy E D . States occupied with electrons are shown with in bold

Fig. 13.9 Hall coefficient (T = 10 K) for a graphene sheet as a function of the free carrier sheet density ρS /e = pS − n S (positive values indicate p-type). Data shown as solid lines from [1249]

RH =

1 pS − n S e (n S + pS )2

(13.11)

for equal electron and hole mobilities.4 From Hall effect measurements the mobility has been determined to be about 104 cm2 /Vs, independent of temperature between 10 and 100 K, and the same for electrons and holes. This value, however, is much smaller than the in-plane mobility of about 106 cm2 /Vs at 4.2 K in high quality samples of highly ordered pyrolithic graphite (HOPG) [1260]. In suspended graphene a mobility of 2.3 × 105 cm2 /Vs has been found, limited by finite sample size [1261]. Thus in graphene layers on a solid surface extrinsic effects such as charge traps, interfacial phonons, ripples or fabrication residue seem to limit the carrier mobility. The QHE has been observed in graphene [1249], reportedly up at room temperature [1262]. The plateaus (4e2 / h)(n + 1/2) correspond to unusual half-integer filling, the first plateau occurring at 2e2 / h, as has been also suggested from theory, and related to the ‘pseudospin’. Another consequence of the Dirac-like behavior of the fermions in graphene is the presence of finite maximum resistivity ρmax = h/4e2 = 6.45 k even at low temperature and E F = E D . It is due to the fact that localization effects, leading to insulating behavior, are strongly suppressed. Then each carrier keeps a mean free path in the order of its Fermi wavelength. The Klein paradox [1263, 1264], the efficient tunneling of Dirac particles through high and thick barriers seems accessible in transport experiments with graphene [1265]. 4 Including sign, μ h

= −μe . For T = 0 and E F = E D , n S = pS = 0 and thus 1/RH should be zero. For finite temperatures there is always n S > 0 and pS > 0, even for E F = E D . Thus 1/RH ∝ 1/( pS − n S ) diverges at ρS = e( pS − n S ) = 0 with a change of sign.

390

13 Two-Dimensional Semiconductors

(a)

(b)

Fig. 13.10 a Scheme for interband absorption in the graphene band structure around one of the Dirac points. b Transmission spectrum of graphene, measured using standard spectroscopy for a uniform membrane that completely covered a 30 µm aperture (blue circles) and measured using an optical microscope (red squares). The inset shows a 50 µm aperture partly covered with monolayer (ML) and bilayer (BL) graphene as labeled (white dashed lines highlight the borders). Adapted from [1266]

13.1.4 Optical Properties The transmission of graphene has been investigated in [1266] over apertures and in [1267] on SiO2 substrate. The band-band absorption process is schematically shown in Fig. 13.10a. A theoretical analysis of this process yields an absorbance of π α ≈ 0.023, α = e2 /( c) being the fine structure constant [1266, 1268]. Effects due to next-to-nearest neighbors are not present theoretically [1269]. This universal number is found in the experimental spectrum in the visible spectral range as shown in Fig. 13.10b. In order to exhibit this value, half the photon energy may not be too large because the band structure will deviate from the linear dependence due to the triangular warping and nonlinearities (cf. Appendix G.3.2 and remember t ≈ 2.8 eV). In the infrared regime, deviations are due to state blocking due to finite temperature and non-zero Fermi level relative to the Dirac point and due to intraband transitions [1267]. For FLG, the transmission decreases stepwise; the step sequence deviates from πα due to inter-layer effects [1270].

13.2 Two-Dimensional Compound Semiconductors Two-dimensional crystals have been reported also for compound semiconductor materials such as BN, MoS2 , NbSe2 , Bi2 Sr2 CaCu2 Ox [1238] or ZnO [1271] and in particular transition metal dichalcogenides (TMDC) of the type MX2 , where M represents a transition metal atom and X a chalcogen atom forming the (W,Mo)(S,Se,Te)2 system [1272, 1273]. But many other materials also form atomically thin sheets [1225, 1255, 1274]. The main difference to graphene is that they form a band gap. A few physical properties are listed in Table 13.1.

13.2 Two-Dimensional Compound Semiconductors

391

Fig. 13.11 Crystal structure of two 2D materials of a hexagonal BN-type and b MX2 -type transition metal dichalcogenides. The unit cell is indicated. Left: Bird’s eye view on the plane and right: side view. The greyed area denotes an elementary cell. Adapted from [1255], reprinted with permission, ©2014 RSC

Table 13.1 Properties of various two-dimensional (monolayer) semiconductors, in-plane nearest neighbor distance dA−B , vertical distance of anions dX−X for MX2 -type TMDC, band gap E g , exciton binding energy E Xb (exfoliated on silica) and spin-splitting SOC in conduction and valence band material

C

BN

MoS2

MoSe2

WS2

WSe2

dA−B (nm) dX−X (nm) E g (eV) E Xb (eV) SOC,CB (meV) SOC,VB (meV)

0.142

0.144

0

7.3 2.2

0

0.184 0.317 2.15 0.31 -3

0.192 0.334 2.18 0.5 -21

0.184 0.314 2.41 0.32 29

0.192 0.334 2.2 0.5 36

0

148

184

430

466

13.2.1 Structural Properties Various two-dimensional configurations are known, the two most prominent that are typical for BN (1H, hexagonal) and for TMDC (2H, trigonal prismatic, ABA-stacking) respectively, are shown in Fig. 13.11. A plane-view TEM of the 2H structure of MoS2 is depicted in Fig. 13.12 [1275]. Other configurations of the TMDC such as an ABC-like stacking (1T, distorted octahedral) are possible [1276]. A variation are Janus TMDC of MXY type where the bottom and top layer consist of different anions [1277]. Two-dimensional alloys can be formed by mixing cations [1279] or anions [1283] (or both). As example, a STEM image of a Mo0.47 W0.53 S2 monolayer is shown in Fig. 13.12b which shows the distribution of W and Mo atoms. Various defects have been investigated for compound 2D semiconductors. For the vacancies in BN we refer to [1284]. Single sulphur vacancies in MoS2 are investigated in [1278]. Various antisite defects in MoS2 have been identified [1280] (Fig. 13.13). Also extended defects such as dislocations [1275], grain boundaries [1281] or rotational stacking faults [1282] have been observed. The phonon spectra of graphene, BN- and BC2 N-sheets are compared in Fig. 13.14. The spectrum of BC2 N is similar to the superposition of the C and BN spectra [1285]. The Raman peaks from MoS2 show discrete peak energies for thickness of 1–5 or 6 monolayers and then merge closely to the bulk

392

13 Two-Dimensional Semiconductors

(a)

(b)

Fig. 13.12 a STEM-ADF image of a MoS2 monolayer; a unit cell with Mo (S) atom shown in blue (orange) is overlaid (cf. Fig. 13.1a). Reprinted (with adaptation) with permission from [1275]. ©2013 American Chemical Society. b STEM image (Fourier filtered) of a Mo0.47 W0.53 S2 monolayer. The bright (dark) spots relate to W (Mo) atoms. Reprinted (with adaptation) with permission from [1279], ©2013 ACS

Fig. 13.13 Various point defects (vacancies and antisites) in MoS2 monolayer as revealed by TEM (a)–(e) together with atomic models (f)–(h). a S vacancy (VS ), b S divacancy (VS2 ), c Mo on S site (MoS ), d 2 Mo on 2 S sites (Mo2S2 ), e S on Mo site (SMo ). Adapted from [1280], reprinted under Creative Commons Attribute (CC BY 4.0) license

values [1286, 1287]. The dispersion of 2D MoS2 [1288] (Fig. 13.15) is quite similar to that of bulk material [1287, 1289]. Of course, due to the mass difference between Mo and S, a clear gap exists between acoustic and optical phonons (which is absent for graphene, cmp. Fig. 13.3a).

13.2.2 Band Structures The band structure of a h-BN monolayer has been calculated to be indirect [1290]. In Fig. 13.16, the band structure for a typical TMDC is depicted for a monolayer, a bilayer and bulk material. The latter features an indirect band structure with the valence band maximum at the -point and the conduction band minimum about half the way to the K-point. Similar band structures are found for multi-layers down to 2. However, for a single layer the band gap is direct at the K-points. The possible optical transitions are indicated in Fig. 13.16 as arrows. For the single layer, the direct transition has a lower energy than the indirect one; in a bilayer it is vice versa. Generally, the band gap increases with decreasing number of layers; this can be understood by thinking about the slab being a quantum well surrounded by a vacuum ’barrier’.

13.2 Two-Dimensional Compound Semiconductors

393

Fig. 13.14 a Crystal structure of BC2 N with unit cell indicated. b Brillouin zone of BC2 N (rectangle) and C, BN (hexagon, cmp. Fig. 13.1b). c Phonon dispersion of graphene (C) and BN- and BC2 N-sheets. Adapted from [1285]

Fig. 13.15 Phonon dispersion of MoS2 monolayer. ZA: out-of plane acoustic mode, NP: non-polar optical modes, HP: homopolar modes. On the right, the phonon density of states (DOS) is shown for Mo2 (red solid line) and for WS2 (blue dashed line) in comparison. Dispersion adapted from [1288], DOS adapted from [1287]

Fig. 13.16 Band structure of monolayer, bilayer and bulk WSe2 . The blue (green) arrows indicate the direct (indirect) band-band transitions. Based on [1272]

394

13 Two-Dimensional Semiconductors

(a)

(b)

Fig. 13.17 a Schematic three-dimensional view of (unsplit) conduction band minima (grey) and spin-split valence band maxima with opposite (red: up, blue: down) spin orientation. b Relativistic band structure of 2H-WSe2 (red dots show band structure without inclusion of spin-orbit splitting) with spin-splittings of conduction and valence band indicated. Adapted from [1296], reprinted with permission, ©2011 APS Fig. 13.18 ARPES measurement of the band structure of monolayer WSe2 . The horizontal dashed white lines indicate the spin-orbit splitting SOC = 513(10) meV of the top of the valence band. Adapted from [1297], reprinted with permission, ©2015 IOP Publishing

The lack of inversion symmetry results in a splitting of the electronic bands due to spin-orbit interaction. This effect is particularly strong in the valence band. Splitting energies SOC from fully relativistic calculations have been predicted for various 2H-MX2 systems [1292, 1293, 1296], ranging between about 150 meV (MoS2 ) and 500 meV (WTe2 ). For WSe2 , an experimental value of about 500 meV has been found [1297] (Fig. 13.18). For the same materials, the spin-splitting in the conduction band5 is an order of magnitude smaller in the range of 3–50 meV [1292, 1293]. Because of time reversal symmetry, the spin-splitting (cf. Sect. 6.2.4) of the bands at K and K’ has opposite sign as visualized in Fig. 13.17a; this property is termed ’spin-valley coupling’.

5 The

splitting is negative (positive) for MoX2 (WX2 ) compounds, i.e. the lowest conduction band at the K-point is spin up (down) [1292, 1294]; the valence band maximum at K is spin up for all cases.

13.2 Two-Dimensional Compound Semiconductors

395

Fig. 13.19 Absorption spectrum of WSe2 monolayer (derived from reflectance spectrum). XA,B (XA,B∗ ) denote the ground state (excited states) of the A- and B-exciton, respectively. XA,T at the low energy side denotes a trion. XC denotes a further transition discussed further in [1299]. Based on data from [1298]

(a)

(b)

Fig. 13.20 a Top: Optical image of MoS2 crystal on a silicon substrate with 1.0 and 1.5 µm diameter holes. Bottom: Photoluminescence intensity image of the same sample. The freely suspended parts of the single layer exhibit the highest intensity. b Photoluminescence spectra (excited at 532 nm) detected from regions with monolayers and bilayers, respectively. The arrows denote the positions of the (indirect) transitions for 2–6 layers. Adapted from [1291]

13.2.3 Optical Properties and Valley Polarization The absorption spectrum of a WSe2 monolayer is shown in Fig. 13.19 as reported in [1298]; various excitonic transitions are labeled that are discussed further below. The A- and B-excitons are formed from the upper and lower state of the spin-split valence band, respectively. The direct-to-indirect transition of the band structure for monolayer and multiplayer TMDC can be directly observed from the photoluminescence. For MoS2 , the single layer exhibits a 2–3 orders of magnitude higher luminescence intensity (Fig. 13.20a) than any multilayer sample since no phonons are needed for the optical band-band transition. The direct transition is at about 1.9 eV; the indirect band gap decreases monotonously and discretely from about 1.6 eV for a bilayer, via that of 3, 4, 5 or 6 layers (Fig. 13.20b) to that of bulk material (E g ≈ 1.3 eV) [1291]. The K- and K’-point pseudo-spin together with the spin-orbit interaction leads to spin-polarized bands as shown schematically in Fig. 13.22a. If excited with polarized light, optical absorption occurs between bands of the same spin orientation. In the absence of any inter-valley scattering, optical

396

13 Two-Dimensional Semiconductors

(a)

(b)

Fig. 13.21 a Photoluminescence spectra (at room temperature) of MoS2 , WS2 , MoSe2 , WSe2 , and MoTe2 monolayers as labeled. From [1300], with permission. b Transition energies of A and B excitons in Wx Mo1−x S2 alloy monolayers as a function of composition (spectra were excited at 514.5 nm for x =0-0.61 and at 457.9 nm for x =0.66-1). The dashed lines are fits with bowing parameters bA = 0.25(4) eV and bB = 0.19(6) eV. Based on data from [1279]

(a)

(b)

Fig. 13.22 a Schematic band structure of MoS2 monolayer around the K- and K’-point with spin-splitting (band order according to [1294]). Circularly polarized absorption and recombination processes are shown. b Circularly polarized detected photoluminescence (T = 83 K) from MoS2 monolayer (red: σ + , blue: σ − ) after excitation with σ + -polarized light at 1.96 eV (at the right end of the energy scale). The degree of circular polarization, (σ + − σ − )/(σ + + σ − ) is depicted as black curve with the left-hand scale. Adapted from data in [1302]

transitions are expected with a high degree of circular polarization [1301], leading to large dichroism effects (without magnetic ions). However, a maximum degree of circular polarization of about 50% was found in [1302] for MoS2 excited with circularly polarized light (Fig. 13.22b). The inter-valley dynamics reducing the polarization effects depends on the time scales of scattering and recombination which both can be in the range of several ps [1303]. The two oppositely polarized peaks in Fig. 13.22b have the same peak energy as expected from time-reversal symmetry; a magnetic field perpendicular to the layer will lift this degeneracy and introduce a K-K’ splitting (valley Zeeman effect) [1304, 1305] (Fig. 13.21).

13.2.4 Excitons The properties of excitons are particular in 2D materials. The purely two-dimensional hydrogen problem [1306, 1307] leads to a series of bound states E = −R/(n − 1/2)2 , where R denotes the Rydberg energy and n = 1, 2, . . . as usual. However, for the excitons in 2D material, the case of a stepwise changing dielectric constant , leading to image charge effects, as known from quantum well het-

13.2 Two-Dimensional Compound Semiconductors

(a)

397

(b)

Fig. 13.23 a Differential reflection contrast spectrum of WS2 monolayer (inset: reflection contrast). XA denotes the A-exciton, XA,T at the low energy side the trion. Based on data from [1311]. b Experimental transition energies (circles) for WS2 from magneto-optical data [1313] (cf. Fig. 15.13) with fits using the modified hydrogen model ∝ 1/(n + δ)2 (solid line) and a 2D hydrogen model with constant dielectric function fitted to the n = 3, 4, 5 levels (both theories displayed for continuous n). The (very similar) band gap E g = 2.239 eV for the two models is shown as lines on the left

erostructures [1188] (cmp. Sect. 12.3.2), must be considered. The thin slab is surrounded by vacuum which gives a huge contrast in . Even when packed, as often done in experiments, between other layers such as h-BN ( ≈ 4.5) or on a substrate, the contrast in dielectric constant is very large.6 This problem has been treated theoretically first in [1308, 1309] and recently rigorously in [1310]. The exciton binding energy is typically increased by this effect to several 100 meV. Also, the strongly anisotropic dielectric surrounding affects different quantum states differently, leading to non-hydrogenic terms in the exciton spectrum [1311] (Fig. 13.23). Schematics of the field lines for the 1s- and 2s-states are depicted in Fig. 13.24c, motivating that the anisotropic dielectric environment acts differently on these states. The higher the quantum number n is, the lower is the average dielectric constant ’seen’ by the 2D-exciton. In the example of excitons in WS2 , the effective dielectric constant changes from about 5 for the 1s state to 2.5 for the 2s state to values close to 1 for the higher states [1311]. In [1312] it has been discussed that the exciton level can be well described by the formula E n = E g − R ∗ /(n − δ)2 , with δ being a fitting parameter. Such parameter δ is known as ’quantum defect’ in the description of alkali spectra [1314]. For WSe2 (embedded between h-BN layers), E g = 1.873 eV, R ∗ = 140.5 meV and δ = 0.083 has been found [1312]. The data from [1313] for WS2 (also sandwiched between slabs of exfoliated hexagonal h-BN) can be fitted with E g = 2.239 eV, R ∗ = 140.4 meV and δ = 0.118 (Fig. 13.23b). The calculated plane-view of the electron wave function of the exciton ground state (A-exciton) in a MoS2 monolayer is depicted in Fig. 13.24a; the contributions to the exciton wave packet stem, from around the K-points as shown in Fig. 13.24b [1299]. Magneto-optical spectroscopy of 2D excitons and the Zeeman splittings and diamagnetic shifts up to the 5s state in WS2 and Mo(S,Se,Te)2 monolayers are reported in [1313] and (on Si/SiO2 substrate) [1315]; the g-factor (cf. Sect. 15.2) of the exciton is very close to 4 μB (cf. Fig. 15.13d), a fact that is under theoretical consideration [1316]. Charged excitons have been discussed in [1317, 1318]. The influence of various surrounding media to the TMDC on the dielectric screening has been investigated theoretically [1319] and experimentally [1320].

6 In

QW heterostructures, the differences in are typically around 1 or smaller [1188].

398

13 Two-Dimensional Semiconductors

Fig. 13.24 Plane-view of the electron wave function of the exciton ground state in MoS2 monolayer in a real space and b k-space. Adapted from [1299], reprinted with permission, ©2013 APS. c Schematic 1s and 2s exciton wave functions with different sensing of the low- environment

(c)

13.3 Van-der-Waals Heterostructures Let’s recall that graphite is a stacked arrangement of graphene layers. It is called the ’Bernal’-phase or -stacking and relates to the AB- or 2H-stacking like in a hcp crystal (Fig. 13.25a). Other meta-stable arrangements are the AA’-stackings (twisted bilayer graphene), in which the crystallographic axes of the two layers have an arbitrary angle ϑ between zero and 30◦ as depicted in Fig. 13.25b); the stacking vor ϑ = 0 is also termed AA. Electronic properties depend on the twist angle [1321]. A refined theory considering the super-periodicities (moiré pattern) of interlayer hopping potential has been reported in [1322, 1323]. The different stackings can be distinguished, e.g., in infrared spectroscopic imaging [1324]. As an extension of this concept, van-der-Waals heterostructures been conceived [1326, 1327] which consist of vertically stacked atomic sheets of various 2D materials, a kind of molecular LEGO™ (Fig. 13.26a). Virtually any combination is possible for various electronic, sprintronic and photonic applications [1329, 1330]. An advantage is the well controlled tunneling effect by the present exact layer thicknesses in the device.

Fig. 13.25 Vertical stacking phases of graphene in a AB-type, Bernal-stacking and b AA’-type, non-Bernal stacking. The rotation angle ϑ is indicated. Adapted from [1325]

13.3 Van-der-Waals Heterostructures

(a)

399

(b)

Fig. 13.26 a Example of van-der-Waals heterostructure from various 2D materials as proposed in [1326]. Reprinted with permission, ©2013, Springer Nature. b Van-der-Waals heterostructure with twisted layers. Adapted from [1328], reprinted with permission, ©2018, Springer Nature Fig. 13.27 Resistance of BN-graphene-BN van-der-Waals heterostructure (insets show optical image and cross section TEM as well as the device and its schematic measurement scheme). Adapted from [1331]

The field effect for a graphene layer between BN flakes is shown in Fig. 13.27. The measured mobility (at room temperature) is in the range of 105 cm2 /Vs for a 2D carrier density below 1 × 1012 cm−2 and thus larger than values achieved for InSb or InAs [1331]. Van-der-Waals heterostructures of boron nitride and graphene are reviewed in [1332]. The effect of surrounding media via the modified dielectric screening on excitons has been mentioned already above [1319, 1320]. Encapsulation by h-BN monolayers can enhance the luminescence yield and reduce the recombination time constant of a TMDC monolayer, as demonstrated in [1334] for a three monolayer h-BN/WS2 /h-BN heterostructure. Generally, in van-der-Waals heterostructures, the weak interlayer bonding allows a new degree of freedom, the twist angle ϑ (cf. Fig. 13.25b for twist of two graphene layers) between two 2D crystals (Fig. 13.26b). The situation is similar to the twist boundary between two grains (Sect. 4.4.3). This rotation causes the formation of moiré patterns that are directly observable in STM images as depicted in Fig. 13.28. The physical properties of the heterostructure can drastically depend on the twist angle [1335]. A prominent consequence is the periodic modification of the energy landscape for

400

13 Two-Dimensional Semiconductors

Fig. 13.28 STM images of ReSe2 monolayers on graphene. The twist angle ϑ (cmp. Fig. 13.26b), as deducted from comparison with theoretical calculations, is indicated. The red arrows indicate the moiré pattern’s periodicity. Adapted from [1333], reprinted unter Creative Commons Attribute (CC BY-NC 4.0) license

excitons leading to localization and modification of spectra [1336]. A particularly intriguing effect is the occurrence of superconductivity with a critical temperature of up to 1.7 K for a graphene bilayer with the ’magic’ twist angle of ϑ ≈ 1.1◦ and specific (gate-controlled) carrier densities in the range of (1–2)×1012 cm−2 [1337].

Chapter 14

Nanostructures

The principles of physics, as far as I can see, do not speak against the possibility of maneuvering things atom by atom.

R.P. Feynman, 1959 [1338]

Abstract One-dimensional nanostructures (quantum wires) and zero-dimensional ones (quantum dots) are discussed with regard to their various fabrication methods and the tunable physical properties in such systems. Main effects covered are the modified density of states, confined energy levels, (envelope) wave-function symmetry and the resulting novel electrical and optical properties.

14.1 Introduction When the structural size of functional elements enters the size range of the de Broglie matter wavelength, the electronic and optical properties are dominated by quantum-mechanical effects. The most drastic impact can be seen from the density of states (Fig. 14.1). The quantization in a potential is ruled by the Schrödinger equation with appropriate boundary conditions. These are simplest if an infinite potential is assumed. For finite potentials, the wavefunction leaks out into the barrier. Besides making the calculation more complicated (and more realistic), this allows electronic coupling of nanostructures. Via the Coulomb interaction, a coupling is even given if there is no wavefunction overlap. In the following, we will discuss some of the fabrication techniques and properties of quantum wires (QWR) and quantum dots (QD). In particular for the latter, several textbooks can also be consulted [1339, 1340].

14.2 Quantum Wires 14.2.1 V-Groove Quantum Wires Quantum wires with high optical quality, i.e. high recombination efficiency and well-defined spectra, can be obtained by employing epitaxial growth on corrugated substrates. The technique is shown schematically in Fig. 14.2. A V-groove is etched, using, e.g., an anisotropic wet chemical etch, into a ¯ . Even when the etched pattern is not very sharp GaAs substrate. The groove direction is along 110 on the bottom, subsequent growth of AlGaAs sharpens the apex to a self-limited radius ρl of the order © Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_14

401

402

14 Nanostructures

Fig. 14.1 Schematic geometry and density of states for 3D, 2D, 1D and 0D electronic systems Fig. 14.2 Schematic cross section of a GaAs/AlGaAs heterostructure grown on a channeled substrate, illustrating the concept of self-ordered quantum-wire fabrication. Adapted from [1341], reprinted with permission, ©1992, Elsevier Ltd

of 10 nm. The side facets of the groove are {111}A. Subsequent deposition of GaAs leads to a larger upper radius ρu > ρl of the heterostructure. The GaAs QWR formed in the bottom of the groove is thus crescent-shaped as shown in Fig. 14.3a. A thin GaAs layer also forms on the side facets (sidewall quantum well) and on the top of the ridges. Subsequent growth of AlGaAs leads to a resharpening of the V-groove to the initial, self-limited value ρl . The complete resharpening after a sufficiently thick AlGaAs layer allows vertical stacking of crescent-shaped QWRs of virtually identical size and shape, as shown in Fig. 14.3b. In this sense, the self-limiting reduction of the radius of curvature and its recovery during barrier-layer growth leads to self-ordering of QWR arrays whose structural parameters are determined solely by growth parameters. The lateral pitch of such wires can be down to 240 nm. To directly visualize the lateral modulation of the band gap, a lateral cathodoluminescence (CL) linescan perpendicular across the wire is displayed in Fig. 14.4. In Fig. 14.4a, the secondary electron (SE) image of the sample from Fig. 14.3a is shown in plan view. The top ridge is visible in the upper and lower parts of the figure, while in the middle the sidewalls with the QWR in the center are apparent. In Fig. 14.4b, the CL spectrum along a linescan perpendicular to the wire (as indicated by the white line in Fig. 14.4a) is displayed. The x-axis is now the emission wavelength, while the y-axis is the lateral position along the linescan. The CL intensity is given on a logarithmic scale to display the full dynamic range. The top QW shows almost no variation in band gap energy (λ = 725 nm); only directly at the edge close to the sidewall does a second peak at lower energy (λ = 745 nm) appear, indicating a thicker region there. The sidewall QW exhibits a recombination wavelength of 700 nm at the edge to the top QW, which gradually increases to about 730 nm at the center of the V-groove. This directly

14.2 Quantum Wires

(a)

403

(b)

Fig. 14.3 a Transmission electron microscopy cross-sectional image of a crescent-shaped single GaAs/AlGaAs quantum wire. From [1342], reprinted with permission, ©1994 IOP. (b) TEM cross-sectional image of a vertical stack of identical GaAs/AlGaAs crescent-shaped QWRs. From [1341], reprinted with permission, ©1992, Elsevier Ltd

Fig. 14.4 a Plan-view SE image of single QWR, showing top and sidewall with QWR in the center. The white dashed line indicates the position of the linescan on which the CL spectra linescan b has been taken at T = 5 K. The CL intensity is given on a logarithmic false color scale to display the full dynamic range as a function of wavelength and position. Adapted from [1342], reprinted with permission, ©1994 IOP

visualizes a linear tapering of the sidewall QW from about 2.1 nm thickness at the edge to 3 nm in the center. The QWR luminescence itself appears at about 800 nm. After fast capture from the barrier into the QWs and, to a much smaller extent corresponding to its smaller volume, into the QWR, excess carriers will diffuse into the QWR via the adjacent sidewall QW and the vertical QW. The tapering of the sidewall QW induces an additional drift current.

14.2.2 Cleaved-Edge Overgrowth Quantum Wires Another method to create quantum wires of high structural perfection is cleaved-edge overgrowth (CEO) [1343], shown schematically in Fig. 14.5. First, a layered structure is grown (single or multiple quantum wells or superlattice). Then, a {110} facet is fabricated by cleaving (in vacuum) and epitaxy

404

14 Nanostructures

50nm

QW cleavage plane

[001] QW

Fig. 14.5 Principle of CEO quantum wires and 2-fold CEO quantum dots. Part (a) depicts a layered structure (quantum wells or superlattice, blue), (b) describes the growth on the cleaved facet used for fabrication of quantum wires. In (c) a second cleave and growth on top of the plane allows the fabrication of quantum dots. From [1344]. (d) Cross-sectional TEM image of CEO GaAs/AlGaAs quantum wires. Two quantum wells (QW) and the QWR at their junction are labeled. The first epitaxy was from left to right. The second epitaxy step was on top of the cleavage plane (dashed line) in the upward direction. Adapted from [1345], reprinted with permission, ©1997 APS

is continued on the cleaved facet. At the junctures of the {110} layer and the original quantum wells QWRs form. Due to their cross-sectional form they are also called T-shaped QWRs. A second cleave and another growth step allow fabrication of CEO quantum dots [1344, 1345] (Fig. 14.5c).

14.2.3 Nanowhiskers Whiskers are primarily known as thin metal spikes and have been investigated in detail [1346]. Semiconductor whiskers can be considered as (fairly short) quantum wires. They have been reported for a number of materials, such as Si, GaAs, InP and ZnO [1347]. A field of ZnO whiskers is shown in Fig. 14.6. If heterostructures are incorporated along the whisker axis [1348], quantum dots or tunneling barriers can be created (Fig. 14.7a). The growth mode relies often a VLS (vapor-liquid-solid) mechanism in which the wire materials are first incorporated into a liquid catalyzer (most often gold) drop at the tip and then used to build up the nanocrystal. In [1349], the layer-by-layer growth of a GaAs nanowire via this mechanism has been observed in-situ by TEM (Fig. 14.7b) and is also available as an impressive video. Another nanowire growth mechanism is the VSS (vapor-solid-solid) mechanism that works without liquid drop on top of the wire.

14.2 Quantum Wires

405

(b)

(a)

Fig. 14.6 a Array of ZnO nanowhiskers on sapphire, fabricated using thermal evaporation. Adapted from [1353]. b Single, free-standing ZnO nanowire fabricated using PLD. Adapted from [1354]

Au InAs InP InAs InP InAs (a)

(b)

Fig. 14.7 a TEM image of a part of an InAs whisker 40 nm in diameter that contains InP barriers. The zooms show sharp interfaces. On top of the whisker is a gold droplet from the so-called vapor–liquid–solid growth mechanism. The whisker axis is [001], the viewing direction is [110]. Adapted from [1348], reprinted with permission, ©2002 AIP. b Subsequent growth stages of the tip of a GaAs nanowire with Au cap; times at which (in-situ) TEM image has been taken are labelled. The arrows indicate the position of the growth front. Adapted from [1349], reprinted with permission, ©2018 APS

Such nanocrystals can also act as a nanolaser [1350, 1351]. In ZnO nanowhiskers the conversion of mechanical energy into electrical energy has been demonstrated [1352] based on the piezoelectric effect (Sect. 16.4). The critical thickness h c in nanowire heterostructure is strongly modified from the 2D situation (Sect. 5.4.1). Based on the strain distribution of a misfitted slab in a cylindrical wire [1355] the dependence of critical thickness on the nanowhisker radius r was developed [1356, 1357]. For given misfit there is a critical radius rc for which h c is infinite for r < rc (Fig. 14.8).

406

14 Nanostructures

Fig. 14.8 Critical radius rc above which an infinitely thick layer with misfit grows coherently on a cylindrical nanowire (relaxation by 60◦ dislocations, b = 0.4 nm, ν = 1/3). Adapted from [1357]

Fig. 14.9 a SEM image of an ensemble of ZnO nanobelts. b HRTEM image of a single ZnO nanobelt, viewing direction is [00.1]. The inset shows the diffraction pattern. Adapted from [1358], reprinted with permission, ©2004 AIP

Fig. 14.10 a Bright field and b dark field TEM image of a ZnO nanoring formed by the ‘slinky’-like growth of a nanobelt. c SEM image of an open ZnO nanospiral. The insets in (a, c) show schematically the surface charge distribution. Adapted from [1359], ©2006 IOP

14.2.4 Nanobelts A number of belt-shaped nanostructures has been reported [1347]. These are wire-like, i.e. very long in one dimension. The cross-section is rectangular with a high aspect ratio. In Fig. 14.9a ZnO nanobelts ¯ are shown. The wire direction is [21.0]. The large surface is (00.1), the thickness of the belt extends in [01.0]-direction. High resolution transmission microscopy (Fig. 14.9b) shows that these structures are defect-free. The pyroelectric charges on the ZnO (0001) surfaces (Sect. 16.2) lead to the formation of open (Fig. 14.10c) spirals. Closed spirals (Fig. 14.10a) occur if the short dimension is along [00.1] and alternating charges become compensated in a ‘slinky’-like ring (Fig. 14.10b).

14.2 Quantum Wires

407

Fig. 14.11 Electron wavefunctions (||2 on logarithmic grey scale) for the first three confined levels for the QWR of Fig. 14.3a. From [1342]

n=1

n=2

n=3

Fig. 14.12 a Three-dimensional view of the electron and (heavy) hole part of the excitonic wavefunction in a 4 nm × 5 nm T-shaped In0.2 Ga0.8 As/GaAs QWR. The orbitals correspond to 70% probability inside. b Cross section through the electron and hole orbitals in their center along the wire direction. Reprinted with permission from [1361], ©1998 APS

hh

e [110] (a) [110]

[001]

[110] (b) [001]

14.2.5 Quantization in Two-Dimensional Potential Wells The motion of carriers along the quantum wire is free. In the cross-sectional plane the wavefunction is confined in two dimensions. The simplest case is for constant cross section along the wire. However, generally the cross section along the wire may change and therefore induce a potential variation along the wire. Such potential variation will impact the carrier motion along the longitudinal direction. Also, a twist of the wire along its axis is possible. In Fig. 14.11, the electron wavefunctions in a V-groove GaAs/AlGaAs QWR are shown. Further properties of V-groove QWRs have been reviewed in [1360]. In Fig. 14.12, the excitonic electron and hole wavefunctions are shown for a (strained) T-shaped QWR. In Fig. 14.13a the atomic structure of a very thin ZnO nanowhisker with a cross-section consisting of seven hexagonal unit cells is shown. The theoretical one-dimensional band structure [1362] is shown in Fig. 14.13b together with the charge density of the lowest conduction band state (LUMO) and the highest valence band state (HOMO). The band gap is generally too small because of the LDA method used.1 In [1362] also the properties of nanowires with various diameters are compared. The HOMO at lies only 80 meV above the top of valence band of bulk ZnO, and its position changes little with 1 The

LDA in [1362] yields E g = 0.63 eV for the bulk ZnO band gap; its experimental value is 3.4 eV.

408

14 Nanostructures

Fig. 14.13 a Atomic arrangement of a 1 nm wide ZnO nanowire. b Theoretical band structure and charge density of the c lowest conduction band and d highest valence band state. Adapted from [1362], reprinted with permission, ©2006 AIP

the wire diameter. It is mainly composed by surface oxygen 2p like dangling bonds (Fig. 14.13d). The LUMO (Fig. 14.13c) is delocalized in the whole nanowire, indicating that it is a bulk state. The delocalized distribution is also responsible for the large dispersion of the LUMO from to A. The energy of the LUMO increases substantially with decreasing diameter due to the radial confinement.

14.3 Carbon Nanotubes 14.3.1 Structure A carbon nanotube (CNT) is a part of a graphene sheet (cf. Sect. 13.1) rolled up to form a cylinder. CNTs were first described as multi-walled nanotubes by Iijima [1363] in 1991 (Fig. 14.14b) and in their single-walled form (Fig. 14.14a) in 1993 [1364]. Reviews can be found in [1247, 1365]. The chirality and diameter of a nanotube are uniquely described by the chiral vector

Fig. 14.14 a TEM image of single-walled carbon nanotubes (SWNT). b TEM images of various multi-walled carbon nanotubes (MWNT). Adapted from [1363], reprinted with permission, ©1991, SpringerNature

14.3 Carbon Nanotubes

409

Fig. 14.15 Schematic atomic arrangement in graphene; the C–C bond length is dC−C = 0.142 nm. Several vectors for making carbon nanotubes (cf. Sect. 14.3) are shown

Fig. 14.16 Structure of different types of carbon nanotubes that have similiar diameter of 0.8 nm. a Armchair (6, 6), b zigzag (8, 0) and c chiral symmetry. Adapted from [1247]

ch = n 1 a1 + n 2 a2 ≡ (n 1 , n 2 ) ,

(14.1)

where a1 and a2 are the unit vectors of the graphene sheet. The chiral vector denotes two crystallographic equivalent sites which are brought together along the circumference of the nanotube. The possible vectors are visualized in Fig. 14.15 for −30◦ ≤ θ ≤ 0◦ . The fiber diameter is given by a 2 |ch | = n 1 + n 1 n 2 + n 22 , (14.2) π π √ with the graphene lattice constant a = 3 dC−C = 0.246 nm. Ab-initio calculations show that the diameter becomes a function of the chiral angle below 0.8 nm; deviations from (14.2) are below 2% for tube diameters d > 0.5 nm [1366]. The (n, 0) tubes (θ = 0) are termed ‘zig-zag’ and an example is depicted in Fig. 14.16b. Nanotubes with θ = ±π/6, i.e. of the (n, n) (and (2n, −n)) type, are called ‘armchair’. All others are termed ‘chiral’. The extension along the wire axis is large compared to the diameter. The tip of a nanotube is part of a buckminster-fullerene type molecule (Fig. 14.17). When the nanotube if formed by rolling a single sheet of graphene (SLG), a single-walled nanotube (SWNT) is formed. A FLG sheet creates a multiwalled nanotube (MWNT). For small number of layers they are called double-walled, triple-walled and so forth. d=

410

14 Nanostructures

Fig. 14.17 A chiral nanotube (chiral vector is (10, 5), θ = −19.11◦ ) with hemispherical caps at both ends based on an icosahedral C140 fullerene. The tube diameter is 1.036 nm. Adapted from [1367]

The mechanical strength of carbon nanotubes is very large. For SWNT Young’s moduli of 103 GPa have been found experimentally [1368] in agreement with theoretical predictions [1369].

14.3.2 Band Structure In carbon nanotubes there is some mixing of the π (2pz ) and σ (2s and 2pz ) carbon orbitals due to the radial curvature. This mixing is, however, small and can be neglected near the Fermi level [1370]. The band structure of a nanotube is mainly determined by zone-folding of the graphene band structure. The vector along the (infinitely extended) wire k z is continuous. The vector k⊥ around the nanotube is discrete with the periodic boundary condition ch · g⊥ = 2π m ,

(14.3)

where m is an integer. The distance of allowed k⊥ -values is (5.5) k⊥ =

2π 2 = . πd d

(14.4)

The character of the nanotube band structure depends on how the allowed k-values lie relative to the graphene Brillouin zone and its band structure. This is visualized in Fig. 14.18. For the case of an armchair tube (n, n), as shown in Fig. 14.18a, the K-point of the graphene band structure always lies on an allowed k-point. Therefore, the nanotube is metallic, i.e. zero-gap, as seen in the bandstructure in Fig. 14.18b. The Dirac point is between and X. For a zig-zag nanotube, the k-space is shown in Fig. 14.18c for a (6, 0) nanotube. The corresponding band structure for a (6, 0) nanotube is also metallic (Fig. 14.18d) with the Dirac point at the point. In Fig. 14.19c the band structure of another metallic (12, 0) zig-zag nanotube is shown. However, only for (3 m, 0) the K-point is on an allowed state and thus the tube metallic. For the other cases, as shown for the k-space of a (8, 0) nanotube in Fig. 14.19b, this is not the case. The corresponding band structure (Fig. 14.19c for (13, 0)) has a gap and thus the nanotube is a semiconductor. Generally, the condition for a nanotube to be metallic is with an integer m n1 − n2 = 3 m .

(14.5)

There are two semiconducting ‘branches’ with ν = (n 1 − n 2 ) mod 3 = ±1. The tubes with ν = +1 have a small band gap, those with ν = −1 have a larger band gap. √ The density of states is a series of one-dimensional DOS, proportional to E (6.79). It is compared in Fig. 14.20 for a metallic and a semiconducting nanotube. Within 1 eV from the Fermi energy the DOS can be expressed in an universal term [1373].

14.3 Carbon Nanotubes

411

Fig. 14.18 a Brillouin zone of the graphene lattice (bold line) and allowed k-values for a (6, 6) armchair nanotube. b Band structure of a (6, 6) carbon nanotube. Adapted from [1371]. c Brillouin zone of the graphene lattice (bold line) and allowed k-values for a (6, 0) zig-zag carbon nanotube. In the lower part the real space structure is visualized. (d) Band structure of graphene (left) and a (6, 6) nanotube (right). Adapted from [1372]

Fig. 14.19 a, b Brillouin zone of the graphene lattice (bold line) and allowed k-values for a (a) (6, 0) and a (b) (8, 0) zig-zag nanotube. c Band structures of a (12,0) metallic and (13, 0) semiconducting armchair carbon nanotube. Adapted from [1371]

14.3.3 Optical Properties Optical transitions occur with high probability between the van-Hove singularities of the DOS. The theoretical absorption spectrum of a (10, 0) nanotube is shown in Fig. 14.21. In an ensemble of nanotubes various types and sizes occur. The transition energies of all possible nanotubes sorted by diameter are assembled in the Kataura plot (Fig. 14.22a). Experimental data are shwon in Fig. 14.22b. The two branches of semiconducting nanotubes ν = ±1 yield different transition energies. The overall dependence of the transition energy follows a 1/d-law.

412

14 Nanostructures

Fig. 14.20 Density of states for a (9, 0) metallic and (10, 0) semiconducting zig-zag carbon nanotube within the tight-binding approximation (13.2). The energy scale is given in units of the tight-binding parameter T ≈ 3 eV. The dashed lines are the DOS of graphene. Adapted from [1367]

Fig. 14.21 Calculated absorption spectra for a (semiconducting) (10, 0) carbon nanotube for parallel (solid line) and perpendicular (dotted line) polarization. The thick (thin) lines are calculated with (without) the matrix element included. Adapted from [1374]

14.3.4 Other Anorganic Nanotubes Structures similar to carbon nanotubes have been reported for BN [1378, 1379]. A boron nitride nanotube is a cylindrically rolled part of a BN sheet. BN tubes are always semiconducting (Fig. 14.23) and have a band gap beyond 5 eV similar to hexagonal BN which is mostly independent on chirality and diameter [1380]. Thus, while carbon nanotubes appear black since they absorb within 0–4 eV, BN is transparent (or white if scattering). For high energies larger than 10 eV C and BN tubes are quite similar since they are isoelectronic and the high-lying unoccupied states are less sensitive to the difference in the nuclear charges than the states at and below the Fermi energy [1381].

14.4 Quantum Dots

413

Fig. 14.22 a Theoretical transition energies of semiconducting (filled symbols) and metallic (open symbols) carbon nanotubes as a function of tube diameter (Kataura plot). Energies are calculated from van-Hove singularities in the JDOS within the third-order tight-binding approximation [1252]. b Experimental Kataura plot for the first two semiconducting (S, closed symbols) and the first metallic (M, open symbols) transition. Dashed lines connect the (near-to) armchair tubes; full lines connect tubes in a branch, ν = (n 1 − n 2 ) mod 3. Data from photoluminescence [1375] and resonant Raman scattering [1376]. Adapted from [1377]

Fig. 14.23 Band structure and density of states (DOS) of C(3,3) and BN(3,3) nanotubes, calculated with DFT-LDA. Adapted from [1381]

14.4 Quantum Dots 14.4.1 Quantization in Three-Dimensional Potential Wells The solutions for the d-dimensional (d = 1, 2, or 3) harmonic oscillator, i.e. the eigenenergies for the Hamiltonian d 1 p2 + m ω02 xi2 (14.6) Hˆ = 2m 2 i=1 are given by

d ω0 , En = n + 2

(14.7)

with n = 0, 1, 2, . . .. More detailed treatments can be found in quantum-mechanics textbooks. Next, we discuss the problem of a particle in a centrosymmetric finite potential well with different masses m 1 in the dot and m 2 in the barrier. The Hamiltonian and the potential are given by

414

14 Nanostructures

2 ∇ + V (r ) Hˆ = ∇ 2m −V0 , r ≤ R0 V (r ) = . 0 , r > R0

(14.8) (14.9)

The wavefunction can be separated into radial and angular components (r) = Rnlm (r ) Ylm (θ, φ), where Ylm are the spherical harmonic functions. For the ground state (n = 1) the angular momentum l is zero and the solution for the wavefunction (being regular at r = 0) is given by

R(r ) =

sin(k r ) kr sin(k R0 ) k R0

, r ≤ R0 exp (−κ (r − R0 )) , r > R0

2 m 1 (V0 + E) 2 E 2 m 2 . κ2 = − 2 k2 =

(14.10a) (14.10b) (14.10c)

From the boundary conditions that both R(r ) and r = R0 , the transcendental equation k R0 cot (k R0 ) = 1 −

1 ∂ R(r ) m ∂r

are continuous across the interface at

m1 (1 + κ R0 ) m2

(14.11)

is obtained. From this formula the energy of the single particle ground state in a spherical quantum dot can be determined. For a given radius, the potential needs a certain strength V0,min to confine at least one bound state; this condition can be written as V0,min =

π 2 2 8 m ∗ R02

(14.12)

for m 1 = m 2 = m ∗ . For a general angular momentum l, the wavefunctions are given by spherical Bessel functions jl in the dot and spherical Hankel functions h l in the barrier. Also, the transcendental equation for the energy of the first excited level can be given: k R0 cot (k R0 ) = 1 +

k 2 R02 2 m 1 2+2κ R0 +κ 2 R0 m2 1+κ R0

−2

.

(14.13)

In the case of infinite barriers (V0 → ∞), the wavefunction vanishes outside the dot and is given by (normalized) 2 jl (knl r ) , (14.14) Rnml (r ) = 3 j R0 l+1 (knl R0 ) where knl is the n-th zero of the Bessel function jl , e.g. kn0 = nπ . With two-digit precision the lowest levels are determined by knl

l=0 l=1 l=2 l=3

l=4 l=5

n=0 n=1 n=2

3.14 6.28 9.42

8.18

4.49 7.73

5.76 9.10

6.99 10.42

9.36

14.4 Quantum Dots

415

C0

C1

C2

C3

(a)

Electrons

V0

V1

V2

V3

(b)

V0

87.6%

V1

81.8%

V2

76.2%

V3

74.6%

V0

9.6%

V1

13.7%

V2

17.6%

V3

21.0%

V0

2.3%

V1

3.6%

V2

5.3%

V3

3.0%

(c) Holes

(d)

(e)

Fig. 14.24 Isosurface plots (25% of maximum value) of the total probability densities a, b and valence-band projections (c)–(e) of bound electron (a) and hole (b)–(e) states in a model pyramidal InAs/GaAs quantum dot with base length b = 11.3 nm. The percentages are the integrals of the projections to the bulk heavy, light and split-off hole bands, respectively, and the isosurfaces show the corresponding projection shapes. For each valence-band state the difference ∞ from 100% is the integral −∞ |ψs↑ |2 +|ψs↓ |2 d3 r of the s-type (conduction band) Bloch function projection (not shown). Reprinted with permission from [1385], ©2002, Springer

The (2l+1) degenerate energy levels E nl are (V0 = ∞, m = m 1 ): E nl =

2 2 1 k . 2m nl R02

(14.15)

The 1s, 1p, and 1d states have smaller eigenenergies than the 2s state. A particularly simple solution is given for a cubic quantum dot of side length a0 and infinite potential barriers. One finds the levels E n x n y n z : Enx n y nz =

π2 2 2 n x + n 2y + n 2z , 2m a02

(14.16)

with n x , n y , n z = 1, 2, . . . . For a sphere, the separation between the ground and first excited state is E 1 − E 0 ≈ E 0 , for a cube and a two-dimensional harmonic oscillator it is exactly E 0 . For a threedimensional harmonic oscillator this quantity is E 1 − E 0 = 2E 0 /3. For realistic quantum dots a full three-dimensional simulation of strain, piezoelectric fields and the quantum-mechanical confinement must be performed [1382, 1383]. In Fig. 14.24, the lowest four electron and hole wavefunctions in a pyramidal InAs/GaAs quantum dot (for the strain distribution see Fig. 5.34 and for the piezoelectric fields see Fig. 16.16) are shown. The figure shows that the lowest hole states have dominantly heavy-hole character and contain admixtures of the other hole bands. The wavefunction in such quantum dots can be imaged using scanning tunneling microscopy [1384].

416

14 Nanostructures

(a)

(b)

Fig. 14.25 a Schematic drawing of a quantum dot (QD) with tunnel contacts and gate electrode. The inset depicts an equivalent circuit with capacitances. b Realization with an in-plane gate structure. The distance between ‘F’ and ‘C’ (gate electrode) is 1 µm. Electron transport occurs from a 2DEG between 3/F to 4/F through the quantum points contacts 1/3 and 2/4. Part (b) from [1386], reprinted with permission, ©1991, Springer Nature

14.4.2 Electrical and Transport Properties The classical electrostatic energy of a quantum dot with capacitance CG that is capacitively coupled to a gate (Fig. 14.25) at a bias voltage VG is given by E=

Q2 − Q α VG , 2CG

(14.17)

where α is a dimensionless factor relating the gate voltage to the potential of the island and Q is the charge of the island. Mathematically, minimum energy is reached for a charge Q min = α CG VG . However, the charge has to be an integer multiple of e, i.e. Q = N e. If Vg has a value, such that Q min /e = Nmin is an integer, the charge cannot fluctuate as long as the temperature is low enough, i.e. kT

e2 . 2 CG

(14.18)

Tunneling into or out of the dot is suppressed by the Coulomb barrier e2 /2CG , and the conductance is very low. Analogously, the differential capacitance is small. This effect is called Coulomb blockade. Peaks in the tunneling current (Fig. 14.26b), conductivity (Fig. 14.26a) and the capacitance occur, when the gate voltage is such that the energies for N and N + 1 electrons are degenerate, i.e. Nmin = N + 21 . The expected level spacing is e2 + N , (14.19) e α VG = CG where N denotes the change in lateral (kinetic) quantization energy for the added electron. e2 /C will be called the charging energy in the following. A variation of the source–drain voltage (for a given gate voltage) leads to a so-called Coulomb staircase since more and more channels of conductivity contribute to the current through the device (Fig. 14.27). In Fig. 14.28 the tunneling current is shown as a function of the potential of a dot, formed by gates on a WSe2 flake [1388], and the source-drain voltage. The iso-current lines form so-called ‘Coulomb blockade diamonds’. The charge Q on the QD is determined by the charges on the gate, source and drain capacities, Q = Q G − Q S + Q D . Together with Q S = CS VS , Q D = CD VD and VSD = VS + VD and Q G =

14.4 Quantum Dots

417

2

1.0

0.5

0 -0.6

-0.55

(a)

-0.5 G

(b)

Fig. 14.26 a Conductivity (Coulomb oscillations) and b current–voltage diagram at different gate voltages (Coulomb staircase, shifted vertically for better readability) of a tunnel junction with a quantum dot as in Fig. 14.25. Adapted from [1386], reprinted with permission, ©1991, SpringerNature Fig. 14.27 Chemical potentials of source and drain and of a quantum dot in between them. a, b, and c show the sequence for a variation of the gate voltage and visualize the origin of the Coulomb oscillations (see Fig. 14.26a). d, e and f visualize a variation of the source–drain voltage and the origin of the Coulomb staircase (cf. Fig. 14.26b)

CG (VG − VS ), we find (C = CG + CS + CD ), 1 (Q + CG VG + CD VSD ) C 1 VD = (−Q − CG VG + (C − CD ) VSD ) . C VS =

(14.20) (14.21)

Now, if for a given pair of (VG , VSD ) in a diagram like Fig. 14.28b the current is Coulomb-blocked and low, then it is for all voltages with the same charge Q on the dot and either the same VS or VD . The derivatives of (14.20) and (14.21) yield the slopes ∂ VSD /∂ VG = γ1 = −CG /CD and γ2 = +CG /(CG + CS ), respectively, that defined the borders of the diamond in the schematic stability diagram as depicted in Fig. 14.29. We note that such analysis is allowed when |VS |, |VD | e/2C and the quantum dot circuit can be treated as a system of capacitors (inset in Fig. 14.25a). Changing Q to Q − e requires VG to increase by e/CG for the same VS,D , yielding the periodicity of the stability diagram. Single electron tunneling (SET) circuits [1387] are investigated with respect to metrology for a novel ampere standard [1389].

418

14 Nanostructures

(a)

(b)

Fig. 14.28 a Top: Sketch of WSe2 flake with gate structure, defining a lateral quantum dot. Bottom: SEM image of the structure. The outline of the WSe2 flake (thickness 4.5 nm) is indicated as dotted line. BG: back gate, PG: plunger gate. b Current (in false colors) as a function of the back gate voltage VBG and the source-drain voltage VSD (T = 240 mK). On the top is a current trace as a function of VG (for VSD = 0, along the red dashed line in the diagram). SEM image in panel (a) and panel (b) adapted from [1388] with permission from RSC Fig. 14.29 Schematic Coulomb diamond stability diagram. The slopes γ1 and γ2 are discussed in the text. The periodicity in the gate voltage is given by e/CG . The charge on the dot is Q = (−e) n

A lot of research so far has been done on lithographically defined systems where the lateral quantization energies are small and smaller than the Coulomb charging energy. In this case, periodic oscillations are observed, especially for large N . A deviation from periodic oscillations for small N and a characteristic shell structure (at N = 2, 6, 12) consistent with a harmonic oscillator model (ω0 ≈ 3 meV) has been reported for ≈500-nm diameter mesas (Fig. 14.30b,c). In this structure, a small mesa has been etched and contacted (top contact, substrate back contact and side gate). The quantum dot consists of a 12-nm In0.05 Ga0.95 As quantum well that is laterally constricted by the 500-nm mesa and vertically confined due to 9- and 7.5-nm thick Al0.22 Ga0.68 As barriers (Fig. 14.30a). By tuning the gate voltage, the number of electrons can be varied within 0 and 40. Measurements are typically carried out at a sample temperature of 50 mK. In the sample shown in Fig. 14.31, self-assembled QDs are positioned in the channel under a splitgate structure. In a suitable structure, tunneling through a single QD is resolved. In small self-assembled quantum dots single-particle level separations can be larger than or similar to the Coulomb charging energy. Classically, the capacitance for a metal sphere of radius R0 is given as C0 = 4π 0 r R0 ,

(14.22)

e.g.. C0 ≈ 6 aF for R0 = 4 nm in GaAs, resulting in a charging energy of 26 meV. Quantum mechanically, the charging energy is given in first-order perturbation theory by

14.4 Quantum Dots

419

Fig. 14.30 a Schematic sample geometry for side-gated In0.05 Ga0.95 As/Al0.22 Ga0.68 As disk-shaped quantum dot. b Coulomb oscillations in the current versus gate voltage at B = 0 T observed for a D = 0.5 µm disk-shaped dot. c Addition energy versus electron number for two different dots with D = 0.50 and 0.44 µm. Adapted from [1391]

Fig. 14.31 a Schematic layer sequence of epitaxial structure comprising a n-AlGaAs/GaAs heterointerface with a twodimensional electron gas and a layer of InAs/GaAs quantum dots. b and c are corresponding band diagrams with no gate bias and gate voltage below the critical value, respectively. d Experimental dependence of drain current on gate voltage in a split-gate structure at a drain source voltage of 10 µV. Inset: Dependence of valley current on temperature (squares) with theoretical fit. Reprinted with permission from [1392], ©1997 AIP

E 21 = 00|Wee |00 =

02 (re1 ) Wee (re1 , re2 ) 02 (re2 ) d3 re1 d3 re2 ,

(14.23)

where Wee denotes the Coulomb interaction of the two electrons and 0 the ground state (single particle) electron wavefunction. The matrix element gives an upper bound for the charging energy since the wavefunctions will rearrange to lower their overlap and the repulsive Coulomb interaction. For lens-shaped InAs/GaAs quantum dots with radius 25 nm a charging energy of about 30 meV has been predicted.

420

14 Nanostructures

Fig. 14.32 Lithography and etching techniques for the fabrication of semiconductor structures

14.4.3 Self-Assembled Preparation The preparation methods for QDs split into top-down (lithography and etching) and bottom-up (selfassembly) methods. The latter achieve typically smaller sizes and require less effort (at least concerning the machinery). Artificial Patterning Using artificial patterning, based on lithography and etching (Fig. 14.32), quantum dots of arbitrary shape can be made (Fig. 14.33). Due to defects introduced by high-energy ions during reactive ion etching the quantum efficiency of such structures is very low when they are very small. Using wetchemical etching techniques the damage can be significantly lowered but not completely avoided. Since the QDs have to compete with other structures that can be made structurally perfect, this is not acceptable. Template Growth Template growth is another technique for the formation of nanostructures. Here, a mesoscopic structure is fabricated by conventional means. The nanostructure is created using size-reduction mechanisms, e.g., faceting, (Fig. 14.34). This method can potentially suffer from low template density, irregularities of the template, and problems of reproducibility. Colloids Another successful route to nanocrystals is the doping of glasses with subsequent annealing (color filters). When nanocrystals are prepared in a sol-gel process, the nanoparticles are present as a colloid in wet solution. With the help of suitable stabilizing agents they are prevented from sticking to each other

14.4 Quantum Dots

421

Fig. 14.33 Quantum dots of various shapes created by lithography and etching techniques. From [1393]

Fig. 14.34 a Schematic representation of growth on top of a predefined template, b cross-sectional TEM of quantum dot formation at the apex. Reprinted with permission from [1394], ©1992 MRS

(a)

(b)

and can be handled in ensembles and also individually. Such nanocrystals have been synthesized and investigated in particular for II–VI (Fig. 14.35a) and halide perovskite (Fig. 14.35b) semiconductors. Mismatched Epitaxy The self-assembly (or self-organization) relies on strained heterostructures that achieve energy minimization by island growth on a wetting layer (Stranski-Krastanow growth mode, see Sect. 12.2.3 and [1339]). Additional ordering mechanisms [1397, 1398] lead to ensembles that are homogeneous in size2 [1399] and shape [1400] (Fig. 14.36). When a thin layer of a semiconductor is grown on top of a flat substrate with different lattice constant, the layer suffers a tetragonal distortion (Sect. 5.3.3). Strain can only relax along the growth direction (Fig. 14.37). If the strain energy is too large (highly strained layer or large thickness), plastic relaxation via dislocation formation occurs. If there is island geometry, strain can relax in all three directions and about 50% more strain energy can relax, thus making this type of relaxation energetically favorable. When the island is embedded in the host matrix, the strain energy is similar to the 2D case and the matrix becomes strained (metastable state). When such QD layers are vertically stacked, the individual quantum dots grow on top of each other (Fig. 14.38) if the separation is not too large (Fig. 14.40). This effect is due to the effect of the underlying QD. In the case of InAs/GaAs (compressive strain), the buried QD stretches the surface above it (tensile surface strain). Thus, atoms impinging in the next QD layer find a smaller strain right on top of the buried QDs. In STM images of the cross section through (XSTM) such a stack (Fig. 14.39) individual indium atoms are visible and the shape can be analyzed in detail [1402]. 2 The ordering in size is remarkable. Typically Ostwald ripening (due to the Gibbs-Thomson effect; smaller droplets have larger vapor pressure and dissolve, larger droplets accordingly grow) occurs in an ensemble of droplets or nuclei. In the case of strained QDs, surface energy terms stabilize a certain QD size.

422

14 Nanostructures

(a)

(b)

Fig. 14.35 a CdSe colloidal (hexagonal) nanoparticles. From [1395]. b CsPbBr3 perovskite (cubic) colloidal nanocrystals. Adapted from [1396] under Creative Commons Attribution (CC BY 4.0) license

Fig. 14.36 Self-organized formation of InGaAs/GaAs quantum dots during epitaxy. Left: Plan-view and cross-sectional transmission electron micrographs. Right: Histogram of vertical and lateral size of the quantum dots. Reprinted with permission from [1401], ©1993 AIP

embedded

(eV/nm3)

vacuum

E strain

GaAs

2.2

InAs

EQD E2D GaAs

QD

2D

GaAs

Barr

QD

0

Fig. 14.37 Distribution of strain energy for (left) uncapped island and (right) island embedded in host matrix. Numerical values are for InAs/GaAs

14.4 Quantum Dots

423

Fig. 14.38 Cross-sectional TEM image of a stack of five layers of quantum dots. Due to strain effects, vertical arrangement is achieved Fig. 14.39 Cross-sectional STM image of a stack of five InAs quantum dots in a GaAs matrix. Individual In atoms can be observed in-between the wetting layers and the quantum dots. Each quantum dot layer was formed by growing 2.4 ML of InAs. The intended distance between the quantum dot layers was 10 nm. Image size is 55 × 55 nm2 . Reprinted with permission from [1402], ©2003 AIP Fig. 14.40 Experimentally observed pairing probability in MBE-grown stacks of InAs/GaAs quantum dots as a function of the spacer-layer thickness. Data are taken from (a) (110) and (b) (1–10) cross-sectional TEM images. The filled circles are fit to data from theory of correlated island formation under strain fields. Reprinted with permission from [1403], ©1995 APS

424

14 Nanostructures

Fig. 14.41 Lateral ordering of QD array. d Plan-view TEM of QD array on which the statistical evaluation is based. a Two-dimensional histogram of QDs as a function of the nearest-neighbor distance and direction, (b, c) projections of part (a). Solid lines in (b) and (c) are theory for square array with σ = 20% deviation from ideal position. Adapted from [1339, 1397]

Fig. 14.42 a AFM image of a Si (001) substrate after 960 min of ion sputtering (1.2 keV Ar+ , normal incidence). b Two-dimensional autocorrelation function from a 400 × 400 nm2 area of image in part (a). Adapted from [1406] with permission, ©2001 AIP

The vertical arrangement can lead to further ordering since a homogenization in lateral position takes place. If two QDs in the first layers are very close, their strain fields overlap and the second layer ‘sees’ only one QD. The lateral (in-plane) ordering of the QDs with respect to each other occurs in square or hexagonal patterns and is mediated via strain interaction through the substrate. The interaction energy is fairly small, leading only to short-range in-plane order [1397] as shown in Fig. 14.41. The in-plane ordering can be improved up to the point that regular one- or two-dimensional arrays form or individual quantum dots are placed on designated positions using directed self-assembly [1339]. Among others, dislocation networks buried under the growth surface of the nanostructure, surface patterning and modification have been used to direct the QD positioning. Ion-Beam Erosion During the erosion of a surface with low-energy ion beam sputtering ordered patterns of dots appear [1404–1407]. Isotropic [1408] and hexagonal [1404, 1406] (Fig. 14.42) near-range ordering has been observed. The pattern formation mechanism is based on the morphology-dependent sputter yield and further mechanisms of mass redistribution [1409]. Also linear patterns have been reported [1410].

14.4 Quantum Dots

425

Fig. 14.43 Optical emission spectra (T = 2.3 K) of a single InGaAs/GaAs quantum dot at different laser excitation levels P as labeled. The single exciton (X) and biexciton (XX) lines are indicated. Adapted from [1411]

14.4.4 Optical Properties The optical properties of QDs are related to their electronic density of states. In particular, optical transitions are allowed only at discrete energies due to the zero-dimensional density of states. Photoluminescence from a single QD is shown in Fig. 14.43. The δ-like sharp transition is strictly true only in the limit of small carrier numbers ( 1 exciton per dot on average) since otherwise many-body effects come into play that can encompass recombination from charged excitons or multiexcitons. At very low excitation density the recombination spectrum consists only of the one-exciton (X) line. With increasing excitation density small satellites on either side of the X-line develop that are attributed to charged excitons (trions) X+ and X− . On the low-energy side, the biexciton (XX) appears. Eventually, the excited states are populated and a multitude of states contribute with rich fine structure. In bulk material the biexciton (Sect. 9.7.10) is typically a bound state, i.e. its recombination energy E XX is lower than that of the exciton E X . A similar situation is present in Fig. 14.43. It was pointed out in [1412] that in QDs the biexciton recombination energy can also be larger than the exciton recombination energy. In [1413] the modification of the QD confinement potential of InAs/GaAs QDs by annealing was reported. The exciton binding energy (E X -E XX ) is tuned from positive (‘normal’) to negative values upon annealing (Fig. 14.44). The charging state of the exciton can be controlled in a field-effect structure. The recombination energy is modified due to Coulomb and exchange effects with the additional carriers. In charge-tunable quantum dots [1414] and rings [1415] exciton emission has been observed in dependence of the number of additional electrons. The electron population can be controlled in a Schottky-diode-like structure through the manipulation of the Fermi level with the bias voltage. At high negative bias all charge carriers tunnel out of the ring and no exciton emission is observed. A variation of the bias then leads to an average population with N = 1, 2, 3, . . . electrons. The recombination of additional laser-excited

426

14 Nanostructures

Fig. 14.44 Biexciton binding energy determined for a single InAs/GaAs quantum dot for various annealing times. Data from [1413]

Fig. 14.45 Luminescence of charged excitons from a single quantum ring at T = 4.2 K versus the bias voltage with which the number of electrons in the quantum dot N is tuned from zero to N > 3. Adapted from [1415], reprinted with permission, ©2000, Springer Nature

excitons depends (due to the Coulomb interaction) on the number of the electrons present (Fig. 14.45). The singly negatively charged exciton X− is also called a trion. The interaction of a spin with an exciton in a CdTe quantum dot has been observed in [1416]. If the CdTe quantum dot is pure, a single line arises. If the dot contains a single Mn atom, the exchange interaction of the exciton with the Mn S = 5/2 spin leads to a six-fold splitting of the exciton line (Fig. 14.46. In an external magnetic field a splitting into a total of twelve lines due to Zeeman effect at the Mn spin is observed. In a QD ensemble, optical transitions are inhomogeneously broadened due to fluctuations in the QD size and the size dependence of the confinement energies (Fig. 14.47). Interband transitions involving electrons and holes suffer from the variation of the electron and hole energies: ∂ Ee ∂ Eh + δL . σ E ∝ ∂L ∂L

(14.24)

A typical relative size inhomogeneity of σ L /L of 7% leads to several tens of meV broadening. Additional to broadening due to different sizes fluctuations of the quantum dot shape can also play a role. The confinement effect leads to an increase of the recombination energy with decreasing quantumdot size. This effect is nicely demonstrated with colloidal quantum dots of different size as shown in Fig. 14.48.

14.4 Quantum Dots Fig. 14.46 Photoluminescence spectrum of a single CdTe/ZnSe quantum dot containing a single Mn atom (T = 5 K). Adapted from [1416], reprinted with permission, ©2004 APS

Fig. 14.47 Ensemble photoluminescence spectrum (T = 293 K, excitation density 500 W/cm2 ) of InAs/GaAs QDs

Fig. 14.48 Luminescence (under UV excitation) from flasks of colloidal CdTe quantum dots with increasing size (from left to right). From [1395]

427

Chapter 15

External Fields

Abstract The effects of external electric and magnetic fields on the electronic and optical properties of bulk materials and quantum wells are discussed including the Stark effect and quantum-confined Stark effect, the Hall effect and Quantized Hall Effects. The energy levels of the solid and its optical and electronic properties depend on external electric and magnetic fields. In high magnetic fields and at low temperatures the quantum Hall effects give evidence for new states of matter in many-body systems.

15.1 Electric Fields 15.1.1 Bulk Material The center-of-mass motion of the exciton is not influenced by a homogeneous electric field. The Hamilton operator for the relative motion of an electron-hole pair of reduced mass μ along z in the presence of an electric field E along the z direction is Hˆ = − −eEz . 2μ 2

(15.1)

Here, the Coulomb interaction, leading to the formation of bound exciton states, is neglected. In the plane perpendicular to the field (here the z direction) the solutions for the relative motion are just plane waves. In the electric field the bands are tilted (Fig. 15.1), i.e. there is no longer an overall band gap. Accordingly, the wavefunctions are modified and have exponential tails in the energy gap. After separation of the motion in the (x,y) plane the Schrödinger equation for the motion in the z direction is 2 d 2 (15.2) − e E z − E z φ(z) = 0 , − 2μ dz 2 which is of the type

d2 f (ξ ) − ξ f (ξ ) = 0 , dξ 2

© Springer Nature Switzerland AG 2021 M. Grundmann, The Physics of Semiconductors, Graduate Texts in Physics, https://doi.org/10.1007/978-3-030-51569-0_15

(15.3)

429

430

15 External Fields E=0 e2

e2

e1

e1

h

h

EC h

E 0

Eg

h1

h1 h2 h3 h4 h5

EV (b)

(a)

h2 h3 h4 h5

Fig. 15.1 Impact of an electric field on a bulk material (tilt of bands) and b a quantum well (quantum confined Stark effect, QCSE)

0.4 0.5 0.2 0

0

-0.5

-0.2 -0.4

(a)

-10

-8

-6

-4

-2

0

2

4

(b)

-1

-10

-8

-6

-4

-2

0

2

4

Fig. 15.2 a Airy function Ai(x), b Ai’(x)

2 2 2 1/3 1/3 e E with ξ = Ez − z 2μ e E and the optoelectronic energy = . The solution of (15.3) is 2 2μ given by the Airy function Ai (cf. Fig. 15.2): √ φ E z (ξ ) =

eE Ai(ξ ) .

(15.4)

The pre-factor guaranties the orthonormality (with regard to the E z ). The absorption spectrum is then given by 1√ π Ai 2 (η) − η Ai 2 (η) , (15.5) α(ω, E) ∝ ω with η = (E g − E)/ and Ai (x) = d Ai(x)/dx. Optical transitions below the band gap become possible that are photon-assisted tunneling processes. The below-bandgap transitions have the form of an exponential tail. Additionally, oscillations develop above the band gap, the so-called Franz-Keldysh oscillations (FKO) [1417, 1418] (Fig. 15.3a). The absorption spectrum scales with the optoelectronic energy . The energy position of the FKO peaks E n is periodic with (ν ∼ 0.5)

En − Eg

3/2

∝ (n − ν) E

√ μ.

(15.6)

15.1 Electric Fields

30

0.10

e-hh

25 -1

(10 cm )

0.05

3

0 = (E)- (0)

Fig. 15.3 a Theoretical absorption (top panel) with (solid line) and without (dash-dotted line) electric field for a volume semiconductor (without Coulomb interaction) and theoretical change of absorption (bottom panel). b Experimental absorption spectra of (In,Ga)As on InP at T = 15 K for various applied voltages as labeled. Adapted from [1421]

431

2

0.005

4

3 1

0.80

(a)

5

0.84

e-lh

15 10

0 -0.005

20

5

0.3V 0.2V 0V 0.5V

InGaAs 2.0V 0 0.80 0.81 0.82 0.83 0.84

0.88

(b)

A more detailed theory including interband coupling and excitonic effects can be found in [1419]. The effect is best determined with modulation spectroscopy can measuring the difference of absorption with and without field [1420] since it exhibits more defined features (Fig. 15.3a, lower panel). A nonperiodicity can indicate a nonparabolicity of the mass. Also, the contributions of heavy and light holes merge. For a given mass the electric field strength can be determined. Well-pronounced oscillations are only present for homogeneous fields. Experimental spectra show additionally the peaks due to excitonic correlation (Fig. 15.3b) at low field strength. At higher fields the FKO evolve and the amplitude of the excitonic peaks decreases because the excitons are ionized in the field.

15.1.2 Quantum Wells In a quantum well an electric field along the confinement direction (z direction) causes electrons and holes to shift their mean position to opposite interfaces (Fig. 15.1b). However, excitons are not ionized due to the electric field. With increasing field (for both field directions) the energy position of the absorption edge and the recombination energy is reduced. This is the quantum confined Stark effect (QCSE). Corresponding experimental data are shown in Fig. 15.4i–v. The shift depends quadratically on the electric field since the exciton has no permanent dipole moment (mirror symmetry of the quantum well). Thus, only the second-order Stark effect is present (as for the hydrogen atom) in which the field first induces a dipole p = αE. This dipole interacts with the field with an energy E = −p · E = −αE2 . The carrier separation in opposite sides of the quantum well (Fig. 15.4b) leads to a reduced overlap of the electron and hole wavefunctions and subsequently to an increased recombination lifetime (see Fig. 12.43). If the field is within the quantum-well interface plane, the field leads to the ionization of excitons without shift of the energy position. The loss of the excitonic peak is visualized in the spectra in Fig. 15.4a–c.

432

15 External Fields

AlGaAs/ GaAs

(ii)

(i)

AlGaAs/ GaAs

(iii)

(iii)

(iv) (v)

(ii) (i)

(a)

1.42

1.46

1.50

(b)

1.43

1.45

1.47

Fig. 15.4 Impact of electric fields on the absorption spectrum of n × (9.5 nm GaAs/9.8 nm Al0.32 Ga0.68 As) multiple quantum well structures. a Electric field along the [001] growth direction (n = 50), (i)–(v) E = 0, 0.6, 1.1, 1.5, and 2 × 105 V/cm. b Electric field within the interface plane (n = 60), (i, ii, iii) E = 0, 1.1, and 2×105 V/cm. Adapted from [1422]

15.2 Magnetic Fields In magnetic fields, electrons (or holes) perform a cyclotron motion with frequency ωc = eB/m ∗ , i.e. a motion perpendicular to the magnetic field on a line of constant energy in k-space. This line is the intersection of a plane perpendicular to the magnetic field and the respective isoenergy surface in kspace. For semiconductors with anisotropic mass, such as Si and Ge, the quantum theory of cyclotron resonance has been given in [1423]. The physics of semiconductors in magnetic fields is covered in detail in [1424]. The ballistic cyclotron motion can only occur between two scattering events. Thus, a significantly long path along the cyclotron trajectory (classically speaking) and the connected magnetotransport properties are only possible when – ωc τ 1, i.e. when the average scattering time τ is sufficiently large. This requires high mobility. – the magnetic field is sufficiently strong and the temperature sufficiently low, i.e. ωc kT , such that thermal excitations do not scatter electrons between different Landau levels. – the cyclotron path is free of geometric obstructions. An external magnetic field also produces a Zeeman-like splitting of the spin states. For the electron, the energy splitting E is given by (15.7) E = ge∗ μB B , where B is the magnetic-field amplitude and ge∗ the (effective) electron g-factor. This value differs from the free-electron value in vacuum of ge = 2.0023 due to the presence of spin-orbit interaction (see Sect. 15.2.3). Values for ge∗ at low carrier density and low temperatures are 2 for Si, 1.2 for InP and ZnSe, −1.65 for CdTe, −0.44 for GaAs, −15 in InAs, and −50 for InSb. In [1425] the temperature dependence of ge∗ in GaAs, InP and CdTe is also measured and discussed. The electron g-factor increases in thin GaAs/(Al,Ga)As quantum wells [1426].

15.2.1 Classical Hall Effect An electrical current along the x (longitudinal) direction in a perpendicular magnetic field B = (0, 0, B) along z causes an electric field E y along the transverse (y) direction (Fig. 15.5). The charge accumu-

15.2 Magnetic Fields

433

B

z y

v F

B

x

w V

I

H

Fig. 15.5 Scheme of the Hall-effect geometry. The movement of one electron in the longitudinal electric current I is shown schematically. The coordinate system (x, y, z) and the directions of the magnetic field B, the drift velocity of an electron v and the resulting Lorentz force F are given. The transverse field E y is given by VH /w

Vxx

Fig. 15.6 Hallbar geometry. The current I is driven by a source from contact 1 to 2. The Hall voltage is measured between contacts 3 and 4, the longitudinal voltage between 3 and 5

5

3

I

1

Bz

Vxy=VH

4

2

I

6

lation is due to the Lorentz force. The related transverse voltage is called the Hall voltage and the resistivity ρx y = E y /jx the Hall resistivity [28, 31, 32]. Many aspects of the Hall effect are discussed in [1427]. For thin-film samples typically Hall bars [1428] (see Fig. 15.6 and also Fig. 15.19, for a reasonable measurement of the Hall voltage the ratio of length and width of the Hall bar should be at least 3) or the van-der-Pauw geometry (Fig. 15.7) and method are used [1429–1431]. For band transport in the relaxation time approximation (Chap. 8.2), the steady-state equation of motion is (in the vicinity of an isotropic extremum) m∗

v = q (E + v × B) . τ

(15.8)

We note that this equation of motion is also valid for holes, given the convention of Sect. 6.10.1, i.e. positive effective mass and charge. With the cyclotron frequency ωc = q B/m ∗ the conductivity tensor is (j = qnv = σ E) ⎞ σx x σx y 0 σ = ⎝ σ yx σ yy 0 ⎠ 0 0 σzz 1 1 = σ0 σx x = σ yy = σ0 1 + ωc2 τ 2 1 + μ2 B 2 μB ωc τ = σ0 σx y = −σ yx = σ0 2 2 1 + ωc τ 1 + μ2 B 2 ⎛

(15.9a) (15.9b) (15.9c)

434

15 External Fields

(a)

(b)

(c)

(d)

(e)

Fig. 15.7 a–d Geometry for van-der-Pauw Hall measurements. a Best geometry (cloverleaf), b acceptable square geometry with small contacts on the corners, c,d not recommended geometries with contacts on the edge centers or inside the square, respectively. e Current distribution, as visualized by lock-in thermography [1432], in epitaxial ZnO layer on sapphire with Hall geometry as in part b. Grey dashed line indicates the outline of the 10 × 10 mm2 substrate, grey areas indicate gold ohmic contacts

σzz = σ0 =

q2 n τ =qnμ . m∗

(15.9d)

Perpendicular to the magnetic field, the conductivity (σzz ) is given by (8.5). If only one type of carrier (charge q, density n) is considered, the condition j y = 0 leads to E y = μB E x and jx = σ0 E x . The Hall coefficient is defined as RH = E y /( jx B) or more precisely as RH =

ρx y , B

(15.10)

where the resistivity tensor ρ is the inverse of the conductivity tensor σ , ⎛ ρ = σ −1 = ρx x = ρ yy = ρx y = −ρ yx = ρzz =

⎞ ρx x ρx y 0 ⎝ ρ yx ρ yy 0 ⎠ 0 0 ρzz σx x 2 σx x + σx2y σx y σx2x + σx2y 1 1 = . σzz σ0

(15.11a) (15.11b) (15.11c) (15.11d)

For a single type of carriers, the Hall coefficient is therefore given by RH =

μ 1 . = σ0 qn

(15.12)

It is negative (positive) for electron (hole) conduction. We note that electrons and holes are deflected in the same y-direction by the magnetic field and collect at the same electrode. Thus the Hall effect

15.2 Magnetic Fields

435

allows the determination of the carrier type and the carrier density.1 If both types of carriers are present simultaneously, the conductivity (two-band conduction) is given by the sum of electron and hole conductivity (8.11), σ = σe + σh .

(15.13)

−n μ2e (1 + μ2h B 2 ) + p μ2h (1 + μ2e B 2 ) 1 . e n 2 μ2e (1 + μ2h B 2 ) − 2 n p μe μh (1 + μe μh B 2 ) + p 2 μ2h (1 + μ2e B 2 )

(15.14)

The Hall constant (15.10) is then RH =

Under the assumption of small magnetic fields,2 i.e. μB 1, the Hall coefficient is 1 RH = e

−n μ2e + p μ2h n p (−n + p) μ2e μ2h (μe − μh )2 2 + B + ... . (−n μe + p μh )2 (−n μe + p μh )4

(15.15)

For small magnetic field this can be written as RH =

1 p − n β2 , e ( p − n β)2

(15.16)

with β = μe /μh < 0. For large magnetic fields, i.e. μB 1, the Hall coefficient is given by RH =

1 1 . e p−n

(15.17)

In Fig. 15.8, the absolute value of the Hall coefficient for InSb samples with different doping concentrations is shown. The p-doped samples exhibit a reverse of the sign of the Hall coefficient upon increase of temperature when intrinsic electrons contribute to the conductivity. The zero in RH occurs for n = p μ2h /μ2e = n i /|β|. For high temperatures, the Hall coefficient for n- and p-doped samples is dominated by the electrons that have much higher mobility (Table 8.2). The simultaneous conduction in a band and an impurity band (cmp. Sect. 8.6) has been separated with a suitable model assuming two conduction channels for holes [1434] (Fig. 15.9). In (15.8) an isotropic mass was considered. For semiconductors with multiple valleys and anisotropic extrema, in particular the conduction bands of Si and Ge (cf. Sect. 6.9.2), the Hall coefficient has been derived in [1435, 1436]. With K = m l /m t being the mass anisotropy (cmp. Table 6.5), the Hall coefficient (15.12) changes to, RH =

1 3 K (K + 2) . q n (2K + 1)2

(15.18)

In the derivation of the (unipolar) Hall coefficient we had assumed that all carriers involved in the transport have the same properties, in particular that they are subject to the same scattering time. This assumption is generally not the case (cmp. Chap. J) and we need to operate with the ensemble average of the discussed quantities. The ensemble average of an energy-dependent quantity ζ (E) over the

1 Using the Hall effect, the net free charge carrier concentration is determined. We note that the concentration of fixed charges in semiconductors can be investigated by depletion layer spectroscopy (Sect. 21.2.4). 2 We note that for a mobility of 104 cm2 /Vs, μ−1 is a field of B = 1 T.

436

15 External Fields

Fig. 15.8 a Conductivity and b absolute value of the Hall coefficient versus inverse temperature for four p-doped (A–D) and two n-doped (E, F) InSb samples. The doping levels are given in (a). Adapted from [1433] Fig. 15.9 Carrier densities in valence band (circles) and impurity band (triangles) from evaluating the Hall effect on GaAs doped with lithium (and annealed) taking into account two conduction channels. Adapted from [1434]

Hole concentration (cm-3)

1018

200

Temperature (K) 100 70

50

GaAs:Li impurity band

1017

1016

1015

valence band

5

10 15 1000/T (1/K)

20

(electron) distribution function f (E) is denoted as ζ and is given as3 ζ =

ζ (e) f (E) dE . f (E) dE

(15.19)

In particular, the average τ 2 is now different from τ 2 . Considering the equation j = σ E for the ensemble-averaged current density we find (for one type of carrier, cf. (15.12))

3 For this consideration it is assumed that the energy dependence is the decisive one. Generally, averaging may have to be performed over other degrees of freedom as well, such as the spin or, in the case of anisotropic bands, the orbital direction.

15.2 Magnetic Fields

437

RH =

1 rH , qn

(15.20)

with the so-called Hall factor rH given by γ , α 2 + ωc2 γ 2 τ2 τ , γ = . α= 1 + ωc2 τ 2 1 + ωc2 τ 2

rH =

(15.21)

The Hall factor depends on the scattering mechanisms and is of the order of 1. For large magnetic fields the Hall factor approaches 1. For small magnetic fields we have RH =

1 τ 2

. q n τ 2

(15.22)

The mobility calculated from (cf. (15.9d)) σ0 RH is called the Hall mobility μH and is related to the mobility via (15.23) μH = rH μ . It is assumed so far that the free carrier density and mobility are homogeneous within the volume of current transport. Multi-layer models can be fitted to experimental Hall data in order to account for different conduction channels in different layered parts of the sample [1437]. E.g., in a two-layer model, contributions from bulk and surface/interface conduction can be separated [1438–1440]. The magnetic field dependence of σ can be used in a general case to separate contributions of carriers with different density and mobility (including its sign) without assumptions and obtain the mobility spectrum s(μ) (MSA, mobility spectral analysis), ∞ σx x =

s(μ)

1 dμ 1 + μ2 B 2

(15.24a)

s(μ)

μB dμ , 1 + μ2 B 2

(15.24b)

−∞ ∞

σx y = −∞

as a generalization of (15.13), (15.9b) and (15.9c) [1441–1443]. Examples are the separation of electron conductivity in (GaAs-) - and (InAs-) X-Minima in a GaAs/(Al,Ga)As/InAs double quantum well structures [1441] (Fig. 15.10a), substrate and 2DEG electron conductivity in (Al,Ga)N/GaN heterostructures [1444], and electrons and holes in an InAs/GaSb quantum well [1442] (Fig. 15.10b). In the case of hopping conduction (Chap. 8.8), the theory of Hall effect is more involved [1445, 1446]. If carriers are transported by hopping, generally, they may not be free to move as expected by (15.8) in response to the applied magnetic field and the Lorentz force. A Hall effect occurs only at the junction of three (or more) hopping sites [1445]. The sign of the experimentally determined Hall coefficient is often opposite to the one expected from the carrier type according to (15.12), e.g., as studied in a-Si [1447, 1448]. The sign anomaly depends on intricacies such as the local site geometry and interference processes taking place among bonding and antibonding orbitals of various numbers as summarized in [1449].

438

15 External Fields 5

104

10

10

(a)

10

AlAs/GaAs

Conductivity (arb. units)

Conductivity (arb. units)

10

X 3

10

2 4

3

InAs/GaSb

electrons

104

electrons

-10 -10 -10 2 Mobility (cm /Vs)

5

10

2

holes 3D 3

2D 2

-10

5

-10

4

3

2

2

-10 -10 10 2 Mobility (cm /Vs)

(b)

10

3

10

4

Fig. 15.10 a Mobility spectrum of GaAs/(Al,Ga)As/InAs double quantum well structure. Adapted from [1441]. b Mobility spectrum of InAs/GaSb quantum well structure. Adapted from [1442]

15.2.2 Free-Carrier Absorption The absorption of free carriers was treated in Sect. 9.9.1 without the presence of a static magnetic field. Solving (15.8) for a static magnetic field B = μ0 H with H = H (h x , h y , h z ) and a harmonic electric field E ∝ exp(−iωt) yields for the dielectric tensor (cf. (9.72)) =

i 0 ω

σ ,

(15.25)

and by comparing to j = σ E = q n v, ⎡

⎛

⎞⎤−1 0 −h z h y (ω) = −ωp∗2 ⎣(ω2 + i ω γ ) 1 − i ωc2 ⎝ h z 0 −h x ⎠⎦ , −h y h x 0

(15.26)

where 1 denotes the (3 by 3) unity matrix and γ = 1/τ = q/(m ∗ μ) is the damping parameter with μ representing the optical carrier mobility (in the non-isotropic case a tensor γ needs to be used). The (unscreened) plasma frequency is given by (cmp. (9.77)) ωp∗ =

n

The free-carrier cyclotron frequency is ωc = e

e2 . 0 m ∗

(15.27)

μ0 H . m∗

(15.28)

If the effective mass is treated as a tensor, 1/m ∗ is replaced by m∗ −1 in (15.27) and (15.28). For zero magnetic field the classical Drude theory for one carrier species is recovered (cf. (9.74a)) (ω) = −

ωp∗2 ω (ω + iγ )

.

(15.29)

15.2 Magnetic Fields

439

With the magnetic field perpendicular to the sample surface, i.e. B = μ0 (0, 0, H ) the magneto-optic dielectric tensor simplifies to (cf. (15.9d)) (ω) = ˜x x = ˜zz = ˜x y =

⎞ ˜x x i˜x y 0 − 2 ⎝ −i˜x y ˜x x 0 ⎠ ω 0 0 ˜zz 1 + iγ /ω (1 + iγ /ω)2 − (ωc /ω)2 1 (1 + iγ /ω) ωc /ω . (1 + iγ /ω)2 − (ωc /ω)2 ωp∗2

⎛

(15.30a) (15.30b) (15.30c) (15.30d)

The in-plane component x x provides information about ωp∗ and γ , i.e. two of the three parameters n, μ and m ∗ are known. Additionally, the antisymmetric tensor component x y is linear in the cyclotron frequency and provides q/m ∗ . This subtle but finite birefringence depends on the strength (and orientation) of the magnetic field and can be experimentally determined in the infrared using magneto-ellipsometry [1450, 1451]. Such ‘optical Hall effect’ experiment allows the determination of the carrier density n, the mobility μ, the carrier mass4 m ∗ and the sign of the carrier charge sgn(q) with optical means. The electrical Hall effect (Sect. 15.2.1) can reveal n, μ and sgn(q) but cannot reveal the carrier mass.

15.2.3 Energy Levels in Bulk Crystals In a 3D electron gas (the magnetic field is along z, i.e. B = B (0, 0, 1)) the motion in the (x, y) plane is described by Landau levels. Quantum mechanically they correspond to levels of a harmonic oscillator. The magnetic field has no impact on the motion of electrons along z, such that in this direction a free dispersion relation ∝ k z2 is present. The energy levels are given as 1 2 2 ωc + k . E nkz = n + 2 2m z

(15.31)

Thus, the states are on concentric cylinders in k-space (Fig. 15.11a). The populated states of the 3D electron gas (at 0 K) lie within the Fermi vector of length kF . For the 3D system the density of states at the Fermi energy is a square root function of the Fermi energy (6.71). In the presence of a magnetic field the density of states diverges every time that a new cylinder (with a one-dimensional density of states, (6.79)) touches the Fermi surface at E F . In real systems, the divergence will be smoothed, however, a pronounced peak or the periodic nature of the density of states is often preserved. The period is given by the number n m of cyclotron orbits (Landau levels) within the Fermi surface. 1 nm + ωc = E F . 2

(15.32)

If the number of carriers is constant, the density of states at the Fermi energy at varying magnetic field varies periodically with 1/B. From the conditions (n m + 21 )eB1 /m = E F and (n m + 1 + 21 )eB2 /m = E F with 1/B2 = 1/B1 + 1/B we find, 4 We note that mobility and effective mass defined and measured in this way may be referred to as ‘optical’. Other definitions and approaches to the mobility or effective mass may give different results.

440

15 External Fields

kz

h

B

c

n=0 n=1 n=...

3D

n=nm

ky

kx EF

(a)

(b)

0 1/2

3/2

5/2

7/2

EF

E

Fig. 15.11 3D electron gas in an external magnetic field. a Allowed states in k-space for magnetic field along the z direction. b Density of states (DOS) ρ versus energy (in units of ωc ). Dashed line is three-dimensional DOS without magnetic field. Based on [1123]

e 1 = ∗ . B m EF

(15.33)

This periodicity is used to determine experimentally, e.g., the properties of the Fermi surface in metals using the Shubnikov-de Haas oscillations (of the magnetoresistance) or the de Haas-van Alphén effect (oscillation of the magnetic susceptibility). Equation (15.31) needs to be extended to account for the splitting (15.7) of the Landau level due to the electron spin. According to [1452], the electron Landau level energy can be written as e B 1 ± ge∗ (E) μB B , En = n + 2 m ∗ (E)

(15.34)

with energy dependent effective mass and g-factor 2 1 E g (E g + 0 ) 1 1 = + m ∗ (E) m ∗ (0) 3E g + 20 E + Eg E + E g + 0 E (E + ) 1 1 g g 0 ge∗ (E) = ge∗ (0) − 0 E + Eg E + E g + 0

(15.35a) (15.35b)

The band edge value m ∗ (0) of the effective mass is given by (6.43) and that of the g-factor by ge∗ (0) = 2 1 −

2 0 EP 3 E g (E g + 0 )

.

(15.36)

For large spin-orbit splitting, the value of the g-factor deviates strongly from 2 and becomes negative.

15.2.4 Magnetic Field Effect on Impurities The Zeeman effect is the magnetic field dependence (and the lifting of degeneracies) of spectral lines. For semiconductor physics this is a tool to investigate properties of defect related states with sufficiently sharp spectral features. As example we refer to the investigation of the Si:P donor system

15.2 Magnetic Fields

441

(cmp. Fig. 9.33) and its linear and quadratic Zeeman effect [1453] as visualized in Fig. 15.12. The difference in transition energies for lines 4 and 1 depends linearly on the magnetic field and is equal to the electron spin splitting. The quadratic Zeeman effect is also termed ‘diamagnetic shift’ and allows a determination of the wavefunction size. In the present case, the electron Bohr radius at the neutral phosphorus donor in Si was found to be aD = 1.33(5) nm (cmp. (7.22)) [1453].

15.2.5 Magnetic Field Effect on Excitons The effect of an magnetic field on excitons is similar to that on the wave function at an impurity, except that the electron and hole are effected simultaneously. The effect is two-fold: The Zeeman-like effect on the spin states leads to a splitting of the exciton lines which become circularly polarized; for ‘weak’ fields the splitting is linear with the field. Additionally, the magnetic field leads to a reduction of exciton size leading to a quadratic shift of the line center to larger energies, the so-called diamagnetic shift. Calculations for various confinement geometries have been given in [1454]. The change of exciton size leads also to modification of localization effects in disordered quantum wells [1455]. As example the magnetic field dependence of quasi two-dimensional excitons in a WS2 monolayer is shown in Fig. 15.13 (cf. Sect. 13.2.4).

15.2.6 Energy Levels in a 2DEG In a 2D electron gas (2DEG), e.g., in a quantum well or a potential well at a modulation-doped heterointerface, a free motion in z is not possible and k z is quantized. The energy levels (for each 2D subband) are only given by the cyclotron energy (Fig. 15.14a). The density of states is a sequence of δ-like peaks (Fig. 15.14b). Each peak contributes (degeneracy gˆ of a Landau level) a total number of gˆ =

(a)

eB h

(15.37)

(b)

Fig. 15.12 a Schematic level scheme and transitions (and their polarization) of donor bound excitons at Si:P. b Experimental magnetic field dependent shift of photoluminescence transition energies (from about E = 1.150 eV at B = 0 T) (symbols) together with fits for heavy (dashed lines) and light (solid lines) hole transitions. Adapted from [1453]

442

15 External Fields

Fig. 15.13 Magnetic field effect on excitons in WS2 monolayer. a Normalized transmission spectra. b Energy position of E σ + and E σ − of (circularly polarized) spectral lines of the 1–5 s exciton lines. c Calculated energy (E σ + + E σ − )/2, showing the diamagnetic shift. Solid lines are model calculation with reduced exciton mass m ∗r = 0.175 (and further parameters), d Zeeman splitting E σ + − E σ − of the 1–3 s states together with linear fits (dashed line), g-factors are around 4, as labelled. Adapted from [1313], reprinted under Creative Commons Attribute (CC BY 4.0) license Fig. 15.14 2D electron gas in an external magnetic field. a Allowed states in k-space. b Density of states (DOS) ρ versus energy. Dashed line is two-dimensional DOS without magnetic field. Thick vertical lines: δ-like DOS without broadening, curves: broadened DOS. Based on [1123]

ky

h

c

kx

2D

n=0 n=1 n=2 (a)

EF(0)

(b) E1

E1+h c/2

EF(0)

E

states (per unit area without spin degeneracy and without the degeneracy of the band extremum). In reality, disorder effects lead to an inhomogeneous broadening of these peaks. The states in the tails of the peaks correspond to states that are localized in real space. Also, in a 2D system several physical properties exhibit an oscillatory behavior as a function of Fermi level, i.e. with varying electron number, and as a function of the magnetic field at fixed Fermi energy, i.e. at fixed electron number (Fig. 15.15).

15.2.7 Shubnikov-De Haas Oscillations From the 2D density of states (per unit area including spin degeneracy) D 2D (E) = m ∗ /π 2 the sheet density of electrons n s can be expressed as a function of the Fermi level (at T = 0 K without spin degeneracy) m∗ EF . (15.38) ns = 2π 2 Using (15.33) we thus find (without spin degeneracy, without valley degeneracy), that the period of 1/B is ∝ n s :

15.2 Magnetic Fields

(meV)

35

(a)

30 25 30

Magnetization

Fig. 15.15 Oscillatory (theory, T = 6 K) behavior of a 2DEG (GaAs/(Al,Ga)As) in a magnetic field: a Fermi level, b magnetization, c specific heat, d thermoelectric power. A Gaussian broadening of 0.5 meV was assumed. Adapted from [1123, 1456]

443

(b)

20 10 0 -10 -20 -30 15

(c)

10 5

Thermoelectric

0

0.2 0.1 0 0

e 1 1 = . B h ns

(d)

0.3

2

4

6

8

10

(15.39)

The carrier density of a 2DEG can therefore be determined from the oscillations of magnetoresistance, and is proportional to the density of states at the Fermi level (Shubnikov-de Haas effect). A corresponding measurement with varying field and fixed electron density is shown in Fig. 15.16. The periodicity with 1/B is obvious. Since only the component of the magnetic field perpendicular to the layer affects the (x, y) motion of the carriers, no effect is observed for the magnetic field parallel to the layer. In another experiment the carrier density was varied at constant field (Fig. 15.17). The electron density in an inversion layer in p-type silicon is (linearly) varied with the gate voltage of a MOS (metal-oxide-semiconductor) structure (inset in Fig. 15.17, for MOS diodes cf. Sect. 24.5). In this experiment, the Fermi level was shifted through the Landau levels. The equidistant peaks show that indeed each Landau level contributes the same number of states.

444

15 External Fields

Fig. 15.16 Shubnikov-de Haas oscillations at a modulation-doped (Al,Ga)As/GaAs heterostructure with a 2DEG, n = 1.7 × 1017 cm−2 and μ = 11 400 cm2 /Vs. Data from [1457]

Fig. 15.17 Shubnikov-de Haas oscillations of a 2DEG at the (100) surface of p-type silicon (100 cm) at a magnetic field of B = 3.3 T and T = 1.34 K. The inset shows schematically the contact geometry. Data from [1458]

oxide n+

n+ silicon

0

20

40

60

80

100

15.2.8 Quantum Hall Effect In high magnetic fields, at low temperatures and for high-mobility, 2D electron gases exhibit a deviation from the classical behavior. We recall that the classical Hall effect (i.e. considering the Lorentz force, classical Drude theory), the generation of a field E y perpendicular to a current flow jx (cf. Sect. 15.2.1), was described with the conductivity tensor σ (here, for the (x, y)-plane only) σ0 1 ωc τ 1 + ωc2 τ 2 −ωc τ 1 1 = σ0 →0 1 + ωc2 τ 2 ωc τ ne , = σ0 → 2 2 1 + ωc τ B

σ = σx x σx y

(15.40a) (15.40b) (15.40c)

where σ0 is the zero-field conductivity σ0 = ne2 τ/m ∗ (8.5). The arrows denote the limit for ωc τ → ∞, i.e. large fields. The resistivity tensor ρ = σ −1 is given by ρx x ρx y −ρx y ρx x σx x = 2 →0 σx x + σx2y

ρ= ρx x

(15.41a) (15.41b)

15.2 Magnetic Fields

445

Fig. 15.18 Hall resistivity ρx y and longitudinal resistivity ρx x for a modulation-doped GaAs/(Al,Ga)As heterostructure (n = 4 × 1011 cm−2 , μ = 8.6 × 104 cm2 /Vs) at 50 mK as a function of magnetic field (10 kG=1 T). The numbers refer to the quantum number and spin polarization of the Landau level involved. The inset shows schematically the Hall bar geometry, VL (VH ) denotes the longitudinal (Hall) voltage drop. Reprinted with permission from [1459], ©1982 APS

ρx y =

15.2.8.1

−σx y B . →− σx2x + σx2y ne

(15.41c)

Integer QHE

Experiments yield strong deviations from the linear behavior of the transverse resistivity ρx y ∝ B (15.41c) for large magnetic fields at low temperatures for samples with high carrier mobility, i.e. ωc τ 1 (Fig. 15.18). In Fig. 15.19a, b, Hall bars are shown for 2DEGs in silicon metal-oxidesemiconductor field-effect transistor (Si-MOSFET) electron inversion layers and at GaAs/(Al,Ga)As heterostructures, respectively. The Hall resistivity exhibits extended Hall plateaus with resistivity values that are given by e2 1 , =ν ρx y h

(15.42)

446

15 External Fields

( a)

(b)

Fig. 15.19 a Silicon MOS (metal-oxide-semiconductor) structure of K. v. Klitzing’s et al. original experiments. b GaAs/(Al,Ga)As heterostructure sample grown with molecular beam epitaxy for QHE measurements, chip carrier and bond wires. Reprinted with permission from [1460]

with ν ∈ N, i.e. integer fractions of the quantized resistance ρ0 = h/e2 = 25812.807… , which is also called the von-Klitzing constant. In Fig. 15.18, a spin splitting is seen for the n = 1 Landau level (and a small one for the n = 2). We note that the topmost Hall plateau is due to the completely filled n = 0 Landau level; the resistance is ρ0 /2 due to the spin degeneracy of 2. The integer quantum Hall effect, first reported in [1461, 1462], and the value for ρ0 are found for a wide variety of samples and conditions regarding sample temperature, electron density or mobility of the 2DEG and the materials of the heterostructure. Besides the Hall effect in Si-based structures and record mobility (Al,Ga)As/GaAs heterostructures (cf. Fig. 12.37), also (Mg,Zn)O/ZnO heterostructures exhibit the effect [1463, 1464] in the same fashion. Within the plateau, the resistivity is well defined within 10−7 or better up to the 10−9 regime. A precise determination allows for a new normal for the unit Ohm [1389, 1465], being two orders of magnitude more precise than the realization in the SI system, and an independent value for the finestructure constant α = (e2 / h)/(2 c 0 ). At the same time, the longitudinal resistivity, starting from the classical value for small magnetic fields, exhibits oscillations and eventually it is close to zero for the plateaus in ρx y . For ρx x values of 10−10 / have been measured, which corresponds to 10−16 /cm for bulk material, a value three orders of magnitude smaller than for any non-superconductor. The interpretation of the quantum Hall effect(s) is discussed in [1466] among many other treatises. The simplest explanation is that the conductivity is zero when a Landau level is completely filled and the next is completely empty, i.e. the Fermi level lies between them. The temperature is small, i.e. kT ωc , such that no scattering between Landau levels can occur. Thus no current, similar to a completely filled valence band, can flow. The sheet carrier density n s is given by counting the i filled Landau levels (degeneracy according to (15.37)) as ns = i

eB . h

(15.43)

In the transverse direction energy dissipation takes place and the Hall resistivity ρx y = B/(n s e) takes the (scattering-free) values given in (15.42). However, this argument is too simple as it will not explain the extension of the plateaus. As soon as the system has one electron more or less, the Fermi energy will (for a system with δ-like density of

15.2 Magnetic Fields

447

states) be located in the upper or lower Landau level, respectively. Then, the longitudinal conductivity should no longer be zero and the Hall resistivity deviates from the integer fraction of ρ0 . In general, a single particle picture is insufficient to model the IQHE. The accepted model for the explanation of the QHE, supported now with plenty of experimental evidence, is the edge state model where quantized one-dimensional conductivity of edge channels, i.e. the presence of conductive channels along the sample boundaries, is evoked [1475]. The most fundamental arguments for the origin of the IQHE come from gauge invariance and the presence of a macroscopic quantum state of electrons and magnetic flux quanta [1468]. This model holds as long as there are any extended states at all in the inhomogeneously broadened density of states (Landau levels) (Fig. 15.14). These edge states arise from the fact that the quantum Hall state has another topology than the (topologically trivial) surrounding [463, 1469, 1470]. Each plateau corresponds to a distinct topological phase characterized by a Chern number (cmp. (6.29)) related to the ‘Hofstadter butterfly’ [1471, 1472] (cf. Sect. G.3.1). It is remarkable that the classical Hall effect is based on homogeneous conduction for a proper evaluation (cf. Fig. 15.7e), while the quantum Hall effect involves electrical transport only along the edges. A detailed microscopic picture of the edge channels is also of interest. Due to depletion at the boundary of the sample, the density of the 2DEG varies at the edge of the sample and ‘incompressible’ stripes develop for which ∂μ/∂n s → ∞. When the filling factor is far from an integer, the Hall voltage is found to vary linearly across the conductive channel and the current is thus homogeneous over the sample (Fig. 15.20d). In the Hall plateau, the Hall voltage is flat in the center of the channel and exhibits drops at the edges, indicating that the current flows along the boundary of the sample (edge current) [1473] in agreement with predictions from [1476]. Although the current pattern changes with varying magnetic field, the Hall resistivity remains at its quantized value. In graphene, the IQHE plateaus take on the resistance values [1249, 1477], 1 = ±4 ρx y

n+

1 2

e2 , h

(15.44)

with n ∈ N0 . This new ‘half integer’ quantization condition can be translated into the quantized filling factor ν = ±4 (n + 1/2) in the usual QHE formalism of (15.42). The condition (15.44) is due to the different nature of Landau levels for a linear dispersion (Dirac spectrum) [1478]. The +/−-sign denotes the QHE for electrons and holes, respectively. The factor g = 4 stems from the degeneracy of the Landau levels, accounting for spin degeneracy (when the Landau level separation is much larger than the Zeeman spin splitting) and for the sublattice degeneracy. The two n = 0 Hall plateaus have even been observed (for B = 45 T) at room temperature [1479].

15.2.8.2

Fractional QHE

For very low temperatures and in the extreme quantum limit, novel effects are observed when the kinetic energy of the electrons is smaller than their Coulomb interaction. New quantum Hall plateaus are observed at various fractional filling factors ν = p/q. We note that the effects of the fractional quantum Hall effect (FQHE) in Fig. 15.21 mostly arise for magnetic fields beyond the n = 1 IQHE plateau. The filling factor ν = n/(eB/ h) is now interpreted as the number of electrons per magnetic flux quantum φ0 = h/e. The effects of the FQHE cannot be explained by single-electron physics. The plateaus at fractional fillings ν occur when the Fermi energy lies within a highly degenerate Landau (or spin) level and imply the presence of energy gaps due to many-particle interaction and the result of correlated 2D electron motion in the magnetic field.

448

15 External Fields

Fig. 15.20 Normalized Hall potential profile for different magnetic fields around filling factor ν = 2. The overall voltage drop corresponds to 20 mV. The insets show the sample geometry and transport data. The 2DEG is from a GaAs/Al0.33 Ga0.67 As modulation-doped heterostructure, n s = 4.3 × 1011 cm−2 , μ = 5 × 105 cm2 /Vs, T = 1.4 K. Adapted from [1473]

A decisive role is played by the magnetic flux quanta. The presence of the magnetic field requires the many-electron wavefunction to assume as many zeros per unit area as there are flux√quanta penetrating it. The decay of the wavefunction has a length scale of the magnetic length l0 = /(eB). Since the magnetic field implies a 2π phase shift around the zero, such an object is also termed a vortex, being the embodiment of the magnetic flux quanta in the electron system. Such a vortex represents a charge deficit (compared to a homogeneous charge distribution) and thus electrons and vortices attract each other. If a vortex and an electron are placed onto each other, considerable Coulomb energy is gained. At ν = 1/3, there are three times more vortices than there are electrons, each vortex representing a charge deficit of 1/3 e. Such a system is described with many-particle wavefunctions, such as the Laughlin theory for ν = 1/q [1468] and novel quasi-particles called composite fermions [1481, 1482] for other fractional fillings. For further reading we refer readers to [1483] and references therein.

449

Rxx

Rxy (h/e2)

15.2 Magnetic Fields

Fig. 15.21 Hall resistance Rx y and magnetoresistance Rx x of a two-dimensional electron system (GaAs/(Al,Ga)As heterostructure) of density n = 2.33 × 1011 cm−2 at a temperature of 85 mK, versus magnetic field B. Numbers identify the filling factor ν, which indicates the degree to which the sequence of Landau levels is filled with electrons. Plateaus are due to the integral (ν = i) quantum Hall effect (IQHE) and fractional (ν = p/q) quantum Hall effect (FQHE). Adapted from [1480], reprinted with permission, ©1990 AAAS

(a)

(b)

(a)

(b)

Fig. 15.22 Weiss oscillations: a magnetoresistance and b Hall resistance of an antidot lattice (inset in (a)) with pattern (solid lines) and without pattern (dashed lines) at T = 1.5 K. b Schematic of the different orbits: (‘p’: pinned, ‘d’: drifting, ‘s’: scattered). Reprinted with permission from [1484], ©1991 APS

450

15.2.8.3

15 External Fields

Weiss Oscillations

In Fig. 15.22, measurements are shown for a Hall bar in which an array of antidots (in which no conduction is possible) has been introduced by dry etc.hing. The antidot size is 50 nm (plus depletion layer) and the period is 300 nm. These obstructions for the cyclotron motion lead to a modification of the magnetotransport properties. Before etc.hing of the antidot array the 2DEG has a mean free path length of 5–10 µm at 4 K for the mobility of ≈ 106 cm2 /Vs. At low magnetic fields there is a strong deviation of the Hall resistivity from the straight line to which the QHE levels converge. Similarly, ρx x shows a strong effect as well. These